Topics in Applied Physics Volume 104
Topics in Applied Physics is part of the SpringerLink service. For all customers w...

This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!

Topics in Applied Physics Volume 104

Topics in Applied Physics is part of the SpringerLink service. For all customers with standing orders for Topics in Applied Physics we offer the full text in electronic form via SpringerLink free of charge. Please contact your librarian who can receive a password for free access to the full articles by registration at: springerlink.com → Orders If you do not have a standing order you can nevertheless browse through the table of contents of the volumes and the abstracts of each article at: springerlink.com → Browse Publications

Topics in Applied Physics Topics in Applied Physics is a well-established series of review books, each of which presents a comprehensive survey of a selected topic within the broad area of applied physics. Edited and written by leading research scientists in the field concerned, each volume contains review contributions covering the various aspects of the topic. Together these provide an overview of the state of the art in the respective field, extending from an introduction to the subject right up to the frontiers of contemporary research. Topics in Applied Physics is addressed to all scientists at universities and in industry who wish to obtain an overview and to keep abreast of advances in applied physics. The series also provides easy but comprehensive access to the fields for newcomers starting research. Contributions are specially commissioned. The Managing Editors are open to any suggestions for topics coming from the community of applied physicists no matter what the field and encourage prospective editors to approach them with ideas.

Managing Editors Dr. Claus E. Ascheron

Dr. Hans J. Koelsch

Springer-Verlag GmbH Tiergartenstr. 17 69121 Heidelberg Germany Email: [email protected]

Springer-Verlag New York, LLC 233, Spring Street New York, NY 10013 USA Email: [email protected]

Assistant Editor Adelheid H. Duhm Springer-Verlag GmbH Tiergartenstr. 17 69121 Heidelberg Germany Email: [email protected]

David A. Drabold Stefan K. Estreicher (Eds.)

Theory of Defects in Semiconductors

With 60 Figures and 15 Tables

123

David A. Drabold Department of Physics and Astronomy Ohio University Athens, OH 45701, USA [email protected]

Stefan K. Estreicher Physics Department Texas Tech University Lubbock, TX 79409-1051, USA [email protected]

Library of Congress Control Number: 2006934116

Physics and Astronomy Classiﬁcation Scheme (PACS): 71.10.-w, 71.17.-m, 71.23.-k, 71.55.-i, 63.20Mt

ISSN print edition: 0303-4216 ISSN electronic edition: 1437-0859 ISBN-10 3-540-33400-9 Springer Berlin Heidelberg New York ISBN-13 978-3-540-33400-2 Springer Berlin Heidelberg New York This work is subject to copyright. All rights are reserved, whether the whole or part of the material is concerned, specifically the rights of translation, reprinting, reuse of illustrations, recitation, broadcasting, reproduction on microfilm or in any other way, and storage in data banks. Duplication of this publication or parts thereof is permitted only under the provisions of the German Copyright Law of September 9, 1965, in its current version, and permission for use must always be obtained from Springer. Violations are liable for prosecution under the German Copyright Law. Springer is a part of Springer Science+Business Media springer.com © Springer-Verlag Berlin Heidelberg 2007 The use of general descriptive names, registered names, trademarks, etc. in this publication does not imply, even in the absence of a specific statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. Typesetting: DA-TEX · Gerd Blumenstein · www.da-tex.de ockler GbR, Leipzig Production: LE-TEX Jelonek, Schmidt & V¨ Cover design: WMXDesign GmbH, Heidelberg Printed on acid-free paper

57/3100/YL

543210

Contents

Foreword Manuel Cardona . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 1 Early History and Contents of the Present Volume . . . . . . . . . . . . . . . 1 2 Bibliometric Studies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9 Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10 Defect Theory: An Armchair History David A. Drabold, Stefan K. Estreicher . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 The Evolution of Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 A Sketch of First-Principles Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Single-Particle Methods: History . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Direct Approaches to the Many-Electron Problem . . . . . . . . . . . 3.3 Hartree and Hartree–Fock Approximations . . . . . . . . . . . . . . . . . 3.4 Density-Functional Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4.1 Thomas–Fermi Model . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4.2 Modern Density-Functional Theory . . . . . . . . . . . . . . . . . . 4 The Contributions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Supercell Methods for Defect Calculations Risto M. Nieminen . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Density-Functional Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Supercell and Other Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Issues with the Supercell Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 The Exchange-Correlation Functionals and the Semiconducting Gap . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Core and Semicore Electrons: Pseudopotentials and Beyond . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7 Basis Sets . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8 Time-Dependent and Finite-Temperature Simulations . . . . . . . . . . . . 9 Jahn–Teller Distortions in Semiconductor Defects . . . . . . . . . . . . . . .

11 11 13 16 17 18 18 19 19 20 22 23 26 29 29 31 32 34 36 40 42 43 44

X

Contents

9.1 Vacancy in Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.2 Substitutional Copper in Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . 10 Vibrational Modes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11 Ionization Levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12 The Marker Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 13 Brillouin-Zone Sampling . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14 Charged Defects and Electrostatic Corrections . . . . . . . . . . . . . . . . . . 15 Energy-Level References and Valence-Band Alignment . . . . . . . . . . . 16 Examples: The Monovacancy and Substitutional Copper in Silicon . 16.1 Experiments . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 16.2 Calculations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 17 Summary and Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

45 46 47 48 50 51 52 55 56 56 58 60 61 64

Marker-Method Calculations for Electrical Levels Using Gaussian-Orbital Basis Sets J.P. Goss, M.J. Shaw,, P.R. Briddon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Computational Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Gaussian Basis Set . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 Choice of Exponents . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3 Case Study: Bulk Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4 Charge-Density Expansions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Electrical Levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Formation Energy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Calculation of Electrical Levels Using the Marker Method . . . . 4 Application to Defects in Group-IV Materials . . . . . . . . . . . . . . . . . . . 4.1 Chalcogen–Hydrogen Donors in Silicon . . . . . . . . . . . . . . . . . . . . 4.2 VO Centers in Silicon and Germanium . . . . . . . . . . . . . . . . . . . . 4.3 Shallow and Deep Levels in Diamond . . . . . . . . . . . . . . . . . . . . . . 5 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

69 69 71 72 75 76 80 80 81 83 84 84 86 87 89 90 92

Dynamical Matrices and Free Energies Stefan K. Estreicher, Mahdi Sanati . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Dynamical Matrices . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Local and Pseudolocal Modes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Vibrational Lifetimes and Decay Channels . . . . . . . . . . . . . . . . . . . . . . 5 Vibrational Free Energies and Speciﬁc Heats . . . . . . . . . . . . . . . . . . . . 6 Theory of Defects at Finite Temperatures . . . . . . . . . . . . . . . . . . . . . . 7 Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

95 95 97 99 100 101 105 108 110

Contents

XI

Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 112 The Calculation of Free-Energies in Semiconductors: Defects, Transitions and Phase Diagrams E. R. Hern´ andez, A. Antonelli, L. Colombo, P. Ordej´ on . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 The Calculation of Free-Energies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Thermodynamic Integration and Adiabatic Switching . . . . . . . 2.2 Reversible Scaling . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3 Phase Boundaries and Phase Diagrams . . . . . . . . . . . . . . . . . . . . 3 Applications . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Thermal Properties of Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Melting of Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.3 Phase Diagrams . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Conclusions and Outlook . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Quantum Monte Carlo Techniques and Defects in Semiconductors R. J. Needs . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Quantum Monte Carlo Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 The VMC Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 The DMC Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3 Trial Wavefunctions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4 Optimization of Trial Wavefunctions . . . . . . . . . . . . . . . . . . . . . . 2.5 QMC Calculations within Periodic Boundary Conditions . . . . . 2.6 Using Pseudopotentials in QMC Calculations . . . . . . . . . . . . . . . 3 DMC Calculations for Excited States . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Sources of Error in DMC Calculations . . . . . . . . . . . . . . . . . . . . . . . . . 5 Applications of QMC to the Cohesive Energies of Solids . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Applications of QMC to Defects in Semiconductors . . . . . . . . . . . . . . 6.1 Using Structures from Simpler Methods . . . . . . . . . . . . . . . . . . . 6.2 Silicon Self-Interstitial Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.2.1 DFT Calculations on Silicon Self-Interstitials . . . . . . . . . 6.2.2 QMC Calculations on Silicon Self-Interstitials . . . . . . . . . 6.3 Neutral Vacancy in Diamond . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.1 VMC and DMC Calculations on the Neutral Vacancy in Diamond . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.4 Schottky Defects in Magnesium Oxide . . . . . . . . . . . . . . . . . . . . . 7 Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

115 115 116 117 120 122 125 125 128 132 136 136 138

141 141 142 143 144 146 147 147 148 149 149 150 151 151 152 154 156 157 157 158 160 161 163

XII

Contents

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces Arno Schindlmayr, Matthias Scheﬄer . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Computational Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Density-Functional Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 Many-Body Perturbation Theory . . . . . . . . . . . . . . . . . . . . . . . . . 3 Electronic Structure of Defect-Free Surfaces . . . . . . . . . . . . . . . . . . . . 4 Defect States . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 Charge-Transition Levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

165 165 168 168 171 176 179 184 187 188 190

Multiscale Modeling of Defects in Semiconductors: A Novel Molecular-Dynamics Scheme G´ abor Cs´ anyi, Gianpietro Moras, James R. Kermode, Michael C. Payne, Alison Mainwood, Alessandro De Vita . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 A Hybrid View . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Hybrid Simulation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 The LOTF Scheme . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 Applications . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

193 193 194 197 200 203 210 210 211

Empirical Molecular Dynamics: Possibilities, Requirements, and Limitations Kurt Scheerschmidt . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction: Why Empirical Molecular Dynamics? . . . . . . . . . . . . . . 2 Empirical Molecular Dynamics: Basic Concepts . . . . . . . . . . . . . . . . . 2.1 Newtonian Equations and Numerical Integration . . . . . . . . . . . . 2.2 Particle Mechanics and Nonequilibrium Systems . . . . . . . . . . . . 2.3 Boundary Conditions and System Control . . . . . . . . . . . . . . . . . 2.4 Many-Body Empirical Potentials and Force Fields . . . . . . . . . . 2.5 Determination of Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Extensions of the Empirical Molecular Dynamics . . . . . . . . . . . . . . . . 3.1 Modiﬁed Boundary Conditions: Elastic Embedding . . . . . . . . . . 3.2 Tight-Binding-Based Analytic Bond-Order Potentials . . . . . . . 4 Applications . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1 Quantum Dots: Relaxation, Reordering, and Stability . . . . . . . 4.2 Bonded Interfaces: Tailoring Electronic or Mechanical Properties? . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 Conclusions and Outlook . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

213 213 216 216 218 220 221 224 225 225 227 230 231 233 236

Contents

XIII

References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 237 Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 241 Defects in Amorphous Semiconductors: Amorphous Silicon D.A. Drabold, T.A. Abtew . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Amorphous Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Defects in Amorphous Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Deﬁnition of Defect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Long-Time Dynamics and Defect Equilibria . . . . . . . . . . . . . . . . 3.3 Electronic Aspects of Amorphous Semiconductors . . . . . . . . . . . 3.4 Electron Correlation Energy: Electron–Electron Eﬀects . . . . . . 4 Modeling Amorphous Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1 Forming Structural Models . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2 Interatomic Potentials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.3 Lore of Approximations in Density-Functional Calculations . . 4.4 The Electron–Lattice Interaction . . . . . . . . . . . . . . . . . . . . . . . . . 5 Defects in Amorphous Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Light Induced Eﬀects in Amorphous and Glassy Solids S. I. Simdyankin, S. R. Elliott . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Photoinduced Metastability in Amorphous Solids: An Experimental Survey . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.2 Photoinduced Eﬀects in Chalcogenide Glasses . . . . . . . . . . . . . . 2 Theoretical Studies of Photoinduced Excitations in Amorphous Materials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Application of the Density-Functional-Based Tight-Binding Method to the Case of Amorphous As2 S3 . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

245 245 246 248 248 250 250 252 253 253 255 255 257 258 264 266 269 269 269 271 272 273 283 285

Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 287

This book is dedicated to Manuel Cardona, who has done so much for the ﬁeld of defects in semiconductors over the past decades, and convinced so many theorists to calculate beyond what they thought possible.

Preface

Semiconductor materials emerged after World War II and their impact on our lives has grown ever since. Semiconductor technology is, to a large extent, the art of defect engineering. Today, defect control is often done at the atomic level. Theory has played a critical role in understanding, and therefore controlling, the properties of defects. Conversely, the careful experimental studies of defects in Ge, Si, then many other semiconductor materials have generated a huge database of measured quantities that allowed theorists to test their methods and approximations. Dramatic improvement in methodology, especially density-functional theory, along with inexpensive and fast computers, has impedance matched the experimentalist and theorist in ways unanticipated before the late 1980s. As a result, the theory of defects in semiconductors has become quantitative in many respects. Today, more powerful theoretical approaches are still being developed. More importantly perhaps, the tools developed to study defects in semiconductors are now being adapted to approach many new challenges associated with nanoscience, a very long list that includes quantum dots, buckyballs and buckytubes, spintronics, interfaces, and many others. Despite the importance of the ﬁeld, there have been no modern attempts to treat the computational science of the ﬁeld in a coherent manner within a single treatise. This is the aim of the present volume. This book brings together several leaders in theoretical research on defects in semiconductors. Although the treatment is tutorial, the level at which the various applications are discussed is today’s state-of-the-art in the ﬁeld. The book begins with a “big picture” view from Manuel Cardona, and continues with a brief summary of the historical development of the subject in Chap. 1. This includes an overview of today’s most commonly used method to describe defects. We have attempted to create a balanced and tutorial treatment of the basic theory and methodology in Chaps. 3–6. They include detailed discussions of the approximations involved, the calculation of electrically active levels, and extensions of the theory to ﬁnite temperatures. Two emerging electronic structure methodologies of special importance to the ﬁeld are discussed in Chaps. 7 (quantum Monte-Carlo) and 8 (the GW method). Then come two chapters on molecular dynamics (MD). In Chap. 9, a combination of high-

VIII

Preface

level and approximate MD is developed, with applications to the dynamics of extended defect. Chapter 10 deals with semiempirical treatments of microstructures, including issues such as wafer bonding. The book concludes with studies of defects and their role in the photoresponse of topologically disordered (amorphous) systems. The intended audience for the book is graduate students as well as advanced researchers in physics, chemistry, materials science, and engineering. We have sought to provide self-contained descriptions of the work, with detailed references available when needed. The book may be used as a text in a practical graduate course designed to prepare students for research work on defects in semiconductors or ﬁrst-principles theory in materials science in general. The book also serves as a reference for the active theoretical researcher, or as a convenient guide for the experimentalist to keep tabs on their theorist colleagues. It was a genuine pleasure to edit this volume. We are delighted with the contributions provided in a timely fashion by so many busy and accomplished people. We warmly thank all the contributors and hope to have the opportunity to share some nice wine(s) with all of them soon. After all, When Ptolemy, now long ago, Believed the Earth stood still, He never would have blundered so Had he but drunk his ﬁll. He’d then have felt it circulate And would have learnt to say: The true way to investigate Is to drink a bottle a day. (author unknown) published in Augustus de Morgan’s A Budget of Paradoxes, (1866). Athens, Ohio, Lubbock, Texas February 2006

David A. Drabold Stefan K. Estreicher

Contents

Foreword Manuel Cardona . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 1 Early History and Contents of the Present Volume . . . . . . . . . . . . . . . 1 2 Bibliometric Studies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9 Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10 Defect Theory: An Armchair History David A. Drabold, Stefan K. Estreicher . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 The Evolution of Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 A Sketch of First-Principles Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Single-Particle Methods: History . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Direct Approaches to the Many-Electron Problem . . . . . . . . . . . 3.3 Hartree and Hartree–Fock Approximations . . . . . . . . . . . . . . . . . 3.4 Density-Functional Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4.1 Thomas–Fermi Model . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4.2 Modern Density-Functional Theory . . . . . . . . . . . . . . . . . . 4 The Contributions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Supercell Methods for Defect Calculations Risto M. Nieminen . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Density-Functional Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Supercell and Other Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Issues with the Supercell Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 The Exchange-Correlation Functionals and the Semiconducting Gap . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Core and Semicore Electrons: Pseudopotentials and Beyond . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7 Basis Sets . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8 Time-Dependent and Finite-Temperature Simulations . . . . . . . . . . . . 9 Jahn–Teller Distortions in Semiconductor Defects . . . . . . . . . . . . . . .

11 11 13 16 17 18 18 19 19 20 22 23 26 29 29 31 32 34 36 40 42 43 44

X

Contents

9.1 Vacancy in Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.2 Substitutional Copper in Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . 10 Vibrational Modes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11 Ionization Levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12 The Marker Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 13 Brillouin-Zone Sampling . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14 Charged Defects and Electrostatic Corrections . . . . . . . . . . . . . . . . . . 15 Energy-Level References and Valence-Band Alignment . . . . . . . . . . . 16 Examples: The Monovacancy and Substitutional Copper in Silicon . 16.1 Experiments . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 16.2 Calculations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 17 Summary and Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

45 46 47 48 50 51 52 55 56 56 58 60 61 64

Marker-Method Calculations for Electrical Levels Using Gaussian-Orbital Basis Sets J.P. Goss, M.J. Shaw,, P.R. Briddon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Computational Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Gaussian Basis Set . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 Choice of Exponents . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3 Case Study: Bulk Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4 Charge-Density Expansions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Electrical Levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Formation Energy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Calculation of Electrical Levels Using the Marker Method . . . . 4 Application to Defects in Group-IV Materials . . . . . . . . . . . . . . . . . . . 4.1 Chalcogen–Hydrogen Donors in Silicon . . . . . . . . . . . . . . . . . . . . 4.2 VO Centers in Silicon and Germanium . . . . . . . . . . . . . . . . . . . . 4.3 Shallow and Deep Levels in Diamond . . . . . . . . . . . . . . . . . . . . . . 5 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

69 69 71 72 75 76 80 80 81 83 84 84 86 87 89 90 92

Dynamical Matrices and Free Energies Stefan K. Estreicher, Mahdi Sanati . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Dynamical Matrices . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Local and Pseudolocal Modes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Vibrational Lifetimes and Decay Channels . . . . . . . . . . . . . . . . . . . . . . 5 Vibrational Free Energies and Speciﬁc Heats . . . . . . . . . . . . . . . . . . . . 6 Theory of Defects at Finite Temperatures . . . . . . . . . . . . . . . . . . . . . . 7 Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

95 95 97 99 100 101 105 108 110

Contents

XI

Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 112 The Calculation of Free-Energies in Semiconductors: Defects, Transitions and Phase Diagrams E. R. Hern´ andez, A. Antonelli, L. Colombo, P. Ordej´ on . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 The Calculation of Free-Energies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Thermodynamic Integration and Adiabatic Switching . . . . . . . 2.2 Reversible Scaling . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3 Phase Boundaries and Phase Diagrams . . . . . . . . . . . . . . . . . . . . 3 Applications . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Thermal Properties of Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Melting of Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.3 Phase Diagrams . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Conclusions and Outlook . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Quantum Monte Carlo Techniques and Defects in Semiconductors R. J. Needs . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Quantum Monte Carlo Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 The VMC Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 The DMC Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3 Trial Wavefunctions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4 Optimization of Trial Wavefunctions . . . . . . . . . . . . . . . . . . . . . . 2.5 QMC Calculations within Periodic Boundary Conditions . . . . . 2.6 Using Pseudopotentials in QMC Calculations . . . . . . . . . . . . . . . 3 DMC Calculations for Excited States . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Sources of Error in DMC Calculations . . . . . . . . . . . . . . . . . . . . . . . . . 5 Applications of QMC to the Cohesive Energies of Solids . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Applications of QMC to Defects in Semiconductors . . . . . . . . . . . . . . 6.1 Using Structures from Simpler Methods . . . . . . . . . . . . . . . . . . . 6.2 Silicon Self-Interstitial Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.2.1 DFT Calculations on Silicon Self-Interstitials . . . . . . . . . 6.2.2 QMC Calculations on Silicon Self-Interstitials . . . . . . . . . 6.3 Neutral Vacancy in Diamond . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.1 VMC and DMC Calculations on the Neutral Vacancy in Diamond . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.4 Schottky Defects in Magnesium Oxide . . . . . . . . . . . . . . . . . . . . . 7 Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

115 115 116 117 120 122 125 125 128 132 136 136 138

141 141 142 143 144 146 147 147 148 149 149 150 151 151 152 154 156 157 157 158 160 161 163

XII

Contents

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces Arno Schindlmayr, Matthias Scheﬄer . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Computational Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Density-Functional Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 Many-Body Perturbation Theory . . . . . . . . . . . . . . . . . . . . . . . . . 3 Electronic Structure of Defect-Free Surfaces . . . . . . . . . . . . . . . . . . . . 4 Defect States . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 Charge-Transition Levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

165 165 168 168 171 176 179 184 187 188 190

Multiscale Modeling of Defects in Semiconductors: A Novel Molecular-Dynamics Scheme G´ abor Cs´ anyi, Gianpietro Moras, James R. Kermode, Michael C. Payne, Alison Mainwood, Alessandro De Vita . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 A Hybrid View . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Hybrid Simulation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 The LOTF Scheme . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 Applications . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

193 193 194 197 200 203 210 210 211

Empirical Molecular Dynamics: Possibilities, Requirements, and Limitations Kurt Scheerschmidt . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction: Why Empirical Molecular Dynamics? . . . . . . . . . . . . . . 2 Empirical Molecular Dynamics: Basic Concepts . . . . . . . . . . . . . . . . . 2.1 Newtonian Equations and Numerical Integration . . . . . . . . . . . . 2.2 Particle Mechanics and Nonequilibrium Systems . . . . . . . . . . . . 2.3 Boundary Conditions and System Control . . . . . . . . . . . . . . . . . 2.4 Many-Body Empirical Potentials and Force Fields . . . . . . . . . . 2.5 Determination of Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Extensions of the Empirical Molecular Dynamics . . . . . . . . . . . . . . . . 3.1 Modiﬁed Boundary Conditions: Elastic Embedding . . . . . . . . . . 3.2 Tight-Binding-Based Analytic Bond-Order Potentials . . . . . . . 4 Applications . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1 Quantum Dots: Relaxation, Reordering, and Stability . . . . . . . 4.2 Bonded Interfaces: Tailoring Electronic or Mechanical Properties? . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 Conclusions and Outlook . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

213 213 216 216 218 220 221 224 225 225 227 230 231 233 236

Contents

XIII

References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 237 Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 241 Defects in Amorphous Semiconductors: Amorphous Silicon D.A. Drabold, T.A. Abtew . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Amorphous Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Defects in Amorphous Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Deﬁnition of Defect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Long-Time Dynamics and Defect Equilibria . . . . . . . . . . . . . . . . 3.3 Electronic Aspects of Amorphous Semiconductors . . . . . . . . . . . 3.4 Electron Correlation Energy: Electron–Electron Eﬀects . . . . . . 4 Modeling Amorphous Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1 Forming Structural Models . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2 Interatomic Potentials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.3 Lore of Approximations in Density-Functional Calculations . . 4.4 The Electron–Lattice Interaction . . . . . . . . . . . . . . . . . . . . . . . . . 5 Defects in Amorphous Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Light Induced Eﬀects in Amorphous and Glassy Solids S. I. Simdyankin, S. R. Elliott . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Photoinduced Metastability in Amorphous Solids: An Experimental Survey . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.2 Photoinduced Eﬀects in Chalcogenide Glasses . . . . . . . . . . . . . . 2 Theoretical Studies of Photoinduced Excitations in Amorphous Materials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Application of the Density-Functional-Based Tight-Binding Method to the Case of Amorphous As2 S3 . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

245 245 246 248 248 250 250 252 253 253 255 255 257 258 264 266 269 269 269 271 272 273 283 285

Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 287

This book is dedicated to Manuel Cardona, who has done so much for the ﬁeld of defects in semiconductors over the past decades, and convinced so many theorists to calculate beyond what they thought possible.

Preface

Semiconductor materials emerged after World War II and their impact on our lives has grown ever since. Semiconductor technology is, to a large extent, the art of defect engineering. Today, defect control is often done at the atomic level. Theory has played a critical role in understanding, and therefore controlling, the properties of defects. Conversely, the careful experimental studies of defects in Ge, Si, then many other semiconductor materials have generated a huge database of measured quantities that allowed theorists to test their methods and approximations. Dramatic improvement in methodology, especially density-functional theory, along with inexpensive and fast computers, has impedance matched the experimentalist and theorist in ways unanticipated before the late 1980s. As a result, the theory of defects in semiconductors has become quantitative in many respects. Today, more powerful theoretical approaches are still being developed. More importantly perhaps, the tools developed to study defects in semiconductors are now being adapted to approach many new challenges associated with nanoscience, a very long list that includes quantum dots, buckyballs and buckytubes, spintronics, interfaces, and many others. Despite the importance of the ﬁeld, there have been no modern attempts to treat the computational science of the ﬁeld in a coherent manner within a single treatise. This is the aim of the present volume. This book brings together several leaders in theoretical research on defects in semiconductors. Although the treatment is tutorial, the level at which the various applications are discussed is today’s state-of-the-art in the ﬁeld. The book begins with a “big picture” view from Manuel Cardona, and continues with a brief summary of the historical development of the subject in Chap. 1. This includes an overview of today’s most commonly used method to describe defects. We have attempted to create a balanced and tutorial treatment of the basic theory and methodology in Chaps. 3–6. They include detailed discussions of the approximations involved, the calculation of electrically active levels, and extensions of the theory to ﬁnite temperatures. Two emerging electronic structure methodologies of special importance to the ﬁeld are discussed in Chaps. 7 (quantum Monte-Carlo) and 8 (the GW method). Then come two chapters on molecular dynamics (MD). In Chap. 9, a combination of high-

VIII

Preface

level and approximate MD is developed, with applications to the dynamics of extended defect. Chapter 10 deals with semiempirical treatments of microstructures, including issues such as wafer bonding. The book concludes with studies of defects and their role in the photoresponse of topologically disordered (amorphous) systems. The intended audience for the book is graduate students as well as advanced researchers in physics, chemistry, materials science, and engineering. We have sought to provide self-contained descriptions of the work, with detailed references available when needed. The book may be used as a text in a practical graduate course designed to prepare students for research work on defects in semiconductors or ﬁrst-principles theory in materials science in general. The book also serves as a reference for the active theoretical researcher, or as a convenient guide for the experimentalist to keep tabs on their theorist colleagues. It was a genuine pleasure to edit this volume. We are delighted with the contributions provided in a timely fashion by so many busy and accomplished people. We warmly thank all the contributors and hope to have the opportunity to share some nice wine(s) with all of them soon. After all, When Ptolemy, now long ago, Believed the Earth stood still, He never would have blundered so Had he but drunk his ﬁll. He’d then have felt it circulate And would have learnt to say: The true way to investigate Is to drink a bottle a day. (author unknown) published in Augustus de Morgan’s A Budget of Paradoxes, (1866). Athens, Ohio, Lubbock, Texas February 2006

David A. Drabold Stefan K. Estreicher

Contents

Foreword Manuel Cardona . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 1 Early History and Contents of the Present Volume . . . . . . . . . . . . . . . 1 2 Bibliometric Studies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9 Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10 Defect Theory: An Armchair History David A. Drabold, Stefan K. Estreicher . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 The Evolution of Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 A Sketch of First-Principles Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Single-Particle Methods: History . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Direct Approaches to the Many-Electron Problem . . . . . . . . . . . 3.3 Hartree and Hartree–Fock Approximations . . . . . . . . . . . . . . . . . 3.4 Density-Functional Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4.1 Thomas–Fermi Model . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4.2 Modern Density-Functional Theory . . . . . . . . . . . . . . . . . . 4 The Contributions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Supercell Methods for Defect Calculations Risto M. Nieminen . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Density-Functional Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Supercell and Other Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Issues with the Supercell Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 The Exchange-Correlation Functionals and the Semiconducting Gap . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Core and Semicore Electrons: Pseudopotentials and Beyond . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7 Basis Sets . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8 Time-Dependent and Finite-Temperature Simulations . . . . . . . . . . . . 9 Jahn–Teller Distortions in Semiconductor Defects . . . . . . . . . . . . . . .

11 11 13 16 17 18 18 19 19 20 22 23 26 29 29 31 32 34 36 40 42 43 44

X

Contents

9.1 Vacancy in Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.2 Substitutional Copper in Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . 10 Vibrational Modes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11 Ionization Levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12 The Marker Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 13 Brillouin-Zone Sampling . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14 Charged Defects and Electrostatic Corrections . . . . . . . . . . . . . . . . . . 15 Energy-Level References and Valence-Band Alignment . . . . . . . . . . . 16 Examples: The Monovacancy and Substitutional Copper in Silicon . 16.1 Experiments . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 16.2 Calculations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 17 Summary and Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

45 46 47 48 50 51 52 55 56 56 58 60 61 64

Marker-Method Calculations for Electrical Levels Using Gaussian-Orbital Basis Sets J.P. Goss, M.J. Shaw,, P.R. Briddon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Computational Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Gaussian Basis Set . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 Choice of Exponents . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3 Case Study: Bulk Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4 Charge-Density Expansions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Electrical Levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Formation Energy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Calculation of Electrical Levels Using the Marker Method . . . . 4 Application to Defects in Group-IV Materials . . . . . . . . . . . . . . . . . . . 4.1 Chalcogen–Hydrogen Donors in Silicon . . . . . . . . . . . . . . . . . . . . 4.2 VO Centers in Silicon and Germanium . . . . . . . . . . . . . . . . . . . . 4.3 Shallow and Deep Levels in Diamond . . . . . . . . . . . . . . . . . . . . . . 5 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

69 69 71 72 75 76 80 80 81 83 84 84 86 87 89 90 92

Dynamical Matrices and Free Energies Stefan K. Estreicher, Mahdi Sanati . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Dynamical Matrices . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Local and Pseudolocal Modes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Vibrational Lifetimes and Decay Channels . . . . . . . . . . . . . . . . . . . . . . 5 Vibrational Free Energies and Speciﬁc Heats . . . . . . . . . . . . . . . . . . . . 6 Theory of Defects at Finite Temperatures . . . . . . . . . . . . . . . . . . . . . . 7 Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

95 95 97 99 100 101 105 108 110

Contents

XI

Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 112 The Calculation of Free-Energies in Semiconductors: Defects, Transitions and Phase Diagrams E. R. Hern´ andez, A. Antonelli, L. Colombo, P. Ordej´ on . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 The Calculation of Free-Energies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Thermodynamic Integration and Adiabatic Switching . . . . . . . 2.2 Reversible Scaling . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3 Phase Boundaries and Phase Diagrams . . . . . . . . . . . . . . . . . . . . 3 Applications . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Thermal Properties of Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Melting of Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.3 Phase Diagrams . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Conclusions and Outlook . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Quantum Monte Carlo Techniques and Defects in Semiconductors R. J. Needs . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Quantum Monte Carlo Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 The VMC Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 The DMC Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3 Trial Wavefunctions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4 Optimization of Trial Wavefunctions . . . . . . . . . . . . . . . . . . . . . . 2.5 QMC Calculations within Periodic Boundary Conditions . . . . . 2.6 Using Pseudopotentials in QMC Calculations . . . . . . . . . . . . . . . 3 DMC Calculations for Excited States . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Sources of Error in DMC Calculations . . . . . . . . . . . . . . . . . . . . . . . . . 5 Applications of QMC to the Cohesive Energies of Solids . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Applications of QMC to Defects in Semiconductors . . . . . . . . . . . . . . 6.1 Using Structures from Simpler Methods . . . . . . . . . . . . . . . . . . . 6.2 Silicon Self-Interstitial Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.2.1 DFT Calculations on Silicon Self-Interstitials . . . . . . . . . 6.2.2 QMC Calculations on Silicon Self-Interstitials . . . . . . . . . 6.3 Neutral Vacancy in Diamond . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.1 VMC and DMC Calculations on the Neutral Vacancy in Diamond . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.4 Schottky Defects in Magnesium Oxide . . . . . . . . . . . . . . . . . . . . . 7 Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

115 115 116 117 120 122 125 125 128 132 136 136 138

141 141 142 143 144 146 147 147 148 149 149 150 151 151 152 154 156 157 157 158 160 161 163

XII

Contents

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces Arno Schindlmayr, Matthias Scheﬄer . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Computational Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Density-Functional Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 Many-Body Perturbation Theory . . . . . . . . . . . . . . . . . . . . . . . . . 3 Electronic Structure of Defect-Free Surfaces . . . . . . . . . . . . . . . . . . . . 4 Defect States . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 Charge-Transition Levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

165 165 168 168 171 176 179 184 187 188 190

Multiscale Modeling of Defects in Semiconductors: A Novel Molecular-Dynamics Scheme G´ abor Cs´ anyi, Gianpietro Moras, James R. Kermode, Michael C. Payne, Alison Mainwood, Alessandro De Vita . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 A Hybrid View . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Hybrid Simulation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 The LOTF Scheme . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 Applications . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

193 193 194 197 200 203 210 210 211

Empirical Molecular Dynamics: Possibilities, Requirements, and Limitations Kurt Scheerschmidt . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction: Why Empirical Molecular Dynamics? . . . . . . . . . . . . . . 2 Empirical Molecular Dynamics: Basic Concepts . . . . . . . . . . . . . . . . . 2.1 Newtonian Equations and Numerical Integration . . . . . . . . . . . . 2.2 Particle Mechanics and Nonequilibrium Systems . . . . . . . . . . . . 2.3 Boundary Conditions and System Control . . . . . . . . . . . . . . . . . 2.4 Many-Body Empirical Potentials and Force Fields . . . . . . . . . . 2.5 Determination of Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Extensions of the Empirical Molecular Dynamics . . . . . . . . . . . . . . . . 3.1 Modiﬁed Boundary Conditions: Elastic Embedding . . . . . . . . . . 3.2 Tight-Binding-Based Analytic Bond-Order Potentials . . . . . . . 4 Applications . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1 Quantum Dots: Relaxation, Reordering, and Stability . . . . . . . 4.2 Bonded Interfaces: Tailoring Electronic or Mechanical Properties? . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 Conclusions and Outlook . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

213 213 216 216 218 220 221 224 225 225 227 230 231 233 236

Contents

XIII

References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 237 Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 241 Defects in Amorphous Semiconductors: Amorphous Silicon D.A. Drabold, T.A. Abtew . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Amorphous Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Defects in Amorphous Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Deﬁnition of Defect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Long-Time Dynamics and Defect Equilibria . . . . . . . . . . . . . . . . 3.3 Electronic Aspects of Amorphous Semiconductors . . . . . . . . . . . 3.4 Electron Correlation Energy: Electron–Electron Eﬀects . . . . . . 4 Modeling Amorphous Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1 Forming Structural Models . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2 Interatomic Potentials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.3 Lore of Approximations in Density-Functional Calculations . . 4.4 The Electron–Lattice Interaction . . . . . . . . . . . . . . . . . . . . . . . . . 5 Defects in Amorphous Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Light Induced Eﬀects in Amorphous and Glassy Solids S. I. Simdyankin, S. R. Elliott . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Photoinduced Metastability in Amorphous Solids: An Experimental Survey . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.2 Photoinduced Eﬀects in Chalcogenide Glasses . . . . . . . . . . . . . . 2 Theoretical Studies of Photoinduced Excitations in Amorphous Materials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Application of the Density-Functional-Based Tight-Binding Method to the Case of Amorphous As2 S3 . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

245 245 246 248 248 250 250 252 253 253 255 255 257 258 264 266 269 269 269 271 272 273 283 285

Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 287

This book is dedicated to Manuel Cardona, who has done so much for the ﬁeld of defects in semiconductors over the past decades, and convinced so many theorists to calculate beyond what they thought possible.

Preface

Semiconductor materials emerged after World War II and their impact on our lives has grown ever since. Semiconductor technology is, to a large extent, the art of defect engineering. Today, defect control is often done at the atomic level. Theory has played a critical role in understanding, and therefore controlling, the properties of defects. Conversely, the careful experimental studies of defects in Ge, Si, then many other semiconductor materials have generated a huge database of measured quantities that allowed theorists to test their methods and approximations. Dramatic improvement in methodology, especially density-functional theory, along with inexpensive and fast computers, has impedance matched the experimentalist and theorist in ways unanticipated before the late 1980s. As a result, the theory of defects in semiconductors has become quantitative in many respects. Today, more powerful theoretical approaches are still being developed. More importantly perhaps, the tools developed to study defects in semiconductors are now being adapted to approach many new challenges associated with nanoscience, a very long list that includes quantum dots, buckyballs and buckytubes, spintronics, interfaces, and many others. Despite the importance of the ﬁeld, there have been no modern attempts to treat the computational science of the ﬁeld in a coherent manner within a single treatise. This is the aim of the present volume. This book brings together several leaders in theoretical research on defects in semiconductors. Although the treatment is tutorial, the level at which the various applications are discussed is today’s state-of-the-art in the ﬁeld. The book begins with a “big picture” view from Manuel Cardona, and continues with a brief summary of the historical development of the subject in Chap. 1. This includes an overview of today’s most commonly used method to describe defects. We have attempted to create a balanced and tutorial treatment of the basic theory and methodology in Chaps. 3–6. They include detailed discussions of the approximations involved, the calculation of electrically active levels, and extensions of the theory to ﬁnite temperatures. Two emerging electronic structure methodologies of special importance to the ﬁeld are discussed in Chaps. 7 (quantum Monte-Carlo) and 8 (the GW method). Then come two chapters on molecular dynamics (MD). In Chap. 9, a combination of high-

VIII

Preface

level and approximate MD is developed, with applications to the dynamics of extended defect. Chapter 10 deals with semiempirical treatments of microstructures, including issues such as wafer bonding. The book concludes with studies of defects and their role in the photoresponse of topologically disordered (amorphous) systems. The intended audience for the book is graduate students as well as advanced researchers in physics, chemistry, materials science, and engineering. We have sought to provide self-contained descriptions of the work, with detailed references available when needed. The book may be used as a text in a practical graduate course designed to prepare students for research work on defects in semiconductors or ﬁrst-principles theory in materials science in general. The book also serves as a reference for the active theoretical researcher, or as a convenient guide for the experimentalist to keep tabs on their theorist colleagues. It was a genuine pleasure to edit this volume. We are delighted with the contributions provided in a timely fashion by so many busy and accomplished people. We warmly thank all the contributors and hope to have the opportunity to share some nice wine(s) with all of them soon. After all, When Ptolemy, now long ago, Believed the Earth stood still, He never would have blundered so Had he but drunk his ﬁll. He’d then have felt it circulate And would have learnt to say: The true way to investigate Is to drink a bottle a day. (author unknown) published in Augustus de Morgan’s A Budget of Paradoxes, (1866). Athens, Ohio, Lubbock, Texas February 2006

David A. Drabold Stefan K. Estreicher

Contents

Foreword Manuel Cardona . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 1 Early History and Contents of the Present Volume . . . . . . . . . . . . . . . 1 2 Bibliometric Studies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9 Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10 Defect Theory: An Armchair History David A. Drabold, Stefan K. Estreicher . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 The Evolution of Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 A Sketch of First-Principles Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Single-Particle Methods: History . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Direct Approaches to the Many-Electron Problem . . . . . . . . . . . 3.3 Hartree and Hartree–Fock Approximations . . . . . . . . . . . . . . . . . 3.4 Density-Functional Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4.1 Thomas–Fermi Model . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4.2 Modern Density-Functional Theory . . . . . . . . . . . . . . . . . . 4 The Contributions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Supercell Methods for Defect Calculations Risto M. Nieminen . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Density-Functional Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Supercell and Other Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Issues with the Supercell Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 The Exchange-Correlation Functionals and the Semiconducting Gap . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Core and Semicore Electrons: Pseudopotentials and Beyond . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7 Basis Sets . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8 Time-Dependent and Finite-Temperature Simulations . . . . . . . . . . . . 9 Jahn–Teller Distortions in Semiconductor Defects . . . . . . . . . . . . . . .

11 11 13 16 17 18 18 19 19 20 22 23 26 29 29 31 32 34 36 40 42 43 44

X

Contents

9.1 Vacancy in Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.2 Substitutional Copper in Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . 10 Vibrational Modes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11 Ionization Levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12 The Marker Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 13 Brillouin-Zone Sampling . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14 Charged Defects and Electrostatic Corrections . . . . . . . . . . . . . . . . . . 15 Energy-Level References and Valence-Band Alignment . . . . . . . . . . . 16 Examples: The Monovacancy and Substitutional Copper in Silicon . 16.1 Experiments . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 16.2 Calculations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 17 Summary and Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

45 46 47 48 50 51 52 55 56 56 58 60 61 64

Marker-Method Calculations for Electrical Levels Using Gaussian-Orbital Basis Sets J.P. Goss, M.J. Shaw,, P.R. Briddon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Computational Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Gaussian Basis Set . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 Choice of Exponents . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3 Case Study: Bulk Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4 Charge-Density Expansions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Electrical Levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Formation Energy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Calculation of Electrical Levels Using the Marker Method . . . . 4 Application to Defects in Group-IV Materials . . . . . . . . . . . . . . . . . . . 4.1 Chalcogen–Hydrogen Donors in Silicon . . . . . . . . . . . . . . . . . . . . 4.2 VO Centers in Silicon and Germanium . . . . . . . . . . . . . . . . . . . . 4.3 Shallow and Deep Levels in Diamond . . . . . . . . . . . . . . . . . . . . . . 5 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

69 69 71 72 75 76 80 80 81 83 84 84 86 87 89 90 92

Dynamical Matrices and Free Energies Stefan K. Estreicher, Mahdi Sanati . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Dynamical Matrices . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Local and Pseudolocal Modes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Vibrational Lifetimes and Decay Channels . . . . . . . . . . . . . . . . . . . . . . 5 Vibrational Free Energies and Speciﬁc Heats . . . . . . . . . . . . . . . . . . . . 6 Theory of Defects at Finite Temperatures . . . . . . . . . . . . . . . . . . . . . . 7 Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

95 95 97 99 100 101 105 108 110

Contents

XI

Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 112 The Calculation of Free-Energies in Semiconductors: Defects, Transitions and Phase Diagrams E. R. Hern´ andez, A. Antonelli, L. Colombo, P. Ordej´ on . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 The Calculation of Free-Energies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Thermodynamic Integration and Adiabatic Switching . . . . . . . 2.2 Reversible Scaling . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3 Phase Boundaries and Phase Diagrams . . . . . . . . . . . . . . . . . . . . 3 Applications . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Thermal Properties of Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Melting of Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.3 Phase Diagrams . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Conclusions and Outlook . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Quantum Monte Carlo Techniques and Defects in Semiconductors R. J. Needs . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Quantum Monte Carlo Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 The VMC Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 The DMC Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3 Trial Wavefunctions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4 Optimization of Trial Wavefunctions . . . . . . . . . . . . . . . . . . . . . . 2.5 QMC Calculations within Periodic Boundary Conditions . . . . . 2.6 Using Pseudopotentials in QMC Calculations . . . . . . . . . . . . . . . 3 DMC Calculations for Excited States . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Sources of Error in DMC Calculations . . . . . . . . . . . . . . . . . . . . . . . . . 5 Applications of QMC to the Cohesive Energies of Solids . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Applications of QMC to Defects in Semiconductors . . . . . . . . . . . . . . 6.1 Using Structures from Simpler Methods . . . . . . . . . . . . . . . . . . . 6.2 Silicon Self-Interstitial Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.2.1 DFT Calculations on Silicon Self-Interstitials . . . . . . . . . 6.2.2 QMC Calculations on Silicon Self-Interstitials . . . . . . . . . 6.3 Neutral Vacancy in Diamond . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.1 VMC and DMC Calculations on the Neutral Vacancy in Diamond . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.4 Schottky Defects in Magnesium Oxide . . . . . . . . . . . . . . . . . . . . . 7 Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

115 115 116 117 120 122 125 125 128 132 136 136 138

141 141 142 143 144 146 147 147 148 149 149 150 151 151 152 154 156 157 157 158 160 161 163

XII

Contents

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces Arno Schindlmayr, Matthias Scheﬄer . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Computational Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Density-Functional Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 Many-Body Perturbation Theory . . . . . . . . . . . . . . . . . . . . . . . . . 3 Electronic Structure of Defect-Free Surfaces . . . . . . . . . . . . . . . . . . . . 4 Defect States . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 Charge-Transition Levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

165 165 168 168 171 176 179 184 187 188 190

Multiscale Modeling of Defects in Semiconductors: A Novel Molecular-Dynamics Scheme G´ abor Cs´ anyi, Gianpietro Moras, James R. Kermode, Michael C. Payne, Alison Mainwood, Alessandro De Vita . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 A Hybrid View . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Hybrid Simulation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 The LOTF Scheme . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 Applications . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

193 193 194 197 200 203 210 210 211

Empirical Molecular Dynamics: Possibilities, Requirements, and Limitations Kurt Scheerschmidt . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction: Why Empirical Molecular Dynamics? . . . . . . . . . . . . . . 2 Empirical Molecular Dynamics: Basic Concepts . . . . . . . . . . . . . . . . . 2.1 Newtonian Equations and Numerical Integration . . . . . . . . . . . . 2.2 Particle Mechanics and Nonequilibrium Systems . . . . . . . . . . . . 2.3 Boundary Conditions and System Control . . . . . . . . . . . . . . . . . 2.4 Many-Body Empirical Potentials and Force Fields . . . . . . . . . . 2.5 Determination of Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Extensions of the Empirical Molecular Dynamics . . . . . . . . . . . . . . . . 3.1 Modiﬁed Boundary Conditions: Elastic Embedding . . . . . . . . . . 3.2 Tight-Binding-Based Analytic Bond-Order Potentials . . . . . . . 4 Applications . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1 Quantum Dots: Relaxation, Reordering, and Stability . . . . . . . 4.2 Bonded Interfaces: Tailoring Electronic or Mechanical Properties? . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 Conclusions and Outlook . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

213 213 216 216 218 220 221 224 225 225 227 230 231 233 236

Contents

XIII

References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 237 Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 241 Defects in Amorphous Semiconductors: Amorphous Silicon D.A. Drabold, T.A. Abtew . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Amorphous Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Defects in Amorphous Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Deﬁnition of Defect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Long-Time Dynamics and Defect Equilibria . . . . . . . . . . . . . . . . 3.3 Electronic Aspects of Amorphous Semiconductors . . . . . . . . . . . 3.4 Electron Correlation Energy: Electron–Electron Eﬀects . . . . . . 4 Modeling Amorphous Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1 Forming Structural Models . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2 Interatomic Potentials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.3 Lore of Approximations in Density-Functional Calculations . . 4.4 The Electron–Lattice Interaction . . . . . . . . . . . . . . . . . . . . . . . . . 5 Defects in Amorphous Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Light Induced Eﬀects in Amorphous and Glassy Solids S. I. Simdyankin, S. R. Elliott . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Photoinduced Metastability in Amorphous Solids: An Experimental Survey . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.2 Photoinduced Eﬀects in Chalcogenide Glasses . . . . . . . . . . . . . . 2 Theoretical Studies of Photoinduced Excitations in Amorphous Materials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Application of the Density-Functional-Based Tight-Binding Method to the Case of Amorphous As2 S3 . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

245 245 246 248 248 250 250 252 253 253 255 255 257 258 264 266 269 269 269 271 272 273 283 285

Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 287

This book is dedicated to Manuel Cardona, who has done so much for the ﬁeld of defects in semiconductors over the past decades, and convinced so many theorists to calculate beyond what they thought possible.

Preface

Semiconductor materials emerged after World War II and their impact on our lives has grown ever since. Semiconductor technology is, to a large extent, the art of defect engineering. Today, defect control is often done at the atomic level. Theory has played a critical role in understanding, and therefore controlling, the properties of defects. Conversely, the careful experimental studies of defects in Ge, Si, then many other semiconductor materials have generated a huge database of measured quantities that allowed theorists to test their methods and approximations. Dramatic improvement in methodology, especially density-functional theory, along with inexpensive and fast computers, has impedance matched the experimentalist and theorist in ways unanticipated before the late 1980s. As a result, the theory of defects in semiconductors has become quantitative in many respects. Today, more powerful theoretical approaches are still being developed. More importantly perhaps, the tools developed to study defects in semiconductors are now being adapted to approach many new challenges associated with nanoscience, a very long list that includes quantum dots, buckyballs and buckytubes, spintronics, interfaces, and many others. Despite the importance of the ﬁeld, there have been no modern attempts to treat the computational science of the ﬁeld in a coherent manner within a single treatise. This is the aim of the present volume. This book brings together several leaders in theoretical research on defects in semiconductors. Although the treatment is tutorial, the level at which the various applications are discussed is today’s state-of-the-art in the ﬁeld. The book begins with a “big picture” view from Manuel Cardona, and continues with a brief summary of the historical development of the subject in Chap. 1. This includes an overview of today’s most commonly used method to describe defects. We have attempted to create a balanced and tutorial treatment of the basic theory and methodology in Chaps. 3–6. They include detailed discussions of the approximations involved, the calculation of electrically active levels, and extensions of the theory to ﬁnite temperatures. Two emerging electronic structure methodologies of special importance to the ﬁeld are discussed in Chaps. 7 (quantum Monte-Carlo) and 8 (the GW method). Then come two chapters on molecular dynamics (MD). In Chap. 9, a combination of high-

VIII

Preface

level and approximate MD is developed, with applications to the dynamics of extended defect. Chapter 10 deals with semiempirical treatments of microstructures, including issues such as wafer bonding. The book concludes with studies of defects and their role in the photoresponse of topologically disordered (amorphous) systems. The intended audience for the book is graduate students as well as advanced researchers in physics, chemistry, materials science, and engineering. We have sought to provide self-contained descriptions of the work, with detailed references available when needed. The book may be used as a text in a practical graduate course designed to prepare students for research work on defects in semiconductors or ﬁrst-principles theory in materials science in general. The book also serves as a reference for the active theoretical researcher, or as a convenient guide for the experimentalist to keep tabs on their theorist colleagues. It was a genuine pleasure to edit this volume. We are delighted with the contributions provided in a timely fashion by so many busy and accomplished people. We warmly thank all the contributors and hope to have the opportunity to share some nice wine(s) with all of them soon. After all, When Ptolemy, now long ago, Believed the Earth stood still, He never would have blundered so Had he but drunk his ﬁll. He’d then have felt it circulate And would have learnt to say: The true way to investigate Is to drink a bottle a day. (author unknown) published in Augustus de Morgan’s A Budget of Paradoxes, (1866). Athens, Ohio, Lubbock, Texas February 2006

David A. Drabold Stefan K. Estreicher

Foreword Manuel Cardona Max-Planck-Institut f¨ ur Festk¨ orperforschung, 70569 Stuttgart, Germany [email protected]

Man sollte sich mit Halbleitern nicht besch¨ aftigen, das sind Dreckeﬀekte – wer weiss, ob sie wirklich existieren. Wolfgang Pauli, 1931

1 Early History and Contents of the Present Volume This volume contains a comprehensive description of developments in the ﬁeld of defects in semiconductors that have taken place during the past two decades. Although the ﬁeld of defects in semiconductors is at least 60 years old, it had to wait, in order to reach maturity, for the colossal increase in computer power that has more recently taken place, following the predictions of Moore’s law [1]. The ingenuity of computational theorists in developing algorithms to reduce the intractable many-body problem of defect and host to one that can be handled with existing and aﬀordable computer power has also played a signiﬁcant role: much of it is described in the present volume. As computational power grew, the simplifying assumptions of these algorithms, some of them hard to justify, were reduced. The predictive accuracy of the new calculations then took a great leap forward. In the early days, the real-space structure of the defect had to be postulated in order to get on with the theory and self-consistency of the electronic calculations was beyond reach. During the past two decades emphasis has been placed in calculating the real-space structure of defect plus host and achieving self-consistency in the electronic calculations. The results of these new calculations have been a great help to experimentalists groping to interpret complicated data related to defects. I have added up the number of references in the various chapters of the book corresponding to years before 1990 and found that they amount to only 25 % of the total number of references. Many of the remaining 75 % of references are actually even more recent, having been published after the year 2000. Thus one can say that the contents of the volume represent the state-of-the-art in the ﬁeld. Whereas most of the chapters are concerned with defects in crystalline semiconductors, Chaps. 10 and 11 deal with defects in amorphous materials, in particular amorphous silicon, a ﬁeld about which much less information is available. D. A. Drabold, S. K. Estreicher (Eds.): Theory of Defects in Semiconductors, Topics Appl. Physics 104, 1–10 (2007) © Springer-Verlag Berlin Heidelberg 2007

2

Manuel Cardona

The three aspects of the defect problem, real-space structure, electronic structure and vibrational properties are discussed in the various Chapters of the book, mainly from the theoretical point of view. Defects break the translational symmetry of a crystal, a property that already made possible rather realistic calculations of the host materials half a century ago. Small crystals and clusters with a relatively small number of atoms (including impurities and other defects), have become useful to circumvent, in theoretical calculations, the lack of translational symmetry in the presence of defects or in amorphous materials. The main source of uncertainty in the state-ofthe-art calculations remains the small number of cluster atoms imposed by the computational strictures. This number is often smaller than that corresponding to real-world samples, even including nanostructures. Clusters with a number of atoms that can be accommodated by extant computers are then repeated periodically so as to obtain a crystal lattice, with a supercell and a mini-Brillouin zone. Although these lattices do not exactly correspond to physical reality, they enable the use of k-space techniques and are instrumental in keeping computer power to available and aﬀordable levels. Another widespread approach is to treat the cluster in real space after passivating the ﬁctitious surface with hydrogen atoms or the like. When using these methods it is good practice to check convergence with respect to the cluster size by performing similar calculations for at least two sets of clusters with numbers of atoms diﬀering, say, by a factor of two. The epigraph above, attributed to Wolfgang Pauli, translates as One should not keep busy with semiconductors, they are dirt eﬀects – Who knows whether they really exist. The 24 authors of this book, like many tens of thousands of other physicists and engineers, have fortunately not heeded Pauli’s advice (given in 1931, 14 years before he received the Nobel Prize). Had they done so, not only would the world have missed a revolutionary and nowadays ubiquitous technology, but basic physical science would have lost some of the most fruitful, beautiful and successful applications of quantum mechanics. “Dreckeﬀekte” is often imprecisely translated as eﬀects of dirt, i.e., as eﬀects of impurities. However, eﬀects of structural defects would also fall into the category of Dreckeﬀekte. In Pauli’s days applications of semiconductors, including variation of resistivity through doping leading to photocells and rectiﬁers, had been arrived at purely empirically, through some sort of trial and error alchemy. I remember as a child using galena (PbS) detectors in crystal radio sets. I had lots of galena from various sources: some of it worked, some not but nobody seemed to know why. Sixty years later, only a few months ago, I was measuring PbS samples in order to characterize the number of carriers (of nonstoichiometric origin involving vacancies) and their type (n or p) so as to wrap up original research on this canonical material [2]. Today, GOOGLE lists 860 000 entries under the heading “defects in

Foreword

3

semiconductors”. The Web of Science (WoS) lists 3736 mentions in the title and abstract of source articles1 . The modern science of defects in semiconductors is closely tied to the invention of the transistor at Bell Laboratories in 1948 (by Bardeen, Shockley and Brattain [3], Physics Nobel laureates for 1956). Early developments took place mainly in the United States, in particular at Bell Laboratories, the Lincoln Lab (MIT) and Purdue University. Karl Lark-Horovitz, an Austrian immigrant, started at Purdue a program to investigate the growth and doping (n- and p-type) of germanium and all sorts of electrical and optical properties of this element in crystalline form [4]. The initial motivation was the development of germanium detectors for radar applications. During the years 1928 till his untimely death in 1958 he built up the Physics Department at Purdue into the foremost center of academic semiconductor research. Work similar to that at Purdue for germanium was carried out at Bell Labs, also as a spinoﬀ of the development of silicon rectiﬁers during World War II. At Bell, Scaﬀ et al. [5] discovered that crystalline silicon could be made n- or p-type by doping with atoms of the ﬁfth (P, As, Sb) or the third (B, Al, Ga, In) column of the periodic table, respectively. n-type dopants were called donors, p-type ones acceptors. Pearson and Bardeen performed a rather extensive investigation of the electrical properties of intrinsic and doped silicon [6]. These authors proposed the simplest possible expression for estimating the binding energy of the so-called hydrogenic energy levels of those impurities: The ionization energy of the hydrogen atom (13.6 eV) had to be divided by the square of the static dielectric constant ( = 12 for silicon) and multiplied by an eﬀective mass (typical values m∗ ≈ 0.1) that simulated the presence of a crystalline potential. According to this Ansatz, all donors (acceptors) would have the same binding energy, a fact that we now know is only approximately true (see Fig. 5 of Chap. 3 for diamond). The simple hydrogenic Ansatz applies to semiconductors with isotropic extrema, so that a unique eﬀective mass can be deﬁned (e.g., n-type GaAs). It does not apply to electrons in either Ge or Si because the conduction-band extrema are strongly anisotropic. The hydrogen-like Schr¨ odinger equation can, however, be modiﬁed so as to include anisotropic masses, as apply to germanium and silicon [7]. The maximum of the valence bands of most diamond and zincblende-like semiconductors occurs at or very close to k = 0. It is fourfold degenerate in the presence of spin-orbit interaction and sixfold if such interaction is neglected [8]. The simple Schr¨ odinger equation of the hydrogen atom must be replaced by a set of four coupled equations (with spin-orbit coupling) with eﬀective-mass parameters to be empirically determined [9]. Extensive applications of Kohn’s prescriptions were performed by several Italian theorists [10]. 1

A source article is one published in a Source Journal as deﬁned by the ISIThomson Scientiﬁc. There are about 6000 such journals, including all branches of science.

4

Manuel Cardona

In the shallow (hydrogenic) level calculations based on eﬀective-mass Hamiltonians the calculated impurity eigenvalues are automatically referred to the corresponding band edges, thus obviating the need for using a marker, of the type discussed in Chap. 3 of this book. This marker was introduced in order to avoid errors inherent to the “ﬁrst-principles” calculations, such as those related to the so-called “gap problem” found when using local-density functionals to represent many-body exchange and correlation. For a way to palliate this problem using the so-called GW approximation see Chap. 7, where defects at surfaces are treated. We have discussed so far the electronic levels of shallow substitutional impurities. In this volume a number of other defects, such as vacancies, interstitial impurities, clusters, etc., will be encountered. Energy levels related to structural defects were ﬁrst discussed by Lark-Horovitz and coworkers [11]. These levels were produced by irradiation with either deuterons, alpha particles or neutrons. After irradiation, the material became more p-type. It was thus postulated that the defect levels introduced by the bombardment were acceptors (vacancies?). It was also discovered by Lark-Horovitz that neutron bombardment, followed by annealing in order to reduce structural damage, could be used to create electrically active impurities by nuclear transmutation [12]. The small amount of the 30Si isotope (≈ 4 %) present in natural Si converts, by neutron capture, into radioactive 31Si, which decays through β-emission into stable 31 P, a donor. This technique is still commercially used nowadays for producing very uniform doping concentrations. Since Kohn–Luttinger perturbation theory predicts reasonably well the electronic levels of shallow impurities (except for the so-called central-cell corrections [13]) this book covers mainly deep impurity levels that not only are diﬃcult to calculate for a given real-space structure but also require relaxation of the unperturbed host crystal around the defect. Among these deep levels, native defects such as vacancies and self-interstitials are profusely discussed. Most of these levels are related to transition-metal atoms, such as Mn, Cu, and Au (I call Au and Cu transition metals for obvious reasons). The solubility of these transition-metal impurities is usually rather low (less than 1015 cm−3 . Exceptions: Cd1 − x Mnx Te and related alloys). They can go into the host lattice either as substitutional or as interstitial atoms,2 a point that can be clariﬁed with EPR and also with ab initio total-energy calculations. These dopants were used in early applications in order to reduced the residual conductivity due to shallow levels (because of the fact that transition-metal impurities have levels close to the middle of the gap). One can even nowadays ﬁnd in the market semi-insulating GaAs obtained by doping with chromium. 2

The reader who tries to do a literature search for interstitial gold may be surprised by the existence of homonyms: Interstitial gold is important in the treatment of prostate cancer. It has, of course, nothing to do with our interstitial gold. See [14].

Foreword

5

I remember having obtained in 1957 semi-insulating germanium and silicon (doped with either Mn or Au) with carrier concentrations lower than intrinsic (this makes a good exam question!). They were used for measurements of the low-frequency dielectric constants of these materials, in particular vs. temperature and pressure [15] while I was working at Harvard on my PhD under W. Paul. Rough estimates of the positions of deep levels of many impurity elements in the gap of group IV and III–V semiconductors were obtained by Hjalmarson et al. [8, 16] using Green’s function methods. In the case of GaAs and related materials, two kinds of defect complexes, involving structural changes and metastability have received a lot of attention because of technological implications: the so-called EL2 and DX centers. Searching the Web of Science for EL2 one ﬁnds 1055 mentions in abstracts and titles of source articles. Likewise 695 mentions are found for the DX centers. Chadi and coworkers have obtained theoretical predictions for the structure of these centers and their metastability [17, 18]. Although these theoretical models explain a number of observations related to these centers, there is not yet a general consensus concerning their structures. An aspect of the defect problem that has not been dealt with explicitly in this volume is the errors introduced by using nonrelativistic Schr¨ odinger equations, in particular the neglect of mass–velocity corrections and spin– orbit interaction (the latter, however, is explicitly included in the Kohn– Luttinger Hamiltonian, either in its 4 × 4 or its 6 × 6 version). Discrepancies between calculated and measured gaps are attributed to the “gap problem” inherent in the local-density approximation (LDA). However, already for relatively heavy atoms (Ge, GaAs) the mass–velocity correction decreases the s–like conduction levels and, together with the LDA gap problem. converts the semiconductor into a metal in the case of germanium. For GaAs it is stated several times in this volume that the LDA calculated gap is about half the experimental one. This is for a nonrelativistic Hamiltonian. Even a scalar relativistic one reduces the gap even further, to about 0.2 eV (experimental gap: 1.52 eV at 4 K) [19]. This indicates that the gap problem is more serious than previously thought on the basis of nonrelativistic LDA calculations. Another relativistic eﬀect is the spin-orbit coupling. For moderately heavy atoms such as Ge, Ga and As the spin-orbit splitting at the top of the valence bands (≈ 0.3 eV) is much larger than the binding energy of hydrogenic acceptors. Hence we can calculate the binding energies of the latter by solving the decoupled 4 × 4 (J = 3/2) and 2 × 2 (J = 1/2) eﬀective-mass equations. This leads to two series of acceptor levels separated by a “spin-orbit” splitting basically equal to that of the band-edge states. In the case of silicon, however, the spin-orbit splitting at k = 0 (∆ = 0.044 eV) is of the order of shallowimpurity binding energies. The impurity potential thus couples the J = 3/2 and J = 1/2 bands and the apparent spin-orbit splitting of the corresponding impurity series becomes smaller than that at the band edges [20, 21]. The diﬀerence between band-edge spin-orbit splitting (∆ = 0.014 eV) and that of

6

Manuel Cardona

the acceptor levels becomes even larger in diamond. Using a simple Green’s functions technique and a Slater–Koster δ-function potential, the impuritylevel splittings have been calculated and found to be indeed much smaller than ∆ = 0.014 eV. This splitting depends strongly on the binding energy of the impurity. Another aspect that has hardly been treated in the present volume (see, however, Chap. 10 for amorphous silicon) is the temperature dependence of the electronic energy levels that is induced by the electron–phonon interaction. Whenever this question appears in this volume, it is assumed that we are in the classical high-temperature limit, in which the corresponding renormalization of electronic gaps and states is proportional to temperature. At low temperatures, the electron–phonon interaction induces a zero-point renormalization of the electronic states that can be estimated from the measured temperature dependence. It is also possible to determine the zero-point renormalization of gaps by measuring samples with diﬀerent isotopic compositions. The interested reader should consult the review by Cardona and Thewalt [22]. When an atom of the host lattice of a semiconductor has several stable isotopes (e.g., diamond, Si, Ge, Ga, Zn samples grown with natural material lose, strictly speaking, their translational symmetry. In the past 15 years a large number of semiconductors have been grown using isotopically pure elements (which have become available in macroscopic and aﬀordable quantities after the fall of the Iron Curtain). A diﬀerent isotope added to an isotopically pure sample can thus be considered as an impurity, probably the simplest kind of defect possible: Only the atomic mass of such an impurity diﬀers from that of the host, the electronic properties remain nearly the same.3 The main effect of isotope mass substitution is found in the vibrational frequencies of host as well as local vibrational modes: such frequencies are inversely proportional to the square root of the vibrating mass (see Chap. 4). Although this eﬀect sounds rather trivial it often induces changes in phonon widths and in the zero-point anharmonic renormalizations (see [22]) that in some cases can be rather drastic and unexpected [23]. The structural relaxation around isotopic impurities is rather small. The main such eﬀect corresponds to an increase of the lattice constant with increasing isotopic mass, about 0.015 % between 12C and 13C diamond. Its origin lies in the change in the zero-point renormalization of the lattice constant: ab initio calculations are available [24]. The third class of eﬀects of the isotopic impurities refers to electronic states and energy gaps and their renormalization on account of the electron– phonon interaction. The zero-point renormalizations also vary as the inverse square root of the relevant isotopic mass. By measuring a gap energy at low temperatures for samples with two diﬀerent isotopic masses, one can 3

Except for the electron–phonon renormalization of the electronic states and gaps that is usually rather small. See [22].

Foreword

7

extrapolate to inﬁnite mass and thus determine the unrenormalized value of the gap. Renormalizations of around 60 meV have been found for Ge and Si. For diamond, however, this renormalization seems to be much larger [25], around 400 meV.4 This large renormalization is a signature of strong electron– phonon interaction that seems to be responsible for the superconductivity recently observed in heavily boron doped (p-type) diamond (Tc higher than 10 K) [26,27]. Ab initio calculations of the electronic and vibronic structure of heavily boron doped diamond have been performed and used for estimating the critical temperature Tc [28].

2 Bibliometric Studies In the previous section I have already discussed the number of times certain topics appear in titles, keywords and abstracts in source journals (about 6000 publications chosen by the ISI among ≈ 100 000, as those that contribute signiﬁcantly to the progress of science). While titles go back to the present starting date of the source journal selection (the year 1900), abstracts and keywords have only been collected since 1990. In the Web of Science (WoS) one can completely eliminate the latter in order to avoid distortions but, for simplicity, I kept them in the qualitative survey presented here. In this section, a more detailed bibliometric analysis will be performed using the WoS that draws on the citation index as the primary database. In order to get a feeling for the standing of the various contributors to this volume, we could simply perform a citations count (it can be done relatively easily within the WoS using the cited reference mode). However, a more taletelling index has been recently suggested by Hirsch [29], the so-called h-index. This index is easily obtained for anyone with access to the WoS going back to the ﬁrst publication of the authors under scrutiny (1974 for Nieminen and Shaw). How far back your access to the WoS goes depends on how much your institution is willing to pay to ISI-Thomson Scientiﬁc. The h-index is obtained by using the general search mode of the WoS and ordering the results of the search for a given individual according to the number of citations (there is a function key to order the author’s contributions from most cited to less cited). You then go down the list till the order number of a paper equals its number of citations (you may have to take one more or less citation if equality does not exist). The number so obtained is the h-index. It rewards more continued, sustained well-cited publications rather than only a couple with a colossal number (such as those that deserve the Nobel Prize). Watch out for possible homonyms although, on the average, they appear seldom. They can be purged by hand if the number of terms is not too high. I had problems with homonyms only for ﬁve out of the 24 (excluding myself) contributors 4

Theorists: beware (and be aware) of this large renormalization when comparing your fancy GW calculations of gaps with experimental data.

8

Manuel Cardona

to this volume (Antonelli, Colombo, Hern´ andez, Sanati and Shaw). I simply excluded them from the count. The average h-factor of the remaining 19 authors is h = 20. Hirsch mentions in [29] that recently elected fellows of the American Physical Society have typically h ≈ 15–20. Advancement of a physicist to full professor at a reputable US university corresponds to h ≥ 18. The high average h already reveals the high standing of the authors of this book. In several cases, the authors involve a senior partner (h ≥ 20, Chaps. 3, 4, 5, 7, 8, 10 and 11) and a junior colleague. I welcome this decision. It is a good procedure for introducing junior researchers to the intricacies and ordeals involved in writing a review article of such extent. In this connection, I should mention that the h-index is roughly proportional to the scientiﬁc age (counted from the ﬁrst publication or the date of the PhD thesis). The values of h given above for faculty and NAS membership are appropriate to physicists and chemists. Biomedical scientists often have, everything else being equal, twice as large h-indices, whereas engineers and mathematicians (especially the latter) have much lower ones. After having discussed the average h-index of our contributors, I would like to mention the range they cover without mentioning speciﬁc names.5 The h-indices of our contributors cover the range 6 ≤ h ≤ 64. Four very junior authors who have not yet had a chance of being cited have been omitted (one could have set h = 0 in their case). Hirsch mentions in his seminal article [29] that election to the National Academy of Sciences of the US is usually associated with h = 45. We therefore must have some potential academicians among our contributors. Because of the ease in the use of the h-algorithm just described and its usefulness to evaluate the “impact” of a scientist’s career, bibliometrists have been looking for other applications of the technique. Instead of people one can apply it to journals (provided they are not too large in terms of published articles), institutions, countries, etc. One has to keep in mind that the resulting h-number always reverts to an analysis of the citations of individuals that are attached to the investigated items (e.g., countries, institutions, etc.). One can also use the algorithm to survey the importance of keywords or title subjects. The present volume has 11 chapters and this gives it a certain (albeit small) statistical value to be of use in such a survey. We thus attach to each chapter title a couple of keywords and evaluate the corresponding h-index entering these under “topic” in the general search mode of the WoS. In the table below we list these words, the number of items we ﬁnd for each set of them and the corresponding h-index. There is considerable arbitrariness in the procedure to choose the keywords but we must keep in mind that these applications are just exploratory and at their very beginning. 5

Mentioning the h-indices of the authors, one by one, may be invidious. The interested reader with access to the WoS can do it by following the prescription given above.

Foreword

9

We display in Table 1 the keywords we have assigned to the eleven chapters, the number of terms citing them and the corresponding h-index that weights them according to the number of times each citing term is cited. One can draw a number of conclusions from this table. Particularly interesting are the low values of n and h for empirical molecular dynamics, which probably signals the turn towards ab initio techniques. Amorphous semiconductors, including defect and the metastabilities induced by illumination plus possibly their applications to photovoltaics are responsible for the large values of n and h. Table 1. Keywords assigned (somewhat arbitrarily) to each of the 11 chapters in the book together with the corresponding number n of source articles citing them in abstract, keywords or title. Also, Hirsch number h that can be assigned to each of the chapters according to the keywords Chapter Keyword (topic in WoS) 1 2 3 4 5 6 7 8 9 10 11

defects and semiconductors supercell calculations Gaussian orbitals dynamical matrix free energy and defect quantum Monte Carlo point defect and surface defect and molecular dynamics empirical molecular dynamics defect and amorphous light and amorphous

n

h

3735 165 190 231 494 2551 426 2023 23 4492 5747

76 27 27 26 36 71 38 67 7 77 87

References [1] G. E. Moore: Electronics 38, 114 (1965) 1 [2] R. Sherwin, R. J. H. Clark, R. Lauck, M. Cardona: Solid State Commun. 134, 265 (2005) 2 [3] J. Bardeen, W. Brattain: Phys. Rev. 74, 230 (1948) 3 [4] K. Lark-Horovitz, V. A. Johnson: Phys. Rev. 69, 258 (1946) 3 [5] J. A. Scaﬀ, H. C. Theuerer, E. E. Schumacher: J. Metals: Trans. Am. Inst. Mining Metall. Eng. 185, 383 (1949) 3 [6] G. L. Pearson, J. Bardeen: Phys. Rev. 75, 865 (1949) 3 [7] W. Kohn, J. M. Luttinger: Phys. Rev. 97, 1721 (1975) 3 [8] P. Y. Yu, M. Cardona: Fundamentals of Semiconductors, vol. 3 (Springer, Berlin, Heidelberg 2005) 3, 5 [9] W. Kohn, D. Schechter: Phys. Rev. 99, 1903 (1955) 3 [10] A. Baldereschi, N. Lipari: Phys. Rev. B 9, 1525 (1974) 3 [11] W. E. Johnson, K. Lark-Horovitz: Phys. Rev. 76, 442 (1949) 4

10

Manuel Cardona

[12] K. Lark-Horovitz: Nucleon-bombarded semiconductors, in Semiconducting Materials (Butterworths, London 1950) p. 47 4 [13] W. Kohn: Solid State Physics, vol. 5 (Academic, New York 1957) 4 [14] Lannon, et al.: Br. J. Urol. 72, 782 (1993) 4 [15] M. Cardona, W. Paul, H. Brooks: J. Phys. Chem. Solids 8, 204 (1959) 5 [16] H. P. Hjalmarson, P. Vogl, D. J. Wolford, J. D. Dow: Phys. Rev. Lett. 44, 810 (1980) 5 [17] D. J. Chadi, K. J. Chang: Phys. Rev. Lett. 60, 2187 (1988) 5 [18] S. B. Chang, D. J. Chadi: Phys. Rev. B 42, 7174 (1990) 5 [19] M. Cardona, N. E. Christensen, G. Fasol: Phys. Rev. B 38, 1806 (1988) 5 [20] N. O. Lipari: Solid State Commun. 25, 266 (1978) 5 [21] J. Serrano, A. Wysmolek, T. Ruf, M. Cardona: Physica B 274, 640 (1999) 5 [22] M. Cardona, M. L. V. Thewalt: Rev. Mod. Phys. 77, 1173 (2005) 6, 10 [23] J. Serrano, F. J. Manj´ on, A. H. Romero, F. Widulle, R. Lauck, M. Cardona: Phys. Rev. Lett. 90, 055510 (2003) 6 [24] P. Pavone, S. Baroni: Solid State Commun. 90, 295 (1994) 6 [25] M. Cardona: Science and technology of advanced materials, in press. See also [22] 7 [26] E. A. Ekimov, V. A. Sidorov, E. D. Bauer, N. N. Mel’nik, N. J. Curro, J. D. Thompson, S. M. Stishov: Nature 428, 542 (2004) 7 [27] Y. Takano, M. Nagao, I. Sakaguchi, M. Tachiki, T. Hatano, K. Kobayashi, H. Umezawa, H. Kawarada: Appl. Phys. Lett. 85, 2851 (2004) 7 [28] L. Boeri, J. Kortus, O. K. Andersen: Phys. Rev. Lett. 93, 237002 (2004) 7 [29] J. E. Hirsch: Proc. Nat. Acad. Sci. (USA) 102, 16569 (2005) 7, 8

Index amorphous, 1, 2, 6, 9 Brillouin zone, 2

Ge, 5–7 Green’s function, 5, 6 GW, 4, 7

cluster, 2

Hamiltonian, 4, 5

dopant, 3, 4 DX, 5

isotope, 4, 6 LDA, 5

eﬀective mass, 3–5 EL2, 5 electron–phonon, 6, 7 EPR, 4 GaAs, 3–5

phonon, 6 Si, 6, 7 Slater, 6 spin-orbit, 3, 5

Defect Theory: An Armchair History David A. Drabold and Stefan K. Estreicher 1

2

Dept. of Physics and Astronomy, Ohio University, Athens, OH 45701 [email protected] Physics Department, Texas Tech University, Lubbock, TX 79409-1051 [email protected]

Abstract. This introductory chapter begins with a summary of the developments of the theory of defects in semiconductors in the past 50 years. This is followed by an overview of single-particle methods and today’s ﬁrst-principles approach, rooted in density-functional theory. Much more detail about this theory and the approximations it involves is found in subsequent chapters. The last section discusses the various contributions to this book.

1 Introduction The voluntary or accidental manipulation of the properties of materials by including defects has been performed for thousands of years. The most ancient example we can think of is well over 5000 years old. It happened when someone realized that adding trace amounts of tin to copper lowers the melting temperature, increases the viscosity of the melt, and results in a metal considerably harder than pure copper: bronze. This allowed the manufacture of a variety of tools, shields and weapons. Not long afterwards, the early metallurgists realized that sand mixed with a metal is relatively easy to melt and produces glass. The Ancient Egyptians discovered that glass beads of various brilliant colors can be obtained by adding trace amounts of speciﬁc transition metals, such as gold for red or cobalt for blue [1]. Defect engineering is not something new. However, materials whose mechanical, electrical, optical, and magnetic properties are almost entirely controlled by defects are relatively new: semiconductors [2, 3]. Although the ﬁrst publication describing the rectifying behavior of a contact dates back to 1874 [4], the systematic study of semiconductors began only during World War II. The ﬁrst task was to grow high-quality Ge (then Si) crystals, that is removing as many defects as possible. The second task was to manipulate the conductivity of the material by adding selected impurities that control the type and concentration of charge carriers. This involved theory to understand as quantitatively as possible the physics involved. Thus, theory has played a key role since the very beginning of this ﬁeld. These early developments have been the subject of several excellent reviews [5–8]. For a long time, theory has been trailing the experimental work. Approximations at all levels were too drastic to allow quantitative predictions. D. A. Drabold, S. K. Estreicher (Eds.): Theory of Defects in Semiconductors, Topics Appl. Physics 104, 11–28 (2007) © Springer-Verlag Berlin Heidelberg 2007

12

David A. Drabold and Stefan K. Estreicher

Indeed, modeling a perfect solid is relatively easy since the system is periodic. High-level calculations can be done in the primitive unit cell. This periodicity is lost when a defect is present. The perturbation to the defect-free material is often large, in particular when some of the energy eigenvalues of the defect are in the forbidden gap, far from band edges. However, in the past decade or so, theory has become quantitative in many respects. Today, theorists often predict geometrical conﬁgurations, binding, formation, and various activation energies, charge and spin densities, vibrational spectra, electrical properties, and other observable quantities with suﬃcient accuracy to be useful to experimentalists and sometimes device scientists. Furthermore, the theoretical tools developed to study defects in semiconductors can be easily extended to other areas of materials theory, including many ﬁelds of nanoscience. It is the need to understand the properties of defects in semiconductors, in particular silicon, that has allowed theory to develop as much as it has. One key reason for this was the availability of microscopic experimental data, ranging from electron paramagnetic resonance (EPR) to vibrational spectroscopy, photoluminescence (PL), or electrical data, all of which provided critical tests for theory at every step. The word “defect” means a native defect (vacancy, self-interstitial, antisite, . . . ), an impurity (atom of a diﬀerent kind from the host atoms), or any combination of those isolated defects: small clusters, aggregates, or even larger defect structures such as precipitates, interfaces, grain boundaries, surfaces, etc. However, nanometer-size defects play many important roles and are the building blocks of larger defect structures. Therefore, understanding the properties of defects begins at the atomic scale. There are many examples of the beneﬁcial or detrimental roles of defects. Oxygen and nitrogen pin dislocations in Si and allow wafers to undergo a range of processing steps without breaking [9]. Small oxygen precipitates provide internal gettering sites for transition metals, but some oxygen clusters are unwanted donors that must be annealed out [10]. Shallow dopants are often implanted. They contribute electrons to the conduction band or holes to the valence band. Native defects, such as vacancies or self-interstitials, promote or prevent the diﬀusion of selected impurities, in particular dopants. Selfinterstitial precipitates may release self-interstitials that in turn promote the transient enhanced diﬀusion of dopants [11]. Transition-metal impurities are often associated with electron–hole recombination centers. Hydrogen [12], almost always present at various stage of device processing, passivates the electrical activity of dopants and of many deep-level defects, or forms extended defect structures known as platelets. Mg-doped GaN must be annealed at rather high temperatures to break up the {Mg, H} complexes that prevent ptype doping [13]. Magnetic impurities such as Mn can render a semiconductor ferromagnetic. The list goes on. Much of the microscopic information about defects comes from electrical, optical, and/or magnetic experimental probes. The electrical data are often obtained from capacitance techniques such as deep-level transient spec-

Defect Theory: An Armchair History

13

troscopy (DLTS). The sensitivity of DLTS is very high and the presence of defects in concentrations as low as 1011 cm−3 can be detected. However, even in conjunction with uniaxial stress experiments, these data provide little or no elemental and structural information and, by themselves, are insuﬃcient to identify the defect responsible for electrical activity. Local vibrational mode (LVM) spectroscopy, Raman, and Fourier transform infrared absorption (FTIR), often give sharp lines characteristic of the Raman- or IR-active LVMs of impurities lighter than the host atoms. When uniaxial stress, annealing, and isotope substitution studies are performed, the experimental data provide a wealth of critical information about a defect. This information can be correlated, e.g., with DLTS annealing data. However, Raman and FTIR are not as sensitive as DLTS. In the case of Raman, over 1017 cm−1 defect centers must be present in the surface layer exposed to the laser. In the case of FTIR, some 1016 cm−3 defect centers are needed, although much higher sensitivities have been obtained from multiple-internal reﬂection FTIR [14]. Photoluminescence is much more sensitive, sometimes down to 1011 cm−1 , but the spectra can be more complicated to interpret [15]. Finally, magnetic probes such as EPR are wonderfully detailed and a lot of defect-speciﬁc data can be extracted: identiﬁcation of the element(s) involved in the defect and its immediate surrounding, symmetry, spin density maps, etc. However, the sensitivity of EPR is rather low, of the order of 1016 cm−3 . Further, localized gap levels in semiconductors often prefer to be empty or doubly occupied as most defect centers in semiconductors are unstable in a spin- 21 state. The sample must be illuminated in order to create an EPR-active version of the defect under study [16–18]. This introductory Chapter contains brief reviews of the evolution of theory [19, 20] since its early days and of the key ingredients of today’s state-ofthe-art theory. It concludes with an overview of the content of this book.

2 The Evolution of Theory The ﬁrst device-related problem that required understanding was the creation of electrons or holes by dopants. These (mostly substitutional) impurities are a small perturbation to the perfect crystal and are well described by eﬀective mass theory (EMT) [21]. The Schr¨ odinger equation for the nearly-free charge carrier, trapped very close to a parabolic band edge, is written in hydrogenic form with an eﬀective mass determined by the curvature of the band. The calculated binding energy of the charge carrier is that of a hydrogen atom but reduced by the square of the dielectric constant. As a result, the associated wavefunction is substantially delocalized, with an eﬀective Bohr radius some 100 times larger than that of the free hydrogen atom. EMT has been reﬁned in a variety of ways [22] and provided a basic understanding of doping. However, it cannot be extended to defects that have energy eigenvalues far from band edges. These so-called “deep-level” defects

14

David A. Drabold and Stefan K. Estreicher

are not weak perturbations to the crystal and often involve substantial relaxations and distortions. The ﬁrst such defects to be studied were the byproducts of radiation damage, a hot issue in the early days of the cold war. EPR data became available for the vacancy [16, 23] and the divacancy [24], in silicon (the Si self-interstitial has never been detected). Transition-metal (TM) impurities, which are common impurities and active recombination centers, have also been studied by EPR [25]. In most charge states, the undistorted vacancy (Td symmetry) or divacancy (D3d symmetry) is an orbital triplet or doublet, respectively, and therefore should undergo Jahn–Teller distortions. The EPR studies showed that this is indeed the case. Although interstitial oxygen, the most common impurity in Czochralski-grown Si, was known to be at a puckered bond-centered site [26, 27], it was not realized how much energy is involved in relaxations and distortions. It was believed that the chemistry of defects in semiconductors is well described in ﬁrst order by assuming high-symmetry, undistorted, lattice sites. Relaxations and distortions were believed to be a second-order correction. The important issue then was to correctly predict trends in the spin densities and electrical activities of speciﬁc defects centers in order to explain the EPR and electrical data (see, e.g., [28, 29]). The critical importance of carefully optimizing the geometry around defects and the magnitudes of the relaxation energies were not fully realized until the 1980s [30, 31]. The host-atom displacements can be of several tenths of an ˚ A, and the chemical rebonding can lead to energy changes as large as several eV (undistorted vs. relaxed structures). The ﬁrst theoretical tool used to describe localized defects in semiconductors involved Green’s functions [2, 19, 32, 33]. These calculations begin with the Hamiltonian H0 of the perfect crystal. Its eigenvalues give the crystal’s band structure and the eigenfunctions are Bloch or Wannier functions. In principle, the defect-free host crystal is perfectly described. The localized defect is represented by a Hamiltonian H that includes the defect potential V . The Green’s function is G(E) = 1/(E − H ). Therefore, the perturbed energies E coincide with its poles. The new eigenvalues include the gap levels of the defect and the corresponding eigenfunctions are the defect wavefunctions. In principle, Green’s functions provide an ideal description of the defect in its crystalline environment. In practice, there are many diﬃculties associated with the Hamiltonian, the construction of perfect-crystal eigenfunctions that can be used as a basis set for the defect calculation [34, 35], and the construction of the defect potential itself. This is especially true for those defects that induce large lattice relaxations and/or distortions. The ﬁrst successful Green’s functions calculations for semiconductors date back to the late 1970s [36–38]. They were used to study charged defects [39], calculate forces [40–42], total energies [43, 44], and LVMs [45, 46]. These calculations also provided important clues about the role of native defects in impurity diﬀusion [47]. However, while Green’s functions do provide a nearideal description of the defect in a crystal, their implementation is diﬃcult

Defect Theory: An Armchair History

15

and not very intuitive. Clusters or supercells are much easier to use and provide a physically and chemically appealing description of the defect and its immediate surroundings. Green’s functions have mostly been abandoned since the mid-1980s, but a rebirth within the GW formalism [48] is now taking place (see the Chapter by Schindlmayr and Scheﬄer ). In order to describe the distortions around a vacancy, Friedel et al. [49] completely ignored the host crystal and limited their description to rigid linear combinations of atomic orbitals (LCAO). Messmer and Watkins [50,51] expanded this approach to linear combinations of dangling-bond states. These simple quantum-chemical descriptions provided a much-needed insight and a correct, albeit qualitative, explanation of the EPR data. Here, the defect was assumed to be so localized that the entire crystal could be ignored in zeroth order. The natural extension of this work was to include a few host atoms around the defect, thus deﬁning a cluster . These types of calculations were performed in real space with basis sets consisting of localized functions such as Gaussians or LCAOs. The dangling bonds on the surface atoms must be tied up in some way, most often with H atoms. However, without the underlying crystal and its periodicity, the band structure is missing and the defect’s energy eigenvalues cannot be placed within a gap. Further, the ﬁnite size of the cluster artiﬁcially conﬁnes the wavefunctions. This aﬀects charged defects the most, as the charge tends to distribute itself on the surface of the cluster. However, the local covalent interactions are well described. The Schr¨ odinger equation for a cluster containing a defect can be solved using almost any electronic-structure method. The early work was empirical or semiempirical, with heavily approximated quantum-chemical methods. At ﬁrst, extended H¨ uckel theory [52, 53] was used then self-consistent semiempirical Hartree–Fock: CNDO [54], MNDO [55], MINDO [56]. Geometries could be optimized, albeit often with symmetry assumptions. The methods suﬀered from a variety of problems such as cluster size and surface eﬀects, basis-set limitations, lack of electron correlation, and the use of adjustable parameters. Their values are normally ﬁtted to atomic or molecular data, and transferability is a big issue. In order to bypass the surface problem, cyclic clusters have been designed, mostly in conjunction with semiempirical Hartree–Fock. Cyclic clusters can be viewed as clusters to which Born–von-Karman periodic boundary conditions are applied [57, 58]. These boundary conditions can be diﬃcult to handle, in particular when 3- and 4-center interactions are included [59]. DeLeo and coworkers [60, 61] extensively used the scattering-Xα method in clusters to study trends for interstitial TM impurities and hydrogen–alkalimetal complexes. The results provided qualitative insight into these issues. Ultimately, the method proved diﬃcult to bring to self-consistency and the rather arbitrarily deﬁned muﬃn-tin spheres rendered it poorly suited to the calculation of total energies vs. atomic positions.

16

David A. Drabold and Stefan K. Estreicher

The method of partial retention of diatomic diﬀerential overlap [62, 63] (PRDDO) was ﬁrst used for defects in diamond and silicon in the mid-1980s. It is self-consistent, contains no semiempirical parameters, and allows geometry optimizations to be performed without symmetry assumptions. Convergence is very eﬃcient and relatively large clusters (44 host atoms) could be used. However, PRDDO is a minimal basis-set technique and ignores electron correlation. Its earliest success was to demonstrate [30, 31] the stability of bond-centered hydrogen in diamond and silicon. It was not expected at all that an impurity as light as H could indeed force a Si–Si bond to stretch by over 1 ˚ A. Substantial progress in the theory of defects in semiconductors occurred in the mid-1980s with the combination of periodic supercells to represent the host crystal, ab-initio-type pseudopotentials [64–66] for the core regions, DF theory for the valence regions, and ab-initio molecular dynamics (MD) simulations [67, 68] for nuclear motion. This combination is now referred to as “ﬁrst-principles” as opposed to “semiempirical”. There are parameters in the theory. They include the size of the supercell, k-point sampling, type and size of the basis set, chosen by the user, as well as the parameters associated with the basis sets and pseudopotentials. However, these parameters and user inputs are not ﬁtted to an experimental database. Instead, some are determined self-consistently, other are calculated from ﬁrst principles or obtained from high-level atomic calculations. Note that the ﬁrst supercell calculations were done in the 1970s in conjunction with approximate electronic-structure methods [69–71]. PRDDO was used to study cluster size and surface eﬀects [72] and many defects (see, e.g., [73, 74]). It provided good input geometries for single-point ab-initio Hartree–Fock calculations (see, e.g., [75]). However, it suﬀered from the problems associated with all Hartree–Fock techniques, such as unreasonably large gaps and inaccurate LVMs. A number of research groups have used Hartree–Fock and post-Hartree–Fock techniques [76–78] to study defects in clusters, but these eﬀorts have now been mostly abandoned. Density-functional (DF) theory [79–82] with local basis sets (see, e.g., [83]) in large clusters allowed more quantitative predictions. The DF-based AIMPRO code [84, 85] uses Gaussian basis sets and has been applied to many defect problems (this code handles periodic supercells as well). In addition to geometries and energetics, rather accurate LVMs for light impurities can be predicted [86, 87]. Large clusters have been used [88, 89] to study the distortions around a vacancy or divacancy in Si. However, all clusters suﬀer from the surface problem and lack of periodicity.

3 A Sketch of First-Principles Theory The theoretical approach known as “ﬁrst principles” has proven to be a revolutionary tool to predict quantitatively some key properties of defects. An elementary exposition of the theory follows.

Defect Theory: An Armchair History

17

3.1 Single-Particle Methods: History After the Born–Oppenheimer approximation is made, so that electronic and ionic degrees of freedom are separated, we face the time-independent manyelectron problem [82]: −2 /2m ∇2j − Zl e2 /|rj − Rl | + 1/2 e2 /|r j − r j | − E Ψ = 0 . j

j,l

j=j

(1) Here, rj are electron coordinates, Rl and Zl are positions and atomic numbers of the nuclei and E is the energy. It is worth reﬂecting on the remarkable simplicity of this equation: it is exact (nonrelativistically), and the meaning of each term is entirely transparent. In one of the celebrated legends of science, P. A. M. Dirac is said to have implied that chemistry was just an application of (1), though he also acknowledged that the equation was intractable. It is true that the quantum mechanics of the many-electron problem is beautifully and succinctly represented in (1). Kohn gives an interesting argument [82] stating that even in principle, (1) is hopeless as a practical tool for calculation if the number of electrons exceeds 103 or so. His argument is a development of a paper of Van Vleck [90]1 and points out that it appears to be fundamentally impossible to obtain an approximate many-electron function Ψ with signiﬁcant overlap with the “true” many-body wavefunction for large systems. He further points out that the sheer dimensionality of the problem rapidly makes it unrepresentable on any conceivable computer. Thus, a credible case can be made that for large systems it does not even make sense to estimate Ψ directly. Kohn has named this the “exponential wall”. To some extent this is disconcerting, because of the simplicity of the form of (1), but it points to the need for new concepts if we are to make sense of solids – to say nothing of defects! Empirical experience with solids also suggests that the unfathomable complexity of the many-body wavefunction is unnecessary. If all of the information contained in Ψ was really required for estimating the properties of solids that we care about, e.g., experimental observables, molecular physics would reach exhaustion with tiny molecules, and solid-state physics would never get oﬀ the ground at all. The fact is that many characteristics of materials are independent of system size. For example, in a macroscopic sample, the electronic density of states has the same form for a system with N atoms and an identically prepared one with 2N atoms. Yet Ψ is immeasurably more complex for the second system than the ﬁrst. Thus, the additional complexity 1

In this prescient paper on Heisenberg’s theory of ferromagnetism, Van Vleck introduces what later was called the “Van Vleck Catastrophe”, and emphasizes the fundamentally nonlocal character of quantum mechanics as expressed in (1), the associated factorial growth in complexity, and its dire implications for attempts to compute many-particle states for large systems.

18

David A. Drabold and Stefan K. Estreicher

of the 2N system ψ must be completely irrelevant to our observable, in this case the density of states. The saturation of complexity of the preceding paragraph is connected to Kohn’s “principle of nearsightedness” [91], which states that in fact quantum mechanics in the solid state is intrinsically local (how local depends sensitively on the system [92, 93]). The natural gauge of this locality is the decay ρ|x : of the density operator in the position representation: ρ(x, x ) = x|ˆ a function of |x − x |, decaying as a power law in metals and exponentially in systems with a gap. For systems with a gap, the exponential fall oﬀ enables accurate calculations of all local properties by undertaking a calculation in a ﬁnite volume determined by the rate of decay. The decay in semiconductors and insulators can be exploited to produce eﬃcient order-N methods for computing total energies and forces, with computational cost scaling linearly with the number of atoms or electrons [94]. 3.2 Direct Approaches to the Many-Electron Problem While this book emphasizes single-particle methods, there is one important exception. Needs shows in his Chapter in this volume that remarkable progress can be made for the computation of expectation values of observables using quantum Monte Carlo methods, with no essential approximations to (1). This is a promising class of methods that oﬀers the most accurate calculations available today for complex systems. Several groups are advancing these methods, and even the stochastic calculation of forces is becoming possible. One can be certain that quantum Monte Carlo will play an important role in systems needing the most accurate calculations available, and certainly this is the case for the theory of defects. 3.3 Hartree and Hartree–Fock Approximations In 1928, Hartree [95] started with (1) with a view to extracting useful singleparticle equations from it. He used the variational principle for the groundstate wavefunction adopting a simple product trial function: Ψ (x1 , x2 , . . . , xn ) = ψ1 (x1 )ψ2 (x2 ) . . . ψn (xn ). The product ansatz did not enforce Fermion antisymmetry requirements; this was built in with a Slater determinant ansatz as proposed by Fock in 1930 [96]: the Hartree–Fock method. These methods map the many-body ground-state problem onto a set of challenging single-particle equations. The structure of the Hartree equations is a Schr¨ odinger equation with a potential depending upon all the orbitals: −2 /2m∇2 ψl + Veﬀ ψl = εl ψl ,

(2)

where the eﬀective potential Veﬀ (r) = j= d3 r ψj∗ (r )ψ (r )/|r − r |, and the sum is over occupied states. This appealing equation prescribes an eﬀective Coulomb ﬁeld for electron l arising from all of the other electrons. Since

Defect Theory: An Armchair History

19

computing the potential requires knowledge of the other wavefunctions, the equation must be solved self-consistently with a scheme of iteration. While the equation is intuitive, it is highly approximate. Curiously, it will turn out that the equations of density-functional theory have the mathematical structure of (2), but with quite a diﬀerent (and far more predictive) Veﬀ (see (7) below), derived from a very diﬀerent point of view. The Hartree–Fock approximation includes that part of the exchange energy implied by the exclusion principle and has well-known analytic problems at the Fermi surface in metals [94] and a tendency to exaggerate charge ﬂuctuations at atomic sites in molecules or solids [97]. In molecular calculations, the correlation energy (roughly speaking, what is missing from Hartree–Fock) can be estimated in perturbation theory. This is computationally expensive: the most popular fourth-order perturbation theory (MP4) scales as n3 N 4 , where n is the number of electrons and N the number of orbitals (basis set size). Such methods are important for molecular systems, but challenging to apply to condensed systems. 3.4 Density-Functional Theory 3.4.1 Thomas–Fermi Model Not long after the dawn of quantum mechanics, Thomas and Fermi [98, 99] suggested a key role for the electron-density distribution as the determiner of the total energy of an inhomogeneous electron gas. This was the ﬁrst serious attempt to express the energy as a functional of the electron density ρ: E[ρ] =

3

2

d rV (r)ρ(r) + e /2

d3 r d3 r ρ(r)ρ(r )/|r − r | + α/m 3 × d rρ5/3 (r) . (3)

Here, α is a numerical constant, m and e are the electron mass and charge respectively, and V is an external potential. The ﬁrst two terms are evidently obtained from classical electrostatics. Quantum mechanics appears only in the third term, derived from the kinetic energy of a homogeneous electron gas. Already this equation is making a “local-density approximation”, forming an estimate for the inhomogeneous electron kinetic energy from the result from a homogeneous gas; an approximation that is expected to succeed if |∇ρ|/ρ is suﬃciently small. Variation of (3) with respect to ρ with ﬁxed electron number leads to the coupled self-consistent Thomas–Fermi equations (see, e.g., the treatment by Fulde [97]). The coarse treatment of the kinetic energy greatly limits the predictive power of the method – for example, the shell structure of atoms is not predicted [100]. However, the Thomas–Fermi model is conceptually a density-functional theory.

20

David A. Drabold and Stefan K. Estreicher

3.4.2 Modern Density-Functional Theory For atomistic force calculations on solids, the overwhelming method of choice is density-functional theory, due to Kohn, Hohenberg and Sham [101, 102]. This Chapter only sketches the concepts in broad outline, as a detailed treatment focused on defect calculations is available in this book (Niemenen Chapter). For additional discussion we strongly recommend the books of Martin (see [94]) and Fulde [97]. The following statements embody the foundation of zero-temperature density-functional theory: 1. The ground-state energy of a many-electron system is a functional of the electron density ρ(x): 3 E[ρ] = d xV (x)ρ(x) + F [ρ] , (4) where V is an external potential (due, for example, to interaction with ions, external ﬁelds, e.g., not with electrons), and F [ρ] is a universal functional of the density. The trouble is that F [ρ] is not exactly known, though there is continuing work to determine it. The practical utility of this result derives from: 2. The functional E[ρ] is minimized by the true ground-state electron density. It remains to estimate the functional F [ρ], which in conjunction with the variational principle 2, enables real calculations. To estimate F [ρ], the usual procedure is to note that we already know some of the major contributions to F [ρ], and decompose the functional in the form: 3 3 (5) F [ρ] = e2 /2 d x d x ρ(x)ρ(x )/|x − x | + Tni (ρ) + Exc (ρ) . Here, the integral is just the electrostatic (Hartree) interaction of the electrons, Tni is the kinetic energy of a noninteracting electron gas of density ρ, and Exc (ρ) is yet another unknown functional, the exchange-correlation functional, which includes nonclassical eﬀects of the interacting electrons. Equation (5) is diﬃcult to evaluate directly in terms of ρ, because of orbitals |χi , for which the term Tni . Thus, one introduces single-electron Tni = iocc χi | − 2 /2m∇2 |χi , and ρ = iocc |χi (x)|2 is the charge density of the physically relevant interacting system. The value of this decomposition is that Exc (ρ) is smooth and reasonably slowly varying, and therefore a functional that we can successfully approximate: we have included the most diﬃcult and rapidly varying parts of F in Tni and the Hartree integral, as can be seen from essentially exact many-body calculations on the homogeneous electron gas [103]. The Hartree and noninteracting kinetic energy terms are

Defect Theory: An Armchair History

21

easy to compute if one makes the local-density approximation, that is assuming that the electron density is locally uniform. With information about the homogeneous electron gas, the functional (5) is fully speciﬁed. With noninteracting orbitals |χi , (with ρ(x) = 2 iocc |x|χi |2 ), then the minimum principle plus the constraint that χi |χj = δij can be translated into an eigenvalue problem for the |χi : {−2 ∇2 /2m + Veﬀ [ρ(x)]}|χi = εi |χi ,

(6)

where the eﬀective density-dependent (in practical calculations, orbitaldependent) potential Veﬀ is: 3 (7) Veﬀ [ρ(x)] = V (x) + e2 d x ρ(x )/|x − x | + δεxc /δρ . In this equation εxc is the parameterized exchange-correlation energy density from the homogeneous electron gas. The quantities to be considered as physical in local-density functional calculations are: the total energy (electronic or system), the ground-state electronic charge density ρ(x), and related ground-state properties like the forces. In particular, it is tempting to interpret the |χi and εi as genuine electronic eigenstates and energies, and indeed this can often be useful. Such identiﬁcations are not rigorous [94]. It is instructive to note that the starting point of density-functional theory was to depart from the use of orbitals and formulate the electronic-structure problem rigorously in terms of the electron density ρ; yet a practical implementation (which enables an accurate estimate of the electronic kinetic energy) led us immediately back to orbitals! This illustrates why it would be very worthwhile to know F (ρ), or at least the kinetic energy functional since we would then have a theory with a structure close to the Thomas–Fermi form and would therefore be able to seek one function ρ rather than the cumbersome collection of orthonormal |χi . The initiation of modern ﬁrst-principles theory and its development into a standard method with widespread application was due to Car and Parrinello [67]. They developed a powerful method for simultaneously solving the electronic problem and evolving the positions of the ions. The method is usually applied to plane-wave basis sets, though the key ideas are independent of the choice of representation. One of the early applications to defects in silicon was the diﬀusion of bond-centered hydrogen [104]. An alternative ab-initio approach to MD simulations, based on a tight-binding perspective, was proposed by Sankey and Niklewski [68]. Their basis sets consist of pseudoatomic orbitals with s, p, d, . . . symmetry. The wavefunctions are truncated beyond some radius and renormalized. The early version of this code was not self-consistent and was restricted to minimum basis sets. A more recent version [105] is self-consistent and can accommodate expanded and polarized basis sets. This is also the case for the highly ﬂexible SIESTA code [106, 107] (Spanish initiative for the electronic structure with thousands

22

David A. Drabold and Stefan K. Estreicher

of atoms). Although basis sets of local orbitals (typically, LCAOs) are highly intuitive and allow population analysis and other chemical information to be calculated, they are less complete than plane-wave basis sets. The latter can easily be checked for convergence. On the other hand, when an atom such as Si is given two sets of 3s and 3p plus a set of 3d orbitals, the basis set is suﬃcient to describe quite well virtually all the chemical interactions of this element, as the contribution of the n = 4 shell of Si is exceedingly small, except such under extreme conditions that a ground-state theory is not capable of handling anyway. Many details of the implementation of densityfunctional methods are given in the contribution of Nieminen in his Chapter in this volume. The power of these methods is that they yield parameter-free estimates for the structure of defects and even topologically disordered systems, provide accurate estimates of total energies, formation energies, vibrational states, defect dynamics, and with suitable caveats information about electronic structure, defect levels, localization, etc. There are many subtle aspects to their applications to defect physics, partly because high accuracy is often required in such studies.

4 The Contributions In his Chapter in this volume, Nieminen carefully discusses the use of periodic boundary conditions in supercell calculations, detailing both strengths and weaknesses, and other basic features of these calculations. In their Chapter, Goss and coworkers discuss the marker method to extract electronic energy levels, and include several important applications. In their Chapter, Estreicher and Sanati describe the calculation and remarkable utility of vibrational modes in systems containing defects, including novel analysis of ﬁnite-temperature properties of defects. Then, in their Chapter, Hernandez and coworkers work out a proper theory of free energies and phase diagrams for semiconductors. Needs describes in his Chapter the most rigorous attack of the book on the quantum many-body problem, as Needs explores quantum Monte Carlo methods and their promise for defects in semiconductors. Schindlmayr and Scheﬄer describe the theory and application of self-energy corrected density-functional theory, the “GW” approximation in their Chapter. Like the work of Needs, this technique has predictive power beyond DFT. Csanyi and coworkers present a multiscale modeling approach in their Chapter with applications. Scheerschmidt oﬀers a comprehensive view of molecular dynamics in his Chapter, focusing on empirical methods, though much of his Chapter is applicable to ﬁrst-principles simulation as well. In their Chapter, Drabold and Abtew discuss defects in amorphous semiconductors with a special emphasis on hydrogenated amorphous silicon. Last but not least, in their Chapter, Simdyankin and Elliott write on the theory of light-induced eﬀects

Defect Theory: An Armchair History

23

in amorphous materials, an area of great basic and practical interest, which nevertheless depends very much upon the defects present in the material.

References [1] J. L. Mass, M. T. Wypyski, R. E. Stone: Mater. Res. Soc. Bull. 26, 38 (2001) 11 [2] A. M. Stoneham: Theory of Defects in Solids (Clarendon, Oxford 1985) 11, 14 [3] H. J. Queisser, E. E. Haller: Science 281, 945 (1998) 11 [4] F. Braun: Ann. Phys. Chem. (Leipzig) 153, 556 (1874) 11 [5] A. B. Fowler: Phys. Today 46, 59 (1993) 11 [6] F. Seitz: Phys. Today 48, 22 (1995) 11 [7] M. Riordan, I. Hoddeson: Phys. Today 50, 42 (1997) 11 [8] I. M. Ross: Phys. Today 50, 34 (1997) 11 [9] F. Shimura (Ed.): Oxygen in Silicon, Semicond. Semimet. 42 (Academic, Boston 1994) 12 [10] R. Jones (Ed.): Early Stages of Oxygen Precipitation in Silicon (Kluwer, Dordrecht 1996) 12 [11] R. Scholtz, U. G¨ osele, J. Y. Y. Huh, T. Y. Tan: Appl. Phys. Lett. 72, 200 (1998) 12 [12] S. K. Estreicher: Mater. Sci. Eng. R 14, 319 (1995) 12 [13] S. J. Pearton: GaN and Related Materials (Gordon and Breach, Amsterdam 1997) p. 333 12 [14] F. Jiang, M. Stavola, A. Rohatgi, D. Kim, J. Holt, H. Atwater, J. Kalejs: Appl. Phys. Lett. 83, 931 (2003) 13 [15] G. Davies: Phys. Rep. 176, 83 (1989) 13 [16] G. D. Watkins: Deep Centers in Semiconductors (Gordon and Breach, New York 1986) p. 147 13, 14 [17] Y. V. Gorelkinskii, N. N. Nevinnyi: Physica B 170, 155 (1991) 13 [18] Y. V. Gorelkinskii, N. N. Nevinnyi: Mater. Sci. Eng. B. 36, 133 (1996) 13 [19] S. T. Pantelides (Ed.): Deep Centers in Semiconductors (Gordon and Breach, New York 1986) 13, 14 [20] S. K. Estreicher: Mater. Today 6, 26 (2003) 13 [21] W. Kohn: Solid State Phys. 5, 257 (1957) 13 [22] S. T. Pantelides: Rev. Mod. Phys. 50, 797 (1978) 13 [23] G. D. Watkins: Radiation Damage in Semiconductors (Dunod, Paris 1964) p. 97 14 [24] G. D. Watkins, J. W. Corbett: Phys. Rev. 138, A543 (1965) 14 [25] G. W. Ludwig, H. H. Woodbury: Solid State Phys. 13, 223 (1962) 14 [26] W. Kaiser, P. H. Keck, C. F. Lange: Phys. Rev. 101, 1264 (1956) 14 [27] J. W. Corbett, R. S. McDonald, G. D. Watkins: J. Phys. Chem. Solids 25, 873 (1964) 14 [28] G. G. DeLeo, G. D. Watkins, W. Beal Fowler: Phys. Rev. B 25, 4972 (1982) 14 [29] A. Zunger, U. Lindefelt: Phys. Rev. B 26, 5989 (1982) 14

24

David A. Drabold and Stefan K. Estreicher

[30] T. L. Estle, S. K. Estreicher, D. S. Marynick: Hyp. Inter. 32, 637 (1986) 14, 16 [31] T. L. Estle, S. K. Estreicher, D. S. Marynick: Phys. Rev. Lett. 58, 1547 (1987) 14, 16 [32] G. F. Koster, J. C. Slater: Phys. Rev. 95, 1167 (1954) 14 [33] J. Callaway: J. Math. Phys. 5, 783 (1964) 14 [34] J. Callaway, A. J. Hughes: Phys. Rev. 156, 860 (1967) 14 [35] J. Callaway, A. J. Hughes: Phys. Rev. 164, 1043 (1967) 14 [36] J. Bernholc, S. T. Pantelides: Phys. Rev. B 18, 1780 (1978) 14 [37] J. Bernholc, N. O. Lipari, S. T. Pantelides: Phys. Rev. Lett. 41, 895 (1978) 14 [38] G. A. Baraﬀ, M. Schl¨ uter: Phys. Rev. Lett. 41, 892 (1978) 14 [39] G. A. Baraﬀ, E. O. Kane, M. Schl¨ uter: Phys. Rev. Lett. 43, 956 (1979) 14 [40] M. Scheﬄer, J. P. Vigneron, G. B. Bachelet: Phys. Rev. Lett. 49, 1756 (1982) 14 [41] U. Lindefelt: Phys. Rev. B 28, 4510 (1983) 14 [42] U. Lindefelt, A. Zunger: Phys. Rev. B 30, 1102 (1984) 14 [43] G. A. Baraﬀ, M. Schl¨ uter: Phys. Rev. B 28, 2296 (1983) 14 [44] R. Car, P. J. Kelly, A. Oshiyama, S. T. Pantelides: Phys. Rev. Lett. 52, 1814 (1984) 14 [45] D. N. Talwar, M. Vandevyver, M. Zigone: J. Phys. C 13, 3775 (1980) 14 [46] R. M. Feenstra, R. J. Hauenstein, T. C. McGill: Phys. Rev. B 28, 5793 (1983) 14 [47] R. Car, P. J. Kelly, A. Oshiyama, S. T. Pantelides: Phys. Rev. Lett. 54, 360 (1985) 14 [48] F. Aryasetiawan, O. Gunnarsson: Rep. Prog. Phys. 61, 237 (1998) 15 [49] J. Friedel, M. Lannoo, G. Leman: Phys. Rev. 164, 1056 (1967) 15 [50] R. P. Messmer, G. D. Watkins: Phys. Rev. Lett. 25, 656 (1970) 15 [51] R. P. Messmer, G. D. Watkins: Phys. Rev. B 7, 2568 (1973) 15 [52] F. P. Larkins: J. Phys. C: Solid State Phys. 4, 3065 (1971) 15 [53] R. P. Messmer, G. D. Watkins: Proc. Reading Conf. on Radiation Damage and Defects in Semiconductors (Insitute of Physics, Bristol 1973) p. 255 15 [54] A. Mainwood: J. Phys. C: Solid State Phys. 11, 2703 (1978) 15 [55] J. W. Corbett, S. N. Sahu, T. S. Shi, L. C. Snyder: Phys. Lett. 93A, 303 (1983) 15 [56] P. De´ ak, L. C. Snyder: Radiat. Eﬀ. Def. Solids 111–112, 77 (1989) 15 [57] P. De´ ak, L. C. Snyder: Phys. Rev. B 36, 9619 (1987) 15 [58] P. De´ ak, L. C. Snyder, J. W. Corbett: Phys. Rev. B 45, 11612 (1992) 15 [59] J. Mir´ o, P. De´ ak, C. P. Ewels, R. Jones: J. Phys.: Condens. Matter 9, 9555 (1997) 15 [60] G. G. DeLeo, G. D. Watkins, W. B. Fowler: Phys. Rev. B 23, 1819 (1981) 15 [61] G. G. DeLeo, W. B. Fowler, G. D. Watkins: Phys. Rev. B 29, 1851 (1984) 15 [62] T. A. Halgren, W. N. Lipscomb: J. Chem. Phys. 58, 1569 (1973) 16 [63] D. S. Marynick, W. N. Lipscomb: Proc. Nat. Acad. Sci. (USA) 79, 1341 (1982) 16 [64] D. R. Hamann, M. Schl¨ uter, C. Chiang: Phys. Rev. Lett. 43, 1494 (1979) 16

Defect Theory: An Armchair History

25

[65] G. B. Bachelet, D. R. Hamann, M. Schl¨ uter: Phys. Rev. B 26, 4199 (1982) 16 [66] L. Kleinman, D. M. Bylander: Phys. Rev. Lett. 48, 1425 (1982) 16 [67] R. Car, M. Parrinello: Phys. Rev. Lett. 55, 2471 (1985) 16, 21 [68] O. Sankey, D. J. Niklewski: Phys. Rev. B 40, 3979 (1989) 16, 21 [69] A. Zunger, A. Katzir: Phys. Rev. B 11, 2378 (1975) 16 [70] S. G. Louie, M. Schl¨ uter, J. R. Chelikowsky, M. L. Cohen: Phys. Rev. B 13, 1654 (1976) 16 [71] W. Pickett, M. L. Cohen, C. Kittel: Phys. Rev. B 20, 5050 (1979) 16 [72] S. K. Estreicher, A. K. Ray, J. L. Fry, D. S. Marynick: Phys. Rev. Lett. 55, 1976 (1985) 16 [73] S. K. Estreicher: Phys. Rev. B 41, 9886 (1990) 16 [74] S. K. Estreicher: Phys. Rev. B 41, 5447 (1990) 16 [75] S. K. Estreicher: Phys. Rev. B 60, 5375 (1999) 16 [76] A. A. Bonapasta, A. Lapiccirella, N. Tomassini, M. Capizzi: Phys. Rev. B 36, 6228 (1987) 16 [77] E. Artacho, F. Yndur´ ain: Solid State Commun. 72, 393 (1989) 16 [78] R. Luchsinger, P. F. Meier, N. Paschedag, H. U. Suter, Y. Zhou: Philos. Trans. Roy. Soc. Lond. A 350, 203 (1995) 16 [79] P. Hohenberg, W. Kohn: Phys. Rev. 136B, 468 (1964) 16 [80] W. Kohn, L. J. Sham: Phys. Rev. 140A, 1133 (1965) 16 [81] L. J. Sham, W. Kohn: Phys. Rev. 145, 561 (1966) 16 [82] W. Kohn: Rev. Mod. Phys. 71, 1253 (1999) 16, 17 [83] M. Saito, A. Oshiyama: Phys. Rev. B 38, 10711 (1988) 16 [84] R. Jones, A. Sayyash: J. Phys. C 19, L653 (1986) 16 [85] R. Jones, P. R. Briddon: The ab-initio cluster method and the dynamics of defects in semiconductors, in M. Stavola (Ed.): Identiﬁcation of Defects in Semiconductors, vol. 51A, Semicond. Semimet. (Academic, Boston 1998) Chap. 6, p. 287 16 ¨ Phys. Rev. Lett. [86] J. D. Holbech, B. Bech Nielsen, R. Jones, P. Sitch, S. Oberg: 71, 875 (1993) 16 [87] R. Jones, B. J. Coomer, P. R. Briddon: J. Phys.: Condens. Matter 16, S2643 (2004) 16 [88] S. Og¨ ut, J. R. Chelikowsky: Phys. Rev. Lett. 83, 3852 (1999) 16 [89] S. Og¨ ut, J. R. Chelikowsky: Phys. Rev. B 64, 245206 (2001) 16 [90] J. H. Van Vleck: Phys. Rev. 49, 232 (1936) 17 [91] W. Kohn: Phys. Rev. Lett. 76, 3168 (1996) 18 [92] X. P. Li, R. W. Nunes, D. Vanderbilt: Phys. Rev. B 47, 10891 (1993) 18 [93] S. N. Taraskin, D. A. Drabold, S. R. Elliott: Phys. Rev. Lett. 88, 196405 (2002) 18 [94] R. M. Martin: Electronic Structure, Basic Theory and Practical Applications (Cambridge University Press, Cambridge 2004) 18, 19, 20, 21 [95] D. R. Hartree: Proc. Cambridge Philos. Soc. 24, 89 (1928) 18 [96] F. Fock: Z. Phys. 61, 126 (1930) 18 [97] P. Fulde: Electron Correlations in Molecules and Solids (Springer, Berlin, Heidelberg 1993) 19, 20 [98] E. Fermi: Z. Phys. 48, 73 (1928) 19 [99] L. H. Thomas: Proc. Cambridge Philos. Soc. 23, 542 (1927) 19

26

David A. Drabold and Stefan K. Estreicher

[100] R. G. Parr, W. Yang: Density-Functional Theory of Atoms and Molecules (Clarendon, Oxford 1989) 19 [101] P. Hohenberg, W. Kohn: Phys. Rev. 136, B864 (1964) 20 [102] W. Kohn, L. J. Sham: Phys. Rev. 140, A1133 (1965) 20 [103] D. M. Ceperley, G. J. Alder: Phys. Rev. Lett. 45, 566 (1980) 20 [104] F. Buda, G. L. Chiarotti, R. Car, M. Parrinello: Phys. Rev. Lett. 63, 4294 (1989) 21 [105] A. A. Demkov, J. Ortega, O. F. Sankey, M. P. Grumbach: Phys. Rev. B 53, 10441 (1995) 21 [106] D. S´ anchez-Portal, P. Ordej´ on, E. Artacho, J. M. Soler: Int. J. Quant. Chem. 65, 453 (1997) 21 [107] E. Artacho, D. S´ anchez-Portal, P. Ordej´ on, A. Garc´ıa, J. M. Soler: Phys. Stat. Sol. (b) 215, 809 (1999) 21

Index ab initio, 16, 21 absorption, 13 AIMPRO, 16 amorphous, 22, 23 annealing, 12, 13 antisite, 12 band edge, 12, 13 band structure, 14, 15 basis set, 14–16, 21, 22 Bloch, 14 Bohr, 13 bond-centered, 14, 16, 21 Born–Oppenheimer, 17 Born–von-Karman, 15 Car, 21 charge state, 14 charged defect, 15 classical, 19, 20 cluster, 12, 15, 16 complex, 12, 15 concentration, 11, 13 conduction band, 12 conductivity, 11 core, 16 correlation, 15, 16, 19 Coulomb, 18 covalent, 15 cyclic cluster, 15 Czochralski, 14

dangling bond, 15 decay, 18 deep level, 12, 13 deep-level transient spectroscopy, 13 defect engineering, 11 delocalized, 13 density of states, 17, 18 density-functional theory, 16, 19–22 DFT, 22 diamond, 16 diﬀusion, 12, 14, 21 Dirac, 17 dislocation, 12 disorder, 22 distortion, 14–16 divacancy, 14, 16 DLTS, 13 donor, 12 dopant, 12, 13 doping, 12, 13 eﬀective mass, 13 eigenstates, 21 eigenvalues, 12–15 electron, 12, 13, 17–20 electron paramagnetic resonance, 12 empirical, 15, 22 EMT, 13 energy level, 22 EPR, 12–15

Defect Theory: An Armchair History exchange, 19 exchange-correlation, 20, 21 exclusion principle, 19 fermion, 18 ﬁrst principles, 16, 21, 22 ﬂuctuation, 19 force, 14, 18, 20, 21 Fourier, 13 free energy, 22 FTIR, 13 GaN, 12 gap, 12–16, 18 gap levels, 13, 14 Gaussian, 16 Ge, 11 gettering, 12 glass, 11 grain boundary, 12 Green’s function, 14, 15 ground-state, 18, 20–22 GW, 15, 22 H¨ uckel, 15 Hamiltonian, 14 Hartree, 18, 20 Hartree–Fock, 15, 16, 18, 19 hole, 12, 13 hydrogen, 12, 13, 15, 16, 21 impurity, 12, 14, 16 interface, 12 interstitial, 14, 15 isotope, 13 Jahn–Teller, 14 LCAO, 15, 22 localization, 22 magnetic, 11–13 marker, 22 melting, 11 minimal basis, 16 molecular dynamics, 16, 22 muﬃn-tin, 15 multiscale, 22 nanometer, 12

nanoscience, 12 nonlocal, 17 optical, 11, 12 order-N , 18 oxygen, 12, 14 Parrinello, 21 periodic, 12, 16 periodic boundary conditions, 15, 22 periodicity, 12, 15, 16 perturbation, 12–14, 19 phase diagram, 22 photoluminescence, 12, 13 PL, 12 plane-wave, 21, 22 platelet, 12 population, 22 potential, 14, 18–21 PRDDO, 16 precipitates, 12 pseudopotential, 16 quantum Monte Carlo, 18, 22 radiation damage, 14 Raman, 13 real space, 15 recombination, 12, 14 relaxation, 14 Sankey, 21 scattering, 15 scattering-Xα, 15 Schr¨ odinger, 13, 15, 18 self-energy, 22 self-interstitial, 12, 14 semiempirical, 15, 16 shallow, 12 Si, 11, 12, 14, 16, 22 SIESTA, 21 silicon, 14, 16, 21, 22 Slater, 18 spin, 12–14 stress, 13 substitutional, 13 supercell, 15, 16, 22 surface, 12, 13, 15, 16, 19 symmetry, 13–16, 21

27

28

David A. Drabold and Stefan K. Estreicher

temperature, 11, 12, 20, 22 Thomas–Fermi, 19, 21 tight binding, 21 total energy, 19, 21 transferability, 15 transient-enhanced diﬀusion, 12 transition metal, 11, 12, 14 uniaxial stress, 13

vacancy, 12, 14–16 valence band, 12 variational, 18, 20 vibrational modes, 22 vibrational spectroscopy, 12, 13 Wannier, 14 Watkins, 15

Supercell Methods for Defect Calculations Risto M. Nieminen COMP/Laboratory of Physics, Helsinki University of Technology, POB 1100, 02015 HUT, Finland [email protected]

Abstract. Periodic boundary conditions enable fast density-functional-based calculations for defects and their complexes in semiconductors. Such calculations are popular methods to estimate defect energetics, structural parameters, vibrational modes and other physical characteristics. However, the periodicity introduces spurious defect–defect interactions and dispersion of the defect-induced electronic states. For charged defects, compensating background charging has to be introduced to avoid electrostatic divergences. These factors, together with the intrinsic limitation of standard density-functional theory for accurate estimation of semiconducting gaps, pose challenges for quantitatively accurate and properly controlled calculations. This chapter discusses these issues, including point sampling, electrostatic (Madelung) corrections, valence-band (reference energy) alignment, and other ﬁnite-size eﬀects in supercell calculations. These are important for reliable estimation of formation and migration energies as well as ionization-level prediction. Moreover, the chapter discusses the various ways of generating transferable pseudopotentials, the choice of the exchange-correlation functional, and other topics related to total-energy calculations. Methods to calculate excitation energies and other spectroscopic properties as well as atomic motions are also discussed. Examples of applications of the supercell methods to a few selected semiconductor defects are presented.

1 Introduction An important role for theory and computation in studies of defects in semiconductors is to provide means for reliable, robust interpretation of defect ﬁngerprints observed by many diﬀerent experimental techniques, such as deep-level transient spectroscopy, various methods based on positron annihilation (PA), local-vibrational-mode (LVM) spectroscopy, and spin-resonance techniques [1]. High-resolution studies can provide a dizzying zoo of defectrelated features, the interpretation and assignment of which requires accurate calculations of both the defect electronic and atomic properties as well as quantitative theory and computation also for the probe itself. Materials processing can also draw signiﬁcant advantages of the predictive computational studies. The kinetics of defect diﬀusion and reactions during thermal treatment depend crucially on the atomic-scale energetics (formation energies, migration barriers, etc.), derived from the bond-breaking, D. A. Drabold, S. K. Estreicher (Eds.): Theory of Defects in Semiconductors, Topics Appl. Physics 104, 29–68 (2007) © Springer-Verlag Berlin Heidelberg 2007

30

Risto M. Nieminen

bond-making and other chemical interactions between the atoms in question. Accurately calculated estimates for defect and impurity energetics can considerably facilitate the design of strategies for doping and thermal processing to achieve the desired materials properties. Parameter values calculated atomistically, from the electronic degrees of freedom, can be fed into multiscale modeling methods for defect evolution, such as kinetic Monte Carlo, cellular automaton, or phase-ﬁeld simulation tools [2]. A defect in otherwise perfect material breaks the crystalline symmetry and introduces the possibility of localized electronic states in the fundamental semiconducting or insulating gap. Depending on the position of the host-material Fermi level of the host semiconductor, these states are either unoccupied or occupied by one or more electrons, depending on their degeneracy and the spin assignment. The defects thus appear in diﬀerent charge states, with varying degrees of charge localization around the defect center. To achieve a new ground state, the neighboring atoms relax around the defect to new equilibrium positions. For a point defect a new point symmetry group can be deﬁned. The energy levels in the gap, also known as “ionization levels”, “occupation energy levels” or “transition levels”, correspond to the Fermi-level positions where the ground state of the system changes from one charge state to another. Their values can be computationally estimated by the “∆SCF” approach, i.e., from total-energy diﬀerences between diﬀerent charge states. These gap levels can be probed experimentally by temperature-dependent Hall conductivity measurements, deep-level transient spectroscopy (DLTS), and photoluminescence (PL). The nature of the defect-related gap-state wavefunctions can be examined with electron paramagnetic resonance (EPR) and electron-nuclear double-resonance (ENDOR) measurements. Experimentally, the defect energy levels can often be located with the precision of the order of 0.01 eV with respect to host material band edges. The proper interpretation of the levels and the physical features associated with them pose demanding challenges for theory and computation. At present, the computational accuracy of the level position is typically a few tenths of an eV. It follows that sometimes diﬀerent calculations for the same physical system lead to very diﬀerent conclusions and interpretations of the experiments. Defect calculations may also fail to predict correctly the symmetrybreaking distortions around defects undisputedly revealed by experiments. While theoretical modeling has had considerable success and a major impact in semiconductor physics, there are still severe limitations to its capabilities. The purpose of this Chapter is to point out and discuss these. Density-functional theory (DFT) [3, 4] is the workhorse of atomic-scale computational materials science and is also widely used to study defects in semiconductors, predict their structures and energetics, vibrational and diffusional dynamics, and elucidate their electronic and optical properties, as observed by the various experimental probes. The central quantity in DFT is the electron density. The ground-state total energy is a functional of the

Supercell Methods for Defect Calculations

31

electron density and can be obtained via variational minimization of the functional. The wave-mechanical kinetic energy part of the total-energy functional is obtained not from the density directly but through a mapping to a noninteracting Kohn–Sham system. The mean-ﬁeld electrostatic Hartree energy is obtained from the density, as are in principle the remaining exchange and correlation terms, coded into the exchange-correlation functional. The purpose of this Chapter is to examine critically the methodological status of calculations of defects in semiconductors, especially those based on the so-called supercell methods. As will be discussed in more detail below, there are three main sources of error in such calculations. The ﬁrst is the proper quantum-mechanical treatment of electron–electron interactions, which at the DFT level is dependent on the choice of the exchange-correlation functional. The popular local or semilocal density approximations lead to underestimation, sometimes serious, of the semiconducting gap. The underlying reasons for this are the neglect of self-interactions and the unphysical continuity of the exchange-correlation energy functional as a function of leveloccupation number. This has naturally serious consequences to the mapping of the calculated defect electronic levels onto the experimental energy gap. The second source of errors is related to the geometrical description of the defect region, often known as the ﬁnite-size eﬀect. The third source of error is the numerical implementation of DFT, i.e., the self-consistent solution of the eﬀective-particle Kohn–Sham equations and the evaluation of the total electronic energy.

2 Density-Functional Theory The quantum physics of electrons in materials is governed by the Schr¨odinger equation. Density-functional theory (DFT) provides a parameter-free framework for casting the formidable many-electron problem to a numerically tractable form involving only the three spatial coordinates of the N interacting electrons (as opposed to 3N in the full solution of the Schr¨ odinger equation). The fundamental starting point is the DFT expression for the total energy Etot of the electronic system: 1 2 2 Etot {ψiσ (r), {Rα } = ψiσ (r) − ∇ ψiσ (r) 2m i,σ 2 e2 n(r)n(r ) + dr dr 2 |r − r | Zα Zβ 1 + drVion (r)n(r) + 2 |Rα − Rβ | α,β;α=β

+ Exc [n↑ (r), n↓ (r)] ,

(1)

32

Risto M. Nieminen

2 where the total electronic density n(r) = i,σ fiσ |ψiσ (r)| is expressed as a summation of the one-electron states ψiσ (r), dependent on the spin index σ =↓, ↑ and with the occupation number fiσ . Above, Vion is the nuclear (ionic) potential, and Zα denotes the charge of ion α at Rα . The coupled Kohn–Sham eigenvalue equations −

2 2 ∇ ψiσ (r) + Veﬀ [n↑ (r), n↓ (r)] ψiσ (r) = εiσ ψiσ (r) 2m

(2)

resulting from the minimization of Etot with respect to the density recast the complex many-body interactions into an eﬀective single-electron potential Veﬀ via the exchange-correlation functional Exc . In practice, the functional Exc has to be approximated. The popular choices are functionals where exchange and correlation are treated as functions of the local density and/or its gradients. This sounds drastic, because electronic Pauli exchange is a manifestly nonlocal object, as demonstrated by the Hartree–Fock theory. However, there is a partial cancelation of errors, and these methods are surprisingly robust and accurate. The generalization to spin degrees of freedom is also straightforward in scalar-relativistic DFT. A useful primer for designing DFT calculations has been written by Mattsson et al. [5]. The design of any calculation, whether using periodic boundary conditions, ﬁnite clusters or embedding techniques, involves the choice of the exchange-correlation functional. The choice, whether a particular ﬂavor of local-density (LDA) or local spin-density (LSDA) approximation, a generalized-gradient approximation (GGA), full Hartree–Fock-type exchange, screened exchange, or a “hybrid” between a nonlocal orbital-based functional and a density-dependent functional, deﬁnes the physical accuracy of the calculation. The numerical accuracy of the calculation depends on such technical things as basis-set completeness, accuracy of integration in both real and reciprocal space, convergence criteria, etc. The model accuracy depends naturally on how faithfully the chosen supercell, cluster or embedding methods describe the desired situation. In the context of defects in semiconductors, the ground-state properties can be obtained via the minimization of the total energy Etot with respect to the charge density n(r) and the ionic positions Rα through the Hellmann– Feynman interatomic forces. This enables the calculation of not only the formation energy of a defect in a given lattice position, but also its lowenergy vibrational excitations, and any observables accessible via the charge and spin densities, such as positron-annihilation parameters [6] or hyperﬁne ﬁelds [7–9].

3 Supercell and Other Methods A popular way to calculate defect energetics from ﬁrst principles (i.e., from electronic degrees of freedom) is based on the supercell idea. In this method

Supercell Methods for Defect Calculations

33

Fig. 1. Schematic presentation of the supercell construction. (a) lattice vacancy in a solid, (b) surfaces in a stack of slabs, (c) isolated molecules

one conﬁnes the atoms deﬁning the defect area of interest into an otherwise arbitrary box, which is then repeated inﬁnitely in one or more spatial directions (see Fig. 1). In other words, this box (the supercell) now becomes the new unit cell of the system, and periodic boundary conditions are applied at one or more of its boundaries. For a point-defect assembly in a three-dimensional solid, the system now becomes a three-dimensional periodic defect array. For a line defect (e.g., a dislocation) the result is a regular line-defect network. For a surface, the system becomes a sandwich of material slabs interlaced by vacuum regions. Typical sizes of the supercell are nowadays 64 atoms or larger in a cubic system, and the increasing computational power has enabled supercells with hundreds of atoms. The supercell method is one of the three main approaches to defect calculations. The other two are the ﬁnite-cluster methods [10, 11] and the Green’s function embedding techniques [12–14]. In the former the interesting defect is simply incorporated in a ﬁnite atomic cluster (with often atoms added to the cluster surface to saturate any dangling electron bonds). The ﬁnite-cluster method is well suited for studies of local defect properties (such as vibrational modes), provided that the cluster is large enough and thus the surface eﬀects small. However, care should be taken to make sure that manipulating the cluster surface does not interfere with the defect-localized electrons. Estreicher and Marinyck [15] have shown how this can inﬂuence, for example, the defect-related hyperﬁne ﬁelds. The embedding techniques, in turn, match the perturbed defect region to the known DFT Green’s function of the unperturbed host material, and oﬀer in principle the best way to study isolated defects. However, the numerical implementation of the Green’s function method is challenging for accurate interatomic forces and long-range atomic relaxations, as it requires a well-

34

Risto M. Nieminen

localized defect potential and usually short-range basis functions. Thus, supercell methods have surpassed the Green’s function methods in popularity. The great advantage of supercell calculations is that the periodic boundary conditions allow the utilization of the many eﬃcient techniques derived for the quantum physics of periodic systems. The wavevectors of the Brillouin zone (BZ) in the reciprocal space of the supercell are good quantum numbers, and the standard “band-structure methods” of periodic solids can be applied in full force. Particularly fast computation methods can be performed by using Fourier analysis (plane-wave basis sets), as they adopt naturally to periodic boundary conditions and oﬀer spatially uniform resolution. The supercell approach enables the full relaxation of the structure to minimize total energy, and the calculation of the formation and migration energies of defects in diﬀerent charge states as a function of the Fermi-level position of the host semiconductor, and as a function of the chemical potentials of the atoms building up the material. Thus, the method can be conveniently adapted to describe such eﬀects as the host material stoichiometry on the energetics of isolated defects in compound semiconductors [16]. From supercell calculations one can extract several useful physical properties, such as: 1. the probabilities of certain types of defect to form under given chemical and thermodynamical conditions during the growth, 2. the basic nature (acceptor, donor, deep level) of the defect electronic states, 3. the migration and recombination barriers, 4. vibrational modes, hyperﬁne ﬁelds, positron-annihilation parameters and other ground-state properties, and 5. within certain limitations, excited-state (for example optical) properties as well. The ground-state properties are those most reliably accessible. For example, the defect-induced electronic energy levels in the fundamental gap are obtained as diﬀerences between formation energies for diﬀerent charge states.

4 Issues with the Supercell Method The obvious drawback of the supercell methods for defect calculations is that the periodicity is artiﬁcial and can lead to spurious interactions between the defects. They have a ﬁnite density, and do not necessarily mimic the true physical situation with an aperiodic, very low density defect distribution. The supercell method, widely used and with demonstrated success in defect studies, requires a critical examination of the ﬁnite-size and periodicity eﬀects. The ﬁrst consequence of the ﬁnite-size supercell approximation is the broadening of the defect-induced electronic levels to “defect bands”, with a bandwidth of the order of 0.1 eV for 64-atom supercells. This translates into a diﬃculty in placing accurately the ionization levels, also in the total-energy based ∆SCF approach. The one-electron Kohn–Sham states associated with the defect are often assigned a position by averaging over the supercell Brillouin zone, or just values at the Brillouin zone origin (the Γ point) are dis-

Supercell Methods for Defect Calculations

35

cussed as they exhibit the full symmetry of the defect. It can be argued that the defect-state dispersion has a smaller eﬀect on the total energies that include summations and integrations of the Kohn–Sham states over the entire Brillouin zone. Thus, ionization levels determined from the total-energy differences would also be less sensitive to the defect-band dispersion. However, this is hard to prove systematically. Another source of diﬃculty is the accurate determination of the host crystal band edges (valence-band maximum, conduction-band minimum), which are the natural reference energies for the defect-induced gap states. In the defect-containing supercell, the band-edge states themselves are aﬀected by the defect. The band-edge positions are often determined by aligning a chosen reference level between the defect-containing and perfect solid. For example, the eﬀective potential in a localized region far from the defect can be aligned with the potential in the same region in a perfect crystal. The calculated band-edge distances from the reference energy in a perfect crystal can then be used to align the band edges in the system containing the defect. Alternatively, one can consider a deeper, core-level energy of an atom as a local reference. Another possibility is to deﬁne as the “crystal zero” the electrostatic potential at a Wigner–Seitz cell boundary far away from the defect. This is particularly convenient when the atomic-sphere approximation (ASA) is used in the context of minimal basis sets, such as the LMTO [17]. Another, more diﬃcult problem arises with charged defects. In order to avoid divergences in electrostatic energies, a popular solution is to introduce a homogeneous neutralizing background charge to the supercell array, which enables the evaluation of electrostatic (Coulomb) energies. This, however, introduces an electrostatic interaction between the periodic charge distribution in the supercells and the background, which vanishes only at the limit of inﬁnitely large supercells. The inﬂuence of the ﬁctitious charge has to be subtracted in the end, and this is a highly nontrivial task, as discussed below. Point defects induce elastic stress in the host lattice, which is relieved by ion displacements, i.e., lattice relaxation. The lattice-relaxation pattern is restrained by the supercell geometry. The argument, often used in supercell calculations, is that the ion displacements vanish near the borders of the supercell. However, this does not necessarily guarantee that the long-range ionic relaxations are correctly described, as the supercell symmetry itself may ﬁx the positions of the border ions. According to elastic continuum theory, the strain ﬁeld at large distances from the point defect should fall oﬀ as |r|−3 and −2 the ionic displacements should fall oﬀ as |r| . In tetrahedrally coordinated covalent materials the distances between the periodic images along the rigid [110] zigzag chains are typically more important to the convergence of lattice relaxations than the volume relaxations. A case in point is the vacancy in silicon [18], where the sense of the lattice relaxation changes from outward to inward only at large enough cell sizes. A similar behavior is also observed in ﬁnite-cluster calculations [19].

36

Risto M. Nieminen

The ﬁnite size of the supercell thus restricts also the ionic relaxations around the defect. The relaxation pattern is truncated midway between a defect and its nearest periodic replica. In the case of long-range relaxations this cutoﬀ may be reﬂected dramatically close to the defect, as was demonstrated by Puska et al. [18] by detailed calculations for vacancies in silicon. Further comparison of the supercell to the ﬁnite-cluster and Green’s function methods reveals the following. The supercell and Green’s function methods have a well-deﬁned electron chemical potential (they are coupled to a reservoir of electrons) whereas the cluster method does not. This has consequences for the treatment of ionization levels, which is somewhat problematic for the cluster method. The ﬁnite-size eﬀect is there in the cluster method as well, as the clusters can contain spurious surface-related eﬀects. The Green’s function method is mathematically elegant and in principle the best for isolated defects, but its computational implementation is diﬃcult in view of the accuracy required for total electronic energies and derived quantities (such as interatomic Hellmann–Feynman forces). Finally, it is important to note that defect and impurity calculations should, as a rule, be carried out using the theoretical lattice constant, optimized for the bulk unit cell. This is crucial in order to avoid spurious elastic interactions with defects or impurities in the neighboring supercells. The purpose is to investigate properties of isolated defects or impurities in the dilute limit. If the volume of the defect-containing supercell is relaxed (in addition to relaxing the positions of the atoms near the defect), the calculation would in fact correspond to ﬁnding the lattice parameter of the system containing an ordered array of defects at a high concentration.

5 The Exchange-Correlation Functionals and the Semiconducting Gap The fundamental semiconductor gap Eg is deﬁned as the diﬀerence between the ionization energy I and the electron aﬃnity EA of the bulk material, Eg = I − EA .

(3)

As both quantities can be written in terms of total energies of systems with diﬀerent numbers of electrons, the value of the gap Eg is, in principle, a ground-state property and can thus be calculated within the Kohn–Sham DFT. The fundamental gap can also be written as Eg = EgKS + ∆xc .

(4)

EgKS is the diﬀerence between the highest occupied and lowest unoccupied Kohn–Sham eigenvalues εiσ . ∆xc is the discontinuity (as a function of the occupation number) of the exchange-correlation potential at the Fermi level.

Supercell Methods for Defect Calculations

37

The estimation of semiconductor bandgaps and positions is one of the classic failures of local(-spin-)density (L(S)DA) formulation of the Kohn– Sham DFT. There are two origins of this error. First is the self-interaction error inherent in the LDA potential, and the second is the vanishing of the discontinuity ∆xc of the local-density exchange potential as a function of the level occupation at the Fermi level. They lead to both wrong absolute energy positions and too small or entirely absent bandgaps for many materials. This is not remedied by semilocal approximations for exchange and correlation, such as the generalized-gradient approximations (GGA) where the discontinuity also vanishes. In fact, the experience is that GGA approximations tend to make the gap even smaller than local-density approximations [20]. This can be traced to the property of GGA methods increasing the interatomic distances and lattice constants compared to LSDA. It is another well-known ﬂaw of local-density methods that they overbind molecules and solids and underestimate bond and lattice distances. GGA methods correct and sometimes overcorrect this, but give even smaller bandgap values. A qualitatively opposite problem is encountered with the Hartree–Fock method, which is known to considerably overestimate the bandgaps. Moreover, its application to metallic systems leads to well-known problems, such as the vanishing density of states at the Fermi level. Thus, intuitively, a hybrid method “interpolating” between the two seems an attractive approach. Nonlocal descriptions of exchange are expected to improve the Kohn– Sham bandgaps as they remove the self-exchange error and exhibit discontinuity at the Fermi level. In the “exact exchange” (EXX) formulation one evaluates the exchange energy and potential using the Kohn–Sham (rather than Hartree–Fock) wavefunctions. St¨ adele et al. [21] have shown that the discontinuity ∆x in the exchange potential is much larger than the bandgap for several semiconductors, which points to the existence of a large cancellation between the exchange ∆x and the corresponding correlation ∆c . The EEX method has been reported to give very good values for the bandgap and many other properties for sp semiconductors [22]. However, when applied to rare-gas solids, EXX fails to reproduce the experimental bandgaps [23]. A related problem is the position of the d band in many solids. Again, the self-interaction error in local-density methods displaces the d states and contributes to the bandgap error. The d band positions can be improved by the explicit removal of self-interactions [24], but the application of the nonlocal EXX does not seem to lead to a consistent improvement of both d band positions and bandgap values. This points to the important interplay between treatment of nonlocal exchange and the description of the lower-lying and core states in semiconductors and insulators. It has recently been pointed out [25] that the lack of explicitly treated core-valence interactions can lead to an anomalously good agreement of the calculated Kohn–Sham gap with the experimental gap in sp semiconductors. The inclusion of these interactions worsens the agreement, while leading to a consistent treatment of semiconductors and insulators. It

38

Risto M. Nieminen

thus appears that the EXX alone does not solve the bandgap problem, although it is a marked improvement over LDA or GGA. A major drawback is also the high computational cost of EEX, which has so far prohibited its widespread use in defect calculations. In the screened-exchange LDA (sx-LDA) scheme [26] the Kohn–Sham single-particle orbitals are used to construct a nonlocal exchange operator, again improving the description compared to the local-density approximation. The many-body correlations and screening missing from the Hartree–Fock method are treated in a form of model screening and LDA correlation. This approach can solve the gap problem, but contains a phenomenological constant (e.g., the Thomas–Fermi screening constant). Lento and Nieminen [27] have applied this method for a prototypical supercell defect calculation (vacancy in Si). While the method can in principle give accurate total energies and thus ionization levels (and the correct gap), its full exploitation is still prohibitively expensive computing-wise. As with other hybrid functionals and with EXX, the computational cost is typically two orders of magnitude larger than with LDA or GGA. Thus the calculations with full lattice relaxation have so far been limited to supercells not large enough to allow the correct pattern to emerge (see Sect. 16 below). There are other suggested approaches to overcome the failure of DFT to produce accurate bandgaps and excited-state properties. However, currently no method is available that would go beyond standard DFT and yet be feasible for total-energy calculations for the large supercells required to investigate defects. The class of methods, such as the GW approach [28] which are mainly aimed at calculating the (quasiparticle) band structure and properties derived thereof, are prohibitively expensive for large supercells. Presently, such calculations can be carried out with supercells with less than twenty atoms. However, this size is perfectly adequate for treating well-localized excitations, such as self-trapped excitons [29]. The gap problem may sometimes make calculations for certain defect levels impossible. The too-narrow gap may induce the defect level to be a resonance in the conduction or valence band. In this case some charge states would not be accessible at all. It should be noted that this can also happen in just some part of the Brillouin zone because of the defect-level dispersion in the supercell approach. A possible remedy is then to simply occupy the defect level, ignoring the fact that the state lies above the conduction-band minimum at other k points. Apart from underestimating the bandgap and thus hampering the positioning of the possible ionization levels, the local (or quasilocal)-density approximation for exchange and correlation can sometimes lead to other difﬁculties with the defect-localized electron states. This has recently been discussed by Laegsgaard and Stokbro [30]. They considered a substitutional Al impurity on the Si site in SiO2 . LDA and GGA calculations predict a structure that has the full tetrahedral symmetry. However, ENDOR experiments show unambiguously that the defect wavefunction is localized on just one of

Supercell Methods for Defect Calculations

39

the four neighboring oxygen atoms, as the hyperﬁne splittings are radically diﬀerent from those expected for four equivalent neighbors. The source of this problem can again be traced to the self-interaction error in LDA and GGA. In LDA/GGA, there is a penalty for localizing a single electron as the cancelation between self-exchange/correlation and self-Coulomb interactions is not complete. Thus, one overestimates the Coulomb energy of a localized state, which then leads to charge delocalization. In the true situation, there is just a single electron state contributing to the Coulomb energy. Thus, the calculated charge delocalization is completely due to self-interaction. If exchange is treated correctly as in the Hartree–Fock theory, self-interaction is eliminated and one obtains the correct distorted structure with the wavefunction localized on a single oxygen atom. As noted above, the problem with Hartree–Fock is that it seriously overestimates the bandgap and spin splittings, and is as such usually not a good tool for calculations of semiconductor defects. A self-interaction-corrected (SIC) scheme for the case of hole trapping in SiO2 was recently suggested by d’Aveszac et al. [31]. In their approach the Coulomb energy arising from the charge density of a single defect orbital and the associated contribution to the exchange-correlation energy are explicitly subtracted. This is technically straightforward for methods using localized basis sets, but can also be implemented using projection techniques with plane-wave methods. The physical idea of this self-interaction correction is that delocalized states do not suﬀer as much from self-interaction error as localized states do. In the standard SIC [32, 33] approaches there is some ambiguity in choosing the states to which the correction should be applied. For defect calculations, the localized state in the gap is well deﬁned and the application of the correction is quite straightforward. The LDA/GGA gap error is a persistent and rather harmful problem in semiconductor defect physics. The Kohn–Sham eigenvalues of (2) are Lagrange parameters used to orthogonalize the states in total-energy minimization, but cannot be interpreted as true electron-excitation energies. These could be obtained from quasiparticle theories such as Hedin’s GW approach [34] or time-dependent density-functional theory [35]. The GW method is computationally expensive and cannot be applied to defect supercells with many atoms. Its ability to give converged total energies is not clear. However, it is a powerful approach for doing perturbative calculations for optical and other excitation spectra, and can be generalized to include the ﬁnal-state electron–hole interactions through the Bethe–Salpeter equation [36]. One simple, obvious and often used possibility is to use the “scissor operator”, i.e., to correct the bandgap by simply shifting the unoccupied and occupied states further away from each other. This, of course, destroys the self-consistency between Kohn–Sham eigenvalues and eigenfunctions, which may be detrimental for observables calculated from them. For defect physics, the question arises whether to shift the defect levels or not in such a process.

40

Risto M. Nieminen

Intuitively, one would expect acceptor-like levels to move with the valenceband edge and donor-like states with the conduction-band edge, while levels deep in the bandgap would not move at all. This reasoning is, of course, quite arbitrary and unsatisfactory. A recent example of these diﬃculties is the work on the oxygen vacancy in ZnO, where the LDA gap is again considerably in error. Two calculations [37, 38] have addressed this system using the LDA+U method [39], where an onsite Coulomb repulsion U is added “by hand” when calculating the Zn d-states. This shifts the occupied d bands and subsequently the valence-band minimum downwards. The defect level associated with the oxygen vacancy then moves deeper into the gap from the valence-band maximum. If one leaves the defect level in place and shifts just the conduction bands up, there is a single level in the lower half of the gap. If, on the other hand, one decides from LDA+U calculation how much valence/conduction band character the state has, one ends up moving the state further up in the gap, into the upper half. As the experiments are ambiguous at this time, the matter is undecided and again calls for a better solution to the gap problem. Finally, one should mention the quantum Monte Carlo (QMC) methods that look promising for addressing total-energy calculations for defects and impurities. They approach the problem of interacting electrons by addressing the correlations explicitly and build in the Pauli exchange by starting from a Slater determinant. The ﬁxed-node QMC method has been applied to study self-interstitials in Si [40]. The formation energy of the split-110 interstitial defect was found to be signiﬁcantly higher with QMC than LDA, which can be explained by the upward shift of the defect-induced level in the bandgap. Further work includes QMC studies of optical and diﬀusive properties of vacancies in diamond [41]. If QMC methods can be extended to large enough supercells, to force and relaxation calculations, and to secured convergence with respect to k-point summation, they can provide a most useful set of benchmarks for accurate total-energy calculations for defects in semiconductors. The above discussion may give an overly pessimistic impression of the capabilities of DFT calculations for defects in semiconductors. The other side of the coin is much brighter. There is a vast inventory of “standard” DFT calculations that have produced robust and reliable results for semiconductor defects and have thus decisively contributed to their identiﬁcation. An illustrative example is the extensive work on III–V nitride semiconductors, recently reviewed by Van de Walle and Neugebauer [42].

6 Core and Semicore Electrons: Pseudopotentials and Beyond The widespread use and success of DFT in predicting various materials properties stems largely from the successful application of the pseudopotential (PP) concept. Only relatively few “valence” electrons of an atom are

Supercell Methods for Defect Calculations

41

chemically active. The replacement of chemically inert “core” electrons with an eﬀective core potential both reduces the number of electronic degrees of freedom and avoids the numerical challenge posed by rapidly varying wavefunctions near the nucleus. Eﬃcient numerical techniques such as the fast Fourier transform (FFT) can be used. The replacement of the all-electron potential with a PP is, however, a nontrivial task where a balance has to be struck between optimal transferability (accurate reproduction of all-electron atom behavior) and computational eﬃciency (slow spatial variability). Several methods are popular for generating PPs. They include the generalized norm-conserving pseudopotentials of Hamann [43], Troullier and Martins [44], Hartwigsen et al. [45] and the ultrasoft, non-norm-conserving PPs of Vanderbilt [46]. It is important to realize that the true ﬁgure of merit of a PP is not how well its results match experiment, but how well it reproduces the results of all-electron calculations when using otherwise similar methods. The separable PPs commonly used in the context of plane-wave calculations, such as those of the Kleinman–Bylander [47] form, are built from norm-conserving PPs. The separation process can sometimes add complications, for example, in the form of so-called ghost states. The construction of reliable ultrasoft pseudopotentials [46] or projected-augmented-wave (PAW) potentials [48, 49] presents additional challenges, but the latter is quickly gaining in popularity as it has proven a particularly robust and transparent approximation. To compare calculated values reported in the literature for defects in semiconductors, speciﬁc details of the PP generation are important for the reproduction of a given result. Several parameters usually enter the PP construction, such as the core radii for diﬀerent angular-momentum channels and the core-matching radii. The eﬀectiveness of a given PP needs to be checked and validated in every new chemical environment before being used in quantitative studies. Constructing PPs thus involves compromises, and in reporting computational results it is important to state those compromises clearly. In particular, the choice of a given state as an “active” valence state vs. its treatment via perturbative, nonlinear core-valence corrections [50] are crucial. For example, it has been demonstrated [51] that a nonlinear core-valence correction is necessary to get spin-polarized states of ﬁrst-row atoms O and N properly described. Unlike previously assumed, the 1s core in these atoms is not so deep as to be uninvolved in the chemistry important in deﬁning the valenceelectron potential. An interesting approach that yields bulk band structures in good agreement with experiment is based on the idea of self-interaction and relaxationcorrected pseudopotentials (SIRC) [52]. The removal of self-interactions has important consequences for ionization levels in the semiconducting gap, as discussed above. However, it seems that the SIRC approach does not allow a simple self-consistent calculation of total energies.

42

Risto M. Nieminen

Finally, it should be emphasized that consistency in the choice of the exchange-correlation functional for pseudopotential construction and their application is highly advisable. The problems of using a diﬀerent functional for the two have been demonstrated, especially in the cases where polarizable semicore states are present [53].

7 Basis Sets The use of DFT is not limited to static electronic-structure problems such as total energies and bond distances. The potential-energy (Born–Oppenheimer) surface deﬁned by the positions of the nuclei deﬁnes the interatomic forces, and in recent years there has been rapid growth in the use of ﬁrst-principles molecular dynamics (FPMD) within the ﬁnite-temperature DFT framework for studying many materials properties, including atomic vibration and migration, and the full equation of state (EOS). If the force ﬁelds or pressure or stress tensor of the system are of interest, additional care must be taken to ensure that the calculated quantities are of suﬃcient numerical accuracy. Whereas errors in the total energy are second order with respect to errors in the electron density or Kohn–Sham eigenfunctions, errors in the interatomic forces and pressure are ﬁrst order. The errors are signiﬁcantly aﬀected by the completeness and accuracy of the basis set. A popular choice is the plane-wave expansion for the Kohn–Sham states, ψnσk (G) exp[−i(k + G) · r] . (5) ψiσ (r) = ψnσk (r) = G

The summation is over the reciprocal lattice vectors G of the superlattice. In plane-wave calculations the accuracy of the basis set is determined by 2 2 max ) the chosen kinetic energy cutoﬀ or maximum wavevector Ecut = (k+G . 2m It is important to realize that while a lower cutoﬀ may be suﬃcient for the convergence of total energies, it may be totally unacceptable for calculating interatomic force constants or pressure/stress tensors. The reason that forces are more sensitive to the plane-wave cutoﬀ than total energies is that the real-space force formula contains the derivatives with respect to coordinates (see (6)). This derivative will introduce an extra factor of the reciprocal lattice vectors G into the reciprocal-space formulae and the maximum value Gmax is determined by the cutoﬀ. It also follows that exchange-correlation functionals involving gradients of the density (such as GGA) are more sensitive to the cutoﬀ than LDA. The issue of basis-set suﬃciency is even more critical when using local basis sets, for example linear combinations of numerical atomic orbitals [54, 55] or Gaussians [56]. A great advantage of local-orbital methods is the much smaller size of the basis (typically up to twenty basis functions per atom),

Supercell Methods for Defect Calculations

43

reﬂecting their economy when ﬁtting rapidly varying wavefunctions. However, as a discrete set the convergence of a local basis is not simply controlled by a single parameter. Local basis sets always require “optimization” and experience, and tested basis sets are collected into libraries with limited possibilities for modiﬁcation. The words of caution about plane-wave basis-set convergence apply even more strongly to local basis sets. While a well-designed basis set (for example, the “double-zeta plus polarization” (DZP)) does match the accuracy of a fully converged plane-wave calculation, the omission of the polarization term or calculation with single s and p functions can lead to large errors. This is particularly true for forces. For atoms far from equilibrium (e.g., under large strain) it may be necessary to increase variational freedom by expanding the basis to triple functions to achieve convergence. In some cases, especially for systems with large open volumes, it is advisable to augment the basis set by introducing “ﬂoating orbitals”, i.e., basis functions not centered at atoms. Finally, one should mention the real-space methods quickly gaining popularity [57,58]. They use ﬁnite-diﬀerence approximations for the kinetic-energy operator (ﬁnite elements are also a possibility), and the quality of the basis set can be controlled simply by the choice of the spacing of the real-space grid. The great advantage of real-space techniques is their easy adaptability to diﬀerent boundary conditions (periodic, open, etc.), which is especially useful for studies of defects in low-symmetry nanostructures, where supercell methods can be quite wasteful.

8 Time-Dependent and Finite-Temperature Simulations Within the Born–Oppenheimer approximation, the electronic and ionic motion and timescales are well separated. First-principles molecular dynamics (FPMD) can be implemented on the Born–Oppenheimer hypersurface by calculating an instantaneous value for the electronic total energy Etot [{Ri }] as determined by all the ionic positions {Ri }. The forces acting on the atoms are then evaluated as Fi = −

∂Etot ∂Ri

(6)

and Newton’s equations of motion are solved for the ionic degrees of freedom, using standard algorithms for the second-order temporal diﬀerential equations. Periodic boundary conditions are routinely implemented, and allow simulations of disordered amorphous or liquid phases. A ﬁxed-volume supercell with conserved total energy corresponds to the microcanonical statistical ensemble. The constant-temperature (canonical) ensemble can be simulated using the Nos´e–Hoover thermostat [59, 60]. Allowing the supercell volume to change as a dynamical variable leads to the constant-pressure ensemble,

44

Risto M. Nieminen

and structural phase transformations are enabled by making the directional vectors spanning the supercell also dynamical [61]. The molecular-dynamics techniques also enable free-energy simulations. The thermodynamic integration formula for the (Helmholtz) free energy reads 1 dλ H1 − H0 λ , (7) ∆F = 0

where ∆F is the free-energy diﬀerence between the actual system with the Hamiltonian H1 and a reference system with the Hamiltonian H0 , and . . . λ denotes a temporal average along an isobaric-isothermal trajectory generated from the Hamiltonian H(λ) = λH1 + (1 − λ)H0 .

(8)

Under ergodic conditions this is equivalent to an ensemble average. If the free energy of the reference system is known, (7) allows one to compute the free energy of the actual system. The FPMD method is particularly well adaptable to the supercell geometry. The quantum dynamics associated with the electronic degrees of freedom can be described by the time-dependent Schr¨ odinger equation. Within the density-functional formulation of many-body systems, this leads to the powerful formulation of time-dependent density-functional theory [62]. It can be cast in the form of time-dependent Kohn–Sham equations with a generalized, time-dependent exchange-correlation potential. These equations can be explicitly solved by time-propagation algorithms and starting from an appropriately prepared initial state. The time evolution of the wavefunctions and the density can then be analyzed to obtain the desired physical quantities, such as the full response of the system to an external, polarizing ﬁeld or exciting pulse. The Kohn–Sham equations with an external time-dependent perturbation can also be treated in the linear-response limit if the perturbation is weak. As the Kohn–Sham states are noninteracting, the linear-response function of the system can be constructed. The linearization leads to integrodiﬀerential equations with an exchange-correlation kernel derived from the description of Exc . Linear-response TDDFT is a popular method [63] to estimate excitation energies, polarizabilities and inelastic-loss properties (such as photoabsorption cross sections), especially for ﬁnite systems. The treatment of extended systems (periodic boundary conditions) within TDDFT requires the consistent handling of electronic currents in the system, and is best characterized as time-dependent current-density-functional theory (TCDFT) [64].

9 Jahn–Teller Distortions in Semiconductor Defects The Jahn–Teller eﬀect is the removal of electronic degeneracy by spontaneous lowering of spatial symmetry of atoms surrounding a defect, which leads to

Supercell Methods for Defect Calculations

45

Fig. 2. The splitting of the defect-related gap states for a vacancy in Si. The point symmetry group is denoted for defects in diﬀerent charge states. The arrows denote the population of the two spin states

the lowering of total energy. This is the result of a general theorem [65], with several well-known consequences in solid-state physics. It is easiest to discuss the Jahn–Teller mechanism by using the monovacancy and a substitutional metal impurity in a tetrahedrally bonded semiconductor (Si) as examples. These same systems will later be presented as examples of state-of-the-art supercell DFT calculations in Sect. 16. 9.1 Vacancy in Silicon In the pioneering linear combination of atomic-orbitals (LCAO) model by Watkins [66] (see Fig. 2), the electronic conﬁguration of a neutral vacancy in Si (VSi ) with full cubic (Td ) symmetry is a21 t21 , analogous to a Si atom ([N e]3s2 2p2 ). The a1 state lies in the valence band (is a resonance) and is doubly occupied. The other state t1 is in the fundamental gap and can contain up to six electrons. It is pushed into the gap by the repulsive potential due to the removal of a positive ion in the lattice. In compound semiconductors, therefore, the states are expected to lie higher for anion vacancies with a larger number of removed valence electrons than for cation vacancies. The ﬁlling of the gap states with rising Fermi level is associated with the relaxations of the atoms neighboring the defect. If there are no electrons in these levels, the Td symmetry of the ideal vacancy (ideal crystal) is preserved. The only possible relaxation is of the breathing-mode symmetry around the defect center. Adding one or more electrons to the levels splits the degeneracy through the Jahn–Teller eﬀect, and lowers the symmetry through atomic relaxation. The main component of this distortion is tetragonal, giving D2d symmetry. This can occur in two senses, giving either a short, broad (“type A”) or long, thin (“type B”) shape for the box bounding the nearest-neighbor atoms (see Fig. 3). This determines the order of the resulting b2 and e states. For VSi , the latter option turns out to be valid. One electron added to the gap level thus results in a singly positively charged vacancy with D2d symmetry. Adding more electrons usually implies

46

Risto M. Nieminen

Fig. 3. The bounding boxes for the Si vacancy with distortions of diﬀerent pointsymmetry orientation

higher total energies because of the intraelectron Coulomb repulsion between the localized electrons in the gap states. However, adding a second electron to the vacancy in Si can enhance the pairing distortions (while retaining D2d symmetry) and the Jahn–Teller splitting, possibly outweighing the increased Coulomb repulsion. This is the negative-U phenomenon [67] often encountered in semiconductor defects. Another way of stating the eﬀect is to say that the energy to remove two electrons from VSi0 is less than to remove one electron. Thus VSi+ would be unstable. A trigonal distortion from Td symmetry occurs when a third electron is added and the vacancy is in the charge state q = −1. This lowers the symmetry to or C2v or C3v and splits the e state to b2 and b1 . The quantitative results of state-of-the-art supercell calculations for the charge-state-dependent relaxation and how they match the Watkins model are given in Sect. 16. 9.2 Substitutional Copper in Silicon Neutral CuSi [68] is isoelectronic with the negatively charged VSi (see Fig. 4). The triplet state t32 is partially occupied, in the bandgap, and susceptible to the Jahn–Teller eﬀect. If onsite electronic repulsion prevails, the high-spin S = 3/2 states would be stabilized, as for example in the case of negatively charged substitutional Ni in diamond or the silicon vacancy in SiC [69]. Spinorbit coupling also aﬀects the orbital degeneracy, especially for the heavier impurity elements.

Supercell Methods for Defect Calculations

47

Fig. 4. The evolution of the defect-related states of substitutional Cu in Si from those for a Cu atom and Si vacancy

In general, it is in principle possible to reach higher positive and negative charge states by adding/removing electrons to/from the localized levels. The stability of a given charge state requires accurate calculation of its total energy, and is subject to the computational limitations discussed above and further expanded upon in Sects. 13–15.

10 Vibrational Modes The phonon modes of a vibrating solid can be calculated using the powerful linear-response formalism [70], where the DFT total-energy hypersurface enters as the ground state and determines the elastic response. This formalism has been implemented using diﬀerent basis sets for bulk calculations, including short-range local orbitals [71]. For defects in semiconductors, it is, however, the localized vibrational modes (LVMs) associated with defects that are often useful ﬁngerprints for defect identiﬁcation. In the case of defectassociated localized modes, a more economical route than the full phonon response is provided by considering only a single supercell. This is because the interaction between the defect replicas can be made small by using a large enough cell, whereby the vibrations do not mix and there is no phonon dispersion. The total energy of the supercell can be written as a Taylor series around the equilibrium positions in the harmonic approximation as 1 ∂ 2 Etot sαi sβj + · · · , Etot [{Rαi + sαi }] = Etot {Rαi } + 2 ∂Rαi ∂Rβj αi,βj

(9)

48

Risto M. Nieminen

where sαi is the ith Cartesian component of the atomic displacement of the ion α. The coupling constants ∂ ∂Etot

(10) ≡ Φαi βj ∂Rαi ∂Rβj are conveniently obtained as numerical derivatives of the (Hellmann–Feynman) forces on the atoms as they are shifted a small distance from their equilibrium positions around the defect (“frozen phonons”). The frequencies ω and amplitudes u of the localized vibrations can then be obtained as the normal-mode solutions to the equations βj −ω 2 uαi + Dαi , uβj = 0 , (11) βj

where

βj Dαi

is the dynamical matrix. If Mα is the mass of ion α,

1 βj Dαi ≡ Φαi βj . Mα Mβ

(12)

In practical LVM calculations, selected atoms in the supercell are displaced to all three Cartesian directions, and after each displacement the ground-state electronic total energy is obtained and the Hellmann–Feynman forces calculated. This is done for all atoms that are a priori considered important for the description of the local vibrational modes around the defect. The dynamical matrix is then calculated by the ﬁnite-diﬀerence approximation using these forces and displacements. The normal modes and the corresponding vibrational frequencies can then be obtained by diagonalizing the dynamical matrix. The harmonic modes can easily be quantized and the zero-point vibrational motion estimated. Within the harmonic approximation, the phonon spectrum can be used to estimate the vibrational entropy of a given defect, which can then be entered as the prefactor when estimating absolute defect concentrations in thermal equilibrium. Alternatively, the phonon spectrum, including the localized modes, can be obtained by MD simulation. The simulation time has to be long enough so that all the relevant vibrational modes have undergone several oscillation periods. The vibrational frequencies can then be obtained by Fourier transforming the velocity autocorrelation function of the moving ions. This usually requires that the LVM is well separated from the density of states for host-lattice vibrations. The MD approach includes also the anharmonic contributions to the vibrations, but not the zero-point motion.

11 Ionization Levels The formation energy of a defect or impurity X in the charge state q is ni µi + q [µe + Ev ] , (13) E f [X q ] = Etot [X q ] − Etot [bulk] − i

Supercell Methods for Defect Calculations

49

where Etot [X q ] is the total energy from a supercell calculation with a defect or an impurity in the cell, and Etot [bulk] is the total energy of the equivalent bulk supercell. ni indicates the number of atoms of type i (host or impurity), either added (ni > 0) or removed (ni < 0) from the defected supercell, and µi denote the corresponding atomic chemical potentials. They represent the energy of the reservoirs with which atoms are exchanged when assembling the crystal in question. µe is the electron chemical potential (Fermi level), referenced here to the valence-band maximum Ev in the bulk material. The valence-band maximum of defect supercell has to be aligned with that in the bulk (see below). For a monoatomic solid, the formation energy for a defect in the charge state q reads Eqf = Eqdef − N µ + q(Ev + µe ) ,

(14)

where Eqdef is the total energy of the defect-containing supercell and N the total number of atoms in it. The thermodynamic ionization (transition) level of a given defect Ed (q/q ) is deﬁned as the Fermi-level position where the charge states q and q have equal total energy. In experiments where the ﬁnal charge state can relax to its equilibrium conﬁguration after the transition (excitation), this is the energy level that would be observed. The ionization levels are therefore observed in DLTS experiments or (for shallow levels near band edges) as the thermal ionization energies derived from temperature-dependent conductivity or Hall eﬀect data. The optical energy Edopt (q/q ) associated with a transition between charge states q and q is deﬁned similarly to the thermodynamic transition energy, but now the ﬁnal state with charge q is calculated using the atomic geometry of the initial state q. The optical level is observed in “vertical” absorption experiments where the ﬁnal charge state cannot relax to its equilibrium. In emission experiments, on the other hand, the initial excited state has evolved towards its minimum-energy conﬁguration, which is diﬀerent from the ground-state structure. Optical emission and absorption peaks are thus separated by the so-called Stokes shift. This poses challenges for both the experimental assignment of peaks and the theoretical analysis. For a two-component (compound) semiconductor, (13) can be rewritten [16] in a form that reﬂects the stoichiometry of the host material. It is gauged by the chemical potential diﬀerence ∆µ of an AB compound as ∆µ = µA − µB − [µA (bulk) − µB (bulk)] ,

(15)

with an allowed range −∆H ≤ ∆µ ≤ ∆H ,

(16)

50

Risto M. Nieminen

where the lower limit corresponds to A-rich and the upper limit B-rich material. ∆H is the heat of formation of the compound from its bulk constituents, ∆H = µA (bulk) + µB (bulk) − µAB (bulk) .

(17)

By deﬁning E1f [X q ] ≡ Etot [X q ] − 12 (nA + nB )µAB (bulk) − 12 (nA − nB )[µA (bulk) − µB (bulk)] + qEv

(18)

one can write (13) in the short form E f [X q ] = E1f [X q ] + qµe − 12 (nA − nB )∆µ .

(19)

Equations (14) or (19) provide a basis for evaluating the ionization level between charge states q and q + 1 as the value of µe where the two formation energies are equal. This is a widely used technique for defects in semiconductors. It requires the accurate determination of the supercell total energies, and uses the valence-band maximum as the absolute reference energy (alternatively, the electron chemical potential can be measured from the conduction-band minimum). Although it makes no explicit reference to the eigenvalues of the Kohn–Sham gap states, the method can suﬀer from the DFT underestimation of the bandgap, especially if the state in question is far from the reference energy, close to the opposite band edge.

12 The Marker Method The problems of bandgap underestimation and valence-band alignment can to some extent be avoided in using the so-called marker method for calculating ionization-level positions [72]. Let us deﬁne the conﬁguration energy for a defect labeled d as the total energy diﬀerence per unit charge between two charge states

(20) Cd (q/q ) = Etot X q − Etot [X q ] (q − q ) . If there is a measured or otherwise accurately known reference (“marker”) defect m with the ionization level Em (p/p ) between charge states p and p in the region of interest in the semiconductor bandgap, one can calculate its conﬁguration energy Cm (p/p ) and the conﬁguration energy diﬀerence of d from the marker as Dd (q/q ) = Cd (q/q ) − Cm (p/p ) .

(21)

Then the ionization level of interest can be estimated as Ed (q/q ) ≈ Dd (q/q ) + Em (p/p ) .

(22)

Supercell Methods for Defect Calculations

51

The idea is to achieve systematic cancelation of computational errors. This happens best when the defects d and m are similar and all computational parameters are the same. The reference energy may also be taken as the valence-band maximum and the conduction-band bottom of the bulk supercell with the same number of atoms as the defect supercell, whereby bulk (0/ + 1) = Ev Cm

bulk and Cm (−1/0) = Ec ,

(23)

and the bandgap is bulk bulk Eg = Cm (−1/0) − Cm (0/ + 1) .

(24)

The marker method can provide a useful alternative for ionization-level determination, but requires the knowledge of a suitable known transition level in the vicinity of the level under scrutiny.

13 Brillouin-Zone Sampling For a perfect (no defects) lattice, the convergence of electronic properties can be achieved either by increasing the number of k points in the BZ or the product of the number of atoms (N ) in the calculational unit cell and the number of k points. The computational cost increases linearly with the number of k points but is proportional to at least N 3 . Thus increasing simply the number of k points would seem most economical. However, for defect calculations the spurious defect–defect interactions are a more subtle issue. For defects in metals already quite small supercells may give well-converged results if the number of k points is large enough. For defects in semiconductors the situation is more diﬃcult. Their description involves localized gap states. The description of these is not straightforwardly improved as the number of k points increases, i.e., the detailed choice of the k-point sampling may aﬀect the convergence. In supercell calculations, the evaluation of a ground-state property P of the system, such as total energy, requires integration over the Brillouin zone (BZ) of the reciprocal cell 1 3 d k pn (k)f [εn (k)] , (25) P = VBZ BZ n where VBZ is the volume of the BZ, n enumerates Kohn–Sham states with the wavevector k and eigenvalue εn (k), and pn deﬁnes the physical property. f [εn (k)] is the occupation number of the Kohn–Sham state, given by the Fermi–Dirac distribution around the chemical potential µe as 1

f [εn (k)] = e

µe −εn (k) kB T

. +1

(26)

52

Risto M. Nieminen

For semiconductors with a ﬁnite gap between occupied and unoccupied states, the integrand in (25) is continuous, and consequently the integral can, in principle, be replaced by a ﬁnite sampling of discrete k points. The computational cost increases linearly with the number of k points, and “special point” schemes are popular to reduce the computational cost to obtain the desired accuracy [73]. In particular, the uniform k-point mesh approach suggested by Monkhorst and Pack [74] has been widely used in practical calculations. For very large actual supercell sizes, the BZ shrinks towards a point (the Γ -point, the k = 0 of the BZ). Γ -point sampling oﬀers additional savings in computing as the Kohn–Sham wavefunctions are purely real at k = 0. The simplest scheme to sample the BZ in supercell calculations is to use the Γ point only. When the size of the supercell increases, the wavefunctions calculated correspond to several k points of the underlying perfect bulk lattice, and the perfect lattice k space is evenly sampled. In order to improve the description of, in particular, that of the delocalized bulk-like states and the description of the electron density, it is beneﬁcial to use k points other than the Γ point. Thereby also components with wavelengths larger than the supercell lattice constant are included. This idea leads to the special k-point schemes mentioned above. They are widely used to sample the BZ also in defect calculations. The accuracy of a given k-point mesh depends naturally on the supercell size (BZ volume). Makov et al. [75] utilized this fact to suggest sampling meshes that would in fact extrapolate the integration result towards larger unit-cell sizes. They proposed a scheme to choose k points for supercell calculations so that the electronic defect–defect interactions are minimized in the total energy. Defect calculations often focus on total-energy diﬀerences, and a tacit assumption is that errors due to BZ sampling largely cancel out when taking the diﬀerences (bulk vs. defect, for example) treated with equal-size supercells. This assumption is not a priori warranted and should be checked carefully. It has been demonstrated [76] that even for relatively large supercells the sampling errors can depend on the defect type and charge state and thus do not cancel when taking the diﬀerence. Shim et al. [76] investigated vacancy and interstitial defects in diamond and silicon, and found that for a given supercell size, the k-point sampling errors in the total energy can vary considerably depending on the charge state and defect type.

14 Charged Defects and Electrostatic Corrections Although the supercell approximation describes accurately and in an economical way the crucial local rearrangement of bonding between atoms and the underlying crystal structure, it also introduces artiﬁcial long-range interactions between the periodic images. The most dramatic artefact is the

Supercell Methods for Defect Calculations

53

divergence of the overall electrostatic (Coulomb) energy for charged defects in the periodic superlattice. This divergence of the total energy of charged defects in the supercell approximation is usually circumvented by the introduction of a ﬁctitious neutralizing background charge, often in the form of a uniform “jellium” distribution. The inﬂuence of this neutralizing charge in the total energy of the supercell needs to be included. This is known as the electrostatic or Madelung correction ∆Ec . With the neutralizing background added, in the large-supercell limit the electrostatic interaction of a charged defect with its periodic images in an overall neutralized system becomes, in principle, negligible. However, there is no guarantee that the convergence of the Coulomb energy as a function of the supercell size is particularly fast [77]. In fact, classical electrostatics for localized charges in an overall neutral system predicts an asymptotic L−1 √ 3 dependence, where L = V and V is the supercell volume. This scaling law is unfortunately slow in converging, and, moreover, its prefactor is in general unknown. Consequently, electrostatic errors are easily introduced into totalenergy calculations and they do not necessarily cancel when taking energy diﬀerences, as the magnitude depends on the details of the charge distribution within the supercell. Over the years, several attempts to reliably estimate ∆Ec have been proposed. Leslie and Gillan [78] and Payne and coworkers [79, 80] have developed correction formulae to be applied for electrostatic correction of charged-defect arrays. They considered an array of localized charges immersed in a structureless dielectric and neutralized by jellium compensation. By considering the multipole expansion of the defect charge distribution, the correction formula can be derived in the form ∆Ec ≈ −

2πqQ q2α − + O(L−5 ) , 2εL 3εL3

(27)

where q is the charge of the defect, α the Madelung constant of the superlattice, and ε the static dielectric constant of the host material. For cubic geometries, α is 2.837 3, 2.888 3 and 2.885 for SC, BCC and FCC supercells, respectively. The ﬁrst term corresponds to a point-charge array and a compensating background in a uniform dielectric. The second term in the right-hand side of (27) arises from the shapedependent interaction charge distribution inside the supercell with the neutralizing background. The parameter Q is the second radial moment of the defect charge density (28) Q = d3 rr2 [ρd (r) − ρb (r)] . Kantorovich [81] re-examined the method for arbitrary supercell shapes, and suggested a modiﬁed formula ignoring dipole–dipole interactions.

54

Risto M. Nieminen

There is obvious ambiguity in this correction scheme. First, the static dielectric constant is introduced as an external parameter and is not consistently deﬁned. Secondly, the correction scheme is derived assuming that the charge perturbation introduced by the defect is well localized within the supercell. This is strictly speaking not valid, as in classical theory the polarization and thus the aperiodic screening charge distribution extend over the whole macroscopic crystal. Thus, as described in detail by Lento et al. [82], Q depends on the size of the supercell and (27) does not lead to a well-deﬁned correction value. Nevertheless, (27), often known as the Makov–Payne formula, is popular in estimations of electrostatic corrections. Segev and Wei [83] showed that for charges with a Gaussian distribution with a certain width σ interacting with the background, the Madelung correction should vanish as σ becomes large. Moreover, situations may arise where local symmetry-breaking distortions in fact induce a net dipole in the supercell. Dipole contributions cannot be discarded in such a situation, as they do not cancel in the total-energy diﬀerences between perfect and defected supercells. Shim et al. [84] have systematically studied the behavior of the electrostatic correction for supercells of diﬀerent sizes for vacancy and interstitial defects in diamond. For negatively charged vacancies and positively charged interstitials, the formation energies show a clear dependence on the supercell size and are in qualitative agreement with the Makov–Payne trend. For positively charged vacancies and negatively charged interstitials, the electrostatic corrections are weak. An analysis of the spatial charge density distributions reveals that these large variations in electrostatic terms with defect type originate from diﬀerences in the screening of the defect-localized charge. A strongly localized charge is close to the point-ion model, whereas delocalized defect states spread out and result in weak Madelung corrections. To convince oneself of the proper elimination of the spurious electrostatic energy, one should, in the general case, carry out a proper scaling analysis of the L−1 behavior and extrapolate to the inﬁnite-L limit. Another approach is based on ﬁtting a multicenter Gaussian distribution to the defect charge density, and calculating and subtracting explicitly the electrostatic interactions between the Gaussian distributions and the background. This approach has so far only been used for charged molecules in vacuum [85], but it may be possible to generalize to defect supercells with aperiodic densities. A diﬀerent route to the electrostatic correction for charged defects was taken by Schultz [86], based again on the linearity of the Poisson equation but avoiding the neutralizing homogeneous background. An aperiodic defect charge distribution ρLM (r) is constructed so that it matches the electrostatic moments of the system up to a given order. When this charge density is separated from the supercell charge distribution, the remaining periodic distribution has zero net charge and is momentless. Thus, its electrostatic energy can be accurately calculated within the periodic boundary conditions. The

Supercell Methods for Defect Calculations

55

Coulomb energy of ρLM (r) is calculated using “cluster boundary conditions”, with the surrounding polarizable, defect-free crystal replaced by perfect, nonpolarizable bulk crystal. There is no analytical formula similar to (27) for this local-moment counter-charge (LMCC) method. Its main content is to use periodic boundary conditions to solve the Kohn–Sham equations but not for the Poisson equation. One can then calculate the electrostatic energy of a single defect-containing supercell surrounded by cells with the perfect crystal charge density. In order to correctly align the arbitrarily referenced potentials, Schultz [87] has suggested a method where a common reference potential can be calculated for all types of defects and also for the valence-band edge of the perfect crystal. The LMCC method should, in principle, lead to a rigorous 1/L convergence of the supercell energy, with a prefactor proportional to (1 − ε−1 )q 2 . This method does not need a compensating background, and there are no interactions between the defect charge and its periodic images. It also provides a way to deﬁne a reference energy independent of the defect charge state for aligning the band edges. The implementation of the LMCC method would thus seem very much worth the eﬀort for calculations of charged defects.

15 Energy-Level References and Valence-Band Alignment As is obvious from (13), another important parameter for supercell-based total-energy calculations is the position of the valence-band maximum (VBM), Ev , which is usually taken as the reference energy for the electron chemical potential. The position of the VBM of the defect-containing supercell is diﬀerent from that of the defect-free supercell, and this diﬀerence depends, in general, on the charge state of the defect. Consequently, a valence-band alignment (VBA) correction is usually applied by matching the two values. The magnitude of this correction is eﬀ eﬀ − Vdefect , (29) ∆EVBA = Vbulk where V eﬀ is the eﬀective Kohn–Sham potential and the brackets denote averaging over the bulk and defect supercells, respectively. Other potential-energy references are naturally possible. One possibility is to align an electronic core or semicore level energy (in all-electron calculations), or deﬁne all energies with respect to the so-called crystal zero, the potential energy at the surface of a neutral Wigner–Seitz cell. This choice is particularly simple and useful when using the atomic-sphere approximation (ASA), for example in the context of the linear-muﬃn-tin-orbital (LMTO) method.

56

Risto M. Nieminen

16 Examples: The Monovacancy and Substitutional Copper in Silicon The literature on supercell calculations of defects in semiconductors is vast and not even a partial review is attempted here. Instead, we discuss in more detail a recent systematic case study, where the practical implementations of two popular approaches were critically examined. The study involves the prototypical (but far from trivial) point defects in Si, the monovacancy VSi and substitutional copper CuSi . The fundamental nature of VSi means that it is a much-studied defect. It has four unpaired electrons, and in a simple LCAO picture they occupy four orbitals in the atoms surrounding the vacancy in the diamond structure [66]. These induce electronic states in the gap, which are modiﬁed by symmetrylowering structural distortions driven by the Jahn–Teller eﬀect. A comprehensive study of the convergence of the formation energy of the neutral silicon vacancy as a function of the supercell size has been given by Puska et al. [18] (see also [88]). The result is shown in Fig. 5. It turns out that very large supercells are necessary for proper convergence of the vacancy formation energy, and that the relaxation pattern around the vacancy undergoes a qualitative change (from outward to inward relaxation) as the supercell size grows. This is also shown by calculations for large ﬁnite clusters [19]. The total-energy hypersurface is ﬂat, especially for negatively charged defects, which makes the unambiguous determination of the point symmetry diﬃcult. This is also reﬂected in the diﬃculty of determining the ionization levels accurately. This will now be discussed for both VSi and CuSi . CuSi has a similar structure to VSi : the vacancy is perturbed by the Cu 3d states that lie in the valence band. The Jahn–Teller theorem predicts that CuSi should undergo a symmetry-lowering distortion with magnitude constrained by the presence of the metal atom. Spin-orbit coupling eﬀects may also reduce the amount of distortion by lifting the orbital degeneracy. 16.1 Experiments The greater structural freedom of VSi introduces another possible (and often encountered) complication. The total energy gained by pairing electrons in dangling bonds, associated with a structural distortion, can outweigh their mutual Coulomb repulsion. This is the famous “negative” eﬀective-U phenomenon, which leads to unexpected ordering of the ionization levels in the bandgap. In the case of VSi the pairing for the neutral defect is much stronger than for the singly positive +1 state, which shifts the ionization (donor) level Ed (0/ + 1) below that for the second donor Ed (+1/ + 2). Thus the singly positive silicon vacancy is a metastable state, a fact conﬁrmed with DLTS and EPR measurements by Watkins and Troxell [89]. The energy position measured in these experiments gives for the double donor level + the value Ed (+1/ + 2) ≈ Ev + 0.13 eV, while EPR studies show that VSi

Supercell Methods for Defect Calculations

57

Fig. 5. Formation energy of the neutral vacancy in Si. The supercell size (number of atoms) is given on the top of each panel, and the k-point set used for Brillouin-zone sampling is indicated as 1 = Γ , 2 = 23 , 3 = 33 , 4 = (1/4, 1/4, 1/4) and 5 = Γ + L. From [18]

ionized by photoexcitation decays to the neutral state from a donor level at Ed (0/ + 1) ≈ Ev + 0.05 eV. EPR studies together with stress-alignment experiments also demonstrate that the Jahn–Teller eﬀect causes structural distortions in accord with a straightforward one-electron model. This model predicts that the neutral and positively charged defects have D2d symmetry, while the negative charge states have C2v symmetry. The energies of the acceptor levels Ed (−1/0) and Ed (−2/ − 1) are experimentally unknown. For CuSi , there are accurate experimental values [90, 91] for its ionization levels and thus it provides a good testing ground for theory and computation, even if experimental structural information is lacking. The defect has a single donor level at Ed (0/ + 1) ≈ Ev + 0.207 eV, an acceptor level Ed (−1/0) at ≈ Ev + 0.478 eV ≈ Ec − 0.69 eV, and a double acceptor at Ed (−2/ − 1) at Ec − 0.167 eV. The Jahn–Teller distortions for VSi and CuSi (and more generally substitutional transition-metal impurities in Si) possess two components. The main one is tetragonal in character and gives the defects D2d symmetry. The direction of this distortion may occur in two senses, and this determines the relative energetic ordering of the resulting electronic states. The two senses correspond to two diﬀerent shapes for the bounding box with {100} faces that contains the four atoms surrounding the center: one is short and broad

58

Risto M. Nieminen

while the other is long and thin. They correspond to diﬀerent relative lengths for the six Si–Si distances between these four atoms. For the D2d point group, four of the distances belong to one equivalent set and two belong to the second equivalent set. One type of distortion (type A) has the pair longer than the four, and for the other (type B) it is the other way round. Type A splits the t2 state into a singlet a1 state above the doublet e state, while type B does the opposite. Transition-metal impurities relax in the A pattern, and monovacancies in Si relax in the opposite sense, B. When the system contains suﬃcient electrons to occupy the e state, a weaker trigonal distortion is expected. It lowers the symmetry to C2v . The equivalent pair of Si–Si lengths in the D2d case become unequal. This splits the e state into orbitals of b1 and b2 character. Spin-orbit coupling may also aﬀect the splitting of these states for transition-metal impurities [92]. 16.2 Calculations In a recent study, Latham et al. [93] carried out a systematic quantitative study of the electrical levels and associated structural relaxations of VSi and CuSi . To conduct the study, two diﬀerent computer programs, AIMPRO [94] and VASP [95, 96] were used. The former uses localized Gaussian orbitals as the basis set for the Kohn–Sham wavefunctions, while the charge density is expanded in plane waves. VASP uses plane waves throughout. In AIMPRO, the core electrons of atoms are represented by pseudopotentials constructed according to the Hartwigsen–Goedecker–H¨ utter (HGH) normconserving scheme [45]. The VASP package includes pseudopotentials based on the Vanderbilt ultrasoft [46] construction or, alternatively, the projectedaugmented-wave (PAW) method [48]. The Cu 3d electrons are included explicitly in the HGH and PAW schemes, while they are not in the Vanderbilt pseudopotential. In both methods, the exchange-correlation energy is evaluated using the LSDA formula described by Perdew and Wang [97]. Unit cells of 216 atoms are used in all cases, and the supercell band structure is sampled by using the Monkhorst–Pack scheme with 23 k points, folded according to the symmetry of the system and shifted to avoid the Γ point. This enables the total energy convergence of better than 10−4 eV per supercell, with the plane-wave kinetic energy cutoﬀs chosen to meet this requirement (in AIMPRO the Coulomb energy is evaluated also using the plane-wave expansion). The actual value of the cutoﬀ depends on the atoms present and the chosen pseudopotential. For charged defects, a compensating background charge is introduced as discussed in Sect. 13, and a ﬁnite-size scaling is performed. For bulk Si, both methods reproduce the lattice parameter a and the bulk modulus B0 well (see Table 1). The calculation of the bandgap Eg is a deﬁciency of LSDA-DFT formalism, as discussed above. The two methods give similar values, Eg (AIMPRO) = 0.71 while Eg (VASP) = 0.60 eV. The

Supercell Methods for Defect Calculations

59

VASP results do not depend on whether the core electrons are treated by the ultrasoft pseudopotential or PAW. Table 1. Calculated and measured values for the lattice parameter a and the bulk modulus B0 of Si Method

a (˚ A) B0 (GPa)

AIMPRO+HGH VASP+VUS VASP+PAW Experiment

5.395 5.390 5.403 5.431

97.0 87.7 72.8 97.9

All the defect electron levels considered here are suﬃciently deep so that the energies of donors can be given with respect to Ec and acceptors with respect to Ev . As reference (marker) energies Latham et al. choose addition/removal energies of ideal Si supercells with the same size (216 atoms) as used for the defect calculations. This means that the energy levels are referenced to the nearest ideal-crystal band edge (i.e., the marker method with respect to the two band edges). None of the studied defects are so shallow that their energy would be between the theoretical and true bandgap. If this were the case, it would be necessary to use the opposite ideal-crystal band edge as the reference potential. A summary of the calculated electrical levels, compared with experimental data, is presented in Table 2. Table 2. Calculated and measured electrical levels [93] for VSi and CuSi Transition AIMPRO VASP state VUS VSi VSi VSi VSi VSi VSi CuSi CuSi CuSi

0/+2 +1/+2 0/+1 −1/0 −2/−1 −2/0 0/+1 −1/0 −2/−1

Ev + 0.0 Ev + 0.05 Ev − 0.04 Ec − 0.31 Ec − 0.43 Ec − 0.37 Ev + 0.17 Ec − 0.50 Ec − 0.24

VASP PAW

Ev + 0.06 Ev + 0.11 Ev + 0.02 Ec − 0.34 Ec − 0.23 Ec − 0.29 Ev + 0.07 Ev + 0.17 Ec − 0.45 Ec − 0.34 Ec − 0.18 Ec − 0.26

[15]

Expt. [66, 90, 91]

Ev + 0.15 Ev + 0.19 Ev + 0.11 Ec − 0.57 Ec − 0.40 Ec − 0.49

Ev + 0.09 Ev + 0.13 Ev + 0.05 exists exists Ev + 0.21 Ec − 0.69 Ec − 0.17

When both program packages are set to use similar thresholds in terms of energies and forces to decide structural optimization, the outcome shows some diﬀerences. The AIMPRO package ﬁnds that the direction of the main tetragonal distortion (D2d symmetry) is in the expected direction, type B

60

Risto M. Nieminen

for VSi and type A for CuSi . The VASP package also ﬁnds type B D2d for neutral VSi . VASP yields type A D2d distortion for CuSi when the Vanderbilt pseudopotential is used, but no signiﬁcant deviation from the perfect Td symmetry when PAW is used. Both methods give equal energies for the (0/ + 1) level of CuSi . Regardless of constraint choice, no clear evidence is seen for the expected trigonal component of the distortion of CuSi . The situation is more complex for VSi . While the optimized structure in positive and neutral charge states has D2d symmetry as expected, the unconstrained lowest-energy structure is a D3d symmetry “split-vacancy” conﬁguration. The split-vacancy conﬁguration is one where a Si atom is located between two unoccupied lattice sites, and is 0.04 eV lower in energy than the ideal Td monovacancy. This result for negatively charged vacancies was also found by Puska et al. [18]. According to Latham et al., the energy diﬀerences between the C2v and C3v conﬁgurations of VSi in the q = −1 and q = −2 charge states are 0.02 eV and 0.20 eV, respectively. This means that VSi in the C3v symmetry is calculated to have a negative-U behavior also for the acceptor levels. Little is presently known from experiment about the negative charge states other than that they apparently exist. The calculated energy for the (−1/0) acceptor level of CuSi near midgap is somewhat deeper than the measured value, while the second acceptor is shallower. The Jahn–Teller eﬀect moves these levels apart, moving each by 0.1 eV. Thus, the calculations seem to slightly underestimate the magnitude of the Jahn–Teller eﬀect. It is reasonable to suppose that a similar pattern will be found for the acceptor states of VSi if they can be measured, and the expected C2v model without a negative-U eﬀect would prevail.

17 Summary and Conclusions Calculations based on the density-functional theory and the supercell method enable quantitative estimates for the formation energies, diﬀusion barriers, structural parameters and electrical levels of defects in semiconductors. Moreover, vibrational entropies and free energies can be estimated from the calculated force ﬁelds, which also enable ﬁrst-principles molecular dynamics simulations. It is also possible to feed the ﬁrst-principles results for migration and reaction barriers into kinetic Monte Carlo simulations based on master equations. This opens up the possibility for multiscale simulations of annealing kinetics and related phenomena. Quantitatively accurate total-energy calculations open the way to ﬁrst-principles thermodynamics and kinetics. However, reaching the desired quantitative accuracy in the total-energy calculations is not always straightforward, and requires careful consideration of several possible sources of error. In particular, the positioning of defectrelated electronic levels in the fundamental semiconducting gap can be quite problematic. The sources of errors may be divided into three main categories.

Supercell Methods for Defect Calculations

61

One is the underlying theory, especially the treatment of electronic exchange and correlation. Local and semilocal approximations do not properly describe the discontinuity of the corresponding density functional, which contributes to the underestimation of the fundamental gap. The second source of error are the ﬁnite-size eﬀects inherent in the supercell method, which need proper scaling analysis as a function of the cell size. These errors include the spurious defect–defect interaction, dispersion of defect-related electronic states, incomplete sampling of the reciprocal cell, and the constrained relaxation of atoms around the defect. The third source of errors are the approximations required to construct a speciﬁc implementation, including the pseudopotential generation, basis-set construction, and numerical accuracy of the algorithms. The power of the density-functional methods is considerable in revealing and rationalizing the systematic trends in electronic and structural properties of defects in semiconductors. These include the nature (acceptor or donor) of the deep levels, their spin structure, point symmetry, and energetics. They can also predict the localized vibrational modes associated with defects, and provide the starting point (for example, the ground-state electron density) for quantitative calculations of many experimentally observed characterizing signals (such as positron-annihilation parameters). Total-energy calculations also reveal the details of the potential-energy hypersurfaces for defects moving in the lattice, which makes it possible to study the long-time kinetics by using Monte Carlo techniques. Quantitatively accurate supercell calculations for defects in semiconductors are notoriously diﬃcult and demand considerable computational resources. While many confusing and seemingly contradictory results have been published in the scientiﬁc literature, the available computational methods have steadily matured. With the increase of computer power available for such calculations, it is now possible to perform well-benchmarked calculations with considerable predictive power. Acknowledgements I have beneﬁted from several useful discussions with Chris Latham and Maria Ganchenkova. This work has been supported by the Academy of Finland through the Center of Excellence Grant (2000–2005).

References [1] J. Bourgoin, M. Lannoo: Point Defects in Semiconductors II. Experimental Aspects, vol. 35, Springer Series in Solid State Sciences (Springer, Berlin, Heidelberg 1983) 29 [2] R. M. Nieminen: J. Phys.: Condens. Matter 14, 2859 (2002) 30 [3] W. Kohn, L. J. Sham: Phys. Rev. 136, B864 (1964) 30 [4] R. Martin: Electronic Structure: Basic Theory and Practical Methods (Cambridge University Press, Cambridge 2004) 30

62

Risto M. Nieminen

[5] A. E. Mattsson, P. A. Schultz, M. P. Desjarlais, T. R. Mattsson, K. Leung: Modelling Simul. Mater. Sci. Eng. 13, R1 (2005) 32 [6] M. J. Puska, R. M. Nieminen: Rev. Mod. Phys. 66, 841 (1994) 32 [7] C. G. van de Walle, P. E. Bl¨ ochl: Phys. Rev. B 47, 4244 (1993) 32 [8] C. J. Pickard, F. Mauri: Phys. Rev. B 63, 245101 (2001) 32 [9] C. J. Pickard, F. Mauri: Phys. Rev. Lett. 88, 086403 (2002) 32 [10] R. P. Messmer, G. D. Watkins: Phys. Rev. Lett. 25, 656 (1970) 33 ¨ [11] S. Ogut, H. Kim, J. R. Chelikowsky: Phys. Rev. B 56, R11353 (1997) 33 [12] G. Baraﬀ, M. Schl¨ uter: Phys. Rev. B 19, 4965 (1979) 33 [13] O. Gunnarsson, O. Jepsen, O. K. Andersen: Phys. Rev. 27, 7144 (1983) 33 [14] M. J. Puska, O. Jepsen, O. Gunnarsson, R. M. Nieminen: Phys. Rev. B 34, 2695 (1986) 33 [15] S. K. Estreicher, D. S. Marinyck: Phys. Rev. Lett. 56, 1511 (1986) 33, 59 [16] S. B. Zhang, J. E. Northrup: Phys. Rev. Lett. 67, 2339 (1991) 34, 49 [17] H. Dreyss´e (Ed.): Electronic Structure and Physical Properties of Solids. The Uses of the LMTO Method, Lecture Notes in Physics (Springer, Berlin, Heidelberg 2000) 35 [18] M. J. Puska, S. P¨ oykk¨ o, M. Pesola, R. M. Nieminen: Phys. Rev. B 58, 1318 (1998) 35, 36, 56, 57, 60 ¨ [19] S. Ogut, J. R. Chelikowsky: Phys. Rev. B 64, 245206 (2001) 35, 56 [20] K. Laaksonen, H. P. Komsa, E. Arola, T. T. Rantala, R. M. Nieminen: Phys. Rev. B in press 37 [21] M. St¨ adele, J. A. Majewski, P. Vogl, A. G¨ orling: Phys. Rev. Lett. 79, 2089 (1997) 37 orling: Phys. Rev. B [22] M. St¨ adele, M. Moukara, J. A. Majewski, P. Vogl, A. G¨ 59, 10031 (1999) 37 [23] R. J. Magyar, A. Flezsar, E. K. U. Gross: Phys. Rev. B 69, 045111 (2004) 37 [24] D. Vogel, P. Kr¨ uger, J. Pollmann: Phys. Rev. B 54, 5495 (1996) 37 [25] S. Sharma, J. K. Dewhurst, C. Ambrosch-Draxl: Phys. Rev. Lett. 95, 136402 (2005) 37 [26] A. Seidl, A. G¨ orling, P. Vogl, J. A. Majewski, M. Levy: Phys. Rev. B 53, 3764 (1996) 38 [27] J. Lento, R. M. Nieminen: J. Phys.: Condens. Matter 15, 4387 (2003) 38 [28] M. S. Hybertsen, S. G. Louie: Phys. Rev. B 34, 5390 (1986) 38 [29] S. Ismail-Beigi, S. G. Louie: Phys. Rev. Lett. 95, 156401 (2005) 38 [30] J. Laegsgaard, K. Stokbro: Phys. Rev. Lett. 86, 2834 (2001) 38 [31] M. d’Aveszac, M. Calandra, F. Mauri: Phys. Rev. B 71, 205210 (2005) 39 [32] J. Perdew, A. Zunger: Phys. Rev. B 23, 5048 (1981) 39 [33] A. Svane, O. Gunnarsson: Phys. Rev. B 37, 9919 (1988) 39 [34] L. Hedin: Phys. Rev. 139, A796 (1965) 39 [35] G. Onida, L. Reining, A. Rubio: Rev. Mod. Phys. 74, 601 (2002) 39 [36] M. Rohlﬁng, S. G. Louie: Phys. Rev. B 62, 4927 (2000) 39 [37] A. Janotti, C. G. van de Walle: Appl. Phys. Lett. 87, 122102 (2005) 40 [38] S. Lang, A. Zunger: Phys. Rev. B 72, 035215 (2005) 40 [39] V. I. Anisimov, F. Aryasetiawan, A. I. Liechtenstein: J. Phys.: Condens. Matter 9, 767 (1997) 40 [40] W. K. Leung, R. J. Needs, G. Rajagopal, S. Itoh, S. Ihara: Phys. Rev. Lett. 83, 2351 (1999) 40

Supercell Methods for Defect Calculations

63

[41] R. Q. Hood, P. R. C. Kent, R. J. Needs, P. R. Briddon: Phys. Rev. Lett. 91, 076403 (2003) 40 [42] C. G. Van de Walle, J. Neugebauer: J. Appl. Phys. 95, 3851 (2004) 40 [43] D. R. Hamann: Phys. Rev. B 40, 2980 (1989) 41 [44] N. Troullier, J. L. Martins: Phys. Rev. B 43, 1993 (1991) 41 [45] C. Hartwigsen, S. Goedecker, J. H¨ utter: Phys. Rev. B 58, 3641 (1998) 41, 58 [46] D. Vanderbilt: Phys. Rev. B 41, 7892 (1990) 41, 58 [47] L. Kleinman, D. M. Bylander: Phys. Rev. Lett. 48, 1425 (1982) 41 [48] P. E. Bl¨ ochl: Phys. Rev. B 50, 17953 (1994) 41, 58 [49] G. Kresse, D. Joubert: Phys. Rev. B 59, 1758 (1999) 41 [50] S. G. Louie, S. Froyen, M. L. Cohen: Phys. Rev. B 26, 1738 (1982) 41 [51] D. Porezag, M. R. Pederson, A. V. Liu: Phys. Rev. B 60, 14132 (1999) 41 [52] D. Vogel, P. Kr¨ uger, J. Pollmann: Phys. Rev. B 55, 12836 (1997) 41 [53] M. Fuchs, M. Bockstedte, E. Pehlke, M. Scheﬄer: Phys. Rev. B 57, 2134 (1998) 42 [54] P. Ordejon, E. Artacho, J. M. Soler: Phys. Rev. B 53, R10441 (1995) 42 [55] J. M. Soler, E. Artacho, J. D. Gale, A. Garcia, J. Junquera, P. Ordej´ on, D. Sanchez-Portal: J. Phys.: Condens. Matter 14, 2745 (2002) 42 [56] O. Treutler, R. Ahlrichs: J. Chem. Phys. 102, 346 (1995) 42 [57] T. L. Beck: Rev. Mod. Phys. 72, 1041 (2000) 43 [58] M. Heiskanen, T. Torsti, M. J. Puska, R. M. Nieminen: Phys. Rev. B 63, 245106 (2001) 43 [59] S. Nos´e: J. Chem. Phys. 81, 511 (1984) 43 [60] G. H. Hoover: Phys. Rev. A 31, 1695 (1985) 43 [61] M. Parrinello, A. Rahman: J. Appl. Phys. 52, 7182 (1980) 44 [62] E. Runge, E. K. U. Gross: Phys. Rev. Lett. 52, 997 (1984) 44 [63] M. Petersilka, U. J. Gossmann, E. K. U. Gross: Phys. Rev. Lett. 76, 1212 (1996) 44 [64] G. Vignale, W. Kohn: Phys. Rev. Lett. 77, 2037 (1996) 44 [65] H. A. Jahn, E. Teller: Proc. Roy. Soc. A 161, 220 (1937) 45 [66] G. D. Watkins: The Lattice Vacancy in Silicon (Gordon and Breach, Yverdon 1992) 45, 56, 59 [67] G. Baraﬀ, E. O. Kane, M. Schl¨ uter: Phys. Rev. Lett. 43, 956 (1979) 46 [68] G. D. Watkins: Physica B 117–118, 9 (1983) 46 [69] L. Torpo, R. M. Nieminen, S. P¨ oykk¨ o, K. Laasonen: Appl. Phys. Lett. 74, 221 (1999) 46 [70] S. Baroni, S. de Gironcoli, A. Dal Corso: Rev. Mod. Phys. 73, 515 (2001) 47 [71] J. M. Pruneda, S. K. Estreicher, J. Junquera, J. Ferrer, P. Ordejon: Phys. Rev. B 65, 075210 (2002) 47 [72] J. Coutinho, V. J. B. Torres, R. Jones, P. R. Briddon: Phys. Rev. B 67, 035205 (2003) 50 [73] D. J. Chadi, M. L. Cohen: Phys. Rev. B 8, 5747 (1973) 52 [74] H. J. Monkhorst, J. D. Pack: Phys. Rev. B 13, 5188 (1976) 52 [75] G. Makov, R. Shah, M. C. Payne: Phys. Rev. B 53, 15513 (1996) 52 [76] J. Shim, E.-K. Lee, Y. J. Lee, R. M. Nieminen: Phys. Rev. B 71, 035206 (2005) 52 [77] S. W. de Leeuw, J. W. Perram, E. R. Smith: Proc. Roy. Soc. London, Ser. A 373, 27 (1980) 53 [78] M. Leslie, M. J. Gillan: J. Phys. C 18, 973 (1985) 53

64

Risto M. Nieminen

[79] G. Makov, M. C. Payne: Phys. Rev. B 51, 4014 (1995) 53 [80] M. R. Jarvis, I. D. White, R. W. Godby, M. C. Payne: Phys. Rev. B 56, 14972 (1997) 53 [81] L. N. Kantorovich: Phys. Rev. B 60, 15476 (1999) 53 [82] J. Lento, J.-L. Mozos, R. M. Nieminen: J. Phys.: Condens. Matter 14, 2637 (2002) 54 [83] D. Segev, S. H. Wei: Phys. Rev. Lett. 91, 126406 (2003) 54 [84] J. Shim, E.-K. Lee, Y. J. Lee, R. M. Nieminen: Phys. Rev. B 71, 245204 (2005) 54 [85] P. Bl¨ ochl: J. Chem. Phys. 103, 7482 (1995) 54 [86] P. A. Schultz: Phys. Rev. B 60, 1551 (1999) 54 [87] P. A. Schultz: Phys. Rev. Lett. 84, 1942 (2000) 55 [88] D. A. Drabold, J. D. Dow, P. A. Fedders, A. E. Carlsson, O. F. Sankey: Phys. Rev. B 42, 5345 (1990) 56 [89] G. D. Watkins, J. R. Troxell: Phys. Rev. Lett. 44, 593 (1980) 56 [90] S. Knack, J. Weber, H. Lemke: Physica B 273–274, 387 (1999) 57, 59 [91] S. Knack, J. Weber, H. Lemke, H. Riemann: Phys. Rev. B 65, 165203 (2002) 57, 59 [92] G. D. Watkins, P. M. Williams: Phys. Rev. B 52, 16575 (1995) 58 [93] C. D. Latham, M. Ganchenkova, R. M. Nieminen, S. Nicolaysen, M. Alatalo, ¨ S. Oberg, P. R. Briddon: Phys. Scr. T126, 61 (2006) 58, 59 ¨ [94] J. Coutinho, R. Jones, P. R. Briddon, S. Oberg: Phys. Rev. B 62, 10824 (2000) 58 [95] G. Kresse, J. Furthm¨ uller: Comp. Mater. Sci. 6, 15 (1996) 58 [96] G. Kresse, J. Furthm¨ uller: Phys. Rev. B 54, 11169 (1996) 58 [97] J. P. Perdew, Y. Wang: Phys. Rev. B 46, 12947 (1992) 58

Index Γ point, 34, 52, 58 absorption, 44, 49 acceptor, 34, 40, 57, 59–61 AIMPRO, 58, 59 algorithm, 43, 44, 61 alignment, 35, 49, 50, 55, 57 all-electron, 41, 55 amorphous, 43 anharmonic, 48 annealing, 60 atomic-sphere approximation, 35, 55 autocorrelation function, 48 background charge, 35, 53, 58 band edge, 30, 35, 40, 49, 50, 55, 59 band structure, 38, 41, 58 bandwidth, 34

basis set, 32, 34, 39, 42, 43, 47, 58, 61 Bethe–Salpeter, 39 Born–Oppenheimer, 42, 43 Brillouin zone, 34, 35, 38, 51, 52 bulk, 36, 41, 47, 49, 50, 52, 55, 58 canonical, 43 charge delocalization, 39 charge state, 30, 34, 38, 46–50, 52, 55, 57, 60 charged defect, 35, 53–58 chemical potential, 36, 49–51, 55 classical, 53, 54 cluster, 32, 33, 35, 36, 55, 56 concentration, 36, 48 conduction band, 35, 38, 40, 50, 51 conductivity, 30, 49 core, 35, 37, 41, 55, 58, 59

Supercell Methods for Defect Calculations core radius, 41 core-valence, 37, 41 correlation, 31, 32, 37–40, 61 Coulomb, 35, 39, 40, 46, 53, 55, 56, 58 coupling, 46, 48, 56, 58 covalent, 35 cutoﬀ, 36, 42, 58 dangling bond, 56 decay, 57 deep level, 34, 61 deep-level transient spectroscopy, 29 defect band, 34, 35 degeneracy, 30, 44–46, 56 delocalization, 39 delocalized, 39, 52, 54 density of states, 37, 48 density-functional theory, 30, 31, 44, 60 DFT, 30–33, 36–38, 40, 42, 45, 47, 50, 58 diamond, 40, 46, 52, 54, 56 diﬀusion, 29, 60 dipole, 53, 54 dislocation, 33 disorder, 43 dispersion, 35, 38, 47, 61 distortion, 30, 45, 46, 54, 56–60 DLTS, 30, 49, 56 donor, 34, 40, 56, 57, 59, 61 doping, 30 double-zeta, 43 dynamical matrix, 48 DZP, 43 eigenvalues, 36, 39, 50 electrical level, 58–60 electron, 30, 31, 33, 36, 40, 41, 45–47, 56, 58, 59 electron aﬃnity, 36 electron states, 32, 38 electron-nuclear double resonance, 30 electrostatic energy, 54, 55 embedding, 32, 33 emission, 49 ENDOR, 30, 38 energetics, 29, 30, 32, 34, 61 energy cutoﬀ, 42, 58 energy level, 30, 34, 49, 59 entropy, 48

65

EPR, 30, 56, 57 equilibrium, 30, 43, 47–49 ergodic, 44 exact exchange, 37, 38 exchange, 31, 32, 37–40, 49, 61 exchange-correlation, 31, 32, 36, 39, 42, 44, 58 excitation, 32, 38, 39, 44, 49, 57 excited state, 34, 38 exciton, 38 fast Fourier transform, 41 Fermi level, 30, 36, 37, 45, 49 Fermi–Dirac, 51 ﬁnite diﬀerence, 43, 48 ﬁnite element, 43 ﬁrst principles, 32, 42, 43, 60 ﬂoating orbitals, 43 force, 32–34, 36, 40, 42, 43, 48, 59, 60 formation energy, 32, 40, 48, 49, 56 Fourier, 34, 48 free energy, 44, 60 frozen phonon, 48 fundamental gap, 34, 36, 45, 61 gap, 30, 31, 35–38 gap levels, 30 gap states, 30, 35, 45, 46, 50 Gaussian, 42, 54, 58 general gradient approximation, 32, 37 GGA, 32, 37–39, 42 ghost, 41 Green’s function, 33, 34, 36 ground state, 30, 32, 34, 36, 47–49, 51, 61 GW, 38, 39 Hall conductivity, 30 Hamiltonian, 44 Hartree, 31 Hartree–Fock, 32, 37–39 Hedin, 39 Hellmann–Feynman, 32, 36, 48 Helmholtz, 44 hole, 39 hybrid, 32, 37, 38 hyperﬁne, 32–34, 39 impurity, 30, 36, 45, 46, 48, 49 interstitial, 52, 54

66

Risto M. Nieminen

Jahn–Teller, 44–46, 56, 57, 60 jellium, 53

potential, 32, 34–37, 41, 42, 44, 45, 49–51, 55, 59, 61 projected augmented wave, 41, 58 pseudopotential, 40–42, 58, 60, 61

Kohn–Sham, 31, 32, 34–39, 42, 44, 50–52, 55, 58

quantum Monte Carlo, 40 quasiparticle, 38

LCAO, 56 LDA, 37–40, 42 LDA+U , 40 liquid, 43 localization, 30 LSDA, 32, 37, 58

real space, 42, 43 reciprocal space, 32, 34, 42 recombination, 34 relativistic, 32 relaxation, 33, 35, 36, 45, 58 repulsive, 45 resonance, 29, 38, 45

ionization, 34–36, 38, 41, 49, 50, 56, 57

Madelung, 53, 54 Makov–Payne, 54 marker, 50, 51, 59 microcanonical, 43 midgap, 60 migration, 29, 34, 42, 60 minimal basis, 35 molecular dynamics, 42–44, 60 multipole, 53 multiscale, 60 negative-U , 60 Newton, 43 nonlocal, 32, 37, 38 normal mode, 48 optical, 30, 34, 39, 40, 49 oxygen, 39, 40 pairing, 46, 56 Pauli, 32, 40 Perdew–Wang, 58 periodic, 33–36, 52–55 periodic boundary conditions, 33, 34, 43, 44, 54, 55 periodicity, 34 perturbation, 44, 54 phonon, 47, 48 photoluminescence, 30 PL, 30 plane wave, 34, 39, 41–43, 58 point defect, 30, 33, 35, 56 Poisson, 54, 55 polarization, 43, 54 positron annihilation, 29, 32, 34, 61

Schr¨ odinger, 31, 44 scissor, 39 screened exchange, 32, 38 screening, 38, 54 self-interaction, 31, 37, 39, 41 self-interstitial, 40 self-trapped, 38 semicore, 42, 55 shallow, 49, 59, 60 Si, 38–40, 45, 46, 56–60 silicon, 35, 36, 46, 52, 56 Slater, 40 special point, 52 spin, 29, 30, 32, 37, 39, 41, 46, 61 spin-orbit, 46, 56, 58 split-vacancy, 60 statistical, 43 stoichiometry, 34, 49 Stokes, 49 strain, 35, 43 stress, 35, 42, 57 substitutional, 38, 45, 46, 56, 57 supercell, 31–36, 38–40, 43–56, 58–61 surface, 33, 36, 42, 43, 55, 61 symmetry, 30, 35, 38, 44–46, 56, 57, 59, 60 symmetry breaking, 30, 54 Taylor, 47 temperature, 30, 42, 43, 49 tetrahedral, 35, 38, 45 thermal equilibrium, 48 thermodynamic integration, 44

Supercell Methods for Defect Calculations

67

thermodynamic ionization, 49 thermostat, 43 Thomas–Fermi, 38 time-dependent density-functional theory (TDDFT), 39, 44 time-dependent Schr¨ odinger equation (TDSE), 44 total energy, 30–32, 34, 43, 45, 47–53, 56, 58 trajectory, 44 transferability, 41 transition, 49 transition level, 30, 49, 51 transition metal, 57, 58 trigonal, 46, 58, 60

vacancy, 35, 38, 40, 45, 46, 52, 54, 56, 60 valence band, 35, 38, 40, 49–51, 55, 56 variational, 31, 43 VASP, 58–60 velocity autocorrelation, 48 vibrational dynamics, 30 vibrational entropy, 48, 60 vibrational free energy, 60 vibrational modes, 29, 33, 34, 47, 48, 61 vibrational spectroscopy, 29

ultrasoft pseudopotential, 41, 58, 59

ZnO, 40

Watkins, 45, 46, 56 wavelength, 52 Wigner–Seitz, 35, 55

Marker-Method Calculations for Electrical Levels Using Gaussian-Orbital Basis Sets J.P. Goss, M.J. Shaw, and P.R. Briddon School of Natural Science, University of Newcastle, Newcastle upon Tyne, NE1 7RU {J.P.Goss,M.J.Shaw,Patrick.Briddon}@newcastle.ac.uk Abstract. The introduction of defect-related states in the bandgap of semiconductors can be both advantageous and deleterious to conduction, and it is therefore of great importance to have quantitative computational methods for determining the location of electrical levels. In particular, where the defect levels are deep in the bandgap, the states involved are typically highly localized and the application of real-space, localized basis sets have clear advantages. In this chapter the use of such basis sets both for cluster and supercell geometries is discussed. Agreement with experiment is often hampered by problems such as the underestimate of bandgaps when using density-functional theory. We show that these can be somewhat mitigated by the use of “markers”, either experimental or theoretical, to largely eliminate such systematic errors.

1 Introduction It is well known that the electrical and optical properties of a crystalline material are inﬂuenced by impurities and other defects. In particular, conductivity at a given temperature is related to the free-carrier concentration, that in turn depends on the depth of the donor or acceptor level of the dominant dopant. Therefore one requires dopants with the smallest ionization energy, a value that is limited to the eﬀective-mass level of the host material [1]. Conversely, electron and hole traps deep in the bandgap are detrimental to the conductivity because they reduce the free-carrier concentration and the resultant charged defects are scattering centers that reduce carrier mobility. Deep levels are also nonradiative recombination centers aﬀecting optical properties. The importance of the electrical characteristics of defects has driven a huge eﬀort to develop reliable computational methods that can both explain experimental observations and predict new dopants with the desired properties. Currently, most calculations in this ﬁeld are performed using densityfunctional theory (DFT) [2, 3], chieﬂy simulating crystalline materials using periodic boundary conditions (PBCs), and plane wave (PW) basis sets1 to represent the wavefunctions of the electrons. 1

Plane waves represent functions in a Fourier-transformed phase space and are of the form exp(ik.r), where k is the wavevector that is related to an energy by E = 2 k2 /2m.

D. A. Drabold, S. K. Estreicher (Eds.): Theory of Defects in Semiconductors, Topics Appl. Physics 104, 69–94 (2007) © Springer-Verlag Berlin Heidelberg 2007

70

J.P. Goss et al.

With PBCs, a section of host material containing the dopant or defect is constructed and this “supercell” is repeated periodically throughout space. Such a construction represents a crystal of defects, and thus the use of PWs is a natural choice. If the defect and its periodic images are suﬃciently spatially separated they do not interact signiﬁcantly and the calculated properties represent those of isolated defects. This means that in order to obtain reliable data for defects (especially shallow dopants with large wavefunction extents) large supercells must be used. However, the computational cost increases rapidly with system size and in practice most of today’s calculations contain up to a few hundred atoms. The DFT-PBC approach has at least two major problems when calculating electrical properties. The ﬁrst is that within most commonly used localdensity (LDA) or generalized-gradient (GGA) approximations, the bandgap is underestimated, sometimes catastrophically. For example, crystalline Ge, in reality a semiconductor with a bandgap 0.74 eV [4], is found to be a semimetal [5]! Secondly, in order to obtain information about the capacity for defects to adopt diﬀerent charge states one needs to know the properties of charged systems. Strictly this is not possible with PBCs, but charged systems can be approximated by the use of a uniform background charge that exactly cancels the charge on the defect. Even then, this represents a space-ﬁlling array of charges that have an associated electrostatic energy that does not correspond to the properties of isolated defects. These problems are both mitigated by the use of atomic clusters. Here, defects are imbedded into large sections of the host material, but instead of repeating it periodically, the surface of the material is passivated (usually by hydrogen) eﬀectively forming a large molecule. The cluster geometry imposes an artiﬁcial conﬁning potential increasing the bandgap and localizing electronic states. However, although this eﬀect counteracts the inherent underestimate of the bandgap, the surface–defect interactions are of a similar nature to the defect–defect interactions in supercells. Although there are several sources of error in the calculations, many of them are somewhat systematic in nature, and hence relative locations of electrical levels may be more reliable than absolute values. This has led to the use of so-called marker methods [6–8], where one references the system of interest to one that is well understood: for example, the donor level of P in diamond is known, whereas those of As and Sb are not. Theory shows that they are shallower than phosphorus [9] and may therefore represent an improvement in the production of n-type diamond. (Of course, such calculations do not reﬂect on the relative solubilities of these dopants.) Finally, let us introduce the role of the basis functions used to describe the electrons in our problem. The use of PWs does not represent a fundamental problem, but in order to treat many systems of interest where the wavefunctions and charge density vary rapidly in space, the use of PWs often necessitates additional eﬀort (such as high-energy cutoﬀs) or the use of so-called ultrasoft pseudopotentials where one systematically removes the as-

Electrical Levels with Gaussian Bases

71

pects of the electrons that are diﬃcult to represent eﬃciently with PWs due to their localized nature. It is true that PWs may be viewed as a near-ideal basis set for eﬀective-mass-like shallow levels, since such donor and acceptor states are built out of the band-edge Bloch states. However, for deep levels the wavefunctions are often highly localized and can be characterized rather more simply by the use of molecular orbitals. The DFT package AIMPRO (Ab-Initio Modeling PROgram) uses a realspace basis made up from Gaussian functions [10, 11]. The real-space basis also allows the same electronic-structure methods to be applied to atomic clusters and molecules. In this Chapter, we ﬁrst present a detailed description of the basis sets used in our calculations. In Sect. 3 we describe the computational methods for calculating electrical levels, and in particular the marker method and present a review a range examples of its use in diﬀerent group-IV materials in Sect. 4.

2 Computational Method Our intention is to detail the calculation of electrical levels and not review the entire formalism used in the calculations. However, brieﬂy, AIMPRO is an electronic-structure program using LDA- and GGA-DFT. Atoms are treated using pseudopotentials [12] to remove the core electrons, and the distribution of the electrons solved self-consistently for a given set of atoms. AIMPRO can be used with a range of pseudopotential types, including the seminonlocal forms [13–15], and the dual-space separable pseudopotentials [16]. In addition to the eﬃciencies oﬀered by their separability, the latter pseudopotentials oﬀer extended norm conservation, accounting for a large number of occupied and unoccupied atomic levels. Currently, by default, AIMPRO uses the Perdew– Wang functional [17] for PBC calculations and a Pad´e approximation to this functional [18] for cluster calculations, although a number of alternative functionals are available. Historically, cluster calculations used an extremely fast parameterized analytic form for the exchange-correlation functional as described in detail previously [11]. GGA calculations are performed using a White–Bird [19] implementation of the GGA functional [20]. AIMPRO can be used both in periodic and cluster modes and the atomic structures optimized either using static minimization methods or molecular dynamics. From these calculations a range of observables can be derived, such as the electrical levels introduced above, vibrational-mode frequencies and symmetries, electronic-structures, hyperﬁne and zero-ﬁeld splitting tensors, electron energy loss spectra, migration barriers, and so on. However, in contrast to the majority of PBC calculations, AIMPRO represents the wavefunctions using a range of real-space, Gaussian-orbital functions.

72

J.P. Goss et al.

2.1 Gaussian Basis Set In order to construct and solve the Hamiltonian for our systems we expand our wavefunctions in terms of a basis set. Many diﬀerent basis types are used for ﬁrst-principles calculations, and each has associated advantages and disadvantages. There is no ﬁrm consensus on the optimum basis set to use, and since the choice of basis set plays a signiﬁcant role in determining the structure and nature of the calculations, the particular bases used and issues concerning them are worthy of some comment here. In the discussion that follows we shall consider only the arguments surrounding the selection of basis sets for pseudopotential calculations: clearly all-electron calculations, which must describe the rapid ﬂuctuations of the wavefunctions in the ionic core region place additional demands on the basis set. As alluded to above, of the many basis sets that are routinely used, perhaps the most signiﬁcant distinction lies between the expansion in terms of PWs, and the use of basis functions that are localized functions in real space. AIMPRO uses the latter type, speciﬁcally a set of Cartesian Gaussian orbitals (CGOs) centered on atoms and possibly other positions. These basis functions are products of a simple Gaussian and a polynomial in the position vector relative to the center of the Gaussian: φi,n1 n2 n3 (r) = xn1 y n2 z n3 e−αi r , 2

(1)

where αi reﬂects the spatial extent of the function; larger (smaller) values correspond to more localized (diﬀuse). The term xn1 y n2 z n3 deﬁnes the angular dependence, and relates to the spherical-harmonic associated with the angular-momentum and magnetic quantum numbers, l and m. For example, a px -orbital has n1 = 1, n2 = n3 = 0. These polynomial combinations enable the basis to describe atomic-like states of arbitrary angular momentum. The basis-set is deﬁned by the combination of Gaussian exponents and angular-momentum to which the combinations of polynomial functions extend. The advantages and disadvantages of PW and these real-space basis sets are already documented in the literature [11], however, it is useful to consider some of the key diﬀerences between them. A key advantage of CGOs is that they can be nonuniformly distributed in space, lending a more ﬂexible basis to regions that require it (for example in the region of a defect in a crystal). Such an approach cannot be taken with PW bases: the region with greatest complexity deﬁnes the density of PWs everywhere. For systems containing a small region in which the wavefunctions vary rapidly a high-energy cutoﬀ might be required, and this dense PW basis set must exist throughout the whole crystal. This leads to a very large Hamiltonian and slow calculation. A particular example of this problem is where surfaces are treated using a PBC via the inclusion of regions of vacuum. An advantage of a PW representation is that the basis functions are necessarily orthogonal. Consequently, the number of PWs can be increased without

Electrical Levels with Gaussian Bases

73

limit while retaining the stability of the calculation. CGOs are not orthogonal and the use of too large a basis set can result in numerical instability developing. The stability of the basis becomes a signiﬁcant issue when one attempts to address the question of how one should choose the basis for a particular problem. For a PW calculation it is possible to ensure that one has arrived at a converged result by systematically increasing the PW cutoﬀ. For a CGO basis set it is not possible to perform a systematic test to ensure that a convergent basis has been arrived at. Indeed, the choice of exponents for the functions in the basis set is a nontrivial one. We shall discuss the details of the basis set optimization procedure in more detail below. We now consider the CGOs in more detail. The task is to obtain a set of exponents for which the pseudowavefunctions are accurately described without rendering the calculations unstable. In order to achieve this, the variational principle is employed: when one compares any two basis sets, that which allows the wavefunctions to describe the true wavefunction most accurately results in the lowest total energy. The minimization of the total energy with respect to the exponents of the CGOs therefore results in the optimum basis set for a given number of functions. This process may then be repeated for diﬀerent numbers of functions to assess whether the basis is large enough. Again, the number of CGOs included cannot be increased without limit as the calculations become unstable. However, it is typically possible to obtain a convergent set of exponents prior to the onset of instability. Of course, an increased number of exponents increases the size of the Hamiltonian, and in turn the computational cost. Typically, the optimum number of basis functions is obtained by balancing the absolute quality of the basis and the associated accuracy of the results against the computational load. In addition to the number and value of the exponents, αi , the polynomial functions included with a given Gaussian (s, p, d, f and so on) must also be chosen. In general, a basis set contains a range of values of angular momentum and each CGO is treated independently. The angular momentum has a dramatic impact upon the number of functions in the basis set: for example, angular momentum up to s, p and d results in 1, 4 and 10 functions per exponent, respectively2 . As an example, four exponents per atom each of which include s and p, gives rise to 16 functions per atom. Increasing the basis to include d-functions increases the basis size to 40, and since diagonalization of the Hamiltonian scales as the cube of the basis size, the time to obtain a total energy would increase by more than an order of magnitude. 2

It should be noted that the linear combinations of six functions with n1 + n2 + n3 = 2 in (1) produce the ﬁve d-type functions (xy, xz, yz, 2z 2 − x2 − y 2 and x2 −y 2 ), and an s-type function (x2 +y 2 +z 2 ). Our standard practice in using the uncontracted basis sets discussed here is to include this additional s-type function, and hence the n1 = n2 = n3 = 0, n1 + n2 + n3 = 1 and n1 + n2 + n3 = 2 terms yield ten rather than nine functions.

74

J.P. Goss et al.

It is therefore paramount that basis functions of higher angular momentum are used selectively where the physical demands of the system merit them. Indeed, using a small number of high angular momentum functions is common practice in Hartree–Fock calculations where the basis sets are relatively small due to the extreme computational cost of this method, and are built up using the angular momentum of the atomic species with the addition of a single, higher angular momentum orbital as a polarization function. For most calculations all of the CGOs are centered on atoms, and move with the atoms during structural optimization. It is also possible to center basis functions at sites where there are no atoms. For example, historically, centering basis functions at appropriate positions on the bonds between adjacent atoms in the crystal was used to improve the description of the angular variations due to the formation of bonding orbitals. Locating basis functions at bond centers allows for polarization to be incorporated without increasing the maximum angular momentum, reducing the computational cost, but introducing a poorly deﬁned set of sites: during relaxation, structural changes may change the atoms between which bonding is present. However, increases in the speed of computational resources, together with improved algorithms has meant that bond-centered orbitals have largely been superseded by the use of basis sets containing higher angular momentum. The higher angular momentum components provide the necessary angular ﬂuctuations without the need for the additional complexity of bond-centered basis functions. Another situation in which localized basis functions may be centered away from atoms is the use of “ghost” atoms when treating surfaces. In this case, basis functions are placed in the vacuum region as though atoms were there (although of course, no atomic potential is included). This approach can provide additional basis functions to help describe the evanescent wavefunction variations close to the surface. For the majority of calculations the basis functions are atom-centered CGOs. A set of basis functions is therefore associated with each atom. The size of the basis set, and the particular exponents in it, will be optimized for each species of atom. Additionally, it is sometimes appropriate to treat diﬀerent atoms of the same species with diﬀerent basis sets within the same calculation (for example, surface atoms may require a larger basis than bulk atoms in a surface calculation). In the basis sets speciﬁed so far, all of the CGOs are independent basis functions, with coeﬃcients free to change during the calculation, and each contributes to the overall dimension of the Hamiltonian. It is possible, however, to exploit the physical properties of the system to take linear combinations CGOs to form more complex basis functions that provide a comparable accuracy but with a reduced number of independent parameters. These are referred to as contracted basis sets and are developed in the following way.

Electrical Levels with Gaussian Bases

75

A small reduction in the basis sets involving d-type (and higher angular momentum) functions can be obtained by taking linear combinations of the functions in (1). Formally, cnlm,n1 n2 n3 φi,n1 n2 n3 . (2) ψi,nlm = In the case containing up to quadratic prefactors there are ten functions φ, from which we may choose to produce a set of nine functions, ψ, which transform with angular momentum l = 0, 1, 2. A more radical approach to reduce the size of a basis set uses combinations of these ψi,nlm : Ψnlm = Cinl ψi,nlm , (3) where the number of functions of the form of Ψ is dramatically less than the related set of ψ. Particular examples of these contracted bases appear below in Sect. 2.3. 2.2 Choice of Exponents As mentioned above, the values of αi may be chosen by consideration of the total energy. Typically, this optimization process is performed for a prototypical example of the system to be studied. For example, in the case of studies of defects in silicon, the basis associated with the Si atoms is chosen to best represent a bulk Si cell. A problem of optimizing the values of the exponents is a multidimensional minimization problem, and may be tackled by one of the many standard minimization procedures available. AIMPRO allows for the optimization of the exponents by a downhill simplex or a conjugate gradient minimization of the total energy. Given that a typical element will require of the order of four diﬀerent exponents in its basis set, the free optimization of the exponents is a fourdimensional minimization problem. Calculations have shown that the fourdimensional energy surface generally is very ﬂat and undulating, resulting in many local minima, and causing diﬃculties in producing a unique choice of exponent. This is mitigated by the use of “even-tempered” basis sets in which the n exponents are constrained to be in a geometric series, and although it is generally true that an unrestricted basis set will lower the total energy, it is found that this is often not a signiﬁcant eﬀect. For contracted basis sets, as with the full Gaussian basis sets, ﬁxed parameters (in this case both coeﬃcients and exponents) may be obtained with reference to an appropriate prototypical system. Each combined contracted basis function adds just one to the dimension of the Hamiltonian, and yet contains variations over a number of diﬀerent length scales that reﬂect the properties of the physical system used in the ﬁtting procedure. Once the contraction coeﬃcients have been optimized, which is typically performed

76

J.P. Goss et al.

Fig. 1. Total energy of Si bulk unit cell during basis-exponent optimization. The energy is shown as a function of the number of simplex iterations

using a simplex optimization within AIMPRO, they remain ﬁxed during the subsequent self-consistent ﬁeld calculations. The optimization of the exponents is an important step prior to commencing a real calculation. Clearly, a poorly chosen basis may impact on the accuracy of the ﬁnal calculation, by aﬀecting the accuracy of the wavefunction description. However, as we shall demonstrate in the example below, the physical properties of the material (for example lattice constant and bulk modulus) are not sensitive to the ﬁne tuning of the basis. Only when the basis set has been carelessly chosen is there a signiﬁcant impact upon the physical properties. 2.3 Case Study: Bulk Silicon Let us consider the case of a range of basis sets for bulk silicon. Here, we shall consider the optimization of exponents in a four-exponent basis set, with angular momenta up to d on the ﬁrst and second exponent, and up to p on the third and fourth exponent (where the ﬁrst α is smallest). We refer to this as a ddpp basis. As an initial guess for the exponents we shall use the values {0.1, 0.3, 1.5, 4.0}. The range of these values results from a simple consideration of the length scales of the CGOs, the lowest exponent (longest-ranging Gaussian) allowing our basis to represent functions extending into the space between adjacent atoms, the highest exponent (shortest-range Gaussian) allowing us to describe the short-ranged variations of the valence pseudowavefunctions. (Note: the basis sets are described here for pseudopotential calculations – if all-electron calculations are to be performed, very much larger bases would be required, the highest exponents of which would be far greater than those needed for pseudopotentials.)

Electrical Levels with Gaussian Bases

77

We show in Fig. 1 the total energy as a function of the number of steps in a simplex optimization of this basis. Note how the reduction in energy is relatively steep in the early stages followed by a long tail, reﬂecting how a modest attempt to obtain exponents that reﬂect the properties of the system is suﬃcient to obtain a reasonably well-converged total energy. Several of the partially optimized bases were used to compute the lattice constant and bulk modulus of the Si by ﬁtting to the Birch–Murnaghan equation of state. These data are presented in Table 1. Table 1. Total energies (Hartrees) at energy minimum, lattice constants (au ) and bulk moduli (GPa ) for Si basis sets at various stages of optimization. For comparison, the experimental lattice constant and bulk modulus of silicon are 10.263 au and 97.9 GPa, respectively [21, 22] Iterations

Total energy

Lattice constant

Bulk modulus

1 4 6 15 24 30 100

−7.9234 −7.9250 −7.9269 −7.9271 −7.9276 −7.9280 −7.9280

10.24 10.23 10.21 10.21 10.21 10.21 10.20

91 91 94 95 93 94 96

Since the LDA is generally expected to obtain lattice constants to around 1 % accuracy, and bulk moduli to around 5 % to 10 % it can be seen from Table 1 that the variation in the structural parameters with basis is relatively small. In particular, the initial, somewhat arbitrary parameters yield reasonable results, and after only around ten iterations do the changes in lattice constant and bulk modulus become minimal on this scale. Table 2. Total energies (Hartrees) at energy minimum, lattice constants (au ) and bulk moduli (GPa ) for diﬀerent optimized Si basis sets Basis

No. functions per atom

Total energy

Lattice constant

Bulk modulus

dddd ddpp pdpp pppp

40 28 22 12

−7.9335 −7.9280 −7.9268 −7.8974

10.17 10.20 10.21 10.35

95 96 95 85

We must also consider the role of the angular momentum in the CGOs. The size of basis set increases with higher angular momentum, slowing the calculation but providing a more ﬂexible and accurate basis set. There is a

78

J.P. Goss et al.

compromise to make between accuracy and computational cost. Typically, for materials like diamond and silicon pdpp or ddpp bases are found to be suﬃcient. However, in calculations of defects it is often the case that heavier bases are used for the atoms at the defect itself, such as dddd. This exploits the localized nature of the CGOs, improving the accuracy of the basis in a particular region with little eﬀect on the overall accuracy or computational cost of the calculation. Table 2 details the eﬀect on the structural properties of silicon for various basis sets. The additional cost of the extra functions in the dddd basis is unnecessary since the results are eﬀectively the same as the computationally cheaper pdpp basis. However, the pppp basis set is seen to be too small and the omission of any higher angular momentum functions prevents a suﬃciently accurate description of the directional bonds found in covalent semiconductors. As with the plain CGO basis, a number of diﬀerent contracted basis sets can be deﬁned according to the number of diﬀerent combinations of the functions, and the angular momentum to which they extend. To label these contracted basis sets we draw on the conventional nomenclature of quantum chemistry, and specify, for example, a 4G basis to be one in which four CGOs (the “G”) of diﬀerent exponents are combined into ﬁxed functions. Separate combinations are formed for n and l representing the occupied atomic valence states of the element in question. For example, for the s and p orbitals in silicon this results in a total of four independent functions, one s- and three p-polynomial combinations. The same contraction coeﬃcients are used for diﬀerent components of a given function (for example px , py and pz ), although they are of course included as independent basis functions. This level of contraction is known as a minimal basis set as they cannot change shape during the calculation. To improve the ﬂexibility of the basis set, a second set of contracted coefﬁcients may be deﬁned resulting in an additional set of four basis functions (a total of eight basis functions, two s-types and 6 p-type). In our nomenclature this would be referred3 to as 44G. Such basis sets are greatly restricted due to the fact that the highest angular momentum that can be represented is limited to the angular momentum of the occupied atomic states. Although these can describe the isolated atom well, higher angular momentum components are needed to describe directional bonds. To account for these we may introduce additional “polarization” functions of higher angular momentum CGOs (for example d functions in silicon) with a single free exponent. The inclusion of polarization functions in a basis set is indicated by a ∗ in the notation, for example 44G∗ . The addition of the polarization functions increases the basis 3

This is similar to the “31” part of the quantum chemists standard 6-31G basis set. The only diﬀerence is that in our two contractions are combinations of all four underlying Gaussians; the 6-31G basis has 3 functions contracted together and one function left uncontracted, a more restrictive prescription.

Electrical Levels with Gaussian Bases

79

from 8 to 13 functions per atom, which remains considerably smaller than the ddpp plain Gaussian basis. We have extensively studied the eﬀect of reducing the degrees of freedom in our basis sets by moving to increasingly small contracted sets. In Table 3, the minimum total energy, lattice parameter and bulk modulus are presented for contracted basis sets, and compared with the uncontracted ddpp basis. Table 3. Total energies (Hartrees) at energy minimum, lattice constants (au ) and bulk moduli (GPa ) for contracted basis sets 44G∗ , 4G∗ , and 4G, as deﬁned in the text Basis No. functions per atom Total energy Lattice constant Bulk modulus ddpp 44G∗ 4G∗ 4G

28 13 9 4

−7.9280 −7.9269 −7.9226 −7.8854

10.20 10.19 10.21 10.39

96 97 103 91

A 44G∗ basis for materials such as Si and diamond is found to be as effective as a 28-function ddpp basis. In other words, the 44G∗ basis provides a convergent description of our wavefunctions for our typical host elements, at a much reduced cost in terms of the Hamiltonian. These contracted basis sets are therefore used in many of our calculations, giving an optimum performance with regard to computational cost. Cheaper bases still, such as the 4G basis are found to result in wider variations of lattice constant and bulk modulus, as well as giving poor electronic band structures, particularly in the conduction band. Although the 4G bases are not suitable for routine calculations, there are a number of potential applications for these basis sets. One possibility is that these extremely cheap bases (just four functions per atom in Si) could be used for bulk regions in very large unit cell calculations. Fuller bases could be used to describe the essential regions of the material (for example the defect region and adjacent atoms) with the 4G bases ﬁlling the remainder of the bulk-like unit cell. For such schemes to work it is necessary to match the optimum lattice constant of the two bases to avoid unphysical internal strain at the boundary between the two diﬀerent bases. Although we have implemented this approach and tested the idea with encouraging results, it has yet to be used in a real application.

80

J.P. Goss et al.

2.4 Charge-Density Expansions In AIMPRO the charge density, n(r), is also ﬁtted to a set of basis functions. With the PBC n(r) is expanded in PWs, so that the approximate charge density n ˜ (r) = n(G)eiG · r , (4) G

where all PWs with G2 /2 < Ecut-oﬀ are included, with the energy cutoﬀ chosen according to the atomic species present. The number of PWs is suﬃcient to make n ˜ a very accurate representation of the charge density n(r) given by the underlying Gaussian basis set. This does not incur signiﬁcant penalties in either speed or memory as the expansion is performed only for one function, n(r), rather than each occupied band as is the case in conventional fully PW basis set calculations. As a consequence, the energy cutoﬀ can be very large: typical values are 300 Ry and 80 Ry for carbon and silicon, respectively. In a cluster calculation, the charge density is expanded in uncontracted Gaussians (1) typically up to d-type functions. More details regarding the charge-density basis functions in cluster calculations can be found elsewhere [11].

3 Electrical Levels We now turn our attention to the calculation of electrical levels. Since the marker method, which forms the main part of this section, can be understood in terms of the more commonly used formation-energy method, we brieﬂy describe this and its associated problems. Before we do so, however, it is important to deﬁne what is meant by an electrical level. The electrical levels of a dopant (or any active defect) correspond to a thermodynamic property of the system, and relate to the chemical potential, µe of the electrons (sometimes erroneously referred to as a Fermi level, which is strictly only a zero-temperature quantity). Where µe lies below, say, the donor level of an impurity, energy is released by moving an electron from the defect to the electron reservoir at µe , and so this transfer of charge proceeds. Conversely, if µe is higher in the bandgap than the donor level of the defect it would cost energy to move the electron from the donor to the electron reservoir, and therefore it does not happen. It should therefore be noted that these levels relate to a change of charge state and cannot be obtained from the electronic-structure of any one of the charge states involved alone.

Electrical Levels with Gaussian Bases

81

3.1 Formation Energy The charge-state- (q) dependent, zero-temperature formation energy of a system of atoms and electrons (X) is usually written [23]: µi + q {Ev (X, q) + µe } + ξ(X, q) , (5) E f (X, q) = E t (X, q) − atoms

where E t is the total energy calculated for the system such as that obtained using AIMPRO, µi and µe are the atomic and electron chemical potentials, Ev (X, q) is the energy of the valence-band top and ξ(X, q) is a term that takes into account artifacts introduced by the computational framework. For PBCs ξ(X, q) reﬂects defect–defect interactions, whereas for clusters it relates to defect–surface interactions including quantum conﬁnement. Usually, the relevant E t (X, q) is that of the lowest-energy conﬁguration of X in charge state q, but not always, as noted below. For PBCs ξ may take the form of a power series in moments of the electron distribution, which can be viewed as terms arising from an array of monopoles, dipoles, quadrupoles and so on. The magnitudes of each term may be taken from a simple model, such as that of Makov and Payne [24] where only the terms in a Madelung energy and a quadrupole term are typically retained. The material is taken into account simply using the static dielectric constant, ε. Note, the Madelung term scales as q 2 and hence grows rapidly with q so that, for example, for a cubic supercell of diamond of side length 2a0 , the Madelung correction for q = ±3e is already of the order of the bandgap! This simple approach has received considerable criticism over recent years, so other, often computationally demanding, approaches have been adopted [25–28]. Notwithstanding the details of ξ(X, q), one can use E f (X, q) to estimate the electrical levels of X. The approach is to determine the thermodynamically most stable charge state for all relevant values of µe , and the critical values at which charge states change are the electrical levels. For example, the acceptor level is given by the value of µe that satisﬁes E f (X, 0) = E f (X, −1): µe = E t (X, −1) − E t (X, 0) + [ξ(X, −1) − ξ(X, 0)] − Ev (X, −1) , (6) as illustrated in Fig. 2. The diagram also illustrates the diﬃculties in interpreting levels that lie in the energy range between the theoretical and experimental bandgaps. Note, usually the electrical levels represent the transition between the lowest-energy structural conﬁgurations of each charge state, but not always. For example, there may be a considerable energy barrier between conformations of a set of atoms, so that the electrical levels relate to the change of charge state of a speciﬁc arrangement of atoms. An example of this is that of boron-vacancy complexes in silicon, where the equilibrium number of host sites between the impurity and the lattice vacancy is charge state

82

J.P. Goss et al.

Fig. 2. Illustration of the use of the formation energy to obtain an acceptor level for the system X in silicon. Above the acceptor level X − is thermodynamically more stable that X 0 , whereas below the reverse is true. The shaded area indicates the region between the theoretical and experimental bandgaps. The inclusion of ξ in the charged formation energy pushes the acceptor level above the theoretical value for Ec , but it remains deep in the experimental bandgap

dependent [29]. Such metastability must be taken into account when trying to assign calculated electrical transitions to those measured experimentally. This approach has perhaps three chief problems, the ﬁrst of which is the poorly deﬁned correction term, ξ which we have already touched upon. The second is that µe is deﬁned relative to the valence-band top in the defective system, which may be diﬃcult to establish with any precision. If one does not wish simply to use the approximation Ev (X, −1) = Ev (bulk, 0) then one might use corrections obtained either by examination of the lowest occupied Kohn–Sham level [30], or of the electrostatic potentials in bulk and defective systems [31] (see Sect. 3.2). The third, and often most critical problem that may aﬀect the location of electrical levels is the underestimate of the bandgap. For instance, the bandgap of hexagonal ZnO is around 3.4 eV [4], but simple application of the LDA- or GGA-DFT leads to bandgaps around 1 eV. Recently, hydrogen has been shown to be a shallow donor in this material [32, 33], but chargedependent formation energies yield donor levels around Ev + 2 eV [34, 35]. However, as previously suggested, for a given material it is often found that many of the problems introduce systematic errors. Therefore, one chooses alternative reference states that mitigate the charged systems, bandgap error and other interactions introduced by the geometry: this is the marker method.

Electrical Levels with Gaussian Bases

83

3.2 Calculation of Electrical Levels Using the Marker Method We may avoid the problems highlighted above by referencing, say, the acceptor level of one system to that of another. Equation (6) for two diﬀerent systems, X and Y , where the acceptor level µe (Y ) is known combine to yield the expression: µe (X) = µe (Y ) + E t (X, −1) − E t (Y, −1) − E t (X, 0) − E t (Y, 0) − [Ev (X, −1) − Ev (Y, −1)] + [{ξ(X, −1) − ξ(Y, −1)} − {ξ(X, 0) − ξ(Y, 0)}] .

(7)

If terms in ξ cancel and Ev (X, −1) = Ev (Y, −1) this simply reduces to: µe (X) = µe (Y ) + E t (X, −1) − E t (Y, −1) − E t (X, 0) − E t (Y, 0) . (8) This deﬁnes an unknown acceptor level, µe (X), with respect to the known marker at µe (Y ) with reference only to total energies. Note, (7) and (8) explicitly show that the calculations involve diﬀerences of energies between systems with the same charge. However, we have made at least two rather bold assumptions, and it is necessary to explore where and why they are likely to be valid. We ﬁrst examine the notion that Ev (X, q) = Ev (Y, q). Since one can add a constant potential to any system (i.e., the zero of the potential energy scale is often poorly deﬁned in PBC calculations), the valence-band states may be rigidly oﬀset from those of a defect-free system, and one can estimate the potential diﬀerence between X and Y by ﬁnding the average electrostatic potential in bulk-like regions of these systems [31]. For example, for substitutional impurities in a diamond-structure material, one might characterize the diﬀerence in the background potentials by ﬁnding the diﬀerence in the total electrostatic potentials at the T-interstitial sites far from the impurities. Alternatively, the potential diﬀerence between two systems can be estimated by the diﬀerence in the energies of the lowest occupied levels in X and Y [30] under the assumption that these characterize the average potentials in these systems. In our experience, such corrections may be up to a few tenths of an eV, but are usually small [31]. We now turn to the assumption that the ξ terms cancel. The suggested corrections for PBCs of Makov and Payne [24] assume an array of point charges, but it is clear from several studies that this approach tends to give a rather poor estimate. However, it is instructive to consider ξ(X, q) as arising from a series of multipole interactions. For chemically similar systems, the larger terms in the series would naturally be close in magnitude. Therefore, the best accuracy using the marker method is expected when comparing structurally and chemically similar systems. This remains true even when considering transitions between highly charged states, which is important because of the q 2 dependence of the simple Makov–Payne type of correction. However, there are two important areas where the marker method may be diﬃcult to apply. The ﬁrst is where the available markers are far in energy and

84

J.P. Goss et al.

chemical nature from that of the system of interest, such as using a shallow donor as a reference for a very deep donor. Under these circumstances there is unlikely to be very complete cancellation in the ξ, and hence the error bars in the calculation become more signiﬁcant. Furthermore, problems associated with the underestimate of the bandgap will also become more important. The second is that in some materials there may be no experimental data. For example, to our knowledge there are no unambiguous observations of double donors or acceptors in diamond. Where there are no appropriate markers, one might use a bulk system as the reference, Y , in (7) and (8). Such an approach was detailed for boron in silicon [7] and defects in diamond [8]. Here, the ﬁrst donor and acceptor levels of a bulk system are, by deﬁnition, Ev and Ec , respectively. However, one should exercise some caution in using a bulk system as a marker; deep levels and band edges are typically very diﬀerent in character. Furthermore, the levels of shallow defects are referenced to markers at the other extreme of the bandgap, making the underestimate of the bandgap a signiﬁcant factor. Finally, in the preceding discussion we have largely emphasized the use of the marker method for PBCs, but the principles are the same for cluster calculations. Indeed, the use of clusters for narrow-gap materials has two important advantages over the supercell approach. The ﬁrst is that the lack of periodicity means that there is no dispersion in the electronic-structure. Secondly, the conﬁnement of an atomic cluster tends to oppose the typical underestimation of the bandgap. For materials such as germanium for which the underestimation is acute, this is a very signiﬁcant, qualitative eﬀect, as reﬂected in the results presented below. In the ﬁnal section we review a number of examples of the application of the marker method using AIMPRO in both supercell and cluster modes.

4 Application to Defects in Group-IV Materials 4.1 Chalcogen–Hydrogen Donors in Silicon AIMPRO was recently used to analyze the properties of a range of chalcogens and their complexes with hydrogen in silicon. In this study [31] many of the issues raised above were explicitly examined, including the role of supercell size, Brillouin-zone sampling, basis and the average electrostatic potentials. One signiﬁcant factor in using chalcogens and their complexes with hydrogen in this study is that they have been characterized extensively by experiment, with spin densities, vibrational modes and for the substitutional chalcogens, electrical levels being available. It was therefore possible to show that the calculations were able to reproduce important aspects of the defects of interest other than the electrical characteristics, thereby validating the conclusions drawn. In particular, Mulliken bond-population analysis indicated that the donor wavefunctions were being faithfully reproduced in

Electrical Levels with Gaussian Bases

85

Fig. 3. Schematics of the partially passivated chalcogen–H complex in silicon. White and black circles represent host and impurity atoms, respectively, H being represented by the smaller black circle. Dashed lines indicated the cubic axes

these calculations, and that the characteristics were similar for the diﬀerent chalcogen species, indicating that the marker method should be appropriate. Additionally, for the chalcogens the defect-level dispersions are very similar suggesting that this eﬀect also would cancel out using an empirical marker. The chalcogens S, Se, and Te lie onsite, each having two donor levels, as listed in Table 4. The calculated donor levels listed were obtained using the formation energies with a Madelung correction and the marker method using bulk silicon and S as references. Table 4. Electrical levels relative to Ec ( eV ) of chalcogen and chalcogen–hydrogen complexes in silicon (see [31]). Experimental data from [36]

Defect

Experiment (0/+) (+/2+)

Formation energy (0/+) (+/2+)

Bulk marker (0/+) (+/2+)

Sulfur marker (0/+) (+/2+)

S Se Te S–H Se–H Te–H

0.29 0.29 0.20 – – –

0.78 0.79 0.75 0.41 0.37 0.27

0.42 0.40 0.27 0.13 0.10 0.00

0.29 0.28 0.25 0.01 −0.02 −0.12

0.59 0.54 0.36 – – –

1.25 1.23 1.22 1.78 1.77 1.77

0.48 0.45 0.28 1.18 1.18 1.18

0.59 0.55 0.38 1.28 1.28 1.28

The shallow nature predicted for the X–H complexes, the structure of which is shown schematically in Fig. 3, was viewed to be consistent with the fact that they had not been detected using deep-level transient spectroscopy [37, 38], but had been detected via their vibrational modes [39]. Three important conclusions can be drawn from this study. The ﬁrst is that the formation-energy approach yields qualitatively erroneous results: S, Se, and Te have no double-donor level in the bandgap, and the single-

86

J.P. Goss et al.

Fig. 4. Schematics of the VO center in Si and Ge. White and black circles represent host and oxygen atoms, respectively. The dark bond in (a) indicates the reconstruction present in the neutral charge state. (b) shows the unreconstructed center characteristic of the negative charge state

donor levels are far too deep. This can be traced to the underestimate in the bandgap and the nature of the correction terms, ξ. The second is that, although the single-donor levels are reasonably reproduced using the bulkmarker method, the second donor level is very poor, due to an underestimate of the correlation energy. Finally, the positive result is that, at least for classes of similar defects, the empirical marker method yields very good agreement with experiment. 4.2 VO Centers in Silicon and Germanium The properties of oxygen in silicon and germanium have been studied extensively as a consequence of the incorporation of O during growth and the properties that it lends to the materials. Of all the various roles and structures in which oxygen is involved, one of the most primitive is oxygen substituting for a host atom. Oxygen is a relatively small atom so that this center is generally referred to as a complex of (interstitial) oxygen with a lattice vacancy (VO), the structure of which is shown schematically in Fig. 4. VO centers in the neutral charge state can be understood as follows. The removal of a host atom creates four “dangling bonds”. Divalent oxygen passivates two of these and the remaining two dangling-bonds then combine together in a reconstruction, resulting in a defect that is fully chemically coordinated. However, these centers can trap additional electrons by breaking the relatively weak reconstruction, and the resultant dangling bonds lead to states in the bandgap. Experimentally, the VO center in silicon has an acceptor level at Ev + 1 eV [40]. However, the DFT calculations using supercells and formation energies have resulted in a rather poor agreement, predicting an acceptor level at Ev + 0.4 eV [41]. However, recalling that in these calculations the bandgap of bulk silicon is underestimated by more than 50 % of the experimental value, this donor level is approximately the correct depth below

Electrical Levels with Gaussian Bases

87

the theoretical Ec , which might be viewed as agreeing with experiment, and it is not clear how to interpret this calculation. The marker method using atomic clusters [6] where the bandgap underestimate is mitigated and using the acceptor level of interstitial carbon (Ec − 0.10 eV [42]) as a marker yielded an acceptor level for VO in silicon at Ec − 0.13 eV, in close agreement with the experimental level. Indeed, the small error is a testament to how robust the method is since, although they are close by in energy, the character of the acceptor wavefunctions for the VO and carbon interstitials are not closely related. The importance of the bandgap error is even greater when considering Ge. Recent calculations have also adopted the cluster conﬁguration of AIMPRO to analyze a range of defects in this material [43]. In particular, VO experimentally has acceptor and double-acceptor levels at Ev + 0.27 eV and Ev + 0.49 eV, respectively [44]. Using AIMPRO and atomic clusters that have approximately the experimental bandgap of 0.7 eV the two acceptor levels of VO have been calculated relative to the acceptor and double-acceptor levels of substitutional Zn at Ev + 40 m eV and Ev + 100 m eV, respectively [4]. The calculated second acceptor level is in excellent agreement with the experimental result, lying at Ev + 0.47 eV. However, the ﬁrst acceptor level calculated at around Ev + 0.42 eV is in less good agreement, but still within 0.2 eV. The reason for the larger deviation in the single-acceptor level is unclear, but even such an error bar is useful in the context of the more traditional supercell approaches that suggest this material has no bandgap at all. 4.3 Shallow and Deep Levels in Diamond In contrast to Si and Ge, diamond, with an indirect bandgap of around 5.5 eV [4], is a good example of an insulator, not obviously to be associated with the semiconductor industry. However, p- and n-type diamond can be produced via doping with boron and phosphorus, respectively, with heavily boron-doped materials becoming metallic and opaque. However, although phosphorus acts as a donor, the activation energy is very high at around 0.6 eV, so the room-temperature ionization fraction, and hence the number of free electrons, is rather small. This has led to an eﬀort to deduce which, if any, other system may result in a shallow donor level. As well as the electrical properties of diamond, the optical transparency, especially in the infrared, of the pure material has led to applications in high-speciﬁcation optics. However, as-grown diamond may contain deep-level defects that absorb and luminesce, and an understanding of these centers is also obviously of relevance. Regrettably, the number of deﬁnitively characterized donor and acceptor levels in diamond is relative small, and it is unsurprising that computational methods have been used in an attempt to assess both shallow and deep centers. We ﬁrst address examples of potential shallow donors. Since P is the

88

J.P. Goss et al.

Fig. 5. Location of donor levels in the bandgap relative to Ev for pnictogen donors in diamond. (a) and (b) shows values calculated using phosphorus and the bulk supercell being used as a marker, respectively. Empty and ﬁlled circles show 64 and 216 atom cells, respectively. The dashed and dotted lines show the experimental donor levels for P and N, and the shaded area shows the experimental conduction band

best-established shallow donor in diamond, it seems a good idea to establish if, as in silicon, the other pnictogens may have useful donor properties. Figure 5 plots the calculated donor levels using AIMPRO as described in [9]. Figure 5a shows the use of the experimental donor level [45] for P at Ec − 0.6 eV as a marker for supercells containing 64 or 216 atoms (cubes of side length 2a0 and 3a0 , respectively). The trends are the same for both curves and both supercells reproduce the experimental donor level of nitrogen. Figure 5b shows the same data, but referenced to bulk diamond. Now, the marker is the valence-band top, so it is far (around 5 eV!) from the anticipated location of the pnictogen donor levels. This exempliﬁes the need for appropriate markers for the method to have a quantitative role. However, irrespective of the marker, the important result in this application is that shallower donors of a simple nature, i.e., As and Sb, are expected to lead to improved n-type diamond. Recently, we also used supercell calculations to compare the use of the more traditional formation energy approach with the marker method for a range of centers, and in particular for those for which electrical levels are known experimentally [8]. Table 5 lists some of these results. The overall agreement between the marker method and experiment is conspicuously better than using the formation-energy approach, indicating that the marker method may usefully be applied to wide-gap materials for both deep and shallow electrical levels. For the small set of data presented in Table 5 one could adopt any acceptor and donor as an empirical marker and get very similar accuracy.

Electrical Levels with Gaussian Bases

89

Table 5. Electrical levels ( eV ) for various centers in diamond from experiment, compared to those calculated using the formation-energy method and the marker method using a bulk cell as a marker. For the formation-energy method, we quote the levels above Ev and below the theoretical and experimental locations of Ec (Ecth = Ev + 4.2 eV and Ecexpt = Ev + 5.5 eV). Asterisks indicate the markermethod results where the bandgap energy of 5.5 eV has been used to reference to the opposite band edge. Subscript s indicate substitutional impurities and v represents a lattice vacancy

Defect

Experiment

Formation energy Ev Ecth Ecexpt

Bulk marker Ev Ec

Ev + 0.37 [46] Ec − 2.49 [47, 48] Ec − 2.583 [49]

0.2 3.3 1.8

4.0 0.9 2.4

5.3 2.2 3.7

0.5* 3.0* 2.2*

5.0 2.5 3.3

Ec − 1.7 [50] Ec − 0.6 [45] Ec − 3.8 [51]

3.0 4.2 0.8

1.2 0.0 3.6

2.5 1.3 4.7

4.0 5.2 1.8

1.5* 0.3* 3.7*

Acceptors Bs Nis V–Ns Donors Ns Ps Ns –Ns

5 Summary The characterization of the electrical properties of defects and dopants using standard methodologies such as LDA- and GGA-DFT is a demanding problem. The most common approach of calculating charge-dependent formation energies has well-publicized frailties associated with periodic boundary conditions for charged systems, but these may be somewhat reduced by employing schemes where the electrical levels of two or more systems are compared. Additionally, when comparing total energies for chemically and structurally similar systems in the PBC approach, the dispersion of the defect levels in the ﬁrst Brillouin-zone and multipole interaction, which are present even for neutral systems, are likely to be comparable and cancel to a large degree. In addition, for electrical levels in narrow-gap materials, such as germanium, the use of carefully constructed atomic clusters also signiﬁcantly reduces the underestimation of bandgaps in these methods, allowing a fully quantitative analysis of the levels in these materials. We have also shown that the marker method is eﬀective in wide-gap materials where excellent agreement may be obtained over the full range of the bandgap, provided that one has a suitable marker available. Since the marker method is applicable when looking at similar systems, it may be of particular use when studying dilute alloys such as SiGe. Here, a known marker in silicon (for a Si-rich alloy) could be used to determine the eﬀect of having a nearby Ge atom, such as that of VO centers in such alloys [52].

90

J.P. Goss et al.

The use of bulk materials as markers is a qualiﬁed success in the sense that single donor and acceptor levels are in many cases in good agreement with experiment. However, multiple charges introduce larger errors and, for example with the chalcogen species in silicon, the second donor levels are in much less good agreement. We conclude that where experimental data allow, the most accurate quantitative method for predicting electrical levels in crystalline semiconductors and insulators is by comparison of a chemically and structurally similar defect for which the electrical levels are known. Other marker species, including the bulk supercells, are likely to introduce larger errors, but in our experience even then the results are rather favorable. Acknowledgements The authors would like to thank J. Coutinho, R. Jones and colleagues for useful discussions and access to data presented in this Chapter.

References [1] G. Burns: Solid State Physics, International ed. (Academic, Orlando, Florida 1985) 69 [2] P. Hohenberg, W. Kohn: Phys. Rev. 136, 864 (1964) 69 [3] W. Kohn, L. J. Sham: Phys. Rev. 140, A1133 (1965) 69 [4] S. M. Sze: Physics of Semiconductor Devices, 2nd ed. (Wiley-Interscience, New York 1981) 70, 82, 87 [5] G. E. Engel, W. E. Pickett: Phys. Rev. B 54, 8420 (1996) 70 ¨ [6] A. Resende, R. Jones, S. Oberg, P. R. Briddon: Phys. Rev. Lett. 82, 2111 (1999) 70, 87 [7] J.-W. Jeong, A. Oshiyama: Phys. Rev. B 64, 235204 (2001) 70, 84 [8] J. P. Goss, P. R. Briddon, S. J. Sque, R. Jones: Diamond Relat. Mater. 13, 684 (2004) 70, 84, 88 [9] S. J. Sque, R. Jones, J. P. Goss, P. R. Briddon: Phys. Rev. Lett. 92, 017402 (2004) 70, 88 [10] R. Jones, P. R. Briddon: Identiﬁcation of defects in semiconductors, in M. Stavola (Ed.): Semicond. Semimet., vol. 51A (Academic, Boston 1998) Chap. 6, p. 287 71 [11] P. R. Briddon, R. Jones: Phys. Stat. Sol. B 217, 131 (2000) 71, 72, 80 [12] W. E. Pickett: Comput. Phys. Rep. 9, 115 (1989) 71 [13] D. R. Hamann, M. Schl¨ uter, C. Chiang: Phys. Rev. Lett. 43, 1494 (1979) 71 [14] G. B. Bachelet, D. R. Hamann, M. Schl¨ uter: Phys. Rev. B 26, 4199 (1982) 71 [15] N. Troullier, J. L. Martins: Phys. Rev. B 43, 1993 (1991) 71 [16] C. Hartwigsen, S. Goedecker, J. Hutter: Phys. Rev. B 58, 3641 (1998) 71 [17] J. P. Perdew, Y. Wang: Phys. Rev. B 45, 13244 (1992) 71 [18] S. Goedecker, M. Teter, J. Hutter: Phys. Rev. B 54, 1703 (1996) 71 [19] J. A. White, D. M. Bird: Phys. Rev. B 50, R4954 (1994) 71 [20] J. P. Perdew, K. Burke, M. Ernzerhof: Phys. Rev. Lett. 77, 3865 (1996) 71

Electrical Levels with Gaussian Bases [21] [22] [23] [24] [25] [26] [27] [28] [29] [30] [31] [32]

[33]

[34] [35] [36] [37] [38] [39] [40] [41] [42] [43] [44] [45] [46] [47] [48] [49] [50]

91

E. R. Cohen, B. N. Taylor: J. Res. Nat. Bur. Standards 92, 85 (1987) 77 H. J. McSkimin, P. Andreatch, Jr.: J. Appl. Phys. 35, 2161 (1964) 77 S. B. Zhang, J. E. Northrup: Phys. Rev. Lett. 67, 2339 (1991) 81 G. Makov, M. C. Payne: Phys. Rev. B 51, 4014 (1995) 81, 83 H. Nozaki, S. Itoh: Phys. Rev. E 62, 1390 (2000) 81 U. Gerstmann, P. De´ ak, R. Rurali, B. Aradi, T. Frauenheim, H. Overhof: Physica B 340–342, 190 (2003) 81 C. W. M. Castleton, S. Mirbt: Phys. Rev. B 70, 195202 (2004) 81 J. Shim, E.-K. Lee, Y. J. Lee, R. M. Nieminen: Phys. Rev. B 71, 035206 (2005) 81 ¨ J. Adey, R. Jones, D. W. Palmer, P. R. Briddon, S. Oberg: Phys. Rev. B 71, 165211 (2005) 82 P. De´ ak, B. Aradi, A. Gali, U. Gerstmann: Phys. Stat. Sol. B 325, 139 (2003) 82, 83 J. Coutinho, V. J. B. Torres, R. Jones, P. R. Briddon: Phys. Rev. B 67, 035205 (2003) 82, 83, 84, 85 S. F. J. Cox, E. A. Davis, S. P. Cottrell, P. J. C. King, J. S. Lord, J. M. Gil, H. V. Alberto, R. C. Vil˜ ao, J. Piroto Duarte, N. Ayres de Campos, A. Weidinger, R. L. Lichti, S. J. C. Irvine: Phys. Rev. Lett. 86, 2601 (2001) 82 D. M. Hofmann, A. Hofstaetter, F. Leiter, H. Zhou, F. Henecker, B. K. Meyer, S. B. Orlinskii, J. Schmidt, P. G. Baranov: Phys. Rev. Lett. 88, 45504 (2002) 82 C. G. Van de Walle: Phys. Rev. Lett. 85, 1012 (2000) 82 M. G. Wardle, J. P. Goss, P. R. Briddon: Phys. Rev. B 71, 155205 (2005) 82 H. G. Grimmeiss, E. Janz´em: in S. T. Pantelides (Ed.): Deep Centers in Semiconductors, 2nd ed. (Gordon and Breach, Switzerland 1996) p. 97 85 G. Pensl, G. Roos, C. Holm, E. Sirtl, N. M. Johnson: Appl. Phys. Lett. 51, 451 (1987) 85 G. Roos, G. Pensl, N. M. Johnson, C. Holm: J. Appl. Phys. 67, 1897 (1990) 85 R. E. Peale, K. Muro, A. J. Sievers: Mater. Sci. Forum 65–66, 151 (1990) 85 G. D. Watkins, J. W. Corbett: Phys. Rev. 121, 1001 (1961) 86 M. Pesola, J. von Boehm, T. Mattila, R. M. Nieminen: Phys. Rev. B 60, 11449 (1999) 86 L. W. Song, G. D. Watkins: Phys. Rev. B 42, 5759 (1990) 87 ¨ R. Jones, A. Carvalho, J. Coutinho, V. J. B. Torres, S. Oberg, P. R. Briddon: Sol. St. Phenom. 108–109, 697 (2005) 87 V. P. Markevich, I. D. Hawkins, A. R. Peaker, V. V. Litvinov, L. I. Murin, L. Dobaczewski, J. L. Lindstr¨ om: Appl. Phys. Lett. 81, 1821 (2002) 87 E. Gheeraert, S. Koizumi, T. Teraji, H. Kanada, M. Nesl´ adek: Phys. Stat. Sol. A 174, 39 (1999) 88, 89 P. A. Crowther, P. J. Dean, W. F. Sherman: Phys. Rev. 154, 772 (1967) 89 D. M. Hofmann, M. Ludwig, P. Christmann, D. Volm, B. K. Meyer, L. Pereira, L. Santos, E. Pereira: Phys. Rev. B 50, 17618 (1994) 89 R. N. Pereira, W. Gehlhoﬀ, N. A. Sobolev, A. J. Neves, D. Bimberg: J. Phys. Condens. Matter 13, 8957 (2001) 89 J. W. Steeds, S. J. Charles, J. Davies, I. Griﬃn: Diamond Relat. Mater. 9, 397 (2000) 89 R. Farrer: Solid State Commun. 7, 685 (1969) 89

92

J.P. Goss et al.

[51] G. Davies: J. Phys. C 9, L537 (1976) 89 ¨ [52] V. P. Markevich, A. R. Peaker, J. Coutinho, R. Jones, V. J. B. Torres, S. Oberg, P. R. Briddon, L. I. Murin, L. Dobaczewski, N. V. Abrosimov: Phys. Rev. B 69, 125218 (2004) 89

Index acceptor, 69, 71, 81, 83, 84, 86–88, 90 AIMPRO, 71, 72, 75, 76, 80, 81, 84, 87, 88 algorithm, 74 all-electron, 72, 76 background charge, 70 band edge, 84 band structure, 79 basis set, 69, 71–80 Bloch, 71 bond-centered, 74 boron, 81, 84, 87 Brillouin zone, 84, 89 bulk, 74, 76, 79, 84, 86, 90 bulk modulus, 76, 77, 79 carbon, 80, 87 chalcogen, 84, 85, 90 charge state, 70, 80, 81, 86 chemical potential, 80 cluster, 70, 71, 80, 81, 84, 87, 89 complex, 81, 84–86 concentration, 69 conduction band, 79 conductivity, 69 conformation, 81 conjugate gradient, 75 core, 71, 72 correlation, 86 covalent, 78 deep level, 69, 71, 84, 87 density-functional theory, 69 DFT, 69–71, 82, 86, 89 diamond, 70, 78, 79, 81, 83, 84, 87, 88 dipole, 81 dispersion, 84, 85, 89 DLTS, 85 donor, 69–71, 80, 82, 84–88, 90

dopant, 69, 70, 80, 89 doping, 87 electrical level, 71, 80, 81, 88–90 electron, 69–71, 80, 81, 86, 87 electrostatic energy, 70 empirical, 85, 86, 88 energy barrier, 81 equilibrium, 81 exchange-correlation, 71 ﬁrst principles, 72 ﬂuctuation, 72, 74 formation energy, 80, 81, 88 Fourier, 69 gap, 81, 82, 89 Gaussian, 71–73, 75, 76, 79, 80 Ge, 70, 87, 89 general gradient approximation, 70 germanium, 84, 86, 89 GGA, 70, 71, 82, 89 ghost, 74 Hamiltonian, 72–75, 79 Hartree–Fock, 74 hole, 69 hydrogen, 70, 82, 84 hyperﬁne, 71 impurity, 80 interstitial, 87 ionization, 69, 87 Kohn–Sham, 82 LDA, 71, 77, 82, 89 Madelung, 81, 85 magnetic, 72 Makov–Payne, 83

Electrical Levels with Gaussian Bases marker, 71, 80, 82–90 metastablity, 82 migration, 71 mobility, 69 molecular dynamics, 71 Mulliken, 84 multipole, 83, 89 narrow-gap, 84, 89 optical, 69, 87 oxygen, 86 Perdew–Wang, 71 periodic, 70, 71 periodic boundary conditions, 69, 89 periodicity, 84 phosphorus, 70, 87 plane wave, 69–73, 80 pnictogen, 88 polarization, 74, 78 population, 84 potential, 70, 74, 79–84, 87 pseudopotential, 71, 72, 76

real space, 71, 72 recombination, 69 scattering, 69 shallow, 70, 71, 82, 84, 85, 87, 88 Si, 75, 77, 79, 87 SiGe, 89 silicon, 75, 76, 78, 80, 81, 84–90 spherical harmonics, 72 spin, 84 strain, 79 substitutional, 83, 84, 87 supercell, 70, 81, 84, 86–88, 90 surface, 70, 72, 74, 75, 81 temperature, 69, 80, 81, 87 total energy, 73, 75, 79 transition, 81–83 ultrasoft pseudopotential, 70

quadrupole, 81

vacancy, 81, 86 valence band, 81–83, 88 variational, 73 vibrational modes, 71, 84, 85

radiative, 69

ZnO, 82

93

Dynamical Matrices and Free Energies Stefan K. Estreicher and Mahdi Sanati Physics Department, Texas Tech University, Lubbock, TX 79409-1051 [email protected]

Abstract. The calculation of the entire dynamical matrix of a periodic supercell (containing a defect or not) provides several most useful pieces of information. At ﬁrst, the eigenvalues of this matrix are all the normal mode frequencies of the cell, including the local, pseudolocal, and resonant modes associated with the defect under study. The eigenvalues can also be used to construct phonon densities of state which in turn allow the calculation of (Helmholtz) free energies, vibrational entropies, and speciﬁc heats. The eigenvectors of the dynamical matrix can be used to prepare a system in thermal equilibriumat a desired temperature. This allows constant-temperature MD simulations to be peformed without thermalization or thermostat. Applications to the calculation of vibrational lifetimes and decay channels are discussed. Finally, the vibrational, rotational, and charge-carrier contributions to the free energy are described. Conﬁgurational entropies are calculated in realistic systems.

1 Introduction Vibrational spectroscopy provides essential experimental data about defects in semiconductors, not only because of the microscopic nature of the information it provides but also because many of the quantities measured can be calculated from ﬁrst principles. Fourier transform infrared absorption (FTIR) and Raman spectroscopies often produce sharp lines associated with local vibrational modes (LVMs) of impurities lighter than the hosts atoms. These lines are often above the highest normal mode of the crystal, the Γ phonon but, when the phonon density of states has a gap (as in the case of GaN [1]), they can be between the acoustic and optic modes as well. Isotope substitutions provide element identiﬁcation as well as information about how many atoms of a given species are part of the defect. Uniaxial stress experiments give the symmetry of the defect through the splitting of the IR or Raman lines. Annealing studies provide various activation energies. Examples of such studies and a discussion of the techniques are found in [2]. By themselves, the measured LVMs, isotope shifts, symmetry, and activation energies are often insuﬃcient to identify a unique structure for the defect. However, they are precious to theorists who use ﬁrst-principles techniques to calculate the structures (symmetry), LVMs and their isotope shifts, binding, migration and/or reorientation energies, and thus prove or disprove D. A. Drabold, S. K. Estreicher (Eds.): Theory of Defects in Semiconductors, Topics Appl. Physics 104, 95–114 (2007) © Springer-Verlag Berlin Heidelberg 2007

96

Stefan K. Estreicher and Mahdi Sanati

the assignment of an IR or Raman spectrum to a speciﬁc defect. The interplay between vibrational spectroscopy and ﬁrst-principles theory has led to the unambiguous identiﬁcation of many defects and has provided realistic tests of the accuracy of theory. For many years, the calculation of defect-related vibrational modes has been limited to those LVMs that are IR or Raman active. The stretch mode of a Si–H bond, in a Si vacancy for example, can be predicted quite accurately by calculating the total energy of a supercell containing this defect in its equilibrium conﬁguration as well as for several (at least 2) positions of H along the Si–H bond. The 1-dimensional potential along this axis is ﬁtted to a polynomial and the frequency and zero-point energy of this mode are calculated. The same can also be done for wag modes. There are many examples of such calculations [3–5]. This method works well, but a lot of additional and very useful information can be obtained when the entire dynamical matrix of the supercell is calculated. For a system of N atoms and therefore 3N normal modes, the dimension of this matrix is 3N × 3N and its calculation is computationally expensive. The eigenvalues of the dynamical matrix are all the normal mode frequencies of the supercell: acoustic and optic phonons as well as defectrelated modes. These can be LVMs, located above the Γ phonon, resonant and/or pseudolocal vibrational modes (pLVMs). Resonant modes occur when the strain (associated with a defect) stretches or compresses host–atom bonds, resulting in new vibrational frequencies near the Γ phonon. pLVMs are localized impurity-related modes buried in the phonon continuum. Such modes are sometimes visible experimentally as phonon sidebands in photoluminescence (PL) spectra [6, 7]. Two copper-related centers in Si have recently been theoretically identiﬁed [8,9] thanks to such pLVMs. Further, the knowledge of all the normal mode frequencies allows the construction of phonon densities of state, which are needed to calculate (Helmholtz) free energies. The eigenvectors of the dynamical matrix make it possible to ﬁnd (and identify the symmetry of) all the localized modes associated with any atom or group of atoms in the supercell. The eigenvectors can also be used to prepare the supercell in thermal equilibrium and any temperature, thus allowing constant-temperature molecular dynamics (MD) simulations to be performed without the need for thermalization or even a thermostat. This in turn makes it possible to calculate vibrational lifetimes and decay channels of speciﬁc modes as a function of temperature. For all these reasons, the calculation of dynamical matrices is well worth its cost. Our results are obtained from self-consistent, ﬁrst-principles theory based on local density-functional theory in 64-host-atom periodic supercells. The calculations are performed with the SIESTA code [10, 11]. The exchangecorrelation potential is that of Ceperley–Alder [12] as parameterized by Perdew and Zunger [13]. Norm-conserving pseudopotentials in the Kleinman– Bylander form [14] are used to remove the core regions from the calculations. The basis sets for the valence states are linear combinations of numerical

Dynamical Matrices and Free Energies

97

atomic orbitals of the Sankey type [15–17], generalized to be arbitrarily complete with the inclusion of multiple-zeta orbitals and polarization states [10]. We use double-zeta (two sets of s and p orbitals) for ﬁrst- and second-row atoms (H through Ne) and add a set of polarization functions (e.g., one set of d orbitals) for third-row atoms and below. The charge density is projected on a real-space grid with an equivalent cutoﬀ of 150 Ry to calculate the exchange-correlation and Hartree potentials. A 2 × 2 × 2 Monkhorst–Pack k-point sampling [18] is used to optimize the structures. An overview of dynamical matrices is given in Sect. 2. Examples of LVMs and pLVMs are given in Sect. 3. The calculation of vibrational lifetimes is given in Sect. 4. Vibrational free energies and speciﬁc heats are discussed in Sect. 5, and the properties of defects at ﬁnite temperatures in Sect. 6.

2 Dynamical Matrices The calculation of dynamical matrices is a well-known topic discussed in many textbooks, such as [19]. Further, the calculation of the force-constant matrix F is implemented in many (if not all) software packages that have MD capabilities. The brief summary below is therefore only necessary in order to deﬁne the notation to be used in this Chapter and make a few comments. We consider a solid represented by periodic supercells of N atoms of mass mα (with α = 1, 2, . . . , N ). The nuclei oscillate around their equilibrium positions. The dynamical matrix is related to the force-constant matrix by Fαβ,ij Dαβ,ij = √ , mα mβ

(1)

where i, j = x, y, z are Cartesian indices. The calculation of Fαβ,ij is computationally intensive for the type of systems required in the study of defects in semiconductors. Today’s typical supercells contain of the order of 100 atoms, and there is little doubt that several hundred (or even thousand) atoms will become the norm in the near future. Once F is known, changing the masses of selected atoms (that is, playing with isotopes) is trivial. Techniques to calculate F are well known, ranging from the direct “frozen phonon” approach implemented in many MD software packages to MD-based methods based on correlation functions [20, 21], or linear-response theory [22–25]. Note that dynamical matrices can also be computed using order-N methods [26]. The eigenvalues of the dynamical matrix are the normal mode frequencies of the system ωs , and the corresponding eigenvectors esα,i are orthonormal: α,i

esα,i esα,i = δss

and

s

esα,i esβj = δαβ δij .

(2)

98

Stefan K. Estreicher and Mahdi Sanati

In the harmonic approximation, the normal-mode coordinates qs are √ qs (t) = As cos(ωs t + ϕs ) = mα uα,i esα,i ,

(3)

α,i

where the amplitudes As are temperature dependent and the uα,i are Cartesian displacements of the nucleus α away from equilibrium. This relationship can be used to prepare a system in equilibrium at a temperature T , then perform MD runs at constant temperature without the need for thermalization or even a thermostat [27]. Indeed, the unknown amplitudes of the normal modes can be obtained by requiring that the kinetic energy of each mode is, on the average, kB T /2, that is 1 ∂q 2 s

2

∂t

=

1 2 2 2 ωs As

sin2 (ωs t + ϕs ) = 14 ωs2 A2s = 12 kB T .

(4)

√ Thus, the average amplitude of the normal mode s is As = 2kB T /ωs . Note that assigning the amplitudes As = As to each mode s implies that the total energy of each mode is exactly kB T . It is better to pick a random distribution Es 1 −E/kB T e dE (5) ζs = k BT 0 with 0 < ζs < 1. This leads to As = −2kB T ln(1 − ζs )/ωs . Thus, in the harmonic approximation, the Cartesian coordinates and corresponding velocities needed to prepare the system in equilibrium at the temperature T are 2kB T 1 uαi = − ln(1 − ζs ) cos(ωs t + ϕs )esαi , (6) mα s ω s and ∂uαi =− ∂t

2kB T − ln(1 − ζs ) sin(ωs t + ϕs )esαi . mα s

(7)

The initial phases 0 ≤ ϕs < 2π are random, as each mode has a random amount of kinetic and potential energy at the time t = 0. A similar transformation has been used by Gavartin and Stoneham [28] to calculate the energy dissipation in quantum dots. However, we discuss it here in the context of establishing initial conditions with the appropriate random distribution of energies and phases. This is used in Sect. 4 to calculate vibrational lifetimes and decay channels from ﬁrst principles.

Dynamical Matrices and Free Energies

99

Fig. 1. LVMs pLVMs associated with H+ bc in the Si64 supercell. The plots and 2 s 2 |e | , where α is H (left), or its two Si nearest neighbors (right) of d (α) = α,i i show the vibrational modes localized on the impurity and its two Si neighbors. The vertical dashed lines show the calculated Γ phonon

3 Local and Pseudolocal Modes The simplest and most immediate consequence of the knowledge of the dynamical matrix is the identiﬁcation of all the localized modes of a defect, and their symmetry. Indeed, a plot of i |esα,i |2 vs. s (that is, vs. the normal mode frequencies ω) for a speciﬁc atom α (or set of atoms) provides quantitative information about the localization of the modes associated with the given atom(s). For example, Fig. 1 shows the localized modes associated with bond-centered (bc) hydrogen in crystalline Si (H+ bc ): the asymmetric stretch (IR active) of H is a LVM at 2004 cm−1 (observed [29] at 1998 cm−1), the two degenerate wag modes (not observed) are pLVMs, far below the Γ phonon, at 264 cm−1 , and the symmetric stretch is a pLVM at 452 cm−1 (also not observed). The latter does not involve any H motion at all, but shows up when i |esα,i |2 includes the two Si nearest neighbors to H. Figure 2 shows the eigenvectors of the dynamical matrix in one of the two degenerate wag modes at 264 cm−1 . The H displacement in this mode accounts for about 70 % the displacements of all the atoms in the cell. Note that the eigenvectors only give the relative amplitudes of the atomic displacements. Their absolute values depend on the temperature, and are exaggerated in the ﬁgure. Thus, plotting i |esα,i |2 quantiﬁes the localization of all the local modes associated with an atom or group of atoms. The corresponding eigenvectors allow the identiﬁcation of the symmetry of the mode, which is needed to establish whether a mode is IR active or not, and whether it can produce phonon sidebands in PL spectra or not [6]. This is precisely how two lowfrequency copper-related defects have recently been identiﬁed [8, 9]. A very

100

Stefan K. Estreicher and Mahdi Sanati

Fig. 2. Eigenvectors of the dynamical matrix in one of the 264 cm−1 wag modes of H+ bc . The H atom is the small black ball, the gray balls are all Si. The size of the arrows is exaggerated to make the smaller oscillation amplitude more visible. The arrows only show the relative amplitudes of the motion of the atoms in this mode

useful software package1 readily reads dynamical matrices and graphically displays the eigenvectors for any chosen normal mode.

4 Vibrational Lifetimes and Decay Channels The vibrational lifetimes of the LVMs of light impurities in Si have recently been measured by transient bleaching spectroscopy [30, 31]. Surprisingly, the lifetimes of nearly identical H-related LVMs diﬀer by some two orders of magnitude. For example, at low temperatures, the measured lifetimes of the 2072 cm−1 mode of the divacancy–dihydrogen complex (VH · HV), the −1 1998 cm−1 mode of H+ mode of the H∗2 pair [31] are bc [30], and the 2062 cm 295 ps, 8 ps, and 4 ps, respectively. Since the decay of all these modes must involve at least four phonons (six phonon processes are proposed [29, 31]), it is not clear why the lifetimes of LVMs with almost identical frequencies vary by two orders of magnitude or why any of them would be short-lived at all. 1

For information about the Molekel visualization package, see www.cscs.ch/ molekel/.

Dynamical Matrices and Free Energies

101

The calculations of vibrational lifetimes begin with the dynamical matrices of the supercells containing the defects. The eigenvectors of this matrix determine the equilibrium background temperature of the cell at the time t = 0, as discussed in Sect. 2. This is used to prepare the cell in equilibrium at the same sample temperatures as in the experimental work. The initial excitation of the LVM of interest is assigned to be its zero-point energy plus one phonon, that is 3ω/2 (kinetic energy at t = 0). This mimics the laser excitation of the speciﬁc LVM. Then, constant-temperature (classical) MD simulations are performed, with a time step of 0.3 fs in the case of H. Since ab initio MD simulations are limited to real times of a few times 10 ps, it is critical to be able to begin the MD runs at a relatively elevated background temperature, because the measured lifetimes are much shorter at higher temperatures. The calculations are then repeated at lower temperatures to monitor the increase in the lifetime until such low temperatures that the calculations become computationally prohibitive. Note that at very low temperatures, all the normal modes of the system have amplitudes consistent with their zero-point energy. In classical MD simulations, these amplitudes go to zero, the modes become harmonic and the lifetimes very long [27]. At every time step, the 3N Cartesian coordinates of the atoms are written as linear combinations of the 3N normal modes of the supercell. Thus, the energies of all the modes can be plotted as a function of time. This approach allows not only the decay of the LVM of interest to be calculated, but also the identiﬁcation of the receiving modes, all of it as a function of time for various background temperatures of the cell. The pLVMs of the defect play a critical role in the decay process. We illustrate this approach with the case of the asymmetric stretch of H+ bc [30]. The result of the run performed at a background temperature of 75 K is shown in Fig. 3. The calculated decay of the LVM produces a good exponential ﬁt leading to a calculated lifetime of 7.8 ps at 75 K, a value that agrees very well with experiment [30]. An analysis of the time dependence of the energies of the normal modes of the cell shows that both wag modes and the symmetric stretch of the defect (at 262 cm−1 and 452 cm−1 , respectively) play important roles in the decay.

5 Vibrational Free Energies and Speciﬁc Heats Although the calculation of potential-energy surfaces is playing a most useful role in our understanding of the behavior of defects in semiconductors, the real-world involves nonzero temperatures. Samples undergo various thermal anneals, they are implanted and exposed to light, and most devices function at or above room temperature. The physics and chemistry of defects is obviously temperature dependent, as one observes processes such as diﬀusion and association or dissociation at various temperatures.

102

Stefan K. Estreicher and Mahdi Sanati

−1 Fig. 3. Plot of the energy (eV) of the asymmetric stretch mode of H+ bc at 2004 cm in the Si64 supercell, at the background temperature of 75 K vs. time (ps). The energies of 194 other modes of the cell are plotted as well. The ﬁrst step of the decay involves the pLVMs of the defect, which themselves have very short lifetimes

In all these processes, the Gibbs free energy is the most relevant quantity since virtually all experiments are done at constant pressure. However, we focus here on the Helmholtz free energy. Working at constant volume rather than constant pressure is appropriate up to several hundred degrees Celsius in most semiconductors because their thermal expansion coeﬃcient is very small. In Si for example, this coeﬃcient is 4.68 ×10−6 K−1 at room temperature and the phonon frequencies shift slowly with T . Indeed, the diﬀerence between the constant-pressure and constant-volume speciﬁc heats [32]2 CP − CV is 0.0165 J/mol · K at room temperature, a correction of only 0.08 % to CP = 20 J/mol · K. Thus, in the case of semiconductors such as Si and in the temperature range where the use of harmonic dynamical matrices is justiﬁed, calculating the phonon density of states g(ω) at T = 0 K and ignoring the temperature dependence of the lattice constant are reasonable approximations. Note that this ignores the frequency shifs associated with the anharmonicity. This greatly simpliﬁes the calculations. In fact, it renders them possible since calculating temperature-dependent phonon densities of state is a formidable task. 2

In this paper, “cal/g atom” should read “cal/mol” (or the numbers be divided by the atomic mass of Si).

Dynamical Matrices and Free Energies

103

Fig. 4. Phonon densities of state g(ω) calculated from harmonic dynamical matrices of the Si64 supercell evaluated at 90 q points in the BZ of the cell. The dashed line (ﬁrst peak at low frequency) was obtained with a double-zeta basis set and a 1×1×1 Monkhorst–Pack k-point sampling, the solid line (second peak) with a double-zeta polarized basis set and a 2 × 2 × 2 k-point sampling, and the long-dash line with a double-zeta polarized basis set and a 1 × 1 × 1 k-point sampling. As expected, the solid line best matches the experimental data [33]

The phonon densities of states of perfect (defect-free) crystals are normally calculated from the dynamical matrix of the primitive unit cell evaluated at thousands of q points in the Brillouin zone (BZ) of the crystal. When studying defects, large periodic supercells must be used, and the BZ of the supercell is distinct from that of the perfect solid. The eigenvalues of the dynamical matrix only provide a small number of normal mode frequencies, and the phonon density of states extrapolated from those few hundred frequencies lead to rather poor g(ω)s. However, evaluating the dynamical matrix at many q points in the BZ of the supercell works very well. Figure 4 shows three phonon densities of state obtained from harmonic dynamical matrices extrapolated at about 90 q points in the BZ of the supercell. The dynamical matrices were calculated with diﬀerent basis sets and Monkhorst–Pack k-point sampling in the Si64 supercell. The best ﬁt to the measured data [33] is obtained with the largest basis set (double-zeta polarized) and k-point sampling (2 × 2 × 2). In the harmonic approximation, the Helmholtz free energy is given by ∞ ln{sinh(ω/2kB T )}g(ω) dω , (8) Fvib (T ) = kB T 0

104

Stefan K. Estreicher and Mahdi Sanati

Fig. 5. Calculated and measured peak in the speciﬁc heat over T 3 for various isotopically pure samples of Ge. The dashed line (expt: crosses) is for 73 Ge, the solid line (expt: circles) is for the natural isotopic abundance, and the dotted line (expt: squares) is for 70 Ge

where kB is the Boltzmann constant. In the perfect cell, the integration is carried out up to the Γ phonon. With a defect in the supercell, the integral extends up to the highest normal mode of the cell (perturbed Γ phonon) and becomes a simple sum for the higher LVMs. Note that Fvib (T = 0) gives the total zero-point energy. Once Fvib is calculated, the vibrational entropy and speciﬁc heat at constant volume are given by 2 ∂Fvib ∂ Fvib CV = −T . (9) Svib = − ∂T ∂T 2 V V The latter can be compared to the measured Cp in order to determine up to what temperature the constant-volume and harmonic approximations are appropriate. We have demonstrated that the approximations work quite well up to some 700 K in the case of c-C, Si, Ge, and GaN (see [1, 34, 35]), and that the agreement with even ﬁne features is very good at low temperature. Figure 5 shows the calculated isotope-dependent peak in C/T 3 in Ge. The temperature at which it is predicted to occur and the splitting associated with various isotopes quantitatively reproduce the experimental data [36]. These tests give us conﬁdence that the phonon densities of states calculated in the manner described above are also accurate when defects are present in the same supercell, and therefore that the calculated Helmholtz vibrational free energies are accurate up to several hundred degrees Celsius. Of course, the Fvib obtained for a defect in a 64-host-atom cell correspond to a defect concentration of about 1.5 atomic per cent, which is very high. However, the few calculations we have performed with 128- and 216-atom cells

Dynamical Matrices and Free Energies

105

show that cell-size eﬀects are not very signiﬁcant, probably because g(ω) is only the weight function used in the integration, and small changes in this function have a minor impact on the result.

6 Theory of Defects at Finite Temperatures We are always interested in energy diﬀerences. This could be the energy diﬀerence between two conﬁgurations of the same defect, the energy diﬀerence between a bound complex and its dissociation products (binding energy), etc. At ﬁnite temperatures, such a total free-energy diﬀerence may contain several contributions: ∆F = ∆U + ∆Fvib + ∆Fe/h + ∆Frot + · · · − T ∆Sconﬁg .

(10)

∆U is the potential-energy diﬀerence obtained (in this Chapter) from ﬁrstprinciples density-functional theory. The vibrational free energy ∆Fvib has been discussed above. Depending on the defect under study, there may be diﬀerent concentrations of electrons (in the conduction band) or holes (in the valence band) because diﬀerent conﬁgurations of a given defect have diﬀerent electrical activities. This has nothing to do with the electrons or holes provided by the background dopants, which can be numerous. Instead, ∆Fe/h refers only to the change in the number of free carriers associated with the two conﬁgurations of the defect under study and the contributions of the background (dopant-associated) charge carriers cancel out. Unless one is dealing with unusually high changes in carrier concentrations, this term is very small and can be neglected [37]. Additional contributions to the free energy are associated with energy levels arising from rotational, magnetic, spin or other degrees of freedom speciﬁc to a particular defect. These terms can often be calculated directly from the appropriate partition functions [37]. One example is provided by the rotational free energies of interstitial H2 , HD, and D2 molecules (for a review of interstitial hydrogen molecules in semiconductors, see [38]) in Si. The rotational energies are Ej = j(j + 1)2 /M R2 , where M is the nuclear mass and R the internuclear separation. Since H2 consists of two protons (fermions), there are three ortho states (even combinations of spin: ↑↑, ↓↓, and ↑↓ + ↓↑) for which only odd values of j are allowed, and one para state (odd combination of spin: ↑↓ − ↓↑) for which only even values of j are allowed. This leads to the familiar set of two Raman lines with 3 : 1 intensity ratio. Since D2 consists of two bosons, the total wavefunction must be symmetric, and a similar argument leads to two Raman lines with 1 : 2 intensity ratios. Thus, the rotational free energy per molecule is given by Frot (T ) = −go kB T ln Zo − gp kB T ln Zp ,

(11)

106

Stefan K. Estreicher and Mahdi Sanati

where the partition functions are Zo = Σj=1,3,5,... (2j + 1)e−j(j+1)θ/T Zp = Σj=0,2,4,... (2j + 1)e

−j(j+1)θ/T

(12) ,

(13)

and {go , gp } = {3/4, 1/4} for H2 and {1/3, 2/3} for D2 . Since HD has no symmetry restrictions, all the values of j are allowed (single Raman line) and Frot (T ) = −kB T ln Z with Z = Σj (2j + 1)e−j(j+1)θ/T . The eﬀective temperature θ = 2 /2IkB contains the (classical) moment of inertia I of the molecule, which depends on the host. For free H2 , θ = 85.4 K. In Si, the molecule has a longer bond length than in free space [39] and θ = 73.0 K, 48.7 K and 36.5 K for H2 , HD and D2 , respectively. The values of the rotational free energies at 77 K, 300 K, and 800 K for interstitial H2 , HD, and D2 in Si are in Table 1. The largest rotational free energy per molecule occurs in the case of HD. When comparing the free energies of the interstitial H2 molecule with the interstitial H∗2 complex (which consists of a Si–Si replaced by two Si–H bonds: Si–Hbc · · · Si–Hab along a trigonal axis) which has no rotational degrees of freedom, the sum ∆Fvib + ∆Frot clearly favors H2 at higher temperatures [37]. This prediction is consistent with the fact that samples hydrogenated at high temperatures then rapidly quenched [40] show the presence of only H2 molecules. Table 1. Rotational free energy Frot (eV) for interstitial H2 , HD, and D2 in Si T (K)

77

300

800

H2 HD D2

−0.005 −0.004 −0.004

−0.030 −0.048 −0.040

−0.129 −0.194 −0.168

The importance of the conﬁgurational entropy term depends on the situation. When comparing the two metastable conﬁgurations of the CH∗2 complex [37], ∆Sconﬁg is exactly zero. When comparing interstitial H2 and H∗2 , the conﬁgurational entropy contribution is not zero but very small. Indeed, interstitial H2 occupies tetrahedral interstitial (t) sites, while H∗2 is at a bc site. Since there are twice as many bc as t sites, a (very) small ∆Sconﬁg results. The situation is very diﬀerent when calculating binding free energies. Indeed, for a complex {A, B} with dissociation products A and B, there are often vastly diﬀerent numbers of conﬁgurations for the dissociated species than for the complexes, sometimes leading to large values for ∆Sconﬁg . The calculation must be done using realistic concentrations of the species involved, and its details depend on the speciﬁc situation. The diﬀerence in conﬁgurational entropy per complex is ∆Sconﬁg = (kB /[{A, B}]) ln(Ωpair /Ωnopair ), where [{A, B}] is the number of complexes,

Dynamical Matrices and Free Energies

107

and Ωpair and Ωnopair are the number of conﬁgurations with all possible complexes forming and with all complexes dissociated, respectively. We set {A, B} to be “dissociated” when no B species is within a sphere of radius rc (eﬀective capture radius) of any A. The results are not very sensitive to the actual value of rc . The sites of A, B, and {A, B} are known and the concentrations [A] and [B] are estimated from experiment. If [A] is larger than [B], the maximum number of complexes is [{A, B}] = [B]. Although a real sample has traps for the dissociation products A and/or B that are distinct from isolated A and/or B in a perfect crystal, we ignore this additional complication. We consider here two boron–oxygen complexes in Si. Both of them contain an interstitial oxygen dimer ({Oi }2 ) trapped at either substitutional (Bs ) or interstitial (Bi ) boron. Thus, we consider the binding free energies of the {Bs , Oi , Oi } and {Bi , Oi , Oi } complexes (both in the +1 charge state). We do not discuss here the reasons why these complexes are important, how they form, and the consequences of complex formation for the sample at hand. These issues are discussed elsewhere [41, 42]. The conﬁgurations of the complexes and their dissociation products have been obtained from conjugate gradient geometry optimizations in the appropriate charge states. The binding energies at T = 0 K are ∆U = 0.54 eV and 0.61 eV for {Bs , Oi , Oi } and {Bi , Oi , Oi }, respectively. All the vibrational free energies have been calculated. We are faced now with the calculation of ∆Sconﬁg . Since we know the equilibrium sites of all the species involved, we know the number of equivalent orientations. However, we need to assume the concentrations of the various species in order to calculate the total number of conﬁgurations. We assume a sample with N = 5 × 1022 substitutional sites, [{Oi }2 ] = 1014 oxygen dimers, [Bs ] = 1019 substitutional and [Bi ] = 1014 interstitial boron impurities. The numbers depend on the sample, but these are realistic values that could correspond to an actual experimental situation. In a 1 cm3 sample, the number of sites for Bs , split-interstitial sites for Bi and staggered or square conﬁgurations [42] for {Oi }2 is 5 × 1022 . At low temperatures, all the Bs s trap one {Oi }2 . The number of ways one can arrange [{Oi }2 ] dimers among N sites is N !/[{Oi }2 ]!(N − [{Oi }2 ])!. Each {Oi }2 traps at one Bs and each {Bs , Oi , Oi } has 12 equivalent orientations. leading to 12[{Oi }2 ] possibilities. The remaining [Bs ] − [{Oi }2 ] borons are distributed among the remaining N − 12[{Oi }2 ] sites. Thus, the number of conﬁgurations for {Bs , Oi , Oi } complexes is Ωpairs =

12[{Oi }2 ] N !(N − 12[{Oi }2 ])! . [{Oi }2 ]!(N − [{Oi }2 ])!([Bs ] − [{Oi }2 ])!(N − [Bi ] − 11[{Oi }2 ])! (14)

At high temperatures, all the {Bs , Oi , Oi } complexes are dissociated. We can arrange [Bs ] borons among N substitutional sites in N !/[Bs ]!(N − [Bs ])! ways. If rc = 10 ˚ A, no oxygen dimer is within a sphere of radius 10 ˚ A of any boron, implying that about 150 substitutional sites around each Bs are

108

Stefan K. Estreicher and Mahdi Sanati

not allowed, which means that the number of sites available for the [{Oi }2 ] oxygen dimers is N − 150[Bs ]. The number of conﬁgurations for the {Oi }2 ’s is therefore (N − 150[Bs ])!/[{Oi }2 ]!(N − 150[Bs ] − [{Oi }2 ])!. Thus, the number of conﬁgurations for the dissociated complexes is Ωnopairs =

N !(N − 150[Bs ])! . [Bs ]!(N − [Bs ])![{Oi }2 ]!(N − 150[Bs ] − [{Oi }2 ])!

(15)

Using Sterling’s formula and an expansion for ln(1 + ε) with ε 1, we get 12[Bs ] 278[Bs ] [{Oi }2 ] ∆Sconﬁg = kB ln + − . (16) N N [Bs ] Similar calculations for {Bi , Oi , Oi } lead to [Bi ] [{Oi }2 ] 24[{Oi }2 ] − 1 + 32 + ∆Sconﬁg = kB ln . N N N

(17)

With the concentrations assumed, this gives ∆Sconﬁg = −0.515 meV/K and −1.538 meV/K for {Bs , Oi , Oi } and {Bi , Oi , Oi }, respectively. The diﬀerence between these situations is huge, and the reason for it is quite obvious. Consider an {A, B} complex that dissociates into A and B. If A and/or B are abundant (as is the case for Bs ), there are many conﬁgurations resulting in pairs and relatively few conﬁgurations with A away from B. On the other hand, when both A and B are scarce (as is the case for Bi and {Oi }2 ), there are far fewer ways to make pairs and a great number of dissociated conﬁgurations. The binding free energies of the {Bs , Oi , Oi } and {Bi , Oi , Oi } complexes are plotted as a function of temperature in Fig. 6. As shown in [41], the contribution of ∆Fvib is very small and the slope is almost entirely determined by the diﬀerence in conﬁgurational entropy. Thus, for a given {A, B} complex, the smaller the concentration of A or B, the larger the conﬁgurational entropy associated with the dissociated species and the smaller the entropy associated with complex formation. Then, the slope of the binding free energy Eb (T ) is much steeper. The opposite holds if A and/or B exist in high concentrations. In the example discussed in this Chapter, changing one component of the complex from Bs to Bi changes the relevant concentration from 1019 to 1014 , and this change of ﬁve orders of magnitudes roughly triples ∆Sconﬁg . Note that above the temperature T0 where Eb (T0 ) = 0, the interactions become repulsive. The value of T0 depends on Eb (0) and on the slope, that is on ∆Sconﬁg , which in turn depends on the concentrations of the dissociation products in the sample.

7 Discussion First-principles calculations of the properties of defects in periodic supercells have become quantitative in many respects. The conﬁgurations, energetics,

Dynamical Matrices and Free Energies

109

Fig. 6. Binding free energies of the {Bs , Oi , Oi } and {Bi , Oi , Oi } complexes in Si. The latter complex will not form above room temperature, where the interactions between Bs and {Oi }2 are repulsive because of conﬁgurational entropy

selected LVMs, spin densities and, to a lesser extent, electrical activities of localized defects can be predicted with very good accuracy. However, the knowledge of the entire dynamical matrix of the system provides much more information. The eigenvalues of this matrix give all the local, pseudolocal, and resonant defect-related modes, as well as the crystal phonon frequencies. They can be used to obtained high-quality phonon densities of states that in turn allow the calculation of vibrational free energies. Although the latter are limited to the constant-volume (and, in our case, harmonic) approximation, the calculated speciﬁc heats show that the results are reliable up to several hundred degrees Celsius. The eigenvectors of the dynamical matrix allow the localization of local modes to be quantiﬁed and their symmetry predicted. The eigenvectors can also be used to prepare a system in thermal equilibrium at any temperature without the need for lengthy thermalizations or even a thermostat. This feature is needed to calculate vibrational lifetimes as a function of temperature. The calculation of defect energetics at ﬁnite temperatures is relatively straightforward once the vibrational free energy is known. Indeed, rotational and other contributions can be obtained (or approximated) analytically. The most tricky, and sometimes most critical, part is the contribution of the conﬁgurational entropy. One example has been discussed here in detail. The result depends on the concentrations of the species involved, that is, on the sample. The binding free energy of an {A, B} complex in a crystal varies linearly with temperature, with a slope largely dominated by the diﬀerence in

110

Stefan K. Estreicher and Mahdi Sanati

conﬁgurational entropy between {A, B} and A away from B. If R is a dissociation rate, R exp{−Eb /kB T } = R exp{∆Sconﬁg /kB } exp{−Eb (0)/kB T }, and an Arrhenius plot yields a straight line with slope −Eb (0)/kB and intercept (ln R + ∆Sconﬁg /kB ). Thus, Arrhenius plots of the dissociation of an {A, B} complex in samples containing diﬀerent concentrations of A and/or B should produce parallel lines since the slopes are the same but the intercepts diﬀer. This suggests a way to measure conﬁgurational entropies. If we take R = 1011 and ∆Sconﬁg = −0.5 meV/K or −1.0 meV/K, the intercepts will be at 25.3 − 5.8 = 19.5 or 25.3 − 11.6 = 13.7, a measurable change. Even though the potential energy surface describing the interactions between A and B has a pronounced minimum when the {A, B} complex forms, these interactions become repulsive at temperatures T > T0 , where the critical temperature T0 is deﬁned from Eb (T0 ) = 0. If complex formation begins at a temperature near (but below) T0 , the variations of the slope of Eb (T ) with time (that is: as complex formation takes place and the concentrations of the various species change) will cause the interactions to shift from attractive to repulsive, probably resulting in a maximum precipitate size. Finally, since the diﬀerence in conﬁgurational entropy depends on the concentrations [A] and [B] in the sample, the binding free energy of a speciﬁc complex {A, B} at a speciﬁc temperature will be diﬀerent in samples containing diﬀerent concentrations of A or B. Many of these consequences of the temperature dependence of binding free energies are unexpected, not to say counterintuitive, because many of us are used to thinking in terms of potential energy alone. Yet, regardless of the value of the conﬁgurational entropy or the way it is calculated, the consequences are inescapable. Acknowledgements This work is supported in part by the R. A. Welch Foundation and the National Renewable Energy Laboratory.

References [1] R. K. Kremer, M. Cardona, E. Schmitt, J. Blumm, S. K. Estreicher, M. Sanati, M. Bockowski, I. Grzegory, T. Suski, A. Jezowski: Phys. Rev. B 72, 075209 (2005) 95, 104 [2] S. J. Pearton, J. W. Corbett, M. Stavola: Hydrogen in Crystalline Semiconductors (Springer, Berlin, Heidelberg 1991) 95 [3] S. Limpijumnong, C. G. Van de Walle: Phys. Rev. B 68, 235203 (2003) 96 [4] A. F. Wright, C. H. Seager, S. M. Myers, D. D. Koleske, A. A. Allerman: J. Appl. Phys. 94, 2311 (2003) 96 [5] A. Carvalho, R. Jones, J. Coutinho, P. R. Briddon: J. Phys.: Condens. Matter 17, L155 (2005) 96

Dynamical Matrices and Free Energies

111

[6] G. Davies: Phys. Rep. 176, 83 (1989) 96, 99 [7] S. Knack: Mater. Sci. Semic. Proc. 7, 125 (2005) 96 [8] S. K. Estreicher, D. West, J. Goss, S. Knack, J. Weber: Phys. Rev. Lett. 90, 035504 (2003) 96, 99 [9] S. K. Estreicher, D. West, M. Sanati: Phys. Rev. B 72, R13532 (2005) 96, 99 [10] D. S´ anchez-Portal, P. Ordej´ on, E. Artacho, J. M. Soler: Int. J. Quant. Chem. 65, 453 (1997) 96, 97 [11] E. Artacho, D. S´ anchez-Portal, P. Ordej´ on, A. Garc´ıa, J. M. Soler: phys. stat. sol. (b) 215, 809 (1999) 96 [12] D. M. Ceperley, B. J. Adler: Phys. Rev. Lett. 45, 566 (1980) 96 [13] S. Perdew, A. Zunger: Phys. Rev. B 32, 5048 (1981) 96 [14] L. Kleiman, D. M. Bylander: Phys. Rev. Lett. 48, 1425 (1982) 96 [15] O. F. Sankey, D. J. Niklevski: Phys. Rev. B 40, 3979 (1989) 97 [16] O. F. Sankey, D. J. Niklevski, D. A. Drabold, J. D. Dow: Phys. Rev. B 41, 12750 (1990) 97 [17] A. A. Demkov, J. Ortega, O. F. Sankey, M. P. Grumbach: Phys. Rev. B 52, 1618 (1995) 97 [18] H. J. Monkhorst, J. D. Pack: Phys. Rev. B 13, 5188 (1976) 97 [19] T. Inui, Y. Tanabe, Y. Onodera: Group Theory and Its Applications in Physics (Springer, Berlin, Heidelberg 1990) 97 [20] M. P. Allen, D. J. Tildesley: Computer Simulations of Liquids (Clarendon, Oxford 1987) 97 [21] J. L. Gavartin, D. J. Bacon: Comp. Mater. Sci. 10, 75 (1998) 97 [22] S. Baroni, P. Gioannozzi, A. Testa: Phys. Rev. Lett. 58, 1861 (1987) 97 [23] A. Fleszar, X. Gonze: Phys. Rev. Lett. 64, 2961 (1990) 97 [24] X. Gonze, C. Lee: Phys. Rev. B 55, 10355 (1997) 97 [25] J. M. Pruneda, S. K. Estreicher, J. Junquera, J. Ferrer, P. Ordej´ on: Phys. Rev. B 65, 075210 (2002) 97 [26] P. Ordej´ on, D. A. Drabold, R. M. Martin, S. Itoh: Phys. Rev. Lett. 75, 1324 (1995) 97 [27] D. West, S. K. Estreicher: Phys. Rev. Lett. 96, 115504 (2006) 98, 101 [28] J. L. Gavartin, A. M. Stoneham: Phil. Trans. Roy. Soc. Lond. A 361, 275 (2003) 98 [29] M. Budde, G. Luepke, C. Parks Cheney, N. H. Tolk, L. Feldman: Phys. Rev. Lett. 85, 1452 (2000) 99, 100 [30] M. Budde, G. Luepke, C. Parks Cheney, N. H. Tolk, L. C. Feldman: Phys. Rev. Lett. 85, 1452 (2000) 100, 101 [31] G. Lupke, X. Zhang, B. Sun, A. Fraser, N. H. Tolk, L. C. Feldman: Phys. Rev. Lett. 88, 135501 (2002) 100 [32] P. Flubacher, A. J. Leadbetter, J. A. Morrison: Philos. Mag. 4, 273 (1959) 102 [33] F. Widulle, T. Ruf, M. Konuma, I. Silier, M. Cardona, W. Kriegseis, V. I. Ozhogin: Solid State Commun. 118, 1 (2002) 103 [34] M. Cardona, R. K. Kremer, M. Sanati, S. K. Estreicher, T. R. Anthony: Solid State Commun. 133, 465 (2005) 104 [35] M. Sanati, S. K. Estreicher, M. Cardona: Solid State Commun. 131, 229 (2004) 104 [36] W. Schnelle, E. Gmelin: J. Phys.: Condens. Matter 13, 6087 (2001) 104

112

Stefan K. Estreicher and Mahdi Sanati

[37] S. K. Estreicher, M. Sanati, D. West, F. Ruymgaart: Phys. Rev. B 70, 125209 (2004) 105, 106 [38] S. K. Estreicher: Acta Phys. Polon. A 102, 403 (2002) 105 [39] S. K. Estreicher, K. Wells, P. A. Fedders, P. Ordej´ on: J. Phys.: Condens. Matter 13, 62 (2001) 106 [40] E. E. Chen, M. Stavola, W. B. Fowler: Phys. Rev. B 65, 245208 (2002) 106 [41] M. Sanati, S. K. Estreicher: Phys. Rev. B 72, 165206 (2005) 107, 108 ¨ [42] J. Adey, R. Jones, D. W. Palmer, P. R. Briddon, S. Oberg: Phys. Rev. Lett. 93, 055504 (2004) 107

Index ab initio, 101 absorption, 95 anharmonic, 102 annealing, 95 asymmetric, 99, 101 basis set, 96, 103 Boltzmann, 104 bond-centered, 99–101, 106 boron, 107, 108 Brillouin zone, 103 charge state, 107 classical, 101, 106 complex, 100, 105–110 concentration, 104–110 conduction band, 105 conﬁgurational entropy, 106, 108–110 conjugate gradient, 107 core, 96 correlation, 97 cutoﬀ, 97 decay, 96, 98, 100, 101 density of states, 95, 102, 103 density-functional theory, 96, 105 diﬀusion, 101 divacancy, 100 dopant, 105 double-zeta, 97, 103 dynamical matrix, 96, 97, 99, 103, 109 eigenvalues, 96, 97, 103, 109 eigenvectors, 96, 97, 99–101, 109 electron, 105

energetics, 108, 109 energy level, 105 entropy, 104, 106, 108–110 equilibrium, 96–98, 101, 107, 109 exchange-correlation, 96, 97 excitation, 101 fermion, 105 ﬁrst principles, 95, 96, 98, 105, 108 force, 97 force-constant matrix, 97 Fourier, 95 free carrier, 105 free energy, 96, 97, 102–110 frozen phonon, 97 FTIR, 95 GaN, 95, 104 Ge, 104 Gibbs, 102 Hartree, 97 Helmholtz, 96, 102–104 hole, 105 hydrogen, 96, 99, 100 impurity, 96, 99 interstitial, 105–107 isotope, 95, 104 linear response, 97 localization, 99, 109 magnetic, 105 migration, 95 molecular dynamics, 96

Dynamical Matrices and Free Energies Monkhorst–Pack, 97, 103 normal mode, 95–101, 103, 104 order-N , 97 oxygen, 107, 108 partition function, 105, 106 periodic, 96, 97, 103, 108 phonon, 95–97, 99–104, 109 photoluminescence, 96, 99 PL, 96, 99 polarization, 97 potential, 96–98, 101, 105, 110 proton, 105 pseudopotential, 96 quantum dot, 98 Raman, 95, 96, 105, 106 real space, 97 repulsive, 108, 110 resonant, 96, 109 rotational, 105, 106, 109 Sankey, 97 Si, 96, 99, 100, 102, 104–107 SIESTA, 96 speciﬁc heat, 97, 102, 104, 109

113

spin, 105, 109 strain, 96 stress, 95 substitutional, 107 supercell, 96, 97, 101, 103, 104, 108 surface, 101, 110 symmetric, 99, 101, 105 symmetry, 95, 96, 99, 106, 109 temperature, 96–102, 104, 106–110 tetrahedral, 106 thermal equilibrium, 96, 109 thermostat, 96, 98, 109 total energy, 96, 98 uniaxial stress, 95 vacancy, 96 valence band, 105 vibrational entropy, 104 vibrational free energy, 97, 104, 105, 107, 109 vibrational lifetime, 96–98, 100, 101, 109 vibrational modes, 95, 96, 99 vibrational spectroscopy, 95, 96 wag, 96, 99, 101

The Calculation of Free-Energies in Semiconductors: Defects, Transitions and Phase Diagrams E. R. Hern´ andez1 , A. Antonelli2 , L. Colombo3 , and P. Ordej´ on1 1

2

3

Institut de Ci`encia de Materials de Barcelona (ICMAB–CSIC), Campus de Bellaterra, 08193 Barcelona, Spain [email protected] Instituto de F´ısica Gleb Wataghin, Universidade Estadual de Campinas, Unicamp, 13083-970, Campinas, S˜ ao Paulo, Brazil SLACS (INFM-CNR) and Department of Physics, University of Cagliari, Cittadella Universitaria, I-09042 Monserrato (Ca), Italy

Abstract. In this chapter we review a series of novel techniques that make possible the eﬃcient calculation of free energies in condensed-matter systems, without resorting to the quasiharmonic approximation. Employing these techniques, it is possible to obtain the free energy of a given system not just at a predeﬁned temperature, but in a whole range of temperatures, from a single simulation. This makes possible the study of phase transitions, as well as the determination of equilibrium concentrations of defects as a function of temperature, as will be illustrated by examples of speciﬁc applications. The same techniques, coupled with a scheme to integrate the Clausius–Clapeyron equation, can lead to the eﬃcient determination of phase diagrams, a capability that will be illustrated with the calculation of the phase diagram of silicon.

1 Introduction The free-energy plays a central role in understanding the thermal properties of materials. From it, other properties of a material may be derived, such as the internal energy, the volume, entropy, etc. The phase behavior of a material is controlled by the values of the free-energy of its diﬀerent phases, and the concentrations of defects or impurities, as well as their partition among coexisting phases, are deﬁned by their chemical potentials, which are themselves obtained from the free-energy. It is clear, therefore, that it is highly desirable to have eﬃcient computational tools that can evaluate the free-energy of modeled materials in diﬀerent conditions of temperature and pressure (or volume). These methods should be accurate, and ideally it should be possible to combine them with ﬁrst-principles electronic structure methods, which provide an accurate picture of the structure, bonding and energetics of materials. In this Chapter we provide a self-contained description of recent theoretical developments that have contributed to making free-energy calculations D. A. Drabold, S. K. Estreicher (Eds.): Theory of Defects in Semiconductors, Topics Appl. Physics 104, 115–140 (2007) © Springer-Verlag Berlin Heidelberg 2007

116

E. R. Hern´ andez et al.

more accessible and eﬃcient, and we illustrate their capabilities with a series of applications, mostly in the ﬁeld of semiconductors, the topic of this book. Our intention in writing this Chapter has been to illustrate the potential of these techniques, some of which are still relatively little known. On the other hand, we have not intended to provide an exhaustive review of free-energy techniques, nor to dwell overmuch on the technical details of implementation. Both topics are covered at length in the excellent book by Frenkel and Smit [1], and also to some extent in the earlier book by Allen and Tildesley [2]. Nor has it been our intention to list the many examples of applications of free-energy techniques to problems in materials science, chemical physics, geology or biomolecular systems. Applications in some of these ﬁelds are reviewed to some extent in the articles by Rickman and LeSar [3] and by Ackland [4]. A very recent review of some of the techniques that will be discussed here, in particular the reversible scaling technique, is that of de Koning and Reinhardt [5].

2 The Calculation of Free-Energies Unlike the total internal energy, which depends only on the positions and velocities of the system at a single point in phase-space, the free-energy depends on all conﬁgurations (all state points) in the phase-space volume accessible to the system of interest in its given conditions of temperature and volume (or pressure). This is, in essence, why it is more arduous to calculate the free-energy in atomistic simulations of condensed-matter systems. From statistical mechanics we have that the free-energy at temperature T has the form F = −kB T ln Z ,

(1)

where kB is Boltzmann’s constant and Z is the partition function. In canonical ensemble conditions, i.e., constant number of particles N , constant volume V and constant temperature T , the partition function has the following expression: 1 ZN V T = dΓ e−βH(Γ ) , (2) N ! h3N V where Γ represents a point in phase-space, i.e., the 6N -dimensional space formed by the 3N momenta and 3N coordinates of the system, dΓ is the corresponding volume element, h is Planck’s constant, H is the Hamiltonian of the system, β = (kB T )−1 , and only conﬁgurations of volume V contribute to the integral. By writing an integral we are implicitly assuming that the system under consideration is being described by classical mechanics. In the quantum case the integral would be replaced by a discrete sum over quantum states.

Free-Energies in Semiconductors

117

Frequently it is desirable to consider the system under conditions of constant temperature and constant pressure (instead of constant volume), conditions that correspond to the so-called isothermal-isobaric or N P T ensemble. In this case, the partition function Z is generalized to ∞ 1 −βP V −βH(Γ ) dV e dΓ e ZNPT = . (3) N ! h3N 0 V In this case the free-energy is called the Gibbs free-energy (and we will label it G), to distinguish it from the canonical free energy (also called the Helmholtz free energy). The partition function plays the role of a normalization factor in thermodynamical averages. Consider, for example, some property A, which depends on the positions, and/or velocities of the particles in the system. Then, the canonical thermal average of A would be given by dΓ A(Γ ) e−βH(Γ ) , (4) AN V T = V −βH(Γ ) V dΓ e where the denominator can be recognized as the canonical partition function of (2) save for some factors that are canceled when taking the quotient of integrals. Such thermal averages are readily estimated by the standard simulation techniques of (canonical) molecular dynamics (MD) or Monte Carlo (MC), but it is important to note that these techniques directly estimate the quotient of integrals appearing in (4), and they cannot evaluate each of the integrals separately. Also, note that the free-energy is not itself a thermal average [it does not have the form of (4)], and therefore it cannot be obtained by direct MD or MC simulation. 2.1 Thermodynamic Integration and Adiabatic Switching Equations (2) and (3) clearly illustrate the diﬃculty of evaluating the freeenergy. These integrals are multidimensional, with as many dimensions as degrees of freedom in the system, and except for very simple models such as the ideal gas or the harmonic solid, they cannot be evaluated analytically. Furthermore, their high dimensionality precludes any attempt of evaluation by numerical quadrature methods. Thus it would seem that we are faced with an unsurmountable diﬃculty, though fortunately this is not the case. A way out of the problem is given by considering the dependence of the Hamiltonian H on some parameter λ, and asking ourselves how does the free-energy change with λ. It is immediately apparent that −βH(Γ ) dΓ ∂H ∂H ∂F ∂λ e V = = . (5) −βH(Γ ) ∂λ ∂λ V dΓ e Equation (5) shows that, while the free energy itself is not a thermal average, its derivative with respect to any parameter λ is a thermal average,

118

E. R. Hern´ andez et al.

and therefore it can be evaluated by employing conventional simulation techniques. This observation forms the basis of the technique known as the thermodynamic integration or coupling parameter [6, 7] method for evaluating free-energies, or rather free-energy diﬀerences. Consider a system, for example a solid, described by some potential U (r ), where r stands for the set of (generalized) coordinates specifying the positions of all degrees of freedom, for which we wish to evaluate the free-energy at some given temperature and volume. Now imagine that there is another system, similar in some sense to the system of interest, for which the free-energy is known at the temperature and volume at which we wish to know it for the system of interest. We noted earlier that one of the systems for which the canonical partition function can be evaluated analytically is the harmonic solid in which each atom is tied to its equilibrium lattice site by means of a harmonic spring. We will refer to the system for which the free-energy is known as the reference system, and will assume it is described by a potential Uref (r ). Let us now deﬁne the λ-dependent Hamiltonian Hλ =

1 p 2i + λU (r ) + (1 − λ)Uref (r ) . 2 i mi

(6)

Notice that when λ = 0 the Hamiltonian corresponds to that of the reference system (in our example the Einstein solid), while when λ = 1 it is that of the system of interest. A direct application of (5) tells us that the derivative of the free-energy Fλ associated with Hλ at λ ∈ [0, 1] is ∂Fλ = U (r ) − Uref (r )λ . ∂λ

(7)

Thus, to obtain the free-energy diﬀerence between the system of interest and the reference all we need to do is to integrate over λ, 1 dλ U (r ) − Uref (r )λ . (8) ∆F = F − Fref = 0

Since Fref is known, the sought F follows immediately. As stated above, the λ-dependent thermal averages U (r)−Uref (r )λ are readily obtained from standard simulation techniques. In practice, a discrete set of λ values in the interval [0, 1] is chosen (usually of the order of 5 to 10), and at each one of them an equilibrium simulation is carried out with Hamiltonian Hλ , from which the average U (r ) − Uref (r )λ is obtained. Then the integral in (8) is evaluated numerically. Note that because one samples directly the potential U (r ) − Uref(r ) using either MD or MC simulation techniques, no harmonic approximation is involved here, and thus anharmonic eﬀects are automatically taken into account. For this procedure to work, the chosen reference system must be in some sense similar to the target system. By this we mean that as λ is changed,

Free-Energies in Semiconductors

119

the system described by Hamiltonian Hλ (6) should not undergo any phase transitions. If that were to occur, some of the work spent in transforming the reference system into the system of interest (or vice versa) would actually be spent in the latent heat of the phase transition, and the resulting free-energy estimate would be inaccurate. Also, with a view to making the numerical integration of (8) accurate, it is desirable that the quantity U (r ) − Uref (r ) is subject to ﬂuctuations as small as possible, and this is another criterion of similarity between target and reference systems. We have already mentioned that a useful reference for free-energy calculations of solids is the Einstein crystal, but this would not be a good reference for a liquid. Fortunately, there are a number of simple model liquids, such as the Lennard–Jones ﬂuid [8] or the inverse-power ﬂuid [9], which have been extensively studied, and for which the free-energy has been tabulated over a wide range of temperature and pressure (density) conditions, and therefore these models serve the purpose of reference systems for liquids. Of course, for systems in the gas phase the ideal gas is an adequate reference. Equation (8) reminds us again of the fact that it is harder to obtain free-energies than it is to calculate thermal averages. A thermal average is typically obtained from a single equilibrium (MD or MC) simulation, while to evaluate the free-energy of the same system one needs several simulations. The eﬀort is increased further if the free-energy must be evaluated at other temperatures or volumes (pressures). It can easily be seen that the amount of work necessary to ﬁnd a coexistence point, let alone map out a phase boundary (where two coexisting phases have the same free-energy), soon becomes a daunting task, if one must resort to the schemes described thus far. Fortunately, starting in the early 1990s, a number of alternative techniques of increased eﬃciency have been developed, which considerably ameliorate this situation, and thanks to them the task of calculating phase boundaries, and even entire phase diagrams is nowadays more accessible. The ﬁrst such development was proposed by Watanabe and Reinhardt [10], who showed that accurate estimations of ∆F could be obtained from a single simulation with Hamiltonian Hλ (6), during which the parameter λ is slowly (i.e., quasiadiabatically) switched from 0 to 1 (or vice versa). Thus, the task of performing several equilibrium simulations at diﬀerent values of λ to obtain ∆F is reduced to that of performing a single nonequilibrium simulation on a system that quasiadiabatically transmutes from the reference system to the system of interest (or the reverse). During this nonequilibrium simulation one computes the irreversible work (reversible in the adiabatic limit) Wirr (t, λ = 0 → 1), given by Wirr (t, λ = 0 → 1) =

t

dt λ˙ {U [r (t )] − Uref [r (t )]} ,

(9)

0

where λ˙ = dλ/ dt is the rate of change of λ, and the time variable corresponds to either real time in an MD simulation, or to simulation time in

120

E. R. Hern´ andez et al.

an MC simulation (each MC sweep corresponding to a unit of simulation time). In the adiabatic limit, Wirr (t = ∞, λ = 0 → 1) would be equal to the free-energy diﬀerence ∆F , but since in practice strict adiabaticity cannot be attained, Wirr (t, λ = 0 → 1) is only an approximation to ∆F , due to entropic dissipation eﬀects (see below). Nevertheless, experience shows that (9) provides satisfactorily accurate results with modest computational eﬀorts, indeed more modest than those required in a full thermodynamic integration calculation. We will refer to the method of Watanabe and Reinhardt as the adiabatic switching method. The adiabatic switching method is based on two key observations. The ﬁrst one is that, by virtue of Liouville’s theorem, any classical trajectory, even one generated by a time-dependent Hamiltonian, preserves the phasespace volume. In other words, the trajectory generated by a time-dependent classical Hamiltonian will evolve on a phase-space hypersurface that, though itself changing shape with time, encloses a ﬁxed amount of phase-space volume. The second observation, due to Hertz [10], applies when the evolution of the Hamiltonian is slow, or adiabatic. Under these conditions, the evolving hypersurface of phase-space on which the trajectory moves corresponds, at each instant t, to a constant energy shell of energy H(t). Therefore, a trajectory generated by an adiabatically evolving Hamiltonian preserves the entropy, deﬁned as S = kB ln Ω, where Ω is the (invariant) phase-space volume enclosed by the adiabatically evolving phase-space hypersurface. This is the mechanical analog of the observation in thermodynamics that an adiabatic process (i.e., one that proceeds along a succession of equilibrium states) exerted on a system preserves its entropy. The consequence of this is that, since ∆S = 0 when λ in (6) is adiabatically switched along the trajectory generated by Hλ in canonical ensemble conditions, the free-energy change involved in this switching process can be measured by the internal energy change alone. As pointed out above, in the limit of strict adiabaticity, we would have that ∆F = Wirr (t = ∞, λ = 0 → 1), but since the switching process cannot be truly adiabatic there will be some entropic dissipative effects, which will cause Wirr (t, λ = 0 → 1) to be an upper bound of ∆F . In fact, one can also run the switching simulation in reverse, i.e., switching λ from 1 to 0, and the resulting irreversible work, −Wirr (t, λ = 1 → 0) then provides a lower bound to ∆F . This proves to be a convenient way of determining error bars for the estimated free-energy [5]. 2.2 Reversible Scaling Another important development allows one to obtain the free energy in a quasicontinuous range of temperatures, starting from a reference temperature at which the free-energy is known, from either a previous adiabatic switching or thermodynamic integration calculation. This method, known as reversible scaling, was introduced by de Koning et al. [11], and is based on the

Free-Energies in Semiconductors

121

formal equivalence that exists, from a statistical-mechanics perspective, between scaling the temperature and scaling the potential. Indeed, the canonical partition function of a system described by potential U (r ) at temperature T is U (r ) 1 −k T B , dr e (10) ZN V T = N ! Λ3N (T ) V where the factor Λ(T ) = (h2 /2πmkB T )1/2 results from integrating out the momenta, and we have assumed that all particles are identical. Now, consider a system described by a scaled potential, λU (r ), at a diﬀerent temperature T0 . For this system, the partition function would be λU (r ) 1 − ZN V T0 (λ) = dr e kB T0 3N N ! Λ (T0 ) V λ3N/2 − k UT(r )/λ B 0 = dr e . (11) N ! Λ3N (T0 /λ) V Now, it is easy to see that, except for a factor of λ3N/2 , the partition function of the scaled system at temperature T0 /λ and that of the unscaled system at temperature T are identical, if we impose that T0 = λT . From this it is easy to derive the following relation between the free-energies of the scaled and unscaled systems: F (T ) Fs (T0 , λ) 3 = + N kB ln λ . T T0 2

(12)

In words, we have related the free-energy of a system at temperature T to that of an appropriately scaled system at temperature T0 such that T0 = λT . From a formal point of view not much has been done. However, using the technique of adiabatic switching described in Sect. 2.1 it is very simple to calculate Fs (T0 , λ), at ﬁxed temperature T0 but in a quasicontinuous range of λ values in some interval λ ∈ [λmin , λmax ], and by virtue of (12), each of these Fs (T0 , λ) values corresponds to the free-energy of the unscaled system in a quasicontinuous range of temperatures T ∈ [T0 /λmax , T0 /λmin ]. Fs (T0 , λ) is obtained as NV T Fs (T0 , λ) = Fs (T0 , λ0 ) + Wirr (λ0 → λ),

(13)

where Fs (T0 , λ0 ) is the free-energy of the scaled system at the initial value of NV T (λ0 → λ) is the scaling parameter λ0 (usually either λmin or λmax ) and Wirr the work done by switching the scaling parameter from λ0 to λ, which, using the adiabatic switching technique is estimated as t NV T (λ0 → λ) = dt λ˙ U [r (t )] . (14) Wirr 0

122

E. R. Hern´ andez et al.

Thus, instead of having to run a separate adiabatic switching or thermodynamic integration calculation to obtain the free-energy of the system of interest for each temperature in a discrete set spanning the desired range of temperatures, one can perform a single adiabatic switching calculation of the scaled system at some appropriately chosen temperature T0 , and simply quasicontinuously vary the scaling parameter λ from λmin to λmax (or vice versa). Note that in (14) each time step leads to a new value of λ and a correNV T (λ0 → λ), which, through (12), leads to an estimate sponding value of Wirr of F (T ) at temperature T = T0 /λ. For the sake of simplicity, we have presented the method in the context of the canonical ensemble, but the same ideas can be applied in the isothermalisobaric case [12], which is of more interest when it comes to studying phase transitions. In this case one ﬁnds that it is necessary not only to scale the potential energy but the pressure as well, so that the scaled system pressure is Ps (λ) = λP , P being the pressure of the unscaled system. Then (12) transforms into Gs [T0 , Ps (λ)] 3 G(T, P ) = + N kB ln λ , T T0 2

(15)

relating the Gibbs free-energies of the scaled and unscaled systems, and NPT Gs (T0 , Ps , λ) = Gs [T0 , Ps (λ0 ), λ0 ] + Wirr (λ0 → λ), with

t dPs (λ) NPT ˙ V (t ) , dt λ U [r (t )] + (16) Wirr (λ0 → λ) = dλ 0 which is obtained from an adiabatic switching calculation carried out under isobaric-isothermal conditions. The reversible scaling technique discussed above provides an eﬃcient procedure for calculating coexistence points between diﬀerent phases of a given material or substance. Using reversible scaling in the isothermal-isobaric ensemble one can easily obtain the Gibbs free energy of the two diﬀerent phases, at constant pressure P , in a range of temperatures bounding the values where the coexistence point is expected to be located. The temperature at which the two free energies match is by deﬁnition the coexistence temperature of the two phases at pressure P . This strategy is illustrated for the particular case of the melting point of Si in the diamond phase at 0 pressure in Fig. 1. Si was simulated with the semiempirical tight-binding (TB) [13] Hamiltonian due to Lenosky and coworkers [14], which describes very well the structural and thermal properties of Si in several of its phases [15]. 2.3 Phase Boundaries and Phase Diagrams If one wishes to map out an entire phase boundary, rather than just a single coexistence point between two phases in equilibrium, one option would be to iterate the procedure illustrated in Fig. 1 to obtain new coexistence temperatures at diﬀerent pressures. However, an alternative method exists

Free-Energies in Semiconductors

123

Fig. 1. Gibbs free-energy of the diamond and liquid phases of Si in the neighborhood of the zero-pressure melting point, as obtained from reversible scaling simulations with the Lenosky et al. [14] model. The simulations contain 128 atoms in each phase, and four k-points were used to sample the Brillouin zone. It can be seen that the two free-energies become equal at approximately 1551 K, and above this temperature the liquid becomes thermodynamically more stable. More details of these calculations can be found in [15, 16]

that is often more eﬃcient and practical, since it does not require any further calculation of free-energies along the phase boundary. This technique was pioneered by Kofke [17, 18], and is known as Gibbs–Duhem or Clausius– Clapeyron integration. In this method, starting from some previously determined coexistence point along the desired phase boundary, one numerically solves the Clausius–Clapeyron equation: ∆V dT =T . dP ∆H

(17)

This equation relates the slope of the phase boundary, dT / dP , at the current coexistence point, given by temperature T and pressure P , with the diﬀerences of molar volumes ∆V and molar enthalpies ∆H of the coexisting phases. Thus, if ∆V and ∆H are known at the current coexistence point, one can estimate how the equilibrium temperature will change if the pressure changes by some small amount. ∆V and ∆H can be obtained from standard equilibrium simulations using MD or MC. Note that the interface between the coexisting phases need not be taken into account: each phase is independently simulated in a separate simulation box, at identical conditions of temperature and pressure. Once the average volume and enthalpy of each phase is known with suﬃcient accuracy, new coexistence conditions are derived from (17),

124

E. R. Hern´ andez et al.

and the process is iterated until the phase boundary has been mapped out. The stability and accuracy of the method have been analyzed in detail by Kofke [18]. This method has been extensively employed, and some particular examples of its use will be illustrated in the next section. A parallelism can be established between Kofke’s Clausius–Clapeyron integration method and thermodynamic integration. In the latter, one performs a series of equilibrium simulations at diﬀerent λ values in the range [0, 1] with the aim of obtaining the free-energy of the system. In Clausius–Clapeyron integration, one performs a series of equilibrium simulations at diﬀerent values of the independent variable (T or P ), and uses (17) to ﬁnd how the dependent variable (P or T ) adapts to the change in the independent variable such that the two phases remain in equilibrium. However, as we saw in Sect. 2.1, the calculation of the free energy can be made more eﬃciently using adiabatic switching, where instead of several (ca. 5–10) equilibrium simulations, a single nonequilibrium quasiadiabatic simulation is employed. It is therefore natural to ask if a similar gain in eﬃciency is possible in Clausius–Clapeyron integration, and the answer is aﬃrmative, as de Koning et al. [12] have shown. The Clausius–Clapeyron equation (17) is arrived at by demanding that the change in free-energy due to a small change in the independent variable be the same in both phases. For illustrative purposes, let us consider the case in which the temperature T plays the role of independent variable, while the pressure P is the dependent one. As in the reversible scaling method, let us now consider scaled versions of the two phases at constant temperature T0 and pressure Ps . When λ = 1 these correspond to some initial coexistence point. The free-energies of the scaled phases will be GS,a and GS,b , respectively. In the scaled case, now the temperature is ﬁxed, and the role of the independent variable is played by λ. Therefore, as λ is changed, the scaled phases will depart from equilibrium, unless the scaled pressure Ps (λ) evolves in such a way as to make the change in GS,a equal to that in GS,b . By requiring that this be the case, one arrives at a Clausius–Clapeyron equation for Ps (λ), which reads dPs (λ) ∆U =− , dλ ∆V

(18)

where ∆U is the diﬀerence of internal energies between the two phases. If λ is stationary, the values of ∆U and ∆V would be obtained from standard equilibrium simulations, and everything would be exactly as in the case of the Clausius–Clapeyron integration of Kofke, but working with the scaled phases. However, (18) suggests that, as in the reversible scaling method, λ can be varied quasicontinuously (i.e., quasiadiabatically). In these conditions, ∆U and ∆V will adapt to the changing value of λ, and Ps (λ) will evolve according to (18) such that the scaled phases remain in equilibrium. Through the scaling relations T = T0 /λ, P = λPs (λ), the equilibrium pressure P (T ) at temperature T will be obtained for the unscaled phases. De Koning et al. demonstrated the usefulness of the method by calculating the melting curve

Free-Energies in Semiconductors

125

of the Lennard–Jones model for pressures between 0 up to 160 reduced units, obtaining results matching those obtained previously by Agrawal and Kofke [19] employing the standard (equilibrium) Clausius–Clapeyron integration method. In the next section we will see another application, in which this dynamic Clausius–Clapeyron integration method has been recently used to obtain the phase diagram of Si as predicted by a semiempirical TB model.

3 Applications Let us now discuss some examples of applications of the techniques described in Sect. 2 to the study of thermal properties of defects, phase transitions and phase diagrams. Our focus, given the theme of this book, will be mostly on semiconductors, though occasionally we will mention examples of applications to other types of materials, due to their importance or to their illustrative value. Let us remark that we do not intend to provide an exhaustive review of the literature concerned with thermal properties of semiconducting materials, as this would be beyond the scope of this Chapter. Our aim is rather to illustrate the capabilities of the novel techniques discussed above. 3.1 Thermal Properties of Defects Most calculations of the free-energy and other thermal properties of defects in semiconductors to be found in the literature rely on the use of the quasiharmonic approximation, and since this topic is going to be covered at length in Chap. 8, we will not dwell much on it here. However, we must mention two studies that employed techniques described in Sect. 2, and that therefore go beyond the quasiharmonic approximation. Both studies illustrate nicely the potential of the techniques discussed in this Chapter, and make evident the need for incorporating the eﬀects of anharmonicity at suﬃciently high temperatures. The ﬁrst example is the study of J¨ a¨ askel¨ ainen et al. [20], who computed the free-energy of formation of the vacancy and self-interstitial in Si as a function of temperature. A thorough study of self-diﬀusion requires accurate free-energy calculations (aimed at predicting temperature-dependent equilibrium concentrations) and extensive diﬀusivity simulations (aimed at computing migration energies and diﬀusivity prefactors) for all relevant kinds of native defects. In their study, J¨ a¨ askel¨ainen and coworkers considered only self-interstitial (I) and vacancy (V) defects.

126

E. R. Hern´ andez et al.

f f f Once the formation free-energies FI,V = EI,V + T SI,V , as well as migram 0 tion energies EI,V and diﬀusivity prefactors dI,V are known, the self-diﬀusion coeﬃcient DSD (T ) can be cast in the form

EIf − T SIf 0 DSD (T ) = dI exp − exp (−EIm /kB T ) kB T

f E f − T SV m /kB T ) , (19) + d0V exp − V exp (−EV kB T

so that a direct theory vs. experiment comparison is possible. The thermodynamic integration (TI) method [1] was adopted by J¨ a¨ askef in c-Si by means of the tight-binding (TB) l¨ ainen et al. [20] to evaluate FI,V model provided by Kwon et al. [21]. The ensemble average appearing in (8) was performed during constant-volume, constant-temperature molecular dynamics (TBMD) simulations in a 64±1 atom periodically repeated cell. The thermodynamical integration was performed over 16 λ points, while freeenergy calculations were performed at four diﬀerent temperatures, namely 300 K, 500 K, 1000 K and 1400 K. The formation entropy SIf for the selfinterstitial defect was found to be almost constant with temperature, the average value being SIf = 11.2kB . First-principles calculations [22] predict a value of SIf ∼ 10kB when including anharmonic terms through TI calculations as well. The case of a vacancy is more complicated due to its high mobility [23], which eﬀectively adds a sizeable contribution of migration entropy in the TI free-energy calculations. This is conﬁrmed by the fact that f varied in the range 10.2kB to 11.7kB in the sethe computed value of SV f lected temperature interval, with an average value of SV ∼ 10.8kB . In the case of the vacancy, in order to prevent the double counting of the migration entropy, which is already taken into account by the TBMD simulations aimed at measuring d0V , short observation runs were performed, taking care to select only those simulations where V diﬀusion actually did not take place. The resulting average formation (i.e., conﬁgurational + vibrational) entropy f ∼ 8.8kB . was SV f are in good qualitative agreement with These TBMD results for SIf and SV ﬁrst-principles calculations by Bl¨ ochl and coworkers [22] in the sense that the diﬀerence in the entropies of formation for interstitials and vacancies is of the order of 1kB to 2kB in both studies, with a larger formation entropy for the interstitial. Diﬀusivity constants were ﬁnally obtained by using the migration prefactors and energies computed by means of the same TBMD functional, following Tang et al. [23]. The overall reliability of this TI-TBMD approach is summarized in Fig. 2, where the silicon TBMD total self-diﬀusion coeﬃcient DSD = DI + DV is compared with state-of-the-art experimental data [24, 25]. As can be seen, there is extremely good agreement between the diﬀerent sets of experimental data and the theoretical results. These temper-

Free-Energies in Semiconductors

127

-10 Expt. Expt. Theo.

2

Log10 DSD(cm s)

-12

-14

-16

-18

-20 0.55

0.65

0.75

0.85

0.95

-1

1000/T (K )

Fig. 2. Temperature dependence of the total self-diﬀusion coeﬃcient in silicon. The continuous line is the experimental results of [24], the dotted line is the experimental measurements of [25], and the dot-dash line is the theoretical results of [20]. Reprinted with permission from J¨ aa ¨skel¨ ainen et al. [20], Copyright (2001) by the American Physical Society

ature-dependent self-diﬀusion values should be therefore useful in modeling Si bulk processing. As noted above, J¨aa¨skel¨ainen et al. implicitly assumed that the main contributors to self-diﬀusion in Si are the vacancy and interstitial defects, thus neglecting the possible contribution of other kinds of defects, such as clusters of interstitials or vacancies. Indeed, both ﬁrst-principles simulations [26] and tight-binding temperature-accelerated MD simulations have revealed that small clusters of defects can also make substantial contributions to the mobility. In particular, the study of Cogoni et al. [27] shows quite conclusively that in all ranges of temperatures the mobility of the interstitial dimer is comparable to that of the single interstitial. At suﬃciently high temperatures (above 1400 K) even the trimer diﬀuses fairly rapidly. However, it should be noted that to better estimate the signiﬁcance of these clusters of interstitials to self-diﬀusion in Si, their concentrations, as well as their mobilities have to be taken into account. Since their formation energies are larger than that of the single interstitial, it is likely that in equilibrium conditions their net contribution to self-diﬀusion will be rather small. On the other hand, the processing of Si samples may incur nonequilibrium defect populations, and under these conditions the contribution of clusters of interstitials to self-diﬀusion could be important. Let us now focus on another aspect of the thermal properties of Si. At room temperature, Si is a brittle material, but as the temperature is raised, a dramatic change in its mechanical properties takes place in a very narrow

128

E. R. Hern´ andez et al.

range of temperatures around 873 K, and Si becomes a ductile material [28]. It is accepted that this change is due to the fact that at this temperature dislocations can be more easily nucleated and emitted at the tip of cracks, blunting the crack tip and making its propagation through the material more diﬃcult. In Si there are two sets of closely packed {111} slip planes, called shuﬄe and glide. While dislocations nucleated at the shuﬄe set have high Peierls stress and low mobility, the dislocations on the glide set can split into partials, having a smaller Peierls stress and higher mobility. It is believed that the brittle–ductile transition in silicon can be related to the change in dominance of one set over the other. Over 10 years ago, Rice and collaborators [29–31] proposed a model in which the resistance to nucleation of dislocations at the crack tip can be measured by the so-called unstable stacking energy, which is the lowest energy barrier that needs to be crossed when one half of a crystal slips relative to the other half. Through a combination of density-functional theory calculation with Vineyard’s transition state theory, Kaxiras and Duesbery [32] have shown that an abrupt transition from shuﬄe to glide dominance happens with temperature. In this approach, the temperature eﬀects were considered without taking into account the real dynamics of the atoms on either side of the slip plane. The calculations by de Koning et al. [33] using the adibatic switching method within MD simulations fully included such temperature eﬀects. Figure 3 shows the phase diagram for preferable nucleation of dislocations on shuﬄe plane versus glide set. One can see from the ﬁgure that the inclusion of all anharmonic eﬀects in the calculations by de Koning et al. did not change substantially the diagram previously obtained by Kaxiras and Duesbery. 3.2 Melting of Silicon Probably the ﬁrst calculation of the melting point of crystalline Si from simulation was carried out by Broughton and Li [34], employing the well-known Stillinger–Weber [35] potential. Broughton and Li calculated the zero-pressure melting point by obtaining the free-energy of the crystal and liquid phases at diﬀerent temperatures. The free-energy of the crystal was calculated by thermodynamic integration at diﬀerent temperatures, taking as a reference system the harmonic solid. For the liquid phase, the free-energy was obtained by ﬁrst switching oﬀ the attractive two-body part of the potential to avoid the occurrence of a possible ﬁrst-order liquid–vapour transition, and then expanding the system to zero density. They obtained a melting temperature of 1691 K, with an estimated error of ±20 K. This value is in very good agreement with the currently accepted experimental value of 1687 K [36], an agreement that is perhaps not so surprising, as the Stillinger–Weber potential was parametrized on the basis of data from both the crystal and liquid phases. The careful free-energy tabulation of the Stillinger–Weber potential for the crystal and liquid phases of Si achieved by Broughton and Li has al-

Free-Energies in Semiconductors

129

Fig. 3. Coexistence curves separating the preferable nucleation of dislocations on shuﬄe planes versus glide set. The full line is the results obtained from the EDIP potential after applying a correction for the overestimation of γus , the unstable stacking energy, by this potential. The dotted line shows the results obtained with DFT LDA calculations, and the dashed horizontal line gives the value of the experimental brittle fracture stress. Figure reprinted with permission from de Koning et al. [33]. Copyright (1998) by the American Physical Society

lowed subsequent studies (see below) to use this model as a reference system for free-energy calculations of Si employing higher levels of theory. In a subsequent study, Clancy and Cook [37] compared several empirical potential models in their ability to describe the thermal behavior of Si and Ge; in particular they considered the well-known Tersoﬀ potential [38–40], and a form of the embedded atom potential modiﬁed to describe covalent bonding (modiﬁed embedded atom method, MEAM) [41]. In this work the melting point for each model was determined by employing the two-phase coexistence method, i.e., by simulating the solid and liquid in a large cell in direct coexistence. It was found that the Tersoﬀ model for Si led to a melting temperature of 2547 K, well above the experimental value of 1687 K, while the MEAM showed the opposite behavior, underestimating the melting temperature at 1475 K. Both models correctly predict, as does the Stillinger– Weber potential, a slight increase of the density upon melting, though all models underestimate somewhat the crystal and liquid densities. A similar study, comparing several tight-binding models in their ability to reproduce

130

E. R. Hern´ andez et al.

the liquid structure, and the melting temperature of Si has been recently carried out by Kaczmarski et al. [15]. Very soon after the proposal of the adiabatic switching technique by Watanabe and Reinhardt [10], Sugino and Car [42] employed this technique, combined with ﬁrst-principles Car–Parrinello dynamics [43], to study the melting of Si. These authors employed as a reference system the Stillinger– Weber potential for both the crystal and liquid phases, for which the free energy had been previously determined by Broughton and Li [34] as a function of temperature, as discussed above. Sugino and Car thus calculated the free-energy diﬀerence between the reference model and a ﬁrst-principles description of Si employing density-functional theory (DFT) with the local-density approximation (LDA) for the exchange and correlation energy, combined with the pseudopotential approximation. They predicted a melting temperature of 1350 ± 100 K, some 300 K below the experimental value. This error was attributed to the relative destabilization of the solid phase with respect to the liquid in the LDA, which would result in a reduction of the melting point. Any small error in the diﬀerence of free energies translates into a rather large error in the melting temperature, and hence these kind of calculations require very stringent accuracy constraints. More recently, Alf`e and Gillan [44] have revisited the theme of the melting of Si from ﬁrst-principles simulations. These authors, employing the LDA approximation obtained a melting temperature of 1300 ± 50 K, in good agreement with the value reported earlier by Sugino and Car. They also performed calculations employing a generalized gradient approximation (GGA) to the exchange and correlation energy, obtaining in this case a somewhat improved value of the melting temperature of 1492 ± 50 K, which, although still below the experimental value by nearly 200 K, clearly improves upon the LDA result. This observation conﬁrms the suggestion made by Sugino and Car that the underestimation of the melting point was most likely attributable to errors in the exchange and correlation functional, and not in any other of the approximations involved in the simulations (pseudopotential, basis set, etc.). It is worth noting that Si is a troublesome case, as the melting point separates two phases of diﬀerent electronic character: while the crystal is semiconducting, the liquid is metallic. Errors due to the approximate nature of the functionals may, in general, be of diﬀerent size in insulators and metals. Indeed, when systems in which the electronic character of the material does not change upon melting have been studied, DFT methods can predict melting temperatures within a few tens of K of the experimental result. This is the case for Al, which has been studied by de Wijs et al. [45], who reported a value of Tm = 890 ± 20 K, compared to an experimental value of 933.47 K. Both liquid silicon (l-Si) and water present an anomalous behavior of the density and speciﬁc heat with temperature. Also, like water, l-Si is a very poor glass former, in the sense that it is extremely diﬃcult to experimentally obtain the amorphous phase by quenching from the melt. In the case of silicon, as a matter of fact, this has never been achieved. Due to these similarities, it has

Free-Energies in Semiconductors

131

Fig. 4. Kauzmann plot for the environment-dependent interatomic potential (EDIP)-Si. Normalized entropy diﬀerence between the disordered and crystalline phases according to the EDIP model as a function of normalized temperature. Reprinted with permission from [46]. Copyright (2004), American Institute of Physics

been proposed that, as in water, supercooled l-Si could present polymorphism, as well as polyamorphism. Experiments have suggested the existence of a ﬁrst-order-like liquid–liquid (l–l) transition in supercooled l-Si [47, 48]. Also, it has been considered, based on experimental results, that the transition from amorphous silicon (a-Si) to l-Si (l–a transition) would also be a discontinuous transition [47]. From the computational point of view, MD simulations using the Stillinger–Weber potential [49] have determined a l–l transition at about 1060 K, but have not found evidence of a l–a transition. Other computational results, using the EDIP [50] model for silicon, found a ﬁrst-order-like l–a transition at 1170 K and no evidence of a l–l transition [51]. In a recent study using the reversible scaling method within MC simulations and also using the EDIP model, Miranda and Antonelli [46] have shown that a l–l transition occurs at 1135 K and a l–a transition takes place at 843 K. Figure 4 shows the normalized excess entropy of the liquid phase with respect to the crystalline phase as a function of the normalized temperature. From the ﬁgure one can see that as the temperature is lowered, ﬁrst a discontinuous transition takes place, and as the temperature is lowered further, a glass-like transition occurs, beyond which the excess entropy becomes constant. This would be in agreement with recent experiments [52] that have indicated that a glasslike transition takes place at about 1000 K. Also, the conﬁgurational entropy obtained by Miranda and Antonelli for the amorphous phase is in agreement with that obtained by Vink and Barkema [53] using a methodology based on graph and information theories.

132

E. R. Hern´ andez et al.

Fig. 5. Phase diagram of water. The left panel shows the phase diagram predicted by the TIP4P potential; the left panel that obtained from the SPC/E model, and the central panel displays the experimental phase diagram. The SPC/E phase diagram has been shifted by 0.1 GPa in order to make phase I visible, as this phase appears at small negative pressures, according to this model. Figure reprinted with permission from Sanz et al. [54]. Copyright (2004) by the American Physical Society

3.3 Phase Diagrams As discussed above, the eﬃcient free-energy techniques exposed in Sect. 2, combined with Kofke’s Clausius–Clapeyron integration method, can be employed to calculate phase diagrams of materials entirely from simulation. Two particularly interesting examples of applications of these techniques are the determination of the phase diagram of water by Sanz et al. [54], and the phase diagram of carbon by Ghiringhelli et al. [55]. The phase diagram of water is very rich, with at least nine stable ice phases documented. Many diﬀerent empirical potentials aiming at describing this complicated system have been proposed in the literature, and Sanz and coworkers [54] have compared two of them, namely the so-called TIP4P model of Jorgensen et al. [56], and the SPC/E model of Berendsen et al. [57], in their ability to reproduce the experimental phase diagram of water. Sanz et al. used standard thermodynamic integration to locate coexistence points between the diﬀerent phases, and then obtained the corresponding coexistence lines by using Clausius–Clapeyron integration as proposed by Kofke [17, 18]. The theoretical phase diagrams derived from TIP4P and SPC/E models are compared with the experimental water phase diagram in Fig. 5. As can be seen in Fig. 5, the phase diagram predicted by the TIP4P model agrees fairly well with the experimental one, while that resulting from the SPC/E model deviates noticeably. The TIP4P model correctly predicts ice phases I, II, III, V, VI, VII and VIII to be stable, as indeed they are found to be in real water, while the SPC/E model, on the other hand, predicts wrongly that phases III and V are metastable (i.e., there is no temperature– pressure domain in which these phases are found to have the lowest Gibbs free-energy). A second example, more within the theme of this book, is provided by the phase diagram of carbon obtained by Ghiringhelli et al. [55]. If mod-

Free-Energies in Semiconductors

133

Fig. 6. Phase diagram of carbon as obtained by Ghiringhelli and coworkers [55]. This ﬁgure shows the phase diagram only up to pressures of 60 GPa, but the diamond melting line was followed up to pressures of 400 GPa. The solid black triangle, blue diamond and red square are the three coexistence points from which later the phase boundaries were obtained by Clausius–Clapeyron integration. The pink solid circle is an experimental estimate of the liquid–graphite–diamond triple point. Figure reprinted with kind perission from Ghiringhelli et al. [55]. Copyright (2005) by the American Physical Society

eling water accurately is a signiﬁcant challenge for empirical potentials, as the work of Sanz et al. [54] so nicely illustrates, the situation with carbon is by no means easier. The three phases considered in the study of Ghiringhelli and coworkers, namely graphite, diamond and the liquid phase, have markedly diﬀerent structures and types of bonding, and devising an empirical potential that is capable of reproducing not only these structural and bonding diﬀerences, but also the thermodynamic behavior of each phase, is a signiﬁcant achievement. In this study, the recently developed model of Los and Fasolino [58] was used. Ghiringhelli et al. proceeded, as in the previously discussed example of water, by ﬁrst locating coexistence points between the diﬀerent phases (graphite–diamond, graphite–liquid, and diamond–liquid), and then using Clausius–Clapeyron integration to determine the corresponding phase diagram. A portion of the phase diagram they obtained is shown in Fig. 6, where also some experimentally measured coexistence points are shown for comparison.1 The phase diagram of carbon is a challenge not only for simulation, but even more so for experiments. Indeed the melting temperature of graphite 1

Shortly after this Chapter was sent to the printer, ﬁrst principles calculations of the phase diagram of carbon were published by Wang, Scandolo and Car, [59].

134

E. R. Hern´ andez et al.

occurs well above 4000 K. The melting line of diamond has not to date been experimentally characterized. The situation is a little better for the graphite– diamond coexistence line, for which some measurements exist. As can be seen from Fig. 6, the carbon model of Los and Fasolino [58] predicts a phase diagram that agrees well with the available experimental data. In particular, the slope of the graphite–diamond coexistence curve seems to be well reproduced, although the model predicts this transition to occur at slightly higher pressures than observed experimentally. The graphite melting line occurs at somewhat lower temperatures (ca. 4000 K) than the experimental values, and is predicted to be monotonic with a slight positive pressure derivative, while it appears that the experimental curves show a maximum at around 6 GPa. It should be noticed, however, that the experimental values do not correspond to real measurements, and are in fact indirect estimations based on the ambient-pressure value [55]. A ﬁnal example that we wish to discuss is that of the phase diagram of Si obtained recently by Kaczkarski and coworkers [16]. These authors employed the tight-binding model of Lenosky et al. [14], as it is known that no empirical potential currently available predicts correctly the structure of the liquid phase in this system. The range of temperatures and pressures considered by Kaczmarski et al. encompassed four phases, namely the diamond phase, which is the stable one at ambient conditions, the liquid phase, the β-Sn structure, into which the diamond phase transforms when subject to a sufﬁcient amount of compressive pressure, and the Si36 clathrate phase, which becomes stable at negative (expansive) pressures. As in the case of C, not much experimental data exists concerning the equilibrium conditions of these phases of Si. It is known, however, that the zero-pressure melting point of the diamond phase occurs at 1687 K, and that its melting line has a negative slope, which results from the fact that the liquid phase is denser than the solid, while having a higher enthalpy. In fact, some potential models and even some tight-binding ones, fail to reproduce this behavior correctly, and would consequently produce a qualitatively wrong melting behavior, even if some of them predict the zero-pressure melting point rather accurately. In a previous study, Kaczmarski et al. [15] compared diﬀerent tight-binding models in their ability not only to accurately reproduce the melting temperature of the Si diamond phase, but also the structural properties of the liquid. The choice of the model due to Lenosky et al. for the study of the phase diagram was based on the results of that comparison. One diﬀerence between the previous examples of water and C and the work of Kaczmarski et al. [16] is that in the latter the dynamical version of the Clausius–Clapeyron integration method due to de Koning et al. was used. Also, coexistence points were located from free-energies obtained from the reversible scaling and adiabatic switching techniques. The combined use of these techniques considerably reduced the computational costs compared to what would have been required if standard thermodynamic and Clausius– Clapeyron integration had been used instead.

Free-Energies in Semiconductors

135

Fig. 7. Silicon phase diagram as predicted by the Lenosky model. The continuous and dashed black curves are calculated coexistence lines. Dashed curves indicate phase boundaries in regions where the separated phases are metastable, while continuous black curves separate thermodynamically stable phases; uncertainty bounds estimated at speciﬁc points of the phase diagram (marked by ﬁlled circles) are provided by the error bars. For comparison purposes, a schematic phase diagram summarizing the experimental data is shown with red dotted lines, and experimental data at speciﬁc temperatures and pressures is shown in the form of colored symbols. The asterisk corresponds to the zero-pressure melting point of phase I (diamond ), 1687 K [36]; the brown circle is the zero-pressure melting point of the (metastable) clathrate phase (C), at 1473 K [60]; the blue diamond is the diamond–liquid–β-Sn triple point, with estimated coordinates of 1003 ± 20 K and 10.5 ± 0.2 GPa [61]; red squares and triangles indicate the pressures at which the β-Sn phase (II) was ﬁrst observed and where the diamond phase ceased to be detected, respectively, in the experiments of Voronin et al. [61]; left and right pointing orange triangles give the same information as obtained by Hu et al. [62]; ﬁnally, the downward-pointing green triangle is the estimated diamond–clathrate–liquid triple point, at 1710 K and −2.5 GPa [60]. Figure reprinted from [16]. Copyright (2005) by the American Physical Society

Figure 7 shows the computed phase diagram for Si, compared with available experimental data. It is seen that the overall features of the phase diagram are qualitatively well reproduced by the model. In particular, the negative slope of the melting line of the diamond phase is correct, even if the actual absolute slope value is probably underestimated. The diamond–β-Sn coexistence line is also predicted to have a negative slope, though again the value seems to be smaller than the experimental one. The coexistence line between the diamond and clathrate phases is in good agreement with the only available experimental data on this transition [60].

136

E. R. Hern´ andez et al.

4 Conclusions and Outlook In this Chapter we have given an overview of recent theoretical developments in the methodology of free-energy calculations, and we have also provided a selection of applications, most of them in the ﬁeld of semiconductors, which illustrate current capabilities and provide a glimpse of what the future may bring in this topic. Many outstanding problems still remain, however, and applications in ﬁelds such as metallurgy and mineral science, particularly when variable chemical composition is involved, are still extremely challenging. We feel sure, nevertheless, that future theoretical and methodological developments will render such problems more accessible than they are at present. Acknowledgements E.R.H. and P.O. thank the Spanish Ministry of Education and Science (MEC) for funding their work through project BFM2003-03372-C03 and the bilateral Italian–Spanish collaborative action HI2003-0337; A. A. acknowledges the support from the Brazilian funding agencies FAPESP, CNPq and FAEP-UNICAMP; L. C. acknowledges ﬁnancial support under project MIUR-FIRB2001 (contract RBAU01LLX2).

References [1] D. Frenkel, B. Smit: Understanding Computer Simulation (Academic, New York 1996) 116, 126 [2] M. P. Allen, D. J. Tildesley: (Clarendon, Oxford 1987) 116 [3] J. M. Rickman, R. LeSar: Annu. Rev. Mater. Res. 32, 195 (2002) 116 [4] G. J. Ackland: J. Phys.: Condens. Matter 14, 2975 (2002) 116 [5] M. de Koning, W. P. Reinhardt: in S. Yip (Ed.): Handbook of Materials Modeling (Springer, Berlin, Heidelberg 2005) 116, 120 [6] J. G. Kirkwood: J. Chem. Phys. 3, 300 (1935) 118 [7] D. Frenkel, A. J. C. Ladd: J. Chem. Phys. 81, 3188 (1984) 118 [8] J. K. Johnson, J. A. Zollweg, K. E. Gubbins: Mol. Phys. 78, 591 (1993) 119 [9] D. A. Young, F. J. Rogers: J. Chem. Phys. 81, 2789 (1984) 119 [10] M. Watanabe, W. P. Reinhardt: Phys. Rev. Lett. 65, 3301 (1990) 119, 120, 130 [11] M. de Koning, A. Antonelli, S. Yip: Phys. Rev. Lett. 83, 3973 (1999) 120 [12] M. de Koning, A. Antonelli, S. Yip: J. Chem. Phys. 115, 11025 (2001) 122, 124 [13] C. M. Goringe, D. R. Bowler, E. R. Hern´ andez: Rep. Prog. Phys. 60, 1447 (1997) 122 [14] T. J. Lenosky, J. D. Kress, I. Kwon, A. F. Voter, B. Edwards, D. F. Richards, S. Yang, J. B. Adams: Phys. Rev. B 55, 1528 (1997) 122, 123, 134 [15] M. Kaczmarski, R. Rurali, E. R. Hern´ andez: Phys. Rev. B 69, 214105 (2004) 122, 123, 130, 134

Free-Energies in Semiconductors

137

[16] M. Kaczmarski, O. N. Bedoya-Mart´ınez, E. R. Hern´ andez: Phys. Rev. Lett. 94, 095701 (2005) 123, 134, 135 [17] D. A. Kofke: Mol. Phys. 78, 1331 (1993) 123, 132 [18] D. A. Kofke: J. Chem. Phys. 98, 4149 (1993) 123, 124, 132 [19] R. Agrawal, D. A. Kofke: Mol. Phys. 85, 43 (1995) 125 [20] A. J¨ aa ¨skel¨ ainen, L. Colombo, R. Nieminen: Phys. Rev. B 64, 233203 (2001) 125, 126, 127 [21] I. Kwon, R. Biswas, C. Z. Wang, K. M. Ho, C. M. Soukoulis: Phys. Rev. B 49, 7242 (1994) 126 [22] R. Car, P. Blochl, E. Smargiassi: Mater. Sci. Forum 83–87, 433 (1992) 126 [23] M. Tang, L. Colombo, J. Zhu, T. Diaz de la Rubia: Phys. Rev. B 55, 14279 (1997) 126 [24] H. Bracht, E. E. Haller, R. Clark-Phelps: Phys. Rev. Lett. 81, 393 (1998) 126, 127 [25] T. Y. Tan, U. G¨ osele: Appl. Phys. A: Solids Surf. 37, 1 (1985) 126, 127 [26] S. K. Estreicher, M. Garaibeh, P. A. Fedders, P. Ordej´ on: Phys. Rev. Lett. 86, 1247 (2001) 127 [27] M. Cogoni, B. P. Uberuaga, A. F. Voter, L. Colombo: Phys. Rev. B 71, 121203 (2005) 127 [28] J. Samuels, S. G. Roberts: Proc. Roy. Soc. London, Ser. A 421, 1 (1989) 128 [29] J. R. Rice: J. Mech. Phys. Solids 40, 239 (1992) 128 [30] J. R. Rice, G. E. Beltz: J. Mech. Phys. Solids 42, 333 (1994) 128 [31] Y. Sun, G. E. Beltz: Mater. Sci. Eng. A 170, 67 (1993) 128 [32] E. Kaxiras, M. S. Duesbery: Phys. Rev. Lett. 70, 3752 (1993) 128 [33] M. de Koning, A. Antonelli, M. Z. Bazant, E. Kaxiras, J. F. Justo: Phys. Rev. B 58, 12555 (1998) 128, 129 [34] J. Q. Broughton, X. P. Li: Phys. Rev. B 35, 9120 (1987) 128, 130 [35] F. H. Stillinger, T. A. Weber: Phys. Rev. B 31, 5262 (1985) 128 [36] R. Hull (Ed.): Properties of Crystalline Silicon (Inspec, London 1999) 128, 135 [37] S. J. Cook, P. Clancy: Phys. Rev. B 47, 7686 (1993) 129 [38] J. Tersoﬀ: Phys. Rev. Lett. 56, 632 (1986) 129 [39] J. Tersoﬀ: Phys. Rev. B 37, 6991 (1988) 129 [40] J. Tersoﬀ: Phys. Rev. B 38, 9902 (1988) 129 [41] M. I. Baskes, J. S. Nelson, A. F. Wright: Phys. Rev. B 40, 6085 (1989) 129 [42] O. Sugino, R. Car: Phys. Rev. Lett. 74, 1823 (1995) 130 [43] R. Car, M. Parrinello: Phys. Rev. Lett. 55, 2471 (1985) 130 [44] D. Alf`e, M. J. Gillan: Phys. Rev. B 68, 205212 (2003) 130 [45] G. A. de Wijs, G. Kresse, M. J. Gillan: Phys. Rev. B 57, 8223 (1998) 130 [46] C. R. Miranda, A. Antonelli: J. Chem. Phys. 120, 11672 (2004) 131 [47] E. P. Donovan, F. Spaepen, D. Turnbull, J. M. Poate, D. C. Jacobson: J. Appl. Phys. 57, 1795 (1985) 131 [48] S. K. Deb, M. Wilding, M. Somayazulu, P. F. McMillan: Nature 414, 528 (2001) 131 [49] S. Sastry, C. A. Angell: Nature Mater. 2, 739 (2003) 131 [50] J. F. Justo, M. Z. Bazant, E. Kaxiras, V. V. Bulatov, S. Yip: Phys. Rev. B 58, 2539 (1998) 131 [51] P. Keblinski, M. Z. Bazant, R. K. Dash, M. M. Treacy: Phys. Rev. B 66, 064104 (2002) 131

138

E. R. Hern´ andez et al.

[52] A. Hedler, S. L. Klaumunze, W. Wesch: Nature Mater. 3, 804 (2004) 131 [53] R. L. C. Vink, G. T. Barkema: Phys. Rev. Lett. 89, 076405 (2002) 131 [54] E. Sanz, C. Vega, J. L. F. Abascal, L. G. MacDowell: Phys. Rev. Lett. 92, 255701 (2004) 132, 133 [55] L. M. Ghiringhelli, J. H. Los, E. J. Meijer, A. Fasolino, D. Frenkel: Phys. Rev. Lett. 94, 145701 (2004) 132, 133, 134 [56] W. L. Jorgensen, J. Chandrasekhar, J. D. Madura, R. W. Impey, M. L. Klein: J. Chem. Phys. 79, 926 (1983) 132 [57] H. J. C. Berendsen, J. R. Grigera, T. P. Straatma: J. Phys. Chem. 91, 6269 (1987) 132 [58] J. H. Los, A. Fasolino: Phys. Rev. B 68, 024107 (2003) 133, 134 [59] X. Wang, S. Scandolo, R. Car: Phys. Rev. Lett. 95, 185701 (2005) 133 [60] P. F. McMillan: Nature Mater. 1, 19 (2002) 135 [61] G. A. Voronin, C. Pantea, T. W. Zerda, L. Wang, Y. Zhao: Phys. Rev. B 68, 020102 (2003) 135 [62] J. Z. Hu, L. D. Merkle, C. S. Menoni, I. L. Spain: Phys. Rev. B 34, 4679 (1986) 135

Index a-Si, 131 adiabatic, 119–122, 124, 130, 134 amorphous, 130, 131 anharmonic, 118, 125, 126, 128 basis set, 130 Berendsen, 132 Boltzmann, 116 bulk, 127 canonical, 116–118, 120–122 Car, 130 carbon, 132–134 classical, 116, 120 Clausius–Clapeyron, 123–125, 132–134 cluster, 127 concentration, 115, 125, 127 conﬁgurational entropy, 131 correlation, 130 coupling, 118 covalent, 129 crack, 128 density-functional theory, 128, 130 DFT, 130 diamond, 122, 133–135 diﬀusion, 126

dislocation, 128 EDIP, 131 embedded, 129 empirical, 132–134 energetics, 115 energy barrier, 128 entropy, 115, 120, 126, 131 equilibrium, 118–120, 122–125, 127, 134 exchange, 130 ﬁrst-principles, 115, 126, 127, 130 ﬂuctuation, 119 free-energy, 115–126, 128–130, 132, 134, 136 Ge, 129 general gradient approximation, 130 GGA, 130 Gibbs, 117, 122, 123, 132 glass, 130, 131 Hamiltonian, 116–120, 122 Helmholtz, 117 interface, 123 internal energy, 115, 116, 120 interstitial, 126, 127

Free-Energies in Semiconductors irreversible, 119 isothermal, 117 LDA, 130 Lennard–Jones, 119, 125 Liouville, 120 liquid, 119, 128–130, 133, 134 melting, 122, 124, 128–130, 133–135 migration, 125, 126 mobility, 126–128 molecular dynamics, 126 Parrinello, 130 partition function, 116–118, 121 periodic, 126 phase boundary, 119, 122–124 phase diagram, 119, 125, 128, 132–135 phase-space, 116, 120 population, 127 potential, 115, 116, 118, 121, 122, 125, 128–134 reversible, 116, 119, 120, 122, 124, 131, 134

139

self-diﬀusion, 125–127 self-interstitial, 125, 126 semiempirical, 122 Si, 122, 125–131, 134, 135 silicon, 126, 128, 130, 131 speciﬁc heat, 130 statistical, 116, 121 Stillinger–Weber, 128–131 stress, 128 surface, 120 temperature, 115–134 Tersoﬀ, 129 thermodynamic integration, 118, 120, 122, 124, 126, 128, 132 tight-binding, 122, 126, 127, 129, 134 trajectory, 120 transition, 119, 122, 125, 128, 131, 134, 135 vacancy, 125–127 vibrational entropy, 126 water, 130–134

Quantum Monte Carlo Techniques and Defects in Semiconductors R. J. Needs Theory of Condensed Matter Group, Cavendish Laboratory, University of Cambridge, J. J. Thomson Avenue, Cambridge, CB3 0HE, United Kingdom [email protected] Abstract. The continuum variational and diﬀusion quantum Monte Carlo (VMC and DMC) techniques are stochastic methods for obtaining expectation values of many-body wavefunctions. These methods are capable of achieving very high accuracy, yet the scaling with system size is suﬃciently favorable to allow applications to condensed-matter systems. Defects in semiconductors pose a variety of challenges to computational electronic-structure methods. As well as the large system sizes required, one is faced with calculating energy diﬀerences between rather disparate interatomic bonding conﬁgurations, and calculating excited state energies, sometimes including the energies of multiplets. Applications of VMC and DMC to defects in semiconductors are still in their infancy but, as I will describe, these methods possess features that make them well suited for addressing some important issues in the ﬁeld. In this chapter I ﬁrst discuss why we expect VMC and DMC calculations to be valuable in studying defects in semiconductors. I then review the techniques themselves, concentrating on the issues most pertinent to calculations for defects in solids. I describe recent applications to self-interstitial defects in crystalline silicon, the low-energy electronic states of the neutral vacancy in diamond, and the Schottky defect energy in magnesium oxide. The chapter ends with a perspective on the future of such studies.

1 Introduction Quantum Monte Carlo (QMC) methods in the variational (VMC) and diﬀusion (DMC) forms are stochastic methods for evaluating expectation values of many-body wavefunctions. (For a review of the VMC and DMC methods and applications to solids, see [1].) One of the main attractions of these methods is that the computational cost scales roughly as the square or cube of the number of particles, which is very favorable compared with quantumchemical many-body techniques, allowing applications to condensed-matter. Applications of QMC to defects in semiconductors are still in their infancy but, as I will describe, these methods possess features that make them well suited for addressing important issues in the ﬁeld. In this Chapter I ﬁrst discuss why we expect VMC and DMC calculations to be valuable in studying defects in semiconductors. I then review the techniques themselves, concentrating on the issues most pertinent to defects in solids. Finally, I describe recent applications to point defects in crystalline silicon, diamond and magnesium oxide, ending with a perspective on the future of such studies. D. A. Drabold, S. K. Estreicher (Eds.): Theory of Defects in Semiconductors, Topics Appl. Physics 104, 141–164 (2007) © Springer-Verlag Berlin Heidelberg 2007

142

R. J. Needs

It is important to treat electron-correlation eﬀects accurately when describing the energetics of condensed-matter systems. Defects in semiconductors are not special in this regard, but they exemplify almost all the diﬃculties that may be encountered. For example, we would like to calculate the formation and migration energies of defects. These quantities are related to the energy diﬀerences between structures, which may involve atoms with diﬀerent coordination numbers and bond lengths. We might also be interested, for example, in the properties of a 3d transition metal impurity in a semiconductor, whose electronic properties are diﬃcult to describe accurately. We may also be interested in the excited electronic states of defects, which may involve calculating the energies of multiplets. These are severe tests of electronicstructure methods, which can only be met by techniques that incorporate a sophisticated description of electronic correlation. QMC methods have the potential to provide very accurate energies and, in principle, there are no restrictions on the types of electronic state that can be treated. The N 2 − N 3 scaling of the computational cost with the number of electrons N allows applications to quite large systems, which are certainly suﬃcient for studies of defects in semiconductors. However, the prefactor is large, and a QMC calculation is generally much more expensive than the corresponding density-functional theory (DFT) one. The DMC calculations of Ceperley and Alder [2] provided accurate energies for the homogeneous electron gas, which have been used in constructing parameterized density functionals. Since then, the DMC method has been used in studies of the electrons in molecules, clusters and solids. The power of the DMC method for describing electronic correlation in large systems has been amply demonstrated by recent applications, including studies of point defects in semiconductors [3, 4], the reconstruction of the silicon (001) surface [5] and its interaction with H2 [6], and the calculation of optical excitation energies [7, 8]. The methodology of QMC calculations is being improved rapidly that, together with advances in computing technologies, will allow them to be applied to more complicated systems. I believe that QMC will play an important role in the future of electronic-structure computations. They will not replace DFT studies, but rather complement them by providing higher accuracy, albeit at considerably higher cost.

2 Quantum Monte Carlo Methods The VMC method is conceptually very simple, the energy being calculated as the expectation value of the Hamiltonian with an approximate manybody trial wavefunction. In the more sophisticated DMC method the estimate of the ground-state energy is improved by performing an evolution of the wavefunction in imaginary-time.

Quantum Monte Carlo Techniques and Defects in Semiconductors

143

2.1 The VMC Method The variational theorem of quantum mechanics states that, for a proper trial wavefunction ΨT , the variational energy, ∗ ˆ T (R) dR Ψ (R)HΨ EV = T∗ , (1) ΨT (R)ΨT (R) dR is an upper bound on the exact ground-state energy E0 , i.e., EV ≥ E0 . In (1), ΨT is the many-body wavefunction, the symbol R denotes the 3N ˆ is the many-body dimensional vector of the electron coordinates, and H Hamiltonian. The VMC method was ﬁrst used by McMillan in a study of liquid 4 He [9]. To facilitate the stochastic evaluation, EV is written as (2) EV = p(R)EL (R) dR , where the probability distribution p is p(R) =

|ΨT (R)|2 , |ΨT (R)|2 dR

(3)

and the local energy, EL , is ˆ T. EL (R) = ΨT−1 HΨ

(4)

In VMC one uses a Metropolis algorithm [10] to sample the distribution p, generating M conﬁgurations, Ri , drawn from p. The variational energy is then estimated as EV

M 1 EL (Ri ) . M i=1

(5)

Equation (2) is an importance sampling transformation of (1). Equation (2) exhibits the zero-variance property; as the trial wavefunction approaches an exact eigenfunction (ΨT → φi ), the local energy approaches the corresponding eigenenergy, Ei , everywhere in conﬁguration space. As ΨT is improved, EL becomes a smoother function of R and the number of sampling points, M , required to achieve an accurate estimate of EV is reduced. VMC is a simple and elegant method. There are no restrictions on the form of trial wavefunction that can be used and it does not suﬀer from a fermion sign problem. The main problem is, essentially, that you get out what you put in. Even if the underlying physics is well understood it is very diﬃcult to prepare trial wavefunctions of equivalent accuracy for diﬀerent systems, and therefore the energy diﬀerences between them will be biased. We use the VMC method mainly to optimize parameters in trial wavefunctions, see Sect. 2.4, and our main calculations are performed with the more sophisticated DMC method, which is described in the next section.

144

R. J. Needs

2.2 The DMC Method The DMC procedure largely overcomes the problem of bias inherent in VMC. ˆ is used to project out the ground-state In DMC the operator exp(−tH) from the initial state. This can be viewed as solving the imaginary-time Schr¨ odinger equation, ∂ ˆ − ET Φ(R, t) , (6) − Φ(R, t) = H ∂t where t is a real variable measuring the progress in imaginary-time and ET is an energy oﬀset. The solution of (6) can be obtained by expanding Φ(R, t) in the eigenstates of the Hamiltonian, ci (t)φi (R) , (7) Φ(R, t) = i

which leads to Φ(R, t) = exp[−(Ei − ET )t]ci (0)φi (R) .

(8)

i

For long times one ﬁnds Φ(R, t → ∞) exp[−(E0 − ET )t] c0 (0)φ0 (R) ,

(9)

which is proportional to the ground-state wavefunction, φ0 . If we interpret the initial state, i ci (0)φi , as a probability distribution, then the time-evolution process can be thought of as taking a set of points in conﬁguration space distributed according to the initial state and subjecting them to diﬀusion and branching (branching is also referred to as “birth” and “death” of conﬁgurations). The diﬀusion process arises from the kinetic energy operator and the branching from the potential energy. So far we have assumed that the wavefunction can be interpreted as a probability distribution, but a wavefunction for more than two identical fermions must have positive and negative regions. One can construct algorithms that use two distributions of conﬁgurations, one for positive regions and one for negative, but such algorithms suﬀer from a fermion sign problem that manifests itself by the signal-to-noise ratio decaying exponentially with imaginary-time. The ﬁxed-node approximation [11, 12] allows us to avoid these problems. This method is equivalent to placing inﬁnite potential barriers everywhere on the nodal surface of a trial wavefunction ΨT . (The nodal surface is the 3N − 1 dimensional surface in conﬁguration space on which the wavefunction is zero and across which it changes sign.) The inﬁnite potential barriers have no eﬀect if the trial nodal surface is correct, but if it is incorrect the energy is always raised. The DMC projection can then be done separately in each nodal pocket, which gives the lowest-energy solution in each pocket. It therefore follows that the DMC energy is always less than or equal to the VMC energy

Quantum Monte Carlo Techniques and Defects in Semiconductors

145

with the same trial wavefunction, and always greater than or equal to the exact ground-state energy, i.e., EV ≥ ED ≥ E0 . In addition, it turns out that all the nodal pockets of the exact fermion ground-state are equivalent [13] and, if ΨT has this tiling property, we do not need to sample all of the pockets. Such a ﬁxed-node DMC algorithm is extremely ineﬃcient and a vastly superior algorithm can be obtained by introducing an importance sampling transformation [14, 15]. Consider the mixed distribution, f (R, t) = ΨT (R)Φ(R, t) ,

(10)

which has the same sign everywhere if the nodal surface of Φ(R, t) is constrained to be the same as that of ΨT (R). Substituting in (6) for Φ we obtain 1 ∂f = − ∇2 f + ∇ · [vf ] + [EL − ET ]f , ∂t 2 where the 3N -dimensional drift velocity is deﬁned as −

(11)

v(R) = ΨT−1 (R)∇ΨT (R) .

(12)

The three terms on the right-hand side of (11) correspond to diﬀusion, drift, and branching processes, respectively. The importance sampling transformation has several consequences. First, the density of conﬁgurations is increased where ΨT is large. Second, the rate of branching is now controlled by the local energy that is generally a much smoother function than the potential energy. Finally, the importance sampling actually enforces the ﬁxed-node constraint in (11). In practice one has to use a short-time approximation (for a review of the VMC and DMC methods and applications to solids see [1]) for the Green’s function diﬀusion equation that means that occasionally conﬁgurations attempt to cross the nodal surface, but such moves are simply rejected. This algorithm generates the distribution f , but fortunately we can calculate the corresponding DMC energy using the formula f EL dR (13) ED = f dR M 1 EL (Ri ) . M i=1

(14)

The importance-sampled ﬁxed-node fermion DMC algorithm was ﬁrst used by Ceperley and Alder [2]. It is not possible to obtain directly from f the proper expectation values of operators that do not commute with the Hamiltonian, such as the chargedensity or pair-correlation functions. There are, however, three methods by which such expectation values can be obtained: the approximate (but often very accurate) extrapolation technique [16], the forward-walking technique (explained in Hammond et al. [17]) that is formally exact but statistically poorly behaved, and the reptation QMC technique of Baroni and Moroni [18], which is formally exact and well behaved, but quite expensive.

146

R. J. Needs

2.3 Trial Wavefunctions It should be clear that the trial wavefunction is of central importance in VMC and DMC calculations. The trial wavefunction introduces importance sampling and controls both the statistical eﬃciency and the accuracy obtained. In DMC the accuracy depends only on the nodal surface of the trial wavefunction via the ﬁxed-node approximation, while in VMC it depends on the entire trial wavefunction, so that VMC energies are more sensitive to the quality of the approximate wavefunction than DMC energies. QMC calculations require a compact trial wavefunction, and most studies of electronic systems have used the Slater–Jastrow form, in which a pair of up- and down-spin determinants is multiplied by a Jastrow correlation factor, ΨT = eJ(R) D↑ (R↑ )D↓ (R↓ ) ,

(15)

where eJ is the Jastrow factor and the D are determinants of single-particle orbitals. The quality of the single-particle orbitals is very important, and they are often obtained from DFT or Hartree–Fock (HF) calculations. The Jastrow factor is a positive, symmetric, function of the electron coordinates, which is chosen to be small when electrons are close to one another, thereby introducing electron-correlation into the wavefunction. The Jastrow factor is also used to enforce the electron–electron Kato cusp conditions [19]. The idea is that when two electrons are coincident the contribution to the local energy from the Coulomb interaction diverges, and therefore the exact wavefunction must have a cusp at this point so that the kinetic energy operator supplies an equal and opposite divergence. It seems very reasonable to enforce these conditions on a trial wavefunction as they are obeyed by the exact wavefunction, and in VMC, and more particularly DMC, calculations they are very important because divergences in the local energy can lead to poor statistical behavior. Many excellent QMC results have been obtained using Slater–Jastrow wavefunctions, but it may be proﬁtable to consider other forms. One variant is to use more than one pair of determinants, αi Di,↑ (R↑ )Di,↓ (R↓ ) , (16) ΨT = eJ(R) i

where the αi are coeﬃcients. This approach is not suitable for improving the energy per atom of a solid because the number of determinants required would have to increase exponentially with system size. It is, however, useful when considering a point defect with an open-shell electronic conﬁguration in a solid, in which case the electronic states of the multiplet may be described by a small number of determinants. An example of this is described in Sect. 6.3. Another possibility is to include backﬂow correlations, which may be derived by demanding that the wavefunction conserves the local current [20]. This approach has been used successfully in QMC studies of the

Quantum Monte Carlo Techniques and Defects in Semiconductors

147

electron gas [21], but it has not been explored much for electrons in real atomic systems [22]. Including backﬂow correlations improves the nodal surface of a wavefunction and leads to a compact form that is suitable for use in QMC calculations, although it is more complicated than the Slater–Jastrow form and the computational cost is increased. 2.4 Optimization of Trial Wavefunctions Optimizing trial wavefunctions is perhaps the most important technical issue in QMC calculations, and it consumes large amounts of human and computing resources. It is standard to include a number of variable parameters in the Jastrow factor whose values are determined by a stochastic optimization procedure. The determinant coeﬃcients, αi , in (16) may also be optimized, and in some calculations the orbitals themselves have been optimized. Developing better wavefunction-optimization techniques is currently a very active ﬁeld, with many new approaches being tested. Rather than delving into the technical details of this enterprise, I will mention some of the key issues. Ideally the wavefunction should be optimized within DMC, but this is generally much too costly and so optimizations are performed at the VMC level. Two measures of wavefunction quality have generally been considered. The most obvious idea is to minimize the expectation value of the VMC energy, although more commonly the variance of the VMC energy has been minimized. There are good reasons to suppose that better DMC results would be obtained by using energy-minimized trial wavefunctions, rather than variance-minimized ones. First, it seems likely that a better nodal surface would be obtained by minimizing the energy rather than the variance. Second, it turns out that the variance of the DMC energy is approximately proportional to the diﬀerence between the VMC and DMC energies, rather than the variance of the VMC energy [23]. Why then has it been more common to minimize the variance of the VMC energy? The answer is simply that it has proved easier to devise algorithms for minimizing the variance that are stable and eﬃcient in the presence of statistical noise [24–26]. Most of the current eﬀort is being devoted to developing energy-minimization schemes, although the applications to defects in semiconductors described in this Chapter were performed using variance minimization. 2.5 QMC Calculations within Periodic Boundary Conditions QMC calculations for defects in solids may be performed using cluster models or periodic boundary conditions, just as in other techniques. Periodic boundary conditions are preferred because they give smaller ﬁnite-size eﬀects. In the standard supercell approach a point defect in an otherwise perfect crystal is modeled by taking a large cell containing a single defect and repeating it throughout space. Just as in other techniques, one must ensure that the

148

R. J. Needs

supercell is large enough for the interactions between defects in diﬀerent supercells to be small. In techniques involving many-electron wavefunctions such as QMC it is not possible to reduce the problem to solving within a primitive unit cell (when a defect is present the primitive unit cell is the supercell). Such a reduction is allowed in single-particle methods because the Hamiltonian is invariant under the translation of a single electronic coordinate by a translation vector of the primitive lattice, but this is not a symmetry of the manybody Hamiltonian. Consequently QMC calculations may be performed only at a single k-point. It is possible to perform QMC calculations at diﬀerent k-points [27, 28] and average the results [29], but this is not exactly equivalent to a Brillouin-zone integration within single-particle theories. In the applications described in this Chapter a single k-point was used. Many-body techniques such as QMC also suﬀer from another source of ﬁnite-size eﬀects – the interaction of the electrons with their periodic images. Such an eﬀect is absent in local DFT calculations because the interaction energy is written in terms of the electronic charge density, but the eﬀect is present in HF calculations. These “Coulomb ﬁnite-size eﬀects” are often corrected for using extrapolation techniques (see [1] and references therein), and they may also be reduced using the so-called model periodic Coulomb (MPC) interaction [30]. 2.6 Using Pseudopotentials in QMC Calculations The cost of a DMC calculation increases rapidly with the atomic number, Z, as roughly Z 5.5 [23, 31]. This eﬀectively rules out applications to atoms with Z greater than about 10, and consequently pseudopotentials are commonly used in DMC calculations. The use of nonlocal pseudopotentials within VMC is quite straightforward, but DMC poses an additional problem, because the matrix element of the imaginary-time propagator is not necessarily positive, which leads to a sign problem analogous to the fermion sign problem. To circumvent this diﬃculty an additional approximation known as the pseudopotential localization approximation has been used [32]. If the trial wavefunction is accurate the error introduced by the localization approximation is small and is proportional to (ΨT − φ0 )2 [33], although the error term can be of either sign. Recently, Casula et al. [34] have introduced a fully variational technique for dealing with nonlocal pseudopotentials within DMC. Currently it is not possible to generate pseudopotentials entirely within a QMC framework, and therefore they are obtained from other sources. There is evidence that indicates that HF theory provides better pseudopotentials than DFT for use within QMC calculations [35], and recently we have developed smooth relativistic HF pseudopotentials for H to Ba and Lu to Hg that are suitable for use in QMC calculations [36, 37].

Quantum Monte Carlo Techniques and Defects in Semiconductors

149

3 DMC Calculations for Excited States It might appear that the DMC method cannot be applied to excited states because the imaginary-time propagation would evolve it towards the groundstate. However, the ﬁxed-node constraint ensures convergence to the lowestenergy state compatible with the nodal surface of the trial wavefunction. If the nodal surface is exactly that of an eigenstate then DMC gives the exact energy of that state. If the nodal surface is approximately that of an excitedstate then the DMC energy gives an approximation to the energy of that excited state. There is, however, an important diﬀerence from the groundstate case, in that the existence of a variational principle for the energy of an excited-state depends on the symmetry of the trial wavefunction [38]. In practice, DMC works quite well for excited-states [39, 40].

4 Sources of Error in DMC Calculations Here we summarize the potential sources of errors in DMC calculations. – Statistical error. The standard error in the mean is proportional to √ 1/ M , where M is the number of moves. It therefore costs a factor of 100 in computer time to reduce the error bars by a factor of 10. On the other hand, a random error is much better than a systematic one. – The ﬁxed-node error. This is the central approximation of the DMC technique, and is often the limiting factor in the accuracy of the results. – Timestep bias. The short-time approximation leads to a bias in the f distribution and hence in expectation values. This bias can be serious and is often corrected for by using several diﬀerent timesteps and extrapolating to zero timestep. – Population control bias. In DMC the f distribution is represented by a ﬁnite population of conﬁgurations that ﬂuctuates due to the branching procedure. The population is usually controlled by occasionally changing the trial energy, ET , in (11) so that the population returns towards a target size. This procedure results in a population-control bias. In practice, the population control bias is normally extremely small, in fact so small that it is diﬃcult to detect. – Pseudopotential errors including the localization error. Pseudopotentials inevitably introduce errors that can be signiﬁcant in some cases. The localization error also appears to be quite small, although this has not been tested in many cases. – Finite-size errors within periodic boundary conditions. It is important to study the ﬁnite-size eﬀects carefully, and to correct for them. A number of correction procedures have been devised, mainly involving extrapolation to the thermodynamic limit.

150

R. J. Needs

In electronic-structure theory one is almost always interested in the diﬀerence in energy between two similar systems. All electronic-structure methods for complex systems rely on large cancelations of the errors in the energy differences between systems. In DMC this helps with all the above sources of error except the statistical errors. Fixed-node errors tend to cancel because the DMC energy is an upper bound, but even though DMC often retrieves 95 % or more of the correlation energy, noncancelation of nodal errors is a severe problem for DMC calculations. As mentioned before, the most straightforward way forward is simply to improve the quality of the trial wavefunctions, but perhaps it might also be possible to balance the errors in diﬀerent systems more successfully than is currently possible.

5 Applications of QMC to the Cohesive Energies of Solids A number of VMC and DMC studies have been performed of the cohesive energies of solids. The cohesive energy is calculated as the energy diﬀerence between the isolated atom and an atom in the solid. This is a severe test of QMC methods because the trial wavefunctions used for the atom and solid must be closely matched in quality. Data for Si [30], Ge [28], C [4], Na [41] and NiO [42] have been collected in Table 1. The local spin density approximation (LSDA) data shows the standard overestimation of the cohesive energy, while the QMC data is in good agreement with experiment. These studies have been important in establishing DMC as an accurate method for calculating the energies of solids. Table 1. LSDA, VMC and DMC cohesive energies of solids in eV per atom (eV per 2 atoms for NiO), compared with the experimental values. The numbers in brackets indicate standard errors in the last signiﬁcant ﬁgure. All calculated values contain a correction for the zero-point energy of the solid Method

Si

Ge

C

Na

NiO

LSDA VMC DMC Exp.

5.28 4.48(1) 4.63(2) 4.62

4.59 3.80(2) 3.85(2) 3.85

8.61 7.36(1) 7.346(6) 7.37

1.20 0.9694(8) 1.0221(3) 1.13

10.96 8.57(1) 9.442(2) 9.45

Quantum Monte Carlo Techniques and Defects in Semiconductors

151

6 Applications of QMC to Defects in Semiconductors 6.1 Using Structures from Simpler Methods In the applications of QMC to defects in semiconductors reported to date, the structures were obtained from DFT calculations and the energies recalculated within QMC. Surely this leads to a bias in the energy diﬀerences that might be considerable? The answer must certainly be yes, it does lead to a bias, but here I argue that it may often be quite small. We can pose the question more clearly as “is it sensible to calculate structures using a simple method of limited accuracy and then recalculate the energy diﬀerence between the structures with a sophisticated method of much higher accuracy?”. Consider a system with a single structural coordinate Q, and suppose there are two structures of interest, denoted by 1 and 2, corresponding to local minima in the energy at coordinates Q1 and Q2 , with energies E1 and E2 . Around the two energy minima the energy can be expanded as Around Q1

E(Q) = E1 + α1 (Q − Q1 )2

(17)

Around Q2

E(Q) = E2 + α2 (Q − Q2 ) .

(18)

2

Suppose further that we have a simple method for calculating the energy E(Q) that gives a smoothly varying error of the form ∆E(Q) = βQ ,

(19)

where β is a constant. Within the simple method the errors in the coordinates of the equilibrium structures are obtained by minimizing E + ∆E, which gives ∆Q1 = −

β , 2α1

∆Q2 = −

β , 2α2

and the error in the energy diﬀerence between these structures is β2 1 1 ∆(E1 − E2 ) = β(Q1 − Q2 ) − − . 4 α1 α2

(20)

(21)

Now suppose that we use the structures from the simple method, but recalculate the energies within a sophisticated method that gives a negligible error in the energy. The error in the energy diﬀerence between the structures is then β2 1 1 . (22) − ∆(E1 − E2 ) = 2 α1 α2 Within the simple method the error in the energy diﬀerence is ﬁrst order in β, while for the sophisticated method it is second order. The error in

152

R. J. Needs

Fig. 1. The energy E versus a structural coordinate Q showing two minima for a model system. Solid line: exact energy, dashed line: approximate energy from a simple theory that has an error of 0.1Q. The error in the energy diﬀerence between the two minima obtained from the simple theory is 0.186, while the error in the energy diﬀerence calculated using the accurate energy curve, but evaluated at the minima obtained from the simple theory, is 0.000 45

the energy diﬀerence within the simple method is proportional to Q1 − Q2 , so that the error is large if the structures are very diﬀerent, while in the sophisticated method the error is independent of Q1 − Q2 . This behavior is illustrated in Fig. 1. We therefore conclude that using the sophisticated method to calculate the energy diﬀerence between structures obtained from the simple method leads to only quite small errors. Note also that within this model the quadratic coeﬃcients in the energy, α1 and α2 , are unaltered by the linear error term, so that the simple method gives accurate values for the vibrational frequencies. The model is, of course, highly simpliﬁed, but it illustrates my contention that it is reasonable to take structures from DFT calculations and recalculate the energy diﬀerences between them within QMC. 6.2 Silicon Self-Interstitial Defects The diﬀusion of dopant impurity atoms during thermal processing limits how small silicon devices can be made, and understanding this eﬀect requires a knowledge of diﬀusion on the microscopic scale in situations far from equilibrium. Dopant diﬀusion is mainly controlled by the presence of intrinsic defects such as self-interstitials and vacancies, and therefore it is important to improve our understanding of these defects. Both experimental and theoretical techniques have been brought to bear on these defects but, unfortunately, it has not been possible to detect silicon self-interstitials directly and we must rely on theoretical studies to elucidate

Quantum Monte Carlo Techniques and Defects in Semiconductors

153

their microscopic properties. Electron paramagnetic resonance studies [43] have determined unambiguously that the symmetry of neutral vacancies in silicon is D2d , which is consistent with a Jahn–Teller distortion. Positronlifetime experiments have given a value for the enthalpy of formation of a neutral vacancy in silicon of 3.6 ± 0.2 eV [44]. The self-diﬀusivity of silicon at high temperatures follows an Arrhenius behavior with an activation energy in the range 4.1 eV to 5.1 eV [45]. Signiﬁcant diﬃculties arise with the interpretation of experimental data when the contributions to the self-diﬀusivity from diﬀerent mechanisms are considered. The self-diﬀusivity is usually written as the sum of contributions from independent diﬀusive mechanisms. The contribution of a particular microscopic mechanism can be written as the product of the diﬀusivity, Di , and the concentration, Ci , of the relevant defect, i.e., Di Ci . (23) DSD = i

G¨ osele et al. [46] give estimates of the contributions to the self-diﬀusivity as DI CI = 914 exp(−4.84/kB T ) cm2 · s−1 ,

(24)

from self-interstitials and DV CV = 0.6 exp(−4.03/kBT ) cm2 · s−1 ,

(25)

from vacancies, where kB T is in units of eV. It is believed that self-diﬀusivity in silicon is dominated by vacancies at low temperatures and self-interstitials above 1300 K. The experimental situation regarding the individual values of Di and Ci is, however, controversial. Indeed, experimental data has been used to support values of the diﬀusivity of the silicon self-interstitial, DI , which diﬀer by ten orders of magnitude at the temperatures of around 1100 K at which silicon is processed [47]. The main challenge to theory is to identify the important defects and to predict their properties, comparing with experimental data where available. This includes identifying the diﬀusive mechanisms of the defects, providing accurate values for the Di and the equilibrium values of Ci , and reproducing the experimental data for the self-diﬀusivity. This programme represents an enormous challenge, and although many theoretical studies of point defects in silicon have been performed, the goal is still far away. A number of diﬀerent structures for silicon self-interstitials have been postulated, including the split-110, hexagonal and tetrahedral defects, see Fig. 2. The consensus view from modern DFT calculations is that the split110 and hexagonal structures are the lowest-energy self-interstitials in silicon [48–50], and that the tetrahedral interstitial is unstable. However, even here there has been a surprise. Recent DFT calculations have shown that the hexagonal interstitial is unstable to a distortion out of the hexagonal ring by

154

R. J. Needs

0.48 ˚ A, which lowers the formation energy by 0.03 eV [50]. Another surprise has been that, within DFT, it turns out that the lowest-energy point defect in silicon is neither an interstitial nor the vacancy! Goedecker et al. [49] found that a fourfold coordinated defect (FFCD) had a formation energy at least 0.5 eV lower than the interstitials and vacancy. It is not clear whether this defect could play a role in self-diﬀusion, as its possible diﬀusive mechanisms have not yet been studied. There are some discrepancies between DFT values reported for the formation energies of the split-110 and hexagonal self-interstitials and for the associated migration energies. However, modern calculations [48–50] indicate that the sum of the DFT formation and migration energies is signiﬁcantly smaller than the exponent of 4.84 eV deduced from experimental studies, see (24). An interesting suggestion by Pandey and coworkers [51, 52], based on the results of DFT calculations, was that an exchange of neighboring atoms in the perfect lattice atoms would contribute to self-diﬀusion in silicon. In Pandey’s concerted exchange mechanism two nearest-neighbor atoms interchange via a complicated 3-dimensional path that allows the atoms to avoid large energy barriers [51, 52]. One of the main planks of Pandey’s argument was that the calculated value for the activation energy for this concerted exchange was within the experimental range for self-diﬀusion of 4.1 eV to 5.1 eV [45]. However, as we have already noted, DFT gives even lower energies for interstitials and vacancies, and therefore Pandey’s argument is unsatisfactory. All of the calculations mentioned so far assumed no thermal motion at all, but it is also important, of course, to study ﬁnite-temperature eﬀects. Two DFT molecular dynamics studies have been reported [53, 54], but the energy barriers to interstitial self-diﬀusion are very small (at least within DFT) and highly accurate calculations are required to obtain reliable results. It is rather easier to calculate the equilibrium concentration of defects including the effects of thermal vibrations, and a recent study [50] using DFT perturbation theory gave results that are broadly in agreement with the rather scattered experimental data. Given this background, what role can QMC calculations play in unravelling this complicated problem? In the medium term its role must be to give accurate values for the energies of various defect structures. Given that the LSDA and generalized gradient approximation (GGA) self-interstitial defectformation energies can diﬀer by 0.5 eV it is valuable to quantify the errors in DFT calculations of the defect formation energies. As argued in Sect. 6.1, it should be suﬃcient to use defect structures obtained from DFT calculations for this purpose. 6.2.1 DFT Calculations on Silicon Self-Interstitials Leung et al. [3] and Needs [48] reported LSDA and PW91-GGA results for various interstitial defect formation energies and the saddle point of Pandey’s

Quantum Monte Carlo Techniques and Defects in Semiconductors

155

Fig. 2. The structures of the split-110, hexagonal, and tetrahedral interstitial defects, the saddle point of the concerted-exchange mechanism, and the perfect silicon crystal. After Needs [48]

concerted-exchange mechanism, see Table 2. This work also indicated that the LSDA and PW91-GGA equilibrium defect structures are very similar. One of the features of the various defect structures is the wide range of interatomic bonding they exhibit. In the split-110 structure the two atoms forming the defect are fourfold coordinated, but two of the surrounding atoms are ﬁvefold coordinated. The hexagonal interstitial is sixfold coordinated and its six neighbors are ﬁvefold coordinated. The tetrahedral interstitial is fourfold coordinated and has four neighbors, which are therefore ﬁvefold coordinated. At the saddle point of Pandey’s concerted exchange two bonds are broken so that the exchanging atoms and two other atoms are ﬁvefold coordinated. The DFT energy barriers to diﬀusive jumps between the low-energy structures were calculated, which gave a path for split-110-hexagonal diﬀusion with a barrier of 0.15 eV (LDA) and 0.20 eV (PW91-GGA), and a barrier for hexagonal–hexagonal diﬀusive jumps of 0.03 eV (LDA) and 0.18 eV (PW91GGA).

156

R. J. Needs

Table 2. LDA, PW91-GGA, and DMC formation energies in eV of the selfinterstitial defects and the saddle point of the concerted-exchange mechanism. a 16atom supercell, b 54-atom supercell Defect

LDA

GGA

DMCa

DMCb

Split-110 Hexagonal Tetrahedral Concerted exchange

3.31 3.31 3.43 4.45

3.84 3.80 4.07 4.80

4.96(24) 4.70(24) 5.50(24) 5.85(23)

4.96(28) 4.82(28) 5.40(28) 5.78(27)

6.2.2 QMC Calculations on Silicon Self-Interstitials The DMC calculations were performed for 16- and 54-atom fcc structures obtained from LDA calculations. The Slater–Jastrow trial wavefunctions were formed from determinants of LDA orbitals and Jastrow factors containing up to 64 parameters, whose optimal values were obtained by minimizing the variance of the energy. The DMC defect-formation energies are shown in Table 2. Note that the DMC results for the 16- and 54-atom simulation cells are consistent, indicating that the residual ﬁnite-size eﬀects are small. The clearest conclusion is that the DMC formation energies are roughly 1 eV larger than the PW91GGA values and 1.5 eV larger than the LDA values. The hexagonal interstitial has the lowest formation energy within DMC, while the split-110 interstitial is slightly higher in energy, and the tetrahedral interstitial has a considerably higher energy. The saddle point of the concerted exchange has an energy that is too high to explain self-diﬀusion in silicon. Calculating the energy barriers to diﬀusion within DMC is currently prohibitively expensive, but they can be roughly estimated as follows. The tetrahedral interstitial is a saddle point of a possible diﬀusion path between neighboring hexagonal sites. The DMC formation energy of 5.4 eV for the tetrahedral interstitial is therefore an upper bound to the formation plus migration energy of the hexagonal interstitial. The true formation plus migration energy is expected to be less than this. Within the LDA there is a diﬀusion path for the hexagonal interstitial with a barrier of only 25 % of the tetrahedralhexagonal energy diﬀerence. Applying the same percentage reduction to the DMC barrier then gives an estimate of the formation plus migration energy of the hexagonal interstitial of 5 eV. This estimate is in good agreement with the experimental activation energy for self-interstitial diﬀusion of 4.84 eV [46]. This study demonstrated the importance of a proper treatment of electron correlation when calculating defect-formation energies in silicon. DFT predicts formation plus migration energies that are smaller than those deduced from experiment. The larger defect-formation energies found in the DMC calculations indicate a possible resolution of this problem, which might be an important step in improving our understanding of self-diﬀusion in silicon.

Quantum Monte Carlo Techniques and Defects in Semiconductors

157

6.3 Neutral Vacancy in Diamond The vacancy in diamond is a dominant defect associated with radiation damage, and it exhibits a wider variety of physical phenomena than its counterpart in silicon. Self-diﬀusion in diamond is relevant to growing single-crystal diamond thin ﬁlms on nondiamond substrates. DFT studies have suggested that self-diﬀusion in diamond is dominated by vacancies [55] and that interstitials do not play a signiﬁcant role. A vacancy may be formed by removing an atom, leaving four danglingbonds. The simplest model of the electronic structure of a vacancy is a oneelectron molecular defect picture in which symmetry-adapted combinations of the four dangling-bond states have a1 and t2 symmetry. These levels are, respectively, singly and triply degenerate. In the neutral defect four electrons are placed in the dangling-bond states, giving a a21 t22 conﬁguration. This system is unstable to Jahn–Teller distortion and a spontaneous reduction in symmetry occurs in which the t2 states split into a doubly occupied a1 and empty e state, and a structure with D2d symmetry results. This model is appropriate for the vacancy in silicon but, because of the large electron–electron interaction eﬀects, not for diamond. The prominent GR1 optical transition at 1.673 eV [56] is associated with the neutral vacancy. Uniaxial stress perturbations show that the GR1 transition is between a ground state that is orbitally doubly degenerate with symmetry E and an orbitally triply degenerate excited-state of T symmetry [57]. Both the ground and excited-states undergo Jahn–Teller relaxations, but the eﬀects are dynamic during absorption and the vacancy therefore appears to maintain the Td point group of an atomic site in diamond [58]. Correlation eﬀects among the electrons in the dangling-bonds are very important, but the strong coupling to the solid-state environment must also be included. The electronic states of the defect form a multiplet requiring a multideterminant description [59, 60]. The GR1 optical transition cannot be expressed as a transition between one-electron states, which makes a ﬁrst-principles approach very diﬃcult. For example, approaches based on one-electron states, such as Kohn–Sham DFT or the GW self-energy approach [61, 62], cannot give a full description of the multiplet structure. Von Barth has suggested an approximate scheme for obtaining multiplet energies from DFT calculations [63], but unfortunately this scheme does not permit the calculation of the energy of what is believed to be the excited-state of the GR1 band [64, 65]. QMC appears to be an ideal method for this problem, as one can use a multideterminant description of the defect states while maintaining the favorable scaling with system size. 6.3.1 VMC and DMC Calculations on the Neutral Vacancy in Diamond Hood et al. [4] performed VMC and DMC calculations of the neutral vacancy in diamond using periodic boundary conditions and a simulation cell

158

R. J. Needs

containing 53 atoms. The relaxed ionic positions were obtained from an LSDA calculation in which each of the t2 states was fractionally occupied. The nearest-neighbor atoms of the vacancy were found to relax outwards by 0.1 ˚ A, while the relaxation of the next nearest neighbors was negligible. The trial wavefunctions were of the Slater–Jastrow type with the singleparticle orbitals obtained from an LSDA calculation using a Gaussian basis set. To calculate the multiplet structure of the electronic states of the vacancy, symmetrized multideterminants were used with the conﬁguration in which the a1 states were fully occupied and the t2 states were doubly occupied. This gives rise to 1 A1 , 1 E, 1 T2 , and 3 T1 states, with orbital degeneracies of 1, 2, 3, 3, respectively. The corresponding trial wavefunctions took the form, Ψ1 A1 = eJ(R) D↑x D↓x + D↑y D↓y + D↑z D↓z (26) Ψ1 E = eJ(R) 2D↑x D↓x − D↑y D↓y − D↑z D↓z (27) (28) Ψ1 T2 = eJ(R) D↑y D↓z − D↑z D↓y Ψ3 T1 = eJ(R) D↑yz D↓ .

(29)

In this notation, the superscripts x, y, z label which of the t2 orbitals are included in the determinant, in addition to the a1 and lower-energy orbitals. The values of the parameters in the Jastrow factors were optimized by minimizing the variance of the local energy [24, 25]. Figure 3 shows the DMC energies of the states obtained by Hood et al. [4]. The 1 E state was found to be the ground-state, in agreement with experiment. The state with the lowest-energy electronic excitation from the groundstate that is spin and orbitally dipole allowed was the 1 T2 state, and these states are identiﬁed as giving rise to the GR1 line. The associated DMC transition energy was calculated to be 1.51(34) eV, which lie within the statistical error bars of the experimental value of 1.673 eV. The vacancy-formation energy was calculated to be 6.98 eV within the LSDA, and 5.96(34) eV within DMC. Both of these values include a correction for the Jahn–Teller relaxation energy of the vacancy, which is estimated to be 0.36 eV [64]. The DMC formation energy indicates that it is approximately one eV more favorable to form a neutral vacancy in diamond than predicted by the LSDA. The vacancy-formation energy in diamond has yet to be measured. 6.4 Schottky Defects in Magnesium Oxide Alf`e and Gillan [66] recently used DMC to study the Schottky defect formation energy in MgO. Although MgO is classiﬁed as an insulator rather than a semiconductor, these calculations illustrate very nicely the methodology that can be used to calculate the energetics of charged defects within QMC.

Quantum Monte Carlo Techniques and Defects in Semiconductors

159

Fig. 3. DMC energy diﬀerences from the ground-state in eV with statistical errors for the lowest-symmetry states of the neutral vacancy in diamond. The dotted arrow indicates the lowest spin and orbitally dipole allowed transition. After Hood et al. [4]

Oxide materials are, of course, of great importance as insulating layers in semiconductor devices. The Schottky defect energy of MgO is deﬁned to be the energy change when a Mg2+ and an O2− ion are removed from a perfect MgO crystal, the ions being replaced to form an additional unit cell of perfect crystal. The Schottky defect energy, ES , governs the concentration of vacancies present in thermal equilibrium. The methodology used for calculating ES follows that used in DFT calculations. One way to model the Schottky defect would be to remove an Mg atom and an O atom from a large supercell, but in electronic-structure calculations it is normally preferable to study supercells containing only a single defect, because otherwise the interactions between the defects would be large. Consider a crystal containing N cation and N anion sites. Let EN (ν + , ν − ) denoted the total energy of a crystal containing ν + cation vacancies and ν − anion vacancies. The Schottky defect energy is then ES = EN (1, 0) + EN (0, 1) −

2(N − 1) EN (0, 0) . N

(30)

The systems with a single Mg2+ vacancy and a single O2− vacancy were modeled by supercells subject to periodic boundary conditions. These supercells would each carry a net charge, in which case the electrostatic energy of the system cannot be deﬁned, and therefore an appropriate uniform background charge was added to each supercell to make them charge neutral. In the limit of large N the presence of the uniform background charges makes no diﬀerence to ES . In reality, a ﬁnite value of N must be used, which introduces ﬁnite-size errors. The ﬁnite-size error due to the interaction between the periodic images of the defects was corrected for by a standard method [67]. The DMC calculations used N = 27, i.e., 53 atoms for the defective crystals and 54 for the perfect crystals, and the relaxed atomic positions were

160

R. J. Needs

obtained from LSDA calculations. Slater–Jastrow wavefunctions were used, with orbitals obtained from plane-wave LSDA calculations, and optimized Jastrow factors. For eﬃcient evaluation within the QMC calculations the orbitals were re-expanded in a basis of B-splines or “blips”, which are functions that are strongly localized in real space [68]. The DMC calculations gave ES = 7.5 ± 0.53 eV, while equivalent LSDA calculations using the same pseudopotentialand cell size gave ES = 6.99 eV, and a highly converged LSDA calculation gave ES = 6.76 eV. It is very diﬃcult to measure the Schottky defect energy, but it is estimated to lie within the range 4 eV to 7 eV.

7 Conclusions QMC techniques provide a uniﬁed treatment of both the ground- and excited-state energies of correlated electron systems. They are therefore widely applicable and hold great promise as a computational method to enhance our understanding of defects in solids. Considering that QMC is very costly, there seems little point in using it unless the results are reliably more accurate than those obtained from less costly methods such as DFT. The pursuit of higher accuracy in QMC calculations is, in my opinion, the most important practical issue facing today’s practitioners. Very high accuracy has already been demonstrated for small systems, but the situation for larger systems is less clear. I believe that many careful studies are required before we can conﬁdently assert that QMC techniques reliably achieve highly accurate results for complicated systems such as defects in semiconductors. QMC techniques are currently in a phase of rapid development. The most challenging problem in fermion QMC is the infamous fermion sign problem. Solving the sign problem is certainly extremely diﬃcult and perhaps impossible [69]. It is thought that exact fermion methods that avoid the sign problem will be exponentially slow on a classical computer. However, it is clear that QMC methods can deliver highly accurate results provided the trial wavefunctions are accurate enough. It is important to appreciate that trial wavefunctions can be improved using optimization techniques, whereas improving DFT results requires the development of better density functionals, which seems likely to be a much harder problem. Another important issue is that currently it is not possible to calculate accurate atomic forces within QMC for large systems, and therefore it is not possible to relax defect structures. So far this problem has been avoided by using relaxed structures obtained from DFT calculations. The problem of calculating accurate forces within QMC for large systems is unlikely to be insurmountable, and I believe that a satisfactory solution will be developed in due course. Although QMC methods have a long way to go before they are routinely applied to defects

Quantum Monte Carlo Techniques and Defects in Semiconductors

161

in semiconductors I hope that I have persuaded the reader that such a goal is both desirable and possible. I have discussed applications of the DMC method to self-interstitials in silicon, the neutral vacancy in diamond and Schottky defects in magnesium oxide. These studies have demonstrated the feasibility of DMC studies of defects in semiconductors, and have already produced interesting results that challenge those from other methods. Acknowledgements I would like to thank all of my collaborators who have contributed so much to our QMC project. Much of this work has been supported by the Engineering and Physical Sciences Research Council (EPSRC), UK.

References [1] W. M. C. Foulkes, L. Mitas, R. J. Needs, G. Rajagopal: Rev. Mod. Phys. 73, 33 (2001) 141, 145, 148 [2] D. M. Ceperley, B. J. Alder: Phys. Rev. Lett. 45, 566 (1980) 142, 145 [3] W.-K. Leung, R. J. Needs, G. Rajagopal, S. Itoh, S. Ihara: Phys. Rev. Lett. 83, 2351 (1999) 142, 154 [4] R. Q. Hood, P. R. C. Kent, R. J. Needs, P. R. Briddon: Phys. Rev. Lett. 91, 076403 (2003) 142, 150, 157, 158, 159 [5] S. B. Healy, C. Filippi, P. Kratzer, E. Penev, M. Scheﬄer: Phys. Rev. Lett. 87, 016105 (2001) 142 [6] C. Filippi, S. B. Healy, P. Kratzer, E. Pehlke, M. Scheﬄer: Phys. Rev. Lett. 89, 166102 (2002) 142 [7] A. J. Williamson, J. C. Grossman, R. Q. Hood, A. Puzder, G. Galli: Phys. Rev. Lett. 89, 196803 (2002) 142 [8] N. D. Drummond, A. J. Williamson, R. J. Needs, G. Galli: Phys. Rev. Lett. 95, 096801 (2005) 142 [9] W. L. McMillan: Phys. Rev. A 138, 442 (1965) 143 [10] N. Metropolis, A. W. Rosenbluth, M. N. Rosenbluth, A. H. Teller, E. Teller: J. Chem. Phys. 21, 1087 (1953) 143 [11] J. B. Anderson: J. Chem. Phys. 63, 1499 (1975) 144 [12] J. B. Anderson: J. Chem. Phys. 65, 4121 (1976) 144 [13] D. M. Ceperley: J. Stat. Phys. 63, 1237 (1991) 145 [14] R. C. Grimm, R. G. Storer: J. Comput. Phys. 7, 134 (1971) 145 [15] M. H. Kalos, D. Levesque, L. Verlet: Phys. Rev. A 9, 257 (1974) 145 [16] D. M. Ceperley, M. H. Kalos: Monte Carlo Methods in Statistical Physics (Springer, Berlin, Heidelberg 1979) pp. 145–194 145 [17] B. L. Hammond, W. A. Lester, Jr., P. J. Reynolds: Monte Carlo Methods in ab initio Quantum Chemistry (World Scientiﬁc, Singapore 1994) 145 [18] S. Baroni, S. Moroni: Phys. Rev. Lett. 82, 4745 (1999) 145 [19] T. Kato: Comm. Pure Appl. Math. 10, 151 (1957) 146 [20] R. P. Feynman, M. Cohen: Phys. Rev. 102, 1189 (1956) 146

162

R. J. Needs

[21] Y. Kwon, D. M. Ceperley, R. M. Martin: Phys. Rev. B 58, 6800 (1998) 147 [22] M. Holzmann, D. M. Ceperley, C. Pierleoni, K. Esler: Phys. Rev. E 68, 046707 (2003) 147 [23] D. M. Ceperley: J. Stat. Phys. 43, 815 (1986) 147, 148 [24] C. J. Umrigar, K. G. Wilson, J. W. Wilkins: Phys. Rev. Lett. 60, 1719 (1988) 147, 158 [25] P. R. C. Kent, R. J. Needs, G. Rajagopal: Phys. Rev. B 59, 12344 (1999) 147, 158 [26] N. D. Drummond, R. J. Needs: Phys. Rev. B 72, 085124 (2005) 147 [27] G. Rajagopal, R. J. Needs, S. Kenny, W. M. C. Foulkes, A. James: Phys. Rev. Lett. 73, 1959 (1994) 148 [28] G. Rajagopal, R. J. Needs, A. James, S. Kenny, W. M. C. Foulkes: Phys. Rev. B 51, 10591 (1995) 148, 150 [29] C. Lin, F. H. Zong, D. M. Ceperley: Phys. Rev. E 64, 016702 (2001) 148 [30] P. R. C. Kent, R. Q. Hood, A. J. Williamson, R. J. Needs, W. M. C. Foulkes, G. Rajagopal: Phys. Rev. B 59, 1917 (1999) 148, 150 [31] A. Ma, N. D. Drummond, M. D. Towler, R. J. Needs: Phys. Rev. E 71, 066704 (2005) 148 [32] M. M. Hurley, P. A. Christiansen: J. Chem. Phys. 86, 1069 (1987) 148 [33] L. Mitas, E. L. Shirley, D. M. Ceperley: J. Chem. Phys. 95, 3467 (1991) 148 [34] M. Casula, C. Filippi, S. Sorella: unpublished 148 [35] C. W. Greeﬀ, W. A. Lester, Jr.: J. Chem. Phys. 109, 1607 (1998) 148 [36] J. R. Trail, R. J. Needs: J. Chem. Phys. 122, 014112 (2005) 148 [37] J. R. Trail, R. J. Needs: J. Chem. Phys. 122, 224322 (2005) 148 [38] W. M. C. Foulkes, R. Q. Hood, R. J. Needs: Phys. Rev. B 60, 4558 (1999) 149 [39] A. J. Williamson, R. Q. Hood, R. J. Needs, G. Rajagopal: Phys. Rev. B 57, 12140 (1998) 149 [40] M. D. Towler, R. Q. Hood, R. J. Needs: Phys. Rev. B 62, 2330 (2000) 149 [41] R. Maezono, M. D. Towler, Y. Lee, R. J. Needs: Phys. Rev. B 68, 165103 (2003) 150 [42] R. J. Needs, M. D. Towler: Int. J. Mod. Phys. B 17, 5425 (2003) 150 [43] G. D. Watkins: Defects and Their Structure in Non-Metallic Solids (Plenum, New York 1976) p. 2003 153 [44] S. Dannefaer, P. Mascher, D. Kerr: Phys. Rev. Lett. 56, 2195 (1986) 153 [45] W. Frank, U. G¨ osele, H. Mehrer, A. Seeger: Diﬀusion in Crystalline Solids (Academic, Orlando 1985) p. 64 153, 154 [46] U. G¨ osele, A. Pl¨ ossl, T. Y. Tan: Process Physics and Modeling in Semiconductor Technology (Electrochemical Society, Pennington 1996) p. 309 153, 156 [47] D. Eaglesham: Phys. World 8, 41 (1995) 153 [48] R. J. Needs: J. Phys.: Condens. Matter 11, 10437 (1999) 153, 154, 155 [49] S. Goedecker, T. Deutsch, L. Billard: Phys. Rev. Lett. 88, 235501 (2002) 153, 154 [50] O. Al-Mushadani, R. J. Needs: Phys. Rev. B 68, 235205 (2003) 153, 154 [51] K. C. Pandey: Phys. Rev. Lett. 57, 2287 (1986) 154 [52] E. Kaxiras, K. C. Pandey: Phys. Rev. B 47, 1659 (1993) 154 [53] P. E. Bl¨ ochl, E. Smargiassi, R. Car, D. B. Laks, W. Andreoni, S. T. Pantelides: Phys. Rev. Lett. 70, 2435 (1993) 154

Quantum Monte Carlo Techniques and Defects in Semiconductors

163

[54] S. J. Clark, G. J. Ackland: Phys. Rev. B 56, 47 (1997) 154 [55] J. Bernholc, A. Antonelli, T. M. Del Sole, Y. Bar-Yam, S. T. Pantelides: Phys. Rev. Lett. 61, 2689 (1988) 157 [56] G. Davies, C. P. Foy: J. Phys. C 13, 4127 (1980) 157 [57] C. D. Clark, J. Walker: Proc. Roy. Soc. London Ser. A 234, 241 (1973) 157 [58] G. Davies: Rep. Prog. Phys. 44, 787 (1981) 157 [59] C. A. Coulson, M. J. Kearsley: Proc. Roy. Soc. London Ser. A 241, 433 (1957) 157 [60] M. Lannoo, J. Bourgoin: Point Defects in Semiconductors I: Theoretical Aspects (Springer, Berlin, Heidelberg 1981) pp. 141–145 157 [61] L. Hedin: Phys. Rev. 139, A796 (1965) 157 [62] G. Onida, L. Reining, A. Rubio: Rev. Mod. Phys. 74, 601 (2002) 157 [63] U. von Barth: Phys. Rev. A 20, 1693 (1979) 157 [64] S. J. Breuer, P. R. Briddon: Phys. Rev. B 51, 6984 (1995) 157, 158 [65] A. Zywietz, J. Furthm¨ uller, F. Bechstedt: Phys. Rev. B 62, 6854 (2000) 157 [66] D. Alf`e, M. J. Gillan: Phys. Rev. B 71, 220101 (2005) 158 [67] M. Leslie, M. J. Gillan: J. Phys. C 18, 973 (1985) 159 [68] D. Alf`e, M. J. Gillan: Phys. Rev. B 70, 161101 (2004) 160 [69] M. Troyer, U.-J. Wiese: Phys. Rev. Lett. 94, 170201 (2005) 160

Index absorption, 157 algorithm, 143–145, 147 backﬂow, 146, 147 background charge, 159 basis set, 158 Brillouin-zone, 148 charged defect, 158 classical, 160 cluster, 142, 147 cohesive energy, 150 concentration, 153, 154, 159 concerted exchange, 154–156 coordination, 142 correlation, 142, 145–147, 150, 156, 157 Coulomb, 146, 148 coupling, 157 cusp, 146 dangling-bond, 157 decay, 144 density-functional theory, 142 DFT, 142, 146, 148, 151–157, 159, 160 diamond, 141, 146, 157, 158, 161

diﬀusion, 141, 144, 145, 152, 155, 156 dipole, 158 distortion, 153, 157 dopant, 152 eigenstates, 144 electron, 142, 146–148, 157 electron paramagnetic resonance, 153 electron states, 157 electrostatic energy, 159 energetics, 142, 158 energy barrier, 154–156 equilibrium, 151–155, 159 exchange, 154 excitation, 142, 158 excited-state, 149, 157, 160 fermion, 143–145, 148, 160 ﬁrst principles, 157 force, 160 formation energy, 154, 156, 158 fourfold, 154, 155 Gaussian, 158 Ge, 150

164

R. J. Needs

general gradient approximation, 154 GGA, 154, 155 Green’s function, 145 ground-state, 142–145, 149, 157, 158, 160 GW, 157 Hamiltonian, 142–145, 148 Hartree–Fock, 146, 148 hydrogen, 148 imaginary, 142, 144, 148, 149 impurity, 142, 152 interstitial, 153–157 Jahn–Teller, 153, 157, 158 Kohn–Sham, 157 LDA, 156 liquid, 143 localization, 148, 149 LSDA, 150, 154, 155, 158, 160 Metropolis, 143 migration, 142, 154 molecular dynamics, 154 nonlocal, 148 optical, 157 periodic, 148, 159 periodic boundary conditions, 147, 149 perturbation, 154, 157 plane wave, 160 point defect, 146, 147, 153, 154 population, 149 potential, 142, 144, 145, 149

pseudopotential, 148, 149, 160 quantum Monte Carlo, 141, 142, 145–148, 150–152, 154, 157, 158, 160, 161 real space, 160 relaxation, 158 resonance, 153 Schottky, 158–161 Schr¨ odinger, 144 self-diﬀusion, 154, 156, 157 self-energy, 157 self-interstitial, 152–154, 156, 161 Si, 150 silicon, 141, 142, 152–154, 156, 157, 161 Slater, 146, 147, 156, 158, 160 spin, 146, 150, 158 statistical, 145–147, 149, 150, 158 stress, 157 supercell, 148, 159 surface, 142, 144–147, 149 symmetric, 146 symmetry, 148, 149, 153, 157 temperature, 153, 154 tetrahedral, 153, 155, 156 thermal equilibrium, 159 tiling, 145 total energy, 159 transition, 157, 158 transition metal, 142 uniaxial stress, 157 vacancy, 153, 154, 157–159, 161 variational, 141, 143, 148, 149

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces Arno Schindlmayr1,2 and Matthias Scheﬄer2 1

2

Institut f¨ ur Festk¨ orperforschung, Forschungszentrum J¨ ulich, 52425 J¨ ulich, Germany [email protected] Fritz-Haber-Institut der Max-Planck-Gesellschaft, Faradayweg 4–6, 14195 Berlin-Dahlem, Germany [email protected]

Abstract. We present a quantitative parameter-free method for calculating defect states and charge-transition levels of point defects in semiconductors. It combines the strength of density-functional theory for ground-state total energies with quasiparticle corrections to the excitation spectrum obtained from many-body perturbation theory. The latter is implemented within the G0 W0 approximation, in which the electronic self-energy is constructed non-self-consistently from the Green’s function of the underlying Kohn–Sham system. The method is general and applicable to arbitrary bulk or surface defects. As an example we consider anion vacancies at the (110) surfaces of III–V semiconductors. Relative to the Kohn–Sham eigenvalues in the local-density approximation, the quasiparticle corrections open the fundamental band gap and raise the position of defect states inside the gap. As a consequence, the charge-transition levels are also pushed to higher energies, leading to close agreement with the available experimental data.

1 Introduction The electric properties of semiconductors, and hence their applicability in electronic devices, are to a large degree governed by defects that are either intrinsic or incidentally or intentionally introduced impurities. Considerable eﬀorts, therefore, focus on determining the factors that lead to the formation of point defects and their inﬂuence on a material’s electric properties. The progress in the understanding of the atomic structure of point defects at cleaved III–V semiconductor surfaces, which serve as an illustration in this work, was recently reviewed by Ebert [1]. The possibility to image individual defects using scanning tunneling microscopy (STM) with atomic resolution, in particular, has yielded a wealth of data, but as STM provides a somewhat distorted picture of the electronic states close to the Fermi energy, these results cannot (and should not) be identiﬁed directly with the atomic geometry. Electronic-structure calculations have hence turned out to be an indispensable tool for the interpretation of the experimental ﬁndings. A deeper discussion of this point together with an example for the practical structure determination of a semiconductor surface is given in [2]. For point D. A. Drabold, S. K. Estreicher (Eds.): Theory of Defects in Semiconductors, Topics Appl. Physics 104, 165–192 (2007) © Springer-Verlag Berlin Heidelberg 2007

166

Arno Schindlmayr and Matthias Scheﬄer

defects at the (110) surfaces of III–V semiconductors several calculations were reported [3–8]. They are based on density-functional theory [9], where the exchange-correlation energy is typically treated in the local-density approximation (LDA) [10] or generalized gradient approximations (GGA) [11]. The agreement with experimental STM data appears to be very good. For example, the enhanced contrast of the empty pz orbitals of the two Ga atoms nearest to an anion vacancy in p-type GaAs(110) observed under positive bias and initially interpreted as an outward relaxation [12] could thus be understood to result, instead, from a downward local band bending accompanied by an inward relaxation [3]. The band bending itself is caused by the positive charge of the defect. Another controversy centers on the lateral relaxation of the positively charged anion vacancy. While STM images show a density of states preserving the mirror symmetry of the surface at the defect site [12], early theoretical studies of the lattice geometry based on total-energy minimization produced conﬂicting evidence for [3] and against [4, 5] a possible breaking of the mirror symmetry. Well-converged electronic-structure calculations later conﬁrmed that the distortion is indeed asymmetric [6–8] and that the apparently symmetric STM image results from the thermally activated ﬂip motion between two degenerate asymmetric conﬁgurations. In contrast, theoretical predictions of the electronic properties of point defects have been less successful and still show signiﬁcant quantitative deviations from experimental results. The principal quantities of interest are the location of defect states in the fundamental band gap as well as the charge-transition levels. We will carefully distinguish in this chapter between these two quantities: “defect states” or “defect levels” on the one hand and “charge-transition levels” on the other. The former are part of the electronic structure and can, in principle, be probed by photoemission spectroscopy, although standard spectroscopic techniques are often not applicable due to the low density of the surface defects. The Franck–Condon principle is typically well justiﬁed, because the rearrangement of the atoms happens on a much slower timescale than the photoemission process. Nevertheless, the coupling of the electrons to the lattice may be visible in the linewidths and lineshapes. The defect levels thus contain the full electronic relaxation in response to the created hole in direct photoemission or the injected extra electron in inverse photoemission, but no atomic relaxation. Although investigations of electronic properties frequently rely on the Kohn–Sham eigenvalues from density-functional theory, these only provide a ﬁrst approximation to the true band structure, and quantitative deviations from experimental results must be expected. In particular, for many materials the eigenvalue gap both in the LDA and the GGA underestimates the fundamental band gap signiﬁcantly. Likewise, the position of defect states in the gap cannot be determined without systematic errors. With these words of warning we note, however, that the Kohn–Sham eigenvalues constitute a good and well-justiﬁed starting point for calculating band structures and defect states [13]. Therefore, a

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces

167

perturbative approach starting from the Kohn–Sham eigenvalue spectrum is indeed appropriate. While the measurement of the defect levels (see the discussion on the page previous of this Chapter) probes the geometry before the electron is added or removed, the charge-transition levels are thermodynamic quantities and specify the values of the Fermi energy where the stable charge state of the defect changes. Therefore, the charge-transition levels are aﬀected noticeably by the atomic relaxation taking place upon the addition or removal of an electron. A quantitative analysis must hence be able to accurately compare the formation energies of competing conﬁgurations with diﬀerent numbers of electrons. Density-functional theory at the level of the LDA or GGA is capable of giving a good account of the atomic geometries for many materials. A critical feature is the nonlinearity of the exchange-correlation functional. The pseudopotential approximation, which eﬀectively removes the inner shells from the calculation by modeling their interaction with the valence electrons in terms of a modiﬁed potential, linearizes the core–valence interaction and thus does not treat this contribution correctly. In particular, freezing the d electrons in the core of a pseudopotential leads to poor lattice constants and a distorted electronic structure for some III–V semiconductors, such as GaN, where the Ga 3d states resonate strongly with the N 2s states [14]. For GaAs and InP this is a lesser problem, because the cation d states are energetically well below the anion 2s states and thus are relatively inert. As a result, the LDA and the GGA yield only small deviations from the experimental lattice constants and provide a good starting point for quasiparticle band-structure calculations. However, when competing conﬁgurations with a diﬀerent number of electrons are compared, the relevant energy diﬀerences lack the required quantitative accuracy. As we will show in more detail below, the reason is that these jellium-based approximations of the exchange-correlation energy ignore important features of the exact functional, such as the discontinuity of the exchange-correlation potential with respect to a change in the particle number. As a consequence, previous calculations of charge-transition levels based on the LDA exhibit systematic errors, for example for anion vacancies at InP(110) [6]. As an alternative approach to the electronic structure of point defects, we employ techniques adapted from many-body perturbation theory that we have found to be very fruitful in the past [15]. Exchange and correlation eﬀects are here described by a nonlocal and frequency-dependent self-energy operator. The solutions of the ensuing nonlinear eigenvalue equations have a rigorous interpretation as excitation energies and can be identiﬁed with the electronic band structure. We discuss the calculation of defect states as well as charge-transition levels within this framework and show that the results improve signiﬁcantly upon earlier values obtained from the Kohn– Sham scheme in the LDA. As an example we consider anion vacancies at GaAs(110) and InP(110), but the method is general and can also be applied to other defects at surfaces as well as in the bulk. The (110) surfaces are not only

168

Arno Schindlmayr and Matthias Scheﬄer

the natural cleavage planes of III–V semiconductors, but they have several characteristics that make them particularly interesting for defect studies. As no surface states exist inside the fundamental band gap [16, 17], the Fermi energy of a system that is clean and free from intrinsic defects is not pinned but controlled by the doping of the crystal. Only imperfections, such as anion vacancies or antisite defects, can introduce gap states and pin the Fermi energy at the surface. STM can probe ﬁlled and empty surface states by reversing the bias voltage [12], and both the GaAs(110) and the InP(110) surface are well characterized experimentally. This Chapter is organized as follows. We start in Sect. 2 by reviewing the computational methods. In Sect. 3 we then explain the physics of the defect-free GaAs(110) and InP(110) surfaces. The calculation of defect levels is discussed in Sect. 4 and that of charge-transition levels in Sect. 5, together with a comparison with the available theoretical and experimental data. Finally, Sect. 6 summarizes our conclusions. Unless explicitly indicated otherwise, we use Hartree atomic units.

2 Computational Methods A quantitative analysis of the electronic properties of point defects requires computational schemes that describe not only the ground state but also the excitation spectrum. While density-functional theory with state-of-theart exchange-correlation functionals can be used to determine ground-state atomic geometries, many-body perturbation theory is the method of choice for excited states. In this work we take the Kohn–Sham eigenvalues in the LDA as a ﬁrst estimate and then apply the G0 W0 approximation for the electronic self-energy as a perturbative correction. The latter provides a good account of the discontinuity as well as other shortcomings of the LDA. For this reason we ﬁrst review both schemes, emphasizing their strengths as well as limitations. 2.1 Density-Functional Theory Density-functional theory is based on the Hohenberg–Kohn theorem [9], which observes that the total energy EN,0 of a system of N interacting electrons in an external potential Vext (r) is uniquely determined by the ground-state electron density nN (r). While the Hohenberg–Kohn theorem itself makes no statement about the mathematical form of this functional, it has inspired algorithms that exploit the reduced number of degrees of freedom compared to a treatment based on many-particle wavefunctions. In the Kohn–Sham scheme [10], which underlies all practical implementations, the

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces

169

density is constructed from the orbitals of an auxiliary noninteracting system according to nN (r) = 2

∞

2

fN,j |ϕN,j (r)| .

(1)

j=1

The occupation numbers fN,j are given by the Fermi distribution; at zero temperature they equal one for states below the Fermi energy and zero for states above. The factor 2 stems from the spin summation. Here we only consider nonmagnetic systems and thus assume two degenerate spin channels throughout, although the formalism can easily be generalized if necessary. The energy functional is decomposed as 3 EN,0 ≡ E[nN ] = Ts [nN ] + Vext (r)nN (r) d r + EH [nN ] + Exc [nN ] , (2) where Ts [nN ] is the kinetic energy of the auxiliary noninteracting system and EH [nN ] the Hartree energy. The last term incorporates all remaining exchange and correlation contributions and is not known exactly. In practical implementations it must be approximated, for example by the LDA, which replaces the exchange-correlation energy Exc [nN ] by that of a homogeneous electron gas with the same local density [10]. A variational analysis ﬁnally shows that the total energy is minimized if the single-particle orbitals satisfy 1 2 − 2 ∇ + Vext (r) + VH ([nN ]; r) + Vxc ([nN ]; r) ϕN,j (r) = εKS N,j ϕN,j (r) . (3) The Hartree potential VH ([nN ]; r) and the exchange-correlation potential Vxc ([nN ]; r) are deﬁned as functional derivatives of the corresponding energy terms with respect to the density. The eigenvalues εKS N,j are Lagrange parameters that enforce the normalization of the orbitals. We use the Kohn–Sham scheme to determine the equilibrium geometry of clean surfaces and surface defects by relaxing the atomic coordinates and allowing the system to explore its energetically most favorable conﬁguration. Although the Kohn–Sham eigenvalues diﬀer from the true excitation energies and constitute only an approximation to the quasiparticle band structure, they are often numerically close in practice. This follows from the transitionstate theorem of Slater [18] and Janak [19] and allows a correction within perturbation theory. Here, we are interested in the position of the defect state, which may be occupied or unoccupied, relative to the surface valence-band maximum. As the defect state is separated from the valence-band maximum by a ﬁnite energy diﬀerence, the location obtained from the Kohn–Sham eigenvalue spectrum contains two sources of errors: In addition to the chosen approximation for the exchange-correlation functional, there is another systematic error that is due to fundamental limitations of the Kohn–Sham scheme and would also be present if the exact functional was employed. In order to understand the latter, we now brieﬂy sketch its origin.

170

Arno Schindlmayr and Matthias Scheﬄer

One rigorous result is that the eigenvalue of the highest occupied Kohn– Sham state matches the corresponding quasiparticle energy [20], which is in turn equal to the ionization potential that marks the threshold for photoemission, i.e., εKS N,N = EN,0 −EN −1,0 . If the highest occupied state corresponds to the valence-band maximum, then the unoccupied defect state equals the electron aﬃnity εKS N +1,N +1 = EN +1,0 −EN,0 , because it is the next to be populated by one extra electron added to the system. Unfortunately, this is not the same as the eigenvalue εKS N,N +1 of the ﬁrst unoccupied state obtained from (3). The diﬀerence is due to the fact that the exchange-correlation potential of an insulator Vxc ([nN +1 ]; r) = Vxc ([nN ]; r) + ∆xc + O(1/N ) with ∆xc > 0 changes discontinuously upon addition of an extra electron [21, 22]. A similar argument can be made if the defect state is occupied. As a consequence, the Kohn–Sham eigenvalue gaps diﬀer systematically from the gaps in the true quasiparticle band structure. The magnitude of the discontinuity is still a matter of controversy but is believed to be signiﬁcant. For pure sp-bonded semiconductors like GaAs the LDA underestimates the experimental band gap by about 50 %. The GGA, designed only to improve the total energy, yields a very similar eigenvalue spectrum as the LDA when applied to the same atomic geometry. An entirely diﬀerent construction that permits a more systematic treatment of exchange and correlation is the optimized eﬀective potential method [23]. When evaluated to ﬁrst order in the coupling constant, this approach yields the exact exchange potential, which can be used in band-structure calculations [24]. Remarkably, for many semiconductors the resulting Kohn–Sham eigenvalue gaps are very close to the true quasiparticle band gaps [25]. The signiﬁcance of this observation is under debate, however, because there are indications that it may not uphold if correlation is treated on the same footing. Preliminary results suggest that the eigenvalue gaps are again close to the LDA values if correlation is included within the random-phase approximation [26, 27], but there is currently too little data to make a deﬁnite statement, and all existing calculations at this level also contain additional simpliﬁcations, for example a shape approximation for the potential in the linearized muﬃn-tin orbital method in [27]. The reasoning above suggests that density-functional theory is still, in principle, applicable for calculating the diﬀerence in total energy between ground-state conﬁgurations with diﬀerent electron numbers, which is needed to determine the energetically most favorable charge state of a point defect. However, all jellium-based functionals lack the derivative discontinuity ∆xc of the exact exchange-correlation potential. This neglect reduces the electron aﬃnity EN +1,0 −EN,0 both in the LDA and the GGA if the additional electron occupies a state separated from the valence-band maximum by a ﬁnite energy diﬀerence. For systems in contact with an electron reservoir, such as defects in solids, it hence lowers the threshold for an increase of the electron population. This is consistent with the observation that the calculated charge-transition levels for materials like InP are signiﬁcantly smaller than the available values deduced from experimental measurements [6]. The exact exchange potential,

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces

171

an implicit functional of the density deﬁned in terms of the Kohn–Sham orbitals, includes a derivative discontinuity [13], but the latter exceeds the experimental band gap signiﬁcantly and must hence be partially canceled by a correlation contribution with similar magnitude and opposite sign [25]. As the total energies are by construction close to the corresponding Hartree– Fock values, the electron aﬃnities EN +1,0 − EN,0 are grossly overestimated, and no reliable charge-transition levels can be obtained in this way. Our implementation of density-functional theory employs the plane-wave pseudopotential method in combination with the LDA. We use the parametrization by Perdew and Zunger [28], which is in turn based on the quantum Monte-Carlo data of Ceperley and Alder for the homogeneous electron gas [29]. The norm-conserving pseudopotentials are of the fully separable Kleinman–Bylander form [30]. We choose d as the local component for all pseudopotentials except for In, where p is used instead. The Kohn–Sham wavefunctions are expanded in plane waves with a cutoﬀ energy of 15 Ry. Our calculations are performed with the FHImd code [31, 32]. The bulk lattice constants obtained in this way, 5.55 ˚ A for GaAs and 5.81 ˚ A for InP in the absence of zero-point vibrations, are in good agreement with previously published data [33] and slightly smaller than the experimental values at room temperature by 1.8 % and 1.1 %, respectively [34]. We use the theoretical lattice constants in order to prevent errors resulting from a nonequilibrium unit-cell volume during the relaxation of the surface geometries. 2.2 Many-Body Perturbation Theory Many-body perturbation theory [35] provides powerful techniques to analyze the electronic structure in the gap region, because the framework is designed speciﬁcally to give access to excited states. Quasiparticle excitations created by the addition or removal of one electron are obtained from the one-particle Green’s function ˆ t)ψˆ† (r , t )}|ΨN,0 , G(r, r ; t − t ) = −iΨN,0 |T {ψ(r,

(4)

where |ΨN,0 denotes the ground-state wavefunction of the interacting elecˆ )ψˆ† (r ) exp(−iHt ˆ ) tron system in second quantization, ψˆ† (r , t ) = exp(iHt ˆ t) = exp(iHt) ˆ exp(−iHt) ˆ ψ(r) ˆ are the electron creation and annihiand ψ(r, lation operators in the Heisenberg picture, respectively, and the symbol T sorts the subsequent list of operators according to ascending time arguments from right to left with a change of sign for every pair permutation. The Green’s function can be interpreted as a propagator: For t > t it describes a process in which an extra electron is added to the system at time t . The ˆ but resulting wavefunction is, in general, no eigenstate of the Hamiltonian H a linear combination of many eigenstates |ΨN +1,j . Between the times t and t each projection evolves with its own characteristic phase, and a Fourier analysis of this oscillatory behavior immediately yields the energy spectrum

172

Arno Schindlmayr and Matthias Scheﬄer

εN,j = EN +1,j − EN,0 of the accessible excited states. Likewise, for t > t the Green’s function describes the propagation of an extra hole between t and t , yielding the energies εN,j = EN,0 − EN −1,j . In mathematical terms, we insert a complete set of eigenstates between the ﬁeld operators in (4) and Fourier transform to the frequency axis. The resulting expression G(r, r ; ω) = lim

η→+0

∞

fN,j

j=1 ∞

(1 − fN,j )

+ lim

η→+0

∗ ψN,j (r)ψN,j (r ) ω − εN,j − iη

j=1

∗ ψN,j (r)ψN,j (r ) ω − εN,j + iη

(5)

shows that the poles of the Green’s function correspond directly to the quasiparticle energies εN,j . Signiﬁcantly, these not only yield the true band structure, but the highest occupied state also equals the exact ionization potential EN,0 − EN −1,0 and the lowest unoccupied state the exact electron aﬃnity EN +1,0 − EN,0 . Therefore, many-body perturbation theory provides a convenient way to analyze both defect states and the energetics of charge tranˆ sitions. The wavefunctions ψN,j (r) = ΨN −1,j |ψ(r)|Ψ N,0 for occupied and ˆ ψN,j (r) = ΨN,0 |ψ(r)|Ψ for unoccupied states are obtained from the N +1,j quasiparticle equations 1 2 − 2 ∇ + Vext (r) + VH (r) ψN,j (r) 3 + Σxc (r, r , εN,j )ψN,j (r ) d r = εN,j ψN,j (r) . (6) The self-energy Σxc (r, r , ε) incorporates all contributions from exchange and correlation processes. In contrast to the exchange-correlation potential of density-functional theory, it is nonlocal, energy dependent and has a ﬁnite imaginary part, which is proportional to the damping rate resulting from electron–electron scattering. Together with other relevant decay channels, such as scattering from phonons or impurities, this mechanism is responsible for a ﬁnite lifetime of the excitations. For real materials the self-energy can only be treated approximately. Like the majority of practical applications, we use the G0 W0 approximation [36] Σxc (r, r ; t − t ) = lim iG0 (r, r ; t − t )W0 (r, r ; t − t + η) . η→+0

(7)

The Fourier transform of G0 (r, r ; t − t ) on the frequency axis is constructed in analogy to (5) from the eigenstates of an appropriate mean-ﬁeld system, in our case from the Kohn–Sham orbitals ϕN,j (r) and eigenvalues εKS N,j . The dynamically screened Coulomb interaction W0 (r, r ; t − t ) can be modeled in diﬀerent ways. Many implementations use plasmon-pole models, in which the frequency dependence is described by an analytic function whose parameters are determined by a combination of known sum rules and asymptotic limits [37,38]. This simpliﬁcation has the advantage that it facilitates an analytic

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces

173

treatment, but it ignores details of the dynamic screening processes in a material and thus constitutes a potential source of errors. Here we take the full frequency dependence of the dielectric function into account by employing the random-phase approximation W0 (k, ω) = v(k) + v(k)P0 (k, ω)W0 (k, ω)

(8)

with the bare Coulomb potential v(k) = 4π/|k|2 and the polarizability P0 (r, r ; t − t ) = −2iG0 (r, r ; t − t )G0 (r , r; t − t) .

(9)

The inclusion of dynamic screening derives from the concept of quasiparticles, which comprise an electron or hole together with its surrounding polarization cloud. The composite is called a quasiparticle because it behaves in many ways like a single entity. The polarization cloud is created by the repulsive Coulomb potential and reduces the eﬀective charge of the quasiparticle compared to that of the bare particle at its center. The G0 W0 expression (7) constitutes the leading term in the expansion of the self-energy and is of ﬁrst order in the dynamically screened interaction. Finally, we exploit the formal similarity between (6) and the Kohn–Sham equations (3) by evaluating the quasiparticle energies within ﬁrst-order perturbation theory as εN,j = εKS N,j + ϕN,j |Σxc (εN,j ) − Vxc [nN ]|ϕN,j .

(10)

The treatment within ﬁrst-order perturbation theory is justiﬁed if the eigenvalues of the underlying Kohn–Sham system are already suﬃciently close to the expected quasiparticle band structure. This is guaranteed by the transition-state theorem [18, 19]. Besides, the orbitals ϕN,j (r) are usually a good approximation to the true quasiparticle wavefunctions. For the homogeneous electron gas both are plane waves and thus coincide exactly. Numerical calculations for bulk semiconductors indicate an overlap close to unity between the Kohn–Sham orbitals in the LDA and the quasiparticle wavefunctions obtained from (6) with the G0 W0 approximation for states near the band edges [39]. Larger eﬀects have been observed for surfaces, especially for image states, because the latter are located outside the surface in a region where the LDA potential is qualitatively wrong [40, 41]. Changes in the wavefunctions of other surface states can also be identiﬁed but have only a minor inﬂuence on the quasiparticle energies in the gap region. For GaAs(110) this has been conﬁrmed explicitly [42]. In principle, the equations (4) to (9) could be solved self-consistently by successively updating the self-energy with the quasiparticle orbitals derived from it. This approach is appealing on formal grounds because it makes the results independent of the original mean-ﬁeld approximation. In addition, the self-consistent Green’s function satisﬁes certain sum rules, including particlenumber conservation [43]. In practice, however, this procedure produces a poor excitation spectrum. The reason lies in the mathematical structure of

174

Arno Schindlmayr and Matthias Scheﬄer

Hedin’s equations, which describe the recipe for constructing the self-energy from the Green’s function by means of functional-derivative techniques [36]. The G0 W0 approximation is the result of a single iteration. Further iterations would not only ensure self-consistency in the Green’s function but would also introduce higher-order self-energy terms, so-called vertex corrections. If the latter are neglected, then the spectral features deteriorate, as was ﬁrst demonstrated for the homogeneous electron gas [44]. For bulk semiconductors self-consistency appears to lead to a gross overestimation of the fundamental band gap [45] in combination with poor spectral weights and linewidths. We hence follow the established procedure for practical applications and terminate the cycle at the G0 W0 approximation. Of course, the ﬁnal results depend on the input Green’s function in this case. Another point that has been raised in the same context concerns possible errors resulting from the pseudopotential approach, which has traditionally dominated applications of the G0 W0 approximation. Numerical deviations must be expected because the matrix elements of the self-energy in (10) are inﬂuenced by the pseudoization of the wavefunctions – that is the neglect of core states plus appropriate smoothening of the valence states in the core region – and the treatment of the core–valence interaction in pseudopotential calculations. Indeed, a number of early all-electron implementations of the G0 W0 approximation, based on the linearized augmented plane-wave or the linearized muﬃn-tin orbital method, found quasiparticle band gaps for prototype semiconductors that were signiﬁcantly smaller than previously reported values and blamed the discrepancy on the pseudopotential approximation [46, 47]. However, this claim was later refuted by all-electron calculations using plane waves [48, 49]. The issue is currently still under debate, but there is mounting evidence that a large part of the observed discrepancy is due to insuﬃcient convergence of the early calculations in combination with deﬁciencies of the linearized basis sets for the description of high-lying unoccupied states [48, 50]. If these factors are properly accounted for, then the deviation is signiﬁcantly reduced, and the all-electron results are again in good agreement with experimental measurements. A certain discrepancy with respect to pseudopotential calculations still remains, although the diﬀerence is small compared to that from the Kohn–Sham eigenvalues. While some errors of the pseudopotential approach can be partially suppressed, for example through a better description of the core–valence interaction [51], many others are inherent. In particular, the pseudopotential construction also entails an incorrect description of high-lying states. A careful analysis of the quantitative implications of the pseudopotential approximation is the subject of active research. The good quantitative agreement between the G0 W0 approximation and experimental band structures has been demonstrated for a wide range of bulk materials, including III–V semiconductors [52–54]. Due to the high computational cost in present implementations, which stems from the evaluation of the nonlocality of the propagators, their frequency dependence, and the

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces

175

Fig. 1. Bulk band structure of GaAs. The G0 W0 approximation (straight lines) opens the too small Kohn–Sham eigenvalue gap in the LDA (dashed lines) and is in very good agreement with the experimental band gap. The calculation is carried out at the theoretical lattice constant 5.55 ˚ A, and the valence-band maximum is set to zero in both schemes

need to include a large number of unoccupied states, there have been relatively few applications to more complex systems so far, however. Furthermore, these often contain additional simpliﬁcations: the two available studies of the quasiparticle band structure of GaAs(110) both employed plasmon-pole models instead of the more accurate random-phase approximation [55, 56], and the only published results for InP(110) were obtained within an even more restrictive tight-binding formalism [57]. For a quasiparticle band-structure calculation the matrix elements of the self-energy in (6) must be evaluated in the frequency domain for states with a given wavevector k. Therefore, most practical implementations of the G0 W0 approximation choose a reciprocal-space representation for all propagators. The cell-periodic part of the wavefunctions is often expanded in plane waves [52, 55], although localized basis sets like Gaussian orbitals have also been used [54]. The disadvantage of the representation in reciprocal space is that the products (7) and (9) turn into numerically expensive multidimensional convolutions. Therefore, we employ a representation in real space and imaginary time [58, 59], in which the self-energy and the polarizability can be calculated by simple multiplications. The projection on wavevectors and imaginary frequencies used to solve the Dyson-type equation (8) can be done eﬃciently by exploiting fast Fourier transforms. The imaginary time and frequency arguments are chosen because the functions are smoother on these axes and can be sampled with fewer grid points, although they contain

176

Arno Schindlmayr and Matthias Scheﬄer

exactly the same information. The physical self-energy on the real frequency axis is eventually recovered by an analytic continuation. As an illustration of the G0 W0 approximation we show the calculated bulk band structure of GaAs in Fig. 1. The band gap is direct and located at Γ in the center of the Brillouin zone. While the LDA underestimates the fundamental band gap and yields a Kohn–Sham eigenvalue gap of only 0.78 eV at a lattice constant of 5.55 ˚ A, the subsequent addition of the self-energy correction opens the band gap to 1.55 eV, which is in very good agreement with the experimental value of 1.52 eV [34]. As we measure all energies relative to the valence-band maximum, we set the latter to zero and align the two sets of curves at this point. The principal eﬀect of the G0 W0 approximation is a rigid upward shift of the conduction bands, although the dispersion is also slightly modiﬁed, as can be seen by the reduced bandwidth at the bottom of the valence band. The band structure of InP looks very similar. In this case we obtain a Kohn–Sham eigenvalue gap of 0.76 eV at the theoretical lattice constant 5.81 ˚ A and a quasiparticle band gap of 1.52 eV that is again close to the experimental value 1.42 eV [34]. Incidentally, the band gap depends sensitively on the lattice constant. For GaAs it decreases at a rate of −4.07 eV/˚ A in the LDA and −4.59 eV/˚ A in the G0 W0 approximation when the lattice constant increases. For InP the values are −3.13 eV/˚ A and −3.68 eV/˚ A.

3 Electronic Structure of Defect-Free Surfaces Before focusing on defect states we ﬁrst brieﬂy discuss the electronic structure of the defect-free GaAs(110) and InP(110) surfaces. The nonpolar (110) surface, illustrated in Fig. 2, is the natural cleavage plane of the zincblende lattice, because it cuts the smallest number of bonds per unit area. Both the cations and anions in the terminating layer are threefold coordinated, and each possess one dangling bond extending into the vacuum. Due to the diﬀerent electron aﬃnities of the two species, charge is transfered from the dangling bonds of the cations to those of the anions. This charge transfer is the driving force for a structural relaxation, which consists of an outward movement of the anion atoms and a corresponding inward movement of the cation atoms [33]. As a result, the orbitals of the latter rehybridize from an sp3 towards an energetically more favorable sp2 bonding situation in a nearly planar environment; the empty pz -like orbitals perpendicular to this plane are pushed to higher energies and form an unoccupied surface band. At the same time, the three bonds between the anions and their neighboring group-III atoms are rearranged at almost right angles and become more p-like in character; the nonbonding electron pairs in the fourth orbital pointing away from the surface are in turn lowered in energy and give rise to an occupied surface band. The relaxation preserves the C1h point-group symmetry with a single mirror plane perpendicular to the [¯ 110] direction.

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces

177

Fig. 2. Geometry of the anion vacancy at the GaAs(110) surface. The As atoms are shown in light and the Ga atoms in dark gray. The three Ga atoms nearest to the vacancy are indicated by arrows

In Fig. 3 we show the calculated band structure of the clean and defectfree GaAs(110) surface at the theoretical lattice constant 5.55 ˚ A, modeled as a slab element placed in a supercell with periodic boundary conditions in all directions. The slab consists of six atomic layers, of which the top three layers are allowed to relax, while the three base layers are kept ﬁxed at their ideal bulk positions. The dangling bonds at the bottom of the slab are passivated by pseudoatoms with noninteger nuclear charges of 0.75 and 1.25 for anion and cation termination, respectively. The slabs are separated by a vacuum region equivalent to four atomic layers. The gray-shaded regions in the ﬁgure mark the projection of the G0 W0 bulk bands onto the two-dimensional surface Brillouin zone, shown in the inset. The dashed lines indicate the occupied and unoccupied surface bands obtained from the LDA, the straight lines are the corresponding G0 W0 results. For the calculation of the groundstate density and the Kohn–Sham eigenvalues we used four Monkhorst–Pack k-points [60] in the irreducible part of the Brillouin zone, while the self energy was evaluated at the four high-symmetry points Γ, X , M, and X. In our implementation the k-point set enters merely as the reciprocal grid of the real-space mesh used to describe the nonlocality of G0 (r, r ; t − t ) and Σxc (r, r ; t − t ) [58]; the four selected k-points correspond to a real-space mesh that extends over four surface unit cells. This is suﬃcient, because the correlation length is of the order of the interatomic distance [61]. The position of the Kohn–Sham surface bands relative to the corresponding bulk bands was determined by aligning the electrostatic potential in the central part of the slab with that of the bulk. We then applied the self-energy correction independently to surface and bulk bands and again chose the valence-band maximum as the energy zero. From the ﬁgure it is evident that the G0 W0 approximation has only a small eﬀect on the dispersion of the surface bands.

178

Arno Schindlmayr and Matthias Scheﬄer

Fig. 3. Surface band structure of GaAs(110) in the LDA (dashed lines) and the A. The G0 W0 approximation (straight lines) at the theoretical lattice constant 5.55 ˚ gray-shaded regions mark the projected G0 W0 bulk bands. The inset indicates the two-dimensional surface Brillouin zone

While the position of the occupied surface band relative to the valence-band edge at Γ remains almost unchanged, the upward shift of the unoccupied surface band (0.86 eV) slightly exceeds that of the bulk conduction bands (0.77 eV). The larger impact of the self-energy correction on the surface gap was noticed before [55, 56]; our result for the gap correction lies between the two previously published values. Small deviations of about 0.1 eV are due to diﬀerences in the implementations, for example the reliance on plasmon-pole models in [55, 56] compared to the random-phase approximation for the dynamically screened Coulomb interaction in this work. Both the occupied and the unoccupied surface bands are in close proximity to the projected bulk bands and, in fact, overlap with them in large parts of the Brillouin zone. As neither extends into the fundamental gap between the bulk valence and conduction band edges at Γ, they do not pin the surface Fermi level. Although prevalent in electronic-structure calculations for surfaces, the supercell approach is a drastic alteration of the system’s geometry whose inﬂuence must be carefully monitored, because the occurrence of electric multipole moments may lead to artiﬁcial long-range interactions between the periodic slabs. Static dipoles, if present, can be eliminated in density-functional theory [62]. With this correction the limit of isolated slabs is quickly reached. Dynamic dipoles are always created in dielectric media, however, and contribute to the polarizability in the G0 W0 approximation. Actually, there are two contributions that must be distinguished. The ﬁrst is the dynamic polarization between the slabs, which gives rise to an additional slowly varying potential that reduces the band gap. This eﬀect can be understood and even

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces

179

quantitatively modeled in terms of classical image charges [63]; for the geometry used in this work it amounts to about 0.1 eV. The model thus allows an a-posteriori extrapolation to the limit of an isolated slab. The second contribution is the ﬁnite width of the slab, which increases the gap due to quantization eﬀects. At present there is no obvious cure for this problem within the G0 W0 approximation, and as the two eﬀects counteract each other, we have not applied any partial correction to eliminate the dynamic polarization between the slabs either. In principle, both problems could be avoided by studying systems comprised of semi-inﬁnite matter and vacuum regions. Within density-functional theory several methods have indeed been proposed for this purpose [64–67]. Their eﬃciency relies on the fact that a perturbation breaking the translational symmetry, such as a surface or defect, modiﬁes the eﬀective potential only in its immediate vicinity. In the G0 W0 formalism this cannot be exploited to the same degree, because all propagators are explicitly nonlocal, and a much larger simulation cell must hence be taken into account. So far, only one G0 W0 calculation for an eﬀectively one-dimensional system, a semi-inﬁnite jellium surface, has been reported [68]. In preparation for later applications to larger supercells, we repeated the G0 W0 calculation with lower cutoﬀ energies and found that the self-energy correction to the surface gap remained stable up to 10 Ry. The reason for the rapid convergence, which is well known and can be exploited to reduce the computational expense considerably, is that the kinetic energy and the electrostatic Hartree potential, the two largest contributions to the quasiparticle energies, are already included in the Kohn–Sham eigenvalues in (10); the matrix elements of the self-energy are less sensitive to the number of plane waves. Besides, we obtained essentially the same surface gap when reducing the width of the slab to four layers. For this geometry and a cutoﬀ energy of 10 Ry, we performed test calculations in which we included up to 1049 unoccupied bands in the Green’s function. With 379 bands the results are already converged within 0.02 eV, suﬃcient for our purpose.

4 Defect States The geometry of the anion vacancy is illustrated in Fig. 2 for the GaAs(110) surface. The removal of the As atom leaves each of the three Ga atoms surrounding the vacancy with a dangling bond. As a consequence, the two GaI atoms in the ﬁrst layer move downwards while the GaII atom in the second layer moves upwards and forms two new bonds with the GaI atoms across the void. Its coordination number thus increases from four to ﬁve, while the threefold coordination of the GaI atoms remains unchanged. The relaxation preserves the C1h point-group symmetry, except in the positive charge state where an asymmetric distortion that pushes the unoccupied defect level in the band gap to higher energies is more favorable [6, 8]. We ﬁnd that the distortion lowers the total energy by 0.17 eV for GaAs and 0.11 eV for InP.

180

Arno Schindlmayr and Matthias Scheﬄer

The anion vacancy gives rise to three electronic states, all localized at the GaI –GaII bond pair. They are labeled as 1a , 1a and 2a , where a denotes states that are even with respect to the mirror plane and a denotes states that are odd. Although the asymmetric relaxation in the positive charge state destroys this symmetry and deforms the orbitals slightly, it leaves the order of the states intact, and we continue to use the same notation for simplicity. The 1a state is located several eV below the valence-band maximum and thus always ﬁlled with two electrons, while the 2a state is too high in energy to become populated. Only the 1a state falls inside the fundamental band gap. Depending on the doping, it can be occupied either by zero, one or two electrons, which corresponds to the positive, neutral or negative charge state, respectively. It is important to note that the charge state inﬂuences the defect geometry, as the GaI –GaII bonds contract with increasing electron occupancy, reﬂecting the bonding character of the 1a state. In the following we examine the position of this defect level for a given charge state; the question of which charge state is preferred under speciﬁc conditions, such as doping, is answered in the next section. For the density-functional calculations we choose a supercell consisting of 2 × 4 surface unit cells and six atomic layers. For charged systems we include a uniform charge density with opposite sign in order to compensate the extra electron or hole and restore overall neutrality in the supercell. Instead of a well-deﬁned defect state, the supercell periodicity gives rise to an artiﬁcial dispersion as illustrated in Fig. 4. At the surface of each slab the defects form a rectangular grid whose lattice parameters ax and ay equal the dimensions of the supercell. Since the 1a state is odd with respect to the mirror plane, one can regard it as a p orbital that exhibits π-type bonding along the [001] and σ-type bonding along the [¯ 110] direction. We hence consider a tight-binding model KS KS KS εKS k = ε1a + 2V1π cos(kx ax ) + 2V1σ cos(ky ay ) KS KS cos(2kx ax ) + 2V3σ cos(2ky ay ) + V2KS cos(kx ax ) cos(kx ax ) + 2V3π (11)

with parameters ﬁtted to the calculated Kohn–Sham band, where εKS 1a equals the eigenvalue of a single defect and the other parameters have the meaning of hopping integrals. The above expression includes interactions up to thirdnearest neighbors and reproduces the dispersion with a correlation coeﬃcient close to 0.999 9 for all systems under consideration. As the G0 W0 formalism involves nonlocal propagators, the amount of data that must be processed grows rapidly with the system size. In order to limit the computational expense we use a smaller (2 × 2) supercell and four atomic layers instead of the (2 × 4) cell to determine the self-energy correction of the 1a state. The stronger defect–defect interaction along the [¯110] direction increases the dispersion but does not change it qualitatively. As the presence of the defect does not modify the range of the nonlocal propagators appre-

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces

181

Fig. 4. Calculated 1a defect level of the As vacancy at GaAs(110) in the (a) positive and (b) negative charge state (dashed line: LDA; solid line: G0 W0 ). The artiﬁcial dispersion in the LDA is due to the supercell periodicity; the horizontal lines mark the actual defect level εKS 1a and the corresponding G0 W0 result. As the calculations in (a) refer to the constrained symmetric relaxation, the additional shift due to the asymmetric distortion is shown separately. The inset in (b) indicates the downfolded Brillouin zone for the (2 × 4) supercell

ciably, we use one k-point and 1500 unoccupied bands for the construction of the Green’s function G0 , which corresponds to the same Brillouin-zone sampling as the four k-points and 379 bands that we found satisfactory for the (1 × 1) unit cell of the defect-free surface. For the positively charged As vacancy at GaAs(110) we evaluated the self-energy correction in the entire Brillouin zone [15]. By relating the calculated quasiparticle dispersion to a tight-binding model equivalent to (11), we found very similar values for the parameters V3π and V3σ as in the LDA, which implies that the inﬂuence of the third-nearest neighbors on the self-energy correction is negligible. This observation can be exploited as follows. At k = (2π/4)(1/ax , 1/ay , 0) the contributions from the ﬁrst- and second-nearest neighbors vanish, so that the Kohn–Sham eigenvalue is given by KS KS KS εKS k = ε1a − 2V3π − 2V3σ ,

(12)

and the corresponding quasiparticle energy by εk = ε1a − 2V3π − 2V3σ .

(13)

182

Arno Schindlmayr and Matthias Scheﬄer

If the surviving hopping integrals on the right-hand sides coincide, then KS the identity ε1a − εKS 1a = εk − εk holds. On the other hand, the self-energy correction is deﬁned through the relation KS KS KS εk − εKS k = ϕk |Σ(εk ) − Vxc |ϕk .

(14)

Instead of a scan over the whole Brillouin zone, we can hence determine the self-energy correction for an isolated defect from a single calculation at k . The quasiparticle results are obtained by adding this correction to the Kohn– Sham value εKS 1a of the larger (2×4) supercell, where the position of the latter relative to the valence-band maximum can be established more accurately. We estimate that the uncertainty of the ﬁnal quasiparticle energies, which results from the discrete k-point sampling, the approximate treatment of the core–valence interaction in the pseudopotential approach, the ﬁnite size of the supercell, and other convergence factors amounts to 0.1 eV to 0.2 eV. We performed explicit G0 W0 calculations for the positive and negative charge states, in the ﬁrst case using a constrained symmetric relaxation. The results for GaAs(110) are displayed in Fig. 4. For the neutral anion vacancy the supercell contains an odd number of electrons; in combination with the requirement of spin degeneracy this leads to fractional occupation numbers in each spin channel. At present we cannot treat such systems. For the positive charge state with the proper asymmetric distortion the defect level in the G0 W0 approximation is not calculated directly but deduced as follows. As the lowest unoccupied state, the 1a defect level equals the electron aﬃnity, i.e., ε1a = E vac (0, Qasym ) − E vac (+, Qasym ), where E vac (q, Q) denotes the + + total energy of a surface featuring an anion vacancy with the actual electron population q ∈ {+, 0, −} and a geometric structure optimized for the charge , Qsym state Q ∈ {Qasym + + , Q0 , Q− }. This expression can be rewritten as ε1a = E vac (0, Qasym ) − E vac (0, Qsym + + ) vac + E vac (0, Qsym (+, Qsym + )−E + ) vac + E vac (+, Qsym (+, Qasym ) (15) + )−E + by adding and subtracting intermediate conﬁgurations. The term in the second line on the right-hand side equals the quasiparticle energy for the corresponding symmetric relaxation, which can be calculated with less computational cost by exploiting the C1h point-group symmetry. The other two terms are simple total-energy diﬀerences between the symmetric and the asymmetric geometry for a constant number of electrons; both are positive and can be obtained from density-functional theory. The calculated defect levels are summarized in Table 1 for GaAs(110) and Table 2 for InP(110). Our LDA results are consistent with most of the previously published calculations [3, 5, 7]. A notable exception are the values by Zhang and Zunger [3] for the negative charge state of the As vacancy at GaAs(110) and for the constrained symmetric geometry of the positive charge

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces

183

Table 1. Calculated defect levels for the As vacancy at GaAs(110) in eV relative to the valence-band maximum. For the positive charge state the ﬁrst column refers to the asymmetric and the second to the constrained symmetric relaxation. The quasiparticle band gap of 1.55 eV in this work, calculated at the theoretical lattice constant 5.55 ˚ A, is close to the experimental value of 1.52 eV Charge state LDA (this work) LDA [3] LDA [5] G0 W0 (this work)

(+1) 0.70 0.73 1.08

(0.06) (0.41) (0.06) (0.59)

(0)

(−1)

0.13

0.24 0.5 0.24 0.48

0.23

Table 2. Calculated defect levels for the P vacancy at InP(110) in eV relative to the valence-band maximum. For the positive charge state the ﬁrst column refers to the asymmetric and the second to the constrained symmetric relaxation. The quasiparticle band gap of 1.52 eV in this work, calculated at the theoretical lattice constant 5.81 ˚ A, slightly exceeds the experimental value of 1.42 eV Charge state LDA (this work) LDA [7] G0 W0 (this work)

(+1) 0.89 1.36

(0.39) (0.326) (0.91)

(0)

(−1)

0.49 0.479

0.60 0.580 1.01

state in Table 1. After a full relaxation of the asymmetric distortion in the latter case, the discrepancy vanishes, however. The agreement with the results of Kim and Chelikowsky [5] for the same system is very good, except for a diﬀerence of 0.1 eV for the neutral charge state. The origin of these deviations cannot be traced, because both groups of authors give very little information about their computational details, and the size of the corresponding Kohn– Sham eigenvalue gap is not stated. For all conﬁgurations with symmetric geometries the defect level moves steadily upwards with increasing electron population. The asymmetric distortion has a large eﬀect on the unoccupied defect level and pushes it to signiﬁcantly higher energies. Concomitant with the opening of the fundamental band gap, the G0 W0 approximation adds a positive quasiparticle correction to all defect levels and predicts larger values than the LDA for all charge states. The size of the self-energy shift depends both on the charge state and the geometry, although the diﬀerences are of the same order as the error bar of the calculation. We note that our numerical values diﬀer slightly from those reported earlier in [15]. The discrepancy is due to an improved description of the anisotropic screening in the slab geometry in this work but lies within the estimated overall error bar of the calculation.

184

Arno Schindlmayr and Matthias Scheﬄer

For the P vacancy at InP(110) we obtain a similar picture, although the defect levels are at higher energies both in the LDA and the G0 W0 approximation. Unfortunately, due to experimental diﬃculties, no direct measurements of the defect states by photoemission are available. In this situation one can only try to extract values from indirect methods like surface photovoltage imaging with STM. One study using this technique claimed a value of 0.62 ± 0.04 eV for the As vacancy in the positive charge state, based on the known position of the sample’s Fermi energy 0.09 eV above the valence-band maximum and a local band bending of 0.53 eV [69]. An STM measurement on a diﬀerent sample found a band bending of only 0.1 eV, however [12]. The origin of this discrepancy is unclear but points to a strong inﬂuence of experimental conditions and/or sample quality. Because of this uncertainty, no experimental values are included in the tables.

5 Charge-Transition Levels The occurrence of diﬀerent charge states is a direct consequence of the position of the defect level inside the fundamental band gap: in p-doped materials the defect state lies above the Fermi energy and is hence depopulated, whereas it is fully occupied in n-doped materials with a higher Fermi energy close to the conduction-band edge. Indeed, a charge state of (+1) has been conﬁrmed experimentally for anion vacancies at p-GaAs(110) [70] and p-InP(110) [71] and a charge state of (−1) at n-GaAs(110) [72] and n-InP(110) [73]. In a theoretical treatment the stable charge state can be identiﬁed by comparing the diﬀerent formation energies E form (q, µA , εF ) = E vac (q, Qq ) + µA + qεF − E surf ,

(16)

where we use the same notation for the total energy of the vacancy as in the previous section. The chemical potential µA of the anion atoms is controlled by the partial pressure and temperature, εF denotes the Fermi level and E surf is the total energy of the defect-free surface. The qualitative behavior of the formation energies is illustrated in Fig. 5: due to their diﬀerent slopes the stable charge state with the lowest formation energy changes from positive to negative as the Fermi energy varies between the valence-band maximum and the conduction-band minimum. In between there may be a region where the neutral vacancy is stable. The charge-transition levels are deﬁned as the values of the Fermi energy where the curves intersect and the stable charge state changes. They are given explicitly by ε+/0 = E vac (0, Q0 ) − E vac (+, Q+ ) for the transition from q = +1 to q = 0 and ε0/− = E vac (−, Q− )−E vac (0, Q0 ) for the transition from q = 0 to q = −1. All quantities in (16) are ground-state energies and can, in principle, be calculated within density-functional theory. As explained above, however, the parametrizations most commonly used in practical implementations lack

formation energy

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces

0

VA +

VA

εVBM

0

185

−

VA

ε +/0 ε 0/− Fermi energy

εCBM0

Fig. 5. Qualitative behavior of the formation energies for anion vacancies in the − 0 positive (V+ A ), neutral (VA ), and negative (VA ) charge state. The Fermi energy is limited by the valence-band maximum and the conduction-band minimum. The charge-transition levels ε+/0 and ε0/− mark the values of the Fermi energy where the stable charge state with the lowest formation energy changes

essential properties of the exact exchange-correlation functional, so that the charge-transition levels obtained in this way suﬀer from systematic errors. For a more accurate quantitative description we use the same trick as in (15) and rewrite ε+/0 as ε+/0 = [E vac (0, Q0 ) − E vac (0, Q+ )] + [E vac (0, Q+ ) − E vac (+, Q+ )]

(17)

by adding and subtracting the total energy E vac (0, Q+ ) of a conﬁguration with the atomic geometry of the positively charged vacancy but with one extra electron. In this way the charge-transition level is naturally decomposed into two distinct contributions. The ﬁrst term on the right-hand side is purely structural and describes the relaxation energy of the neutral system from the atomic structure optimized for the positive charge state to its own equilibrium geometry. It is always negative and can be calculated within density-functional theory. We obtain −0.59 eV for GaAs(110) and −0.54 eV for InP(110) when taking the asymmetric distortion into account. The second term on the right-hand side is purely electronic and equals the electron aﬃnity of the positively charged vacancy, which in a many-body framework corresponds to the lowest unoccupied state, i.e., the empty 1a defect level in the band gap. This was already calculated within the G0 W0 approximation in the preceding section and can be taken from Tables 1 and 2. In the same spirit we rewrite ε0/− as ε0/− = [E vac (−, Q− ) − E vac (0, Q− )] + [E vac (0, Q− ) − E vac (0, Q0 )] . (18) The ﬁrst term now equals the ionization potential of the negatively charged vacancy, corresponding to the highest occupied quasiparticle state. Again this is the 1a defect level, which in this case is ﬁlled with two electrons, and the G0 W0 results can be taken from the tables in the previous section.

186

Arno Schindlmayr and Matthias Scheﬄer

The second term is the energy diﬀerence between the electrically neutral system in the atomic structure optimized for the positive charge state and its own relaxed geometry. This contribution is always positive and can be obtained from density-functional theory. We obtain 0.12 eV for GaAs(110) and 0.08 eV for InP(110). The structural component is much smaller than for ε+/0 because there is no symmetry-breaking distortion in this case, only a minor reduction of the Ga–Ga bond length across the vacancy. Incidentally, the charge-transition levels within the LDA, which are usually obtained according to the deﬁnitions ε+/0 = E vac (0, Q0 ) − E vac (+, Q+ ) and ε0/− = E vac (−, Q− ) − E vac (0, Q0 ) by evaluating the total-energy diﬀerences directly, can also be decomposed into structural and electronic energy contributions. The latter are not given by the Kohn–Sham eigenvalues in Tables 1 and 2, however. Instead, they must be calculated with the help of the transition-state theorem [18] from intermediate conﬁgurations with halfinteger occupation numbers of 1/2 and 3/2 electrons, respectively. Table 3. Calculated charge-transition levels for the As vacancy at GaAs(110) in eV relative to the valence-band maximum. For ε+/0 the ﬁrst column refers to the asymmetric and the second to the constrained symmetric relaxation ε+/0

Transition level LDA (this work) LDA [3] LDA [5] G0 W0 (this work)

0.24 0.32 0.49

(0.07) (0.10) (0.32)

ε0/− 0.15 0.4 0.24 0.60

In Table 3 we summarize the results for the As vacancy at GaAs(110). In contrast to earlier studies [3, 5] that found a small energy window in which the neutral charge state is stable, our own calculation at the level of the LDA predicts ε+/0 > ε0/− if the correct asymmetric distortion is taken into account and hence a direct transition from the positive to the negative charge state, but the small energy diﬀerence is within the uncertainty of the calculation. The G0 W0 approximation, on the other hand, reverses this ordering and simultaneously moves all charge-transition levels to higher energies. The values for the constrained symmetric relaxation are merely shown for the purpose of comparison with earlier work. The deviations from earlier LDA studies, especially by Zhang and Zunger [3], are related to diﬀerences of similar magnitude in the defect states, which were already mentioned above. The results for the P vacancy at InP(110) are given in Table 4. For this material an indirect experimental measurement of ε+/0 , obtained with a combination of scanning tunneling microscopy and photoelectron spectroscopy, is available [6]. Consistent with previous studies [6, 7], we ﬁnd that the LDA signiﬁcantly underestimates the experimentally deduced value. The larger

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces

187

Table 4. Calculated charge-transition levels for the P vacancy at InP(110) Transition level LDA (this work) LDA [6] LDA [7] G0 W0 (this work) Expt. [6]

ε+/0

ε0/−

0.47 (0.39) 0.52 (0.45) 0.388 0.82 (0.79) 0.75 ± 0.1

0.54 0.576 1.09

G0 W0 result, however, lies within the error bar of the experimental measurement. We take this as a conﬁrmation of our approach and an indicator that the other defect states and charge-transition levels calculated within the same framework are also meaningful. Nevertheless, further calculations for diﬀerent systems are necessary to establish the general validity of this scheme.

6 Summary We have presented a parameter-free method for calculating defect states and charge-transition levels of point defects in semiconductors. Compared to previous studies that extracted these quantities directly from the self-consistent iteration of the Kohn–Sham equations, it apparently corrects important errors that are inherent in all jellium-based exchange-correlation functionals and employs a separation of structural and electronic energy contributions. While the former are accurately obtainable in density-functional theory, we use many-body perturbation theory and the G0 W0 approximation for the self-energy to calculate the latter with proper quasiparticle corrections. The scheme is general and can be applied to arbitrary bulk or surface defects. As an example we examined the electronic structure of anion vacancies at the (110) surfaces of III–V semiconductors. For the As vacancy at GaAs(110) our calculation indicates that all three charge states including the neutral conﬁguration are stable, in contrast to the LDA that predicts a direct transition from the positive to the negative charge state. Due to a general lack of experimental data, a direct comparison between theoretical and experimental values is only possible for the charge-transition level ε+/0 of the P vacancy at InP(110). In this case our calculation is in good agreement with the experimentally deduced result and constitutes a clear improvement over previous LDA treatments. Nevertheless, besides an improvement of experimental techniques, further developments in theoretical and computational procedures are highly desirable. Our method only opens the door to novel approaches; with present implementations the results are derived at a cost that may be infeasible for more complex systems, and the numerical uncertainty of 0.1 eV to 0.2 eV is often of the same order as the relevant energy diﬀerences. The

188

Arno Schindlmayr and Matthias Scheﬄer

study of excitons, which, e.g., play an important role at GaAs(110) [74], further requires an extension of the mathematical framework beyond single quasiparticles. Acknowledgements We thank Magnus Hedstr¨ om, G¨ unther Schwarz, and J¨ org Neugebauer for fruitful collaborations in the course of this work and Philipp Ebert for useful discussions. This work was funded in part by the EU through the Nanophase Research Training Network (Contract No. HPRN-CT-2000-00167) and the Nanoquanta Network of Excellence (Contract No. NMP-4-CT-2004-500198).

References [1] P. Ebert: Curr. Opin. Solid State Mater. Sci. 5, 211 (2001) 165 [2] V. P. LaBella, H. Yang, D. W. Bullock, P. M. Thibado, P. Kratzer, M. Scheﬄer: Phys. Rev. Lett. 83, 2989 (1999) 165 [3] S. B. Zhang, A. Zunger: Phys. Rev. Lett. 77, 119 (1996) 166, 182, 183, 186 [4] H. Kim, J. R. Chelikowsky: Phys. Rev. Lett. 77, 1063 (1996) 166 [5] H. Kim, J. R. Chelikowsky: Surf. Sci. 409, 435 (1998) 166, 182, 183, 186 [6] P. Ebert, K. Urban, L. Aballe, C. H. Chen, K. Horn, G. Schwarz, J. Neugebauer, M. Scheﬄer: Phys. Rev. Lett. 84, 5816 (2000) 166, 167, 170, 179, 186, 187 [7] M. C. Qian, M. G¨ othelid, B. Johansson, S. Mirbt: Phys. Rev. B 66, 155326 (2002) 166, 182, 183, 186, 187 [8] M. C. Qian, M. G¨ othelid, B. Johansson, S. Mirbt: Phys. Rev. B 67, 035308 (2003) 166, 179 [9] P. Hohenberg, W. Kohn: Phys. Rev. 136, B864 (1964) 166, 168 [10] W. Kohn, L. J. Sham: Phys. Rev. 140, A1133 (1965) 166, 168, 169 [11] J. P. Perdew, K. Burke, M. Ernzerhof: Phys. Rev. Lett. 77, 3865 (1996) 166 [12] G. Lengel, R. Wilkins, G. Brown, M. Weimer: Phys. Rev. Lett. 72, 836 (1994) 166, 168, 184 [13] A. G¨ orling: Phys. Rev. A 54, 3912 (1996) 166, 171 [14] V. Fiorentini, M. Methfessel, M. Scheﬄer: Phys. Rev. B 47, 13353 (1993) 167 [15] M. Hedstr¨ om, A. Schindlmayr, M. Scheﬄer: phys. stat. sol. (b) 234, 346 (2002) 167, 181, 183 [16] L. Sorba, V. Hinkel, H. U. Middelmann, K. Horn: Phys. Rev. B 36, 8075 (1987) 168 [17] B. Reihl, T. Riesterer, M. Tschudy, P. Perfetti: Phys. Rev. B 38, 13456 (1988) 168 [18] J. C. Slater: Adv. Quant. Chem. 6, 1 (1972) 169, 173, 186 [19] J. F. Janak: Phys. Rev. B 18, 7165 (1978) 169, 173 [20] C.-O. Almbladh, U. von Barth: Phys. Rev. B 31, 3231 (1985) 170 [21] J. P. Perdew, M. Levy: Phys. Rev. Lett. 51, 1884 (1983) 170 [22] L. J. Sham, M. Schl¨ uter: Phys. Rev. Lett. 51, 1888 (1983) 170 [23] A. G¨ orling, M. Levy: Phys. Rev. A 50, 196 (1994) 170

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces

189

[24] A. G¨ orling: Phys. Rev. B 53, 7024 (1996) 170 [25] M. St¨ adele, J. A. Majewski, P. Vogl, A. G¨ orling: Phys. Rev. Lett. 79, 2089 (1997) 170, 171 [26] R. W. Godby, M. Schl¨ uter, L. J. Sham: Phys. Rev. B 37, 10159 (1988) 170 [27] T. Kotani: J. Phys.: Condens. Matter 10, 9241 (1998) 170 [28] J. P. Perdew, A. Zunger: Phys. Rev. B 23, 5048 (1981) 171 [29] D. M. Ceperley, B. J. Alder: Phys. Rev. Lett. 45, 566 (1980) 171 [30] L. Kleinman, D. M. Bylander: Phys. Rev. Lett. 48, 1425 (1982) 171 [31] M. Bockstedte, A. Kley, J. Neugebauer, M. Scheﬄer: Comput. Phys. Commun. 107, 187 (1997) 171 [32] M. Fuchs, M. Scheﬄer: Comput. Phys. Commun. 119, 67 (1999) 171 [33] J. L. A. Alves, J. Hebenstreit, M. Scheﬄer: Phys. Rev. B 44, 6188 (1991) 171, 176 [34] O. Madelung, U. R¨ ossler, M. Schulz (Eds.): Landolt-B¨ ornstein: Numerical Data and Functional Relationships in Science and Technology – New Series, vol. III/41A (Springer, Berlin, Heidelberg 2001) 171, 176 [35] G. D. Mahan: Many-Particle Physics, 3rd ed. (Springer, Berlin, Heidelberg 2000) 171 [36] L. Hedin: Phys. Rev. A 139, 796 (1965) 172, 174 [37] W. von der Linden, P. Horsch: Phys. Rev. B 37, 8351 (1988) 172 [38] G. E. Engel, B. Farid: Phys. Rev. B 47, 15931 (1993) 172 [39] M. S. Hybertsen, S. G. Louie: Phys. Rev. B 34, 5390 (1986) 173 [40] I. D. White, R. W. Godby, M. M. Rieger, R. J. Needs: Phys. Rev. Lett. 80, 4265 (1998) 173 [41] M. Rohlﬁng, N.-P. Wang, P. Kr¨ uger, J. Pollmann: Phys. Rev. Lett. 91, 256802 (2003) 173 [42] O. Pulci, F. Bechstedt, G. Onida, R. Del Sole, L. Reining: Phys. Rev. B 60, 16758 (1999) 173 alez, R. W. Godby: Phys. Rev. B 64, 235106 [43] A. Schindlmayr, P. Garc´ıa-Gonz´ (2001) 173 [44] B. Holm, U. von Barth: Phys. Rev. B 57, 2108 (1998) 174 [45] W.-D. Sch¨ one, A. G. Eguiluz: Phys. Rev. Lett. 81, 1662 (1998) 174 [46] W. Ku, A. G. Eguiluz: Phys. Rev. Lett. 89, 126401 (2002) 174 [47] T. Kotani, M. van Schilfgaarde: Solid State Commun. 121, 461 (2002) 174 [48] M. L. Tiago, S. Ismail-Beigi, S. G. Louie: Phys. Rev. B 69, 125212 (2004) 174 [49] K. Delaney, P. Garc´ıa-Gonz´ alez, A. Rubio, P. Rinke, R. W. Godby: Phys. Rev. Lett. 93, 249701 (2004) 174 [50] C. Friedrich, A. Schindlmayr, S. Bl¨ ugel, T. Kotani: Phys. Rev. B 74, 045104 (2006) 174 [51] E. L. Shirley, X. Zhu, S. G. Louie: Phys. Rev. B 56, 6648 (1997) 174 [52] R. W. Godby, M. Schl¨ uter, L. J. Sham: Phys. Rev. B 35, 4170 (1987) 174, 175 [53] X. Zhu, S. G. Louie: Phys. Rev. B 43, 14142 (1991) 174 [54] M. Rohlﬁng, P. Kr¨ uger, J. Pollmann: Phys. Rev. B 48, 17791 (1993) 174, 175 [55] X. Zhu, S. B. Zhang, S. G. Louie, M. L. Cohen: Phys. Rev. Lett. 63, 2112 (1989) 175, 178 [56] O. Pulci, G. Onida, R. Del Sole, L. Reining: Phys. Rev. Lett. 81, 5374 (1998) 175, 178 [57] S. J. Jenkins, G. P. Srivastava, J. C. Inkson: Surf. Sci. 254, 776 (1996) 175

190

Arno Schindlmayr and Matthias Scheﬄer

[58] M. M. Rieger, L. Steinbeck, I. D. White, H. N. Rojas, R. W. Godby: Comput. Phys. Commun. 117, 211 (1999) 175, 177 [59] L. Steinbeck, A. Rubio, L. Reining, M. Torrent, I. D. White, R. W. Godby: Comput. Phys. Commun. 125, 105 (2000) 175 [60] H. J. Monkhorst, J. D. Pack: Phys. Rev. B 13, 5188 (1976) 177 [61] A. Schindlmayr: Phys. Rev. B 62, 12573 (2000) 177 [62] J. Neugebauer, M. Scheﬄer: Phys. Rev. B 46, 16067 (1992) 178 [63] P. Eggert, C. Freysoldt, P. Rinke, A. Schindlmayr, M. Scheﬄer: Verhandl. DPG (VI) 40, 2/491 (2005) 179 [64] N. D. Lang, A. R. Williams: Phys. Rev. B 18, 616 (1978) 179 [65] P. J. Braspenning, R. Zeller, A. Lodder, P. H. Dederichs: Phys. Rev. B 29, 703 (1984) 179 [66] M. Scheﬄer, C. Droste, A. Fleszar, F. M´ aca, G. Wachutka, G. Barzel: Physica B 172, 143 (1991) 179 [67] J. Bormet, J. Neugebauer, M. Scheﬄer: Phys. Rev. B 49, 17242 (1994) 179 [68] G. Fratesi, G. P. Brivio, L. G. Molinari: Phys. Rev. B 69, 245113 (2004) 179 [69] S. Aloni, I. Nevo, G. Haase: Phys. Rev. B 60, R2165 (1999) 184 [70] K. J. Chao, A. R. Smith, C. K. Shih: Phys. Rev. B 53, 6935 (1996) 184 [71] P. Ebert, X. Chen, M. Heinrich, M. Simon, K. Urban, M. G. Lagally: Phys. Rev. Lett. 76, 2089 (1996) 184 [72] C. Domke, P. Ebert, K. Urban: Phys. Rev. B 57, 4482 (1998) 184 [73] P. Ebert, K. Urban, M. G. Lagally: Phys. Rev. Lett. 72, 840 (1994) 184 [74] O. Pankratov, M. Scheﬄer: Phys. Rev. Lett. 75, 701 (1995) 188

Index alignment, 176, 177 anion vacancy, 166, 179–182, 184–187 antisite, 168 asymmetric, 166, 179, 180, 182, 183, 185, 186 band bending, 166 band edge, 173, 178, 184 band structure, 166, 167, 169, 170, 172–177 Brillouin zone, 176–178, 181, 182 bulk, 165, 171, 173, 174, 176–178, 187 charge state, 167, 170, 179, 180, 182–187 charge-transition level, 165–167, 170, 171, 184–187 charge-transition state, 169, 172, 173, 184, 186, 187 chemical potential, 184 cleavage, 168, 176

conduction band, 176, 178, 184 coordination, 179 core-valence interaction, 167, 174, 182 correlation, 167, 169–172, 177, 180 dangling bond, 176, 177, 179 decay, 172 defect state, 180 density of states, 166 density-functional theory, 165–168, 170–172, 178, 179, 182, 184–187 dielectric function, 173 dipole, 178 dispersion, 176, 177, 180, 181 distortion, 166, 179, 182, 183, 185, 186 doping, 168, 180 eigenstates, 171, 172 eigenvalues, 165, 166, 168, 169, 172–174, 177, 179, 186 electron aﬃnity, 170, 172, 182, 185

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces exact exchange, 185 exchange-correlation, 166–170, 172, 185, 187 excitation, 165, 167–169, 171–173 exciton, 188 Fermi level, 165, 167–169, 178, 184 formation energy, 184 functional derivative, 169, 174 fundamental gap, 170, 174, 178 G0 W0 approximation, 165, 168, 172–180, 182–187 GaAs(110) surface, 176 GaN, 167 gap states, 168 general gradient approximation (GGA), 166, 167, 170 Green’s function, 165, 171–174, 179, 181 ground state, 165, 168, 170, 171, 177, 184 Hamiltonian, 171 Hartree, 168, 169, 179 Hedin, 174 Heisenberg picture, 171 hole, 166, 172, 173, 180 hopping integral, 180, 182 InP(110) surface, 176 ionization potential, 170, 172, 185 Lagrange parameter, 169 LDA, 166–171, 173, 176, 177, 181–184, 186, 187 many-body perturbation theory, 171 multipole, 178

191

phonon, 172 photoemission, 166, 170, 184 plane wave, 171, 173–175, 179 plasmon, 172, 175, 178 point defect, 165–168, 170 polarizability, 173, 175, 178 polarization, 173, 178, 179 pseudopotential, 167, 171, 174, 182 quasiparticle, 165, 167, 169–176, 179, 181–183, 185, 187, 188 quasiparticle equation, 172 random-phase approximation, 170, 173, 175, 178 real space, 175, 177 reciprocal space, 175 relaxation, 166, 167, 171, 176, 179, 180, 182, 183, 185, 186 scanning tunneling microscopy (STM), 165, 166, 168, 184, 186 scattering, 172 screening, 173, 183 self-energy, 165, 167, 168, 172–183, 187 Slater transition state, 169 spin, 169, 182 supercell, 177–180, 182 surface, 165–169, 171, 173, 176–182, 184, 187 surface band, 176 symmetry, 166, 176, 179, 180, 182, 183, 186 termination, 177 tight binding, 175, 180, 181 total energy, 168–170, 179, 182, 184, 185

nonlocal, 167, 172, 174, 179, 180 periodic, 175, 177, 178, 180 perturbation, 165, 167–169, 171–173, 179, 187

valence band, 169, 170, 176–178, 180, 182, 184 zincblende lattice, 176

Multiscale Modeling of Defects in Semiconductors: A Novel Molecular-Dynamics Scheme G´ abor Cs´anyi1 , Gianpietro Moras2, James R. Kermode1 , Michael C. Payne1, Alison Mainwood2 , and Alessandro De Vita2,3 1

2

3

Cavendish Laboratory, University of Cambridge, Madingley Road, CB3 0HE, United Kingdom {gc121,jrk33,mcp1}@cam.ac.uk Department of Physics, King’s College London, Strand, London, United Kingdom {gianpietro.moras,alison.mainwood,alessandro.de vita}@kcl.ac.uk DEMOCRITOS National Simulation Center and CENMAT-UTS, Trieste, Italy

Abstract. Now that the modeling of simple semiconductor systems has become reliable, accurate and routine, attention is focusing on larger scale, more complex simulations. Many of these necessarily involve multiscale aspects and can only be tackled by addressing the diﬀerent length scales simultaneously. We discuss some of the types of problems that require multiscale approaches. Finally we describe the LOTF (learn-on-the-ﬂy) hybrid scheme with a series of examples to show its versatility and power.

1 Introduction Over the last twenty years, the improvement in computational modeling of materials problems has been remarkable. This is due to the signiﬁcant increase in the capacity and speed of computers matched (and arguably surpassed) by the ingenuity of those who write the computational codes. It would be invidious to do other than refer the reader to other Chapters in this volume to support these assertions. However, these advances are also challenged by the complexities of systems that need to be modeled. There has been a great deal written about diﬀerent scales of modeling, usually where the results of calculations on one scale are used to determine the parameters that are used to model the material at a larger scale. Many of the embedding approaches are designed in this way. Additionally, where dynamic processes are being modeled, it may be useful to treat diﬀerent timescales by diﬀerent means. A combination of molecular-dynamics and quantum-mechanical modeling using a ﬁrst-principles technique for example, can model only a few hundred atoms for a period of a few picoseconds. Using more approximate methods, one may be able to extend the number of atoms to hundreds or thousands, or the time period by a few orders of magnitude. In order to extend the time period to the several seconds for some biological processes, D. A. Drabold, S. K. Estreicher (Eds.): Theory of Defects in Semiconductors, Topics Appl. Physics 104, 193–212 (2007) © Springer-Verlag Berlin Heidelberg 2007

194

G´ abor Cs´ anyi et al.

or years or aeons for geological ones, the activation energies and reaction pathways from the static or picosecond MD calculations have to be inserted into Monte Carlo models or analytical rate equations and their variants. In this Chapter, we suggest a selection of problems where the complexity of such an approach makes it diﬃcult or impossible to treat every length scale with a separate calculation, largely because the physical processes on the various length scales are strongly coupled to each other. We then go on to describe a method that allows some of these complex problems to be tackled.

2 A Hybrid View Radiation or Implantation Damage An important technique for doping semiconductors is to implant the dopant with an energy (or range of energies) that determines the location of the doped area or layer. However, in this process damage in the form of vacancies and interstitials and their complexes are formed, some of which can be electrically active. Annealing may heal most of the damage (e.g., [1]), but invariably some defects remain and can be detected by photoluminescence and positron-annihilation spectroscopy [2]. Intrinsic defects have very low activation energies for diﬀusion, so they may migrate long distances before they are trapped by dopants, or other radiation-induced defects. The same problems arise when the radiation damage of silicon particle detectors is modeled. A very comprehensive empirical analysis of the processes involved in the annealing of damage was undertaken by Huhtinen [3], but he did not attempt to understand the microscopic processes. However, his analysis showed that some long-range migration of radiation damage products and displaced impurities was occurring. It is well within the current state-of-the-art to model the dynamics of the initial impact of a particle or ion with a silicon atom in a small ﬁnite cluster (or periodic supercell), and the subsequent displacement of that atom. If the damage trail formed by the particle, the knock-on atom and any further damage products can all be contained in the ﬁnite cluster or supercell, then a reasonable model of the full process can be built up. More commonly, though, one or more of the damage products may exit the cluster in a direction not easily predicted from the initial conditions, or the intrinsic defects may migrate longer distances than the dimensions of the largest clusters. The problem is then to construct a method to follow the important species such that their interactions are treated with the required level of accuracy, while keeping the whole problem to within acceptable computational limits. Point-Defect Diﬀusion A very similar problem is the annealing of point defects in semiconductors, where an additional complication is the chemical interaction between the im-

Multiscale Modeling of Defects in Semiconductors

195

purity and the defects in the host lattice. As an example, atomic hydrogen in silicon has a stable site in a bond-centered position, which is only stable when the bond is greatly elongated – a self-trapped site [4]. It also has a metastable site at the tetrahedral site, where the migration barrier is very low. To model the migration, a full molecular-dynamics model must be used, but it must also be capable of following the long-range migration of the hydrogen through the tetrahedral-site routes. For hydrogen, a proper model using quantum mechanics for the proton as well as for the electrons is necessary, and has been developed in a limited way [5], but the principles illustrated by this example apply to the diﬀusion of many other impurities and defects. Classical interatomic potentials are available for some of the simpler chemical systems, but they tend to be constructed for bonding situations that are close to equilibrium, and have rather more questionable validity where the local environment of the host–defect complex is greatly distorted. Both the relative stability and the rate of migration of point defects can be altered by the presence of strain ﬁelds and strain gradients that are ubiquitous in semiconductor systems. While the point defects typically alter the local atomic structure only on a scale of a nanometer, the strain ﬁelds of epitaxial layers extend much further due to lattice mismatch. Dislocations also give rise to a slow-decaying strain ﬁeld. This means that while the quantum-mechanical treatment of new bonding arrangements near each individual defect can be accomplished using a few hundred atoms, the environment in which the diﬀusion and possible interaction of the defects takes place needs to be represented by tens of thousands of atoms or more. Dislocation Motion The strength of real materials is dominated by the behavior of its dislocations. Around the core of a dislocation, there is a 1-D region in which the bonding of the host is distorted. Once there is a kink in the dislocation, by which means it moves, the distortions become much more pronounced, and this part of the crystal must be modeled by particularly accurate techniques, see Fig. 1 for a schematic view. Moreover, the movement of the kink means that this highly distorted region also moves, which typically involves bond breaking and forming. More complexity arises when dislocations interact with each other or with grain boundaries, and they may also be sources (or sinks) for point defects. Grain Boundaries Nanocrystalline silicon and other semiconductors are becoming more and more technologically important. Similarly, the crystal quality of many of the newer wide-bandgap semiconductors used in electronics (the nitrides, silicon carbide, diamond) is not nearly as perfect as silicon – it is no longer acceptable to ignore dislocations and grain boundaries when trying to understand the

196

G´ abor Cs´ anyi et al.

Fig. 1. Schematic view of a screw dislocation with a double kink. In covalent materials, dislocations move by the formation of double kinks. Gray circles approximately indicate the region in which active rebonding takes place

degradation or limitations of their electronic properties. The exact role that grain boundaries play in plasticity is far from being completely understood. In particular, the grain boundaries need to be investigated as sources and sinks for dislocations. Signiﬁcant departure from the equilibrium crystalline structure is present. This takes the form of a mixture of locally disordered bonding and longer-range elastic distortion – a situation that needs a multiscale description. Furthermore, the grain boundaries can act as traps for dopants, electrons and holes, adding to the local chemical complexity. Once again, although the longer-range interactions are well described by empirical potentials, the description of the local chemistry requires quantum-mechanical accuracy. Fracture Fracture is perhaps the textbook example of a multiscale problem. The importance of understanding both the catastrophic failure of brittle materials and the conditions under which normally ductile materials become brittle cannot be overemphasized. Classical continuum models of the stress ﬁeld do an excellent job in predicting the enhancement of stress near the crack tip. However, the divergence of components of the stress tensor at the tip imply that elasticity theory must break down in this region since it is not applicable when distortions go beyond the harmonic range. Indeed, during failure the interatomic bonds are stretched well into the anharmonic region and ultimately are broken. In covalent systems this leaves dangling bonds, whose energetics can only be described by a fully quantum-mechanical treatment. Moreover,

Multiscale Modeling of Defects in Semiconductors

197

Fig. 2. Displacement ﬁeld of a propagating crack under uniaxial tension in the opening mode (analytical continuum solution)

the inﬂuence of impurities and corrosive agents on failure processes has never been explored theoretically at this level of detail, yet there is evidence for the critical role they play, e.g., in fracture of silicon notches in a wet environment [6, 7] and in the controlled fabrication of thin Si ﬁlms by hydrogen implantation [8–10]. The key aspect of brittle fracture that makes it amenable to hybrid modeling is that the propagating crack is atomically sharp [11]. Thus, although the crack surface that is opening up is two-dimensional, the active region, where bonds are being broken, is a one-dimensional line, perpendicular to the direction of propagation. The strongly coupled multiscale aspect of crack propagation comes about because the opening crack gives rise to a stress ﬁeld √ that has a singularity (in the continuum approximation), diverging as 1/ r where r is the distance ahead of the crack tip, and in turn, it is this large stress that breaks the bonds and thus advances the crack forward. The extension of the stress ﬁeld is nevertheless very large. If we wish to represent all the atoms that contribute signiﬁcantly to elastic relaxation as the stress ﬁeld advances, we need to include several tens of thousands of atoms. Only then can we hope to be able to quantitatively predict critical loading levels.

3 Hybrid Simulation The general pretext in a hybrid simulation is that we are going to use two diﬀerent physical models to describe the system. It is understood that one of these is accurate enough to describe the physics of the activated regions properly, which, in practice, means we will use some sort of quantum-mechanical

198

G´ abor Cs´ anyi et al.

description, e.g., a tight-binding (TB) formalism, or indeed density-functional theory (DFT); henceforth this ﬁrst model will be referred to as the QM model. Using such sophisticated modeling comes at a price, in the very real terms of computing costs. With the currently available hardware, it is typically possible to simulate thousands of atoms using TB, and hundreds of atoms using DFT for tens of picoseconds. These are evidently modest capabilities if we are faced with any of the above problems, and hence we need to employ a second model, to be used in parts of the system that are not activated at a given instant in time. This second model should capture correctly the basic topology of bonding and the response to small deformations, while at the same time be relatively inexpensive to compute. Empirical atomistic models ﬁt the bill perfectly. It should be noted that the recent progress in the ﬁeld of empirical “ball and spring”-type modeling has been in the direction of reﬁning the analytical forms in an attempt to extend their range of applicability [12–15]. However, once we have decided to employ a hybrid technology there is little beneﬁt in complicating this second, classical model . It is more important that it is as robust as possible and uses only a small number of free parameters since in any particular situation where the classical model would fail we will use the QM model. In theory, one could consider not just two models, but a whole hierarchy of ever more coarse-grained descriptions of physical systems. The next one up from classical atomistic models would be a continuum ﬁnite element model. In our experience, the cost ratio between the QM and the classical models is so extreme, that for all intents and purposes the classical atoms can be regarded as “free” in most applications. If we are at liberty to consider millions of classical atoms, the necessity of a continuum description is less pressing. The standard technical tools of classical molecular-dynamics can thus be used on this large, atomistically modeled region to impose the correct elastic or thermal boundary conditions of the problem under study. The boundary regions between the QM and classical zones need, on the contrary, a special treatment and a separate discussion. Boundary Problems It is not hard to recognize that the biggest challenge in designing a hybrid simulation scheme is to overcome the problems associated with the artiﬁcial boundary that separates regions of the system that are described by the two diﬀerent models. In fact there are two distinct issues that have to be addressed. The ﬁrst one generally goes under the name of termination, and it concerns the accurate computation of forces on atoms near the boundary. If we attempt the most naive partitioning and simply omit the classical atoms from the quantum-mechanical calculation and vice versa, the atoms close to the boundary will behave like those near an open surface. This is clearly wrong. To get accurate forces on these atoms, we should “trick” the system into believing that these surface atoms are really bulk atoms, while avoiding

Multiscale Modeling of Defects in Semiconductors

199

implicit inclusion of all the atoms from the other region (which is the point of the hybrid simulation in the ﬁrst place). The next simplest solution is to use so-called “termination atoms”, which is standard practice in the hybrid simulation schemes of biological systems (called “QM/MM” models [16]). Here, atoms from the region we are presently not considering are also taken away, but wherever covalent bonds are broken by this removal, a monovalent atom (typically a hydrogen) is placed to saturate the dangling bond. For the classical model, this procedure can be seen to be suﬃcient. The classical description of covalent bonding is very near-sighted, i.e., the energy of the “last” classical atom can be essentially perfectly recovered using the terminator-atom technique. Moreover, since the classical total energy is usually expressed as a simple sum of atomic energies, the terminator atom can simply be excluded from this sum. It has to be noted that if we are dealing with a strongly ionic material, even our classical model will not be so near-sighted, and the problems that are usually associated with the termination of the quantum region in standard QM/MM treatments apply to the classical part as well. Terminating the quantum-mechanical subsystem is more tricky. Quantum mechanics is not a nearest-neighbor model, so even if our free surface is terminated by monovalent terminator atoms, the atoms close to the boundary will feel an artiﬁcial environment. Secondly, it is more or less impossible in any QM scheme to exclude the terminator atoms from the total energy in a consistent fashion, so we have just traded artiﬁcial surface atoms for artiﬁcial terminator atoms – not an altogether satisfactory situation. These two problems are solved by the same trick: we stop worrying about the total energy and concentrate on obtaining accurate forces on the atoms in the QM region, which is achieved by allowing a thicker termination region, rather than just terminator atoms. In other words, we include a shell of nominally classical atoms (a thickness of about a nanometer is suﬃcient in silicon) in the QM calculation, which ensures that the forces that we compute for the QM atoms are accurate. Now in contrast to the total energy, the forces are local quantities, so it is trivial to exclude the forces on atoms in the “contaminated” termination region from the subsequent calculations: from the QM calculation, we only keep the forces on atoms in the original QM region, not the termination region. Mechanical Matching And thus we squarely arrive at the second major issue associated with the boundary. Suppose we have computed forces with the desired method in each region, we now have to propagate the system forward in time along its trajectory. On the two sides of the boundary, we originally resolved to compute with diﬀerent models, but these yield diﬀerent, and incompatible trajectories for the atoms on the two sides. The set of forces we just computed (from two diﬀerent models) are not the derivatives of some total energy and do

200

G´ abor Cs´ anyi et al.

not necessarily add up to zero for an isolated system. If we simply plugged them into an integrator formula (e.g., velocity, Verlet [17]), the trajectory may be unstable. The solution to this problem forms the basis of our recently developed method [18–20] called “learn on the ﬂy” (LOTF): instead of using the set of forces directly, we consider a simplistic universal “ball and spring” model, but allow every spring to be diﬀerent, and also to change with time. At every time step, the set of forces we computed using the classical and quantum models are used as targets in an optimization of the spring constants, which are tuned until the forces derived from the universal model match their targets. The trajectory integrator is then used on the universal model, whose forces are now consistent across the whole system. The universal model in eﬀect “interpolates” across the boundary, closely matching the target on both sides, while maintaining global consistency. In practice, a number of simpliﬁcations immediately arise. The target forces do not have to be computed at every time step, as the universal model can be considered an instantaneous interpolator not just in space, but also in time and so it can be used with unchanged spring constants for a few time steps without incurring a signiﬁcant deviation from the true hybrid trajectory. More importantly however, the scheme is greatly simpliﬁed if the universal model is chosen to be the classical model itself! Thus an alternative and complementary point of view is that we take the classical model and remove the constraints from its parameters, allowing them to be diﬀerent for each atom. We then tune them in the QM region to incorporate the quantum-mechanically accurate force information. Another important consequence of this scheme is that we are at liberty to move the QM region in space without upsetting the stability of the simulation. The universal model will adapt to the target forces at each optimization, regardless of where and how we obtained the set of target forces. The use of a thick transition region to pad the quantum-mechanical calculation means that as we shift the quantum region in space together with its padding the Hamiltonian in the nominal quantum region changes smoothly.

4 The LOTF Scheme The Universal Potential We now describe in detail the LOTF scheme that is based on the above ideas. The choice of the universal force model that we will use to interpolate the quantum and classical models is crucial. There are two obvious choices. One, already alluded to above, is to use the classical model itself. This means that there would only be two force models in our scheme, a classical model with variable parameters and a quantum model. Most of the applications in the following sections have been carried out using this approach. An alternative and more ﬂexible choice is to pick a universal force model that oﬀers a good

Multiscale Modeling of Defects in Semiconductors

201

Fig. 3. Examples of cubic spline potentials for the two-body (top) and three-body terms (bottom). The large dots represent spline knots, the red dotted lines are the corresponding functions of the Stillinger–Weber potential [22]

compromise between expressive power and robustness. In particular, we will be changing the model parameters on the ﬂy, so we would like the potential form to change smoothly as we change these parameters. In our search for the parameter set optimized at any given point in the simulation, we will make use of gradient search techniques, so the derivative of the potential with respect to its parameters should be straightforward and easy to evaluate. Keeping the bond lengths and bond angles as fundamental coordinates, a cubic spline functional form ﬁts the above criteria [21]. For the two-body term, we can take a spline with four knots (e.g., at r = {1.5, 2.0, 2.5, 3.5} ˚ A for Si, for other elements scaled appropriately by the atomic radius). The spline function is completely determined by its values at the knot points and its derivatives at the two endpoints. We ﬁx both the value and the derivative at the outer endpoint to be zero, and at the inner endpoint to match the corresponding values of the quantum model for a dimer. This leaves two free parameters, the value of the spline at the two inner knots. Keeping these two values negative guarantees the existence of a single minimum in the spline function between the endpoints. For the three-body term, we could keep the traditional quadratic form in the cosine of the bond angle θ, but with a variable curvature and position of the minimum. To allow more ﬂexibility, and in particular, an asymmetric angular dependence, we can again take a cubic spline of cos θ, with two knots at −1 and 1, the free parameters are then the values and derivatives at the endpoints. As long as we restrict the derivatives to have the appropriate sign,

202

G´ abor Cs´ anyi et al.

we can guarantee that the spline will have a single minimum in (−1, 1) for any set of values of the parameters. Figure 3 shows a pictorial illustration of the splines. Since the spline functions are linear functions of the values at the knot points, our free parameters, evaluating the splines and their derivatives at ﬁxed atomic positions for different parameter values is trivial and fast. Parameters Since we want to optimize potential parameters associated with atoms close to the quantum region, the choice of initial values is important. Unless the elastic constants of our classical and quantum models match closely, acoustic waves will partially reﬂect from the artiﬁcial quantum/classical boundary. Therefore, the starting values of classical parameters have to be set to match the elastic constants of our quantum model. During the dynamics, as the quantum region moves, we have two choices for atoms that are no longer in the quantum region: either we reset the classical parameters to their initial values, or we leave them with the last-ﬁtted parameters. Which is best depends on the application. In the case of defect diﬀusion, once the defect leaves a particular area, it makes sense to reset the parameters. In other cases, if the physical eﬀects in the quantum region have resulted in some permanent topological change, e.g., the opening of a new surface, possibly followed by surface reconstruction, we might want to keep the last-ﬁtted parameters, as they could give a better description of the new topology than the original parameters. It seems diﬃcult to formulate an optimal strategy for the general case. Algorithm The following sequence of steps constitutes the hybrid scheme, a graphical illustration is shown in Fig. 4. 1. Initialize universal force-model parameters. 2. Extrapolate the atomic trajectory for n steps using ﬁxed model parameters. 3. Identify atoms that need quantum treatment. This is done using geometric and topological criteria, e.g., atoms are selected if they are under- or overcoordinated. For each new application, a suitable selection criterion has to be designed that captures the relevant processes. The user-deﬁned goal of the calculation may determine the exact recipe used here. Indeed in calculations involving surface-chemical reactions in a slab geometry, we may choose to treat quantum-mechanically only one surface of the slab, thus eﬀectively halving the accurately rendered area but doubling the simulation time for a given computer budget.

Multiscale Modeling of Defects in Semiconductors

203

Fig. 4. Predictor–corrector-style parameter ﬁtting. The black and red lines represent the predictor and corrector part of the trajectory, respectively. The gray circles denote the assumed domain of validity of the newly ﬁtted parameters at each ﬁt point (black dots)

4. Quantum-mechanical calculations are carried out to obtain accurate forces on the selected quantum atoms. 5. Optimize the force-model parameters to match the target forces both in the quantum and classical regions. 6. Interpolate the trajectory over the previous n steps between the old and new parameters. This achieves a smooth evolution of parameters in time. 7. Back to 2.

5 Applications Point Defects We now present a series of applications of the LOTF scheme in silicon. In all cases, the classical model is that of Stillinger–Weber [22] and, unless stated otherwise, the quantum model is empirical tight-binding with various parametrizations [23,24]. The ﬁrst application is more of a quantitative test of the algorithm, rather than a real application that necessitates a hybrid methodology. We consider the diﬀusion of point defects in crystalline Si, and show that the LOTF scheme, using a spherical QM region around the moving defect, recovers the same diﬀusion coeﬃcient as that calculated from a fully quantum-mechanical trajectory, while both are signiﬁcantly diﬀerent from the case of a purely classical trajectory. Figure 5 shows the diﬀusivity as a function of temperature for a vacancy in silicon calculated in three diﬀerent ways. The LOTF simulations have been performed with two diﬀerent QM

204

G´ abor Cs´ anyi et al.

Fig. 5. Vacancy diﬀusion rate in Si as a function of inverse temperature, as computed using fully quantum (black ), classical (blue) and hybrid (red ) models. The unit cell had 63 atoms

packages (diﬀerent orthogonal tight-binding parametrizations), which – not surprisingly – give diﬀerent values. Critically however, the LOTF simulation reproduces the correct curve, corresponding to whichever QM package was used to get the target forces. Further details can be found in [19] and [20]. Figure 6 shows the mean square displacement of a hydrogen atom, diﬀusing in crystalline silicon at 1000 K. This test shows up an interesting aspect of the LOTF simulation. Because the algorithm retunes the classical model continuously, it eﬀectively uses a time-dependent Hamiltonian, and thus we can no longer deﬁne a total energy that is a constant of motion. A slow (local) heating or cooling of the systems may occur during microcanonic simulations, or in constant-temperature simulations using an inappropriately tuned thermostat, in spite of the forces being all the time accurate within a few per cent. The problem is, however, lifted in the canonic ensemble if a suitable thermostat is used to stabilize the dynamics. In the present case, with two diﬀerent atomic species and a large mass ratio (∼ 28), a simple velocityrescaling thermostat is unable to maintain the correct kinetic temperature for both the hydrogen and the silicon atoms. This problem can be corrected with the use of a more sophisticated thermostat. Figure 7 shows the temperature evolution of the same system, where instead of a real QM engine, LOTF was used to track the classical forces, but the force on the H atoms was scaled by 0.9. The same behavior is observed as shown in Fig. 6: without a thermostat, the system is unstable. With a simple velocity-rescaling thermostat, the kinetic temperature of the hydrogen is diﬀerent from the system (in this case, much larger), while using a Langevin thermostat [25] eliminates this discrepancy. The Langevin thermostat adds a dissipative and a ﬂuctuat-

Multiscale Modeling of Defects in Semiconductors

205

Fig. 6. Mean square displacement of a H atom diﬀusing in Si. Quantum and classical runs are represented by black, blue lines, respectively. The green curve corresponds to the hybrid simulation with a Nos´e–Hoover thermostat, which is unable to maintain, by itself, the correct kinetic temperature of the H atom. Once this is corrected for results match the diﬀusion rate of the fully quantum-mechanical simulation (red line)

ing term to the forces and these are precisely balanced to achieve the desired temperature. In contrast to other schemes, the Langevin thermostat does not rely on eﬃcient coupling of phonons of the hydrogen and the bulk, but couples to each particle directly and separately. Dislocation Glide To demonstrate a simple application of the hybrid scheme in a system that deﬁnitely needs quantum-mechanical accuracy yet is already too large for an ordinary simulation, we consider the glide of partial dislocations. Silicon partial dislocations move by forming kinks that zip along the dislocation line. The most prevalent partial dislocation in silicon is the 30◦ partial, and the kink that most easily forms and migrates on it is the left kink [26]. Figure 8 shows a pair of such partials, oppositely directed, so that the whole unit cell is periodic, and the partials enclose a stacking fault. The unit cell is also skewed slightly, thus forcing the existence of a left kink on each partial. In a molecular-dynamics simulation at high temperature (900 K to 1100 K), the partials move toward each other, and eventually annihilate, leaving behind a number of scattered point defects (mostly fourfold-coordinated

206

G´ abor Cs´ anyi et al.

Fig. 7. Temperature evolution of a hydrogen atom in a 64-atom silicon cell using diﬀerent thermostats with the hybrid scheme. The top panel shows that in such a small system, there is a signiﬁcant energy drift due to the time-dependent Hamiltonian. The middle panel shows that a simple velocity-rescaling thermostat that, like the Nos´e–Hoover, couples to the entire system via one extra degree of freedom to the entire system, is unable to maintain the correct kinetic temperature for the light H atom. The bottom panel shows that a more sophisticated Langevin thermostat, which couples to each atom individually, maintains the correct temperature for all species of atoms

defects [27]). There are a number of salient features of the LOTF simulation that are worth pointing out and that are not observed in a purely classical simulation. First, the glide is an order of magnitude faster in the hybrid simulation. This does not just indicate a lower energy barrier for kink migration, but the conﬁgurations that are most prevalent in the hybrid simulation are very diﬀerent from those in the classical case. The most striking example is the equilibrium state of the left kink itself, shown in Fig. 9. Although the equilibrium conﬁgurations in the quantum and classical models agree at zero temperature, at high temperature, the quantum-mechanical free-energy minimum corresponds to a kink conﬁguration with a square and an ejected antiphase defect. During the classical simulation, the kink spent a large proportion of the time trapped in a metastable state that had the eﬀect of pinning the partial. A unique advantage of a modular hybrid scheme with a black-box quantum engine is that it is easy to investigate the eﬀect of chemical defects. Swapping the empirical tight-binding quantum engine for density-functional tight-binding (DFTB)[28] enables us to simulate the interaction of the partial with dopants without having to worry about constructing a classical model for a new type of atom. If we start the simulation after placing a boron atom

Multiscale Modeling of Defects in Semiconductors

207

Fig. 8. A pair of oppositely directed 30◦ partial dislocations enclosing a stacking fault. The complete unit cell consists of 4536 atoms, but only the (111) plane containing the stacking fault is shown. The red (Si) and green (B impurity) atoms are undercoordinated, so they and the surrounding blue (Si) atoms are treated quantum-mechanically

Fig. 9. Detail of the dislocation kink, showing the conﬁguration that corresponds to equilibrium at zero temperature (dotted lines), and to what is prevalent at 900 K in the hybrid simulation

at the position shown in green in Fig. 8, the right-hand partial is pinned and remains completely stationary, while the left-hand partial advances as before.

208

G´ abor Cs´ anyi et al.

Fig. 10. Von-Mises strain ﬁeld around a stationary crack tip in the opening mode in silicon

Brittle Fracture In recent years, the problem of brittle fracture of covalent materials has been a prototypical problem addressed using hybrid methodology [29–31]. Figure 10 depicts the von-Mises strain around a stationary crack tip, as calculated using the Stillinger–Weber potential by optimizing the positions of the interior atoms, while holding the top and bottom rows of atoms ﬁxed, corresponding to a given load in the opening mode. The stress concentrates near the tip and when the load reaches a critical level, the most strained bond gives way and the crack propagates forward. While analytical values for the required loading for crack propagation are easy to compute in the continuum approximation, it is well known that the discreteness of the atomic lattice gives rise to a barrier to this process, called lattice trapping [32–34]. The height of this barrier depends sensitively on the atomistic model employed and classical models typically overestimate this barrier, resulting in a much higher critical loading. The barrier associated with the Stillinger–Weber potential in particular is so high that, when the crack ﬁnally does propagate, so much elastic energy is released that the opening surfaces roughen, the crack tip blunts, emits dislocations, resulting in a reduction of the local stress ﬁeld and an arrest to crack propagation: in other words, the ductile behavior is incorrectly predicted. An example of such “ductile” crack propagation is shown in Fig. 11. In contrast, real cracks in silicon at low temperature are atomically ﬂat and propagate continuously above the critical load. This is reproduced by the hybrid simulation, a snapshot of which is shown in Fig. 12. This simulation at 300 K shows the 5–7–5 Pandey reconstruction of the opening (111) surfaces. The motion of the crack tip is tracked with the quantum region by noting which atoms have changed their number of nearest neighbors since the start of the simulation, and treating all atoms quantum-mechanically within 5˚ A of these.

Multiscale Modeling of Defects in Semiconductors

209

Fig. 11. Snapshot of “ductile” crack propagation using the Stillinger–Weber model. Defects are produced in the crack-opening region and dissipate energy; the onset of cracking is not sharp

Fig. 12. Snapshot from brittle crack propagation, using the hybrid method at 300 K. Red atoms have been ﬂagged as “active” because they have changed their neighbor count since the start of the simulation, and together with the blue atoms, are treated quantum-mechanically. In contrast to the ductile case, the crack propagates continuously above critical loading

210

G´ abor Cs´ anyi et al.

6 Summary To conclude this overview, we reiterate that a large class of problems in the area of semiconductor mechanical properties are inherently multiscale, and that signiﬁcant advances in computer simulation will only be made by addressing the diﬀerent length scales directly and simultaneously. We have introduced a promising new scheme that scales well to large system sizes and that deals with the intricacies of a hybrid simulation with fully controllable approximations. The scheme is very general, and can be extended to deal with arbitrary classical force-ﬁeld potentials, one foreseen extension being, in particular, in the direction of modeling long-range (classical electrostatic) interactions.

References [1] [2] [3] [4] [5] [6] [7] [8] [9] [10] [11] [12] [13] [14] [15] [16]

[17] [18] [19]

L. Pelaz, L. A. Marques, J. Barbolla: J. Appl. Phys. 96, 5947 (2004) 194 M. Bruzzi, et al.: Nucl. Instr. Meth. A 514, 189 (2005) 194 M. Huhtinen: Nucl. Instr. Meth. A 491, 194 (2002) 194 S. K. Estreicher: Mater. Sci. Eng. Rep. 14, 319 (1995) 195 A. Kerridge, A. H. Harker, A. M. Stoneham: J. Phys. Condens. Matter 16, 8743 (2004) 195 C. L. Muhlstein, E. A. Stach, R. O. Ritchie: Acta Mater. 50, 3579 (2002) 197 H. Kahn, R. Ballarini, J. J. Bellante, A. H. Heuer: Science 298, 1215 (2002) 197 J. Du, W. H. Ko, D. J. Young: Sens. Actuators A 112, 116 (2004) 197 P. Nguyen, I. Cayrefourcq, K. K. Bourdelle, A. Bougassol, E. Guiot, N. B. Mohamed, N. Sousbie, T. Akatsu: J. Appl. Phys. 97, 083527 (2005) 197 J. Weber, T. Fischer, E. Hieckmann, M. Hiller, E. V. Lavrov: J. Phys.: Condens. Matter 17, S2303 (2005) 197 B. Lawn: Fracture of Brittle Solids (Cambridge University Press, Cambridge 1993) 197 A. C. T. van Duin, S. Dasgupta, F. Lorant, W. A. Goddard: J. Phys. Chem. A 105, 9396 (2001) 198 S. J. Stuart, A. B. Tutein, J. A. Harrison: J. Chem. Phys. 112, 6472 (2000) 198 D. G. Pettifor, I. I. Oleinik, D. Nguyen-Manh, V. Vitek: Comp. Mater. Sci. 23, 33 (2002) 198 D. W. Brenner: phys. stat. sol. B 217, 23 (2000) 198 J. Molecular Structure – Theochem, Special Issue, vol. 632 (Elsevier Science BV 2003) Combined QM/MM Calculations in Chemistry and Biochemistry 199 W. C. Swope, H. C. Andersen, P. H. Berens, K. R. Wilson: J. Chem. Phys. 76, 637 (1982) 200 A. De Vita, R. Car: MRS Proc. 491, 473 (1998) 200 G. Cs´ anyi, T. Albaret, M. C. Payne, A. De Vita: Phys. Rev. Lett. 93, 175503 (2004) 200, 204

Multiscale Modeling of Defects in Semiconductors

211

[20] G. Cs´ anyi, T. Albaret, G. Moras, M. C. Payne, A. De Vita: J. Phys. Condens. Matter 17, R691 (2005) 200, 204 [21] W. H. Press, S. A. Teukolsky, W. T. Vetterling, B. P. Flannery: Numerical Recipes in C, 2nd ed. (Cambridge University Press, Cambridge 1992) 201 [22] F. Stillinger, T. Weber: Phys. Rev. B 31, 5262 (1985) 201, 203 [23] I. Kwon, R. Biswas, C. Z. Wang, K. M. Ho, C. M. Soukoulis: Phys. Rev. B 49, 7242 (1994) 203 [24] T. J. Lenosky, J. D. Kress, L. A. Collins, I. Kwon: Phys. Rev. B 55, 1528 (1997) 203 [25] D. Quigley, M. I. J. Probert: J. Chem. Phys. 120, 11432 (2004) 204 [26] V. V. Bulatov, J. F. Justo, W. Cai, S. Yip, A. S. Argon, T. Lenosky, M. de Koning, T. D. de la Rubia: Philos. Mag. A 81, 1257 (2001) 205 [27] S. Goedecker, T. Deutsch, L. Billard: Phys. Rev. Lett. 88, 235501 (2002) 206 [28] T. Frauenheim, G. Seifert, M. Elstner, Z. Hajnal, G. Jungnickel, D. Porezag, S. Suhai, R. Scholz: phys. stat. sol. B 217, 41 (2000) 206 [29] N. Bernstein: Europhys. Lett. 55, 52 (2001) 208 [30] F. F. Abraham, J. Q. Broughton, N. Bernstein, E. Kaxiras: Comp. Phys. 12, 538 (1998) 208 [31] S. Ogata, E. Lidorikis, F. Shimojo, A. Nakano, P. Vashishta, R. K. Kalia: Comp. Phys. Comm. 138, 143 (2001) 208 [32] R. P´erez, P. Gumbsch: Phys. Rev. Lett. 84, 5347 (2000) 208 [33] P. Gumbsch: Brittle fracture and the breaking of atomic bonds, in Materials Science for the 21st Century, vol. A (The Society of Materials Science, JSMS, Japan) pp. 50–58 208 [34] N. Bernstein, D. W. Hess: Phys. Rev. Lett. 91, 025501 (2003) 208

Index algorithm, 203, 204 anharmonic, 196 annealing, 194 asymmetric, 201 bond-centered, 195 boron, 206 bulk, 198 carbide, 195 classical, 195, 196, 198–200, 202–204, 206, 208, 210 cluster, 194 complex, 194, 195 core, 195 coupling, 205 covalent, 196, 199, 208 crack, 196, 197, 208

dangling bond, 196, 199 decay, 195 density-functional theory, 198 DFT, 198 DFTB, 206 diamond, 195 diﬀusion, 194, 195, 202, 203 dislocation, 195, 196, 205, 208 disorder, 196 distortion, 195, 196 dopant, 194, 196, 206 doping, 194 electron, 195, 196 embedding, 193 empirical, 194, 196, 198, 206 energetics, 196 equilibrium, 195, 196, 206

212

G´ abor Cs´ anyi et al.

ﬁnite element, 198 ﬁrst-principles, 193 force, 198–200, 202–205, 210 free-energy, 206 grain, 195, 196 grain boundary, 195, 196 Hamiltonian, 200, 204 hole, 196 hybrid, 197–200, 202, 203, 205, 206, 208, 210 hydrogen, 195, 197, 199, 204, 205 impurity, 195 interstitial, 194

phonon, 205 photoluminescence, 194 point defect, 194, 195, 203 positron annihilation, 194 potential, 195, 196, 201, 202, 208, 210 proton, 195 radiation damage, 194 relaxation, 197 Si, 197, 201, 203, 205 silicon, 194, 195, 197, 199, 203–205, 208 Stillinger–Weber, 203, 208 strain, 195, 208 stress, 196, 197, 208 supercell, 194 surface, 197–199, 202, 208

kink, 195, 205, 206

nanometer, 195

temperature, 203–206, 208 termination, 198, 199 tetrahedral, 195 thermostat, 204, 205 tight-binding, 198, 203, 204, 206 total energy, 199, 204 trajectory, 199, 200, 203 transition, 200

periodic, 194, 205

vacancy, 203

LOTF, 200, 203, 204, 206 migration, 194, 195, 206 molecular-dynamics, 193, 195, 198, 205 multiscale, 196, 197, 210

Empirical Molecular Dynamics: Possibilities, Requirements, and Limitations Kurt Scheerschmidt Max Planck Institute of Microstructure Physics, Weinberg 2, D-06120 Halle, Germany [email protected] Abstract. Classical molecular dynamics enables atomistic structure simulations of nanoscopic systems to be made. The method is extremely powerful in solving the Newtonian equations of motion to predict static and dynamic properties of extended particle systems. However, to yield macroscopically relevant and predictive results, suitable interatomic potentials are necessary, developed on ab-initio-based approximations. The fundamental requirements for performing classical molecular dynamics are presented as well as the relation to statistical methods and particle mechanics, suitable integration and embedding techniques, and the analysis of the trajectories. The applicability of the technique is demonstrated by calculating quantum-dot relaxations and interaction processes at wafer-bonded interfaces.

1 Introduction: Why Empirical Molecular Dynamics? Classical molecular dynamics (MD) enable atomistic structure simulations of nanoscopic systems and are, in principle, a simple tool to approach the manyparticle problem. For given interatomic or intermolecular forces one has to integrate the Newtonian equations of motion assuming suitable boundary conditions for the box containing the model structure. There are at least two advantages of this technique. The molecular dynamics is deterministic and provides the complete microscopic trajectories, i.e., the full static and dynamic information of all particles is available, from which a large number of thermodynamic and mechanically relevant properties of the models can be calculated. Further, one can perform simulations that are macroscopically relevant with the present computational power of even desktop computers. With reasonable computational eﬀort models of nanoscale dimension can be treated for several million particles and up to microseconds of real time. Thus, empirical MD has two main ﬁelds of application: The search for the global energetic minima by relaxing nanoscopic structures and the calculation of dynamical parameters by analyzing the lattice dynamics. Computer simulations are performed on models simulating the reality by using approximations, reduction, localization, linearization, etc., the validity of which has to be critically evaluated for each problem considered. As sketched in Fig. 1, increasing the time and length scales of the models (which is necessary to increase the macroscopic validity and robustness of the calculations) requires an increasing number of approximations and thus leads D. A. Drabold, S. K. Estreicher (Eds.): Theory of Defects in Semiconductors, Topics Appl. Physics 104, 213–244 (2007) © Springer-Verlag Berlin Heidelberg 2007

214

Kurt Scheerschmidt

Fig. 1. Length and timescales in various modeling methods: DFT = densityfunctional theory, TB = tight-binding approximations, BOP = bond-order potentials, MD = empirical molecular dynamics, MC, CGM = Monte-Carlo/conjugategradient techniques, FEM = ﬁnite element methods, CM = continuum mechanics

to a reduction in the ability to predict some physical properties. Densityfunctional theory (DFT) and its approximations (e.g., local-density LDA, generalized gradient GGA), and the diﬀerent kinds of tight-binding treatments (TB) up to the bond-order potential (BOP) approximations start with the Born–Oppenheimer (BO) approximation, thus decoupling the ionic and electronic degrees of freedom. Additional approximations such as pseudopotentials, gradient corrections to the exchange-correlation potential, and incomplete basis sets for the single-particle states are required for DFT calculations. The speciﬁcs of the various methods are discussed in various Chapters in the present book and in a number of review articles on DFT, TB, linear scaling techniques and programs such as SIESTA and CASTEP [1–9]. In ﬁrst-principle MD [10], e.g., using DFT or DFT-TB, the electronic system is treated as parameter free and the resulting Hellmann–Feynman forces are the glue of the ionic interactions. Such simulations are computationally too expensive for large systems. Figure 1 shows that the empirical MD closes the gap between ﬁrst-principles, macroscopic, and continuum techniques (FEM = ﬁnite element methods, CM = continuum mechanics). The latter neglect the underlying interatomic interactions but allow the description of defects, defect interactions, diﬀusion, growth processes, etc. Stochastic Monte Carlo techniques (MC) enable the further increase of the timescales, also at the ﬁrst-principles level, but without access to the dynamics. On the other hand, static energy minimization (e.g., conjugate gradient methods, CGM) enable a drastic increase in the model size. However, this does not necessarily provide the global mini-

Empirical Molecular Dynamics

215

Fig. 2. Interface structures at 90◦ twist boundaries ((a): P mm(m)-layer, (b): 42m-dreidl, cf. text in Sect. 4.2), predicted by empirical MD and revealed by abnitio DFT simulations yielding semimetallic/isolating behavior as a function of the interface bonding state as demonstrated by the corresponding DFT band structures (c) and (d), respectively

mum of the potential energy surface. The largest model dimensions (number of atoms) accessible to empirical MD (or MC, CGM) has approximately the same extension as the smallest devices in microelectronics and micromechanics. Thus, today’s atomistic modeling approaches the size of actual nanoscale systems. The assumption of the existence, validity, and accuracy of known empirical interatomic potentials or force ﬁelds in analytic form always ignores the underlying electronic origin of the forces, i.e., the quantum structure of the interactions (cf. Sect. 2.4). Therefore, it is important to have better approximations, such as the bond-order potential (BOP), which is developed from tight-binding approximations and discussed brieﬂy in Sect. 3.2. Other possibilities to include electronic properties of the interaction consist in continuously reﬁtting an empirical potential during the calculation, called learning on the ﬂy (see Chap. 9 and [11]). Separated subsystems can be treated at an ab-initio level. Suitable handshaking methods can be designed to bridge the embedded subsystem with its surrounding, which is treated semiclassically (cf. [12–15]). However, well-constructed potentials describing suﬃciently accurate physical properties also give physical insights and enable a thorough understanding of the underlying processes [2]. Figure 2 shows a simple example demonstrating the diﬀerence in the approximation levels. Using empirical MD the correct structural relaxation of special interfaces created by wafer bonding can be treated, as described later

216

Kurt Scheerschmidt

in Sect. 4.2. Two conﬁgurations exist, a metastable one (Fig. 2a) and the global minimum structure shown in Fig. 2b, called dreidl [16]. The electronic properties demand ab-initio level simulations, done here using a smaller periodic subunit of the interface and applying DFT techniques. It is shown that the higher-level approximation reproduces the structure predicted by the semiempirical techniques, whereas the correct energies and electronic properties (the band structure and the semimetallic or isolating behavior of the interfaces as shown in Figs. 2c,d) can only be described using the DFT formalism. A second kind of embedding problem occurs because even millions of particles only describe a small part of reality that, even for smaller pieces of matter, is characterized by Avogadro’s number (6 × 1023 mol−1 ). Since isolated systems introduce strong surface eﬀects, each model has to be embedded in suitable surroundings. For a discussion of various types of boundary conditions, see Sect. 3.1, Chap. 9 and [13–15]. The fundamental requirements of classical MD simulations, the relation to statistical methods and particle mechanics, suitable integration and embedding techniques and the analysis of the trajectories are presented in Sect. 2. The enhancements of potentials (bond-order potentials) and boundary conditions (elastic embedding) are discussed in Sect. 3. Selected application of semiempirical MD (relaxation of quantum dots and wafer-bonded interfaces) are given in Sect. 4 together with some examples from the literature. They strongly depend on the approximations assumed in the simulations.

2 Empirical Molecular Dynamics: Basic Concepts The main steps for applying empirical molecular dynamics consist of the integration of the basic equations (cf. Sect. 2.1) using a suitable interaction potential and embedding the model in a suitable surrounding (cf. Sect. 2.4 and Sect. 2.3, respectively). Textbooks of classical molecular dynamics, e.g., [17– 23], describe the technical and numerical details, and provide a good insight into possible applications and the physical properties, which may be predictable. Here, only the main ideas of empirical MD simulations, viz. the basic equations, methods of numerical treatment and the analysis of the trajectories are discussed. 2.1 Newtonian Equations and Numerical Integration The basic equations of motion solved in empirical MD are the Newtonian equations for N particles (i = 1, . . . , N ) characterized by their masses mi , f i . These may their coordinates ri , and the forces acting on each particle include external forces F i and interatomic interactions f i = j=i f ij : ¨i = f i = − mi r

∂V(r1 , r 2 , . . . , r N ) . ∂ri

(1)

Empirical Molecular Dynamics

217

The assumption that a potential V exists presupposes conservative (nondissipative) interactions and needs some more general considerations, cf. 2.2. Sect. V(r If one assumes pairwise central potentials, V(r1 , r 2 , ..., r N ) = ij ) i,j with rij = |r j − r i | (the dash means that the sum is restrictedto i < j), it follows that the virial of the external and internal forces is M = i,j rij f ij = the conservation i r i F i . If the system is isolated (microcanonical ensemble), of total energy E = K + V (with kinetic energy K = i mi r˙i 2 ) is guaranteed: r˙ i f i = 0 . E˙ = K˙ + V˙ = mi r˙i · r¨i − (2) i

i

Given an initial conﬁguration of particles and suitable boundary conditions (cf. Sect. 2.3), the diﬀerential equations can be integrated using one of the standard methods, e.g., Runge–Kutta techniques, predictor–corrector methods, Verlet or Gear algorithm. The numerical integration is equivalent to a Taylor expansion of the particle positions ri (t + δt) at a later time in terms of atomic positions ri and velocities v i . The forces f i are the time derivatives of r i with an increasing order at previous time steps: ri (t + δt) = ri (t) + a1 δtv i (t) + a2 (δt)2 f i (t) + . . . + O(δtn ) .

(3)

In addition to good potentials and system restrictions (cf. Sect. 2.3 and Sect. 2.4, respectively) an eﬃcient and stable integration procedure is required to accurately propagate the system. The conservation of energy during the simulation is an important criterion. An increase in order allows larger time increments δt to be used, if the evaluation of the higher derivatives is not too time consuming, which happens with more accurate potentials, like the BOP (Sect. 3.2). The eﬃciency and the accuracy of the integration can be controlled by choosing suitable series-expansion coeﬃcients aj , j = 1, 2, ..., n − 1 and the order n of the method or by mixing the derivatives of r i at diﬀerent times in (3) to enhance the procedure. However, the increment δt, of the order of fs, must be at least so small that the fastest particle oscillations are suﬃciently sampled. Better or faster MD calculations may be performed using special acceleration techniques, the three most important methods being: 1) Localization: By using the linked-cell algorithm and/or neighbor lists, it is assumed that for suﬃciently rapidly decaying potentials (faster than Coulomb 1/r for r → ∞) only a small number of particles have a direct and signiﬁcant interaction. A cutoﬀ rc is deﬁned and the interaction potential is assumed to be zero for r > rc . A transition region is ﬁtted using splines or other suitable functions. Then the system is divided into cells. Their minimum dimension is given by 2rc to avoid self-interaction of the particles (minimum image convention). Only the interactions of the atoms within a cell and its 26 neighboring cells are considered, which reduces the simulation time drastically from the ∝ N 2 behavior for all particle interactions to linear behavior ∝ 729cN N , where cN is the average number of particles per cell.

218

Kurt Scheerschmidt

The problem is to ﬁnd a suitable rc for a smooth transition and screening behavior that includes a suﬃcient number of next-neighbor atoms and cells. One also needs a suitable criterion to update the neighbor lists and reorder the cells whenever particles leave a cell during the propagation of the system. The Coulomb potential may also be screened. However, summations over the long-range 1/r potential, representing inﬁnite point-charge distributions, are only conditionally convergent. Thus, it is better to apply the Ewald method (originally developed to calculate cohesive energies and Madelung constants [24]) and its extensions [25, 26] based on successive charge neutralization by including next-neighbor shells around the origin. 2) Parallelization: Using replicas, or dividing the structure into several parts, which are then distributed to diﬀerent processors, thus allowing parallelization [27, 28]. The replica technique needs suitable criteria for dividing the system into small parts with minimum interaction. More importantly, one must bear in mind that the replicas are not independent over long times. A careful control of the time interval after which the communication between the diﬀerent parts is required in order to achieve the same results as nonparallelized simulations. This issue is the bottleneck of the technique. 3) Time stretching: Such techniques as hyperdynamics, temperature acceleration, basin-constrained dynamics, on-the-ﬂy Monte-Carlo, and others are subsumed brieﬂy here, because their common idea consists in replacing the true time evolution by a shorter one increasing the potential minima, transition frequencies, system temperature, etc. (see [28]). 2.2 Particle Mechanics and Nonequilibrium Systems In classical mechanics a system is characterized either by its Lagrangian L(q, q) ˙ = K(q, q) ˙ − V(q) or its Hamiltonian related to the Lagrangian by q˙i pi − L = K + V(q), where q i , pi are a Legendre transform H(q, p) = generalized coordinates and momenta (conjugate coordinates), respectively, which have to be independent or unrestricted. One derives the generalized momenta from the derivatives of the Lagrangian pi = ∂∂L q˙ i , whereas the derivatives of the Hamiltonian q˙i =

∂H , ∂pi

p˙i = −

∂H ∂qi

(4)

reproduce Newton’s law of motion (1). Hamilton’s principle of least action enables a simple generalization of the mechanics of many-particle systems. The integral over the Lagrangian function has to be an extremum. Variational methods yields, applying the extremal principle: ∂L d ∂L − = 0. dt ∂ q˙ i ∂q i

(5)

Empirical Molecular Dynamics

219

The advantage of the general formulation (5) is that it allows a simple extension to nonconservative systems by including an explicit time dependence or to systems with constraints, such as ﬁxed bond lengths in subsystems, friction of particles, outer forces, etc. If there are holonomic constraints describing relations between the coordinates fl (q k ) = 0, one gets the generalized additional coordinates alk = ∂fl /∂qk and al = ∂f l /∂t creating an additional term on the right-hand side of (5) in the form l λl alk with the set of Lagrange multipliers λl . This formalism is the basis for the enhancement of the boundary conditions in Sect. 3.1 and the handshaking methods mentioned above. In addition, the Lagrangian and Hamiltonian formalisms correlate classical dynamics to statistical thermodynamics and to quantum theory, and allow the evaluation of properties from the trajectories (cf. Sect. 2.5). The set of time-dependent coordinates q (the conﬁguration space) and timedependent momenta p (momentum space) together is called the phase space Γ = (q, p) = (q 1 , q 2 , ..., q n , p1 , p2 , ..., pn ). Presenting Γ in a 6-dimensional hyperspace yields N trajectories, one for each molecule, and allows the study of the behavior of the system using statistical methods. It is called the µ-space (following Ehrenfest) or the Boltzmann molecule phase space. The whole Γ set as one trajectory in a 6N -dimensional hyperspace presents the Gibbs phase space, with the advantage to include better interactions and restrictions. However, the system must now be described as a virtual assembly for statistical relations. The phase space Γ contains the complete information on the microscopic state of the many-particle system. Several basic quantities ˙ p). ˙ may be derived such as the phase-space ﬂow or the “velocity ﬁeld” Γ˙ = (q, Applying the relations (4) yields the Liouville equation ∂ q˙i ∂ p˙i + = 0, (6) ∇Γ Γ = ∂q i ∂pi showing that the ﬂow Γ˙ behaves like an incompressible liquid, i.e., although the µ-trajectories are independent, their related phase-space volume is constant. An equivalent formulation of the Liouville statement (6) is the equation of continuity for Γ˙ , ρ, ˙ and the local change of the density ρ(q, p, t), similar to the Heisenberg equation for observables in quantum theory. The density ρ(q, p, t) describes the probability of ﬁnding the system within the region p, q and p + dp, q + dq of the phase-space volume dpdq. Because the systems must be somewhere in the phase space, the density can be normalized in the entire phase space. The integral over the whole phase space of the non-normalized density yields the partition function. Integration over (N − k) particles yields the k-particle phase-space density ρ(k) (q, p, t) = ρ(N ) (q, p, t)dp(N −k) dq (N −k) , and the integration over the whole momentum space the corresponding k-particle distribution function n(k) (q) = ρ(N ) (q, p, t)dq (N −k) dp. Very important for the trajectory analy-

220

Kurt Scheerschmidt

sis (Sect. 2.5) are the cases k = 1, 2 deﬁning the (radial) pair-distribution functions g(q i , q j ): n(1) (q i )n(1) (q j )g(q i , q j ) = n(2) (q i , q j ).

(7)

The phase-space trajectories allow the classiﬁcation of the dynamics of many-particle systems. They may be Poincare-recurrent (the same phasespace conﬁguration occurs repeatedly), Hamiltonian (nondissipative), conservative (no explicit time dependence for the Hamiltonian), or integrable (number of constants of motion equals the number of degrees of freedom, resulting in stable periodic or quasiperiodic systems). Nonintegrable systems may be ergodic or mixing, etc., i.e., the trajectory densely covers diﬀerent hypersurfaces in the phase space, and allow the characterization of diﬀerent kinds of instabilities of the system. 2.3 Boundary Conditions and System Control As mentioned above, even for systems considered large in MD simulations, the number of atoms is small compared to real systems and therefore dominated by surface eﬀects. They are caused by interactions at free surfaces or with the box boundaries. In order to reduce nonrealistic surface eﬀects, periodic boundary conditions are applied, or the box containing the model (supercell) has to be enlarged so that the inﬂuence of the boundaries may be neglected. For further discussion and enhancements including elastic embedding, see Sect. 3.1. Periodic boundary conditions means that the supercell is repeated periodically in all space directions with identical image frames or mirror cells. In contrast to the case of ﬁxed boundaries, under periodic boundary conditions the particles can move across the boundaries. If this happens, the positions r have to be replaced by r −α where α is a translation vector to the image frame to which the particle is moved. Particle number, total mass, total energy, and momenta are conserved in periodic boundary conditions, but the angular momenta are changed and only an average of them is conserved. It should be mentioned here that periodic boundary conditions repeat defects, which in small supercells create high defect concentrations. Antiperiodic and other special boundary conditions may be chosen, where additional shifts of the positions and momenta along the box borders allow correction of a disturbed periodic continuation and a description of reﬂective walls at free surfaces to be obtained. According to the boundary conditions and system restrictions, the virtual Gibbs entities are either isolated microcanonical ensembles with constant volume, total energy, and particle numbers (N V E ensembles) or systems that exchange and interact with the environment. Closed ensembles (e.g., canonical N V T or isothermic-isobar N P T systems) have only an energy exchange with a thermostat, whereas open systems have in addition particle exchange with the environment (e.g., grand-canonical T µV , where µ is the chemical potential).

Empirical Molecular Dynamics

221

Simple tools exist to equilibrate systems at a well-deﬁned temperature. For example, velocity rescaling is numerically equivalent to a simple extension of the original microcanonical system with nonholonomic constraints in the Lagrangian formalism and is called the Berendsen thermostat. A similar simple extension may be used for pressure rescaling. It is called the Berendsen barostat [29]. The simple velocity rescaling works by conserving the Maxwell distribution and yielding maximum entropy. However, such nonisolated ensembles are better described using constraints in the Lagrangian similar to those discussed in Sect. 2.2. The extension of L in (5) by adding terms Lconstr introduces additional generalized variables having extra equations of motion and also additional force terms in the Newtonian equations (1). Some of the most important methods for Lconstr are given below without further comments: – Nos´e–bath and generalized Nos´e–Hoover thermostat [30–32]: Lconstr = mi , the M s˙ 2 /2 − nf T ln(s) with the ﬁctive or the whole mass M = degrees of freedom nf = 3N + 1, and the new generalized variable s playing the role of an entropy. – Andersen isothermic-isobaric system control (NPH ensemble) Lconstr = V˙ 2 /2 + P V introduces volume and pressure as generalized variables [33]. – Generalized stresses according to Parrinello and Rahman [34] N T Lσensembles: the Lagrangian is extended by Lconstr = −1/2T rΣG with a generalized symmetric tensor Σ and the metric tensor G of the crystal structure. A further specialization, e.g., for constant strain rates N T Lxσyy σzz -ensemble [35], is in principle a mixture of the isothermicisobaric system with the generalized stress constraint. – Brownian ﬂuctuations, transport and ﬂow processes, density and other gradients, Langevin damping ∝ v(t), etc. demand nonequilibrium MD [36, 37], which is mostly done by including the perturbation as a suitable virtual ﬁeld F (p, q, t) into the equations of motion via the Lagrange formalism. 2.4 Many-Body Empirical Potentials and Force Fields Empirical potentials and force ﬁelds exist with a wide variety of forms, and also diﬀerent classiﬁcation schemes are used according to their structure, applicability, or physical meaning. It makes no sense to describe a large number of potentials or many details in the present review, therefore only some of the existing and most used potentials are brieﬂy listed below (a good overview can be found in [38–48]. A classiﬁcation by Finnis [2] (and many references therein) describes recent developments and discusses in an excellent way the justiﬁcation of the potentials by ﬁrst-principle approximations, which is important for the physical reliability and the insight into the electronic structure of potentials. Interatomic forces are accurate only if the inﬂuence of the local environment according to the electronic structure is included. The most

222

Kurt Scheerschmidt

important property of a potential is transferability, that is the applicability of the potential to varied bonding environments. An important additional criterion is its ability to predict a wide range of properties without reﬁtting the parameters. The number of ﬁt parameters decreases as the sophistication of the force ﬁelds increases. According to [2] one has: Pair potentials – Valid for s-p bonded metals and mostly approximated by a sum of pairwise potentials. They may be derived as the response to a perturbation in jellium, which can be visualized in the pseudoatom picture as an ionic core and a screening cloud of electrons. Ionic potentials – To use Coulomb interactions directly for ionic structures, the problem of screening (Ewald summation, Madelung constant) has to be considered as mentioned above. The interactions were originally described by Born and others as the rigid-ion approximation. Starting from the Hohenberg–Kohn–Sham formulation of the DFT-LDA, shell or deformable ion models may be developed beyond the rigid-ion approximation, where the additional shell terms [49] look like electron-density diﬀerences in noble gases. Tight-binding models – Diﬀerent derivations and approximations for TBrelated potentials exist and are nowadays applicable to semiconductors, transition metals, alloys and ionic systems. The analytic bond-order potential is such an approximation and will be discussed in more detail in Sect. 3.2. Hybrid schemes – Combinations of pair potentials with TB approximations are known as generalized pseudopotentials, eﬀective media theories (EMT [50]), environmental-dependent ionic potentials (EDIP [51]), or embedded atom models (EAM [52]); for details see [2]. From the empirical point of view the simplest form of potentials may be considered to be a Taylor-series expansion of the potential energy with respect to 2-, 3-,. . ., n-body atomic interactions. Pair potentials have a shortrange repulsive part, and a long-range attractive part, e.g., of the Morse or Lennard–Jones (LJ) type, mostly “12–6”, i.e., ar−12 − br−6 . LJ potentials are successfully applied to noble gases, biological calculations, or to model long-range van der Waals interactions (e.g. [53]). For quasicrystals [54] an LJ potential was constructed with two minima in a golden number distance relation. However, simple pair potentials are restricted in their validity to very simple structures or to small deviations from the equilibrium. Therefore many-body interactions are added and ﬁtted for special purposes, e.g., the MD of molecules and molecule interactions [55,56]. Separable 3-body interactions are widely used: Stillinger–Weber [57] (SW), Biswas–Hamann [58], and Takai–Halicioglu–Tiller [59] potentials. The SW is perhaps the best-known 3-body-type potential. It includes anharmonic eﬀects necessary to reproduce the thermal lattice expansion of Si and Ge [60]. Hybrid force ﬁelds are sometimes used to include the interaction of diﬀerent types of atoms, such as Born–

Empirical Molecular Dynamics

223

Mayer–Huggins, Rahmann–Stillinger–Lemberg terms and others applicable to silicate glasses and interdiﬀusing metal ions or water molecules [61–65]. As mentioned above, other force ﬁelds are developed from ﬁrst-principle approximations that combine suﬃcient simplicity with high rigor. They are not based upon an expansion involving N -body interactions (cluster potentials). The more or less empirical forms of TB potentials and eﬀective medium force ﬁelds are the modiﬁed embedded atom model (MEAM, [66] for cubic structures and references therein for other structures), the Finnis–Sinclair (FS) [67] and the Tersoﬀ-type (TS) potentials [68–70]. The TS potential is an empirical bond-order potential with the functional form: V (rij ) = ae−λrij − bij e−µrij .

(8)

The bonds are weighted by the bond order bij = F (r ik , r jk , γijk ) including all next neighbors k = i, j, which gives the attractive interaction the form of an embedded many-body term. The diﬀerent parameterizations (TI, TII, TIII) of the Tersoﬀ potential have been intensively tested. Other parameterizations exist [71]. They involve other environmental functions and ﬁrst-principle derivations [72, 73], as well as extensions to include further interactions, H in Si [74], C, Ge [75], C–Si–H [76, 77], AlAs, GaAs, InAs, etc. [78]. Finally, a reﬁtted MEAM potential with SW terms is available for Si [79]. Multipole expansions replaced by spherical harmonics [80] are an alternative to TS potentials. A comparative study of empirical potentials shows advantages and disadvantages in the range of validity, physical transparency, ﬁtting and accuracy as well as applicability [81]. Restrictions exist for all empirical potential types, even if special environmental dependencies are constructed to enhance the elastic properties near defects. In addition, not all potentials are applicable to long-range interactions, and the electronic structure and the nature of the covalent bonds can only be described indirectly. Thus, it is of importance to ﬁnd physically motivated semiempirical potentials, as mentioned above and discussed in Sect. 3.2 for TB-based analytic BOPs. The parameters of the empirical force ﬁeld have to be ﬁtted to experimental data or ﬁrst-principle calculations. First, the cohesive energy, lattice parameter and stability of the crystal structures have to be tested or ﬁtted. The bulk modulus, elastic constants, and phonon spectra are very important properties for the ﬁt. The following section describes some of the quantities that may be used for the ﬁt or to be evaluated from the MD simulations if not ﬁtted. Very important details concerning point defects and defect clusters – necessary to get the higher-order interaction terms – are given by the energy and structure of such defects. The data may be given by DFT or TB dynamics or geometry optimizations, as, e.g., [82–85].

224

Kurt Scheerschmidt

2.5 Determination of Properties Static properties of systems simulated by empirical MD can be directly calculated from the radial- or pair-distribution function (7). Dynamic properties follow from the trajectories using averages or correlations: t 1 dtA[r(t)], C(t) = A(τ )B(t + τ )τ , (9) At = lim t→∞ t − t0 t 0 which in principle correspond to time averages. However, they are sampled at discrete points, so that it is necessary to choose suitable sampling procedures to reduce the eﬀects of the ﬁnite size of the system, stochastic deviations, and large MD runs. Two basic relations are central for the analysis of the properties. The ergodic hypothesis states that the ensemble average Ae is equal to the time average At , which relates the averages to the measurement of a sin2 0 )] t gle equilibrium system. The Green–Kubo formula limt→∞ [A(t)−A(t = t−t 0 ∞ ˙ ˙ with time correlations. t0 dτ (A(τ )A(t0 )e ) relates mean square deviations 1 2 The diﬀusion coeﬃcient D = limt→∞ 6N [r (t) − r j j (0)] (Einstein relat tion) is equivalent to the velocity autocorrelation function, which is a special ∞ 1 v (t) · v (0). Similarly, one form of the Green–Kubo formula D = 3N j j 0 uses the crosscorrelation of diﬀerent stress components to obtain shear viscosities. Other transport coeﬃcients may be derived analogously. In thermodynamic equilibrium the kinetic energyK per degree of freedom is determined by the equipartition theorem K = i mi v˙ i2 /2 = 3N kB T /2 (kB = Boltzmann constant) which yields a measure of the system temperature T . The strain tensor σ and the pressure P are obtained from the generalized virial theorem σkl = 1/V [ j v jk · v jl + ij r ijk · f ijl ]. Thus, the pressure is the canonical expectation value P = 1/3V [2K − M] of the total virial M. Alternatively, one can use the pair distribution in the ∞ 3 4πr dr, which may be useful for correcting form P = ρkB T − ρ2 0 g(r) ∂U ∂r sampling errors. Using the densities ρ(r, p) as deﬁned above and Z = ρ(r, p)dr as normalization, statistical mechanics deals with ensemble averages, which in general are written as (10) Qe = 1/Z Q(r, p)ρ(r, p)dr . All thermodynamic functions may be derived from the partition function Z, for example the free energy F (T, V, N ) = −kB T ln[Q(T, V, N )]. In addition, one can obtain all the thermodynamic response coeﬃcients. With the internal energy U , one computes the isochoric heat capacity CV = (∂U/∂T )N,V and thus a measure for the quality of the temperature equilibration (T 2 − T 2 )/T 2 = 3/2N (1 − 3kN )/2cV . From the volume V follows the isothermal compression χT = −1/V (∂V /∂P )N,T , etc. One has to choose according to the diﬀerent ensembles:

Empirical Molecular Dynamics

225

– Microcanonical: ρN V E = δ[H(r, p) − E] conserving entropy S(E, N, V ). – Canonical: ρN V T = e(H/kB T ) ∝ eV (r)/kB T conserving free energy F (T, V, N ) – Isothermic-isobaric: ρN P T = e(H−T S)/kB T conserving Gibbs free energy G(T, P, N ) – Grand canonical: ρT µV = e(H−µN )/kB T conserving Massieu function J(T, µ, V ) (Legendre transformation in entropy representation). Finally, it should be mentioned that the Fourier transform of pair distributions is connected to the scattering functions in X-ray, neutron and electron diﬀraction. MD-relaxed structure models allow the simulation of the transmission electron microscope (TEM) or high-resolution electron microscope (HREM) image contrast and therefore make the contrast analysis more quantitative. For this purpose, snapshots of the atomic conﬁgurations are cut into thin slices, which are folded with atomic scattering amplitudes and each other to describe the electron scattering (multislice formulation of the dynamical scattering theory), cf. the applications in Sect. 4 using this technique to interpret HREM investigations of quantum dots and bonded interfaces.

3 Extensions of the Empirical Molecular Dynamics Coupling of length and timescales in empirical MD means bridging the ﬁrstprinciples particle interactions and the box environment (1). It can be done either using embedding and handshaking or by a separate treatment and a transfer parameter between the subsystems. MD simulations of the crack propagation [86] and the analysis of submicrometer MEMS [87] are successfully applications of the FEM coupling between MD and an environmental continuum. In Sect. 3.1 enhanced boundary conditions for MD are discussed: where the coupling between MD and an elastic continuum is a handshaking method based on an extended Lagrangian [88, 89]. The main steps in the development of an analytic TB-based BOP [90] are sketched in Sect. 3.2 as an example of using enhanced potentials. 3.1 Modiﬁed Boundary Conditions: Elastic Embedding Elastic continua may be coupled to MD when the potential energy of an inﬁnite crystal with a defect as shown in Fig. 3a is approximated in the outer region II by generalized coordinates ak [89]: E({ri }, {rj }) = E({ri }, {ak }) .

(11)

In the defect region I, characterized by large strains, the positions of atoms r i (i = 1, . . . , N ) are treated by empirical MD. The atomic positions rj (j > N ) in the outer regions II and III result from the linear theory of elasticity rj = Rj + u(0) (Rj ) + u(Rj , {ak }) ,

(12)

226

Kurt Scheerschmidt

Fig. 3. Dislocation geometry ((a), I = MD region, II = elastic, III = overlap, cf. text) to apply elastic boundary conditions for a dipole of 60◦ dislocations, and snapshots during MD annealing: 500 K (b), 600 K (c), 0 K (d)

where the ﬁelds u0 (R) and u(R) describe the displacements of atoms from their positions Rj in the perfect crystal, and satisfy the equilibrium equations of a continuous elastic medium with defects; u0 (R) is the static displacement ﬁeld of the defect and independent of the atomic behavior in I; u(R) is related to the atomic shifts in region I and can be represented as a multipole expansion: u(R, {ak }) =

∞

ak U (k) (R)

(13)

k=1

over homogeneous eigensolutions U (k) (R) [88]. The U (k) are rapidly decreasing with R, thus the sum in (13) is truncated to a ﬁnite number K of terms. The equilibrium positions of atoms in the entire crystal are obtained from the minimization of the potential energy given in (11) with respect to r i and ak . This is equivalent to a dynamic formulation based on the extended Lagrangian as discussed above (Sect. 2.2 and Sect. 2.3) with the extension (11): L=

N mi r˙ 2 i

i=1

2

+

K µa˙k 2 k=1

2

− E({r i }, {ak }) .

(14)

Here, mi are the atomic masses and µ is a parameter playing the role of mass for the generalized coordinates ak . If µ is properly chosen, the phonons are smooth from I to II and the outer regions oscillate slower than the MD subsystem as demonstrated in the snapshots Figs. 3b–d. The corresponding system deﬁning the forces reads Fi = −

∂E({ri }, {ak }) , ∂r i

Fk = −

∂E({ri }, {rj }) ∂rj ∂E({ri }, {ak }) =− = F j U (k) (Rj ) . ∂ak ∂rj ∂ak

(15)

j>N

j∈II

(16)

Empirical Molecular Dynamics

227

These must vanish in the equilibrium F i = Fk = 0. The sum in (16) expands only over the atoms in region II surrounding region I, since in region III the linear elasticity alone is suﬃcient and the forces on these atoms are nearly vanishing. However, region II must be completely embedded in region III. The forces on atoms in region II must be derived from the interatomic potential, therefore the size of region II must be extended beyond the potential cutoﬀ rc . The Lagrangian (14) results in the equations of motion m¨ ri = F i ,

(i = 1, . . . , N ) ,

µ¨ ak = Fk ,

(k = 1, . . . , K) ,

(17)

thus extending Newton’s equations by equivalent ones for the generalized coordinates. 3.2 Tight-Binding-Based Analytic Bond-Order Potentials As discussed before, the use of TB methods allows much larger models than accessible to DFT. TB formulations exist in many forms (e.g., [2, 6–8, 91– 93]). The application of an analytical BOP, developed mainly by Pettifor and coworkers [90, 94–98], may further enhance empirical MD by providing better justiﬁed force ﬁelds while allowing faster simulations than numerical TB-MD. The approximations to develop analytic TB potentials from DFT may be summarized by the following steps (cf. also [2, 99]): 1. Construct the TB matrix elements by Slater–Koster two-center integrals including s- and p-orbitals, 2. transform the matrix to the bond representation, 3. replace the diagonalization by Lanczos recursion, 4. get the momenta of the density of states from the continued fraction representation of the Green’s function up to order n for an analytic BOP-n potential. The basic ideas sketched with a few more details are as follows. The cohesive energy of a solid in the TB formulation can be written in terms of the pairwise repulsion Urep of the atomic cores and the energy due to the formation of electronic bonds Ucoh = Urep + Uband − Uatoms 1 atom = φ(rij ) + 2 (n) − Niα εiα , 2 i,j iα

(18)

n(occ)

where the electronic energy ε of the free atoms has to be subtracted from the energy of the electrons on the molecular orbitals . Replacing (n) with the eigenstates of the TB-Hamiltonian for orbital α at atom i, (n) (n) (n) = (n) n|n = n| (n) |n = n|H|n = Ciα Hiα,jβ Cjβ , (19) iα,jβ

the electronic contributions to the cohesive energy Uband − Uatom = Ubond + Uprom can be rearranged and separated in the diagonal and oﬀdiagonal parts: atom 2ρiα,iα − Niα εiα . Ubond = 2 ρjβ,iα Hiα,jβ , Uprom = (20) iα,jβ

iα

228

Kurt Scheerschmidt

The third contribution, the promotion energy Uprom compares the occupancy of the atomic orbitals of the free atoms with the occupation of the corresponding molecular orbitals [100]. The bond energy Ubond describes the energy connected with the exchange or hopping of electrons between arbitrary pairs of atomic neighbors {i(j), j(i)}, the factor 2 is due to the spin degeneracy. The transition matrix elements of the Hamiltonian are hopping energies, and their transition probability is given by the corresponding element of the density matrix. The contribution for one bond between the atoms i and j is thus characterized by the part of the density called the bond order Θjβ,iα that may be expressed as a trace: i,j Ubond = Hiα,jβ Θjβ,iα = T r(HΘ) . (21) α,β

Besides the bond energy, the force exerted on any atom i must be given analytically and therefore one needs the gradient of the potential energy in (18) at the position of the atom i: ∂Ucoh ∂Ubond 1 ∂φ(rij ) = + . −F i = ∂ri ∂r i 2 j ∂r i j=i

(22)

This expression includes electronic bonds and ionic pairwise repulsions from all atoms of the system. The general form is still expensive to cope with for the simulation of mesoscopic systems. O(N ) scaling behavior is provided if the cohesive energy of the system is approximated by the Tersoﬀ potential i,j and a suitable cutoﬀ with resulting in (8), where bij e−µrij is replaced by Ubond balanced interatomic forces is added. To ﬁnd an eﬃcient way to obtain the bond energy in a manner that scales bond of the bond energy linearly with the system size, too, the derivative ∂U∂r i in (22) is replaced assuming a stationary electron density ρ in the electronic ground state and applying the Hellmann–Feynman theorem. The forces can now be obtained without calculating the derivatives of the electronic states and leads to the Hellmann–Feynman force [101, 102]: ∂Hiα,jβ −F HF = Θjβ,iα . (23) i ∂r i iα,jβ

Both the elements of the density matrix and the hopping elements of the Hamiltonian are functions of the relative orientation and separation of the bonding orbitals and have been calculated by Slater and Koster [103] assuming a linear combination of atomic orbitals (LCAO). To introduce the Slater–Koster matrix elements, usually denoted by ssσ, spσ, ppπ, etc., corresponding to the contributing orbitals and its interaction type, the TB Hamiltonian operator is transformed to a tridiagonal form. This can be done using the Lanzcos transformation [104]: Um HUn = an δm,n + bn δm,n−1 + bn+1 δm,n+1 ,

(24)

H|Un = an |Un + bn |Un−1 + bn+1 |Un+1 ,

(25)

Empirical Molecular Dynamics

229

where the orthonormal basis at the higher level n is recursively developed from |U0 . The coeﬃcients an , bn are the elements of the continuous fraction of the Green’s function below. The oﬀdiagonal elements of the density matrix are related to the Green’s function [105], ρiα,jβ

1 = − lim π η→0

Ef

dE Giα,jβ (Z) ,

(26)

where the complex variable Z = E + iη is the real energy E with a positive, imaginary inﬁnitesimal to perform the integration (theorem of residues). This intersite Green’s function can be connected to the site-diagonal Green’s function [105] via Giα,jβ (Z) =

∂GΛ 00 (Z) + GΛ 00 (Z)δi,j δα,β , ∂Λiα,jβ

(27)

and the latter can be evaluated recursively [106] using the coeﬃcients of the Lanczos recursion algorithm as mentioned above: GΛ 00 (Z) =

1 Z − aΛ 0 −

(bΛ1 )2 (bΛ2 )2 Z−aΛ − 1

.

(28)

Z−aΛ −... 2

The bond order can now be expressed in terms of the derivatives of the Λ recursion coeﬃcients aΛ n and bn , ∞

∞ ∂aΛ ∂bΛ n n Λ Λ χ0n,n0 +2 χ0(n−1),n0 , (29) Θiα,jβ = −2 ∂Λiα,jβ ∂Λiα,jβ n=0 n=1 E Λ with the response function χ0m,n0 (Ef ) = π1 limη→0 f dEGΛ 0m (Z)Gn0 (Z) and the elements G0n = Gn0 following from the system of equations (Z − an )Gnm (Z) − bn Gn−1,m (Z) − bn+1 Gn+1,m (Z) = δn,m . The more recursion coeﬃcients included in (29), the more accurately the bond order will be approximated. The recursion coeﬃcients are related to the moments of the local density of states (LDOS) [105] and the site-diagonal Green’s function of (26) and (27) relates to the LDOS itself. Therefore, the recursive solution of (28) gives an approximation to LDOS in terms of its moments [107] (n) Hiα,j1 β1 Hj1 β1 ,j2 β2 . . . Hjn−1 βn−1 ,iα (30) µiα = E n niα (E)dE = alljk βk

and may be interpreted as self-returning (closed) loops of hops of length n for electrons over neighboring atoms. The local atomic environment deﬁnes the LDOS via the moments (30), which in turn is used to calculate the bond

230

Kurt Scheerschmidt

order in (21) and the (local) atomic force (23). The remaining free paramei,j instead of bij may be ﬁtted in the ters in the analytic form (8) with Ubond usual way. This is still a hard task, because the bond and the promotion energy involve diﬀerent parameters as the repulsive part and cutoﬀ parameters and screening functions for all terms have to be included. Besides an accurate ﬁt, the BOP requires well-parameterized TB matrix elements or parameter optimizing, and the problem of transferability [99, 108–110] has to be considered separately. For BOP of order n = 2 the bond-order term in the TS-representation reads bij = (−ssσij + ppσij )Θiσ,jσ − 2ppπij Θiπ,jπ and the numerical behavior of BOP2 and TS are approximately equivalent. The details for higher-order BOP are given in the papers of Pettifor’s group [2, 99]. The bij terms of the analytic BOP4 involve complex angular dependencies, partially beyond those neglected in Pettifor’s formalism. For structures with defects as well as the wafer bonding of diamond surfaces where π-bonds cannot be neglected, BOP can be found in [111–114] and will soon be published elsewhere with detailed derivations.

4 Applications It is impossible to review the rapidly growing number of successful applications of empirical MD in materials research. A few representative examples may give an impression of the wide range of problems considered. Isolated point defects are mainly simulated to check the quality of the ﬁt of the potential parameters. Surface reconstructions, adatom and absorption phenomena, growth processes, and especially extended defect structures and interactions can be investigated in detail. The analysis of dislocation core-structures [115], the use of core-structure data for studying dislocation kink motion [116] or the dislocation motion during nanoindentation [117] are examples. Interface investigations have a long tradition, as illustrated in the standard book for grain-boundary structure [118] and growth [119]. Heterophase interfaces, e.g., using a Khor–de-Sama potential for Al and TS for SiC [120] to simulate Al/SiC interfaces, demand special attention to the correct description of the misﬁt [121] to get good interface energies. Simulations with the Tersoﬀ potential and its modiﬁcations yield the correct diameter of the critical nuclei for the growth of Ge nanocrystals in an amorphous matrix [122], allow the study of growth, strains, and stability of Si- and C-nanotubes [123, 124], and SiC surface reconstructions to propose SiC/Si interface structures [125]. A review of atomistic simulations of diﬀusion and growth on and in semiconductors [126] demonstrates the applicability of SW and TS potentials in comparison with data from TB and DFT calculations. In the following, two examples of our work are discussed. Empirical MD simulations of ﬁrst, high-resolution electron microscopy (HREM) image contrasts in quantum dots (Sect. 4.1) and second, the physical processes at interfaces during wafer bonding (Sect. 4.2).

Empirical Molecular Dynamics

231

4.1 Quantum Dots: Relaxation, Reordering, and Stability A quantum dot (QD) is a nanometer-scaled island or region of suitable material free-standing on or embedded in semiconductor or other matrices. The possibility to arrange QDs into complex arrays implies many opportunities for scientiﬁc investigations and technological applications. However, depending on the growth techniques applied (mainly MBE and MOCVD), the islands diﬀer in size, shape, chemical composition and lattice strain, which strongly inﬂuences the conﬁnement of electrons in nanometer-scaled QDs. The shape, size and strain ﬁeld of single QDs, as well as quality, density, and homogeneity of equisized and equishaped dot arrangements determine the optical properties, the emission and absorption of light, the lasing eﬃciency, and other optoelectronic device properties [127, 128]. A critical minimum QD size is required to conﬁne at least one electron/exciton in the dot. A critical maximum QD size is related to the separation of the energy levels for thermally induced decoupling. Uniformity of the QD size is necessary to ensure coupling of states between QDs. The localization of states and their stability depend further on composition and strain of the QDs. The strain relaxation at facet edges and between the islands is the driving force behind self-organization and lateral arrangement, vertical stacking on top or between buried dots, or preordering by surface structuring. In addition, an extension of the emission range towards longer wavelengths needs a better understanding and handling of the controlled growth via lattice mismatched heterostructures or self-assembling phenomena (see, e.g., [129]). A wide variety of imaging methods are used to investigate growth, selfassembly, and physical properties of quantum dots. Among these the crosssectional HREM and the plan-view TEM imaging techniques are suitable methods to characterize directly shape, size, and strain ﬁeld [130]. But the HREM and TEM techniques images are diﬃcult to interpret phenomenologically, especially when separating shape and strain eﬀects. Modeling is essential to uniquely determine the features and provide contrast rules. In Fig. 4, the atomic structure of an InGaAs-QD in a GaAs matrix (for other systems cf. [130, 131]) is prescribed by geometric models and relaxed by MD simulations. Very diﬀerent dot shapes have been proposed and theoretically investigated: lens-shaped dots, conical islands, volcano-type QDs, and pyramids with diﬀerent side facets of type {011}, {111}, {112}, {113}, {136}, and both {011} + {111} mixed, etc. Some of these and a spherical cap are schematically presented in Fig. 4a; in simulations one or two monolayers (ML) thick wetting layers are included, too. The most important diﬀerence between the various structures is the varying step structure of the facets due to their diﬀerent inclination. There are at least two reasons to investigate these conﬁgurations [130]. First, small embedded precipitates always have facets; a transition between dome-like structure and pyramids due to changes in spacer distance, change the number and arrangement of the facets, and thus strain and electronic properties. Second, for highly faceted struc-

232

Kurt Scheerschmidt

Fig. 4. Structure modeling and image simulation of diﬀerent pyramidal-shaped quantum-dot conﬁgurations: (a) diﬀerent faceting, truncation, and wetting of pyramidal start models (matrix removed, models related to (001)-base planes), (b) relaxed complete model of a {011} pyramid (base length about 6 nm, 10 × 10 × 10supercell length 10 nm), (c) energy relaxation of a {011} quantum dot (potential Epot and total Etot energy versus time steps), (d) cross-sectional HREM and bright-ﬁeld diﬀraction contrast simulated for model (b) before and after relaxation assuming a standard 400 kV microscope at the Scherzer focus (i.e., ∆ = −40 nm, Cs = 1 mm, α = 1.2 nm−1 , t = 9 nm, δ = 8 nm−1 , cf. [130])

Empirical Molecular Dynamics

233

tures the continuum elasticity is practically inapplicable and ﬁnite element calculations must be done in 3-D instead of 2-D. However, the technique of ab-initio MC provides a more accurate prediction of the QD shapes than empirical MD [132]. The embedding of one perfect {011} pyramid in a matrix is demonstrated in Fig. 4b after prerelaxation. Figure 4c shows typical annealing behavior during empirical MD calculation, characterized by the potential Epot and the total energy Etot per atom. The energy diﬀerence Etot − Epot is equal to the mean kinetic energy and is thus directly related to the temperature of the system. After the prerelaxation of 5 ps at 0 K, an annealing cycle follows, 60 ps stepwise heat up to 600 K and cool down to 0 K, equilibrating the system at each heating step. The example here demonstrates a short cycle; most of the embedded QDs are relaxed at each T -step for at least 10 000 timesteps of 0.25 fs, followed by annealing up to about 900 K (the temperature is not well deﬁned with empirical potentials but is below the melting temperature). Whereas the structure in Fig. 4b is less strained, highly strained conﬁgurations occur due to the self-interaction of the QD in small supercells that correspond to a stacked sequence with very small dot distances. The extension of the supercell chosen in the simulations depends on the extension of the QD to be investigated, as well as on the overlap of the strain ﬁelds at the borders, to avoid self-interactions. Whereas Fig. 4b shows a relatively small supercell, investigations are made for supercells of up to 89 × 89 × 89 unit cells with a base length of the QD of 9 nm containing several million atoms. For the image simulations, subregions of the supercells are used, sliced into one atomic layer and applying the multislice image simulation technique. By comparing imaging for structures before and after relaxation, Fig. 4d demonstrates the enormous inﬂuence of the relaxations on the image contrast in cross-sectional HREM and TEM [130, 131]. In summarizing some of the results one can state that MD calculations with SW (CdZnSe) and TII (InGaAs, Ge) allow us to obtain well-relaxed structures, in contrast to the static relaxations performed with the Keating potential [133, 134]. With this insight into the atomic processes of rearranging and straining QDs at an atomic level the growth conditions for quantum dots may be enhanced as a ﬁrst step to tailoring their properties. 4.2 Bonded Interfaces: Tailoring Electronic or Mechanical Properties? Wafer bonding, i.e., the creation of interfaces by joining two wafer surfaces, has become an attractive method for many practical applications in microelectronics, micromechanics or optoelectronics [135]. The macroscopic properties of bonded materials are mainly determined by the atomic processes at the interfaces (clean and polished hydrophobic or hydrophilic surfaces, as schematically shown in Fig. 5) during the transition from adhesion to chemical bonding. For this, elevated temperatures or external forces are required, as could be revealed by MD simulations of hydrogen-passivated interfaces [136]

234

Kurt Scheerschmidt

Fig. 5. Wafer bonding at Si[100] surfaces: simulations of surface rearrangement for perfect alignment and slow heating. The ﬁgure describes the evolution of the atomic relaxation leading to bonded wafers

or of silica bonding [65]. Thus, describing atomic processes is of increasing interest to support experimental investigations or to predict bonding behavior. Already, slightly rescaled SW potentials predict the bond behavior via bond breaking and dimer reconﬁguration as shown in the snapshots explaining the possibility of covalent bonding at room temperature for very clean hydrophobic surfaces under UHV conditions [137]. Whereas the bonding of two perfectly aligned, identical wafers gives a single, perfectly bonded wafer without defects, miscut of the wafer results in steps on the wafer surfaces and edge dislocations at the bonded interfaces are created. In Fig. 6 the red color describes the potential energy above the ground state during wafer bonding over two-atomic steps. The upper terraces behave like perfect surfaces and the dimerized starting conﬁguration of Fig. 6a is rearranged and new bonds are created. The energy gained is dissipated and for slow heat transfer the avalanche eﬀect leads to bonding of the lower terraces, too. Two 60◦ dislocations remain and, depending on the rigid shift of the start conﬁguration, an additional row of vacancies [137]. The dislocations may split as simulated and observed in experiments [138].

Empirical Molecular Dynamics

235

Fig. 6. MD simulation of wafer bonding over surface steps. Note the dislocation relaxation for the initial conﬁguration (left), a snapshot during annealing up to 900 K, after 12.5 ps (middle) and the ﬁnal relaxed state (right)

Bonding wafers with rotational twist leads to a network of screw dislocations at the interface. A special situation is the 90◦ twist, which always occurs between monoatomic steps. A Stillinger–Weber potential applied to a 90◦ twist bonded wafer pair [16] yields a metastable ﬁvefold-coordinated interface with a mirror symmetry normal to the interface characterized by a P mm(m)layer group (cf. Fig. 2a). Using the Tersoﬀ or BOP-like potentials [113] and metastable or well-prepared starting conﬁgurations allows further structure relaxation and energy minimization. Figure 2b shows this relaxed conﬁguration, which is (2 × 2) reconstructed and consists of structural units with a 42m-(D2d) point group symmetry, called the 42m-dreidl. It should be emphasized that the dreidl structure is found to be the minimum energy conﬁguration also in DFT-LDA simulations [16]. However, the energies diﬀer from those given in [139, 140]. Much more important is the modiﬁcation of the band structure due to the diﬀerent interface relaxation that may enable engineering of the electronic properties: whereas the metastable conﬁguration (cf. Fig. 2c) yields semimetallic behavior, the dreidl structure (cf. Fig. 2d) yields a larger bandgap than in perfect lattices. The dreidl interface structure and its band-structure modiﬁcation is very similar to the essential building blocks proposed by Chadi [141] for group-IV materials. They describe geometry and properties of the transformation of Si and Ge under pressure and the special allo-phases as a new class of crystalline structures. A small misalignment of the wafers during wafer bonding yields bonded interfaces with twist rotation resulting in a checkerboard-like interface structure [142, 143]. Figure 7 shows some of the resulting minimum structures gained for higher annealing temperatures and diﬀerent twist rotation angles. Before the bonding process takes place, the superposition of the two wafers looks like a Moir´e pattern in the projection normal to the interface. After bonding and suﬃcient relaxation under slow heat-transfer conditions, almost all atoms have a bulk-like environment separated by misﬁt screw dislocations, which may have many kinks. The screw dislocation-network of the bonded wafer has a period half that of the Moir´e pattern. One ﬁnds more imperfectly bonded regions around the screw dislocations for smaller twist

236

Kurt Scheerschmidt

Fig. 7. MD relaxations of bonding rotationally twisted wafers ([001] and [110] views) with diﬀerent angles: (a) 2.8◦ , 22 nm box, orthogonal dimers, [001] view; (b) 6.7◦ , 9.2 nm box, orthogonal dimers, [001] and [110] views; (c) as (a) and (d) as (b) with parallel dimers

angles, whereas bonding at higher angles results in more or less widely spread strained interface regions. In Fig. 7 bonding with orthogonal start conﬁgurations (a,b) is compared to those with parallel dimer start conﬁgurations (c,d). Thus the bonding of Figs. 7a and b may be considered as bonding with an additional 90◦ twist rotation. Clearly the periodicity of the defect region is twice those of Figs. 7b and c smoothing out the interface, but creating additional shear strains. Irrespective of the chosen twist angles and box dimensions all ﬁnal structures yield bond energies of approximately 4.5 eV/atom at 0 K, however, varying slightly with the twist angle. A maximum occurs between 4◦ and 6◦ twist related to a change of the bonding behavior itself. The higher the annealing temperature the better the screw formation. In conclusion, simulation of the atomic processes at wafer-bonded interfaces oﬀers not only the tailoring of electronic properties, it is also an important step in understanding how to control the creation of special interface structures for strain accommodation or prepatterned templates (compliant substrates) [135] by rotational alignment.

5 Conclusions and Outlook Molecular dynamics simulations based on empirical potentials provide a suitable tool to study atomic processes that inﬂuence macroscopic materials properties. The applicability of the technique is demonstrated by calculating quantum-dot relaxations and interaction processes with defect creation at wafer-bonded interfaces. A brief overview describes the method itself and its advantages and limitations, i.e., the macroscopic relevance of the simulations versus the limited transferability of the potentials. The quality of the simulations and the reliability of the results depend on the coupling of the

Empirical Molecular Dynamics

237

atomistic simulations across length and timescales. Whereas the Lagrange formalism is well established for the embedding into suitable environments at the continuum level, the approximations of ﬁrst-principles-based potentials need continuous future work.

References [1] W. Kohn: Rev. Mod. Phys. 71, 1253 (1999) 214 [2] M. W. Finnis: Interatomic forces in condensed matter, in Oxford Series on Materials Modelling (Oxford University Press, Oxford 2003) 214, 215, 221, 222, 227, 230 [3] K. Ohno, K. Esforjani, Y. Kawazoe: Computational Materials Science: From ab initio to Monte Carlo Methods (Springer, Berlin, Heidelberg 1999) 214 [4] M. C. Payne, M. P. Teter, D. C. Allen, et al: Rev. Mod. Phys. 64, 1045 (1992) 214 [5] G. Galli, A. Pasquarello: First-principles molecular dynamics, in M. P. Allen, D. J. Tildesley (Eds.): Computer Simulation in Chemical Physics (Academic Publisher, Dordrecht, Netherlands 1993) pp. 261–313 214 [6] T. Frauenheim, G. Seifert, M. Elstner, et al: phys. stat. sol. B 217, 41 (2000) 214, 227 [7] D. R. Bowler, T. Miyazaki, M. J. Gillan: J. Phys.: Condens. Matter 14, 2781 (2002) 214, 227 [8] J. M. Soler, E. Artacho, J. D. Gale, et al: J. Phys.: Condens. Matter 14, 2745 (2002) 214, 227 [9] M. D. Segall, P. J. D. Lindan, M. J. Probert, et al: J. Phys.: Condens. Matter 14, 2717 (2002) 214 [10] R. Car, M. Parinello: Phys. Rev. Lett. 55, 2471 (1985) 214 [11] G. C. Csany, T. Albaret, M. C. Payne, A. DeVita: Phys. Rev. Lett. 93, 175503 (2004) 215 [12] P. Ruggerone, A. Kley, M. Scheﬄer: Bridging the length and time scales: from ab initio electronic structure calculations to macroscopic proportions, Comm. Condens. Matter Phys. 18, 261 (1998) 215 [13] R. M. Nieminen: J. Phys.: Condens. Matter 14, 2859 (2002) 215, 216 [14] R. E. Rudd, J. Q. Broughton: phys. stat. sol. B 217, 251 (2000) 215, 216 [15] B. I. Lundquist, A. Bogicevic, S. Dudy, et al: Comput. Mater. Sci. 24, 1 (2002) 215, 216 [16] K. Scheerschmidt, D. Conrad, A. Belov: Comput. Mater. Sci. 24, 33 (2002) 216, 235 [17] J. M. Haile: Molecular Dynamics Simulation: Elementary Methods (Wiley, New York 1992) 216 [18] D. C. Rapaport: The Art of Molecular Dynamics Simulation (Cambridge Univ. Press, Cambridge 1998) 216 [19] R. Haberlandt: Molekulardynamik: Grundlagen und Anwendungen (Vieweg, Braunschweig, Wiesbaden 1995) 216 [20] W. G. Hoover: Molecular dynamics, in Lecture Notes in Physics, vol. 258 (Springer, Berlin, Heidelberg 1986) 216

238

Kurt Scheerschmidt

[21] I. G. Kaplan: Theory of molecular interactions, in Studies in Physical and Theoretical Chemistry, vol. 42 (Elsevier Science Ltd., Amsterdam 1986) 216 [22] M. Sprik: Introduction to molecular dynamics methods, in K. Binder, G. Cicotti (Eds.): Monte Carlo and Molecular Dynamics of Condensed Matter Systems, vol. 49, Conf. Proc. Vol. (SIF, Bologna 1996) Chap. 2, pp. 47–87 216 [23] D. W. Heermann: Computer Simulation Methods in Theoretical Physics (Springer, Berlin, Heidelberg 1990) 216 [24] J. M. Ziman: Principles of the Theory of Solids (Cambridge Univ. Press, Cambridge 1972) 218 [25] S. W. deLeeuw, J. W. Perram, E. R. Smith: Proc. Roy. Soc. London A 373, 27 (1980) 218 [26] D. Wolf, P. Keblinski, S. R. Phillpot, J. Eggebrecht: J. Chem. Phys. 110, 8254 (1999) 218 [27] A. F. Voter: Phys. Rev. B 57, 13985 (1998) 218 [28] A. F. Voter, F. Montalenti, T. C. Germann: Ann. Rev. Mater. Res. 32, 321 (2002) 218 [29] W. Rullmann, H. Gunsteren, H. Berendsen: Mol. Phys. 44, 69 (1981) 221 [30] S. Nos´e: Mol. Phys. 52, 255 (1984) 221 [31] S. Nos´e: J. Chem. Phys. 81, 511 (1984) 221 [32] W. G. Hoover: Phys. Rev. A 31, 695 (1985) 221 [33] H. C. Andersen: J. Chem. Phys. 72, 2384 (1980) 221 [34] M. Parinello, A. Rahman: J. Appl. Phys. 52, 7182 (1981) 221 [35] L. Yang, D. J. Srolowitz, A. F. Yee: J. Chem. Phys. 107, 4396 (1997) 221 [36] G. P. Morriss, D. J. Evans: Phys. Rev. A 35, 792 (1987) 221 [37] D. J. Evans, G. P. Morriss: Statistical Mechanics of Nonequilibrium Liquids (Academic, London, New York 1990) 221 [38] J. D. Gale: Special Issue: Interatomic Potentials, Philos. Mag. B 73, 3 (1996) 221 [39] A. Horsﬁeld: Special Issue: Interatomic Potentials, Philos. Mag. B 73, 85 (1996) 221 [40] S. C. Price: Special Issue: Interatomic Potentials, Philos. Mag. B 73, 95 (1996) 221 [41] J. N. Murrell: Special Issue: Interatomic Potentials, Philos. Mag. B 73, 163 (1996) 221 [42] D. L. Cooper, T. Thorsteinsson: Special Issue: Interatomic Potentials, Philos. Mag. B 73, 175 (1996) 221 [43] M. C. Payne, I. J. Robertson, D. Thomssen, V. Heine: Special Issue: Interatomic Potentials, Philos. Mag. B 73, 191 (1996) 221 [44] Guest Editor A. F. Voter, V. Vitek: MRS-Bull. 21, 20 (1992) 221 [45] S. M. Foiles: MRS-Bull. 21, 24 (1992) 221 [46] M. Stoneham, J. Hardy, T. Harker: MRS-Bull. 21, 29 (1992) 221 [47] D. W. Brenner: MRS-Bull. 21, 36 (1992) 221 [48] A. P. Sutton, P. D. Goodwin, A. P. Horseﬁeld: MRS-Bull. 21, 42 (1992) 221 [49] N. A. Marks, M. W. Finnis, J. H. Harding, N. C. Pyper: J. Chem. Phys. 114, 4406 (2001) 222 [50] K. W. Jacobsen, J. K. Norskov, M. J. Puskas: Phys. Rev. B 35, 7423 (1987) 222 [51] N. A. Marks: J. Phys. Condens. Matter 14, 2901 (2002) 222 [52] M. S. Daw: Phys. Rev. B 39, 7441 (1989) 222

Empirical Molecular Dynamics

239

[53] Y. C. Wang, K. Scheerschmidt, U. G¨ osele: Phys. Rev. B 61, 12864 (2000) 222 [54] H. R. Trebin: Comp. Phys. Commun. 121–122, 536 (1999) 222 [55] A. K. Rappe, C. J. Casewit, K. S. Colwell, et al: J. Am. Chem. Soc. 114, 10024 (1992) 222 [56] W. F. van Gunsteren, H. J. C. Berendsen: Angew. Chem., Int. Ed. Engl. 29, 992 (1990) 222 [57] F. H. Stillinger, T. A. Weber: Phys. Rev. B 31, 5262 (1985) 222 [58] R. Biswas, D. R. Hamann: Phys. Rev. B 36, 6434 (1987) 222 [59] T. Takai, T. Halicioglu, W. A. Tiller: Scr. Metal. 19, 709 (1985) 222 [60] C. P. Herrero: J. Mater. Res. 16, 2505 (2001) 222 [61] A. K. Nakano, B. J. Berne, P. Vashista, R. K. Kalia: Phys. Rev. B 39, 12520 (1989) 223 [62] S. H. Garofalini: J. Non-Cryst. Solids 120, 1 (1990) 223 [63] D. Timpel, K. Scheerschmidt, S. H. Garofalini: J. Non-Cryst. Solids 221, 187 (1997) 223 [64] D. Timpel, K. Scheerschmidt: J. Non-Cryst. Solids 232–234, 245 (1998) 223 [65] D. Timpel, M. Schaible, K. Scheerschmidt: J. Appl. Phys. 85, 2627 (1999) 223, 234 [66] M. I. Baskes: Phys. Rev. B 46, 2727 (1992) 223 [67] M. W. Finnis, J. E. Sinclair: Philos. Mag. A 50, 45 (1984) 223 [68] J. Tersoﬀ: Phys. Rev. Lett. 56, 632 (1986) 223 [69] J. Tersoﬀ: Phys. Rev. B 38, 9902 (1989) 223 [70] J. Tersoﬀ: Phys. Rev. B 39, 5566 (1989) 223 [71] W. Dodson: Phys. Rev. B 35, 2795 (1987) 223 [72] G. C. Abell: Phys. Rev. B 31, 6184 (1985) 223 [73] D. W. Brenner: phys. stat. sol. B 217, 23 (2000) 223 [74] M. V. R. Murty, H. A. Atwater: Phys. Rev. B 51, 4889 (1995) 223 [75] D. W. Brenner: Phys. Rev. B 42, 9458 (1990) 223 [76] A. J. Dyson, P. V. Smith: Surf. Sci. 355, 140 (1996) 223 [77] K. Beardmore, R. Smith: Philos. Mag. A 74, 1439 (1996) 223 [78] K. Nordlund, J. Nord, J. Frantz, J. Keinonen: Comput. Mater. Sci. 18, 504 (2000) 223 [79] T. J. Lenosky, B. Sadigh, E. Alonso, et al: Model. Simul. Mater. Sci. Eng. 8, 825 (2000) 223 [80] S. D. Chao, J. D. Kress, A. Redondo: J. Chem. Phys. 120, 5558 (2004) 223 [81] H. Balamane, T. Halicioglu, W. A. Tiller: Phys. Rev. B 46, 2250 (1992) 223 [82] M. Kohyama, S. Takeda: Phys. Rev. B. 60, 8075 (1999) 223 [83] M. Gharaibeh, S. K. Estreicher, P. A. Fedders: Physica B 273–274, 532 (1999) 223 [84] S. K. Estreicher: phys. stat. sol. B 217, 513 (2000) 223 [85] W. Windl: phys. stat. sol. B 226, 37 (2001) 223 [86] S. Kohlhoﬀ, P. Gumbsch, H. F. Fischmeister: Philos. Mag. A 64, 851 (1991) 225 [87] R. E. Rudd, J. Q. Broughton: Phys. Rev. B 58, R5893 (1998) 225 [88] A. Y. Belov: Dislocations emerging at planar interfaces, in V. L. Indenbom, J. Lothe (Eds.): Elastic Strain Fields and Dislocation Mobility (Elsevier, Amsterdam 1992) pp. 391–446 225, 226 [89] J. E. Sinclair: J. Appl. Phys. 42, 5321 (1971) 225

240

Kurt Scheerschmidt

[90] D. G. Pettifor: Phys. Rev. Lett. 63, 2480 (1989) 225, 227 [91] C. M. Goringe, D. R. Bowler, E. Hernandez: Rep. Prog. Phys. 60, 1447 (1997) 227 [92] A. P. Horsﬁeld, A. M. Bratkovsky: J. Phys. Condens. Matter 12, R1 (2000) 227 [93] D. A. Papaconstantopoulos, M. J. Mehl: J. Phys. Condens. Matter 15, R413 (2003) 227 [94] D. G. Pettifor, I. I. Oleinik, D. Nguyen-Manh, V. Vitek: Comput. Mater. Sci. 23, 33 (2002) 227 [95] D. Pettifor: From Exact to Approximate Theory: The Tight Binding Bond Model and Many-Body Potentials., vol. 48, Springer Series (Springer, Berlin, Heidelberg 1990) 227 [96] D. G. Pettifor, I. I. Oleinik: Phys. Rev. B 59, 8487 (1999) 227 [97] D. G. Pettifor, I. I. Oleinik: Phys. Rev. Lett. 18, 4124 (2000) 227 [98] D. G. Pettifor, M. W. Finnis, D. Nguyen-Manh, et al: Mater. Sci. Eng. A 365, 2 (2004) 227 [99] A. P. Sutton: Electronic Structure of Materials (Clarendon Press, Oxford 1994) 227, 230 [100] A. P. Sutton, M. W. Finnis, D. G. Pettifor, Y. Ohta: J. Phys. C 35, 35 (1988) 228 [101] H. Hellmann: Einf¨ uhrung in die Quantenchemie (Deuticke, Leipzig 1937) 228 [102] R. P. Feynman: Phys. Rev. 56, 340 (1939) 228 [103] J. C. Slater, G. F. Koster: Phys. Rev. 94, 1498 (1954) 228 [104] C. Lanczos: J. Res. Natl. Bur. Stand. 45, 225 (1950) 228 [105] A. P. Horsﬁeld, A. M. Bratovsky, M. Fear, et al: Phys. Rev. B 53, 12694 (1996) 229 [106] R. Haydock: Recursive Solution of the Schr¨ odinger Equation, vol. 35, Solid State Physics (Academic, London, New York 1980) 229 [107] F. Ducastelle: J. Phys. 31, 1055 (1970) 229 [108] O. F. Sankey, D. J. Niklewski: Phys. Rev. B 40, 3979 (1989) 230 [109] I. Kwon, R. Biswas, C. Z. Wang, et al: Phys. Rev. B 49, 7242 (1994) 230 [110] T. J. Lenosky, J. D. Kress, I. Kwon, et al: Phys. Rev. B 55, 1528 (1997) 230 [111] D. Conrad: Molekulardynamische Untersuchungen f¨ ur Oberﬂ¨ achen und Grenzﬂ¨ achen von Halbleitern, Thesis, Martin-Luther-Universit¨ at, Halle (1996) 230 [112] V. Kuhlmann: Entwicklung analytischer bond-order Potentiale f¨ ur die empirische Molekulardynamik, Thesis, Martin-Luther-Universit¨ at, Halle (2006) 230 [113] D. Conrad, K. Scheerschmidt: Phys. Rev. B 58, 4538 (1998) 230, 235 [114] D. Conrad, K. Scheerschmidt, U. G¨ osele: Appl. Phys. Lett. 77, 49 (2000) 230 [115] T. Harry, D. Bacon: Acta Mater. 50, 195 (2002) 230 [116] V. V. Bulatov, J. F. Justo, W. Cai, et al: Philos. Mag. A 81, 1257 (2001) 230 [117] E. T. Lilleodden, J. A. Zimmermann, S. M. Foiles, W. D. Nix: J. Mech. Phys. Solids 51, 901 (2003) 230 [118] D. Wolf, S. Yip (Eds.): Materials Interfaces: Atomic-Level Structure and Properties (Chapman & Hall, London 1992) 230 [119] A. J. Haslam, D. Moldovan, S. R. Phillpot, et al: Comput. Mater. Sci. 23, 15 (2002) 230 [120] X. Luo, G. Qian, E. G. Wang, C. Chen: Phys. Rev. B 59, 10125 (1999) 230

Empirical Molecular Dynamics

241

[121] R. Benedek, D. N. Seidman, C. Woodward: J. Phys. Condens. Matter 14, 2877 (2002) 230 [122] K. J. Bording, J. Tafto: Phys. Rev. B 62, 8098 (2000) 230 [123] J. W. Kang, J. J. Seo, H. J. Hwang: J. Nanosci. Nanotechnol. 2, 687 (2002) 230 [124] D. Srivasta, D. W. Brenner, J. D. Schall, et al: J. Phys. Chem. B 103, 4330 (1999) 230 [125] C. Koitzsch, D. Conrad, K. Scheerschmidt, U. G¨ osele: J. Appl. Phys. 88, 7104 (2000) 230 [126] E. Kaxiras: Comput. Mater. Sci. 6, 158 (1996) 230 [127] D. Bimberg, M. Grundmann, N. N. Ledentsov: Quantum Dot Heterostructures (John Wiley & Sons., Chicester 1999) 231 [128] L. W. Wang, A. Zunger: Pseudopotential theory of nanometer silicon quantum dots, in P. V. Kamat, D. Meisel (Eds.): Semiconductor Nanoclusters – Physical, Chemical, and Catalytic Aspects (Elsevier, Amsterdam, New York 1997) 231 [129] H. Lee, J. A. Johnson, M. Y. He, et al: Appl. Phys. Lett. 78, 105 (2001) 231 [130] K. Scheerschmidt, P. Werner: Characterization of structure and composition of quantum dots by transmission electron microscopy., in M. Grundmann (Ed.): Nano-Optoelectronics: Concepts, Physics and Devices (Springer, Berlin, Heidelberg, New York, Tokyo 2002) Chap. 3, pp. 67–98 231, 232, 233 [131] K. Scheerschmidt, D. Conrad, H. Kirmse, R. Schneider, W. Neumann: Ultramicroscopy 81, 289 (2000) 231, 233 [132] E. Pehlke, N. Moll, A. Kley, M. Scheﬄer: Appl. Phys. A 65, 525 (1997) 233 [133] P. N. Keating: Phys. Rev. 145, 637 (1966) 233 [134] Y. Kikuchi, H. Sugii, K. Shintani: J. Appl. Phys. 89, 1191 (2001) 233 [135] Q. Y. Tong, U. G¨ osele: Semiconductor Wafer Bonding: Science and Technology (Wiley, New York 1998) 233, 236 [136] D. Conrad, K. Scheerschmidt, U. G¨ osele: Appl. Phys. Lett. 71, 2307 (1997) 233 [137] D. Conrad, K. Scheerschmidt, U. G¨ osele: Appl. Phys. A 62, 7 (1996) 234 [138] A. Y. Belov, R. Scholz, K. Scheerschmidt: Philos. Mag. Lett. 79, 531 (1999) 234 [139] A. Y. Belov, D. Conrad, K. Scheerschmidt, U. G¨ osele: Philos. Mag. 77, 55 (1998) 235 [140] A. Y. Belov, K. Scheerschmidt, U. G¨ osele: Phys. Status Solidi A 159, 171 (1999) 235 [141] D. J. Chadi: Phys. Rev. B 32, 6485 (1985) 235 [142] K. Scheerschmidt: MRS Proc. 681E, I2.3 (2004) 235 [143] K. Scheerschmidt, V. Kuhlmann: Interf. Sci. 12, 157 (2004) 235

Index ab-initio, 215, 216, 233

algorithm, 217, 229

absorption, 230, 231

alignment, 234–236

adatom, 230

amorphous, 230

242

Kurt Scheerschmidt

anharmonic, 222 annealing, 233, 235, 236 autocorrelation function, 224 band structure, 216, 235 basis set, 214 Berendsen, 221 Boltzmann, 219, 224 bond order, 216, 222, 223, 228–230 bond-order potential, 214, 215, 217, 223, 227, 230, 235 Born–Oppenheimer, 214 bulk modulus, 223 canonical, 220, 224, 225 chemical potential, 220 classical, 213, 216, 218, 219 cluster, 223 cohesive energy, 218, 223, 227, 228 concentration, 220 conjugate gradient, 214, 215 conservative, 217, 220 correlation, 224 Coulomb, 217, 218, 222 coupling, 225, 231, 236 covalent, 223, 234 crack, 225 cutoﬀ, 217, 228 decay, 217 degeneracy, 228 density matrix, 228, 229 density of states, 227, 229 density-functional theory, 214 DFT, 214, 216, 222, 223, 227, 230, 235 diamond, 230 diﬀusion, 214, 224, 230 dislocation, 230, 234, 235 distribution function, 219 EDIP, 222 eigenstates, 227 elastic embedding, 216, 220 electron, 222, 227–229, 231 embed, 216, 220, 225, 231, 233, 237 embedded, 215, 216, 222, 223, 227, 231, 233 empirical, 213–216, 222–225, 230, 233, 236

EMT, 222 energy level, 231 entropy, 221, 225 equilibrium, 222, 224, 226, 227 ergodic, 220, 224 Ewald, 218, 222 exchange, 220, 228 exchange-correlation, 214 exciton, 231 ﬁnite element, 214 ﬁrst principles, 214, 225, 237 ﬂuctuation, 221 force, 213–217, 219, 221–223, 226–228, 230, 231, 233 Fourier, 225 free energy, 224, 225 Ge, 223, 230, 233, 235 general gradient approximation, 214 GGA, 214 Gibbs, 219, 220, 225 glass, 223 grain boundary, 230 grand-canonical, 220, 225 Green’s function, 227, 229 Green–Kubo, 224 ground state, 228, 234 Hamiltonian, 218–220, 227, 228 handshaking, 215, 219, 225 Heisenberg, 219 Hellmann–Feynman, 214, 228 heterostructure, 231 hopping, 228 hybrid, 222 hydrogen, 233 imaginary, 229 interface, 215, 216, 225, 230, 233–236 internal energy, 224 isothermal, 224 jellium, 222 kink, 230 Lagrange, 219, 221, 237 Lagrangian, 218, 219, 221, 225–227 LDA, 214

Empirical Molecular Dynamics Lennard–Jones, 222 Liouville, 219 liquid, 219 localization, 213, 217, 231 Madelung, 218, 222 Maxwell, 221 melting, 233 microcanonical, 217, 220, 221, 225 misﬁt, 230, 235 molecular dynamics, 213, 216 Morse, 222 multipole, 223, 226 nanometer, 231 Newton, 227 Nos´e, 221 optical, 231 optoelectronic, 231 pair-distribution function, 220, 224 Parrinello, 221 partition function, 219, 224 periodic boundary conditions, 220 periodicity, 236 perturbation, 221, 222 phase space, 219, 220 phonon, 223, 226 point defect, 223, 230 potential, 214–218, 220–223, 225–228, 230, 233–235 precipitates, 231 pseudoatom, 222 pseudopotential, 214, 222 quantum dot, 225, 230, 231, 233, 236 radial-distribution function, 224 recursion, 227, 229 relaxation, 215, 216, 231, 233, 235, 236 repulsive, 222, 230 rotational, 235, 236

243

scattering, 225 screening, 218, 222, 230 self-interaction, 217, 233 self-organization, 231 semiempirical, 216, 223 shear, 224, 236 Si, 222, 223, 230, 235 SIESTA, 214 Slater, 227, 228 spherical harmonic, 223 spin degeneracy, 228 statistical, 216, 219, 224 Stillinger–Weber, 222, 235 strain, 221, 224, 225, 230, 231, 233, 236 stress, 221, 224 supercell, 220, 233 surface, 215, 216, 220, 230, 231, 233, 234 symmetric, 221 symmetry, 235 Taylor, 217, 222 temperature, 218, 221, 224, 233–236 Tersoﬀ, 223, 228, 230, 235 thermostat, 220, 221 tight binding, 214, 215, 222 total energy, 217, 220, 233 trajectory, 219, 220 transferability, 222, 230, 236 transition, 217, 218, 222, 228, 231, 233 transport, 221, 224 Van der Waals, 222 variational, 218 velocity autocorrelation, 224 Verlet, 217 wafer bonding, 215, 230, 233–235 water, 223 wavelength, 231 X-ray, 225

Defects in Amorphous Semiconductors: Amorphous Silicon D.A. Drabold and T.A. Abtew Department of Physics and Astronomy, Ohio University, Athens, Ohio [email protected]

Abstract. Defects in disordered (amorphous) semiconductors are discussed, with an emphasis on hydrogenated amorphous silicon. The general diﬀerences between defect phenomena in crystalline and amorphous hosts are described, and the special importance of the electron–phonon coupling is stressed. Detailed calculations for amorphous Si are presented using accurate ﬁrst principles (density-functional) techniques. The various approximations of ab-initio simulation aﬀect aspects of the network structure and dynamics, and suitably accurate approximations are suggested. Defect dynamics and the motion of hydrogen in the network are reported.

1 Introduction This book is primarily concerned with defects in crystalline materials. In this Chapter, we depart from this and discuss defects in amorphous materials. In the Chapter of Simdayankin and Elliott, a most interesting feature of amorphous materials, photoresponse, is discussed in detail. As in the case of crystals, defects determine key features of the electronic, vibrational and transport properties of amorphous materials [1–3]. These are often precisely the properties that are relevant to applications. In this Chapter we strongly emphasize amorphous silicon (a-Si), while not focusing on it exclusively. This is signiﬁcantly due to the background of the authors and constraints on the length of the Chapter, but it is also true that a-Si oﬀers at least a somewhat generic theoretical laboratory for the study of disorder, defects, and other aspects of amorphous materials in general. The outline of this Chapter is as follows: First, we brieﬂy survey amorphous semiconductors. Next, we deﬁne the notion of a defect, already a somewhat subtle question in an environment that is intrinsically variable in structure. In the fourth section, we discuss the generic electronic and vibrational attributes of defects in amorphous solids, and brieﬂy comment on the current methods for studying these systems. In Sect. 5, we discuss calculations of the dynamics of defects in the a-Si:H network, of critical importance to the stability and practical application of the material.

D. A. Drabold, S. K. Estreicher (Eds.): Theory of Defects in Semiconductors, Topics Appl. Physics 104, 245–268 (2007) © Springer-Verlag Berlin Heidelberg 2007

246

D.A. Drabold and T.A. Abtew

2 Amorphous Semiconductors Amorphous materials and glasses are among the most important to human experience with applications ranging from primitive obsidian weapons to optoelectronics. Today, every oﬃce in the world contains storage media for computers (for example DVD-RW compact disks) that exploit the special reversible laser-driven amorphization/crystallization transition properties of a particular GeSbTe glass. The same computer uses crystalline Si chips that depend critically upon the dielectric properties of a-SiO2 . With increasing pressure on global energy markets, it is notable that some of the most promising photovoltaic devices are based upon amorphous materials such as a-Si:H because of the low cost of the material (compared to crystalline devices) and the ability to grow thin ﬁlms of device-quality material over wide areas. The internet depends upon ﬁber-optic glass light pipes that enable transmission of information with bandwidth vastly exceeding that possible with wires. This list is the proverbial tip of the iceberg. Experimental measurements for structure determination, such as X-ray or neutron diﬀraction, lead easily to a precise determination of the structure of crystals. Nowadays, protein structures with thousands of atoms per unit cell are readily solved. The reason for this impressive success is that the diﬀraction data (structure factor) consists of a palisade of sharply deﬁned spikes (the Bragg peaks), arising from reﬂection from crystal planes. For amorphous materials, the same experiments are rather disappointing; smooth broad curves replace the Bragg peaks. The wavelength-dependent structure factor may be interpreted in real space through the radial distribution function (RDF), which is easily obtained with a Fourier transform of the structure factor. In crystals, the RDF consists again of spikes, and the radii at which the spikes occur are the neighbor distances. In the amorphous case, the RDF is smooth, and normally has broadened peaks near the locations of the ﬁrst few peaks of the crystal. This similarity in the small-r peak positions reﬂects a tendency of amorphous materials to attempt to mimic the local order of the crystalline phase in the amorphous network, but usually with modest bond-length and bond-angle distortions. At distances beyond several nearest-neighbor spacings, similarities between crystalline and amorphous pair correlations wane, and the pair correlations decay to zero after tens of ˚ Angstroms in the amorphous material (this number is system dependent). From an information theoretic point of view (for example, consideration of the Shannon–Jaynes information entropy [4]), it is clear that there is less information inherent in the (smooth) data for the amorphous case relative to the crystal. So, while it is possible to invert the diﬀraction data from crystals to obtain structure determination (with some assumptions to ﬁx the phase problem), such a process fails for the amorphous case and many studies have emphasized the multiplicity of distinct structures possible that can reproduce measured diﬀraction data. In this sense we are in a situation rather like highenergy or nuclear physics where there are sum rules that must be obeyed,

Defects in Amorphous Semiconductors: Amorphous Silicon

247

but the sum rules by themselves oﬀer an extremely incomplete description of the physical processes. The ﬁrst goal of theoretical work in amorphous materials is to obtain an experimentally realistic model consistent with all trusted experiments and also accurate total energy and force calculations. Early models of amorphous materials were made by hand, but this approach was soon supplanted by simulations with the advent of digital computers. A variety of modeling schemes based upon simulated atomic dynamics (so-called molecular-dynamics), Monte Carlo methods, methods based upon attempts to obtain the structure from the diﬀraction measurements (most sensibly done with constraints to enforce rules on bonding) and even hybrids between the last two are in current use [5–8]. Impressive progress has been made in the last 25 years of modeling, and highly satisfactory models now exist for many amorphous materials, among these: Si, Si:H, Ge, C, silica, elemental and binary chalcogenides [9–12]. Empirically, systems with lower mean coordination (ﬂoppier in the language of Thorpe [13]) are easier to model than higher-coordination systems. Multinary materials tend to be more challenging than elemental systems as the issue of chemical ordering becomes important and also these systems are harder to model accurately with conventional methods. Empirical potentials, tight-binding schemes and ab-initio methods are used for modeling the interatomic interactions [5, 14– 16]. In the area of defects in amorphous semiconductors, it is usually the case that ﬁrst-principles interactions are required. Where electronic properties of amorphous semiconductors are concerned, k-space methods are not useful as the crystal momentum is not a good quantum number (the translation operator does not commute with the Hamiltonian). Rather, one focuses on the density of electron states, and on individual eigenvectors of the Hamiltonian, especially those near the Fermi level. The electronic density of states is usually qualitatively like that of a structurally related crystal, but broadened by disorder. In Fig. 1, we illustrate these features with a “real” calculation on a 10 000-atom model of a-Si [11, 17]. The sharp band edges expected in crystals are broadened into smooth “bandtails”. The tails are created by structural disorder; early Bethe lattice calculations demonstrated that strained bond angles lead to states pushed out of the band (into the forbidden optical gap), and loosely, the more severe the defect, the further into the gap. It is known from optical studies of amorphous semiconductors that all such systems have band-tails decaying exponentially into the gap. While the optical spectrum is a convolution involving both tails, photoemission studies have separately probed the valence tail and conduction tails particularly in a-Si:H [18], and found that both decay exponentially, albeit with diﬀerent rates and a temperature dependence (quite diﬀerent for the two tails) that suggests the importance of thermal disorder beside the structural order we have stressed so far [19]. The ﬁeld of amorphous semiconductors is a vast area in which many books and thousands of papers have been written, and it is impossible to do justice even to the specialized topic of defects. For this reason, we emphasize a few

248

D.A. Drabold and T.A. Abtew

Fig. 1. Electronic density of states near a band edge in a 10 000-atom model of amorphous Si. Insets show |ψ|2 , indicating parts of the cell in which the defect wavefunctions are localized. The mobility edge separating localized and extended states is indicated. The “band-tail” extends from about −15.5 eV to the mobility edge [17]

questions of particular current interest, and recommend the comprehensive treatments of Elliott and Zallen [20, 21] for general discussion of amorphous materials including defects.

3 Defects in Amorphous Semiconductors 3.1 Deﬁnition of Defect Static Network A complete discussion of defects in amorphous materials may be found in Chap. 6 of the book by Elliott [20]. Evidently, the term defect implies a departure from the typical disorder of an amorphous network. Perhaps it is not surprising that it is not possible to produce a deﬁnition of defect without some arbitrary character. Thus, in deﬁning a coordination defect, one introduces a distance that deﬁnes whether a pair of atoms is bonded or not. So long as the model structure contains no bonds very close to the critical length, the deﬁnition is unambiguous. In amorphous materials there is usually

Defects in Amorphous Semiconductors: Amorphous Silicon

249

a well-deﬁned (deep) minimum in the pair-correlation function between the ﬁrst- and second-neighbor peaks, which gives a reasonable justiﬁcation for selecting the distance at which the minimum occurs as a cutoﬀ length for deﬁnition of coordination. When one accounts for thermal motion of the atoms, the situation is murkier, as we describe below. If the primary interest is electronic properties of the amorphous semiconductor, one can introduce an electronic criterion to identify defects. As for the geometrical criterion, such a deﬁnition is necessarily formulated as a suﬃcient departure from the mean. An electronic defect may be deﬁned as a structural irregularity that produces a suﬃciently localized electronic eigenstate. The ambiguous point here is the modiﬁer “suﬃciently”: isolated states in the middle of the gap (such as a threefold “dangling-bond” state in a-Si) are easily recognized as defects with a spatially conﬁned wavefunction. Other less-localized states stemming from other network defects may be better characterized as part of the band-tailing. In the same spirit, the chemical bond order (essentially oﬀdiagonal elements of the single-particle density matrix) may be used to identify defects, but a cutoﬀ will be required as always to deﬁne the line between bonded and not! A simple quantitative measure of localization is given below. To contrast the geometrical and electronic deﬁnitions of defects, welllocalized electronic eigenstates do correspond to network irregularities (either structural, chemical or both) and suﬃciently large geometrical irregularities manifest themselves as localized states in a spectral gap in the electronic spectrum (note that this does not necessarily have to be the optical gap (the gap that contains the Fermi level) – other spectral gaps or even the extremal band edges can exhibit these states). Dynamic Network The schemes to deine defects outlined above are consistent for suﬃcient departure from the mean structure. To a surprising degree, however, room-temperature thermal disorder implies the existence of thermally induced geometrical defect ﬂuctuations. Thus, in an ab-initio simulation of a-Si, the number of ﬁvefold “ﬂoating” bonds varied between 0 and 10 in a 2 ps roomtemperature run for a 216-atom unit cell with coordination deﬁned by a 2.74 ˚ A bond distance [19]. At face value this is astonishing, suggesting that 5 % of the atoms change their coordination in thermal equilibrium at room temperature! If the electronic and geometrical deﬁnitions were identical, it would imply that states should be jumping wildly into and out of the gap. Of course this is not the case, though it is true that instantaneous Kohn–Sham energy eigenvalues in the gap do thermally ﬂuctuate [19]. This example illustrates that geometrical defects are not necessarily electronic defects. One can also easily see that electronic defects are not necessarily coordination defects: while an atom may nominally possess ideal (8-N rule) coordination,

250

D.A. Drabold and T.A. Abtew

substantial bond-angle distortions can also induce localized electronic states. We present new simulations of defect dynamics in Sect. 5. 3.2 Long-Time Dynamics and Defect Equilibria It is apparent from a variety of experiments in a-Si:H that there are reversible, temperature-dependent changes that occur in defect type and concentration. At its simplest, the idea is that particular defects have a characteristic energy in an amorphous material. It may be that these energies are not substantially removed from the typical conformations of the host. Because the amorphous network does not possess long-range order, it is possible for a small number of atoms to move to convert one kind of defect into another, without a huge cost in energy. These ideas can predict the temperature dependence of some electronic properties, for example quantities like the density and character of band-tail states [22–25]. By analyzing a variety of experiments, Street and coworkers [26] have demonstrated that the idea of defect equilibrium is essential. At present the approach is phenomenological to the extent that the microscopic details of the defects involved are not certainly known or even needed, but in principle these ideas could be merged with formation energies and other information from ab-initio simulations to make a ﬁrst-principles theory of defect equilibria. The potential union between the phenomenological modeling and simulation is also potentially a good example of “bridging timescales” though there is much work still required on the simulation side to realize this goal. 3.3 Electronic Aspects of Amorphous Semiconductors Localization A remarkable feature of electron states in crystals is that the wavefunctions have support (are nonzero) throughout the crystal, apart from surface effects. Such states are called extended. The utility of Bloch’s theorem is that it reduces the formulation of the electronic structure problem for the inﬁnite periodic system to a simpler form: calculation within a single unit cell on a grid of k crystal momentum points. Thus, for crystals, information about the electronic structure is provided by band-structure diagrams. Such diagrams are not useful in amorphous systems, and furthermore, in amorphous materials, some states may not be extended. To model the electronic consequences of disorder, it is usual to adopt a tight-binding (either empirical or ab initio) description of the electron states, and a Hamiltonian schematically of the form: εi |ii| + Jij |ij| . (1) H= i

ij,i=j

Defects in Amorphous Semiconductors: Amorphous Silicon

251

To keep the number of indexes to a minimum, we suppose that there is one orbital per site (indexed by i). In this equation, the εi specify the atomic energy at each site (in an elemental system, this would be constant for all sites) and Jij is a hopping integral that depends on the coordinates of the atoms located at sites i and j. The topological disorder of a particular realization of an amorphous network (e.g., a structural model) is manifested through the oﬀdiagonal or hopping terms Jij . An enormous eﬀort has been devoted to studying the properties of the eigenvectors of H, and also the critical properties (e.g., of quantum phase transitions [17]). In realistic studies of the electronic localized–delocalized transition [17] (here “realistic” means large-scale electronic structure calculations in which the disorder in the Hamiltonian matrix is obtained from experimentally plausible structural models, rather than by appealing to a random number generator), it is found that the eigenstates near midgap are spatially compact (localized) and for energies varied from midgap into either the valence or conduction-bands, the states take “island” form: a single eigenstate may consist of localized islands of charge separated by volumes of low charge density. The islands themselves exhibit exponential decay, and the decay lengths for the islands increase modestly from near midgap to the mobility edge. The states become extended with approach to the mobility edge by proliferation (increasing number) of the islands [17, 22]. The qualitative nature of this localized to extended transition is similar for electronic and vibrational disorder of diverse kinds and also conventional Anderson models. Thus, in important ways the localized to extended transition is universal [17]. Characterizing Localized States As we have discussed, the concept of localized states is a central one for amorphous materials and indeed defective systems in general. The question immediately arises: given an electronic eigenvector expressed in some representation, how can we quantify the degree of localization? The most widely adopted gauge of localization is the so-called “inverse participation ratio” (IPR), which is deﬁned as: I(E) =

N

q(n, E)2 ,

(2)

n=1

where N is the number of atoms and q(n, E) is a Mulliken (or other) charge on atom n, and the analysis is undertaken for a particular energy eigenstate with energy E. This measure ranges from N −1 (N number of sites) for an ideally extended state to 1 for a state perfectly localized to one site. One can use other measures, such as the information entropy, but at a practical level, we have found that the IPR and information entropy produce qualitatively (not quantitatively) similar results for the localization. IPR is a simple tool for categorizing the zoo of extended, localized and partly localized states of

252

D.A. Drabold and T.A. Abtew

amorphous semiconductors with defects [27]. As quantum chemists know, all such deﬁnitions are basis dependent, and thus care is needed in the interpretation of local charges, IPR and related quantities [28]. Locality of Interatomic Interactions For atomistic simulation of any materials, a fundamental measure of the spatial nonlocality of interatomic interactions is the decay of the single-particle density matrix, or equivalently, the decay characteristics of the best localized Wannier functions that may be constructed in the material. The density matrix is deﬁned as: ψi∗ (r )ψi (r) , (3) ρ(r, r ) = ioccupied

where ψi are eigenfunctions of the Hamiltonian in position representation. In a typical condensed-matter system, the ψi are oscillating functions, almost all of which will be delocalized through space. Consequently, one can expect “destructive interference” eﬀects as in other wave phenomena when many wiggling functions are superposed as in (3), which can make ρ(r, r ) decay ˆ is the Hamiltonian, then the electronic conrapidly for large |r − r |. If H ˆ If the trace is carried out in tribution to the total energy is E = T r(ˆ ρH). the position representation, one can then see that the decay of the density matrix provides information about the locality of the interatomic potential. The details of the chemistry and structure of the material determine this decay length, and the full results even for the asymptotic decay in a greatly simpliﬁed two-band model are too complicated to reproduce here [29]. For a material with a ﬁnite optical gap as we assume in this Chapter, the decay is ultimately exponential and the decay is faster for larger optical gaps. Recently, the density matrix has been explicitly computed for a structurally realistic 4096-atom model [10] of a-Si that was fourfold coordinated, but with some large bond-angle distortions. There are two key conclusions from this work: 1. the spatial nonlocality of interatomic interactions is very similar in a-Si and c-Si (because the density matrix decays in a similar fashion for both) and 2. defect centers in a-Si (in this model associated with bondangle distortions) have Wannier functions with asymptotic decay similar to ordinary (tetrahedral) sites (of course the short-range behavior involving the ﬁrst few neighbors may be quite diﬀerent) [22]. 3.4 Electron Correlation Energy: Electron–Electron Eﬀects For a localized single-particle defect state, one must consider the possibility of the state being occupied by zero, one or two (opposite spin) electrons. Consideration of the energetics of these various occupations led in the 1970s and 1980s to insights into the nature of defects, particularly in chalcogenide materials. Typically the electron–electron Coulomb repulsion costs a net energy

Defects in Amorphous Semiconductors: Amorphous Silicon

253

(usually labeled “U ”) to enable two electrons to occupy the same localized spatial state. This is called a “positive U ” defect center (the name comes from the symbol used in a Hubbard Hamiltonian to model the electron–electron interaction). In a-Si:H, U > 0 for the dangling-bond. It is worth mentioning that the accurate calculation of U is a challenging task for the conventional density-functional methods, as these are essentially mean-ﬁeld methods and appear to consistently overestimate the delocalization of defect states. When the possibility of structural relaxation is considered as the second opposite-spin electron is added to the localized state, a negative eﬀective U , implying a net energy lowering for double occupation, can emerge. This is observed in chalcogens, and as pointed out by early workers, explains the pinned Fermi level and the diamagnetism of the materials (that is, lack of unpaired spins and so the absence of an ESR signal). It follows that double occupancy implies that defects are charged, and the chemistry (p bonding) of the chalcogens like S or Se leads to the occurrence of “valence alternation pair” defects. Thus, careful simulations reveal that isolated dangling-bonds in a-Se are unstable, and are likely to convert instead into VAPs [30]. Elliott discusses these points thoroughly [20].

4 Modeling Amorphous Semiconductors 4.1 Forming Structural Models For amorphous materials we immediately face a challenging problem: What is the atomistic structure of the network? Usually there is a strong tendency for particular local structure (chemical identity of neighbors, and geometrical bonding characteristics), but this preference is only approximately enforced: there is a characteristic distribution of bond lengths and bond angles that is dependent upon both the material and its preparation. Thus, in “better-quality” a-Si samples, almost all of the atoms are four-coordinated, and the bond angle between a reference Si atom and two neighbors is within about 10 degrees of the tetrahedral angle: a strong echo of the chemistry and structure of diamond. In binary glasses (for example GeSe2 ), Ge is essentially always fourfold coordinated, and Ge only rarely bonds to Ge. Also, as one would expect from crystalline phases of GeSe2 or simple considerations of chemical bonding, the glass is made up predominantly of GeSe4 tetrahedral, again with Se–Ge–Se bond angles close to the tetrahedral angle [31–37]. As reviewed by Thorpe [38], the ﬁrst attempt to understand glasses was based upon the idea that amorphous materials were microcrystalline with a very ﬁne grain size. Eventually, it became clear that this model could not explain the structural experiments that were available. The idea that was ultimately accepted was advanced in 1932 by Zachariasen [39] for amorphous SiO2 , the “continuous random network” (CRN) model. Here, the local chemical requirements (four-coordinated Si bonded only to two-coordinated O, and

254

D.A. Drabold and T.A. Abtew

no homopolar bonds) were enforced, but there was local disorder in bond angles and to a smaller degree, bond lengths. Such networks do not possess long-range structural order. Zachariesen’s ideas were taken seriously much later starting in the 1960s, when comparisons to experiment showed that the idea had real promise. The next step was to use computers to help in making the models. An early computation was performed using a Monte Carlo approach. The idea was to put atoms inside a simulated box and move the atoms at random [40]. At each step the radial distribution function was computed and if a random move pushed the model closer to the experimental data, the move was kept, otherwise moves were retained with Metropolis probability. This is very similar in spirit to a current method, the so-called reverse Monte Carlo (RMC) method [8]. These approaches are information theoretic in spirit: use the available information to produce the model. While this is an eminently reasonable idea, the problem is that merely forcing agreement with diﬀraction data (pair correlations) grossly underconstrains the model: there are many conﬁgurations that agree beautifully with diﬀraction data but make no sense chemically or otherwise. In the 1980s, Wooten, Weaire and Winer (WWW) [9], introduced a Monte Carlo scheme for tetrahedral amorphous materials with special bondswitching moves, and energetics described by Keating springs and by requiring the network to be fourfold coordinated. They applied their method to a-Si and a-Ge with remarkable success. Here, the disorder of the real material was somehow captured by what appeared then to be a completely ad-hoc procedure. This method and improved versions of it are still the “gold standard” for creating models of amorphous Si. Years later, Barkema and Mousseau [11] showed that the likely reason for the success of the WWW scheme is that on long time-scales, the WWW moves occur quite naturally! Nowadays, the great majority of computer simulations are done using the molecular-dynamics method. The idea is to mimic the actual process of glass formation. To start with, one needs an interatomic potential that describes the interactions in the material. Typically, a well-equilibrated liquid is formed not far above the melting point, then the kinetic energy of the system is gradually reduced (by using some form of dissipative dynamics, such as velocity rescaling at each time step). Eventually there is structural arrest (the computer version of the glass transition), and a structural model results that may be useful for further study. Such calculations are often useful, but it needs to be clearly understood that there is little real similarity to the actual quenching process for glasses, which proceeds far more slowly in nature. As a ﬁnal oddity, the “melt-quench” approach is often used even for materials that do not form glasses (for example, a-Si). Results are especially poor for this case.

Defects in Amorphous Semiconductors: Amorphous Silicon

255

4.2 Interatomic Potentials To perform a molecular-dynamics simulation, or even a simulation of a mere relaxation of a network near a defect, it is necessary to compute the forces on the atoms in the material. This is never easy, and oﬀers a particular challenge in amorphous materials, as there are usually a variety of bonding environments in the network, and empirical potentials tend to be most accurate/reliable near conformations that were used in a ﬁtting process used to obtain them. The presence of defects exacerbates this further, as coordination or chemical order may be radically diﬀerent for the defect relative to the rest of the material (and thus harder to describe with a simple interatomic interaction). Also, the complexity of interatomic potentials grows rapidly with the number of distinct atomic species, so that even for binary systems, there are very few reliable empirical potentials available. The reason why it is diﬃcult to compute accurate interatomic potentials is that the interatomic forces are obtained from the electronic structure of the material. Thus, the details of bonding, electron hybridization, all depend in minute detail upon the local environment (coordination, bond lengths, bond angles, on the environment of the neighboring atoms and so on). The way out is to adopt an approach in which the electronic structure is directly computed in some approximate form. This has been done with some success using empirical tight-binding Hamiltonians [41, 42]. A tremendous advance for defects in semiconductors, but a particular beneﬁt for study of amorphous materials was the advent of practical densityfunctional codes. The union of density-functional methods and molecular-dynamics is now mature, and one can obtain excellent canned codes that can be used to undertake simulations of complex systems. Of course there is important background knowledge (of amorphous materials, electronic structure and simulation) needed. 4.3 Lore of Approximations in Density-Functional Calculations Defect calculations typically must be carried out using robust approximations for the Kohn–Sham states. The density-functional basis set upon which the Kohn–Sham orbitals are represented, and spin polarization are the main quantities that need to be considered. Where the basis set is concerned, the prime issue is completeness: the adequacy of the basis functions to approximate the “true” (complete basis limit) Kohn–Sham orbitals. Spin polarization is of particular importance in simulations if there are unpaired spins in the model (as for example a singly occupied dangling-bond state at the Fermi level). The choice of density-functionals is most important for an accurate estimate of energetics: the use of gradient approximations tends to ameliorate the tendency of LDA to overbind. One of the most important quantities for calculations involving defects is the positioning of defect energy levels, and also accurate estimates of the defect wavefunctions. DFT is in principle the wrong choice for either of these,

256

D.A. Drabold and T.A. Abtew

Fig. 2. GeSe2 density of electron states: comparison of experiment and theory (Gaussian-broadened Kohn–Sham eigenvalues) [43]. The Fermi-level is at zero for both curves

since it is formally only a ground-state theory, and also because only the charge density (that is, sum of the squares of the occupied Kohn–Sham orbitals) is formally meaningful within the derivation of the Kohn–Sham equations. However, it is clear that this viewpoint is unduly restrictive, and the density of Kohn–Sham eigenvalues is useful for comparing to the single-particle density of states as measured for example in photoemission (see Fig. 2 taken from [43]). The Kohn–Sham DOS systematically underestimates the optical gap (often by a factor of 2). Curiously, local basis function calculations with a limited (single-zeta) basis tend to give approximately the correct gap as the incompleteness of the basis tends to exaggerate the gap thus partly (and fortuitously) ﬁxing the underestimate intrinsic to the Kohn–Sham calculation. A proper job of describing these states requires methods beyond DFT. In this book, there are two relevant Chapters, that of Scheﬄer on the so-called “GW” methods (these provide self-energy corrections to DFT) and also the Chapter of Needs on quantum Monte Carlo. GW calculations of Blase and coworkers have shown that the Kohn–Sham orbitals tend to exaggerate the extent of localized states in crystalline systems; one should expect a similar eﬀect for amorphous systems. Unfortunately, the understanding of these points is only empirical at present.

Defects in Amorphous Semiconductors: Amorphous Silicon

257

4.4 The Electron–Lattice Interaction We have recently shown in some generality that localized electron states associated with defects exhibit a large coupling to the lattice [27]. Thus, for localized electronic eigenstates, deformations of the lattice in the vicinity of the localized state lead to signiﬁcant changes in the associated electronic eigenvalue. This eﬀect is easily tracked with ﬁrst-principles MD (in such an approach, Kohn–Sham eigenvectors are computed for each instantaneous ionic conﬁguration). Beside this empirical observation, it is possible to do a simple analysis of the vibration-induced changes in electron energies using the Hellmann–Feynman theorem [44] and exploiting the locality of the states to show that the electron–lattice coupling is roughly proportional to the localization (as gauged by the inverse participation ratio). Previous thermal simulations with Bohn–Oppenheimer dynamics have indicated that there exists a large electron–phonon coupling for the localized states in the band-tails and in the optical gap [45]. Earlier works on chalcogenide glasses by Cobb and Drabold [46] have emphasized a strong correlation between the thermal ﬂuctuations as gauged by root mean square (RMS) variation in the LDA eigenvalues and wavefunction localization of a gap or tail state (measured by the inverse participation ratio (2). Drabold and Fedders [24] have shown that localized eigenvectors may ﬂuctuate dramatically even at room temperature. Recently, Li and Drabold relaxed the adiabatic (Born–Oppenheimer) approximation to track the time development of electron packets scattered by lattice vibrations [45]. We have recently shown for localized electron states, that the electron–phonon coupling Ξn (ω) (coupling electron n and phonon ω) approximately satisﬁes: Ξn2 (ω) ∼ In × f (ω) ,

(4)

where f (ω) does not depend upon n, In is the IPR of electron state n. It is also the case that the thermally induced variance of electronic eigenvalue n, δλ2n ∝ In . It is remarkable that a simple correlation exists between a static property of the network (the IPR) and a dynamical feature of the system, the thermally induced ﬂuctuation in the Kohn–Sham energy eigenvalues. These predictions are easily veriﬁed from thermal simulation as reported elsewhere. The main assumption in obtaining this connection is that the electron states under study are localized. Beside the thermally induced changes in electronic energies, there are also signiﬁcant variations in the structure of the Kohn– Sham eigenstates, another consequence of the large electron–phonon coupling for localized states.

258

D.A. Drabold and T.A. Abtew

5 Defects in Amorphous Silicon Geometry/Topology Probably the most heavily studied amorphous semiconductor is Si. In its unhydrogenated form, the material is not electronically useful, as there are too many defect states in the optical gap. On the other hand, hydrogenated a-Si (a-Si:H) can be grown in a variety of ways, and can be prepared with defect concentrations of order 10−16 , which is small enough to enable many electronic applications [47]. Of critical importance for these applications, it is possible to dope a-Si:H n(p) type with P(B) donors (acceptors). The doping eﬃciency of the material is very low (meaning that large amounts – of order 1 % impurity is needed to move the Fermi level signiﬁcantly). In a-Si, diﬀraction measurements show that these materials are very tetrahedral (typically more than 99.9 % of atoms are four-coordinated) and have bond angles distributed around the tetrahedral angle (typically with a FWHM of order 10 degrees). The key defect is the threefold-coordinated Si atom, the sp3 dangling-bond, which is known on the basis of experiment and simulation to produce a midgap state. Such states are directly observable in electron spin resonance (ESR) measurements [48, 49]. Several papers have speculated on the importance of ﬁvefold ﬂoating bonds [50], but their signiﬁcance is still uncertain, and it appears that such defects would not produce midgap states, but rather states near the conduction-band edge. Depending upon the details of the local bonding environment, the levels associated with these states could move slightly from their ideal locations. Such conﬁgurations are popular in MD simulations of a-Si (quenches from the liquid). It is unclear, however, whether this implies the existence of ﬂoating bonds in a-Si:H or if there is an overemphasis on higher-coordinated sites because the liquid is roughly 6-fold coordinated. Defects play many roles in a-Si:H, and one of the most interesting defect-dependent properties is associated with light-induced metastability, the “Staebler–Wronski” eﬀect [51], which is usually interpreted as lightinduced creation of defect centers (probably dangling-bonds). A remarkable collection of experiments and models have been undertaken to understand this eﬀect that is obviously important for photovoltaic applications, but for thin-ﬁlm device applications (like thin-ﬁlm transistors) as well [52–65]. This eﬀect is addressed in the Chapter of Simdayankin and Elliott. Level of Approximations: A Cautionary Tale We have undertaken a systematic study of the level of calculation needed to faithfully represent the electron states, total energies and forces in a-Si within the density-functional LDA approximations. This work was performed with the powerful local basis code SIESTA [66]. This calculation was carried out for a-Si:H, but we expect that many of the conclusions should at least be

Defects in Amorphous Semiconductors: Amorphous Silicon

259

considered when applying density-functional techniques to other amorphous or glassy materials. In fact studies analogous to ours for silicon should be implemented for more complex amorphous materials. For a unique “one-stop reference” to methodological issues for density-functional methods, see the book of Martin [67]. In a nutshell, a proper calculation of defect states and geometry, especially in amorphous materials, is diﬃcult. Every approximation needs to be checked and optimized. Depending upon the type of question being asked more or less sophisticated approximations may be required. We divide the discussion into several categories: (1) Pseudopotentials: One of the most important and fortunately reliable approximations used in electronic-structure calculations is the pseudopotential. This is a means to separate the atomic core and valence regions, and enables the use of only valence electrons in the calculation of the Kohn–Sham orbitals. Even for a relatively light atom like Si, this allows a calculation involving 4 electrons per atom rather than 14. When one reﬂects that mere diagonalization of the Hamiltonian scales as the cube of the number of electrons, the payoﬀ is clear. After many years of work, the lore of pseudopotentials is fairly mature, though one must test a new potential carefully before using it widely. (2) Basis Set: The most obvious approximation in any large-scale DF calculation is the use of a ﬁnite basis set to represent a set of continuous functions (the Kohn–Sham orbitals and the charge density). In a planewave calculation, it is easy to check for completeness, as the only “knob” is the plane-wave cutoﬀ (or number of reciprocal lattice vectors). Care is needed with plane-wave calculations as defect states can be quite spatially compact and therefore diﬃcult to approximate without a large collection of reciprocal lattice vectors. For local basis codes, ab initio or empirical, completeness is a delicate question. Most current codes use basis orbitals much in the spirit of the linear combination of atomic orbitals (LCAO) method of chemistry, with s, p, d, f states. The minimal basis is deﬁned to be a set of atom-centered functions that is just adequate to represent the occupied atomic orbitals on that atom. The minimal basis has very limited variational freedom. The ﬁrst improvement on the minimal basis is introducing two functions with the symmetry of the original single-zeta (SZ) functions. Quantum chemists call this a “double-zeta” (DZ) basis. A suitably selected doublezeta basis can reproduce expansion and contraction in local bonding. The zeta proliferation can continue, though it is uncommon to proceed beyond triple-zeta in practical calculations. After adequately ﬁlling out the basis orbitals with the symmetries of the states for the ground-state atom, one proceeds to the next shell of states that are unoccupied in the atomic ground-state. These are called polarization functions (so named because the loss of symmetry caused by application of a (polarizing)

260

D.A. Drabold and T.A. Abtew

electric ﬁeld distorts the ground-state functions into the next angular momentum shell). In a-Si:H we ﬁnd that the choice of basis aﬀects virtually everything. The localization of the Kohn–Sham states depends dramatically on the basis. As one might guess, the less complete basis sets tend to overestimate the localization of the Kohn–Sham eigenvectors (as there are fewer channels for these states to admix into). What was surprising is that the degree of localization, measured by IPR for a well-isolated dangling-bond defect, varies by a factor of two between a single-zeta (four orbitals per site) and a double-zeta polarized (DZP) (thirteen orbitals per site) basis. Similar eﬀects are seen for defects in crystals. Since the single-particle density matrix, the total energy and interatomic forces depend upon the Kohn– Sham eigenvectors, it is to be expected that defect geometry, vibrational frequencies and dynamical properties are all inﬂuenced by the choice of basis. (3) Spin Polarization: Fedders and coworkers [68] have shown that, in order to correlate the degree of localization from dangling-bond states with ESR experiments, it is not enough to look at the wavefunctions, but to the net spin polarization near the danglin-bond. The reason is that the spin density includes contributions from electronic states other than the localized defect wavefunction, which contribute to make the spin polarization more localized than the speciﬁc localized state wavefunction. In order to conﬁrm this result (obtained by Fedders et al. on cells of aSi:H) in our structural models, we performed calculations allowing for spin polarization in our frozen lattice models, using the DZP basis set. We were not able to ﬁnd a spin-polarized solution for any of the amorphous cells. The reason is the existence of two interacting dangling-bonds, which favors the formation of a spin singlet with two electrons paired. In order to force the appearance of a spin moment in our models, we introduce an unpaired spin by removing a single electron from the system. We ﬁnd a contribution of almost 50 % to net spin by the central dangling-bond and its neighbors (the central atom alone contributing 38 %). However, the Mulliken charge contribution to the wavefunction of the corresponding localized state from the defect site is only 0.29e. The hydrogen-terminated dangling-bond sites also contribute about 10 % of the net spin. The remainder is somewhat distributed uniformly at the other sites. For well-isolated dangling-bonds in a-Si, about 54 % of the net spin-localization sits on the dangling-bond and its nearest neighbors, in reasonable agreement with the experiment [49, 69]. The conclusion is that, for a dangling-bond defect state, there is a large diﬀerence between spin localization and wavefunction localization. The degree of spin localization is greater than that of the wavefunction localization at the dangling-bond site. To our knowledge, no experimental methods exist for measuring the extent of wavefunction localization on the dangling-bond orbital as opposed to spin.

Defects in Amorphous Semiconductors: Amorphous Silicon

261

(4) Gradient-Corrected Density-Functional: This has been inadequately studied, although there is no reason to expect large changes in structure with the use of gradient corrections. Typically, bond lengths may change modestly and cohesive energies improve when compared to experiment. Generally one expects gradient corrections to at least partly repair the tendency of LDA to overbind. (5) Brillouin-Zone Sampling: Many current calculations of defects are carried out with a cell that is then periodically repeated to eliminate surface eﬀects. In particular, this construction clearly yields a crystal with a unit cell with typically several hundred or more atoms (such a number is necessary to meaningfully sample the disorder characteristic of the material). Thus, the use of periodic (Born–Von-Karman) boundary conditions really amounts to consideration of a crystal with a large unit cell. Thus, there is a new (and completely artiﬁcial) band-structure (k dispersion) associated with the construction, a Brillouin-zone, etc. It is of course true that as the cell gets larger, the bands become ﬂatter, thus reducing the signiﬁcance of the periodicity. For computational convenience, total energies and forces are inevitably computed at the center (k = 0) of the Brillouin-zone, though in principle these quantities involve quadrature over the ﬁrst Brillouin-zone. However, if results for total energies and especially forces depend upon k in any signiﬁcant way, then it is doubtful that the cell was selected to be large enough in the ﬁrst place. For delicate energetics (an all too familiar state of aﬀairs for defects), it is particularly important to test that the cell is big enough. In our experience a few hundred atoms in a cubic cell is adequate. Defect Identiﬁcation From simulation studies, one ﬁnds the expected point defects of coordination type (threefold dangling-bonds and ﬁvefold atoms ﬂoating bonds), and also strain defects (nominally four-coordinated structures with large deviations in the bond angles). The dangling-bond defect produces electronic states near the middle of the gap, and ﬂoating bonds near the conduction edge. Strain defects are associated with the valence- and conduction-band tails. Defect Dynamics and Diﬀusion An important, but underappreciated aspect of defects in amorphous semiconductors, is their dynamics. In hydrogenated amorphous silicon, the motion of defects and the motion of hydrogen (which are evidently related) are correlated with some of the most important physical properties of the amorphous matrix, such as the light-induced degradation of the material (Staebler–Wronski eﬀect) [51, 70]. The expectation is that H motion consists of small oscillations in a particular potential well associated with a given local environment with rare escape events until the diﬀusing particle falls into

262

D.A. Drabold and T.A. Abtew

Fig. 3. Trajectory for two diﬀerent hydrogen atoms, showing diﬀusion and trapping between silicon bond centers in a 223 atom model of hydrogenated amorphous silicon. The simulation time is 10.0 ps and the temperature is 300 K. ‘Light-oﬀ’ implies that the dynamics are in the electronic ground state

another trap. The time between such rare events depends upon the height of the barrier separating the two metastable conﬁgurations. Sophisticated methods exist for determining diﬀusion pathways and events, particularly the activation-relaxation technique (ART) of Barkema and Mousseau [71]. In a remarkable paper, these authors applied ART with a simple potential to directly compute the atomic “moves” in a model of a-Si. For large barriers and very rare events, there is no substitute for a study of “ART” type. For smaller barriers, we have seen that it is possible to extract interesting short-time diﬀusive dynamics directly from MD simulation. In simulations of Ag dynamics in chalcogenide glass hosts, we found that it was not diﬃcult to track the motion of the Ag atoms from simulations of order 50 ps. The existence of trapping centers, and even some information about trap geometry, and temperature-dependent residence times was obtained [72]. In a-Si:H, we have found that an analogous computation produces new insight into the motion of both Si and H atoms. Using a small cell (61 Si and 10 H atoms) with two dangling-bonds and no other defects, we employed SIESTA with high-level approximations (a double-zeta polarized basis) to monitor atomic motion. On the time-scale of 1 ps we have shown the trajectory of one of the H atoms in Fig. 3 [73]. Representative of the majority of H atoms in the cell, this particular trajectory shows the diﬀusion of the hydrogen atom, including trapping. While the H atoms are diﬀusing in the cell it is followed by breaking old bonds and forming new bonds. We have plotted the time evolution of undercoordinated and ﬂoating bonds formed as a consequence of hydrogen diﬀusion in Fig. 4 [73].

Defects in Amorphous Semiconductors: Amorphous Silicon

263

Fig. 4. (a) Total number of undercoordinated atoms and (b) Total number of overcoordinated atoms in our simulation at T = 300 K. The total time for the graph is 1.0 ps

Fig. 5. Time evolution of coordination for a few selected atoms (H-69, H-65, Si-24, and Si-51) at room temperature T = 300 K. (a) time evolution of atoms, Si-24 which is far from the diﬀusing H with coordination 4 and H-69. (b) time evolution of selected atoms: Si-51, which is close to the diﬀusing H, and H-65

In our simulation we have observed rearrangements of the atoms while the hydrogen atoms are diﬀusing in the cell. The diﬀusion of H causes formation and breaking of bonds. We have also observed the formation of metastable states that trap the mobile hydrogen atoms. The mechanisms for the formation of these structures follow breaking of H atoms from the Si–H bonds and followed by diﬀusion in the cell. These mobile H atoms then collide with another Si+DB structure and form a bond. These processes continue until two hydrogens form a bond to a single Si atom or to two nearby Si atoms to form a metastable conformation. In Fig. 5, [73] we have shown the time evolution of the coordination for selected atoms. Figure 5a shows the stable coordination of a Si atom (Si-24) that is fully coordinated since there is no

264

D.A. Drabold and T.A. Abtew

diﬀusing atom in its vicinity and of H-69 that has an average coordination of 1. However, the Si atom (Si-51) and H-65, which are shown in Fig. 5b, shows change in the coordination as a function of time. This change in the coordination becomes more stable (1 for H and 4 for Si) after the formation of a metastable conﬁguration. Our results suggest that atoms that are reasonably far from the diﬀusing hydrogen have an average coordination of 4 for Si and 1 for H. However, the coordination of the atoms, for instance Si-51, in the direction of the diﬀusing H atoms changes with time. This suggests that while the H atoms are diﬀusing in the cell there is breaking and formation of bonds. Other researchers have emphasized the signiﬁcance of defect and H motion. In particular, Street [74] has pioneered a phenomenological approach to the long-time dynamics with the defect-pool model. Our work on extremely short timescales should ultimately be smoothly connected to the inferred long-time defect dynamics from the defect-equilibria models. While we are very far from this goal at present, it is possible to imagine impacts of both approaches on each other within a few years. Ideally, the short-time simulations could provide ab-initio input into the energetics of the dynamics, and even information about residence times for various defects. Acknowledgements It is a pleasure to thank a number of collaborators for their contributions to the work reported here: R. Atta-Fynn, P. Biswas, J. Dong, S. R. Elliott, P. A. Fedders, H. Jain, J. Li, J. Ludlam, N. Mousseau, P. Ordej´ on, S. N. Taraskin and X. Zhang. We acknowledge the support of the National Science Foundation under NSF-DMR 0600073, 0605890 and the Army Research Oﬃce under MURI W911NF-06-2-0026.

References [1] C. R. A. Catlow (Ed.): Defects and Disorder in Crystalline and Amorphous Solids, vol. 418 (Kluwer, Netherlands 1994) 245 [2] J. D. Joannopoulos, G. Lucovsky (Eds.): The Physics of Hydrogenated Amorphous Silicon II, vol. 56 (Springer, Berlin, Heidelberg 1984) 245 [3] M. Stutzmann, D. K. Biegelsen, R. A. Street: Phy. Rev. B 35, 5666 (1987) 245 [4] E. T. Jaynes: Probability Theory: The Logic of Science (Cambridge University Press, Cambridge 2003) 246 [5] R. Car, M. Parrinello: Phy. Rev. Lett. 60, 204 (1988) 247 [6] O. Gereben, L. Pusztai: Phys. Rev. B 50, 14136 (1994) 247 [7] J. K. Walters, R. J. Newport: Phys. Rev. B 53, 2405 (1996) 247 [8] R. L. McGreevy: J. Phys.: Condens. Matter 13, R877 (2001) 247, 254 [9] F. Wooten, K. Winer, D. Weaire: Phy. Rev. Lett. 54, 1392 (1985) 247, 254

Defects in Amorphous Semiconductors: Amorphous Silicon

265

[10] B. R. Djordjevic, M. F. Thorpe, F. Wooten: Phys. Rev. B 52, 5685 (1995) 247, 252 [11] G. T. Barkema, N. Mousseau: Phy. Rev. B 62, 4985 (2000) 247, 254 [12] R. L. C. Vink, G. T. Barkema: Phys. Rev. B 67, 245201 (2003) 247 [13] M. F. Thorpe: J. Non-Cryst. Solids 57, 355 (1983) 247 [14] A. E. Carlsson: Solid State Physics, Advances in Research and Applications, vol. 43 (Academic, New York 1990) p. 1 247 [15] F. Ercolessi, J. B. Adams: Europhys. Lett. 26, 583 (1994) 247 [16] A. Nakano, L. Bi, R. K. Kalia, P. Vashishta: Phys. Rev. B 49, 9441 (1994) 247 [17] J. J. Ludlam, S. N. Taraskin, S. R. Elliott, D. A. Drabold: J. Phys.: Condens. Matter 17, L321 (2005) 247, 248, 251 [18] S. Aljishi, L. Ley, J. D. Cohen: Phys. Rev. Lett. 64, 2811 (1990) 247 [19] D. A. Drabold, P. A. Fedders, S. Klemm, O. F. Sankey: Phys. Rev. Lett. 67, 2179 (1991) 247, 249 [20] S. R. Elliott: Physics of Amorphous Materials, 2nd ed. (Longman Scientiﬁc, London; New York 1990) 248, 253 [21] R. Zallen: The Physics of Amorphous Solids (Wiley-Interscience, New York 1998) 248 [22] J. Dong, D. A. Drabold: Phys. Rev. Lett. 80, 1928 (1998) 250, 251, 252 [23] P. A. Fedders, D. A. Drabold, S. Nakhmanson: Phys. Rev. B 58, 15624 (1998) 250 [24] D. A. Drabold, P. A. Fedders: Phys. Rev. B 60, R721 (1999) 250, 257 [25] D. A. Drabold: J. Non-Cryst. Solids 269, 211 (2000) 250 [26] R. A. Street, J. Kakalios, T. M. Hayes: Phys. Rev. B 34, 3030 (1986) 250 [27] R. Atta-Fynn, P. Biswas, P. Ordej´ on, D. A. Drabold: Phys. Rev. B 69, 085207 (2004) 252, 257 [28] N. Szabo, N. S. Ostlund: Modern Quantum Chemistry (Dover, New York 1996) 252 [29] S. N. Taraskin, D. A. Drabold, S. R. Elliott: Phys. Rev. Lett. 88, 196405 (2002) 252 [30] X. Zhang, D. A. Drabold: Phys. Rev. Lett. 83, 5042 (1999) 253 [31] M. Cobb, D. A. Drabold, R. L. Cappelletti: Phys. Rev. B 54, 12162 (1996) 253 [32] C. Massobrio, A. Pasquarello, R. Car: Phys. Rev. Lett. 80, 2342 (1998) 253 [33] I. Petri, P. S. Salmon, H. E. Fischer: Phys. Rev. Lett. 84, 2413 (2000) 253 [34] X. Zhang, D. A. Drabold: Phys. Rev. B 62, 15 695 (2000) 253 [35] P. S. Salmon, I. Petri, J. Phys.: Condens. Matter 15, S1509 (2003) 253 [36] D. A. Drabold, J. Li, D. Tafen: J. Phys.: Condens. Matter 15, S1529 (2003) 253 [37] D. N. Tafen, D. A. Drabold: Phys. Rev. B 68, 165208 (2003) 253 [38] M. F. Thorpe, D. J. Jacobs, B. R. Djordjevic: The structure and rigidity of network glasses, in P. Boolchand (Ed.): Insulating and Semiconducting Glasses (World Scientiﬁc, Singapore 2000) p. 95 253 [39] W. H. Zachariasen: J. Am. Chem. Soc. 54, 3841 (1932) 253 [40] R. Kaplow, T. A. Rowe, B. L. Averbach: Phys. Rev. 168, 1068 (1968) 254 [41] A. P. Sutton, M. W. Finnis, D. G. Pettifor, Y. Ohta: J. Phys. C: Solid State Phys. 21, 35 (1988) 255 [42] N. Bernstein, E. Kaxiras: Phys. Rev. B 56, 10488 (1997) 255

266 [43] [44] [45] [46] [47] [48] [49] [50] [51] [52] [53] [54] [55] [56] [57] [58] [59] [60] [61] [62] [63] [64] [65] [66] [67] [68] [69] [70] [71] [72] [73] [74]

D.A. Drabold and T.A. Abtew P. Biswas, D. N. Tafen, D. A. Drabold: Phys. Rev. B 71, 054204 (2005) 256 R. P. Feynman: Phys. Rev. 56, 340 (1939) 257 J. Li, D. A. Drabold: Phys. Rev. B 68, 033103 (2003) 257 M. Cobb, D. A. Drabold: Phys. Rev. B 56, 3054 (1997) 257 J. D. Joannopoulos, G. Lucovsky (Eds.): The Physics of Hydrogenated Amorphous Silicon I, vol. 55 (Springer, Berlin, Heidelberg 1984) 258 R. A. Street, D. K. Biegelsen, J. C. Knights: Phys. Rev. B 24, 969 (1981) 258 D. K. Biegelsen, M. Stutzmann: Phys. Rev. B 33, 3006 (1986) 258, 260 S. T. Pantelides: Phys. Rev. Lett. 57, 2979 (1986) 258 D. L. Staebler, C. R. Wronski: Appl. Phys. Lett. 31, 292 (1977) 258, 261 H. Fritzsche: Annu. Rev. Mater. Res. 31, 47 (2001) 258 T. Su, P. C. Taylor, G. Ganguly, D. E. Carlson: Phys. Rev. Lett. 89, 015502 (2002) 258 S. B. Zhang, W. B. Jackson, D. J. Chadi: Phys. Rev. Lett. 65, 2575 (1990) 258 D. J. Chadi: Appl. Phys. Lett. 83, 3710 (2003) 258 M. Stutzmann, W. B. Jackson, C. C. Tsai: Phys. Rev. B 32, 23 (1985) 258 R. Biswas, I. Kwon, C. M. Soukoulis: Phys. Rev. B 44, 3403 (1991) 258 S. Zafar, E. A. Schiﬀ: Phys. Rev. B 40, 5235 (1989) 258 S. Zafar, E. A. Schiﬀ: Phys. Rev. Lett. 66, 1493 (1991) 258 S. Zafar, E. A. Schiﬀ: J. Non-Cryst. Solids 138, 323 (1991) 258 H. M. Branz: Phys. Rev. B 59, 5498 (1999) 258 R. Biswas, Y.-P. Li: Phys. Rev. Lett. 82, 2512 (1999) 258 N. Kopidakis, E. A. Schiﬀ: J. Non-Cryst. Solids 269, 415 (2000) 258 S. B. Zhang, H. M. Branz: Phys. Rev. Lett. 87, 105503 (2001) 258 T. A. Abtew, D. A. Drabold, P. C. Taylor: Appl. Phys. Lett. 86, 241916 (2005) 258 J. M. Soler, E. Artacho, J. D. Gale, A. Garcia, J. Junquera, P. Ordej´ on, D. Sanch´ez-Portal: J. Phys.: Condens. Matter 14, 2745 (2002) 258 R. M. Martin: Electronic Structure: Basic Theory and Practical Methods (Cambridge University Press, Cambridge 2004) 259 P. A. Fedders, D. A. Drabold, P. Ordej´ on, G. Fabricius, E. Artacho, D. Sanchez-Portal, J. Soler: Phys. Rev. B 60, 10594 (1999) 260 T. Umeda, S. Yamasaki, J. Isoya, et al.: Phys. Rev. B 59, 4849 (1999) 260 T. A. Abtew, D. A. Drabold: J. Phys.: Condens. Matter 18, L1 (2006) 261 N. Mousseau, G. T. Barkema: Phys. Rev. E 57, 2419 (1998) 262 D. N. Tafen, D. A. Drabold, M. Mitkova: phys. stat. sol. (b) 242, R55 (2005) 262 T. A. Abtew, D. A. Drabold: Phys. Rev. B 74, 085201 (2006) 262, 263 R. A. Street: Hydrogenated Amorphous Silicon (Cambridge University Press, Cambridge 1991) 264

Index a-Si, 245–247, 249, 250, 252–254, 258, 260, 262

ab-initio, 247, 249, 250, 259, 264 acceptor, 258

Defects in Amorphous Semiconductors: Amorphous Silicon adiabatic, 257 amorphous, 245–256, 258–261 Anderson, 251 band edge, 247, 249, 258 band-structure, 250, 261 band-tail, 247, 249, 250, 257, 261 bandwidth, 246 basis set, 255, 259, 260 Bloch, 250 bond order, 249 Born–Oppenheimer, 257 Born–von-Karman, 261 Bragg, 246 Brillouin-zone, 261 chalcogen, 253 chalcogenide, 247, 252, 257, 262 cohesive energy, 261 concentration, 250, 258 conduction, 247, 261 conduction-band, 251, 258, 261 conformation, 250, 255, 263 coordination, 247–249, 255, 261, 263, 264 core, 259 Coulomb, 252 coupling, 257 crystal momentum, 247, 250 cutoﬀ, 249, 259 dangling-bond, 249, 253, 255, 258, 260–262 decay, 246, 247, 251, 252 delocalized, 251, 252 density matrix, 249, 252, 260 density of states, 247, 256 DFT, 255, 256 diamond, 253 diﬀusion, 262, 263 disorder, 245, 247–251, 254, 261 dispersion, 261 distortion, 246, 250, 252 donor, 258 doping, 258 double-zeta, 259, 260, 262 DZ, 259 DZP, 260 eigenstates, 249, 251, 257

267

eigenvalues, 249, 256, 257 eigenvectors, 247, 251, 257, 260 electron, 252, 253, 259, 260 electron spin resonance, 258 electron states, 247, 250, 257, 258 electron–phonon, 257 empirical, 247, 250, 255–257, 259 energetics, 252, 254, 255, 261, 264 energy level, 255 entropy, 246, 251 equilibrium, 249, 250 ESR, 253, 258, 260 Fermi level, 247, 249, 253, 255, 258 ﬁrst-principles, 247, 250, 257 ﬂoating bond, 258, 261, 262 ﬂuctuation, 249, 257 force, 247, 255, 258, 260, 261 fourfold, 252–254 Fourier, 246 gap, 249, 252 Ge, 247, 253, 254 general gradient approximation, 255 glass, 246, 253, 254, 257, 262 grain, 253 ground-state, 256, 259, 260 GW, 256 Hamiltonian, 247, 250–253, 255, 259 Hellmann–Feynman, 257 hopping, 251 Hubbard, 253 hybrid, 247, 255 hydrogen, 260–264 impurity, 258 IPR, 251, 252, 257, 260 Kohn–Sham, 249, 255–257, 259, 260 LDA, 255, 257, 258, 261 liquid, 254, 258 localization, 249, 251, 257, 260 melting, 254 metastablity, 258 Metropolis, 254 midgap, 251, 258

268

D.A. Drabold and T.A. Abtew

minimal basis, 259 mobility, 251 molecular-dynamics, 247, 254, 255 Mulliken, 251, 260 neutron diﬀraction, 246 optical, 247, 249, 252, 256–258 pair-correlation function, 246, 249, 254 periodic, 250, 261 periodic boundary conditions, 261 periodicity, 261 phonon, 257 photoemission, 247, 256 photovoltaic, 246, 258 plane-wave, 259 point defect, 261 polarization, 255, 259, 260 potential, 247, 250, 252, 254, 255, 259, 261, 262 pseudopotential, 259

self-energy, 256 Si, 245–247, 249, 250, 252–254, 258–260, 262–264 SIESTA, 258, 262 silicon, 245, 259, 261 spin, 252, 253, 255, 258, 260 Staebler–Wronski, 258, 261 strain, 247, 261 stress, 247 structure factor, 246 surface, 250, 261 symmetry, 259 temperature, 247, 249, 250, 257, 262 tetrahedral, 252–254, 258 thermal disorder, 247, 249 thermal equilibrium, 249 tight-binding, 247, 250, 255 total energy, 247, 252, 260 trajectory, 262 transition, 246, 251, 254 transport, 245

quantum Monte Carlo, 256 variational, 259 radial-distribution function, 246, 254 real space, 246 relaxation, 253, 255, 262 resonance, 258 reversible, 246, 250

Wannier, 252 wavelength, 246 X-ray, 246

Light Induced Eﬀects in Amorphous and Glassy Solids S. I. Simdyankin and S. R. Elliott Department of Chemistry, University of Cambridge, Lensﬁeld Road, Cambridge CB2 1EW, United Kingdom {sis24,sre1}@cam.ac.uk Abstract. In this Chapter, we discuss how exposure to light can aﬀect the properties of disordered materials and review our recent computational studies of these phenomena. Familiarity with the preceding contribution by Drabold and Abtew is beneﬁcial for understanding this Chapter.

1 Photoinduced Metastability in Amorphous Solids: An Experimental Survey 1.1 Introduction Electromagnetic (EM) radiation can interact with amorphous solids in a number of ways, depending on the wavelength of the radiation. EM radiation can be either absorbed or scattered by a solid. In the resonant process of absorption, the photon energy must match a transition energy between two quantum states in the material, e.g., for atomic vibrations corresponding to infrared (IR) wavelengths, or electronic transitions from valence to conduction band across a bandgap in a semiconductor, corresponding to visible/near ultraviolet (UV) wavelengths (depending on the magnitude of the bandgap energy, Eg ). Scattering of EM radiation may be elastic, or inelastic when energy is exchanged between a photon and quantum states of a solid. Examples include X-ray scattering (diﬀraction) from the electrons in atoms, Raman (inelastic light) scattering from atomic vibrations (e.g. molecular-like modes) and Brillouin (inelastic light) scattering from acoustic phonon-like vibrational excitations. The photon–solid interaction can be interrogated in terms of either the ultimate state of the photon (as in the above examples), or in terms of changes in the internal state of the solid. In the latter case, it is often changes in the electronic degrees of freedom that are probed: for the case of most amorphous semiconductors with bandgaps in the range 1 eV < Eg < 3 eV, this involves near-IR or visible-light excitation (although for more ionic oxides, e.g., vitreous (v-)SiO2 with Eg ≈ 10 eV, UV-light excitation is required). Electrons optically excited into the conduction band (CB), or holes excited into the valence band (VB), can be probed, for example, by their enhanced electrical transport (photoconductivity) or by their radiative recombination D. A. Drabold, S. K. Estreicher (Eds.): Theory of Defects in Semiconductors, Topics Appl. Physics 104, 269–286 (2007) © Springer-Verlag Berlin Heidelberg 2007

270

S. I. Simdyankin and S. R. Elliott

(photoluminescence or ﬂuorescence). At suﬃciently high light intensities, the light–solid interaction can become nonlinear, this optical nonlinearity permitting many new phenomena, such as second-harmonic generation, three- and four-wave mixing, to occur. Electronic excitation of structural coordination defects, e.g., dangling bonds, can be probed by electron spin (paramagnetic) resonance (ES(P)R). The optically induced phenomena outlined above can be exhibited by all kinds of semiconducting/insulating solid, whether crystalline or amorphous. However, certain features unique to the amorphous state in general, and to certain types of amorphous materials in particular, mean that some photoinduced phenomena are special to amorphous semiconducting materials, particularly those that are metastable, i.e., which remain after cessation of irradiation. One general characteristic of amorphous semiconductors of relevance in this connection is the occurrence of disorder-induced spatial localization of electronic states in the band-tail states extending into the gap between the VB and CB [1]. The presence of continuous bands of localized states in these tail states, in the energy interval between the “mobility” edges in the VB and CB, marking the transition point between localized and delocalized (extended) electron states [2], as well as localized states deep in the bandgap arising from coordination defects [1], can have a profound inﬂuence on the nature of the photon–solid interaction. These localized states have an enhanced electron–lattice interaction (see the preceding Chapter by Drabold and Abtew ), meaning that optical excitation of such electronic states can have a disproportionate eﬀect on the surrounding atomic structure. Secondly, the radiative-recombination lifetime for an optically created electron–hole pair trapped in localized tail states can be very considerably longer than when the photoexcited carriers are in extended states (as is always the case for crystals), thereby allowing possible nonradiative channels to become signiﬁcant (e.g., involving atomic-structural reconﬁguration). Other relevant aspects are more materials speciﬁc. Optically induced metastability associated with structural reorganization is likely to be more prevalent in those materials in which (some) atoms have a low degree of nearest-neighbor connectivity (e.g., being twofold coordinated, rather than fourfold coordinated), thereby imparting a considerable degree of local structural ﬂexibility. In addition, structural reorganization following optically induced electronic excitation is more probable if the (VB) electronic states involved correspond to easily broken weak bonds. One class of materials satisfying the above constraints consists of chalcogenide glasses, namely alloys of the Gp-VI chalcogen elements (S, Se, Te) with other (metalloid) elements, e.g., B, Ga, P, As, Sb, Si, Ge, etc. These materials are “lone-pair” semiconductors in which (if the chalcogen content is suﬃciently high) the top of the VB comprises chalcogen p-π lone-pair (LP) states [3]. Interatomic, “nonbonding” (Van der Waals-like) interactions involving such LP states are appreciably weaker than for normal covalent

Light Induced Eﬀects in Amorphous and Glassy Solids

271

bonds (those states lying deeper in the VB). Since the ground-state electronic conﬁguration of chalcogen atoms is s2 p4 , the occurrence of nonbonding LP electron states means that each chalcogen atom is ideally twofold coordinated by covalent bonds to its nearest neighbors. Thus, chalcogenide glasses, having a combination of localized electronic tail states, low atomic coordination and weak bonds associated with optically accessible states at the top of the VB, are ideal candidates for exhibiting photoinduced eﬀects. 1.2 Photoinduced Eﬀects in Chalcogenide Glasses Amorphous chalcogenide materials exhibit a plethora of photoinduced phenomena. Such changes can be variously dynamic (i.e., present only whilst a material is illuminated) or metastable (i.e., the eﬀects remain after cessation of illumination). Furthermore, the changes may be either scalar or vectoral in nature (respectively, independent or dependent on either the polarization state, or the propagation direction, of the inducing light). Finally, metastable changes may be irreversible, or reversible with respect to thermal or optical annealing. Examples of dynamic eﬀects are the afore-mentioned phenomena of photoluminescence and photoconductivity [1] and optical nonlinearity [4], which are common to all materials. (Chalcogenide glasses generally exhibit extremely large optical nonlinearities because of the highly electronically polarizable nature of chalcogen atoms present [4].) However, a (scalar) dynamic eﬀect, which is characteristic of chalcogenide glasses, is photoinduced ﬂuidity, wherein the viscosity of a glass (e.g. As2 S3 ) decreases on illumination with subbandgap light or, in other words, light can cause viscous relaxation in a stressed glass [5, 6]. An example of a vectoral dynamic photoeﬀect in chalcogenide glasses is the optomechanical eﬀect [7, 8], wherein linearly polarized light incident on a chalcogenide-coated clamped microcantilever causes it to displace upwards or downwards, depending on whether the polarization axis is, respectively, parallel or perpendicular to the cantilever axis, as a result of anisotropic photoinduced strains introduced into the chalcogenide–cantilever bimorph. Metastable photoinduced changes are perhaps the most interesting (and applicable) of the eﬀects observed in chalcogenide glasses. One such is photodarkening (or bleaching), wherein the optical absorption edge of the material shifts to lower energies (hence the material gets darker at a given wavelength), or to higher energies (bleaching), on illumination with (sub-) bandgap light. For reviews, see [9, 10]. Arsenic-based materials with higher sulfur contents and germanium sulﬁde materials seem to favor photobleaching, for reasons that are not clear at present. Irreversible shifts of the optical absorption edge occur in virgin (as-evaporated) thin ﬁlms of amorphous chalcogenides containing structurally unstable molecular fragments from the vapor phase [11] that are particularly vulnerable to photoinduced (or thermal) change. Reversible photodarkening is observed in bulk glasses and well-annealed thin

272

S. I. Simdyankin and S. R. Elliott

ﬁlms: optical illumination causes a redshift of the absorption edge, whilst subsequent thermal annealing to the glass-transition temperature, Tg , erases the eﬀect [9, 10]. Photodarkening (bleaching) appears to be associated with photoinduced structural changes, such microscopic changes being manifested as macroscopic volume changes. Photocontraction is particularly prevalent in virgin obliquely deposited thin ﬁlms of amorphous chalcogenides having a columnarlike microstructure [12], but photoexpansion is commonly associated with photodarkening in chalcogenide bulk glasses or thin ﬁlms [9, 10]. Giant photoexpansion (up to 5 % expansion) occurs for subbandgap illumination [13]. Another metastable photoinduced structural change exhibited by chalcogenide materials is photoinduced crystallization and amorphization, as used in rewriteable “phase-change” CDs and DVDs [14, 15]. The amorphization process there is believed to result from a photoinduced melting and subsequent very rapid quenching of the material to the glassy state. However, illumination of certain crystalline chalcogenide materials (e.g., As50 Se50 ) can also cause athermal photoamorphization [16]. Light can also cause “chemical” changes in chalcogenide glasses. For example, overlayers of certain metals (notably silver) diﬀuse into the undoped bulk glass on illumination [17, 18]. On the other hand, Ag-containing chalcogenide glasses, rich in Ag, exhibit the opposite eﬀect, namely photoinduced surface deposition, wherein the metal exsolves from the glassy matrix on illumination [19, 20]. A particularly interesting metastable vectoral photoinduced eﬀect exhibited by chalcogenide glasses is photoinduced optical anisotropy (POA), ﬁrst observed in [21], and manifested in absorption, reﬂection (i.e., refractive index) and scattering (for a review, see [10, 22]). Illumination of an initially optically isotropic glass by linearly polarized light causes the material to become dichroic and birefringent. In the case of well-annealed thin ﬁlms and bulk glasses, the eﬀect is completely reversible optically (i.e., the induced optical axis is fully rotated when the light-polarization vector is rotated), and the POA can be annealed out thermally (but at a lower temperature than is the case for scalar photodarkening) or optically (using unpolarized or circularly polarized light).

2 Theoretical Studies of Photoinduced Excitations in Amorphous Materials From the above very brief review, it is apparent that amorphous chalcogenide materials exhibit a wide range of interesting photoinduced phenomena. Although the experimental phenomenology is, for the most part, well developed, a proper theoretical understanding is still lacking. Until very recently, theoretical models have been conﬁned to “hand-waving” models [9,10], involving simple notions of chemical bonding and the eﬀects of light (e.g., bond breaking and defect formation). However, the predictive, and even descriptive, power

Light Induced Eﬀects in Amorphous and Glassy Solids

273

of such approaches is very limited, and for a microscopic (atomic-level) understanding of photoinduced phenomena in amorphous chalcogenides, proper quantum-mechanical calculations need to be performed. Obviously, this is an extremely challenging task, and two essentially opposing methods for making progress in this regard, using diﬀerent approximations, can be employed. The ﬁrst employs all-electron quantum-chemical calculations on small clusters (a few tens) of atoms, in which the optimized electronic and atomic conﬁgurations and energies are found for the ground and electronically excited states (see, e.g. [23–26]). This favors accuracy over dynamics. The other method, (discussed in the Chapter by Drabold and Abtew ), namely ab-initio molecular-dynamics (MD) simulations, takes a converse approach: atomic dynamics are followed at the expense of accuracy. More detail will be given in the following, but the advantages and disadvantages of these two approaches can be summarized as follows. Quantum-chemical methods can only deal with very small clusters (particularly for excited-state calculations) and only initial (ground-state) and ﬁnal (excited-state) conﬁgurations can be studied, not the intermediate dynamics, but the energetics are the most accurate. Ab-initio MD, on the other hand, provides full information about atomic dynamics, but only over very short timescales (typically a few picoseconds) and for relatively few atoms (typically less than a hundred). In order to make the calculations involved tractable, numerous more-or-less severe approximations need to be invoked (e.g., the local-density approximation (LDA) in density-functional theory (DFT)), which make certain results imprecise (e.g., underestimation of the bandgap). Moreover, the Kohn–Sham (KS) orbitals resulting from DFT are ground-state quantities and hence formally inadmissible for a consideration of excited-state behavior. Nevertheless, use of these theoretical methods has provided very useful atomistic information of help in understanding photoinduced phenomena in chalcogenide glasses. Some justiﬁcation for using both occupied and virtual KS orbitals for qualitative, and sometimes partially quantitative, analysis of electronic structure is provided by comparing the shape and symmetry properties, as well as the energy order, of these orbitals with those obtained by wavefunction-based (e.g., at the Hartree–Fock level of theory [27]) and GW [28] calculations. There is a very strong similarity between GW and LDA states, and often identical DFT and GW quasiparticle wavefunctions are assumed in practical calculations [29]. 2.1 Application of the Density-Functional-Based Tight-Binding Method to the Case of Amorphous As2 S3 One approximate ab-initio-based MD scheme that has proved very useful in understanding the electronic behavior of chalcogenide glasses is the densityfunctional-based tight-binding (DFTB) method developed by Frauenheim and coworkers. Although this is reported in [30–32], since this approach is not described elsewhere in this book, we give here a brief description of this

274

S. I. Simdyankin and S. R. Elliott

method and review our recent results on the canonical chalcogenide glass a-As2 S3 obtained by using the DFTB method [33–35]. Although the DFTB method is semiempirical, it allows one to improve upon the standard tight-binding description of interatomic interactions by including a DFT-based self-consistent second order in charge ﬂuctuation (SCC) correction to the total energy [31]. The ﬂexibility in choosing the desired accuracy while computing the interatomic forces brings about the possibility to perform much faster calculations when high precision is not required, and reﬁne the result if needed. As described in [36], the SCC-DFTB model is derived from densityfunctional theory (DFT) by a second-order expansion of the DFT total energy functional with respect to the charge-density ﬂuctuations δn = δn(r ) around a given reference density n0 = n0 (r ): E=

occ i

ˆ 0 |ψi ψi |H

δ 2 Exc 1 + (1) δn δn |r − r | δn δn n0 n0 n0 1 + E − [n ] − Vxc [n0 ]n0 + Eii , xc 0 2 |r − r | ˆ0 = where dr and dr are expressed by and , respectively. Here, H ˆ 0 ] is the eﬀective Kohn–Sham Hamiltonian evaluated at the reference H[n density and the ψi are Kohn–Sham orbitals. Exc and Vxc are the exchangecorrelation energy and potential, respectively, and Eii is the core–core repulsion energy. To derive the total energy of the SCC-DFTB method, the energy contributions in (1) are further subjected to the following approximations: 1. The ˆ 0 |ψi are represented in a basis of conHamiltonian matrix elements ψi |H ﬁned, pseudoatomic orbitals φµ , ψi = ciµ φµ . (2) 1 + 2

µ

To determine the basis functions φµ , the atomic DFT problem is solved by adding an additional harmonic potential ( rr0 )2 to conﬁne the basis func0 , are tions [30]. The Hamiltonian matrix elements in this LCAO basis, Hµν 0 then calculated as follows. The diagonal elements Hµµ are taken to be the 0 are calculated in a atomic eigenvalues and the nondiagonal elements Hµν two-center approximation: 0 Hµν = φµ |Tˆ + veﬀ [n0α + n0β ]|φν µα, νβ,

(3)

which are tabulated, together with the overlap matrix elements Sµν with respect to the interatomic distance Rαβ . veﬀ is the eﬀective Kohn–Sham potential and n0α are the densities of the neutral atoms α.

Light Induced Eﬀects in Amorphous and Glassy Solids

275

2. The charge-density ﬂuctuations δn are written as a superposition of atomic contributions δnα , δn = δnα , (4) α

which are approximated by the charge ﬂuctuations at the atoms α, ∆qα = qα − qα0 . qα0 is the number of electrons of the neutral atom α and the qα are determined from a Mulliken-charge analysis. The second derivative of the total energy in (1) is approximated by a function γαβ , whose functional form for α = β is determined analytically from the Coulomb interaction of two spherical charge distributions, located at Rα and Rβ . For α = β, it represents the electron–electron self-interaction on atom α. 3. The remaining terms in (1), Eii and the energy contributions, which depend on n0 only, are collected in a single energy contribution Erep . Erep is then approximated as a sum of short-range repulsive potentials, U [Rαβ ], (5) Erep = α=β

which depend on the interatomic distances Rαβ . With these deﬁnitions and approximations, the SCC-DFTB total energy ﬁnally reads: Etot =

iµν

0 ciµ ciν Hµν +

1 γαβ ∆qα ∆qβ + Erep . 2

(6)

αβ

Applying the variational principle to the energy functional (6), one obtains the corresponding Kohn–Sham equations: cνi (Hµν − i Sµν ) = 0, ∀ µ, i (7) ν

1 Hµν = φµ |H0 |φν + Sµν (γαζ + γβζ )∆qζ , 2

(8)

ζ

which have to be solved iteratively for the wavefunction expansion coeﬃcients ciµ , since the Hamiltonian matrix elements depend on the ciµ due to the Mulliken charges. Analytic ﬁrst derivatives for the calculation of interatomic forces are readily obtained, and second derivatives of the energy with respect to atomic positions are calculated numerically. The repulsive pair potentials U [Rαβ ] are constructed by subtracting the DFT total energy from the SCC-DFTB electronic energy (ﬁrst two terms on the right-hand side of (6)) with respect to the bond distance Rαβ for a small set of suitable reference systems. To summarize, in order to determine the appropriate parameters for a new element, the following steps have to be taken. First, DFT calculations have to be performed for the neutral atom to determine the LCAO basis functions φµ

276

S. I. Simdyankin and S. R. Elliott

and the reference densities n0α . Here the conﬁnement radius can, in principle, be chosen to be diﬀerent for the density (r0n ) and each type of atomic orbital (r0s,p,d ). The value of r0 is usually taken to be the same for s- and p-functions. In a minimal basis, this yields a total number of two adjustable parameters for elements in the ﬁrst and second rows, while there are three if d-functions are included. After this, the diﬀerent matrix elements can be calculated and the pair potentials U [Rαβ ] are obtained as stated above for every combination of the new element with the ones already parameterized. The single-particle KS occupied, ψi , and unoccupied, ψj , orbitals and the corresponding KS excitation energies ωij = j − i are sometimes used for qualitative analysis of electronic excitations. Although the KS excitation energies can be considered as an approximation to true excitation energies ωI [37] (see also end of the introduction to Sect. 2), the correction terms to this approximation can be very signiﬁcant in many cases. Modeling electronic excitations by varying the occupation of the KS orbitals results in mixed quantum states with undeﬁned contributions from singlet and triplet states. We have performed modeling of electronic excitations at the level of KS orbitals and energies and have attempted to validate the results by using more exact methods. One such method is based on time-dependent densityfunctional response theory (TD-DFRT) [38, 39], where the true excitation energies are found by solving the following eigenvalue problem: √ √ 2 I I [ωij δik δjl δστ + 2 ωij Kijσ,klτ ωkl ]Fijσ = ωI2 Fklτ . (9) ijσ

Here σ and τ are spin indices. The indices i, k correspond to occupied, and j, l to unoccupied, KS orbitals, respectively. The coupling matrix K is deﬁned as (see [40] for a more detailed description of the method): 1 δ 2 Exc + Kijσ,klτ = ψi (r)ψj (r) (10) ψk (r )ψl (r ), |r − r | δnσ δnτ where we use a notation consistent with that in (2). Our structural models of a-As2 S3 were obtained by a “melt-and-quench” procedure [35] similar to the one described in the preceding Chapter by Drabold and Abtew. The structural quality of models can be assessed by examining the radial-distribution function (RDF) and the structure factor (see Fig. 1). Apart from general good agreement with experimental data, an interesting feature revealed by Fig. 1a is the shape of the ﬁrst peak of the RDF. The shoulders on both sides of this peak indicate the presence of homopolar (As–As or S–S) bonds in the material. Such bonds (chemical defects), as well as coordination (or topological) defects, are easily detectable in computer models. An example of a conﬁguration featuring an As–As bond is shown in Fig. 2. Special signiﬁcance can be attributed to the presence of ﬁve-membered rings in models with an appreciable concentration of homopolar bonds (models with all-heteropolar bonds contain only an even number of

Light Induced Eﬀects in Amorphous and Glassy Solids

277

Fig. 1. (a) Pair-correlation functions for a 200-atom model of a-As2 S3 and the neutron-diﬀraction experiment [41]. (b) Reduced structure factors (interference functions) for the same model and experiment

atoms in all rings). When such rings share some of the bonds, the resulting local structure is close to that of cage-like molecules (e.g., As4 S4 ), as found in the vapor phase and in some chalcogenide molecular crystals. Figure 2a shows two such bond-sharing rings. Upon breaking the two bonds connecting the rings to the rest of the network, the distance between the two freed arsenic atoms (connected by a dashed line in Fig. 2a) could be reduced, thus producing another As–As homopolar bond and this group of atoms would then form an As4 S4 molecule (shown in Fig. 2b). Evidence of the presence of such molecules in bulk Asx S1−x glasses from Raman-scattering experiments

278

S. I. Simdyankin and S. R. Elliott

Fig. 2. (a) Fragment of a 200-atom model of a-As2 S3 : two bond-sharing ﬁvemembered rings and the two AsS3 groups connected to this structure. The dangling bonds show where the displayed conﬁguration connects to the rest of the amorphous network. The dashed line connects two As atoms, which, if brought nearer together, would close up to form an As4 S4 molecule shown in panel (b). The shading of the As atoms (all with three neighbors) is darker than that of the S atoms (all with two neighbors)

has recently been reported in [42]. Our result shows that the As4 S4 fragments may not only form discrete cage-like molecules but also may be embedded into the amorphous network. We veriﬁed that the vibrational signatures of the As4 S4 fragment from models 1 and 2 are similar to those from an isolated As4 S4 molecule, apart from a few very symmetric modes of the latter. The observed tendency for formation of quasimolecular structural groups suggests that amorphous chalcogenides can be viewed as nanostructured materials. Localization of the electronic states near the optical bandgap edges is of great interest for studies of photoinduced phenomena. The inverse participation ratios (IPR, deﬁned in the Chapter by Drabold and Abtew ) for a model of a-As2 S3 are shown in Fig. 3. The general picture is that, at the top of the valence band, the eigenstates are predominantly localized at what can be called sulfur-rich regions, where several sulfur atoms are closer than about 3.45 ˚ A, i.e., their interatomic distances are on the low-r side of the second peak in g(r) shown in Fig. 1a or some of these atoms form homopolar S–S bonds. For instance, most of the HOMO (highest occupied molecular orbital) level in this model is localized at two sulfur atoms separated by 3.42 ˚ A and which are part of the molecule-like fragment depicted in Fig. 2a. By inspecting the projected (local) IPRs in Fig. 3b at the optical gap edges, it is seen that the IPRs are greatest for the S atoms. It appears that the localization at the top of the valence band is facilitated by the proximity of the lone-pair p orbitals in the sulfur-rich regions. This observation is consistent with a result for a-GeS2 [44].

Light Induced Eﬀects in Amorphous and Glassy Solids

279

Fig. 3. Local and total electronic density of states (a) and inverse participation ratios (b) for a 200-atom model of a-As2 S3 . The Fermi energy is at the energy origin. The experimental data in (a) are obtained from [43]

At the bottom of the conduction band, the states tend to localize at various anomalous local conﬁgurations, such as four-membered rings, S–S homopolar bonds (some of these bonds are in ﬁve-membered rings) and valencealternation pairs (coordination defects). For example, the LUMO (lowest unoccupied molecular orbital) state for the structure depicted in Figs. 5a,b is localized on an overcoordinated S atom (with three bonded neighbors). We found that a basis set of s, p and d Slater-type orbitals for all atoms is an essential prerequisite for the observation of overcoordinated defects [36,45].

280

S. I. Simdyankin and S. R. Elliott

(a)

(b)

(c)

Fig. 4. Planar trigonal, [S3 ]+ (marked by the letter “A”), and “seesaw”, [As4 ]− (marked by letter “E”), conﬁgurations in (a) a fragment of a 60-atom model of a-As2 S3 (the dangling bonds show where the displayed conﬁguration connects to the rest (not shown) of the network) and, (b) and (c), charged isolated clusters (the dangling bonds are terminated with hydrogen atoms). The shading of the atoms is the same as in Fig. 2

It is possible to analyze individual contributions of orbitals of each type to the total EDOS and IPR, and these contributions are shown in Fig. 3. As mentioned above, in the context of photoinduced metastability, a great deal of signiﬁcance is attributed to the presence of topological and/or chemical defects [9]. It is therefore imperative to create models both with and without such defects in a theoretical investigation that attempts to be conclusive. Defect-free models can be produced by “surgical” manipulations. For example, atoms with undesired coordination can be removed from the model, and, in order to eliminate chemical defects, one can iteratively apply the following algorithm. First, a sulfur atom is inserted in the middle of each As–As homopolar bond. Second, each S–S bond is replaced by a single sulfur atom located at its midpoint so that each local As–S–S–As conﬁguration is turned into As–S–As. Third, the distance between each newly introduced S atom and its two nearest arsenic atoms in the newly created As–S–As units is reduced in order to increase the bonding character of the As–S bonds stretched by the above manipulation. Fourth, the modiﬁed conﬁguration is relaxed in an MD run. We have found that only a few iterations can be suﬃcient in order to obtain models with all-heteropolar (As–S) bonds.

Light Induced Eﬀects in Amorphous and Glassy Solids

(a)

(c)

(b)

(d)

281

Fig. 5. An As4 S10 H8 cluster containing both defect centers [As4 ]− (marked by letter “A”) and [S3 ]+ (“B”). The shading of the atoms is the same as in Fig. 2. The black solid lines signify elongated bonds. (a) Optimized ground-state geometry. Bond lengths are (˚ A): AC = 3.00, AD = 2.32, and BE = 2.4. (b) Isosurfaces corresponding to the value of 0.025 of electron density in the HOMO (darker red surface) and LUMO (lighter cyan surface) states for the structure shown in (a). (c) Optimized geometry in the ﬁrst singlet excited state. Bond lengths are (˚ A): AC = 2.43, AD = 2.44, and BE = 2.82. (d) Same as (b), but for the structure shown in (c)

Elimination of the defects in our models removes some electronic states in the optical bandgap. As a result, the bandgap broadens, which can be viewed as an artiﬁcial bleaching of the material. The states at the band edges, however, are still localized due to disorder. It is possible that exposure to light may lead to bond breaking and defect creation even in such “all-heteropolar” models. Indeed, As–S bond elongation/breaking has been observed in allheteropolar clusters [23,24] and cage-like molecules (unpublished). Such bond breaking under irradiation can lead to the creation of self-trapped excitons (STEs), i.e., oppositely charged defect pairs, as shown in [29] for silicon dioxide where, following Si–O bond breaking, the hole is localized at the oxygen defect center and the electron at the silicon defect center. In analogy with the case of SiO2 , it is possible that positively charged chalcogen defects and negatively charged nonchalcogen defects are introduced in amorphous chalcogenides by a similar mechanism. In the As–S system, such STEs can possibly lead to creation of the [As4 ]− –[S3 ]+ defect pairs described below.

282

S. I. Simdyankin and S. R. Elliott

These defects, as well as those that are always present in real materials and “as-prepared” models, may mediate local structural rearrangements upon photon absorption. Creation of additional states at optical bandgap edges (photodarkening) of a-As2 S3 exposed to light has long been attributed to the generation by illumination of defects in excess of the thermal equilibrium concentration [9], but the exact mechanism of defect creation and the nature of the defects are still enigmatic. Possible candidate defect types, notably valence-alternation pairs, have been proposed over the years [9]. Normally, such defect pairs contain singly coordinated chalcogen atoms having distinct spectroscopic signatures [46]. Experimentally, the concentration of these defects is estimated to be rather small [47], i.e., 1017 cm−3 , compared with the atomic density of about 2 × 1025 cm−3 , in order quantitatively to account for the observed magnitude of the photoinduced eﬀects. In our simulations, in addition to the charged coordination defects previously proposed to exist in chalcogenide glasses, a novel defect pair, [As4 ]− – [S3 ]+ (see Fig. 4), consisting of a fourfold coordinated arsenic site in a “seesaw” conﬁguration and a threefold coordinated sulfur site in a near-planar trigonal conﬁguration, was found in several models [33]. Such defect pairs are unusual in two ways. First, there is an excess of negative charge in the vicinity of the normally electropositive pnictogen (As) atoms and, second, there are no undercoordinated atoms with dangling bonds in these local conﬁgurations. The latter peculiarity may be why such defect pairs have not yet been identiﬁed experimentally. These defect pairs, however, are consistent with the STEs described above. Although electronic excitations, where one electron is promoted from HOMO to LUMO Kohn–Sham states [48], are not especially realistic, we simulate such excitations in order qualitatively to assess defect stability with respect to (optically induced) electronic excitations. In some models, [S3 ]+ – − + S− 1 defect pairs are converted into [As4 ] –[S3 ] pairs as a result of the electronic excitation. The presence of these defect pairs introduces additional localized states at the optical bandgap edges with energies quantitatively consistent with the phenomenon of photodarkening [34]. − A possible mechanism of conversion of [S3 ]+ –S− 1 defect pairs into [As4 ] – + [S3 ] pairs is illustrated in Fig. 5, which shows an As4 S10 H8 cluster containing an [S3 ]+ –S− 1 pair in the ground state. Geometry optimization in the ﬁrst singlet excited state within the linear-response approximation to time-dependent (TD) density-functional theory (which gives a much better description of excited states compared with HOMO-to-LUMO electron excitations [40]) leads to a redistribution of electron density, so that the singly coordinated S atoms become attached to a normally coordinated As atom, thus forming an [As4 ]− defect. At the same time, the [S3 ]+ defect breaks up (we observed that bond breaking/elongation in all our models generally occurs at the groups of atoms where the LUMO is localized, indicating the expected antibonding character of LUMO states.). Perhaps in bulk materials similar rearangements can lead to the creation of an [S3 ]+ center at a diﬀer-

Light Induced Eﬀects in Amorphous and Glassy Solids

283

ent location, which is suggested by the observation that, in our simulations of photoexcitations in supercell models, the [S3 ]+ centers after excitation are not necessarily located at the same S atom as before the excitation.

References [1] S. R. Elliott: Physics of Amorphous Materials, 2nd ed. (Longman Scientiﬁc and Technical, London 1990) 270, 271 [2] J. J. Ludlam, S. N. Taraskin, S. R. Elliott: J. Phys. Condens. Matter 17, L321 (2005) 270 [3] S. R. Elliott: Chalcogenide glasses, in J. Zarzycki (Ed.): Materials Science and Technology, vol. 9 (VCH, Weinheim 1991) p. 375 270 [4] A. Zakery, S. R. Elliott: J. Non-Cryst. Solids 330, 1 (2003) 271 [5] H. Hisakuni, K. Tanaka: Science 270, 974 (1995) 271 [6] S. N. Yannopoulos: Photo-plastic eﬀects in chalcogenide glasses: Raman scattering studies., in A. V. Kolobov (Ed.): Photo-Induced Metastability in Amorphous Semiconductors (Wiley-VCH, Weinheim 2003) p. 119 271 [7] P. Krecmer, A. M. Moulin, T. Rayment, R. J. Stephenson, T. Rayment, M. E. Welland, S. R. Elliott: Science 277, 1799 (1997) 271 [8] M. Stuchlik, S. R. Elliott: Proc. IEE A: Science, Measurement and Technology 151, 131 (2004) 271 [9] A. V. Kolobov (Ed.): Photo-Induced Metastability in Amorphous Semiconductors (Wiley-VCH, Weinheim 2003) 271, 272, 280, 282 [10] K. Shimakawa, A. Kolobov, S. R. Elliott: Adv. Phys. 44, 475 (1995) 271, 272 [11] S. A. Solin, G. V. Papatheodorou: Phys. Rev. B 15, 2084 (1977) 271 [12] S. Rajagopalan, K. S. Harshavardhan, L. K. Malhotra, K. L. Chopra: J. NonCryst. Solids 50, 29 (1982) 272 [13] H. Hisakuni, K. Tanaka: Appl. Phys. Lett. 65, 2925 (1994) 272 [14] S. R. Ovshinsky: Phys. Rev. Lett. 21, 1450 (1968) 272 [15] T. Ohta, S. R. Ovshinsky: Phase-change optical storage media., in A. V. Kolobov (Ed.): Photo-Induced Metastability in Amorphous Semiconductors (Wiley-VCH, Weinheim 2003) p. 310 272 [16] S. R. Elliott, A. V. Kolobov: J. Non-Cryst. Solids 128, 216 (1991) 272 [17] A. Kolobov, S. R. Elliott: Adv. Phys. 40, 625 (1991) 272 [18] T. Wagner, M. Frumar: Optically-induced diﬀusion and dissolution in metals in amorphous chalcogenides., in A. V. Kolobov (Ed.): Photo-Induced Metastability in Amorphous Semiconductors (Wiley-VCH, Weinheim 2003) p. 160 272 [19] S. Maruno, T. Kawaguchi: J. Appl. Phys. 46, 5312 (1975) 272 [20] T. Kawaguchi: Photo-induced deposition of silver particles on amorphous semiconductors., in A. V. Kolobov (Ed.): Photo-Induced Metastability in Amorphous Semiconductors (Wiley-VCH, Weinheim 2003) p. 182 272 [21] V. G. Zhdanov, V. K. Malinovskii: Sov. Tech. Phys. Lett. 3, 943 (1977) 272 [22] V. M. Lyubin, M. L. Klebanov: Photo-induced anisotropy in chalcogenide glassy semiconductors., in A. V. Kolobov (Ed.): Photo-Induced Metastability in Amorphous Semiconductors (Wiley-VCH, Weinheim 2003) p. 91 272 [23] T. Uchino, D. C. Clary, S. R. Elliott: Phys. Rev. Lett. 85, 3305 (2000) 273, 281

284

S. I. Simdyankin and S. R. Elliott

[24] T. Uchino, D. C. Clary, S. R. Elliott: Phys. Rev. B 65, 174204 (2002) 273, 281 [25] T. Uchino, S. R. Elliott: Phys. Rev. B 67, 174201 (2003) 273 [26] T. Mowrer, G. Lucovsky, L. S. Sremaniak, J. L. Whitten: J. Non-Cryst. Solids 338, 543 (2004) 273 [27] R. Stowasser, R. Hoﬀman: J. Am. Chem. Soc. 121, 3414 (1999) 273 [28] M. S. Hybertsen, S. G. Louie: Phys. Rev. B 34, 5390 (1986) 273 [29] S. Ismail-Beigi, S. G. Louie: Phys. Rev. Lett. 95, 156401 (2005) 273, 281 [30] D. Porezag, T. Frauenheim, T. K¨ ohler, G. Seifert, R. Kaschner: Phys. Rev. B 51, 12947 (1995) 273, 274 [31] M. Elstner, D. Porezag, G. Jungnickel, J. Elstner, M. Haugk, T. Frauenheim, S. Suhai, G. Seifert: Phys. Rev. B 58, 7260 (1998) 273, 274 [32] T. Frauenheim, G. Seifert, M. Elstner, T. Niehaus, C. K¨ ohler, M. Amkreutz, M. Sternberg, Z. Hajnal, A. Di Carlo, S. Suhai: J. Phys. Condens. Matter 14, 3015 (2002) 273 [33] S. I. Simdyankin, T. A. Niehaus, G. Natarajan, T. Frauenheim, S. R. Elliott: Phys. Rev. Lett. 94, 086401 (2005) 274, 282 [34] S. I. Simdyankin, M. Elstner, T. A. Niehaus, T. Frauenheim, S. R. Elliott: Phys. Rev. B 72, 020202 (2005) 274, 282 [35] S. I. Simdyankin, S. R. Elliott, Z. Hajnal, T. A. Niehaus, T. Frauenheim: Phys. Rev. B 69, 144202 (2004) 274, 276 [36] T. A. Niehaus, M. Elstner, T. Frauenheim, S. Suhai: J. Mol. Struct. THEOCHEM 541, 185 (2001) 274, 279 [37] A. G¨ orling: Phys. Rev. A 54, 3912 (1996) 276 [38] M. E. Casida: Recent Advances in Density Functional Methods, Part I (World Scientiﬁc, Singapore 1995) p. 155 276 [39] M. E. Casida: Developments and applications of modern density functional theory, in J. M. Seminario (Ed.): Theoretical and Computational Chemistry, vol. 4 (Elsevier Science, Amsterdam 1996) p. 391 276 [40] T. A. Niehaus, S. Suhai, F. Della Sala, P. Lugli, M. Elstner, G. Seifert, T. Frauenheim: Phys. Rev. B 63, 085108 (2001) 276, 282 [41] J. H. Lee, A. C. Hannon, S. R. Elliott: eprint: cond-mat/0402587 277 [42] D. G. Georgiev, P. Boolchand, K. A. Jackson: Philos. Mag. 83, 2941 (2003) 278 [43] S. G. Bishop, N. J. Shevchik: Phys. Rev. B 12, 1567 (1975) 279 [44] S. Blaineau, P. Jund: Phys. Rev. B 70, 184210 (2004) 278 [45] S. I. Simdyankin, S. R. Elliott, T. A. Niehaus, T. Frauenheim: Eﬀect of defects in amorphous chalcogenides on the atomic structure and localisation of electronic eigenstates, in P. Vincenzini, A. Lami, F. Zerbetto (Eds.): Computational Modeling and Simulation of Materials III, vol. A (Techna Group s.r.l., Faenza 2004) p. 149 279 [46] M. Kastner, D. Adler, H. Fritzsche: Phys. Rev. Lett. 37, 1504 (1976) 282 [47] A. Feltz: Amorphous Inorganic Materials and Glasses (VCH, Weinheim 1993) p. 203 282 [48] X. Zhang, D. A. Drabold: Phys. Rev. Lett. 83, 5042 (1999) 282

Light Induced Eﬀects in Amorphous and Glassy Solids

Index a-As2 S3 , 274, 276, 278, 282 ab-initio, 273 absorption, 269, 271, 272, 282 algorithm, 280 all-electron, 273 amorphous, 269–273, 278, 281 anisotropy, 271, 272 annealing, 271, 272 As4 S4 , 277, 278 band edge, 281 basis set, 279 Brillouin scattering, 269 bulk, 271, 272, 277, 282 canonical, 274 chalcogen, 270, 271, 281, 282 chalcogenide, 270–274, 277, 278, 281, 282 cluster, 273, 279, 281, 282 concentration, 276, 282 conduction band, 269, 270, 279 coordination, 270, 271, 276, 279, 280, 282 core, 274 Coulomb, 275 coupling, 276 covalent, 270, 271

excitation, 269, 270, 276, 282, 283 excited state, 273, 282 exciton, 281 ﬂuctuation, 274, 275 force, 274, 275 fourfold, 270, 282 gap, 269 Ge, 270 germanium, 271 glass, 270–274, 277, 282 ground state, 271, 273, 282 GW, 273 Hamiltonian, 274, 275 Hartree–Fock, 273 hole, 269, 270, 281 HOMO, 278, 282 IPR, 280 irreversible, 271 Kohn–Sham, 273–275, 282 LCAO, 275 LDA, 273 localization, 270, 278 LUMO, 279, 282

dangling bond, 270, 282 delocalized, 270 density-functional theory, 273, 274, 276 DFT, 273–275 DFTB, 273–275 disorder, 269, 270, 281

metastability, 280 minimal basis, 276 molecular-dynamics, 273 Mulliken, 275

eigenstates, 278, 284 eigenvalues, 274 electromagnetic radiation, 269 electron, 269, 275 electron spin resonance, 270 electron states, 270 embedded, 278 energetics, 273 equilibrium, 282 exchange, 269 exchange-correlation, 274

phonon, 269 photoconductivity, 269, 271 photodarkening, 271, 272, 282 photoexpansion, 272 photoluminescence, 270, 271 pnictogen, 282 polarization, 271, 272 potential, 274–276 pseudoatom, 274

optical, 270–272, 278, 282 oxygen, 281

quasiparticle, 273

285

286

S. I. Simdyankin and S. R. Elliott

radial-distribution function, 276 radiative, 269, 270 Raman, 269, 277 recombination, 269, 270 relaxation, 271 repulsive, 275 resonance, 270 resonant, 269 reversible, 271, 272 scalar, 271, 272 scattering, 269, 272, 277 self-interaction, 275 self-trapped, 281 semiempirical, 274 Si, 269, 270, 281 silicon, 281 Slater, 279 spin, 270, 276 strain, 271 stress, 271 supercell, 283

surface, 272 symmetric, 278 symmetry, 273 temperature, 272 thermal equilibrium, 282 tight binding, 273, 274 time-dependent density-functional theory (TDDFT), 282 total energy, 274, 275 transition, 269, 270, 272 transport, 269 trigonal, 282 valence band, 269–271, 278 Van der Waals, 270 variational, 275 vectoral, 271, 272 wavelength, 269, 271 X-ray, 269

Index

Γ point, 34, 52, 58 a-As2 S3 , 274, 276, 278, 282 a-Si, 131, 245–247, 249, 250, 252–254, 258, 260, 262 ab initio, 16, 21, 101 ab-initio, 215, 216, 233, 247, 249, 250, 259, 264, 273 absorption, 13, 44, 49, 95, 157, 230, 231, 269, 271, 272, 282 acceptor, 34, 40, 57, 59–61, 69, 71, 81, 83, 84, 86–88, 90, 258 adatom, 230 adiabatic, 119–122, 124, 130, 134, 257 AIMPRO, 16, 58, 59, 71, 72, 75, 76, 80, 81, 84, 87, 88 algorithm, 43, 44, 61, 74, 143–145, 147, 203, 204, 217, 229, 280 alignment, 35, 49, 50, 55, 57, 176, 177, 234–236 all-electron, 41, 55, 72, 76, 273 amorphous, 1, 2, 6, 9, 22, 23, 43, 130, 131, 230, 245–256, 258–261, 269–273, 278, 281 Anderson, 251 anharmonic, 48, 102, 118, 125, 126, 128, 196, 222 anion vacancy, 166, 179–182, 184–187 anisotropy, 271, 272 annealing, 12, 13, 60, 95, 194, 233, 235, 236, 271, 272 antisite, 12, 168 As4 S4 , 277, 278 asymmetric, 99, 101, 166, 179, 180, 182, 183, 185, 186, 201 atomic-sphere approximation, 35, 55 autocorrelation function, 48, 224 backﬂow, 146, 147

background charge, 35, 53, 58, 70, 159 band bending, 166 band edge, 12, 13, 30, 35, 40, 49, 50, 55, 59, 84, 173, 178, 184, 247, 249, 258, 281 band structure, 14, 15, 38, 41, 58, 79, 166, 167, 169, 170, 172–177, 216, 235 band-structure, 250, 261 band-tail, 247, 249, 250, 257, 261 bandwidth, 34, 246 basis set, 14–16, 21, 22, 32, 34, 39, 42, 43, 47, 58, 61, 69, 71–80, 96, 103, 130, 158, 214, 255, 259, 260, 279 Berendsen, 132, 221 Bethe–Salpeter, 39 Bloch, 14, 71, 250 Bohr, 13 Boltzmann, 104, 116, 219, 224 bond order, 216, 222, 223, 228–230, 249 bond-centered, 14, 16, 21, 74, 99–101, 106, 195 bond-order potential, 214, 215, 217, 223, 227, 230, 235 Born–Oppenheimer, 17, 42, 43, 214, 257 Born–von-Karman, 15, 261 boron, 81, 84, 87, 107, 108, 206 Bragg, 246 Brillouin scattering, 269 Brillouin zone, 2, 34, 35, 38, 51, 52, 84, 89, 103, 176–178, 181, 182 Brillouin-zone, 148, 261 bulk, 36, 41, 47, 49, 50, 52, 55, 58, 74, 76, 79, 84, 86, 90, 127, 165, 171, 173, 174, 176–178, 187, 198, 271, 272, 277, 282 bulk modulus, 76, 77, 79, 223

288

Index

canonical, 43, 116–118, 120–122, 220, 224, 225, 274 Car, 21, 130 carbide, 195 carbon, 80, 87, 132–134 chalcogen, 84, 85, 90, 253, 270, 271, 281, 282 chalcogenide, 247, 252, 257, 262, 270–274, 277, 278, 281, 282 charge delocalization, 39 charge state, 14, 30, 34, 38, 46–50, 52, 55, 57, 60, 70, 80, 81, 86, 107, 167, 170, 179, 180, 182–187 charge-transition level, 165–167, 170, 171, 184–187 charge-transition state, 169, 172, 173, 184, 186, 187 charged defect, 15, 35, 53–58, 158 chemical potential, 36, 49–51, 55, 80, 184, 220 classical, 19, 20, 53, 54, 101, 106, 116, 120, 160, 195, 196, 198–200, 202–204, 206, 208, 210, 213, 216, 218, 219 Clausius–Clapeyron, 123–125, 132–134 cleavage, 168, 176 cluster, 2, 12, 15, 16, 32, 33, 35, 36, 55, 56, 70, 71, 80, 81, 84, 87, 89, 127, 142, 147, 194, 223, 273, 279, 281, 282 cohesive energy, 150, 218, 223, 227, 228, 261 complex, 12, 15, 81, 84–86, 100, 105–110, 194, 195 concentration, 11, 13, 36, 48, 69, 104–110, 115, 125, 127, 153, 154, 159, 220, 250, 258, 276, 282 concerted exchange, 154–156 conduction, 247, 261 conduction band, 12, 35, 38, 40, 50, 51, 79, 105, 176, 178, 184, 269, 270, 279 conduction-band, 251, 258, 261 conductivity, 11, 30, 49, 69 conﬁgurational entropy, 106, 108–110, 131 conformation, 81, 250, 255, 263 conjugate gradient, 75, 107, 214, 215 conservative, 217, 220

coordination, 142, 179, 247–249, 255, 261, 263, 264, 270, 271, 276, 279, 280, 282 core, 16, 35, 37, 41, 55, 58, 59, 71, 72, 96, 195, 259, 274 core radius, 41 core-valence, 37, 41 core-valence interaction, 167, 174, 182 correlation, 15, 16, 19, 31, 32, 37–40, 61, 86, 97, 130, 142, 145–147, 150, 156, 157, 167, 169–172, 177, 180, 224 Coulomb, 18, 35, 39, 40, 46, 53, 55, 56, 58, 146, 148, 217, 218, 222, 252, 275 coupling, 46, 48, 56, 58, 118, 157, 205, 225, 231, 236, 257, 276 covalent, 15, 35, 78, 129, 196, 199, 208, 223, 234, 270, 271 crack, 128, 196, 197, 208, 225 crystal momentum, 247, 250 cusp, 146 cutoﬀ, 36, 42, 58, 97, 217, 228, 249, 259 cyclic cluster, 15 Czochralski, 14 dangling bond, 15, 56, 176, 177, 179, 196, 199, 270, 282 dangling-bond, 157, 249, 253, 255, 258, 260–262 decay, 18, 57, 96, 98, 100, 101, 144, 172, 195, 217, 246, 247, 251, 252 deep level, 12, 13, 34, 61, 69, 71, 84, 87 deep-level transient spectroscopy, 13, 29 defect band, 34, 35 defect engineering, 11 defect state, 180 degeneracy, 30, 44–46, 56, 228 delocalization, 39 delocalized, 13, 39, 52, 54, 251, 252, 270 density matrix, 228, 229, 249, 252, 260 density of states, 17, 18, 37, 48, 95, 102, 103, 166, 227, 229, 247, 256 density-functional theory, 16, 19–22, 30, 31, 44, 60, 69, 96, 105, 128, 130, 142, 165–168, 170–172, 178, 179, 182, 184–187, 198, 214, 273, 274, 276

Index DFT, 22, 30–33, 36–38, 40, 42, 45, 47, 50, 58, 69–71, 82, 86, 89, 130, 142, 146, 148, 151–157, 159, 160, 198, 214, 216, 222, 223, 227, 230, 235, 255, 256, 273–275 DFTB, 206, 273–275 diamond, 16, 40, 46, 52, 54, 56, 70, 78, 79, 81, 83, 84, 87, 88, 122, 133–135, 141, 146, 157, 158, 161, 195, 230, 253 dielectric function, 173 diﬀusion, 12, 14, 21, 29, 60, 101, 126, 141, 144, 145, 152, 155, 156, 194, 195, 202, 203, 214, 224, 230, 262, 263 dipole, 53, 54, 81, 158, 178 Dirac, 17 dislocation, 12, 33, 128, 195, 196, 205, 208, 230, 234, 235 disorder, 22, 43, 196, 245, 247–251, 254, 261, 269, 270, 281 dispersion, 35, 38, 47, 61, 84, 85, 89, 176, 177, 180, 181, 261 distortion, 14–16, 30, 45, 46, 54, 56–60, 153, 157, 166, 179, 182, 183, 185, 186, 195, 196, 246, 250, 252 distribution function, 219 divacancy, 14, 16, 100 DLTS, 13, 30, 49, 56, 85 donor, 12, 34, 40, 56, 57, 59, 61, 69–71, 80, 82, 84–88, 90, 258 dopant, 3, 4, 12, 13, 69, 70, 80, 89, 105, 152, 194, 196, 206 doping, 12, 13, 30, 87, 168, 180, 194, 258 double-zeta, 43, 97, 103, 259, 260, 262 DX, 5 dynamical matrix, 48, 96, 97, 99, 103, 109 DZ, 259 DZP, 43, 260 EDIP, 131, 222 eﬀective mass, 3–5, 13 eigenstates, 21, 144, 171, 172, 227, 249, 251, 257, 278, 284 eigenvalues, 12–15, 36, 39, 50, 96, 97, 103, 109, 165, 166, 168, 169,

289

172–174, 177, 179, 186, 249, 256, 257, 274 eigenvectors, 96, 97, 99–101, 109, 247, 251, 257, 260 EL2, 5 elastic embedding, 216, 220 electrical level, 58–60, 71, 80, 81, 88–90 electromagnetic radiation, 269 electron, 12, 13, 17–20, 30, 31, 33, 36, 40, 41, 45–47, 56, 58, 59, 69–71, 80, 81, 86, 87, 105, 142, 146–148, 157, 195, 196, 222, 227–229, 231, 252, 253, 259, 260, 269, 275 electron aﬃnity, 36, 170, 172, 182, 185 electron paramagnetic resonance, 12, 153 electron spin resonance, 258, 270 electron states, 32, 38, 157, 247, 250, 257, 258, 270 electron–phonon, 6, 7, 257 electron-nuclear double resonance, 30 electrostatic energy, 54, 55, 70, 159 embed, 216, 220, 225, 231, 233, 237 embedded, 129, 215, 216, 222, 223, 227, 231, 233, 278 embedding, 32, 33, 193 emission, 49 empirical, 15, 22, 85, 86, 88, 132–134, 194, 196, 198, 206, 213–216, 222–225, 230, 233, 236, 247, 250, 255–257, 259 EMT, 13, 222 ENDOR, 30, 38 energetics, 29, 30, 32, 34, 61, 108, 109, 115, 142, 158, 196, 252, 254, 255, 261, 264, 273 energy barrier, 81, 128, 154–156 energy cutoﬀ, 42, 58 energy level, 22, 30, 34, 49, 59, 105, 231, 255 entropy, 48, 104, 106, 108–110, 115, 120, 126, 131, 221, 225, 246, 251 EPR, 4, 12–15, 30, 56, 57 equilibrium, 30, 43, 47–49, 81, 96–98, 101, 107, 109, 118–120, 122–125, 127, 134, 151–155, 159, 195, 196, 206, 222, 224, 226, 227, 249, 250, 282 ergodic, 44, 220, 224

290

Index

ESR, 253, 258, 260 Ewald, 218, 222 exact exchange, 37, 38, 185 exchange, 19, 31, 32, 37–40, 49, 61, 130, 154, 220, 228, 269 exchange-correlation, 20, 21, 31, 32, 36, 39, 42, 44, 58, 71, 96, 97, 166–170, 172, 185, 187, 214, 274 excitation, 32, 38, 39, 44, 49, 57, 101, 142, 158, 165, 167–169, 171–173, 269, 270, 276, 282, 283 excited state, 34, 38, 273, 282 excited-state, 149, 157, 160 exciton, 38, 188, 231, 281 exclusion principle, 19 fast Fourier transform, 41 Fermi level, 30, 36, 37, 45, 49, 165, 167–169, 178, 184, 247, 249, 253, 255, 258 Fermi–Dirac, 51 fermion, 18, 105, 143–145, 148, 160 ﬁnite diﬀerence, 43, 48 ﬁnite element, 43, 198, 214 ﬁrst principles, 16, 21, 22, 32, 42, 43, 60, 72, 95, 96, 98, 105, 108, 157, 214, 225, 237 ﬁrst-principles, 115, 126, 127, 130, 193, 247, 250, 257 ﬂoating bond, 258, 261, 262 ﬂoating orbitals, 43 ﬂuctuation, 19, 72, 74, 119, 221, 249, 257, 274, 275 force, 14, 18, 20, 21, 32–34, 36, 40, 42, 43, 48, 59, 60, 97, 160, 198–200, 202–205, 210, 213–217, 219, 221–223, 226–228, 230, 231, 233, 247, 255, 258, 260, 261, 274, 275 force-constant matrix, 97 formation energy, 32, 40, 48, 49, 56, 80, 81, 88, 154, 156, 158, 184 fourfold, 154, 155, 252–254, 270, 282 Fourier, 13, 34, 48, 69, 95, 225, 246 free carrier, 105 free energy, 22, 44, 60, 96, 97, 102–110, 224, 225 free-energy, 115–126, 128–130, 132, 134, 136, 206 frozen phonon, 48, 97

FTIR, 13, 95 functional derivative, 169, 174 fundamental gap, 34, 36, 45, 61, 170, 174, 178 G0 W0 approximation, 165, 168, 172–180, 182–187 GaAs, 3–5 GaAs(110) surface, 176 GaN, 12, 95, 104, 167 gap, 12–16, 18, 30, 31, 35–38, 81, 82, 89, 249, 252, 269 gap levels, 13, 14, 30 gap states, 30, 35, 45, 46, 50, 168 Gaussian, 16, 42, 54, 58, 71–73, 75, 76, 79, 80, 158 Ge, 5–7, 11, 70, 87, 89, 104, 129, 150, 223, 230, 233, 235, 247, 253, 254, 270 general gradient approximation, 32, 37, 70, 130, 154, 214, 255 general gradient approximation (GGA), 166, 167, 170 germanium, 84, 86, 89, 271 gettering, 12 GGA, 32, 37–39, 42, 70, 71, 82, 89, 130, 154, 155, 214 ghost, 41, 74 Gibbs, 102, 117, 122, 123, 132, 219, 220, 225 glass, 11, 130, 131, 223, 246, 253, 254, 257, 262, 270–274, 277, 282 grain, 195, 196, 253 grain boundary, 12, 195, 196, 230 grand-canonical, 220, 225 Green’s function, 5, 6, 14, 15, 33, 34, 36, 145, 165, 171–174, 179, 181, 227, 229 Green–Kubo, 224 ground state, 30, 32, 34, 36, 47–49, 51, 61, 165, 168, 170, 171, 177, 184, 228, 234, 271, 273, 282 ground-state, 18, 20–22 ground-state, 142–145, 149, 157, 158, 160, 256, 259, 260 GW, 4, 7, 15, 22, 38, 39, 157, 256, 273 H¨ uckel, 15 Hall conductivity, 30

Index Hamiltonian, 4, 5, 14, 44, 72–75, 79, 116–120, 122, 142–145, 148, 171, 200, 204, 218–220, 227, 228, 247, 250–253, 255, 259, 274, 275 handshaking, 215, 219, 225 Hartree, 18, 20, 31, 97, 168, 169, 179 Hartree–Fock, 15, 16, 18, 19, 32, 37–39, 74, 146, 148, 273 Hedin, 39, 174 Heisenberg, 219 Heisenberg picture, 171 Hellmann–Feynman, 32, 36, 48, 214, 228, 257 Helmholtz, 44, 96, 102–104, 117 heterostructure, 231 hole, 12, 13, 39, 69, 105, 166, 172, 173, 180, 196, 269, 270, 281 HOMO, 278, 282 hopping, 228, 251 hopping integral, 180, 182 Hubbard, 253 hybrid, 32, 37, 38, 197–200, 202, 203, 205, 206, 208, 210, 222, 247, 255 hydrogen, 12, 13, 15, 16, 21, 70, 82, 84, 96, 99, 100, 148, 195, 197, 199, 204, 205, 233, 260–264 hyperﬁne, 32–34, 39, 71 imaginary, 142, 144, 148, 149, 229 impurity, 12, 14, 16, 30, 36, 45, 46, 48, 49, 80, 96, 99, 142, 152, 195, 258 InP(110) surface, 176 interface, 12, 123, 215, 216, 225, 230, 233–236 internal energy, 115, 116, 120, 224 interstitial, 14, 15, 52, 54, 87, 105–107, 126, 127, 153–157, 194 ionization, 34–36, 38, 41, 49, 50, 56, 57, 69, 87 ionization potential, 170, 172, 185 IPR, 251, 252, 257, 260, 280 irreversible, 119, 271 isothermal, 117, 224 isotope, 4, 6, 13, 95, 104 Jahn–Teller, 14, 44–46, 56, 57, 60, 153, 157, 158 jellium, 53, 222 kink, 195, 205, 206, 230

291

Kohn–Sham, 31, 32, 34–39, 42, 44, 50–52, 55, 58, 82, 157, 249, 255–257, 259, 260, 273–275, 282 Lagrange, 219, 221, 237 Lagrange parameter, 169 Lagrangian, 218, 219, 221, 225–227 LCAO, 15, 22, 56, 275 LDA, 5, 37–40, 42, 71, 77, 82, 89, 130, 156, 166–171, 173, 176, 177, 181–184, 186, 187, 214, 255, 257, 258, 261, 273 LDA+U , 40 Lennard–Jones, 119, 125, 222 linear response, 97 Liouville, 120, 219 liquid, 43, 119, 128–130, 133, 134, 143, 219, 254, 258 localization, 22, 30, 99, 109, 148, 149, 213, 217, 231, 249, 251, 257, 260, 270, 278 LOTF, 200, 203–205 LSDA, 32, 37, 58, 150, 154, 155, 158, 160 LUMO, 279, 282 Madelung, 53, 54, 81, 85, 218, 222 magnetic, 11–13, 72, 105 Makov–Payne, 54, 83 many-body perturbation theory, 171 marker, 22, 50, 51, 59, 71, 80, 82–90 Maxwell, 221 melting, 11, 122, 124, 128–130, 133–135, 233, 254 metastability, 280 metastablity, 82, 258 Metropolis, 143, 254 microcanonical, 43, 217, 220, 221, 225 midgap, 60, 251, 258 migration, 29, 34, 42, 60, 71, 95, 125, 126, 142, 154, 194, 195, 206 minimal basis, 16, 35, 259, 276 misﬁt, 230, 235 mobility, 69, 126–128, 251 molecular dynamics, 16, 22, 42–44, 60, 71, 96, 126, 154, 213, 216 molecular-dynamics, 273 molecular-dynamics, 193, 195, 198, 205, 247, 254, 255

292

Index

Monkhorst–Pack, 97, 103 Morse, 222 muﬃn-tin, 15 Mulliken, 84, 251, 260, 275 multipole, 53, 83, 89, 178, 223, 226 multiscale, 22, 60, 196, 197, 210 nanometer, 12, 195, 231 nanoscience, 12 narrow-gap, 84, 89 negative-U , 60 neutron diﬀraction, 246 Newton, 43, 227 nonlocal, 17, 32, 37, 38, 148, 167, 172, 174, 179, 180 normal mode, 48, 95–101, 103, 104 Nos´e, 221 optical, 11, 12, 30, 34, 39, 40, 49, 69, 87, 157, 231, 247, 249, 252, 256–258, 270–272, 278, 282 optoelectronic, 231 order-N , 18, 97 oxygen, 12, 14, 39, 40, 86, 107, 108, 281 pair-distribution function, 220, 224 pair-correlation function, 246, 249, 254 pairing, 46, 56 Parrinello, 21, 130, 221 partition function, 105, 106, 116–118, 121, 219, 224 Pauli, 32, 40 Perdew–Wang, 58, 71 periodic, 12, 16, 33–36, 52–55, 70, 71, 96, 97, 103, 108, 126, 148, 159, 175, 177, 178, 180, 194, 205, 250, 261 periodic boundary conditions, 15, 22, 33, 34, 43, 44, 54, 55, 69, 89, 147, 149, 220, 261 periodicity, 12, 15, 16, 34, 84, 236, 261 perturbation, 12–14, 19, 44, 54, 154, 157, 165, 167–169, 171–173, 179, 187, 221, 222 phase boundary, 119, 122–124 phase diagram, 22, 119, 125, 128, 132–135 phase space, 219, 220 phase-space, 116, 120

phonon, 6, 47, 48, 95–97, 99–104, 109, 172, 205, 223, 226, 257, 269 phosphorus, 70, 87 photoconductivity, 269, 271 photodarkening, 271, 272, 282 photoemission, 166, 170, 184, 247, 256 photoexpansion, 272 photoluminescence, 12, 13, 30, 96, 99, 194, 270, 271 photovoltaic, 246, 258 PL, 12, 30, 96, 99 plane wave, 34, 39, 41–43, 58, 69–73, 80, 160, 171, 173–175, 179 plane-wave, 21, 22 plane-wave, 259 plasmon, 172, 175, 178 platelet, 12 pnictogen, 88, 282 point defect, 30, 33, 35, 56, 146, 147, 153, 154, 165–168, 170, 194, 195, 203, 223, 230, 261 Poisson, 54, 55 polarizability, 173, 175, 178 polarization, 43, 54, 74, 78, 97, 173, 178, 179, 255, 259, 260, 271, 272 population, 22, 84, 127, 149 positron annihilation, 29, 32, 34, 61, 194 potential, 14, 18–21, 32, 34–37, 41, 42, 44, 45, 49–51, 55, 59, 61, 70, 74, 79–84, 87, 96–98, 101, 105, 110, 115, 116, 118, 121, 122, 125, 128–134, 142, 144, 145, 149, 195, 196, 201, 202, 208, 210, 214–218, 220–223, 225–228, 230, 233–235, 247, 250, 252, 254, 255, 259, 261, 262, 274–276 PRDDO, 16 precipitates, 12, 231 projected augmented wave, 41, 58 proton, 105, 195 pseudoatom, 222, 274 pseudopotential, 16, 40–42, 58, 60, 61, 71, 72, 76, 96, 148, 149, 160, 167, 171, 174, 182, 214, 222, 259 quadrupole, 81 quantum dot, 98, 225, 230, 231, 233, 236

Index quantum Monte Carlo, 18, 22, 40, 141, 142, 145–148, 150–152, 154, 157, 158, 160, 161, 256 quasiparticle, 38, 165, 167, 169–176, 179, 181–183, 185, 187, 188, 273 quasiparticle equation, 172 radial-distribution function, 224, 246, 254, 276 radiation damage, 14, 194 radiative, 69, 269, 270 Raman, 13, 95, 96, 105, 106, 269, 277 random-phase approximation, 170, 173, 175, 178 real space, 15, 42, 43, 71, 72, 97, 160, 175, 177, 246 reciprocal space, 32, 34, 42, 175 recombination, 12, 14, 34, 69, 269, 270 recursion, 227, 229 relativistic, 32 relaxation, 14, 33, 35, 36, 45, 58, 158, 166, 167, 171, 176, 179, 180, 182, 183, 185, 186, 197, 215, 216, 231, 233, 235, 236, 253, 255, 262, 271 repulsive, 45, 108, 110, 222, 230, 275 resonance, 29, 38, 45, 153, 258, 270 resonant, 96, 109, 269 reversible, 116, 119, 120, 122, 124, 131, 134, 246, 250, 271, 272 rotational, 105, 106, 109, 235, 236 Sankey, 21, 97 scalar, 271, 272 scanning tunneling microscopy (STM), 165, 166, 168, 184, 186 scattering, 15, 69, 172, 225, 269, 272, 277 scattering-Xα, 15 Schottky, 158–161 Schr¨ odinger, 13, 15, 18, 31, 44, 144 scissor, 39 screened exchange, 32, 38 screening, 38, 54, 173, 183, 218, 222, 230 self-diﬀusion, 125–127, 154, 156, 157 self-energy, 22, 157, 165, 167, 168, 172–183, 187, 256 self-interaction, 31, 37, 39, 41, 217, 233, 275

293

self-interstitial, 12, 14, 40, 125, 126, 152–154, 156, 161 self-organization, 231 self-trapped, 38, 281 semicore, 42, 55 semiempirical, 15, 16, 122, 216, 223, 274 shallow, 12, 49, 59, 60, 70, 71, 82, 84, 85, 87, 88 shear, 224, 236 Si, 6, 7, 11, 12, 14, 16, 22, 38–40, 45, 46, 56–60, 75, 77, 79, 87, 96, 99, 100, 102, 104–107, 122, 125–131, 134, 135, 150, 197, 201, 203, 205, 222, 223, 230, 235, 245–247, 249, 250, 252–254, 258–260, 262–264, 269, 270, 281 SIESTA, 21, 96, 214, 258, 262 SiGe, 89 silicon, 14, 16, 21, 22, 35, 36, 46, 52, 56, 75, 76, 78, 80, 81, 84–90, 126, 128, 130, 131, 141, 142, 152–154, 156, 157, 161, 194, 195, 197, 199, 203–205, 208, 245, 259, 261, 281 Slater, 6, 18, 40, 146, 147, 156, 158, 160, 227, 228, 279 Slater transition state, 169 special point, 52 speciﬁc heat, 97, 102, 104, 109, 130 spherical harmonic, 223 spherical harmonics, 72 spin, 12–14, 29, 30, 32, 37, 39, 41, 46, 61, 84, 105, 109, 146, 150, 158, 169, 182, 252, 253, 255, 258, 260, 270, 276 spin degeneracy, 228 spin-orbit, 3, 5, 46, 56, 58 split-vacancy, 60 Staebler–Wronski, 258, 261 statistical, 43, 116, 121, 145–147, 149, 150, 158, 216, 219, 224 Stillinger–Weber, 128–131, 203, 208, 222, 235 stoichiometry, 34, 49 Stokes, 49 strain, 35, 43, 79, 96, 195, 208, 221, 224, 225, 230, 231, 233, 236, 247, 261, 271

294

Index

stress, 13, 35, 42, 57, 95, 128, 157, 196, 197, 208, 221, 224, 247, 271 structure factor, 246 substitutional, 13, 38, 45, 46, 56, 57, 83, 84, 87, 107 supercell, 15, 16, 22, 31–36, 38–40, 43–56, 58–61, 70, 81, 84, 86–88, 90, 96, 97, 101, 103, 104, 108, 148, 159, 177–180, 182, 194, 220, 233, 283 surface, 12, 13, 15, 16, 19, 33, 36, 42, 43, 55, 61, 70, 72, 74, 75, 81, 101, 110, 120, 142, 144–147, 149, 165–169, 171, 173, 176–182, 184, 187, 197–199, 202, 208, 215, 216, 220, 230, 231, 233, 234, 250, 261, 272 surface band, 176 symmetric, 99, 101, 105, 146, 221, 278 symmetry, 13–16, 21, 30, 35, 38, 44–46, 56, 57, 59, 60, 95, 96, 99, 106, 109, 148, 149, 153, 157, 166, 176, 179, 180, 182, 183, 186, 235, 259, 273 symmetry breaking, 30, 54 Taylor, 47, 217, 222 temperature, 11, 12, 20, 22, 30, 42, 43, 49, 69, 80, 81, 87, 96–102, 104, 106–110, 115–134, 153, 154, 203–206, 208, 218, 221, 224, 233–236, 247, 249, 250, 257, 262, 272 termination, 177, 198, 199 Tersoﬀ, 129, 223, 228, 230, 235 tetrahedral, 35, 38, 45, 106, 153, 155, 156, 195, 252–254, 258 thermal disorder, 247, 249 thermal equilibrium, 48, 96, 109, 159, 249, 282 thermodynamic integration, 44, 118, 120, 122, 124, 126, 128, 132 thermodynamic ionization, 49 thermostat, 43, 96, 98, 109, 204, 205, 220, 221 Thomas–Fermi, 19, 21, 38 tight binding, 21, 175, 180, 181, 214, 215, 222, 273, 274 tight-binding, 122, 126, 127, 129, 134, 198, 203, 204, 206, 247, 250, 255

tiling, 145 time-dependent density-functional theory (TDDFT), 39, 44, 282 time-dependent Schr¨ odinger equation (TDSE), 44 total energy, 19, 21, 30–32, 34, 43, 45, 47–53, 56, 58, 73, 75, 79, 96, 98, 159, 168–170, 179, 182, 184, 185, 199, 204, 217, 220, 233, 247, 252, 260, 274, 275 trajectory, 44, 120, 199, 200, 203, 219, 220, 262 transferability, 15, 41, 222, 230, 236 transient-enhanced diﬀusion, 12 transition, 49, 81–83, 119, 122, 125, 128, 131, 134, 135, 157, 158, 200, 217, 218, 222, 228, 231, 233, 246, 251, 254, 269, 270, 272 transition level, 30, 49, 51 transition metal, 11, 12, 14, 57, 58, 142 transport, 221, 224, 245, 269 trigonal, 46, 58, 60, 282 ultrasoft pseudopotential, 41, 58, 59, 70 uniaxial stress, 13, 95, 157 vacancy, 12, 14–16, 35, 38, 40, 45, 46, 52, 54, 56, 60, 81, 86, 96, 125–127, 153, 154, 157–159, 161, 203 valence band, 12, 35, 38, 40, 49–51, 55, 56, 81–83, 88, 105, 169, 170, 176–178, 180, 182, 184, 269–271, 278 Van der Waals, 222, 270 variational, 18, 20, 31, 43, 73, 141, 143, 148, 149, 218, 259, 275 VASP, 58–60 vectoral, 271, 272 velocity autocorrelation, 48, 224 Verlet, 217 vibrational dynamics, 30 vibrational entropy, 48, 60, 104, 126 vibrational free energy, 60, 97, 104, 105, 107, 109 vibrational lifetime, 96–98, 100, 101, 109 vibrational modes, 22, 29, 33, 34, 47, 48, 61, 71, 84, 85, 95, 96, 99

Index vibrational spectroscopy, 12, 13, 29, 95, 96 wafer bonding, 215, 230, 233–235 wag, 96, 99, 101 Wannier, 14, 252 water, 130–134, 223 Watkins, 15, 45, 46, 56

wavelength, 52, 231, 246, 269, 271 Wigner–Seitz, 35, 55 X-ray, 225, 246, 269 zincblende lattice, 176 ZnO, 40, 82

295

Topics in Applied Physics is part of the SpringerLink service. For all customers with standing orders for Topics in Applied Physics we offer the full text in electronic form via SpringerLink free of charge. Please contact your librarian who can receive a password for free access to the full articles by registration at: springerlink.com → Orders If you do not have a standing order you can nevertheless browse through the table of contents of the volumes and the abstracts of each article at: springerlink.com → Browse Publications

Topics in Applied Physics Topics in Applied Physics is a well-established series of review books, each of which presents a comprehensive survey of a selected topic within the broad area of applied physics. Edited and written by leading research scientists in the field concerned, each volume contains review contributions covering the various aspects of the topic. Together these provide an overview of the state of the art in the respective field, extending from an introduction to the subject right up to the frontiers of contemporary research. Topics in Applied Physics is addressed to all scientists at universities and in industry who wish to obtain an overview and to keep abreast of advances in applied physics. The series also provides easy but comprehensive access to the fields for newcomers starting research. Contributions are specially commissioned. The Managing Editors are open to any suggestions for topics coming from the community of applied physicists no matter what the field and encourage prospective editors to approach them with ideas.

Managing Editors Dr. Claus E. Ascheron

Dr. Hans J. Koelsch

Springer-Verlag GmbH Tiergartenstr. 17 69121 Heidelberg Germany Email: [email protected]

Springer-Verlag New York, LLC 233, Spring Street New York, NY 10013 USA Email: [email protected]

Assistant Editor Adelheid H. Duhm Springer-Verlag GmbH Tiergartenstr. 17 69121 Heidelberg Germany Email: [email protected]

David A. Drabold Stefan K. Estreicher (Eds.)

Theory of Defects in Semiconductors

With 60 Figures and 15 Tables

123

David A. Drabold Department of Physics and Astronomy Ohio University Athens, OH 45701, USA [email protected]

Stefan K. Estreicher Physics Department Texas Tech University Lubbock, TX 79409-1051, USA [email protected]

Library of Congress Control Number: 2006934116

Physics and Astronomy Classiﬁcation Scheme (PACS): 71.10.-w, 71.17.-m, 71.23.-k, 71.55.-i, 63.20Mt

ISSN print edition: 0303-4216 ISSN electronic edition: 1437-0859 ISBN-10 3-540-33400-9 Springer Berlin Heidelberg New York ISBN-13 978-3-540-33400-2 Springer Berlin Heidelberg New York This work is subject to copyright. All rights are reserved, whether the whole or part of the material is concerned, specifically the rights of translation, reprinting, reuse of illustrations, recitation, broadcasting, reproduction on microfilm or in any other way, and storage in data banks. Duplication of this publication or parts thereof is permitted only under the provisions of the German Copyright Law of September 9, 1965, in its current version, and permission for use must always be obtained from Springer. Violations are liable for prosecution under the German Copyright Law. Springer is a part of Springer Science+Business Media springer.com © Springer-Verlag Berlin Heidelberg 2007 The use of general descriptive names, registered names, trademarks, etc. in this publication does not imply, even in the absence of a specific statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. Typesetting: DA-TEX · Gerd Blumenstein · www.da-tex.de ockler GbR, Leipzig Production: LE-TEX Jelonek, Schmidt & V¨ Cover design: WMXDesign GmbH, Heidelberg Printed on acid-free paper

57/3100/YL

543210

Contents

Foreword Manuel Cardona . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 1 Early History and Contents of the Present Volume . . . . . . . . . . . . . . . 1 2 Bibliometric Studies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9 Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10 Defect Theory: An Armchair History David A. Drabold, Stefan K. Estreicher . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 The Evolution of Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 A Sketch of First-Principles Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Single-Particle Methods: History . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Direct Approaches to the Many-Electron Problem . . . . . . . . . . . 3.3 Hartree and Hartree–Fock Approximations . . . . . . . . . . . . . . . . . 3.4 Density-Functional Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4.1 Thomas–Fermi Model . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4.2 Modern Density-Functional Theory . . . . . . . . . . . . . . . . . . 4 The Contributions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Supercell Methods for Defect Calculations Risto M. Nieminen . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Density-Functional Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Supercell and Other Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Issues with the Supercell Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 The Exchange-Correlation Functionals and the Semiconducting Gap . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Core and Semicore Electrons: Pseudopotentials and Beyond . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7 Basis Sets . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8 Time-Dependent and Finite-Temperature Simulations . . . . . . . . . . . . 9 Jahn–Teller Distortions in Semiconductor Defects . . . . . . . . . . . . . . .

11 11 13 16 17 18 18 19 19 20 22 23 26 29 29 31 32 34 36 40 42 43 44

X

Contents

9.1 Vacancy in Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.2 Substitutional Copper in Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . 10 Vibrational Modes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11 Ionization Levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12 The Marker Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 13 Brillouin-Zone Sampling . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14 Charged Defects and Electrostatic Corrections . . . . . . . . . . . . . . . . . . 15 Energy-Level References and Valence-Band Alignment . . . . . . . . . . . 16 Examples: The Monovacancy and Substitutional Copper in Silicon . 16.1 Experiments . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 16.2 Calculations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 17 Summary and Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

45 46 47 48 50 51 52 55 56 56 58 60 61 64

Marker-Method Calculations for Electrical Levels Using Gaussian-Orbital Basis Sets J.P. Goss, M.J. Shaw,, P.R. Briddon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Computational Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Gaussian Basis Set . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 Choice of Exponents . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3 Case Study: Bulk Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4 Charge-Density Expansions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Electrical Levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Formation Energy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Calculation of Electrical Levels Using the Marker Method . . . . 4 Application to Defects in Group-IV Materials . . . . . . . . . . . . . . . . . . . 4.1 Chalcogen–Hydrogen Donors in Silicon . . . . . . . . . . . . . . . . . . . . 4.2 VO Centers in Silicon and Germanium . . . . . . . . . . . . . . . . . . . . 4.3 Shallow and Deep Levels in Diamond . . . . . . . . . . . . . . . . . . . . . . 5 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

69 69 71 72 75 76 80 80 81 83 84 84 86 87 89 90 92

Dynamical Matrices and Free Energies Stefan K. Estreicher, Mahdi Sanati . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Dynamical Matrices . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Local and Pseudolocal Modes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Vibrational Lifetimes and Decay Channels . . . . . . . . . . . . . . . . . . . . . . 5 Vibrational Free Energies and Speciﬁc Heats . . . . . . . . . . . . . . . . . . . . 6 Theory of Defects at Finite Temperatures . . . . . . . . . . . . . . . . . . . . . . 7 Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

95 95 97 99 100 101 105 108 110

Contents

XI

Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 112 The Calculation of Free-Energies in Semiconductors: Defects, Transitions and Phase Diagrams E. R. Hern´ andez, A. Antonelli, L. Colombo, P. Ordej´ on . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 The Calculation of Free-Energies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Thermodynamic Integration and Adiabatic Switching . . . . . . . 2.2 Reversible Scaling . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3 Phase Boundaries and Phase Diagrams . . . . . . . . . . . . . . . . . . . . 3 Applications . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Thermal Properties of Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Melting of Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.3 Phase Diagrams . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Conclusions and Outlook . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Quantum Monte Carlo Techniques and Defects in Semiconductors R. J. Needs . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Quantum Monte Carlo Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 The VMC Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 The DMC Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3 Trial Wavefunctions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4 Optimization of Trial Wavefunctions . . . . . . . . . . . . . . . . . . . . . . 2.5 QMC Calculations within Periodic Boundary Conditions . . . . . 2.6 Using Pseudopotentials in QMC Calculations . . . . . . . . . . . . . . . 3 DMC Calculations for Excited States . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Sources of Error in DMC Calculations . . . . . . . . . . . . . . . . . . . . . . . . . 5 Applications of QMC to the Cohesive Energies of Solids . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Applications of QMC to Defects in Semiconductors . . . . . . . . . . . . . . 6.1 Using Structures from Simpler Methods . . . . . . . . . . . . . . . . . . . 6.2 Silicon Self-Interstitial Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.2.1 DFT Calculations on Silicon Self-Interstitials . . . . . . . . . 6.2.2 QMC Calculations on Silicon Self-Interstitials . . . . . . . . . 6.3 Neutral Vacancy in Diamond . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.1 VMC and DMC Calculations on the Neutral Vacancy in Diamond . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.4 Schottky Defects in Magnesium Oxide . . . . . . . . . . . . . . . . . . . . . 7 Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

115 115 116 117 120 122 125 125 128 132 136 136 138

141 141 142 143 144 146 147 147 148 149 149 150 151 151 152 154 156 157 157 158 160 161 163

XII

Contents

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces Arno Schindlmayr, Matthias Scheﬄer . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Computational Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Density-Functional Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 Many-Body Perturbation Theory . . . . . . . . . . . . . . . . . . . . . . . . . 3 Electronic Structure of Defect-Free Surfaces . . . . . . . . . . . . . . . . . . . . 4 Defect States . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 Charge-Transition Levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

165 165 168 168 171 176 179 184 187 188 190

Multiscale Modeling of Defects in Semiconductors: A Novel Molecular-Dynamics Scheme G´ abor Cs´ anyi, Gianpietro Moras, James R. Kermode, Michael C. Payne, Alison Mainwood, Alessandro De Vita . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 A Hybrid View . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Hybrid Simulation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 The LOTF Scheme . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 Applications . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

193 193 194 197 200 203 210 210 211

Empirical Molecular Dynamics: Possibilities, Requirements, and Limitations Kurt Scheerschmidt . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction: Why Empirical Molecular Dynamics? . . . . . . . . . . . . . . 2 Empirical Molecular Dynamics: Basic Concepts . . . . . . . . . . . . . . . . . 2.1 Newtonian Equations and Numerical Integration . . . . . . . . . . . . 2.2 Particle Mechanics and Nonequilibrium Systems . . . . . . . . . . . . 2.3 Boundary Conditions and System Control . . . . . . . . . . . . . . . . . 2.4 Many-Body Empirical Potentials and Force Fields . . . . . . . . . . 2.5 Determination of Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Extensions of the Empirical Molecular Dynamics . . . . . . . . . . . . . . . . 3.1 Modiﬁed Boundary Conditions: Elastic Embedding . . . . . . . . . . 3.2 Tight-Binding-Based Analytic Bond-Order Potentials . . . . . . . 4 Applications . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1 Quantum Dots: Relaxation, Reordering, and Stability . . . . . . . 4.2 Bonded Interfaces: Tailoring Electronic or Mechanical Properties? . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 Conclusions and Outlook . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

213 213 216 216 218 220 221 224 225 225 227 230 231 233 236

Contents

XIII

References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 237 Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 241 Defects in Amorphous Semiconductors: Amorphous Silicon D.A. Drabold, T.A. Abtew . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Amorphous Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Defects in Amorphous Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Deﬁnition of Defect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Long-Time Dynamics and Defect Equilibria . . . . . . . . . . . . . . . . 3.3 Electronic Aspects of Amorphous Semiconductors . . . . . . . . . . . 3.4 Electron Correlation Energy: Electron–Electron Eﬀects . . . . . . 4 Modeling Amorphous Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1 Forming Structural Models . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2 Interatomic Potentials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.3 Lore of Approximations in Density-Functional Calculations . . 4.4 The Electron–Lattice Interaction . . . . . . . . . . . . . . . . . . . . . . . . . 5 Defects in Amorphous Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Light Induced Eﬀects in Amorphous and Glassy Solids S. I. Simdyankin, S. R. Elliott . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Photoinduced Metastability in Amorphous Solids: An Experimental Survey . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.2 Photoinduced Eﬀects in Chalcogenide Glasses . . . . . . . . . . . . . . 2 Theoretical Studies of Photoinduced Excitations in Amorphous Materials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Application of the Density-Functional-Based Tight-Binding Method to the Case of Amorphous As2 S3 . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

245 245 246 248 248 250 250 252 253 253 255 255 257 258 264 266 269 269 269 271 272 273 283 285

Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 287

This book is dedicated to Manuel Cardona, who has done so much for the ﬁeld of defects in semiconductors over the past decades, and convinced so many theorists to calculate beyond what they thought possible.

Preface

Semiconductor materials emerged after World War II and their impact on our lives has grown ever since. Semiconductor technology is, to a large extent, the art of defect engineering. Today, defect control is often done at the atomic level. Theory has played a critical role in understanding, and therefore controlling, the properties of defects. Conversely, the careful experimental studies of defects in Ge, Si, then many other semiconductor materials have generated a huge database of measured quantities that allowed theorists to test their methods and approximations. Dramatic improvement in methodology, especially density-functional theory, along with inexpensive and fast computers, has impedance matched the experimentalist and theorist in ways unanticipated before the late 1980s. As a result, the theory of defects in semiconductors has become quantitative in many respects. Today, more powerful theoretical approaches are still being developed. More importantly perhaps, the tools developed to study defects in semiconductors are now being adapted to approach many new challenges associated with nanoscience, a very long list that includes quantum dots, buckyballs and buckytubes, spintronics, interfaces, and many others. Despite the importance of the ﬁeld, there have been no modern attempts to treat the computational science of the ﬁeld in a coherent manner within a single treatise. This is the aim of the present volume. This book brings together several leaders in theoretical research on defects in semiconductors. Although the treatment is tutorial, the level at which the various applications are discussed is today’s state-of-the-art in the ﬁeld. The book begins with a “big picture” view from Manuel Cardona, and continues with a brief summary of the historical development of the subject in Chap. 1. This includes an overview of today’s most commonly used method to describe defects. We have attempted to create a balanced and tutorial treatment of the basic theory and methodology in Chaps. 3–6. They include detailed discussions of the approximations involved, the calculation of electrically active levels, and extensions of the theory to ﬁnite temperatures. Two emerging electronic structure methodologies of special importance to the ﬁeld are discussed in Chaps. 7 (quantum Monte-Carlo) and 8 (the GW method). Then come two chapters on molecular dynamics (MD). In Chap. 9, a combination of high-

VIII

Preface

level and approximate MD is developed, with applications to the dynamics of extended defect. Chapter 10 deals with semiempirical treatments of microstructures, including issues such as wafer bonding. The book concludes with studies of defects and their role in the photoresponse of topologically disordered (amorphous) systems. The intended audience for the book is graduate students as well as advanced researchers in physics, chemistry, materials science, and engineering. We have sought to provide self-contained descriptions of the work, with detailed references available when needed. The book may be used as a text in a practical graduate course designed to prepare students for research work on defects in semiconductors or ﬁrst-principles theory in materials science in general. The book also serves as a reference for the active theoretical researcher, or as a convenient guide for the experimentalist to keep tabs on their theorist colleagues. It was a genuine pleasure to edit this volume. We are delighted with the contributions provided in a timely fashion by so many busy and accomplished people. We warmly thank all the contributors and hope to have the opportunity to share some nice wine(s) with all of them soon. After all, When Ptolemy, now long ago, Believed the Earth stood still, He never would have blundered so Had he but drunk his ﬁll. He’d then have felt it circulate And would have learnt to say: The true way to investigate Is to drink a bottle a day. (author unknown) published in Augustus de Morgan’s A Budget of Paradoxes, (1866). Athens, Ohio, Lubbock, Texas February 2006

David A. Drabold Stefan K. Estreicher

Contents

Foreword Manuel Cardona . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 1 Early History and Contents of the Present Volume . . . . . . . . . . . . . . . 1 2 Bibliometric Studies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9 Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10 Defect Theory: An Armchair History David A. Drabold, Stefan K. Estreicher . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 The Evolution of Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 A Sketch of First-Principles Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Single-Particle Methods: History . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Direct Approaches to the Many-Electron Problem . . . . . . . . . . . 3.3 Hartree and Hartree–Fock Approximations . . . . . . . . . . . . . . . . . 3.4 Density-Functional Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4.1 Thomas–Fermi Model . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4.2 Modern Density-Functional Theory . . . . . . . . . . . . . . . . . . 4 The Contributions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Supercell Methods for Defect Calculations Risto M. Nieminen . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Density-Functional Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Supercell and Other Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Issues with the Supercell Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 The Exchange-Correlation Functionals and the Semiconducting Gap . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Core and Semicore Electrons: Pseudopotentials and Beyond . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7 Basis Sets . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8 Time-Dependent and Finite-Temperature Simulations . . . . . . . . . . . . 9 Jahn–Teller Distortions in Semiconductor Defects . . . . . . . . . . . . . . .

11 11 13 16 17 18 18 19 19 20 22 23 26 29 29 31 32 34 36 40 42 43 44

X

Contents

9.1 Vacancy in Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.2 Substitutional Copper in Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . 10 Vibrational Modes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11 Ionization Levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12 The Marker Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 13 Brillouin-Zone Sampling . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14 Charged Defects and Electrostatic Corrections . . . . . . . . . . . . . . . . . . 15 Energy-Level References and Valence-Band Alignment . . . . . . . . . . . 16 Examples: The Monovacancy and Substitutional Copper in Silicon . 16.1 Experiments . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 16.2 Calculations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 17 Summary and Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

45 46 47 48 50 51 52 55 56 56 58 60 61 64

Marker-Method Calculations for Electrical Levels Using Gaussian-Orbital Basis Sets J.P. Goss, M.J. Shaw,, P.R. Briddon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Computational Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Gaussian Basis Set . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 Choice of Exponents . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3 Case Study: Bulk Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4 Charge-Density Expansions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Electrical Levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Formation Energy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Calculation of Electrical Levels Using the Marker Method . . . . 4 Application to Defects in Group-IV Materials . . . . . . . . . . . . . . . . . . . 4.1 Chalcogen–Hydrogen Donors in Silicon . . . . . . . . . . . . . . . . . . . . 4.2 VO Centers in Silicon and Germanium . . . . . . . . . . . . . . . . . . . . 4.3 Shallow and Deep Levels in Diamond . . . . . . . . . . . . . . . . . . . . . . 5 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

69 69 71 72 75 76 80 80 81 83 84 84 86 87 89 90 92

Dynamical Matrices and Free Energies Stefan K. Estreicher, Mahdi Sanati . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Dynamical Matrices . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Local and Pseudolocal Modes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Vibrational Lifetimes and Decay Channels . . . . . . . . . . . . . . . . . . . . . . 5 Vibrational Free Energies and Speciﬁc Heats . . . . . . . . . . . . . . . . . . . . 6 Theory of Defects at Finite Temperatures . . . . . . . . . . . . . . . . . . . . . . 7 Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

95 95 97 99 100 101 105 108 110

Contents

XI

Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 112 The Calculation of Free-Energies in Semiconductors: Defects, Transitions and Phase Diagrams E. R. Hern´ andez, A. Antonelli, L. Colombo, P. Ordej´ on . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 The Calculation of Free-Energies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Thermodynamic Integration and Adiabatic Switching . . . . . . . 2.2 Reversible Scaling . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3 Phase Boundaries and Phase Diagrams . . . . . . . . . . . . . . . . . . . . 3 Applications . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Thermal Properties of Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Melting of Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.3 Phase Diagrams . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Conclusions and Outlook . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Quantum Monte Carlo Techniques and Defects in Semiconductors R. J. Needs . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Quantum Monte Carlo Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 The VMC Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 The DMC Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3 Trial Wavefunctions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4 Optimization of Trial Wavefunctions . . . . . . . . . . . . . . . . . . . . . . 2.5 QMC Calculations within Periodic Boundary Conditions . . . . . 2.6 Using Pseudopotentials in QMC Calculations . . . . . . . . . . . . . . . 3 DMC Calculations for Excited States . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Sources of Error in DMC Calculations . . . . . . . . . . . . . . . . . . . . . . . . . 5 Applications of QMC to the Cohesive Energies of Solids . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Applications of QMC to Defects in Semiconductors . . . . . . . . . . . . . . 6.1 Using Structures from Simpler Methods . . . . . . . . . . . . . . . . . . . 6.2 Silicon Self-Interstitial Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.2.1 DFT Calculations on Silicon Self-Interstitials . . . . . . . . . 6.2.2 QMC Calculations on Silicon Self-Interstitials . . . . . . . . . 6.3 Neutral Vacancy in Diamond . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.1 VMC and DMC Calculations on the Neutral Vacancy in Diamond . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.4 Schottky Defects in Magnesium Oxide . . . . . . . . . . . . . . . . . . . . . 7 Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

115 115 116 117 120 122 125 125 128 132 136 136 138

141 141 142 143 144 146 147 147 148 149 149 150 151 151 152 154 156 157 157 158 160 161 163

XII

Contents

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces Arno Schindlmayr, Matthias Scheﬄer . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Computational Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Density-Functional Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 Many-Body Perturbation Theory . . . . . . . . . . . . . . . . . . . . . . . . . 3 Electronic Structure of Defect-Free Surfaces . . . . . . . . . . . . . . . . . . . . 4 Defect States . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 Charge-Transition Levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

165 165 168 168 171 176 179 184 187 188 190

Multiscale Modeling of Defects in Semiconductors: A Novel Molecular-Dynamics Scheme G´ abor Cs´ anyi, Gianpietro Moras, James R. Kermode, Michael C. Payne, Alison Mainwood, Alessandro De Vita . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 A Hybrid View . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Hybrid Simulation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 The LOTF Scheme . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 Applications . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

193 193 194 197 200 203 210 210 211

Empirical Molecular Dynamics: Possibilities, Requirements, and Limitations Kurt Scheerschmidt . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction: Why Empirical Molecular Dynamics? . . . . . . . . . . . . . . 2 Empirical Molecular Dynamics: Basic Concepts . . . . . . . . . . . . . . . . . 2.1 Newtonian Equations and Numerical Integration . . . . . . . . . . . . 2.2 Particle Mechanics and Nonequilibrium Systems . . . . . . . . . . . . 2.3 Boundary Conditions and System Control . . . . . . . . . . . . . . . . . 2.4 Many-Body Empirical Potentials and Force Fields . . . . . . . . . . 2.5 Determination of Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Extensions of the Empirical Molecular Dynamics . . . . . . . . . . . . . . . . 3.1 Modiﬁed Boundary Conditions: Elastic Embedding . . . . . . . . . . 3.2 Tight-Binding-Based Analytic Bond-Order Potentials . . . . . . . 4 Applications . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1 Quantum Dots: Relaxation, Reordering, and Stability . . . . . . . 4.2 Bonded Interfaces: Tailoring Electronic or Mechanical Properties? . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 Conclusions and Outlook . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

213 213 216 216 218 220 221 224 225 225 227 230 231 233 236

Contents

XIII

References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 237 Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 241 Defects in Amorphous Semiconductors: Amorphous Silicon D.A. Drabold, T.A. Abtew . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Amorphous Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Defects in Amorphous Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Deﬁnition of Defect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Long-Time Dynamics and Defect Equilibria . . . . . . . . . . . . . . . . 3.3 Electronic Aspects of Amorphous Semiconductors . . . . . . . . . . . 3.4 Electron Correlation Energy: Electron–Electron Eﬀects . . . . . . 4 Modeling Amorphous Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1 Forming Structural Models . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2 Interatomic Potentials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.3 Lore of Approximations in Density-Functional Calculations . . 4.4 The Electron–Lattice Interaction . . . . . . . . . . . . . . . . . . . . . . . . . 5 Defects in Amorphous Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Light Induced Eﬀects in Amorphous and Glassy Solids S. I. Simdyankin, S. R. Elliott . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Photoinduced Metastability in Amorphous Solids: An Experimental Survey . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.2 Photoinduced Eﬀects in Chalcogenide Glasses . . . . . . . . . . . . . . 2 Theoretical Studies of Photoinduced Excitations in Amorphous Materials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Application of the Density-Functional-Based Tight-Binding Method to the Case of Amorphous As2 S3 . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

245 245 246 248 248 250 250 252 253 253 255 255 257 258 264 266 269 269 269 271 272 273 283 285

Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 287

This book is dedicated to Manuel Cardona, who has done so much for the ﬁeld of defects in semiconductors over the past decades, and convinced so many theorists to calculate beyond what they thought possible.

Preface

Semiconductor materials emerged after World War II and their impact on our lives has grown ever since. Semiconductor technology is, to a large extent, the art of defect engineering. Today, defect control is often done at the atomic level. Theory has played a critical role in understanding, and therefore controlling, the properties of defects. Conversely, the careful experimental studies of defects in Ge, Si, then many other semiconductor materials have generated a huge database of measured quantities that allowed theorists to test their methods and approximations. Dramatic improvement in methodology, especially density-functional theory, along with inexpensive and fast computers, has impedance matched the experimentalist and theorist in ways unanticipated before the late 1980s. As a result, the theory of defects in semiconductors has become quantitative in many respects. Today, more powerful theoretical approaches are still being developed. More importantly perhaps, the tools developed to study defects in semiconductors are now being adapted to approach many new challenges associated with nanoscience, a very long list that includes quantum dots, buckyballs and buckytubes, spintronics, interfaces, and many others. Despite the importance of the ﬁeld, there have been no modern attempts to treat the computational science of the ﬁeld in a coherent manner within a single treatise. This is the aim of the present volume. This book brings together several leaders in theoretical research on defects in semiconductors. Although the treatment is tutorial, the level at which the various applications are discussed is today’s state-of-the-art in the ﬁeld. The book begins with a “big picture” view from Manuel Cardona, and continues with a brief summary of the historical development of the subject in Chap. 1. This includes an overview of today’s most commonly used method to describe defects. We have attempted to create a balanced and tutorial treatment of the basic theory and methodology in Chaps. 3–6. They include detailed discussions of the approximations involved, the calculation of electrically active levels, and extensions of the theory to ﬁnite temperatures. Two emerging electronic structure methodologies of special importance to the ﬁeld are discussed in Chaps. 7 (quantum Monte-Carlo) and 8 (the GW method). Then come two chapters on molecular dynamics (MD). In Chap. 9, a combination of high-

VIII

Preface

level and approximate MD is developed, with applications to the dynamics of extended defect. Chapter 10 deals with semiempirical treatments of microstructures, including issues such as wafer bonding. The book concludes with studies of defects and their role in the photoresponse of topologically disordered (amorphous) systems. The intended audience for the book is graduate students as well as advanced researchers in physics, chemistry, materials science, and engineering. We have sought to provide self-contained descriptions of the work, with detailed references available when needed. The book may be used as a text in a practical graduate course designed to prepare students for research work on defects in semiconductors or ﬁrst-principles theory in materials science in general. The book also serves as a reference for the active theoretical researcher, or as a convenient guide for the experimentalist to keep tabs on their theorist colleagues. It was a genuine pleasure to edit this volume. We are delighted with the contributions provided in a timely fashion by so many busy and accomplished people. We warmly thank all the contributors and hope to have the opportunity to share some nice wine(s) with all of them soon. After all, When Ptolemy, now long ago, Believed the Earth stood still, He never would have blundered so Had he but drunk his ﬁll. He’d then have felt it circulate And would have learnt to say: The true way to investigate Is to drink a bottle a day. (author unknown) published in Augustus de Morgan’s A Budget of Paradoxes, (1866). Athens, Ohio, Lubbock, Texas February 2006

David A. Drabold Stefan K. Estreicher

Contents

Foreword Manuel Cardona . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 1 Early History and Contents of the Present Volume . . . . . . . . . . . . . . . 1 2 Bibliometric Studies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9 Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10 Defect Theory: An Armchair History David A. Drabold, Stefan K. Estreicher . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 The Evolution of Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 A Sketch of First-Principles Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Single-Particle Methods: History . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Direct Approaches to the Many-Electron Problem . . . . . . . . . . . 3.3 Hartree and Hartree–Fock Approximations . . . . . . . . . . . . . . . . . 3.4 Density-Functional Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4.1 Thomas–Fermi Model . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4.2 Modern Density-Functional Theory . . . . . . . . . . . . . . . . . . 4 The Contributions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Supercell Methods for Defect Calculations Risto M. Nieminen . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Density-Functional Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Supercell and Other Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Issues with the Supercell Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 The Exchange-Correlation Functionals and the Semiconducting Gap . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Core and Semicore Electrons: Pseudopotentials and Beyond . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7 Basis Sets . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8 Time-Dependent and Finite-Temperature Simulations . . . . . . . . . . . . 9 Jahn–Teller Distortions in Semiconductor Defects . . . . . . . . . . . . . . .

11 11 13 16 17 18 18 19 19 20 22 23 26 29 29 31 32 34 36 40 42 43 44

X

Contents

9.1 Vacancy in Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.2 Substitutional Copper in Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . 10 Vibrational Modes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11 Ionization Levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12 The Marker Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 13 Brillouin-Zone Sampling . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14 Charged Defects and Electrostatic Corrections . . . . . . . . . . . . . . . . . . 15 Energy-Level References and Valence-Band Alignment . . . . . . . . . . . 16 Examples: The Monovacancy and Substitutional Copper in Silicon . 16.1 Experiments . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 16.2 Calculations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 17 Summary and Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

45 46 47 48 50 51 52 55 56 56 58 60 61 64

Marker-Method Calculations for Electrical Levels Using Gaussian-Orbital Basis Sets J.P. Goss, M.J. Shaw,, P.R. Briddon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Computational Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Gaussian Basis Set . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 Choice of Exponents . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3 Case Study: Bulk Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4 Charge-Density Expansions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Electrical Levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Formation Energy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Calculation of Electrical Levels Using the Marker Method . . . . 4 Application to Defects in Group-IV Materials . . . . . . . . . . . . . . . . . . . 4.1 Chalcogen–Hydrogen Donors in Silicon . . . . . . . . . . . . . . . . . . . . 4.2 VO Centers in Silicon and Germanium . . . . . . . . . . . . . . . . . . . . 4.3 Shallow and Deep Levels in Diamond . . . . . . . . . . . . . . . . . . . . . . 5 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

69 69 71 72 75 76 80 80 81 83 84 84 86 87 89 90 92

Dynamical Matrices and Free Energies Stefan K. Estreicher, Mahdi Sanati . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Dynamical Matrices . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Local and Pseudolocal Modes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Vibrational Lifetimes and Decay Channels . . . . . . . . . . . . . . . . . . . . . . 5 Vibrational Free Energies and Speciﬁc Heats . . . . . . . . . . . . . . . . . . . . 6 Theory of Defects at Finite Temperatures . . . . . . . . . . . . . . . . . . . . . . 7 Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

95 95 97 99 100 101 105 108 110

Contents

XI

Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 112 The Calculation of Free-Energies in Semiconductors: Defects, Transitions and Phase Diagrams E. R. Hern´ andez, A. Antonelli, L. Colombo, P. Ordej´ on . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 The Calculation of Free-Energies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Thermodynamic Integration and Adiabatic Switching . . . . . . . 2.2 Reversible Scaling . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3 Phase Boundaries and Phase Diagrams . . . . . . . . . . . . . . . . . . . . 3 Applications . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Thermal Properties of Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Melting of Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.3 Phase Diagrams . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Conclusions and Outlook . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Quantum Monte Carlo Techniques and Defects in Semiconductors R. J. Needs . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Quantum Monte Carlo Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 The VMC Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 The DMC Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3 Trial Wavefunctions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4 Optimization of Trial Wavefunctions . . . . . . . . . . . . . . . . . . . . . . 2.5 QMC Calculations within Periodic Boundary Conditions . . . . . 2.6 Using Pseudopotentials in QMC Calculations . . . . . . . . . . . . . . . 3 DMC Calculations for Excited States . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Sources of Error in DMC Calculations . . . . . . . . . . . . . . . . . . . . . . . . . 5 Applications of QMC to the Cohesive Energies of Solids . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Applications of QMC to Defects in Semiconductors . . . . . . . . . . . . . . 6.1 Using Structures from Simpler Methods . . . . . . . . . . . . . . . . . . . 6.2 Silicon Self-Interstitial Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.2.1 DFT Calculations on Silicon Self-Interstitials . . . . . . . . . 6.2.2 QMC Calculations on Silicon Self-Interstitials . . . . . . . . . 6.3 Neutral Vacancy in Diamond . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.1 VMC and DMC Calculations on the Neutral Vacancy in Diamond . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.4 Schottky Defects in Magnesium Oxide . . . . . . . . . . . . . . . . . . . . . 7 Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

115 115 116 117 120 122 125 125 128 132 136 136 138

141 141 142 143 144 146 147 147 148 149 149 150 151 151 152 154 156 157 157 158 160 161 163

XII

Contents

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces Arno Schindlmayr, Matthias Scheﬄer . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Computational Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Density-Functional Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 Many-Body Perturbation Theory . . . . . . . . . . . . . . . . . . . . . . . . . 3 Electronic Structure of Defect-Free Surfaces . . . . . . . . . . . . . . . . . . . . 4 Defect States . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 Charge-Transition Levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

165 165 168 168 171 176 179 184 187 188 190

Multiscale Modeling of Defects in Semiconductors: A Novel Molecular-Dynamics Scheme G´ abor Cs´ anyi, Gianpietro Moras, James R. Kermode, Michael C. Payne, Alison Mainwood, Alessandro De Vita . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 A Hybrid View . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Hybrid Simulation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 The LOTF Scheme . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 Applications . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

193 193 194 197 200 203 210 210 211

Empirical Molecular Dynamics: Possibilities, Requirements, and Limitations Kurt Scheerschmidt . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction: Why Empirical Molecular Dynamics? . . . . . . . . . . . . . . 2 Empirical Molecular Dynamics: Basic Concepts . . . . . . . . . . . . . . . . . 2.1 Newtonian Equations and Numerical Integration . . . . . . . . . . . . 2.2 Particle Mechanics and Nonequilibrium Systems . . . . . . . . . . . . 2.3 Boundary Conditions and System Control . . . . . . . . . . . . . . . . . 2.4 Many-Body Empirical Potentials and Force Fields . . . . . . . . . . 2.5 Determination of Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Extensions of the Empirical Molecular Dynamics . . . . . . . . . . . . . . . . 3.1 Modiﬁed Boundary Conditions: Elastic Embedding . . . . . . . . . . 3.2 Tight-Binding-Based Analytic Bond-Order Potentials . . . . . . . 4 Applications . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1 Quantum Dots: Relaxation, Reordering, and Stability . . . . . . . 4.2 Bonded Interfaces: Tailoring Electronic or Mechanical Properties? . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 Conclusions and Outlook . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

213 213 216 216 218 220 221 224 225 225 227 230 231 233 236

Contents

XIII

References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 237 Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 241 Defects in Amorphous Semiconductors: Amorphous Silicon D.A. Drabold, T.A. Abtew . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Amorphous Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Defects in Amorphous Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Deﬁnition of Defect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Long-Time Dynamics and Defect Equilibria . . . . . . . . . . . . . . . . 3.3 Electronic Aspects of Amorphous Semiconductors . . . . . . . . . . . 3.4 Electron Correlation Energy: Electron–Electron Eﬀects . . . . . . 4 Modeling Amorphous Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1 Forming Structural Models . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2 Interatomic Potentials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.3 Lore of Approximations in Density-Functional Calculations . . 4.4 The Electron–Lattice Interaction . . . . . . . . . . . . . . . . . . . . . . . . . 5 Defects in Amorphous Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Light Induced Eﬀects in Amorphous and Glassy Solids S. I. Simdyankin, S. R. Elliott . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Photoinduced Metastability in Amorphous Solids: An Experimental Survey . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.2 Photoinduced Eﬀects in Chalcogenide Glasses . . . . . . . . . . . . . . 2 Theoretical Studies of Photoinduced Excitations in Amorphous Materials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Application of the Density-Functional-Based Tight-Binding Method to the Case of Amorphous As2 S3 . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

245 245 246 248 248 250 250 252 253 253 255 255 257 258 264 266 269 269 269 271 272 273 283 285

Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 287

This book is dedicated to Manuel Cardona, who has done so much for the ﬁeld of defects in semiconductors over the past decades, and convinced so many theorists to calculate beyond what they thought possible.

Preface

Semiconductor materials emerged after World War II and their impact on our lives has grown ever since. Semiconductor technology is, to a large extent, the art of defect engineering. Today, defect control is often done at the atomic level. Theory has played a critical role in understanding, and therefore controlling, the properties of defects. Conversely, the careful experimental studies of defects in Ge, Si, then many other semiconductor materials have generated a huge database of measured quantities that allowed theorists to test their methods and approximations. Dramatic improvement in methodology, especially density-functional theory, along with inexpensive and fast computers, has impedance matched the experimentalist and theorist in ways unanticipated before the late 1980s. As a result, the theory of defects in semiconductors has become quantitative in many respects. Today, more powerful theoretical approaches are still being developed. More importantly perhaps, the tools developed to study defects in semiconductors are now being adapted to approach many new challenges associated with nanoscience, a very long list that includes quantum dots, buckyballs and buckytubes, spintronics, interfaces, and many others. Despite the importance of the ﬁeld, there have been no modern attempts to treat the computational science of the ﬁeld in a coherent manner within a single treatise. This is the aim of the present volume. This book brings together several leaders in theoretical research on defects in semiconductors. Although the treatment is tutorial, the level at which the various applications are discussed is today’s state-of-the-art in the ﬁeld. The book begins with a “big picture” view from Manuel Cardona, and continues with a brief summary of the historical development of the subject in Chap. 1. This includes an overview of today’s most commonly used method to describe defects. We have attempted to create a balanced and tutorial treatment of the basic theory and methodology in Chaps. 3–6. They include detailed discussions of the approximations involved, the calculation of electrically active levels, and extensions of the theory to ﬁnite temperatures. Two emerging electronic structure methodologies of special importance to the ﬁeld are discussed in Chaps. 7 (quantum Monte-Carlo) and 8 (the GW method). Then come two chapters on molecular dynamics (MD). In Chap. 9, a combination of high-

VIII

Preface

level and approximate MD is developed, with applications to the dynamics of extended defect. Chapter 10 deals with semiempirical treatments of microstructures, including issues such as wafer bonding. The book concludes with studies of defects and their role in the photoresponse of topologically disordered (amorphous) systems. The intended audience for the book is graduate students as well as advanced researchers in physics, chemistry, materials science, and engineering. We have sought to provide self-contained descriptions of the work, with detailed references available when needed. The book may be used as a text in a practical graduate course designed to prepare students for research work on defects in semiconductors or ﬁrst-principles theory in materials science in general. The book also serves as a reference for the active theoretical researcher, or as a convenient guide for the experimentalist to keep tabs on their theorist colleagues. It was a genuine pleasure to edit this volume. We are delighted with the contributions provided in a timely fashion by so many busy and accomplished people. We warmly thank all the contributors and hope to have the opportunity to share some nice wine(s) with all of them soon. After all, When Ptolemy, now long ago, Believed the Earth stood still, He never would have blundered so Had he but drunk his ﬁll. He’d then have felt it circulate And would have learnt to say: The true way to investigate Is to drink a bottle a day. (author unknown) published in Augustus de Morgan’s A Budget of Paradoxes, (1866). Athens, Ohio, Lubbock, Texas February 2006

David A. Drabold Stefan K. Estreicher

Contents

Foreword Manuel Cardona . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 1 Early History and Contents of the Present Volume . . . . . . . . . . . . . . . 1 2 Bibliometric Studies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9 Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10 Defect Theory: An Armchair History David A. Drabold, Stefan K. Estreicher . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 The Evolution of Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 A Sketch of First-Principles Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Single-Particle Methods: History . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Direct Approaches to the Many-Electron Problem . . . . . . . . . . . 3.3 Hartree and Hartree–Fock Approximations . . . . . . . . . . . . . . . . . 3.4 Density-Functional Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4.1 Thomas–Fermi Model . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4.2 Modern Density-Functional Theory . . . . . . . . . . . . . . . . . . 4 The Contributions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Supercell Methods for Defect Calculations Risto M. Nieminen . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Density-Functional Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Supercell and Other Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Issues with the Supercell Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 The Exchange-Correlation Functionals and the Semiconducting Gap . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Core and Semicore Electrons: Pseudopotentials and Beyond . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7 Basis Sets . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8 Time-Dependent and Finite-Temperature Simulations . . . . . . . . . . . . 9 Jahn–Teller Distortions in Semiconductor Defects . . . . . . . . . . . . . . .

11 11 13 16 17 18 18 19 19 20 22 23 26 29 29 31 32 34 36 40 42 43 44

X

Contents

9.1 Vacancy in Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.2 Substitutional Copper in Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . 10 Vibrational Modes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11 Ionization Levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12 The Marker Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 13 Brillouin-Zone Sampling . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14 Charged Defects and Electrostatic Corrections . . . . . . . . . . . . . . . . . . 15 Energy-Level References and Valence-Band Alignment . . . . . . . . . . . 16 Examples: The Monovacancy and Substitutional Copper in Silicon . 16.1 Experiments . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 16.2 Calculations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 17 Summary and Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

45 46 47 48 50 51 52 55 56 56 58 60 61 64

Marker-Method Calculations for Electrical Levels Using Gaussian-Orbital Basis Sets J.P. Goss, M.J. Shaw,, P.R. Briddon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Computational Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Gaussian Basis Set . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 Choice of Exponents . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3 Case Study: Bulk Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4 Charge-Density Expansions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Electrical Levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Formation Energy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Calculation of Electrical Levels Using the Marker Method . . . . 4 Application to Defects in Group-IV Materials . . . . . . . . . . . . . . . . . . . 4.1 Chalcogen–Hydrogen Donors in Silicon . . . . . . . . . . . . . . . . . . . . 4.2 VO Centers in Silicon and Germanium . . . . . . . . . . . . . . . . . . . . 4.3 Shallow and Deep Levels in Diamond . . . . . . . . . . . . . . . . . . . . . . 5 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

69 69 71 72 75 76 80 80 81 83 84 84 86 87 89 90 92

Dynamical Matrices and Free Energies Stefan K. Estreicher, Mahdi Sanati . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Dynamical Matrices . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Local and Pseudolocal Modes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Vibrational Lifetimes and Decay Channels . . . . . . . . . . . . . . . . . . . . . . 5 Vibrational Free Energies and Speciﬁc Heats . . . . . . . . . . . . . . . . . . . . 6 Theory of Defects at Finite Temperatures . . . . . . . . . . . . . . . . . . . . . . 7 Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

95 95 97 99 100 101 105 108 110

Contents

XI

Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 112 The Calculation of Free-Energies in Semiconductors: Defects, Transitions and Phase Diagrams E. R. Hern´ andez, A. Antonelli, L. Colombo, P. Ordej´ on . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 The Calculation of Free-Energies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Thermodynamic Integration and Adiabatic Switching . . . . . . . 2.2 Reversible Scaling . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3 Phase Boundaries and Phase Diagrams . . . . . . . . . . . . . . . . . . . . 3 Applications . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Thermal Properties of Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Melting of Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.3 Phase Diagrams . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Conclusions and Outlook . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Quantum Monte Carlo Techniques and Defects in Semiconductors R. J. Needs . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Quantum Monte Carlo Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 The VMC Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 The DMC Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3 Trial Wavefunctions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4 Optimization of Trial Wavefunctions . . . . . . . . . . . . . . . . . . . . . . 2.5 QMC Calculations within Periodic Boundary Conditions . . . . . 2.6 Using Pseudopotentials in QMC Calculations . . . . . . . . . . . . . . . 3 DMC Calculations for Excited States . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Sources of Error in DMC Calculations . . . . . . . . . . . . . . . . . . . . . . . . . 5 Applications of QMC to the Cohesive Energies of Solids . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Applications of QMC to Defects in Semiconductors . . . . . . . . . . . . . . 6.1 Using Structures from Simpler Methods . . . . . . . . . . . . . . . . . . . 6.2 Silicon Self-Interstitial Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.2.1 DFT Calculations on Silicon Self-Interstitials . . . . . . . . . 6.2.2 QMC Calculations on Silicon Self-Interstitials . . . . . . . . . 6.3 Neutral Vacancy in Diamond . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.1 VMC and DMC Calculations on the Neutral Vacancy in Diamond . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.4 Schottky Defects in Magnesium Oxide . . . . . . . . . . . . . . . . . . . . . 7 Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

115 115 116 117 120 122 125 125 128 132 136 136 138

141 141 142 143 144 146 147 147 148 149 149 150 151 151 152 154 156 157 157 158 160 161 163

XII

Contents

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces Arno Schindlmayr, Matthias Scheﬄer . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Computational Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Density-Functional Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 Many-Body Perturbation Theory . . . . . . . . . . . . . . . . . . . . . . . . . 3 Electronic Structure of Defect-Free Surfaces . . . . . . . . . . . . . . . . . . . . 4 Defect States . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 Charge-Transition Levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

165 165 168 168 171 176 179 184 187 188 190

Multiscale Modeling of Defects in Semiconductors: A Novel Molecular-Dynamics Scheme G´ abor Cs´ anyi, Gianpietro Moras, James R. Kermode, Michael C. Payne, Alison Mainwood, Alessandro De Vita . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 A Hybrid View . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Hybrid Simulation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 The LOTF Scheme . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 Applications . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

193 193 194 197 200 203 210 210 211

Empirical Molecular Dynamics: Possibilities, Requirements, and Limitations Kurt Scheerschmidt . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction: Why Empirical Molecular Dynamics? . . . . . . . . . . . . . . 2 Empirical Molecular Dynamics: Basic Concepts . . . . . . . . . . . . . . . . . 2.1 Newtonian Equations and Numerical Integration . . . . . . . . . . . . 2.2 Particle Mechanics and Nonequilibrium Systems . . . . . . . . . . . . 2.3 Boundary Conditions and System Control . . . . . . . . . . . . . . . . . 2.4 Many-Body Empirical Potentials and Force Fields . . . . . . . . . . 2.5 Determination of Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Extensions of the Empirical Molecular Dynamics . . . . . . . . . . . . . . . . 3.1 Modiﬁed Boundary Conditions: Elastic Embedding . . . . . . . . . . 3.2 Tight-Binding-Based Analytic Bond-Order Potentials . . . . . . . 4 Applications . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1 Quantum Dots: Relaxation, Reordering, and Stability . . . . . . . 4.2 Bonded Interfaces: Tailoring Electronic or Mechanical Properties? . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5 Conclusions and Outlook . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

213 213 216 216 218 220 221 224 225 225 227 230 231 233 236

Contents

XIII

References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 237 Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 241 Defects in Amorphous Semiconductors: Amorphous Silicon D.A. Drabold, T.A. Abtew . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 Amorphous Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Defects in Amorphous Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Deﬁnition of Defect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Long-Time Dynamics and Defect Equilibria . . . . . . . . . . . . . . . . 3.3 Electronic Aspects of Amorphous Semiconductors . . . . . . . . . . . 3.4 Electron Correlation Energy: Electron–Electron Eﬀects . . . . . . 4 Modeling Amorphous Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1 Forming Structural Models . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2 Interatomic Potentials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.3 Lore of Approximations in Density-Functional Calculations . . 4.4 The Electron–Lattice Interaction . . . . . . . . . . . . . . . . . . . . . . . . . 5 Defects in Amorphous Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Light Induced Eﬀects in Amorphous and Glassy Solids S. I. Simdyankin, S. R. Elliott . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 Photoinduced Metastability in Amorphous Solids: An Experimental Survey . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.2 Photoinduced Eﬀects in Chalcogenide Glasses . . . . . . . . . . . . . . 2 Theoretical Studies of Photoinduced Excitations in Amorphous Materials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Application of the Density-Functional-Based Tight-Binding Method to the Case of Amorphous As2 S3 . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

245 245 246 248 248 250 250 252 253 253 255 255 257 258 264 266 269 269 269 271 272 273 283 285

Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 287

This book is dedicated to Manuel Cardona, who has done so much for the ﬁeld of defects in semiconductors over the past decades, and convinced so many theorists to calculate beyond what they thought possible.

Preface

Semiconductor materials emerged after World War II and their impact on our lives has grown ever since. Semiconductor technology is, to a large extent, the art of defect engineering. Today, defect control is often done at the atomic level. Theory has played a critical role in understanding, and therefore controlling, the properties of defects. Conversely, the careful experimental studies of defects in Ge, Si, then many other semiconductor materials have generated a huge database of measured quantities that allowed theorists to test their methods and approximations. Dramatic improvement in methodology, especially density-functional theory, along with inexpensive and fast computers, has impedance matched the experimentalist and theorist in ways unanticipated before the late 1980s. As a result, the theory of defects in semiconductors has become quantitative in many respects. Today, more powerful theoretical approaches are still being developed. More importantly perhaps, the tools developed to study defects in semiconductors are now being adapted to approach many new challenges associated with nanoscience, a very long list that includes quantum dots, buckyballs and buckytubes, spintronics, interfaces, and many others. Despite the importance of the ﬁeld, there have been no modern attempts to treat the computational science of the ﬁeld in a coherent manner within a single treatise. This is the aim of the present volume. This book brings together several leaders in theoretical research on defects in semiconductors. Although the treatment is tutorial, the level at which the various applications are discussed is today’s state-of-the-art in the ﬁeld. The book begins with a “big picture” view from Manuel Cardona, and continues with a brief summary of the historical development of the subject in Chap. 1. This includes an overview of today’s most commonly used method to describe defects. We have attempted to create a balanced and tutorial treatment of the basic theory and methodology in Chaps. 3–6. They include detailed discussions of the approximations involved, the calculation of electrically active levels, and extensions of the theory to ﬁnite temperatures. Two emerging electronic structure methodologies of special importance to the ﬁeld are discussed in Chaps. 7 (quantum Monte-Carlo) and 8 (the GW method). Then come two chapters on molecular dynamics (MD). In Chap. 9, a combination of high-

VIII

Preface

level and approximate MD is developed, with applications to the dynamics of extended defect. Chapter 10 deals with semiempirical treatments of microstructures, including issues such as wafer bonding. The book concludes with studies of defects and their role in the photoresponse of topologically disordered (amorphous) systems. The intended audience for the book is graduate students as well as advanced researchers in physics, chemistry, materials science, and engineering. We have sought to provide self-contained descriptions of the work, with detailed references available when needed. The book may be used as a text in a practical graduate course designed to prepare students for research work on defects in semiconductors or ﬁrst-principles theory in materials science in general. The book also serves as a reference for the active theoretical researcher, or as a convenient guide for the experimentalist to keep tabs on their theorist colleagues. It was a genuine pleasure to edit this volume. We are delighted with the contributions provided in a timely fashion by so many busy and accomplished people. We warmly thank all the contributors and hope to have the opportunity to share some nice wine(s) with all of them soon. After all, When Ptolemy, now long ago, Believed the Earth stood still, He never would have blundered so Had he but drunk his ﬁll. He’d then have felt it circulate And would have learnt to say: The true way to investigate Is to drink a bottle a day. (author unknown) published in Augustus de Morgan’s A Budget of Paradoxes, (1866). Athens, Ohio, Lubbock, Texas February 2006

David A. Drabold Stefan K. Estreicher

Foreword Manuel Cardona Max-Planck-Institut f¨ ur Festk¨ orperforschung, 70569 Stuttgart, Germany [email protected]

Man sollte sich mit Halbleitern nicht besch¨ aftigen, das sind Dreckeﬀekte – wer weiss, ob sie wirklich existieren. Wolfgang Pauli, 1931

1 Early History and Contents of the Present Volume This volume contains a comprehensive description of developments in the ﬁeld of defects in semiconductors that have taken place during the past two decades. Although the ﬁeld of defects in semiconductors is at least 60 years old, it had to wait, in order to reach maturity, for the colossal increase in computer power that has more recently taken place, following the predictions of Moore’s law [1]. The ingenuity of computational theorists in developing algorithms to reduce the intractable many-body problem of defect and host to one that can be handled with existing and aﬀordable computer power has also played a signiﬁcant role: much of it is described in the present volume. As computational power grew, the simplifying assumptions of these algorithms, some of them hard to justify, were reduced. The predictive accuracy of the new calculations then took a great leap forward. In the early days, the real-space structure of the defect had to be postulated in order to get on with the theory and self-consistency of the electronic calculations was beyond reach. During the past two decades emphasis has been placed in calculating the real-space structure of defect plus host and achieving self-consistency in the electronic calculations. The results of these new calculations have been a great help to experimentalists groping to interpret complicated data related to defects. I have added up the number of references in the various chapters of the book corresponding to years before 1990 and found that they amount to only 25 % of the total number of references. Many of the remaining 75 % of references are actually even more recent, having been published after the year 2000. Thus one can say that the contents of the volume represent the state-of-the-art in the ﬁeld. Whereas most of the chapters are concerned with defects in crystalline semiconductors, Chaps. 10 and 11 deal with defects in amorphous materials, in particular amorphous silicon, a ﬁeld about which much less information is available. D. A. Drabold, S. K. Estreicher (Eds.): Theory of Defects in Semiconductors, Topics Appl. Physics 104, 1–10 (2007) © Springer-Verlag Berlin Heidelberg 2007

2

Manuel Cardona

The three aspects of the defect problem, real-space structure, electronic structure and vibrational properties are discussed in the various Chapters of the book, mainly from the theoretical point of view. Defects break the translational symmetry of a crystal, a property that already made possible rather realistic calculations of the host materials half a century ago. Small crystals and clusters with a relatively small number of atoms (including impurities and other defects), have become useful to circumvent, in theoretical calculations, the lack of translational symmetry in the presence of defects or in amorphous materials. The main source of uncertainty in the state-ofthe-art calculations remains the small number of cluster atoms imposed by the computational strictures. This number is often smaller than that corresponding to real-world samples, even including nanostructures. Clusters with a number of atoms that can be accommodated by extant computers are then repeated periodically so as to obtain a crystal lattice, with a supercell and a mini-Brillouin zone. Although these lattices do not exactly correspond to physical reality, they enable the use of k-space techniques and are instrumental in keeping computer power to available and aﬀordable levels. Another widespread approach is to treat the cluster in real space after passivating the ﬁctitious surface with hydrogen atoms or the like. When using these methods it is good practice to check convergence with respect to the cluster size by performing similar calculations for at least two sets of clusters with numbers of atoms diﬀering, say, by a factor of two. The epigraph above, attributed to Wolfgang Pauli, translates as One should not keep busy with semiconductors, they are dirt eﬀects – Who knows whether they really exist. The 24 authors of this book, like many tens of thousands of other physicists and engineers, have fortunately not heeded Pauli’s advice (given in 1931, 14 years before he received the Nobel Prize). Had they done so, not only would the world have missed a revolutionary and nowadays ubiquitous technology, but basic physical science would have lost some of the most fruitful, beautiful and successful applications of quantum mechanics. “Dreckeﬀekte” is often imprecisely translated as eﬀects of dirt, i.e., as eﬀects of impurities. However, eﬀects of structural defects would also fall into the category of Dreckeﬀekte. In Pauli’s days applications of semiconductors, including variation of resistivity through doping leading to photocells and rectiﬁers, had been arrived at purely empirically, through some sort of trial and error alchemy. I remember as a child using galena (PbS) detectors in crystal radio sets. I had lots of galena from various sources: some of it worked, some not but nobody seemed to know why. Sixty years later, only a few months ago, I was measuring PbS samples in order to characterize the number of carriers (of nonstoichiometric origin involving vacancies) and their type (n or p) so as to wrap up original research on this canonical material [2]. Today, GOOGLE lists 860 000 entries under the heading “defects in

Foreword

3

semiconductors”. The Web of Science (WoS) lists 3736 mentions in the title and abstract of source articles1 . The modern science of defects in semiconductors is closely tied to the invention of the transistor at Bell Laboratories in 1948 (by Bardeen, Shockley and Brattain [3], Physics Nobel laureates for 1956). Early developments took place mainly in the United States, in particular at Bell Laboratories, the Lincoln Lab (MIT) and Purdue University. Karl Lark-Horovitz, an Austrian immigrant, started at Purdue a program to investigate the growth and doping (n- and p-type) of germanium and all sorts of electrical and optical properties of this element in crystalline form [4]. The initial motivation was the development of germanium detectors for radar applications. During the years 1928 till his untimely death in 1958 he built up the Physics Department at Purdue into the foremost center of academic semiconductor research. Work similar to that at Purdue for germanium was carried out at Bell Labs, also as a spinoﬀ of the development of silicon rectiﬁers during World War II. At Bell, Scaﬀ et al. [5] discovered that crystalline silicon could be made n- or p-type by doping with atoms of the ﬁfth (P, As, Sb) or the third (B, Al, Ga, In) column of the periodic table, respectively. n-type dopants were called donors, p-type ones acceptors. Pearson and Bardeen performed a rather extensive investigation of the electrical properties of intrinsic and doped silicon [6]. These authors proposed the simplest possible expression for estimating the binding energy of the so-called hydrogenic energy levels of those impurities: The ionization energy of the hydrogen atom (13.6 eV) had to be divided by the square of the static dielectric constant ( = 12 for silicon) and multiplied by an eﬀective mass (typical values m∗ ≈ 0.1) that simulated the presence of a crystalline potential. According to this Ansatz, all donors (acceptors) would have the same binding energy, a fact that we now know is only approximately true (see Fig. 5 of Chap. 3 for diamond). The simple hydrogenic Ansatz applies to semiconductors with isotropic extrema, so that a unique eﬀective mass can be deﬁned (e.g., n-type GaAs). It does not apply to electrons in either Ge or Si because the conduction-band extrema are strongly anisotropic. The hydrogen-like Schr¨ odinger equation can, however, be modiﬁed so as to include anisotropic masses, as apply to germanium and silicon [7]. The maximum of the valence bands of most diamond and zincblende-like semiconductors occurs at or very close to k = 0. It is fourfold degenerate in the presence of spin-orbit interaction and sixfold if such interaction is neglected [8]. The simple Schr¨ odinger equation of the hydrogen atom must be replaced by a set of four coupled equations (with spin-orbit coupling) with eﬀective-mass parameters to be empirically determined [9]. Extensive applications of Kohn’s prescriptions were performed by several Italian theorists [10]. 1

A source article is one published in a Source Journal as deﬁned by the ISIThomson Scientiﬁc. There are about 6000 such journals, including all branches of science.

4

Manuel Cardona

In the shallow (hydrogenic) level calculations based on eﬀective-mass Hamiltonians the calculated impurity eigenvalues are automatically referred to the corresponding band edges, thus obviating the need for using a marker, of the type discussed in Chap. 3 of this book. This marker was introduced in order to avoid errors inherent to the “ﬁrst-principles” calculations, such as those related to the so-called “gap problem” found when using local-density functionals to represent many-body exchange and correlation. For a way to palliate this problem using the so-called GW approximation see Chap. 7, where defects at surfaces are treated. We have discussed so far the electronic levels of shallow substitutional impurities. In this volume a number of other defects, such as vacancies, interstitial impurities, clusters, etc., will be encountered. Energy levels related to structural defects were ﬁrst discussed by Lark-Horovitz and coworkers [11]. These levels were produced by irradiation with either deuterons, alpha particles or neutrons. After irradiation, the material became more p-type. It was thus postulated that the defect levels introduced by the bombardment were acceptors (vacancies?). It was also discovered by Lark-Horovitz that neutron bombardment, followed by annealing in order to reduce structural damage, could be used to create electrically active impurities by nuclear transmutation [12]. The small amount of the 30Si isotope (≈ 4 %) present in natural Si converts, by neutron capture, into radioactive 31Si, which decays through β-emission into stable 31 P, a donor. This technique is still commercially used nowadays for producing very uniform doping concentrations. Since Kohn–Luttinger perturbation theory predicts reasonably well the electronic levels of shallow impurities (except for the so-called central-cell corrections [13]) this book covers mainly deep impurity levels that not only are diﬃcult to calculate for a given real-space structure but also require relaxation of the unperturbed host crystal around the defect. Among these deep levels, native defects such as vacancies and self-interstitials are profusely discussed. Most of these levels are related to transition-metal atoms, such as Mn, Cu, and Au (I call Au and Cu transition metals for obvious reasons). The solubility of these transition-metal impurities is usually rather low (less than 1015 cm−3 . Exceptions: Cd1 − x Mnx Te and related alloys). They can go into the host lattice either as substitutional or as interstitial atoms,2 a point that can be clariﬁed with EPR and also with ab initio total-energy calculations. These dopants were used in early applications in order to reduced the residual conductivity due to shallow levels (because of the fact that transition-metal impurities have levels close to the middle of the gap). One can even nowadays ﬁnd in the market semi-insulating GaAs obtained by doping with chromium. 2

The reader who tries to do a literature search for interstitial gold may be surprised by the existence of homonyms: Interstitial gold is important in the treatment of prostate cancer. It has, of course, nothing to do with our interstitial gold. See [14].

Foreword

5

I remember having obtained in 1957 semi-insulating germanium and silicon (doped with either Mn or Au) with carrier concentrations lower than intrinsic (this makes a good exam question!). They were used for measurements of the low-frequency dielectric constants of these materials, in particular vs. temperature and pressure [15] while I was working at Harvard on my PhD under W. Paul. Rough estimates of the positions of deep levels of many impurity elements in the gap of group IV and III–V semiconductors were obtained by Hjalmarson et al. [8, 16] using Green’s function methods. In the case of GaAs and related materials, two kinds of defect complexes, involving structural changes and metastability have received a lot of attention because of technological implications: the so-called EL2 and DX centers. Searching the Web of Science for EL2 one ﬁnds 1055 mentions in abstracts and titles of source articles. Likewise 695 mentions are found for the DX centers. Chadi and coworkers have obtained theoretical predictions for the structure of these centers and their metastability [17, 18]. Although these theoretical models explain a number of observations related to these centers, there is not yet a general consensus concerning their structures. An aspect of the defect problem that has not been dealt with explicitly in this volume is the errors introduced by using nonrelativistic Schr¨ odinger equations, in particular the neglect of mass–velocity corrections and spin– orbit interaction (the latter, however, is explicitly included in the Kohn– Luttinger Hamiltonian, either in its 4 × 4 or its 6 × 6 version). Discrepancies between calculated and measured gaps are attributed to the “gap problem” inherent in the local-density approximation (LDA). However, already for relatively heavy atoms (Ge, GaAs) the mass–velocity correction decreases the s–like conduction levels and, together with the LDA gap problem. converts the semiconductor into a metal in the case of germanium. For GaAs it is stated several times in this volume that the LDA calculated gap is about half the experimental one. This is for a nonrelativistic Hamiltonian. Even a scalar relativistic one reduces the gap even further, to about 0.2 eV (experimental gap: 1.52 eV at 4 K) [19]. This indicates that the gap problem is more serious than previously thought on the basis of nonrelativistic LDA calculations. Another relativistic eﬀect is the spin-orbit coupling. For moderately heavy atoms such as Ge, Ga and As the spin-orbit splitting at the top of the valence bands (≈ 0.3 eV) is much larger than the binding energy of hydrogenic acceptors. Hence we can calculate the binding energies of the latter by solving the decoupled 4 × 4 (J = 3/2) and 2 × 2 (J = 1/2) eﬀective-mass equations. This leads to two series of acceptor levels separated by a “spin-orbit” splitting basically equal to that of the band-edge states. In the case of silicon, however, the spin-orbit splitting at k = 0 (∆ = 0.044 eV) is of the order of shallowimpurity binding energies. The impurity potential thus couples the J = 3/2 and J = 1/2 bands and the apparent spin-orbit splitting of the corresponding impurity series becomes smaller than that at the band edges [20, 21]. The diﬀerence between band-edge spin-orbit splitting (∆ = 0.014 eV) and that of

6

Manuel Cardona

the acceptor levels becomes even larger in diamond. Using a simple Green’s functions technique and a Slater–Koster δ-function potential, the impuritylevel splittings have been calculated and found to be indeed much smaller than ∆ = 0.014 eV. This splitting depends strongly on the binding energy of the impurity. Another aspect that has hardly been treated in the present volume (see, however, Chap. 10 for amorphous silicon) is the temperature dependence of the electronic energy levels that is induced by the electron–phonon interaction. Whenever this question appears in this volume, it is assumed that we are in the classical high-temperature limit, in which the corresponding renormalization of electronic gaps and states is proportional to temperature. At low temperatures, the electron–phonon interaction induces a zero-point renormalization of the electronic states that can be estimated from the measured temperature dependence. It is also possible to determine the zero-point renormalization of gaps by measuring samples with diﬀerent isotopic compositions. The interested reader should consult the review by Cardona and Thewalt [22]. When an atom of the host lattice of a semiconductor has several stable isotopes (e.g., diamond, Si, Ge, Ga, Zn samples grown with natural material lose, strictly speaking, their translational symmetry. In the past 15 years a large number of semiconductors have been grown using isotopically pure elements (which have become available in macroscopic and aﬀordable quantities after the fall of the Iron Curtain). A diﬀerent isotope added to an isotopically pure sample can thus be considered as an impurity, probably the simplest kind of defect possible: Only the atomic mass of such an impurity diﬀers from that of the host, the electronic properties remain nearly the same.3 The main effect of isotope mass substitution is found in the vibrational frequencies of host as well as local vibrational modes: such frequencies are inversely proportional to the square root of the vibrating mass (see Chap. 4). Although this eﬀect sounds rather trivial it often induces changes in phonon widths and in the zero-point anharmonic renormalizations (see [22]) that in some cases can be rather drastic and unexpected [23]. The structural relaxation around isotopic impurities is rather small. The main such eﬀect corresponds to an increase of the lattice constant with increasing isotopic mass, about 0.015 % between 12C and 13C diamond. Its origin lies in the change in the zero-point renormalization of the lattice constant: ab initio calculations are available [24]. The third class of eﬀects of the isotopic impurities refers to electronic states and energy gaps and their renormalization on account of the electron– phonon interaction. The zero-point renormalizations also vary as the inverse square root of the relevant isotopic mass. By measuring a gap energy at low temperatures for samples with two diﬀerent isotopic masses, one can 3

Except for the electron–phonon renormalization of the electronic states and gaps that is usually rather small. See [22].

Foreword

7

extrapolate to inﬁnite mass and thus determine the unrenormalized value of the gap. Renormalizations of around 60 meV have been found for Ge and Si. For diamond, however, this renormalization seems to be much larger [25], around 400 meV.4 This large renormalization is a signature of strong electron– phonon interaction that seems to be responsible for the superconductivity recently observed in heavily boron doped (p-type) diamond (Tc higher than 10 K) [26,27]. Ab initio calculations of the electronic and vibronic structure of heavily boron doped diamond have been performed and used for estimating the critical temperature Tc [28].

2 Bibliometric Studies In the previous section I have already discussed the number of times certain topics appear in titles, keywords and abstracts in source journals (about 6000 publications chosen by the ISI among ≈ 100 000, as those that contribute signiﬁcantly to the progress of science). While titles go back to the present starting date of the source journal selection (the year 1900), abstracts and keywords have only been collected since 1990. In the Web of Science (WoS) one can completely eliminate the latter in order to avoid distortions but, for simplicity, I kept them in the qualitative survey presented here. In this section, a more detailed bibliometric analysis will be performed using the WoS that draws on the citation index as the primary database. In order to get a feeling for the standing of the various contributors to this volume, we could simply perform a citations count (it can be done relatively easily within the WoS using the cited reference mode). However, a more taletelling index has been recently suggested by Hirsch [29], the so-called h-index. This index is easily obtained for anyone with access to the WoS going back to the ﬁrst publication of the authors under scrutiny (1974 for Nieminen and Shaw). How far back your access to the WoS goes depends on how much your institution is willing to pay to ISI-Thomson Scientiﬁc. The h-index is obtained by using the general search mode of the WoS and ordering the results of the search for a given individual according to the number of citations (there is a function key to order the author’s contributions from most cited to less cited). You then go down the list till the order number of a paper equals its number of citations (you may have to take one more or less citation if equality does not exist). The number so obtained is the h-index. It rewards more continued, sustained well-cited publications rather than only a couple with a colossal number (such as those that deserve the Nobel Prize). Watch out for possible homonyms although, on the average, they appear seldom. They can be purged by hand if the number of terms is not too high. I had problems with homonyms only for ﬁve out of the 24 (excluding myself) contributors 4

Theorists: beware (and be aware) of this large renormalization when comparing your fancy GW calculations of gaps with experimental data.

8

Manuel Cardona

to this volume (Antonelli, Colombo, Hern´ andez, Sanati and Shaw). I simply excluded them from the count. The average h-factor of the remaining 19 authors is h = 20. Hirsch mentions in [29] that recently elected fellows of the American Physical Society have typically h ≈ 15–20. Advancement of a physicist to full professor at a reputable US university corresponds to h ≥ 18. The high average h already reveals the high standing of the authors of this book. In several cases, the authors involve a senior partner (h ≥ 20, Chaps. 3, 4, 5, 7, 8, 10 and 11) and a junior colleague. I welcome this decision. It is a good procedure for introducing junior researchers to the intricacies and ordeals involved in writing a review article of such extent. In this connection, I should mention that the h-index is roughly proportional to the scientiﬁc age (counted from the ﬁrst publication or the date of the PhD thesis). The values of h given above for faculty and NAS membership are appropriate to physicists and chemists. Biomedical scientists often have, everything else being equal, twice as large h-indices, whereas engineers and mathematicians (especially the latter) have much lower ones. After having discussed the average h-index of our contributors, I would like to mention the range they cover without mentioning speciﬁc names.5 The h-indices of our contributors cover the range 6 ≤ h ≤ 64. Four very junior authors who have not yet had a chance of being cited have been omitted (one could have set h = 0 in their case). Hirsch mentions in his seminal article [29] that election to the National Academy of Sciences of the US is usually associated with h = 45. We therefore must have some potential academicians among our contributors. Because of the ease in the use of the h-algorithm just described and its usefulness to evaluate the “impact” of a scientist’s career, bibliometrists have been looking for other applications of the technique. Instead of people one can apply it to journals (provided they are not too large in terms of published articles), institutions, countries, etc. One has to keep in mind that the resulting h-number always reverts to an analysis of the citations of individuals that are attached to the investigated items (e.g., countries, institutions, etc.). One can also use the algorithm to survey the importance of keywords or title subjects. The present volume has 11 chapters and this gives it a certain (albeit small) statistical value to be of use in such a survey. We thus attach to each chapter title a couple of keywords and evaluate the corresponding h-index entering these under “topic” in the general search mode of the WoS. In the table below we list these words, the number of items we ﬁnd for each set of them and the corresponding h-index. There is considerable arbitrariness in the procedure to choose the keywords but we must keep in mind that these applications are just exploratory and at their very beginning. 5

Mentioning the h-indices of the authors, one by one, may be invidious. The interested reader with access to the WoS can do it by following the prescription given above.

Foreword

9

We display in Table 1 the keywords we have assigned to the eleven chapters, the number of terms citing them and the corresponding h-index that weights them according to the number of times each citing term is cited. One can draw a number of conclusions from this table. Particularly interesting are the low values of n and h for empirical molecular dynamics, which probably signals the turn towards ab initio techniques. Amorphous semiconductors, including defect and the metastabilities induced by illumination plus possibly their applications to photovoltaics are responsible for the large values of n and h. Table 1. Keywords assigned (somewhat arbitrarily) to each of the 11 chapters in the book together with the corresponding number n of source articles citing them in abstract, keywords or title. Also, Hirsch number h that can be assigned to each of the chapters according to the keywords Chapter Keyword (topic in WoS) 1 2 3 4 5 6 7 8 9 10 11

defects and semiconductors supercell calculations Gaussian orbitals dynamical matrix free energy and defect quantum Monte Carlo point defect and surface defect and molecular dynamics empirical molecular dynamics defect and amorphous light and amorphous

n

h

3735 165 190 231 494 2551 426 2023 23 4492 5747

76 27 27 26 36 71 38 67 7 77 87

References [1] G. E. Moore: Electronics 38, 114 (1965) 1 [2] R. Sherwin, R. J. H. Clark, R. Lauck, M. Cardona: Solid State Commun. 134, 265 (2005) 2 [3] J. Bardeen, W. Brattain: Phys. Rev. 74, 230 (1948) 3 [4] K. Lark-Horovitz, V. A. Johnson: Phys. Rev. 69, 258 (1946) 3 [5] J. A. Scaﬀ, H. C. Theuerer, E. E. Schumacher: J. Metals: Trans. Am. Inst. Mining Metall. Eng. 185, 383 (1949) 3 [6] G. L. Pearson, J. Bardeen: Phys. Rev. 75, 865 (1949) 3 [7] W. Kohn, J. M. Luttinger: Phys. Rev. 97, 1721 (1975) 3 [8] P. Y. Yu, M. Cardona: Fundamentals of Semiconductors, vol. 3 (Springer, Berlin, Heidelberg 2005) 3, 5 [9] W. Kohn, D. Schechter: Phys. Rev. 99, 1903 (1955) 3 [10] A. Baldereschi, N. Lipari: Phys. Rev. B 9, 1525 (1974) 3 [11] W. E. Johnson, K. Lark-Horovitz: Phys. Rev. 76, 442 (1949) 4

10

Manuel Cardona

[12] K. Lark-Horovitz: Nucleon-bombarded semiconductors, in Semiconducting Materials (Butterworths, London 1950) p. 47 4 [13] W. Kohn: Solid State Physics, vol. 5 (Academic, New York 1957) 4 [14] Lannon, et al.: Br. J. Urol. 72, 782 (1993) 4 [15] M. Cardona, W. Paul, H. Brooks: J. Phys. Chem. Solids 8, 204 (1959) 5 [16] H. P. Hjalmarson, P. Vogl, D. J. Wolford, J. D. Dow: Phys. Rev. Lett. 44, 810 (1980) 5 [17] D. J. Chadi, K. J. Chang: Phys. Rev. Lett. 60, 2187 (1988) 5 [18] S. B. Chang, D. J. Chadi: Phys. Rev. B 42, 7174 (1990) 5 [19] M. Cardona, N. E. Christensen, G. Fasol: Phys. Rev. B 38, 1806 (1988) 5 [20] N. O. Lipari: Solid State Commun. 25, 266 (1978) 5 [21] J. Serrano, A. Wysmolek, T. Ruf, M. Cardona: Physica B 274, 640 (1999) 5 [22] M. Cardona, M. L. V. Thewalt: Rev. Mod. Phys. 77, 1173 (2005) 6, 10 [23] J. Serrano, F. J. Manj´ on, A. H. Romero, F. Widulle, R. Lauck, M. Cardona: Phys. Rev. Lett. 90, 055510 (2003) 6 [24] P. Pavone, S. Baroni: Solid State Commun. 90, 295 (1994) 6 [25] M. Cardona: Science and technology of advanced materials, in press. See also [22] 7 [26] E. A. Ekimov, V. A. Sidorov, E. D. Bauer, N. N. Mel’nik, N. J. Curro, J. D. Thompson, S. M. Stishov: Nature 428, 542 (2004) 7 [27] Y. Takano, M. Nagao, I. Sakaguchi, M. Tachiki, T. Hatano, K. Kobayashi, H. Umezawa, H. Kawarada: Appl. Phys. Lett. 85, 2851 (2004) 7 [28] L. Boeri, J. Kortus, O. K. Andersen: Phys. Rev. Lett. 93, 237002 (2004) 7 [29] J. E. Hirsch: Proc. Nat. Acad. Sci. (USA) 102, 16569 (2005) 7, 8

Index amorphous, 1, 2, 6, 9 Brillouin zone, 2

Ge, 5–7 Green’s function, 5, 6 GW, 4, 7

cluster, 2

Hamiltonian, 4, 5

dopant, 3, 4 DX, 5

isotope, 4, 6 LDA, 5

eﬀective mass, 3–5 EL2, 5 electron–phonon, 6, 7 EPR, 4 GaAs, 3–5

phonon, 6 Si, 6, 7 Slater, 6 spin-orbit, 3, 5

Defect Theory: An Armchair History David A. Drabold and Stefan K. Estreicher 1

2

Dept. of Physics and Astronomy, Ohio University, Athens, OH 45701 [email protected] Physics Department, Texas Tech University, Lubbock, TX 79409-1051 [email protected]

Abstract. This introductory chapter begins with a summary of the developments of the theory of defects in semiconductors in the past 50 years. This is followed by an overview of single-particle methods and today’s ﬁrst-principles approach, rooted in density-functional theory. Much more detail about this theory and the approximations it involves is found in subsequent chapters. The last section discusses the various contributions to this book.

1 Introduction The voluntary or accidental manipulation of the properties of materials by including defects has been performed for thousands of years. The most ancient example we can think of is well over 5000 years old. It happened when someone realized that adding trace amounts of tin to copper lowers the melting temperature, increases the viscosity of the melt, and results in a metal considerably harder than pure copper: bronze. This allowed the manufacture of a variety of tools, shields and weapons. Not long afterwards, the early metallurgists realized that sand mixed with a metal is relatively easy to melt and produces glass. The Ancient Egyptians discovered that glass beads of various brilliant colors can be obtained by adding trace amounts of speciﬁc transition metals, such as gold for red or cobalt for blue [1]. Defect engineering is not something new. However, materials whose mechanical, electrical, optical, and magnetic properties are almost entirely controlled by defects are relatively new: semiconductors [2, 3]. Although the ﬁrst publication describing the rectifying behavior of a contact dates back to 1874 [4], the systematic study of semiconductors began only during World War II. The ﬁrst task was to grow high-quality Ge (then Si) crystals, that is removing as many defects as possible. The second task was to manipulate the conductivity of the material by adding selected impurities that control the type and concentration of charge carriers. This involved theory to understand as quantitatively as possible the physics involved. Thus, theory has played a key role since the very beginning of this ﬁeld. These early developments have been the subject of several excellent reviews [5–8]. For a long time, theory has been trailing the experimental work. Approximations at all levels were too drastic to allow quantitative predictions. D. A. Drabold, S. K. Estreicher (Eds.): Theory of Defects in Semiconductors, Topics Appl. Physics 104, 11–28 (2007) © Springer-Verlag Berlin Heidelberg 2007

12

David A. Drabold and Stefan K. Estreicher

Indeed, modeling a perfect solid is relatively easy since the system is periodic. High-level calculations can be done in the primitive unit cell. This periodicity is lost when a defect is present. The perturbation to the defect-free material is often large, in particular when some of the energy eigenvalues of the defect are in the forbidden gap, far from band edges. However, in the past decade or so, theory has become quantitative in many respects. Today, theorists often predict geometrical conﬁgurations, binding, formation, and various activation energies, charge and spin densities, vibrational spectra, electrical properties, and other observable quantities with suﬃcient accuracy to be useful to experimentalists and sometimes device scientists. Furthermore, the theoretical tools developed to study defects in semiconductors can be easily extended to other areas of materials theory, including many ﬁelds of nanoscience. It is the need to understand the properties of defects in semiconductors, in particular silicon, that has allowed theory to develop as much as it has. One key reason for this was the availability of microscopic experimental data, ranging from electron paramagnetic resonance (EPR) to vibrational spectroscopy, photoluminescence (PL), or electrical data, all of which provided critical tests for theory at every step. The word “defect” means a native defect (vacancy, self-interstitial, antisite, . . . ), an impurity (atom of a diﬀerent kind from the host atoms), or any combination of those isolated defects: small clusters, aggregates, or even larger defect structures such as precipitates, interfaces, grain boundaries, surfaces, etc. However, nanometer-size defects play many important roles and are the building blocks of larger defect structures. Therefore, understanding the properties of defects begins at the atomic scale. There are many examples of the beneﬁcial or detrimental roles of defects. Oxygen and nitrogen pin dislocations in Si and allow wafers to undergo a range of processing steps without breaking [9]. Small oxygen precipitates provide internal gettering sites for transition metals, but some oxygen clusters are unwanted donors that must be annealed out [10]. Shallow dopants are often implanted. They contribute electrons to the conduction band or holes to the valence band. Native defects, such as vacancies or self-interstitials, promote or prevent the diﬀusion of selected impurities, in particular dopants. Selfinterstitial precipitates may release self-interstitials that in turn promote the transient enhanced diﬀusion of dopants [11]. Transition-metal impurities are often associated with electron–hole recombination centers. Hydrogen [12], almost always present at various stage of device processing, passivates the electrical activity of dopants and of many deep-level defects, or forms extended defect structures known as platelets. Mg-doped GaN must be annealed at rather high temperatures to break up the {Mg, H} complexes that prevent ptype doping [13]. Magnetic impurities such as Mn can render a semiconductor ferromagnetic. The list goes on. Much of the microscopic information about defects comes from electrical, optical, and/or magnetic experimental probes. The electrical data are often obtained from capacitance techniques such as deep-level transient spec-

Defect Theory: An Armchair History

13

troscopy (DLTS). The sensitivity of DLTS is very high and the presence of defects in concentrations as low as 1011 cm−3 can be detected. However, even in conjunction with uniaxial stress experiments, these data provide little or no elemental and structural information and, by themselves, are insuﬃcient to identify the defect responsible for electrical activity. Local vibrational mode (LVM) spectroscopy, Raman, and Fourier transform infrared absorption (FTIR), often give sharp lines characteristic of the Raman- or IR-active LVMs of impurities lighter than the host atoms. When uniaxial stress, annealing, and isotope substitution studies are performed, the experimental data provide a wealth of critical information about a defect. This information can be correlated, e.g., with DLTS annealing data. However, Raman and FTIR are not as sensitive as DLTS. In the case of Raman, over 1017 cm−1 defect centers must be present in the surface layer exposed to the laser. In the case of FTIR, some 1016 cm−3 defect centers are needed, although much higher sensitivities have been obtained from multiple-internal reﬂection FTIR [14]. Photoluminescence is much more sensitive, sometimes down to 1011 cm−1 , but the spectra can be more complicated to interpret [15]. Finally, magnetic probes such as EPR are wonderfully detailed and a lot of defect-speciﬁc data can be extracted: identiﬁcation of the element(s) involved in the defect and its immediate surrounding, symmetry, spin density maps, etc. However, the sensitivity of EPR is rather low, of the order of 1016 cm−3 . Further, localized gap levels in semiconductors often prefer to be empty or doubly occupied as most defect centers in semiconductors are unstable in a spin- 21 state. The sample must be illuminated in order to create an EPR-active version of the defect under study [16–18]. This introductory Chapter contains brief reviews of the evolution of theory [19, 20] since its early days and of the key ingredients of today’s state-ofthe-art theory. It concludes with an overview of the content of this book.

2 The Evolution of Theory The ﬁrst device-related problem that required understanding was the creation of electrons or holes by dopants. These (mostly substitutional) impurities are a small perturbation to the perfect crystal and are well described by eﬀective mass theory (EMT) [21]. The Schr¨ odinger equation for the nearly-free charge carrier, trapped very close to a parabolic band edge, is written in hydrogenic form with an eﬀective mass determined by the curvature of the band. The calculated binding energy of the charge carrier is that of a hydrogen atom but reduced by the square of the dielectric constant. As a result, the associated wavefunction is substantially delocalized, with an eﬀective Bohr radius some 100 times larger than that of the free hydrogen atom. EMT has been reﬁned in a variety of ways [22] and provided a basic understanding of doping. However, it cannot be extended to defects that have energy eigenvalues far from band edges. These so-called “deep-level” defects

14

David A. Drabold and Stefan K. Estreicher

are not weak perturbations to the crystal and often involve substantial relaxations and distortions. The ﬁrst such defects to be studied were the byproducts of radiation damage, a hot issue in the early days of the cold war. EPR data became available for the vacancy [16, 23] and the divacancy [24], in silicon (the Si self-interstitial has never been detected). Transition-metal (TM) impurities, which are common impurities and active recombination centers, have also been studied by EPR [25]. In most charge states, the undistorted vacancy (Td symmetry) or divacancy (D3d symmetry) is an orbital triplet or doublet, respectively, and therefore should undergo Jahn–Teller distortions. The EPR studies showed that this is indeed the case. Although interstitial oxygen, the most common impurity in Czochralski-grown Si, was known to be at a puckered bond-centered site [26, 27], it was not realized how much energy is involved in relaxations and distortions. It was believed that the chemistry of defects in semiconductors is well described in ﬁrst order by assuming high-symmetry, undistorted, lattice sites. Relaxations and distortions were believed to be a second-order correction. The important issue then was to correctly predict trends in the spin densities and electrical activities of speciﬁc defects centers in order to explain the EPR and electrical data (see, e.g., [28, 29]). The critical importance of carefully optimizing the geometry around defects and the magnitudes of the relaxation energies were not fully realized until the 1980s [30, 31]. The host-atom displacements can be of several tenths of an ˚ A, and the chemical rebonding can lead to energy changes as large as several eV (undistorted vs. relaxed structures). The ﬁrst theoretical tool used to describe localized defects in semiconductors involved Green’s functions [2, 19, 32, 33]. These calculations begin with the Hamiltonian H0 of the perfect crystal. Its eigenvalues give the crystal’s band structure and the eigenfunctions are Bloch or Wannier functions. In principle, the defect-free host crystal is perfectly described. The localized defect is represented by a Hamiltonian H that includes the defect potential V . The Green’s function is G(E) = 1/(E − H ). Therefore, the perturbed energies E coincide with its poles. The new eigenvalues include the gap levels of the defect and the corresponding eigenfunctions are the defect wavefunctions. In principle, Green’s functions provide an ideal description of the defect in its crystalline environment. In practice, there are many diﬃculties associated with the Hamiltonian, the construction of perfect-crystal eigenfunctions that can be used as a basis set for the defect calculation [34, 35], and the construction of the defect potential itself. This is especially true for those defects that induce large lattice relaxations and/or distortions. The ﬁrst successful Green’s functions calculations for semiconductors date back to the late 1970s [36–38]. They were used to study charged defects [39], calculate forces [40–42], total energies [43, 44], and LVMs [45, 46]. These calculations also provided important clues about the role of native defects in impurity diﬀusion [47]. However, while Green’s functions do provide a nearideal description of the defect in a crystal, their implementation is diﬃcult

Defect Theory: An Armchair History

15

and not very intuitive. Clusters or supercells are much easier to use and provide a physically and chemically appealing description of the defect and its immediate surroundings. Green’s functions have mostly been abandoned since the mid-1980s, but a rebirth within the GW formalism [48] is now taking place (see the Chapter by Schindlmayr and Scheﬄer ). In order to describe the distortions around a vacancy, Friedel et al. [49] completely ignored the host crystal and limited their description to rigid linear combinations of atomic orbitals (LCAO). Messmer and Watkins [50,51] expanded this approach to linear combinations of dangling-bond states. These simple quantum-chemical descriptions provided a much-needed insight and a correct, albeit qualitative, explanation of the EPR data. Here, the defect was assumed to be so localized that the entire crystal could be ignored in zeroth order. The natural extension of this work was to include a few host atoms around the defect, thus deﬁning a cluster . These types of calculations were performed in real space with basis sets consisting of localized functions such as Gaussians or LCAOs. The dangling bonds on the surface atoms must be tied up in some way, most often with H atoms. However, without the underlying crystal and its periodicity, the band structure is missing and the defect’s energy eigenvalues cannot be placed within a gap. Further, the ﬁnite size of the cluster artiﬁcially conﬁnes the wavefunctions. This aﬀects charged defects the most, as the charge tends to distribute itself on the surface of the cluster. However, the local covalent interactions are well described. The Schr¨ odinger equation for a cluster containing a defect can be solved using almost any electronic-structure method. The early work was empirical or semiempirical, with heavily approximated quantum-chemical methods. At ﬁrst, extended H¨ uckel theory [52, 53] was used then self-consistent semiempirical Hartree–Fock: CNDO [54], MNDO [55], MINDO [56]. Geometries could be optimized, albeit often with symmetry assumptions. The methods suﬀered from a variety of problems such as cluster size and surface eﬀects, basis-set limitations, lack of electron correlation, and the use of adjustable parameters. Their values are normally ﬁtted to atomic or molecular data, and transferability is a big issue. In order to bypass the surface problem, cyclic clusters have been designed, mostly in conjunction with semiempirical Hartree–Fock. Cyclic clusters can be viewed as clusters to which Born–von-Karman periodic boundary conditions are applied [57, 58]. These boundary conditions can be diﬃcult to handle, in particular when 3- and 4-center interactions are included [59]. DeLeo and coworkers [60, 61] extensively used the scattering-Xα method in clusters to study trends for interstitial TM impurities and hydrogen–alkalimetal complexes. The results provided qualitative insight into these issues. Ultimately, the method proved diﬃcult to bring to self-consistency and the rather arbitrarily deﬁned muﬃn-tin spheres rendered it poorly suited to the calculation of total energies vs. atomic positions.

16

David A. Drabold and Stefan K. Estreicher

The method of partial retention of diatomic diﬀerential overlap [62, 63] (PRDDO) was ﬁrst used for defects in diamond and silicon in the mid-1980s. It is self-consistent, contains no semiempirical parameters, and allows geometry optimizations to be performed without symmetry assumptions. Convergence is very eﬃcient and relatively large clusters (44 host atoms) could be used. However, PRDDO is a minimal basis-set technique and ignores electron correlation. Its earliest success was to demonstrate [30, 31] the stability of bond-centered hydrogen in diamond and silicon. It was not expected at all that an impurity as light as H could indeed force a Si–Si bond to stretch by over 1 ˚ A. Substantial progress in the theory of defects in semiconductors occurred in the mid-1980s with the combination of periodic supercells to represent the host crystal, ab-initio-type pseudopotentials [64–66] for the core regions, DF theory for the valence regions, and ab-initio molecular dynamics (MD) simulations [67, 68] for nuclear motion. This combination is now referred to as “ﬁrst-principles” as opposed to “semiempirical”. There are parameters in the theory. They include the size of the supercell, k-point sampling, type and size of the basis set, chosen by the user, as well as the parameters associated with the basis sets and pseudopotentials. However, these parameters and user inputs are not ﬁtted to an experimental database. Instead, some are determined self-consistently, other are calculated from ﬁrst principles or obtained from high-level atomic calculations. Note that the ﬁrst supercell calculations were done in the 1970s in conjunction with approximate electronic-structure methods [69–71]. PRDDO was used to study cluster size and surface eﬀects [72] and many defects (see, e.g., [73, 74]). It provided good input geometries for single-point ab-initio Hartree–Fock calculations (see, e.g., [75]). However, it suﬀered from the problems associated with all Hartree–Fock techniques, such as unreasonably large gaps and inaccurate LVMs. A number of research groups have used Hartree–Fock and post-Hartree–Fock techniques [76–78] to study defects in clusters, but these eﬀorts have now been mostly abandoned. Density-functional (DF) theory [79–82] with local basis sets (see, e.g., [83]) in large clusters allowed more quantitative predictions. The DF-based AIMPRO code [84, 85] uses Gaussian basis sets and has been applied to many defect problems (this code handles periodic supercells as well). In addition to geometries and energetics, rather accurate LVMs for light impurities can be predicted [86, 87]. Large clusters have been used [88, 89] to study the distortions around a vacancy or divacancy in Si. However, all clusters suﬀer from the surface problem and lack of periodicity.

3 A Sketch of First-Principles Theory The theoretical approach known as “ﬁrst principles” has proven to be a revolutionary tool to predict quantitatively some key properties of defects. An elementary exposition of the theory follows.

Defect Theory: An Armchair History

17

3.1 Single-Particle Methods: History After the Born–Oppenheimer approximation is made, so that electronic and ionic degrees of freedom are separated, we face the time-independent manyelectron problem [82]: −2 /2m ∇2j − Zl e2 /|rj − Rl | + 1/2 e2 /|r j − r j | − E Ψ = 0 . j

j,l

j=j

(1) Here, rj are electron coordinates, Rl and Zl are positions and atomic numbers of the nuclei and E is the energy. It is worth reﬂecting on the remarkable simplicity of this equation: it is exact (nonrelativistically), and the meaning of each term is entirely transparent. In one of the celebrated legends of science, P. A. M. Dirac is said to have implied that chemistry was just an application of (1), though he also acknowledged that the equation was intractable. It is true that the quantum mechanics of the many-electron problem is beautifully and succinctly represented in (1). Kohn gives an interesting argument [82] stating that even in principle, (1) is hopeless as a practical tool for calculation if the number of electrons exceeds 103 or so. His argument is a development of a paper of Van Vleck [90]1 and points out that it appears to be fundamentally impossible to obtain an approximate many-electron function Ψ with signiﬁcant overlap with the “true” many-body wavefunction for large systems. He further points out that the sheer dimensionality of the problem rapidly makes it unrepresentable on any conceivable computer. Thus, a credible case can be made that for large systems it does not even make sense to estimate Ψ directly. Kohn has named this the “exponential wall”. To some extent this is disconcerting, because of the simplicity of the form of (1), but it points to the need for new concepts if we are to make sense of solids – to say nothing of defects! Empirical experience with solids also suggests that the unfathomable complexity of the many-body wavefunction is unnecessary. If all of the information contained in Ψ was really required for estimating the properties of solids that we care about, e.g., experimental observables, molecular physics would reach exhaustion with tiny molecules, and solid-state physics would never get oﬀ the ground at all. The fact is that many characteristics of materials are independent of system size. For example, in a macroscopic sample, the electronic density of states has the same form for a system with N atoms and an identically prepared one with 2N atoms. Yet Ψ is immeasurably more complex for the second system than the ﬁrst. Thus, the additional complexity 1

In this prescient paper on Heisenberg’s theory of ferromagnetism, Van Vleck introduces what later was called the “Van Vleck Catastrophe”, and emphasizes the fundamentally nonlocal character of quantum mechanics as expressed in (1), the associated factorial growth in complexity, and its dire implications for attempts to compute many-particle states for large systems.

18

David A. Drabold and Stefan K. Estreicher

of the 2N system ψ must be completely irrelevant to our observable, in this case the density of states. The saturation of complexity of the preceding paragraph is connected to Kohn’s “principle of nearsightedness” [91], which states that in fact quantum mechanics in the solid state is intrinsically local (how local depends sensitively on the system [92, 93]). The natural gauge of this locality is the decay ρ|x : of the density operator in the position representation: ρ(x, x ) = x|ˆ a function of |x − x |, decaying as a power law in metals and exponentially in systems with a gap. For systems with a gap, the exponential fall oﬀ enables accurate calculations of all local properties by undertaking a calculation in a ﬁnite volume determined by the rate of decay. The decay in semiconductors and insulators can be exploited to produce eﬃcient order-N methods for computing total energies and forces, with computational cost scaling linearly with the number of atoms or electrons [94]. 3.2 Direct Approaches to the Many-Electron Problem While this book emphasizes single-particle methods, there is one important exception. Needs shows in his Chapter in this volume that remarkable progress can be made for the computation of expectation values of observables using quantum Monte Carlo methods, with no essential approximations to (1). This is a promising class of methods that oﬀers the most accurate calculations available today for complex systems. Several groups are advancing these methods, and even the stochastic calculation of forces is becoming possible. One can be certain that quantum Monte Carlo will play an important role in systems needing the most accurate calculations available, and certainly this is the case for the theory of defects. 3.3 Hartree and Hartree–Fock Approximations In 1928, Hartree [95] started with (1) with a view to extracting useful singleparticle equations from it. He used the variational principle for the groundstate wavefunction adopting a simple product trial function: Ψ (x1 , x2 , . . . , xn ) = ψ1 (x1 )ψ2 (x2 ) . . . ψn (xn ). The product ansatz did not enforce Fermion antisymmetry requirements; this was built in with a Slater determinant ansatz as proposed by Fock in 1930 [96]: the Hartree–Fock method. These methods map the many-body ground-state problem onto a set of challenging single-particle equations. The structure of the Hartree equations is a Schr¨ odinger equation with a potential depending upon all the orbitals: −2 /2m∇2 ψl + Veﬀ ψl = εl ψl ,

(2)

where the eﬀective potential Veﬀ (r) = j= d3 r ψj∗ (r )ψ (r )/|r − r |, and the sum is over occupied states. This appealing equation prescribes an eﬀective Coulomb ﬁeld for electron l arising from all of the other electrons. Since

Defect Theory: An Armchair History

19

computing the potential requires knowledge of the other wavefunctions, the equation must be solved self-consistently with a scheme of iteration. While the equation is intuitive, it is highly approximate. Curiously, it will turn out that the equations of density-functional theory have the mathematical structure of (2), but with quite a diﬀerent (and far more predictive) Veﬀ (see (7) below), derived from a very diﬀerent point of view. The Hartree–Fock approximation includes that part of the exchange energy implied by the exclusion principle and has well-known analytic problems at the Fermi surface in metals [94] and a tendency to exaggerate charge ﬂuctuations at atomic sites in molecules or solids [97]. In molecular calculations, the correlation energy (roughly speaking, what is missing from Hartree–Fock) can be estimated in perturbation theory. This is computationally expensive: the most popular fourth-order perturbation theory (MP4) scales as n3 N 4 , where n is the number of electrons and N the number of orbitals (basis set size). Such methods are important for molecular systems, but challenging to apply to condensed systems. 3.4 Density-Functional Theory 3.4.1 Thomas–Fermi Model Not long after the dawn of quantum mechanics, Thomas and Fermi [98, 99] suggested a key role for the electron-density distribution as the determiner of the total energy of an inhomogeneous electron gas. This was the ﬁrst serious attempt to express the energy as a functional of the electron density ρ: E[ρ] =

3

2

d rV (r)ρ(r) + e /2

d3 r d3 r ρ(r)ρ(r )/|r − r | + α/m 3 × d rρ5/3 (r) . (3)

Here, α is a numerical constant, m and e are the electron mass and charge respectively, and V is an external potential. The ﬁrst two terms are evidently obtained from classical electrostatics. Quantum mechanics appears only in the third term, derived from the kinetic energy of a homogeneous electron gas. Already this equation is making a “local-density approximation”, forming an estimate for the inhomogeneous electron kinetic energy from the result from a homogeneous gas; an approximation that is expected to succeed if |∇ρ|/ρ is suﬃciently small. Variation of (3) with respect to ρ with ﬁxed electron number leads to the coupled self-consistent Thomas–Fermi equations (see, e.g., the treatment by Fulde [97]). The coarse treatment of the kinetic energy greatly limits the predictive power of the method – for example, the shell structure of atoms is not predicted [100]. However, the Thomas–Fermi model is conceptually a density-functional theory.

20

David A. Drabold and Stefan K. Estreicher

3.4.2 Modern Density-Functional Theory For atomistic force calculations on solids, the overwhelming method of choice is density-functional theory, due to Kohn, Hohenberg and Sham [101, 102]. This Chapter only sketches the concepts in broad outline, as a detailed treatment focused on defect calculations is available in this book (Niemenen Chapter). For additional discussion we strongly recommend the books of Martin (see [94]) and Fulde [97]. The following statements embody the foundation of zero-temperature density-functional theory: 1. The ground-state energy of a many-electron system is a functional of the electron density ρ(x): 3 E[ρ] = d xV (x)ρ(x) + F [ρ] , (4) where V is an external potential (due, for example, to interaction with ions, external ﬁelds, e.g., not with electrons), and F [ρ] is a universal functional of the density. The trouble is that F [ρ] is not exactly known, though there is continuing work to determine it. The practical utility of this result derives from: 2. The functional E[ρ] is minimized by the true ground-state electron density. It remains to estimate the functional F [ρ], which in conjunction with the variational principle 2, enables real calculations. To estimate F [ρ], the usual procedure is to note that we already know some of the major contributions to F [ρ], and decompose the functional in the form: 3 3 (5) F [ρ] = e2 /2 d x d x ρ(x)ρ(x )/|x − x | + Tni (ρ) + Exc (ρ) . Here, the integral is just the electrostatic (Hartree) interaction of the electrons, Tni is the kinetic energy of a noninteracting electron gas of density ρ, and Exc (ρ) is yet another unknown functional, the exchange-correlation functional, which includes nonclassical eﬀects of the interacting electrons. Equation (5) is diﬃcult to evaluate directly in terms of ρ, because of orbitals |χi , for which the term Tni . Thus, one introduces single-electron Tni = iocc χi | − 2 /2m∇2 |χi , and ρ = iocc |χi (x)|2 is the charge density of the physically relevant interacting system. The value of this decomposition is that Exc (ρ) is smooth and reasonably slowly varying, and therefore a functional that we can successfully approximate: we have included the most diﬃcult and rapidly varying parts of F in Tni and the Hartree integral, as can be seen from essentially exact many-body calculations on the homogeneous electron gas [103]. The Hartree and noninteracting kinetic energy terms are

Defect Theory: An Armchair History

21

easy to compute if one makes the local-density approximation, that is assuming that the electron density is locally uniform. With information about the homogeneous electron gas, the functional (5) is fully speciﬁed. With noninteracting orbitals |χi , (with ρ(x) = 2 iocc |x|χi |2 ), then the minimum principle plus the constraint that χi |χj = δij can be translated into an eigenvalue problem for the |χi : {−2 ∇2 /2m + Veﬀ [ρ(x)]}|χi = εi |χi ,

(6)

where the eﬀective density-dependent (in practical calculations, orbitaldependent) potential Veﬀ is: 3 (7) Veﬀ [ρ(x)] = V (x) + e2 d x ρ(x )/|x − x | + δεxc /δρ . In this equation εxc is the parameterized exchange-correlation energy density from the homogeneous electron gas. The quantities to be considered as physical in local-density functional calculations are: the total energy (electronic or system), the ground-state electronic charge density ρ(x), and related ground-state properties like the forces. In particular, it is tempting to interpret the |χi and εi as genuine electronic eigenstates and energies, and indeed this can often be useful. Such identiﬁcations are not rigorous [94]. It is instructive to note that the starting point of density-functional theory was to depart from the use of orbitals and formulate the electronic-structure problem rigorously in terms of the electron density ρ; yet a practical implementation (which enables an accurate estimate of the electronic kinetic energy) led us immediately back to orbitals! This illustrates why it would be very worthwhile to know F (ρ), or at least the kinetic energy functional since we would then have a theory with a structure close to the Thomas–Fermi form and would therefore be able to seek one function ρ rather than the cumbersome collection of orthonormal |χi . The initiation of modern ﬁrst-principles theory and its development into a standard method with widespread application was due to Car and Parrinello [67]. They developed a powerful method for simultaneously solving the electronic problem and evolving the positions of the ions. The method is usually applied to plane-wave basis sets, though the key ideas are independent of the choice of representation. One of the early applications to defects in silicon was the diﬀusion of bond-centered hydrogen [104]. An alternative ab-initio approach to MD simulations, based on a tight-binding perspective, was proposed by Sankey and Niklewski [68]. Their basis sets consist of pseudoatomic orbitals with s, p, d, . . . symmetry. The wavefunctions are truncated beyond some radius and renormalized. The early version of this code was not self-consistent and was restricted to minimum basis sets. A more recent version [105] is self-consistent and can accommodate expanded and polarized basis sets. This is also the case for the highly ﬂexible SIESTA code [106, 107] (Spanish initiative for the electronic structure with thousands

22

David A. Drabold and Stefan K. Estreicher

of atoms). Although basis sets of local orbitals (typically, LCAOs) are highly intuitive and allow population analysis and other chemical information to be calculated, they are less complete than plane-wave basis sets. The latter can easily be checked for convergence. On the other hand, when an atom such as Si is given two sets of 3s and 3p plus a set of 3d orbitals, the basis set is suﬃcient to describe quite well virtually all the chemical interactions of this element, as the contribution of the n = 4 shell of Si is exceedingly small, except such under extreme conditions that a ground-state theory is not capable of handling anyway. Many details of the implementation of densityfunctional methods are given in the contribution of Nieminen in his Chapter in this volume. The power of these methods is that they yield parameter-free estimates for the structure of defects and even topologically disordered systems, provide accurate estimates of total energies, formation energies, vibrational states, defect dynamics, and with suitable caveats information about electronic structure, defect levels, localization, etc. There are many subtle aspects to their applications to defect physics, partly because high accuracy is often required in such studies.

4 The Contributions In his Chapter in this volume, Nieminen carefully discusses the use of periodic boundary conditions in supercell calculations, detailing both strengths and weaknesses, and other basic features of these calculations. In their Chapter, Goss and coworkers discuss the marker method to extract electronic energy levels, and include several important applications. In their Chapter, Estreicher and Sanati describe the calculation and remarkable utility of vibrational modes in systems containing defects, including novel analysis of ﬁnite-temperature properties of defects. Then, in their Chapter, Hernandez and coworkers work out a proper theory of free energies and phase diagrams for semiconductors. Needs describes in his Chapter the most rigorous attack of the book on the quantum many-body problem, as Needs explores quantum Monte Carlo methods and their promise for defects in semiconductors. Schindlmayr and Scheﬄer describe the theory and application of self-energy corrected density-functional theory, the “GW” approximation in their Chapter. Like the work of Needs, this technique has predictive power beyond DFT. Csanyi and coworkers present a multiscale modeling approach in their Chapter with applications. Scheerschmidt oﬀers a comprehensive view of molecular dynamics in his Chapter, focusing on empirical methods, though much of his Chapter is applicable to ﬁrst-principles simulation as well. In their Chapter, Drabold and Abtew discuss defects in amorphous semiconductors with a special emphasis on hydrogenated amorphous silicon. Last but not least, in their Chapter, Simdyankin and Elliott write on the theory of light-induced eﬀects

Defect Theory: An Armchair History

23

in amorphous materials, an area of great basic and practical interest, which nevertheless depends very much upon the defects present in the material.

References [1] J. L. Mass, M. T. Wypyski, R. E. Stone: Mater. Res. Soc. Bull. 26, 38 (2001) 11 [2] A. M. Stoneham: Theory of Defects in Solids (Clarendon, Oxford 1985) 11, 14 [3] H. J. Queisser, E. E. Haller: Science 281, 945 (1998) 11 [4] F. Braun: Ann. Phys. Chem. (Leipzig) 153, 556 (1874) 11 [5] A. B. Fowler: Phys. Today 46, 59 (1993) 11 [6] F. Seitz: Phys. Today 48, 22 (1995) 11 [7] M. Riordan, I. Hoddeson: Phys. Today 50, 42 (1997) 11 [8] I. M. Ross: Phys. Today 50, 34 (1997) 11 [9] F. Shimura (Ed.): Oxygen in Silicon, Semicond. Semimet. 42 (Academic, Boston 1994) 12 [10] R. Jones (Ed.): Early Stages of Oxygen Precipitation in Silicon (Kluwer, Dordrecht 1996) 12 [11] R. Scholtz, U. G¨ osele, J. Y. Y. Huh, T. Y. Tan: Appl. Phys. Lett. 72, 200 (1998) 12 [12] S. K. Estreicher: Mater. Sci. Eng. R 14, 319 (1995) 12 [13] S. J. Pearton: GaN and Related Materials (Gordon and Breach, Amsterdam 1997) p. 333 12 [14] F. Jiang, M. Stavola, A. Rohatgi, D. Kim, J. Holt, H. Atwater, J. Kalejs: Appl. Phys. Lett. 83, 931 (2003) 13 [15] G. Davies: Phys. Rep. 176, 83 (1989) 13 [16] G. D. Watkins: Deep Centers in Semiconductors (Gordon and Breach, New York 1986) p. 147 13, 14 [17] Y. V. Gorelkinskii, N. N. Nevinnyi: Physica B 170, 155 (1991) 13 [18] Y. V. Gorelkinskii, N. N. Nevinnyi: Mater. Sci. Eng. B. 36, 133 (1996) 13 [19] S. T. Pantelides (Ed.): Deep Centers in Semiconductors (Gordon and Breach, New York 1986) 13, 14 [20] S. K. Estreicher: Mater. Today 6, 26 (2003) 13 [21] W. Kohn: Solid State Phys. 5, 257 (1957) 13 [22] S. T. Pantelides: Rev. Mod. Phys. 50, 797 (1978) 13 [23] G. D. Watkins: Radiation Damage in Semiconductors (Dunod, Paris 1964) p. 97 14 [24] G. D. Watkins, J. W. Corbett: Phys. Rev. 138, A543 (1965) 14 [25] G. W. Ludwig, H. H. Woodbury: Solid State Phys. 13, 223 (1962) 14 [26] W. Kaiser, P. H. Keck, C. F. Lange: Phys. Rev. 101, 1264 (1956) 14 [27] J. W. Corbett, R. S. McDonald, G. D. Watkins: J. Phys. Chem. Solids 25, 873 (1964) 14 [28] G. G. DeLeo, G. D. Watkins, W. Beal Fowler: Phys. Rev. B 25, 4972 (1982) 14 [29] A. Zunger, U. Lindefelt: Phys. Rev. B 26, 5989 (1982) 14

24

David A. Drabold and Stefan K. Estreicher

[30] T. L. Estle, S. K. Estreicher, D. S. Marynick: Hyp. Inter. 32, 637 (1986) 14, 16 [31] T. L. Estle, S. K. Estreicher, D. S. Marynick: Phys. Rev. Lett. 58, 1547 (1987) 14, 16 [32] G. F. Koster, J. C. Slater: Phys. Rev. 95, 1167 (1954) 14 [33] J. Callaway: J. Math. Phys. 5, 783 (1964) 14 [34] J. Callaway, A. J. Hughes: Phys. Rev. 156, 860 (1967) 14 [35] J. Callaway, A. J. Hughes: Phys. Rev. 164, 1043 (1967) 14 [36] J. Bernholc, S. T. Pantelides: Phys. Rev. B 18, 1780 (1978) 14 [37] J. Bernholc, N. O. Lipari, S. T. Pantelides: Phys. Rev. Lett. 41, 895 (1978) 14 [38] G. A. Baraﬀ, M. Schl¨ uter: Phys. Rev. Lett. 41, 892 (1978) 14 [39] G. A. Baraﬀ, E. O. Kane, M. Schl¨ uter: Phys. Rev. Lett. 43, 956 (1979) 14 [40] M. Scheﬄer, J. P. Vigneron, G. B. Bachelet: Phys. Rev. Lett. 49, 1756 (1982) 14 [41] U. Lindefelt: Phys. Rev. B 28, 4510 (1983) 14 [42] U. Lindefelt, A. Zunger: Phys. Rev. B 30, 1102 (1984) 14 [43] G. A. Baraﬀ, M. Schl¨ uter: Phys. Rev. B 28, 2296 (1983) 14 [44] R. Car, P. J. Kelly, A. Oshiyama, S. T. Pantelides: Phys. Rev. Lett. 52, 1814 (1984) 14 [45] D. N. Talwar, M. Vandevyver, M. Zigone: J. Phys. C 13, 3775 (1980) 14 [46] R. M. Feenstra, R. J. Hauenstein, T. C. McGill: Phys. Rev. B 28, 5793 (1983) 14 [47] R. Car, P. J. Kelly, A. Oshiyama, S. T. Pantelides: Phys. Rev. Lett. 54, 360 (1985) 14 [48] F. Aryasetiawan, O. Gunnarsson: Rep. Prog. Phys. 61, 237 (1998) 15 [49] J. Friedel, M. Lannoo, G. Leman: Phys. Rev. 164, 1056 (1967) 15 [50] R. P. Messmer, G. D. Watkins: Phys. Rev. Lett. 25, 656 (1970) 15 [51] R. P. Messmer, G. D. Watkins: Phys. Rev. B 7, 2568 (1973) 15 [52] F. P. Larkins: J. Phys. C: Solid State Phys. 4, 3065 (1971) 15 [53] R. P. Messmer, G. D. Watkins: Proc. Reading Conf. on Radiation Damage and Defects in Semiconductors (Insitute of Physics, Bristol 1973) p. 255 15 [54] A. Mainwood: J. Phys. C: Solid State Phys. 11, 2703 (1978) 15 [55] J. W. Corbett, S. N. Sahu, T. S. Shi, L. C. Snyder: Phys. Lett. 93A, 303 (1983) 15 [56] P. De´ ak, L. C. Snyder: Radiat. Eﬀ. Def. Solids 111–112, 77 (1989) 15 [57] P. De´ ak, L. C. Snyder: Phys. Rev. B 36, 9619 (1987) 15 [58] P. De´ ak, L. C. Snyder, J. W. Corbett: Phys. Rev. B 45, 11612 (1992) 15 [59] J. Mir´ o, P. De´ ak, C. P. Ewels, R. Jones: J. Phys.: Condens. Matter 9, 9555 (1997) 15 [60] G. G. DeLeo, G. D. Watkins, W. B. Fowler: Phys. Rev. B 23, 1819 (1981) 15 [61] G. G. DeLeo, W. B. Fowler, G. D. Watkins: Phys. Rev. B 29, 1851 (1984) 15 [62] T. A. Halgren, W. N. Lipscomb: J. Chem. Phys. 58, 1569 (1973) 16 [63] D. S. Marynick, W. N. Lipscomb: Proc. Nat. Acad. Sci. (USA) 79, 1341 (1982) 16 [64] D. R. Hamann, M. Schl¨ uter, C. Chiang: Phys. Rev. Lett. 43, 1494 (1979) 16

Defect Theory: An Armchair History

25

[65] G. B. Bachelet, D. R. Hamann, M. Schl¨ uter: Phys. Rev. B 26, 4199 (1982) 16 [66] L. Kleinman, D. M. Bylander: Phys. Rev. Lett. 48, 1425 (1982) 16 [67] R. Car, M. Parrinello: Phys. Rev. Lett. 55, 2471 (1985) 16, 21 [68] O. Sankey, D. J. Niklewski: Phys. Rev. B 40, 3979 (1989) 16, 21 [69] A. Zunger, A. Katzir: Phys. Rev. B 11, 2378 (1975) 16 [70] S. G. Louie, M. Schl¨ uter, J. R. Chelikowsky, M. L. Cohen: Phys. Rev. B 13, 1654 (1976) 16 [71] W. Pickett, M. L. Cohen, C. Kittel: Phys. Rev. B 20, 5050 (1979) 16 [72] S. K. Estreicher, A. K. Ray, J. L. Fry, D. S. Marynick: Phys. Rev. Lett. 55, 1976 (1985) 16 [73] S. K. Estreicher: Phys. Rev. B 41, 9886 (1990) 16 [74] S. K. Estreicher: Phys. Rev. B 41, 5447 (1990) 16 [75] S. K. Estreicher: Phys. Rev. B 60, 5375 (1999) 16 [76] A. A. Bonapasta, A. Lapiccirella, N. Tomassini, M. Capizzi: Phys. Rev. B 36, 6228 (1987) 16 [77] E. Artacho, F. Yndur´ ain: Solid State Commun. 72, 393 (1989) 16 [78] R. Luchsinger, P. F. Meier, N. Paschedag, H. U. Suter, Y. Zhou: Philos. Trans. Roy. Soc. Lond. A 350, 203 (1995) 16 [79] P. Hohenberg, W. Kohn: Phys. Rev. 136B, 468 (1964) 16 [80] W. Kohn, L. J. Sham: Phys. Rev. 140A, 1133 (1965) 16 [81] L. J. Sham, W. Kohn: Phys. Rev. 145, 561 (1966) 16 [82] W. Kohn: Rev. Mod. Phys. 71, 1253 (1999) 16, 17 [83] M. Saito, A. Oshiyama: Phys. Rev. B 38, 10711 (1988) 16 [84] R. Jones, A. Sayyash: J. Phys. C 19, L653 (1986) 16 [85] R. Jones, P. R. Briddon: The ab-initio cluster method and the dynamics of defects in semiconductors, in M. Stavola (Ed.): Identiﬁcation of Defects in Semiconductors, vol. 51A, Semicond. Semimet. (Academic, Boston 1998) Chap. 6, p. 287 16 ¨ Phys. Rev. Lett. [86] J. D. Holbech, B. Bech Nielsen, R. Jones, P. Sitch, S. Oberg: 71, 875 (1993) 16 [87] R. Jones, B. J. Coomer, P. R. Briddon: J. Phys.: Condens. Matter 16, S2643 (2004) 16 [88] S. Og¨ ut, J. R. Chelikowsky: Phys. Rev. Lett. 83, 3852 (1999) 16 [89] S. Og¨ ut, J. R. Chelikowsky: Phys. Rev. B 64, 245206 (2001) 16 [90] J. H. Van Vleck: Phys. Rev. 49, 232 (1936) 17 [91] W. Kohn: Phys. Rev. Lett. 76, 3168 (1996) 18 [92] X. P. Li, R. W. Nunes, D. Vanderbilt: Phys. Rev. B 47, 10891 (1993) 18 [93] S. N. Taraskin, D. A. Drabold, S. R. Elliott: Phys. Rev. Lett. 88, 196405 (2002) 18 [94] R. M. Martin: Electronic Structure, Basic Theory and Practical Applications (Cambridge University Press, Cambridge 2004) 18, 19, 20, 21 [95] D. R. Hartree: Proc. Cambridge Philos. Soc. 24, 89 (1928) 18 [96] F. Fock: Z. Phys. 61, 126 (1930) 18 [97] P. Fulde: Electron Correlations in Molecules and Solids (Springer, Berlin, Heidelberg 1993) 19, 20 [98] E. Fermi: Z. Phys. 48, 73 (1928) 19 [99] L. H. Thomas: Proc. Cambridge Philos. Soc. 23, 542 (1927) 19

26

David A. Drabold and Stefan K. Estreicher

[100] R. G. Parr, W. Yang: Density-Functional Theory of Atoms and Molecules (Clarendon, Oxford 1989) 19 [101] P. Hohenberg, W. Kohn: Phys. Rev. 136, B864 (1964) 20 [102] W. Kohn, L. J. Sham: Phys. Rev. 140, A1133 (1965) 20 [103] D. M. Ceperley, G. J. Alder: Phys. Rev. Lett. 45, 566 (1980) 20 [104] F. Buda, G. L. Chiarotti, R. Car, M. Parrinello: Phys. Rev. Lett. 63, 4294 (1989) 21 [105] A. A. Demkov, J. Ortega, O. F. Sankey, M. P. Grumbach: Phys. Rev. B 53, 10441 (1995) 21 [106] D. S´ anchez-Portal, P. Ordej´ on, E. Artacho, J. M. Soler: Int. J. Quant. Chem. 65, 453 (1997) 21 [107] E. Artacho, D. S´ anchez-Portal, P. Ordej´ on, A. Garc´ıa, J. M. Soler: Phys. Stat. Sol. (b) 215, 809 (1999) 21

Index ab initio, 16, 21 absorption, 13 AIMPRO, 16 amorphous, 22, 23 annealing, 12, 13 antisite, 12 band edge, 12, 13 band structure, 14, 15 basis set, 14–16, 21, 22 Bloch, 14 Bohr, 13 bond-centered, 14, 16, 21 Born–Oppenheimer, 17 Born–von-Karman, 15 Car, 21 charge state, 14 charged defect, 15 classical, 19, 20 cluster, 12, 15, 16 complex, 12, 15 concentration, 11, 13 conduction band, 12 conductivity, 11 core, 16 correlation, 15, 16, 19 Coulomb, 18 covalent, 15 cyclic cluster, 15 Czochralski, 14

dangling bond, 15 decay, 18 deep level, 12, 13 deep-level transient spectroscopy, 13 defect engineering, 11 delocalized, 13 density of states, 17, 18 density-functional theory, 16, 19–22 DFT, 22 diamond, 16 diﬀusion, 12, 14, 21 Dirac, 17 dislocation, 12 disorder, 22 distortion, 14–16 divacancy, 14, 16 DLTS, 13 donor, 12 dopant, 12, 13 doping, 12, 13 eﬀective mass, 13 eigenstates, 21 eigenvalues, 12–15 electron, 12, 13, 17–20 electron paramagnetic resonance, 12 empirical, 15, 22 EMT, 13 energy level, 22 EPR, 12–15

Defect Theory: An Armchair History exchange, 19 exchange-correlation, 20, 21 exclusion principle, 19 fermion, 18 ﬁrst principles, 16, 21, 22 ﬂuctuation, 19 force, 14, 18, 20, 21 Fourier, 13 free energy, 22 FTIR, 13 GaN, 12 gap, 12–16, 18 gap levels, 13, 14 Gaussian, 16 Ge, 11 gettering, 12 glass, 11 grain boundary, 12 Green’s function, 14, 15 ground-state, 18, 20–22 GW, 15, 22 H¨ uckel, 15 Hamiltonian, 14 Hartree, 18, 20 Hartree–Fock, 15, 16, 18, 19 hole, 12, 13 hydrogen, 12, 13, 15, 16, 21 impurity, 12, 14, 16 interface, 12 interstitial, 14, 15 isotope, 13 Jahn–Teller, 14 LCAO, 15, 22 localization, 22 magnetic, 11–13 marker, 22 melting, 11 minimal basis, 16 molecular dynamics, 16, 22 muﬃn-tin, 15 multiscale, 22 nanometer, 12

nanoscience, 12 nonlocal, 17 optical, 11, 12 order-N , 18 oxygen, 12, 14 Parrinello, 21 periodic, 12, 16 periodic boundary conditions, 15, 22 periodicity, 12, 15, 16 perturbation, 12–14, 19 phase diagram, 22 photoluminescence, 12, 13 PL, 12 plane-wave, 21, 22 platelet, 12 population, 22 potential, 14, 18–21 PRDDO, 16 precipitates, 12 pseudopotential, 16 quantum Monte Carlo, 18, 22 radiation damage, 14 Raman, 13 real space, 15 recombination, 12, 14 relaxation, 14 Sankey, 21 scattering, 15 scattering-Xα, 15 Schr¨ odinger, 13, 15, 18 self-energy, 22 self-interstitial, 12, 14 semiempirical, 15, 16 shallow, 12 Si, 11, 12, 14, 16, 22 SIESTA, 21 silicon, 14, 16, 21, 22 Slater, 18 spin, 12–14 stress, 13 substitutional, 13 supercell, 15, 16, 22 surface, 12, 13, 15, 16, 19 symmetry, 13–16, 21

27

28

David A. Drabold and Stefan K. Estreicher

temperature, 11, 12, 20, 22 Thomas–Fermi, 19, 21 tight binding, 21 total energy, 19, 21 transferability, 15 transient-enhanced diﬀusion, 12 transition metal, 11, 12, 14 uniaxial stress, 13

vacancy, 12, 14–16 valence band, 12 variational, 18, 20 vibrational modes, 22 vibrational spectroscopy, 12, 13 Wannier, 14 Watkins, 15

Supercell Methods for Defect Calculations Risto M. Nieminen COMP/Laboratory of Physics, Helsinki University of Technology, POB 1100, 02015 HUT, Finland [email protected]

Abstract. Periodic boundary conditions enable fast density-functional-based calculations for defects and their complexes in semiconductors. Such calculations are popular methods to estimate defect energetics, structural parameters, vibrational modes and other physical characteristics. However, the periodicity introduces spurious defect–defect interactions and dispersion of the defect-induced electronic states. For charged defects, compensating background charging has to be introduced to avoid electrostatic divergences. These factors, together with the intrinsic limitation of standard density-functional theory for accurate estimation of semiconducting gaps, pose challenges for quantitatively accurate and properly controlled calculations. This chapter discusses these issues, including point sampling, electrostatic (Madelung) corrections, valence-band (reference energy) alignment, and other ﬁnite-size eﬀects in supercell calculations. These are important for reliable estimation of formation and migration energies as well as ionization-level prediction. Moreover, the chapter discusses the various ways of generating transferable pseudopotentials, the choice of the exchange-correlation functional, and other topics related to total-energy calculations. Methods to calculate excitation energies and other spectroscopic properties as well as atomic motions are also discussed. Examples of applications of the supercell methods to a few selected semiconductor defects are presented.

1 Introduction An important role for theory and computation in studies of defects in semiconductors is to provide means for reliable, robust interpretation of defect ﬁngerprints observed by many diﬀerent experimental techniques, such as deep-level transient spectroscopy, various methods based on positron annihilation (PA), local-vibrational-mode (LVM) spectroscopy, and spin-resonance techniques [1]. High-resolution studies can provide a dizzying zoo of defectrelated features, the interpretation and assignment of which requires accurate calculations of both the defect electronic and atomic properties as well as quantitative theory and computation also for the probe itself. Materials processing can also draw signiﬁcant advantages of the predictive computational studies. The kinetics of defect diﬀusion and reactions during thermal treatment depend crucially on the atomic-scale energetics (formation energies, migration barriers, etc.), derived from the bond-breaking, D. A. Drabold, S. K. Estreicher (Eds.): Theory of Defects in Semiconductors, Topics Appl. Physics 104, 29–68 (2007) © Springer-Verlag Berlin Heidelberg 2007

30

Risto M. Nieminen

bond-making and other chemical interactions between the atoms in question. Accurately calculated estimates for defect and impurity energetics can considerably facilitate the design of strategies for doping and thermal processing to achieve the desired materials properties. Parameter values calculated atomistically, from the electronic degrees of freedom, can be fed into multiscale modeling methods for defect evolution, such as kinetic Monte Carlo, cellular automaton, or phase-ﬁeld simulation tools [2]. A defect in otherwise perfect material breaks the crystalline symmetry and introduces the possibility of localized electronic states in the fundamental semiconducting or insulating gap. Depending on the position of the host-material Fermi level of the host semiconductor, these states are either unoccupied or occupied by one or more electrons, depending on their degeneracy and the spin assignment. The defects thus appear in diﬀerent charge states, with varying degrees of charge localization around the defect center. To achieve a new ground state, the neighboring atoms relax around the defect to new equilibrium positions. For a point defect a new point symmetry group can be deﬁned. The energy levels in the gap, also known as “ionization levels”, “occupation energy levels” or “transition levels”, correspond to the Fermi-level positions where the ground state of the system changes from one charge state to another. Their values can be computationally estimated by the “∆SCF” approach, i.e., from total-energy diﬀerences between diﬀerent charge states. These gap levels can be probed experimentally by temperature-dependent Hall conductivity measurements, deep-level transient spectroscopy (DLTS), and photoluminescence (PL). The nature of the defect-related gap-state wavefunctions can be examined with electron paramagnetic resonance (EPR) and electron-nuclear double-resonance (ENDOR) measurements. Experimentally, the defect energy levels can often be located with the precision of the order of 0.01 eV with respect to host material band edges. The proper interpretation of the levels and the physical features associated with them pose demanding challenges for theory and computation. At present, the computational accuracy of the level position is typically a few tenths of an eV. It follows that sometimes diﬀerent calculations for the same physical system lead to very diﬀerent conclusions and interpretations of the experiments. Defect calculations may also fail to predict correctly the symmetrybreaking distortions around defects undisputedly revealed by experiments. While theoretical modeling has had considerable success and a major impact in semiconductor physics, there are still severe limitations to its capabilities. The purpose of this Chapter is to point out and discuss these. Density-functional theory (DFT) [3, 4] is the workhorse of atomic-scale computational materials science and is also widely used to study defects in semiconductors, predict their structures and energetics, vibrational and diffusional dynamics, and elucidate their electronic and optical properties, as observed by the various experimental probes. The central quantity in DFT is the electron density. The ground-state total energy is a functional of the

Supercell Methods for Defect Calculations

31

electron density and can be obtained via variational minimization of the functional. The wave-mechanical kinetic energy part of the total-energy functional is obtained not from the density directly but through a mapping to a noninteracting Kohn–Sham system. The mean-ﬁeld electrostatic Hartree energy is obtained from the density, as are in principle the remaining exchange and correlation terms, coded into the exchange-correlation functional. The purpose of this Chapter is to examine critically the methodological status of calculations of defects in semiconductors, especially those based on the so-called supercell methods. As will be discussed in more detail below, there are three main sources of error in such calculations. The ﬁrst is the proper quantum-mechanical treatment of electron–electron interactions, which at the DFT level is dependent on the choice of the exchange-correlation functional. The popular local or semilocal density approximations lead to underestimation, sometimes serious, of the semiconducting gap. The underlying reasons for this are the neglect of self-interactions and the unphysical continuity of the exchange-correlation energy functional as a function of leveloccupation number. This has naturally serious consequences to the mapping of the calculated defect electronic levels onto the experimental energy gap. The second source of errors is related to the geometrical description of the defect region, often known as the ﬁnite-size eﬀect. The third source of error is the numerical implementation of DFT, i.e., the self-consistent solution of the eﬀective-particle Kohn–Sham equations and the evaluation of the total electronic energy.

2 Density-Functional Theory The quantum physics of electrons in materials is governed by the Schr¨odinger equation. Density-functional theory (DFT) provides a parameter-free framework for casting the formidable many-electron problem to a numerically tractable form involving only the three spatial coordinates of the N interacting electrons (as opposed to 3N in the full solution of the Schr¨ odinger equation). The fundamental starting point is the DFT expression for the total energy Etot of the electronic system: 1 2 2 Etot {ψiσ (r), {Rα } = ψiσ (r) − ∇ ψiσ (r) 2m i,σ 2 e2 n(r)n(r ) + dr dr 2 |r − r | Zα Zβ 1 + drVion (r)n(r) + 2 |Rα − Rβ | α,β;α=β

+ Exc [n↑ (r), n↓ (r)] ,

(1)

32

Risto M. Nieminen

2 where the total electronic density n(r) = i,σ fiσ |ψiσ (r)| is expressed as a summation of the one-electron states ψiσ (r), dependent on the spin index σ =↓, ↑ and with the occupation number fiσ . Above, Vion is the nuclear (ionic) potential, and Zα denotes the charge of ion α at Rα . The coupled Kohn–Sham eigenvalue equations −

2 2 ∇ ψiσ (r) + Veﬀ [n↑ (r), n↓ (r)] ψiσ (r) = εiσ ψiσ (r) 2m

(2)

resulting from the minimization of Etot with respect to the density recast the complex many-body interactions into an eﬀective single-electron potential Veﬀ via the exchange-correlation functional Exc . In practice, the functional Exc has to be approximated. The popular choices are functionals where exchange and correlation are treated as functions of the local density and/or its gradients. This sounds drastic, because electronic Pauli exchange is a manifestly nonlocal object, as demonstrated by the Hartree–Fock theory. However, there is a partial cancelation of errors, and these methods are surprisingly robust and accurate. The generalization to spin degrees of freedom is also straightforward in scalar-relativistic DFT. A useful primer for designing DFT calculations has been written by Mattsson et al. [5]. The design of any calculation, whether using periodic boundary conditions, ﬁnite clusters or embedding techniques, involves the choice of the exchange-correlation functional. The choice, whether a particular ﬂavor of local-density (LDA) or local spin-density (LSDA) approximation, a generalized-gradient approximation (GGA), full Hartree–Fock-type exchange, screened exchange, or a “hybrid” between a nonlocal orbital-based functional and a density-dependent functional, deﬁnes the physical accuracy of the calculation. The numerical accuracy of the calculation depends on such technical things as basis-set completeness, accuracy of integration in both real and reciprocal space, convergence criteria, etc. The model accuracy depends naturally on how faithfully the chosen supercell, cluster or embedding methods describe the desired situation. In the context of defects in semiconductors, the ground-state properties can be obtained via the minimization of the total energy Etot with respect to the charge density n(r) and the ionic positions Rα through the Hellmann– Feynman interatomic forces. This enables the calculation of not only the formation energy of a defect in a given lattice position, but also its lowenergy vibrational excitations, and any observables accessible via the charge and spin densities, such as positron-annihilation parameters [6] or hyperﬁne ﬁelds [7–9].

3 Supercell and Other Methods A popular way to calculate defect energetics from ﬁrst principles (i.e., from electronic degrees of freedom) is based on the supercell idea. In this method

Supercell Methods for Defect Calculations

33

Fig. 1. Schematic presentation of the supercell construction. (a) lattice vacancy in a solid, (b) surfaces in a stack of slabs, (c) isolated molecules

one conﬁnes the atoms deﬁning the defect area of interest into an otherwise arbitrary box, which is then repeated inﬁnitely in one or more spatial directions (see Fig. 1). In other words, this box (the supercell) now becomes the new unit cell of the system, and periodic boundary conditions are applied at one or more of its boundaries. For a point-defect assembly in a three-dimensional solid, the system now becomes a three-dimensional periodic defect array. For a line defect (e.g., a dislocation) the result is a regular line-defect network. For a surface, the system becomes a sandwich of material slabs interlaced by vacuum regions. Typical sizes of the supercell are nowadays 64 atoms or larger in a cubic system, and the increasing computational power has enabled supercells with hundreds of atoms. The supercell method is one of the three main approaches to defect calculations. The other two are the ﬁnite-cluster methods [10, 11] and the Green’s function embedding techniques [12–14]. In the former the interesting defect is simply incorporated in a ﬁnite atomic cluster (with often atoms added to the cluster surface to saturate any dangling electron bonds). The ﬁnite-cluster method is well suited for studies of local defect properties (such as vibrational modes), provided that the cluster is large enough and thus the surface eﬀects small. However, care should be taken to make sure that manipulating the cluster surface does not interfere with the defect-localized electrons. Estreicher and Marinyck [15] have shown how this can inﬂuence, for example, the defect-related hyperﬁne ﬁelds. The embedding techniques, in turn, match the perturbed defect region to the known DFT Green’s function of the unperturbed host material, and oﬀer in principle the best way to study isolated defects. However, the numerical implementation of the Green’s function method is challenging for accurate interatomic forces and long-range atomic relaxations, as it requires a well-

34

Risto M. Nieminen

localized defect potential and usually short-range basis functions. Thus, supercell methods have surpassed the Green’s function methods in popularity. The great advantage of supercell calculations is that the periodic boundary conditions allow the utilization of the many eﬃcient techniques derived for the quantum physics of periodic systems. The wavevectors of the Brillouin zone (BZ) in the reciprocal space of the supercell are good quantum numbers, and the standard “band-structure methods” of periodic solids can be applied in full force. Particularly fast computation methods can be performed by using Fourier analysis (plane-wave basis sets), as they adopt naturally to periodic boundary conditions and oﬀer spatially uniform resolution. The supercell approach enables the full relaxation of the structure to minimize total energy, and the calculation of the formation and migration energies of defects in diﬀerent charge states as a function of the Fermi-level position of the host semiconductor, and as a function of the chemical potentials of the atoms building up the material. Thus, the method can be conveniently adapted to describe such eﬀects as the host material stoichiometry on the energetics of isolated defects in compound semiconductors [16]. From supercell calculations one can extract several useful physical properties, such as: 1. the probabilities of certain types of defect to form under given chemical and thermodynamical conditions during the growth, 2. the basic nature (acceptor, donor, deep level) of the defect electronic states, 3. the migration and recombination barriers, 4. vibrational modes, hyperﬁne ﬁelds, positron-annihilation parameters and other ground-state properties, and 5. within certain limitations, excited-state (for example optical) properties as well. The ground-state properties are those most reliably accessible. For example, the defect-induced electronic energy levels in the fundamental gap are obtained as diﬀerences between formation energies for diﬀerent charge states.

4 Issues with the Supercell Method The obvious drawback of the supercell methods for defect calculations is that the periodicity is artiﬁcial and can lead to spurious interactions between the defects. They have a ﬁnite density, and do not necessarily mimic the true physical situation with an aperiodic, very low density defect distribution. The supercell method, widely used and with demonstrated success in defect studies, requires a critical examination of the ﬁnite-size and periodicity eﬀects. The ﬁrst consequence of the ﬁnite-size supercell approximation is the broadening of the defect-induced electronic levels to “defect bands”, with a bandwidth of the order of 0.1 eV for 64-atom supercells. This translates into a diﬃculty in placing accurately the ionization levels, also in the total-energy based ∆SCF approach. The one-electron Kohn–Sham states associated with the defect are often assigned a position by averaging over the supercell Brillouin zone, or just values at the Brillouin zone origin (the Γ point) are dis-

Supercell Methods for Defect Calculations

35

cussed as they exhibit the full symmetry of the defect. It can be argued that the defect-state dispersion has a smaller eﬀect on the total energies that include summations and integrations of the Kohn–Sham states over the entire Brillouin zone. Thus, ionization levels determined from the total-energy differences would also be less sensitive to the defect-band dispersion. However, this is hard to prove systematically. Another source of diﬃculty is the accurate determination of the host crystal band edges (valence-band maximum, conduction-band minimum), which are the natural reference energies for the defect-induced gap states. In the defect-containing supercell, the band-edge states themselves are aﬀected by the defect. The band-edge positions are often determined by aligning a chosen reference level between the defect-containing and perfect solid. For example, the eﬀective potential in a localized region far from the defect can be aligned with the potential in the same region in a perfect crystal. The calculated band-edge distances from the reference energy in a perfect crystal can then be used to align the band edges in the system containing the defect. Alternatively, one can consider a deeper, core-level energy of an atom as a local reference. Another possibility is to deﬁne as the “crystal zero” the electrostatic potential at a Wigner–Seitz cell boundary far away from the defect. This is particularly convenient when the atomic-sphere approximation (ASA) is used in the context of minimal basis sets, such as the LMTO [17]. Another, more diﬃcult problem arises with charged defects. In order to avoid divergences in electrostatic energies, a popular solution is to introduce a homogeneous neutralizing background charge to the supercell array, which enables the evaluation of electrostatic (Coulomb) energies. This, however, introduces an electrostatic interaction between the periodic charge distribution in the supercells and the background, which vanishes only at the limit of inﬁnitely large supercells. The inﬂuence of the ﬁctitious charge has to be subtracted in the end, and this is a highly nontrivial task, as discussed below. Point defects induce elastic stress in the host lattice, which is relieved by ion displacements, i.e., lattice relaxation. The lattice-relaxation pattern is restrained by the supercell geometry. The argument, often used in supercell calculations, is that the ion displacements vanish near the borders of the supercell. However, this does not necessarily guarantee that the long-range ionic relaxations are correctly described, as the supercell symmetry itself may ﬁx the positions of the border ions. According to elastic continuum theory, the strain ﬁeld at large distances from the point defect should fall oﬀ as |r|−3 and −2 the ionic displacements should fall oﬀ as |r| . In tetrahedrally coordinated covalent materials the distances between the periodic images along the rigid [110] zigzag chains are typically more important to the convergence of lattice relaxations than the volume relaxations. A case in point is the vacancy in silicon [18], where the sense of the lattice relaxation changes from outward to inward only at large enough cell sizes. A similar behavior is also observed in ﬁnite-cluster calculations [19].

36

Risto M. Nieminen

The ﬁnite size of the supercell thus restricts also the ionic relaxations around the defect. The relaxation pattern is truncated midway between a defect and its nearest periodic replica. In the case of long-range relaxations this cutoﬀ may be reﬂected dramatically close to the defect, as was demonstrated by Puska et al. [18] by detailed calculations for vacancies in silicon. Further comparison of the supercell to the ﬁnite-cluster and Green’s function methods reveals the following. The supercell and Green’s function methods have a well-deﬁned electron chemical potential (they are coupled to a reservoir of electrons) whereas the cluster method does not. This has consequences for the treatment of ionization levels, which is somewhat problematic for the cluster method. The ﬁnite-size eﬀect is there in the cluster method as well, as the clusters can contain spurious surface-related eﬀects. The Green’s function method is mathematically elegant and in principle the best for isolated defects, but its computational implementation is diﬃcult in view of the accuracy required for total electronic energies and derived quantities (such as interatomic Hellmann–Feynman forces). Finally, it is important to note that defect and impurity calculations should, as a rule, be carried out using the theoretical lattice constant, optimized for the bulk unit cell. This is crucial in order to avoid spurious elastic interactions with defects or impurities in the neighboring supercells. The purpose is to investigate properties of isolated defects or impurities in the dilute limit. If the volume of the defect-containing supercell is relaxed (in addition to relaxing the positions of the atoms near the defect), the calculation would in fact correspond to ﬁnding the lattice parameter of the system containing an ordered array of defects at a high concentration.

5 The Exchange-Correlation Functionals and the Semiconducting Gap The fundamental semiconductor gap Eg is deﬁned as the diﬀerence between the ionization energy I and the electron aﬃnity EA of the bulk material, Eg = I − EA .

(3)

As both quantities can be written in terms of total energies of systems with diﬀerent numbers of electrons, the value of the gap Eg is, in principle, a ground-state property and can thus be calculated within the Kohn–Sham DFT. The fundamental gap can also be written as Eg = EgKS + ∆xc .

(4)

EgKS is the diﬀerence between the highest occupied and lowest unoccupied Kohn–Sham eigenvalues εiσ . ∆xc is the discontinuity (as a function of the occupation number) of the exchange-correlation potential at the Fermi level.

Supercell Methods for Defect Calculations

37

The estimation of semiconductor bandgaps and positions is one of the classic failures of local(-spin-)density (L(S)DA) formulation of the Kohn– Sham DFT. There are two origins of this error. First is the self-interaction error inherent in the LDA potential, and the second is the vanishing of the discontinuity ∆xc of the local-density exchange potential as a function of the level occupation at the Fermi level. They lead to both wrong absolute energy positions and too small or entirely absent bandgaps for many materials. This is not remedied by semilocal approximations for exchange and correlation, such as the generalized-gradient approximations (GGA) where the discontinuity also vanishes. In fact, the experience is that GGA approximations tend to make the gap even smaller than local-density approximations [20]. This can be traced to the property of GGA methods increasing the interatomic distances and lattice constants compared to LSDA. It is another well-known ﬂaw of local-density methods that they overbind molecules and solids and underestimate bond and lattice distances. GGA methods correct and sometimes overcorrect this, but give even smaller bandgap values. A qualitatively opposite problem is encountered with the Hartree–Fock method, which is known to considerably overestimate the bandgaps. Moreover, its application to metallic systems leads to well-known problems, such as the vanishing density of states at the Fermi level. Thus, intuitively, a hybrid method “interpolating” between the two seems an attractive approach. Nonlocal descriptions of exchange are expected to improve the Kohn– Sham bandgaps as they remove the self-exchange error and exhibit discontinuity at the Fermi level. In the “exact exchange” (EXX) formulation one evaluates the exchange energy and potential using the Kohn–Sham (rather than Hartree–Fock) wavefunctions. St¨ adele et al. [21] have shown that the discontinuity ∆x in the exchange potential is much larger than the bandgap for several semiconductors, which points to the existence of a large cancellation between the exchange ∆x and the corresponding correlation ∆c . The EEX method has been reported to give very good values for the bandgap and many other properties for sp semiconductors [22]. However, when applied to rare-gas solids, EXX fails to reproduce the experimental bandgaps [23]. A related problem is the position of the d band in many solids. Again, the self-interaction error in local-density methods displaces the d states and contributes to the bandgap error. The d band positions can be improved by the explicit removal of self-interactions [24], but the application of the nonlocal EXX does not seem to lead to a consistent improvement of both d band positions and bandgap values. This points to the important interplay between treatment of nonlocal exchange and the description of the lower-lying and core states in semiconductors and insulators. It has recently been pointed out [25] that the lack of explicitly treated core-valence interactions can lead to an anomalously good agreement of the calculated Kohn–Sham gap with the experimental gap in sp semiconductors. The inclusion of these interactions worsens the agreement, while leading to a consistent treatment of semiconductors and insulators. It

38

Risto M. Nieminen

thus appears that the EXX alone does not solve the bandgap problem, although it is a marked improvement over LDA or GGA. A major drawback is also the high computational cost of EEX, which has so far prohibited its widespread use in defect calculations. In the screened-exchange LDA (sx-LDA) scheme [26] the Kohn–Sham single-particle orbitals are used to construct a nonlocal exchange operator, again improving the description compared to the local-density approximation. The many-body correlations and screening missing from the Hartree–Fock method are treated in a form of model screening and LDA correlation. This approach can solve the gap problem, but contains a phenomenological constant (e.g., the Thomas–Fermi screening constant). Lento and Nieminen [27] have applied this method for a prototypical supercell defect calculation (vacancy in Si). While the method can in principle give accurate total energies and thus ionization levels (and the correct gap), its full exploitation is still prohibitively expensive computing-wise. As with other hybrid functionals and with EXX, the computational cost is typically two orders of magnitude larger than with LDA or GGA. Thus the calculations with full lattice relaxation have so far been limited to supercells not large enough to allow the correct pattern to emerge (see Sect. 16 below). There are other suggested approaches to overcome the failure of DFT to produce accurate bandgaps and excited-state properties. However, currently no method is available that would go beyond standard DFT and yet be feasible for total-energy calculations for the large supercells required to investigate defects. The class of methods, such as the GW approach [28] which are mainly aimed at calculating the (quasiparticle) band structure and properties derived thereof, are prohibitively expensive for large supercells. Presently, such calculations can be carried out with supercells with less than twenty atoms. However, this size is perfectly adequate for treating well-localized excitations, such as self-trapped excitons [29]. The gap problem may sometimes make calculations for certain defect levels impossible. The too-narrow gap may induce the defect level to be a resonance in the conduction or valence band. In this case some charge states would not be accessible at all. It should be noted that this can also happen in just some part of the Brillouin zone because of the defect-level dispersion in the supercell approach. A possible remedy is then to simply occupy the defect level, ignoring the fact that the state lies above the conduction-band minimum at other k points. Apart from underestimating the bandgap and thus hampering the positioning of the possible ionization levels, the local (or quasilocal)-density approximation for exchange and correlation can sometimes lead to other difﬁculties with the defect-localized electron states. This has recently been discussed by Laegsgaard and Stokbro [30]. They considered a substitutional Al impurity on the Si site in SiO2 . LDA and GGA calculations predict a structure that has the full tetrahedral symmetry. However, ENDOR experiments show unambiguously that the defect wavefunction is localized on just one of

Supercell Methods for Defect Calculations

39

the four neighboring oxygen atoms, as the hyperﬁne splittings are radically diﬀerent from those expected for four equivalent neighbors. The source of this problem can again be traced to the self-interaction error in LDA and GGA. In LDA/GGA, there is a penalty for localizing a single electron as the cancelation between self-exchange/correlation and self-Coulomb interactions is not complete. Thus, one overestimates the Coulomb energy of a localized state, which then leads to charge delocalization. In the true situation, there is just a single electron state contributing to the Coulomb energy. Thus, the calculated charge delocalization is completely due to self-interaction. If exchange is treated correctly as in the Hartree–Fock theory, self-interaction is eliminated and one obtains the correct distorted structure with the wavefunction localized on a single oxygen atom. As noted above, the problem with Hartree–Fock is that it seriously overestimates the bandgap and spin splittings, and is as such usually not a good tool for calculations of semiconductor defects. A self-interaction-corrected (SIC) scheme for the case of hole trapping in SiO2 was recently suggested by d’Aveszac et al. [31]. In their approach the Coulomb energy arising from the charge density of a single defect orbital and the associated contribution to the exchange-correlation energy are explicitly subtracted. This is technically straightforward for methods using localized basis sets, but can also be implemented using projection techniques with plane-wave methods. The physical idea of this self-interaction correction is that delocalized states do not suﬀer as much from self-interaction error as localized states do. In the standard SIC [32, 33] approaches there is some ambiguity in choosing the states to which the correction should be applied. For defect calculations, the localized state in the gap is well deﬁned and the application of the correction is quite straightforward. The LDA/GGA gap error is a persistent and rather harmful problem in semiconductor defect physics. The Kohn–Sham eigenvalues of (2) are Lagrange parameters used to orthogonalize the states in total-energy minimization, but cannot be interpreted as true electron-excitation energies. These could be obtained from quasiparticle theories such as Hedin’s GW approach [34] or time-dependent density-functional theory [35]. The GW method is computationally expensive and cannot be applied to defect supercells with many atoms. Its ability to give converged total energies is not clear. However, it is a powerful approach for doing perturbative calculations for optical and other excitation spectra, and can be generalized to include the ﬁnal-state electron–hole interactions through the Bethe–Salpeter equation [36]. One simple, obvious and often used possibility is to use the “scissor operator”, i.e., to correct the bandgap by simply shifting the unoccupied and occupied states further away from each other. This, of course, destroys the self-consistency between Kohn–Sham eigenvalues and eigenfunctions, which may be detrimental for observables calculated from them. For defect physics, the question arises whether to shift the defect levels or not in such a process.

40

Risto M. Nieminen

Intuitively, one would expect acceptor-like levels to move with the valenceband edge and donor-like states with the conduction-band edge, while levels deep in the bandgap would not move at all. This reasoning is, of course, quite arbitrary and unsatisfactory. A recent example of these diﬃculties is the work on the oxygen vacancy in ZnO, where the LDA gap is again considerably in error. Two calculations [37, 38] have addressed this system using the LDA+U method [39], where an onsite Coulomb repulsion U is added “by hand” when calculating the Zn d-states. This shifts the occupied d bands and subsequently the valence-band minimum downwards. The defect level associated with the oxygen vacancy then moves deeper into the gap from the valence-band maximum. If one leaves the defect level in place and shifts just the conduction bands up, there is a single level in the lower half of the gap. If, on the other hand, one decides from LDA+U calculation how much valence/conduction band character the state has, one ends up moving the state further up in the gap, into the upper half. As the experiments are ambiguous at this time, the matter is undecided and again calls for a better solution to the gap problem. Finally, one should mention the quantum Monte Carlo (QMC) methods that look promising for addressing total-energy calculations for defects and impurities. They approach the problem of interacting electrons by addressing the correlations explicitly and build in the Pauli exchange by starting from a Slater determinant. The ﬁxed-node QMC method has been applied to study self-interstitials in Si [40]. The formation energy of the split-110 interstitial defect was found to be signiﬁcantly higher with QMC than LDA, which can be explained by the upward shift of the defect-induced level in the bandgap. Further work includes QMC studies of optical and diﬀusive properties of vacancies in diamond [41]. If QMC methods can be extended to large enough supercells, to force and relaxation calculations, and to secured convergence with respect to k-point summation, they can provide a most useful set of benchmarks for accurate total-energy calculations for defects in semiconductors. The above discussion may give an overly pessimistic impression of the capabilities of DFT calculations for defects in semiconductors. The other side of the coin is much brighter. There is a vast inventory of “standard” DFT calculations that have produced robust and reliable results for semiconductor defects and have thus decisively contributed to their identiﬁcation. An illustrative example is the extensive work on III–V nitride semiconductors, recently reviewed by Van de Walle and Neugebauer [42].

6 Core and Semicore Electrons: Pseudopotentials and Beyond The widespread use and success of DFT in predicting various materials properties stems largely from the successful application of the pseudopotential (PP) concept. Only relatively few “valence” electrons of an atom are

Supercell Methods for Defect Calculations

41

chemically active. The replacement of chemically inert “core” electrons with an eﬀective core potential both reduces the number of electronic degrees of freedom and avoids the numerical challenge posed by rapidly varying wavefunctions near the nucleus. Eﬃcient numerical techniques such as the fast Fourier transform (FFT) can be used. The replacement of the all-electron potential with a PP is, however, a nontrivial task where a balance has to be struck between optimal transferability (accurate reproduction of all-electron atom behavior) and computational eﬃciency (slow spatial variability). Several methods are popular for generating PPs. They include the generalized norm-conserving pseudopotentials of Hamann [43], Troullier and Martins [44], Hartwigsen et al. [45] and the ultrasoft, non-norm-conserving PPs of Vanderbilt [46]. It is important to realize that the true ﬁgure of merit of a PP is not how well its results match experiment, but how well it reproduces the results of all-electron calculations when using otherwise similar methods. The separable PPs commonly used in the context of plane-wave calculations, such as those of the Kleinman–Bylander [47] form, are built from norm-conserving PPs. The separation process can sometimes add complications, for example, in the form of so-called ghost states. The construction of reliable ultrasoft pseudopotentials [46] or projected-augmented-wave (PAW) potentials [48, 49] presents additional challenges, but the latter is quickly gaining in popularity as it has proven a particularly robust and transparent approximation. To compare calculated values reported in the literature for defects in semiconductors, speciﬁc details of the PP generation are important for the reproduction of a given result. Several parameters usually enter the PP construction, such as the core radii for diﬀerent angular-momentum channels and the core-matching radii. The eﬀectiveness of a given PP needs to be checked and validated in every new chemical environment before being used in quantitative studies. Constructing PPs thus involves compromises, and in reporting computational results it is important to state those compromises clearly. In particular, the choice of a given state as an “active” valence state vs. its treatment via perturbative, nonlinear core-valence corrections [50] are crucial. For example, it has been demonstrated [51] that a nonlinear core-valence correction is necessary to get spin-polarized states of ﬁrst-row atoms O and N properly described. Unlike previously assumed, the 1s core in these atoms is not so deep as to be uninvolved in the chemistry important in deﬁning the valenceelectron potential. An interesting approach that yields bulk band structures in good agreement with experiment is based on the idea of self-interaction and relaxationcorrected pseudopotentials (SIRC) [52]. The removal of self-interactions has important consequences for ionization levels in the semiconducting gap, as discussed above. However, it seems that the SIRC approach does not allow a simple self-consistent calculation of total energies.

42

Risto M. Nieminen

Finally, it should be emphasized that consistency in the choice of the exchange-correlation functional for pseudopotential construction and their application is highly advisable. The problems of using a diﬀerent functional for the two have been demonstrated, especially in the cases where polarizable semicore states are present [53].

7 Basis Sets The use of DFT is not limited to static electronic-structure problems such as total energies and bond distances. The potential-energy (Born–Oppenheimer) surface deﬁned by the positions of the nuclei deﬁnes the interatomic forces, and in recent years there has been rapid growth in the use of ﬁrst-principles molecular dynamics (FPMD) within the ﬁnite-temperature DFT framework for studying many materials properties, including atomic vibration and migration, and the full equation of state (EOS). If the force ﬁelds or pressure or stress tensor of the system are of interest, additional care must be taken to ensure that the calculated quantities are of suﬃcient numerical accuracy. Whereas errors in the total energy are second order with respect to errors in the electron density or Kohn–Sham eigenfunctions, errors in the interatomic forces and pressure are ﬁrst order. The errors are signiﬁcantly aﬀected by the completeness and accuracy of the basis set. A popular choice is the plane-wave expansion for the Kohn–Sham states, ψnσk (G) exp[−i(k + G) · r] . (5) ψiσ (r) = ψnσk (r) = G

The summation is over the reciprocal lattice vectors G of the superlattice. In plane-wave calculations the accuracy of the basis set is determined by 2 2 max ) the chosen kinetic energy cutoﬀ or maximum wavevector Ecut = (k+G . 2m It is important to realize that while a lower cutoﬀ may be suﬃcient for the convergence of total energies, it may be totally unacceptable for calculating interatomic force constants or pressure/stress tensors. The reason that forces are more sensitive to the plane-wave cutoﬀ than total energies is that the real-space force formula contains the derivatives with respect to coordinates (see (6)). This derivative will introduce an extra factor of the reciprocal lattice vectors G into the reciprocal-space formulae and the maximum value Gmax is determined by the cutoﬀ. It also follows that exchange-correlation functionals involving gradients of the density (such as GGA) are more sensitive to the cutoﬀ than LDA. The issue of basis-set suﬃciency is even more critical when using local basis sets, for example linear combinations of numerical atomic orbitals [54, 55] or Gaussians [56]. A great advantage of local-orbital methods is the much smaller size of the basis (typically up to twenty basis functions per atom),

Supercell Methods for Defect Calculations

43

reﬂecting their economy when ﬁtting rapidly varying wavefunctions. However, as a discrete set the convergence of a local basis is not simply controlled by a single parameter. Local basis sets always require “optimization” and experience, and tested basis sets are collected into libraries with limited possibilities for modiﬁcation. The words of caution about plane-wave basis-set convergence apply even more strongly to local basis sets. While a well-designed basis set (for example, the “double-zeta plus polarization” (DZP)) does match the accuracy of a fully converged plane-wave calculation, the omission of the polarization term or calculation with single s and p functions can lead to large errors. This is particularly true for forces. For atoms far from equilibrium (e.g., under large strain) it may be necessary to increase variational freedom by expanding the basis to triple functions to achieve convergence. In some cases, especially for systems with large open volumes, it is advisable to augment the basis set by introducing “ﬂoating orbitals”, i.e., basis functions not centered at atoms. Finally, one should mention the real-space methods quickly gaining popularity [57,58]. They use ﬁnite-diﬀerence approximations for the kinetic-energy operator (ﬁnite elements are also a possibility), and the quality of the basis set can be controlled simply by the choice of the spacing of the real-space grid. The great advantage of real-space techniques is their easy adaptability to diﬀerent boundary conditions (periodic, open, etc.), which is especially useful for studies of defects in low-symmetry nanostructures, where supercell methods can be quite wasteful.

8 Time-Dependent and Finite-Temperature Simulations Within the Born–Oppenheimer approximation, the electronic and ionic motion and timescales are well separated. First-principles molecular dynamics (FPMD) can be implemented on the Born–Oppenheimer hypersurface by calculating an instantaneous value for the electronic total energy Etot [{Ri }] as determined by all the ionic positions {Ri }. The forces acting on the atoms are then evaluated as Fi = −

∂Etot ∂Ri

(6)

and Newton’s equations of motion are solved for the ionic degrees of freedom, using standard algorithms for the second-order temporal diﬀerential equations. Periodic boundary conditions are routinely implemented, and allow simulations of disordered amorphous or liquid phases. A ﬁxed-volume supercell with conserved total energy corresponds to the microcanonical statistical ensemble. The constant-temperature (canonical) ensemble can be simulated using the Nos´e–Hoover thermostat [59, 60]. Allowing the supercell volume to change as a dynamical variable leads to the constant-pressure ensemble,

44

Risto M. Nieminen

and structural phase transformations are enabled by making the directional vectors spanning the supercell also dynamical [61]. The molecular-dynamics techniques also enable free-energy simulations. The thermodynamic integration formula for the (Helmholtz) free energy reads 1 dλ H1 − H0 λ , (7) ∆F = 0

where ∆F is the free-energy diﬀerence between the actual system with the Hamiltonian H1 and a reference system with the Hamiltonian H0 , and . . . λ denotes a temporal average along an isobaric-isothermal trajectory generated from the Hamiltonian H(λ) = λH1 + (1 − λ)H0 .

(8)

Under ergodic conditions this is equivalent to an ensemble average. If the free energy of the reference system is known, (7) allows one to compute the free energy of the actual system. The FPMD method is particularly well adaptable to the supercell geometry. The quantum dynamics associated with the electronic degrees of freedom can be described by the time-dependent Schr¨ odinger equation. Within the density-functional formulation of many-body systems, this leads to the powerful formulation of time-dependent density-functional theory [62]. It can be cast in the form of time-dependent Kohn–Sham equations with a generalized, time-dependent exchange-correlation potential. These equations can be explicitly solved by time-propagation algorithms and starting from an appropriately prepared initial state. The time evolution of the wavefunctions and the density can then be analyzed to obtain the desired physical quantities, such as the full response of the system to an external, polarizing ﬁeld or exciting pulse. The Kohn–Sham equations with an external time-dependent perturbation can also be treated in the linear-response limit if the perturbation is weak. As the Kohn–Sham states are noninteracting, the linear-response function of the system can be constructed. The linearization leads to integrodiﬀerential equations with an exchange-correlation kernel derived from the description of Exc . Linear-response TDDFT is a popular method [63] to estimate excitation energies, polarizabilities and inelastic-loss properties (such as photoabsorption cross sections), especially for ﬁnite systems. The treatment of extended systems (periodic boundary conditions) within TDDFT requires the consistent handling of electronic currents in the system, and is best characterized as time-dependent current-density-functional theory (TCDFT) [64].

9 Jahn–Teller Distortions in Semiconductor Defects The Jahn–Teller eﬀect is the removal of electronic degeneracy by spontaneous lowering of spatial symmetry of atoms surrounding a defect, which leads to

Supercell Methods for Defect Calculations

45

Fig. 2. The splitting of the defect-related gap states for a vacancy in Si. The point symmetry group is denoted for defects in diﬀerent charge states. The arrows denote the population of the two spin states

the lowering of total energy. This is the result of a general theorem [65], with several well-known consequences in solid-state physics. It is easiest to discuss the Jahn–Teller mechanism by using the monovacancy and a substitutional metal impurity in a tetrahedrally bonded semiconductor (Si) as examples. These same systems will later be presented as examples of state-of-the-art supercell DFT calculations in Sect. 16. 9.1 Vacancy in Silicon In the pioneering linear combination of atomic-orbitals (LCAO) model by Watkins [66] (see Fig. 2), the electronic conﬁguration of a neutral vacancy in Si (VSi ) with full cubic (Td ) symmetry is a21 t21 , analogous to a Si atom ([N e]3s2 2p2 ). The a1 state lies in the valence band (is a resonance) and is doubly occupied. The other state t1 is in the fundamental gap and can contain up to six electrons. It is pushed into the gap by the repulsive potential due to the removal of a positive ion in the lattice. In compound semiconductors, therefore, the states are expected to lie higher for anion vacancies with a larger number of removed valence electrons than for cation vacancies. The ﬁlling of the gap states with rising Fermi level is associated with the relaxations of the atoms neighboring the defect. If there are no electrons in these levels, the Td symmetry of the ideal vacancy (ideal crystal) is preserved. The only possible relaxation is of the breathing-mode symmetry around the defect center. Adding one or more electrons to the levels splits the degeneracy through the Jahn–Teller eﬀect, and lowers the symmetry through atomic relaxation. The main component of this distortion is tetragonal, giving D2d symmetry. This can occur in two senses, giving either a short, broad (“type A”) or long, thin (“type B”) shape for the box bounding the nearest-neighbor atoms (see Fig. 3). This determines the order of the resulting b2 and e states. For VSi , the latter option turns out to be valid. One electron added to the gap level thus results in a singly positively charged vacancy with D2d symmetry. Adding more electrons usually implies

46

Risto M. Nieminen

Fig. 3. The bounding boxes for the Si vacancy with distortions of diﬀerent pointsymmetry orientation

higher total energies because of the intraelectron Coulomb repulsion between the localized electrons in the gap states. However, adding a second electron to the vacancy in Si can enhance the pairing distortions (while retaining D2d symmetry) and the Jahn–Teller splitting, possibly outweighing the increased Coulomb repulsion. This is the negative-U phenomenon [67] often encountered in semiconductor defects. Another way of stating the eﬀect is to say that the energy to remove two electrons from VSi0 is less than to remove one electron. Thus VSi+ would be unstable. A trigonal distortion from Td symmetry occurs when a third electron is added and the vacancy is in the charge state q = −1. This lowers the symmetry to or C2v or C3v and splits the e state to b2 and b1 . The quantitative results of state-of-the-art supercell calculations for the charge-state-dependent relaxation and how they match the Watkins model are given in Sect. 16. 9.2 Substitutional Copper in Silicon Neutral CuSi [68] is isoelectronic with the negatively charged VSi (see Fig. 4). The triplet state t32 is partially occupied, in the bandgap, and susceptible to the Jahn–Teller eﬀect. If onsite electronic repulsion prevails, the high-spin S = 3/2 states would be stabilized, as for example in the case of negatively charged substitutional Ni in diamond or the silicon vacancy in SiC [69]. Spinorbit coupling also aﬀects the orbital degeneracy, especially for the heavier impurity elements.

Supercell Methods for Defect Calculations

47

Fig. 4. The evolution of the defect-related states of substitutional Cu in Si from those for a Cu atom and Si vacancy

In general, it is in principle possible to reach higher positive and negative charge states by adding/removing electrons to/from the localized levels. The stability of a given charge state requires accurate calculation of its total energy, and is subject to the computational limitations discussed above and further expanded upon in Sects. 13–15.

10 Vibrational Modes The phonon modes of a vibrating solid can be calculated using the powerful linear-response formalism [70], where the DFT total-energy hypersurface enters as the ground state and determines the elastic response. This formalism has been implemented using diﬀerent basis sets for bulk calculations, including short-range local orbitals [71]. For defects in semiconductors, it is, however, the localized vibrational modes (LVMs) associated with defects that are often useful ﬁngerprints for defect identiﬁcation. In the case of defectassociated localized modes, a more economical route than the full phonon response is provided by considering only a single supercell. This is because the interaction between the defect replicas can be made small by using a large enough cell, whereby the vibrations do not mix and there is no phonon dispersion. The total energy of the supercell can be written as a Taylor series around the equilibrium positions in the harmonic approximation as 1 ∂ 2 Etot sαi sβj + · · · , Etot [{Rαi + sαi }] = Etot {Rαi } + 2 ∂Rαi ∂Rβj αi,βj

(9)

48

Risto M. Nieminen

where sαi is the ith Cartesian component of the atomic displacement of the ion α. The coupling constants ∂ ∂Etot

(10) ≡ Φαi βj ∂Rαi ∂Rβj are conveniently obtained as numerical derivatives of the (Hellmann–Feynman) forces on the atoms as they are shifted a small distance from their equilibrium positions around the defect (“frozen phonons”). The frequencies ω and amplitudes u of the localized vibrations can then be obtained as the normal-mode solutions to the equations βj −ω 2 uαi + Dαi , uβj = 0 , (11) βj

where

βj Dαi

is the dynamical matrix. If Mα is the mass of ion α,

1 βj Dαi ≡ Φαi βj . Mα Mβ

(12)

In practical LVM calculations, selected atoms in the supercell are displaced to all three Cartesian directions, and after each displacement the ground-state electronic total energy is obtained and the Hellmann–Feynman forces calculated. This is done for all atoms that are a priori considered important for the description of the local vibrational modes around the defect. The dynamical matrix is then calculated by the ﬁnite-diﬀerence approximation using these forces and displacements. The normal modes and the corresponding vibrational frequencies can then be obtained by diagonalizing the dynamical matrix. The harmonic modes can easily be quantized and the zero-point vibrational motion estimated. Within the harmonic approximation, the phonon spectrum can be used to estimate the vibrational entropy of a given defect, which can then be entered as the prefactor when estimating absolute defect concentrations in thermal equilibrium. Alternatively, the phonon spectrum, including the localized modes, can be obtained by MD simulation. The simulation time has to be long enough so that all the relevant vibrational modes have undergone several oscillation periods. The vibrational frequencies can then be obtained by Fourier transforming the velocity autocorrelation function of the moving ions. This usually requires that the LVM is well separated from the density of states for host-lattice vibrations. The MD approach includes also the anharmonic contributions to the vibrations, but not the zero-point motion.

11 Ionization Levels The formation energy of a defect or impurity X in the charge state q is ni µi + q [µe + Ev ] , (13) E f [X q ] = Etot [X q ] − Etot [bulk] − i

Supercell Methods for Defect Calculations

49

where Etot [X q ] is the total energy from a supercell calculation with a defect or an impurity in the cell, and Etot [bulk] is the total energy of the equivalent bulk supercell. ni indicates the number of atoms of type i (host or impurity), either added (ni > 0) or removed (ni < 0) from the defected supercell, and µi denote the corresponding atomic chemical potentials. They represent the energy of the reservoirs with which atoms are exchanged when assembling the crystal in question. µe is the electron chemical potential (Fermi level), referenced here to the valence-band maximum Ev in the bulk material. The valence-band maximum of defect supercell has to be aligned with that in the bulk (see below). For a monoatomic solid, the formation energy for a defect in the charge state q reads Eqf = Eqdef − N µ + q(Ev + µe ) ,

(14)

where Eqdef is the total energy of the defect-containing supercell and N the total number of atoms in it. The thermodynamic ionization (transition) level of a given defect Ed (q/q ) is deﬁned as the Fermi-level position where the charge states q and q have equal total energy. In experiments where the ﬁnal charge state can relax to its equilibrium conﬁguration after the transition (excitation), this is the energy level that would be observed. The ionization levels are therefore observed in DLTS experiments or (for shallow levels near band edges) as the thermal ionization energies derived from temperature-dependent conductivity or Hall eﬀect data. The optical energy Edopt (q/q ) associated with a transition between charge states q and q is deﬁned similarly to the thermodynamic transition energy, but now the ﬁnal state with charge q is calculated using the atomic geometry of the initial state q. The optical level is observed in “vertical” absorption experiments where the ﬁnal charge state cannot relax to its equilibrium. In emission experiments, on the other hand, the initial excited state has evolved towards its minimum-energy conﬁguration, which is diﬀerent from the ground-state structure. Optical emission and absorption peaks are thus separated by the so-called Stokes shift. This poses challenges for both the experimental assignment of peaks and the theoretical analysis. For a two-component (compound) semiconductor, (13) can be rewritten [16] in a form that reﬂects the stoichiometry of the host material. It is gauged by the chemical potential diﬀerence ∆µ of an AB compound as ∆µ = µA − µB − [µA (bulk) − µB (bulk)] ,

(15)

with an allowed range −∆H ≤ ∆µ ≤ ∆H ,

(16)

50

Risto M. Nieminen

where the lower limit corresponds to A-rich and the upper limit B-rich material. ∆H is the heat of formation of the compound from its bulk constituents, ∆H = µA (bulk) + µB (bulk) − µAB (bulk) .

(17)

By deﬁning E1f [X q ] ≡ Etot [X q ] − 12 (nA + nB )µAB (bulk) − 12 (nA − nB )[µA (bulk) − µB (bulk)] + qEv

(18)

one can write (13) in the short form E f [X q ] = E1f [X q ] + qµe − 12 (nA − nB )∆µ .

(19)

Equations (14) or (19) provide a basis for evaluating the ionization level between charge states q and q + 1 as the value of µe where the two formation energies are equal. This is a widely used technique for defects in semiconductors. It requires the accurate determination of the supercell total energies, and uses the valence-band maximum as the absolute reference energy (alternatively, the electron chemical potential can be measured from the conduction-band minimum). Although it makes no explicit reference to the eigenvalues of the Kohn–Sham gap states, the method can suﬀer from the DFT underestimation of the bandgap, especially if the state in question is far from the reference energy, close to the opposite band edge.

12 The Marker Method The problems of bandgap underestimation and valence-band alignment can to some extent be avoided in using the so-called marker method for calculating ionization-level positions [72]. Let us deﬁne the conﬁguration energy for a defect labeled d as the total energy diﬀerence per unit charge between two charge states

(20) Cd (q/q ) = Etot X q − Etot [X q ] (q − q ) . If there is a measured or otherwise accurately known reference (“marker”) defect m with the ionization level Em (p/p ) between charge states p and p in the region of interest in the semiconductor bandgap, one can calculate its conﬁguration energy Cm (p/p ) and the conﬁguration energy diﬀerence of d from the marker as Dd (q/q ) = Cd (q/q ) − Cm (p/p ) .

(21)

Then the ionization level of interest can be estimated as Ed (q/q ) ≈ Dd (q/q ) + Em (p/p ) .

(22)

Supercell Methods for Defect Calculations

51

The idea is to achieve systematic cancelation of computational errors. This happens best when the defects d and m are similar and all computational parameters are the same. The reference energy may also be taken as the valence-band maximum and the conduction-band bottom of the bulk supercell with the same number of atoms as the defect supercell, whereby bulk (0/ + 1) = Ev Cm

bulk and Cm (−1/0) = Ec ,

(23)

and the bandgap is bulk bulk Eg = Cm (−1/0) − Cm (0/ + 1) .

(24)

The marker method can provide a useful alternative for ionization-level determination, but requires the knowledge of a suitable known transition level in the vicinity of the level under scrutiny.

13 Brillouin-Zone Sampling For a perfect (no defects) lattice, the convergence of electronic properties can be achieved either by increasing the number of k points in the BZ or the product of the number of atoms (N ) in the calculational unit cell and the number of k points. The computational cost increases linearly with the number of k points but is proportional to at least N 3 . Thus increasing simply the number of k points would seem most economical. However, for defect calculations the spurious defect–defect interactions are a more subtle issue. For defects in metals already quite small supercells may give well-converged results if the number of k points is large enough. For defects in semiconductors the situation is more diﬃcult. Their description involves localized gap states. The description of these is not straightforwardly improved as the number of k points increases, i.e., the detailed choice of the k-point sampling may aﬀect the convergence. In supercell calculations, the evaluation of a ground-state property P of the system, such as total energy, requires integration over the Brillouin zone (BZ) of the reciprocal cell 1 3 d k pn (k)f [εn (k)] , (25) P = VBZ BZ n where VBZ is the volume of the BZ, n enumerates Kohn–Sham states with the wavevector k and eigenvalue εn (k), and pn deﬁnes the physical property. f [εn (k)] is the occupation number of the Kohn–Sham state, given by the Fermi–Dirac distribution around the chemical potential µe as 1

f [εn (k)] = e

µe −εn (k) kB T

. +1

(26)

52

Risto M. Nieminen

For semiconductors with a ﬁnite gap between occupied and unoccupied states, the integrand in (25) is continuous, and consequently the integral can, in principle, be replaced by a ﬁnite sampling of discrete k points. The computational cost increases linearly with the number of k points, and “special point” schemes are popular to reduce the computational cost to obtain the desired accuracy [73]. In particular, the uniform k-point mesh approach suggested by Monkhorst and Pack [74] has been widely used in practical calculations. For very large actual supercell sizes, the BZ shrinks towards a point (the Γ -point, the k = 0 of the BZ). Γ -point sampling oﬀers additional savings in computing as the Kohn–Sham wavefunctions are purely real at k = 0. The simplest scheme to sample the BZ in supercell calculations is to use the Γ point only. When the size of the supercell increases, the wavefunctions calculated correspond to several k points of the underlying perfect bulk lattice, and the perfect lattice k space is evenly sampled. In order to improve the description of, in particular, that of the delocalized bulk-like states and the description of the electron density, it is beneﬁcial to use k points other than the Γ point. Thereby also components with wavelengths larger than the supercell lattice constant are included. This idea leads to the special k-point schemes mentioned above. They are widely used to sample the BZ also in defect calculations. The accuracy of a given k-point mesh depends naturally on the supercell size (BZ volume). Makov et al. [75] utilized this fact to suggest sampling meshes that would in fact extrapolate the integration result towards larger unit-cell sizes. They proposed a scheme to choose k points for supercell calculations so that the electronic defect–defect interactions are minimized in the total energy. Defect calculations often focus on total-energy diﬀerences, and a tacit assumption is that errors due to BZ sampling largely cancel out when taking the diﬀerences (bulk vs. defect, for example) treated with equal-size supercells. This assumption is not a priori warranted and should be checked carefully. It has been demonstrated [76] that even for relatively large supercells the sampling errors can depend on the defect type and charge state and thus do not cancel when taking the diﬀerence. Shim et al. [76] investigated vacancy and interstitial defects in diamond and silicon, and found that for a given supercell size, the k-point sampling errors in the total energy can vary considerably depending on the charge state and defect type.

14 Charged Defects and Electrostatic Corrections Although the supercell approximation describes accurately and in an economical way the crucial local rearrangement of bonding between atoms and the underlying crystal structure, it also introduces artiﬁcial long-range interactions between the periodic images. The most dramatic artefact is the

Supercell Methods for Defect Calculations

53

divergence of the overall electrostatic (Coulomb) energy for charged defects in the periodic superlattice. This divergence of the total energy of charged defects in the supercell approximation is usually circumvented by the introduction of a ﬁctitious neutralizing background charge, often in the form of a uniform “jellium” distribution. The inﬂuence of this neutralizing charge in the total energy of the supercell needs to be included. This is known as the electrostatic or Madelung correction ∆Ec . With the neutralizing background added, in the large-supercell limit the electrostatic interaction of a charged defect with its periodic images in an overall neutralized system becomes, in principle, negligible. However, there is no guarantee that the convergence of the Coulomb energy as a function of the supercell size is particularly fast [77]. In fact, classical electrostatics for localized charges in an overall neutral system predicts an asymptotic L−1 √ 3 dependence, where L = V and V is the supercell volume. This scaling law is unfortunately slow in converging, and, moreover, its prefactor is in general unknown. Consequently, electrostatic errors are easily introduced into totalenergy calculations and they do not necessarily cancel when taking energy diﬀerences, as the magnitude depends on the details of the charge distribution within the supercell. Over the years, several attempts to reliably estimate ∆Ec have been proposed. Leslie and Gillan [78] and Payne and coworkers [79, 80] have developed correction formulae to be applied for electrostatic correction of charged-defect arrays. They considered an array of localized charges immersed in a structureless dielectric and neutralized by jellium compensation. By considering the multipole expansion of the defect charge distribution, the correction formula can be derived in the form ∆Ec ≈ −

2πqQ q2α − + O(L−5 ) , 2εL 3εL3

(27)

where q is the charge of the defect, α the Madelung constant of the superlattice, and ε the static dielectric constant of the host material. For cubic geometries, α is 2.837 3, 2.888 3 and 2.885 for SC, BCC and FCC supercells, respectively. The ﬁrst term corresponds to a point-charge array and a compensating background in a uniform dielectric. The second term in the right-hand side of (27) arises from the shapedependent interaction charge distribution inside the supercell with the neutralizing background. The parameter Q is the second radial moment of the defect charge density (28) Q = d3 rr2 [ρd (r) − ρb (r)] . Kantorovich [81] re-examined the method for arbitrary supercell shapes, and suggested a modiﬁed formula ignoring dipole–dipole interactions.

54

Risto M. Nieminen

There is obvious ambiguity in this correction scheme. First, the static dielectric constant is introduced as an external parameter and is not consistently deﬁned. Secondly, the correction scheme is derived assuming that the charge perturbation introduced by the defect is well localized within the supercell. This is strictly speaking not valid, as in classical theory the polarization and thus the aperiodic screening charge distribution extend over the whole macroscopic crystal. Thus, as described in detail by Lento et al. [82], Q depends on the size of the supercell and (27) does not lead to a well-deﬁned correction value. Nevertheless, (27), often known as the Makov–Payne formula, is popular in estimations of electrostatic corrections. Segev and Wei [83] showed that for charges with a Gaussian distribution with a certain width σ interacting with the background, the Madelung correction should vanish as σ becomes large. Moreover, situations may arise where local symmetry-breaking distortions in fact induce a net dipole in the supercell. Dipole contributions cannot be discarded in such a situation, as they do not cancel in the total-energy diﬀerences between perfect and defected supercells. Shim et al. [84] have systematically studied the behavior of the electrostatic correction for supercells of diﬀerent sizes for vacancy and interstitial defects in diamond. For negatively charged vacancies and positively charged interstitials, the formation energies show a clear dependence on the supercell size and are in qualitative agreement with the Makov–Payne trend. For positively charged vacancies and negatively charged interstitials, the electrostatic corrections are weak. An analysis of the spatial charge density distributions reveals that these large variations in electrostatic terms with defect type originate from diﬀerences in the screening of the defect-localized charge. A strongly localized charge is close to the point-ion model, whereas delocalized defect states spread out and result in weak Madelung corrections. To convince oneself of the proper elimination of the spurious electrostatic energy, one should, in the general case, carry out a proper scaling analysis of the L−1 behavior and extrapolate to the inﬁnite-L limit. Another approach is based on ﬁtting a multicenter Gaussian distribution to the defect charge density, and calculating and subtracting explicitly the electrostatic interactions between the Gaussian distributions and the background. This approach has so far only been used for charged molecules in vacuum [85], but it may be possible to generalize to defect supercells with aperiodic densities. A diﬀerent route to the electrostatic correction for charged defects was taken by Schultz [86], based again on the linearity of the Poisson equation but avoiding the neutralizing homogeneous background. An aperiodic defect charge distribution ρLM (r) is constructed so that it matches the electrostatic moments of the system up to a given order. When this charge density is separated from the supercell charge distribution, the remaining periodic distribution has zero net charge and is momentless. Thus, its electrostatic energy can be accurately calculated within the periodic boundary conditions. The

Supercell Methods for Defect Calculations

55

Coulomb energy of ρLM (r) is calculated using “cluster boundary conditions”, with the surrounding polarizable, defect-free crystal replaced by perfect, nonpolarizable bulk crystal. There is no analytical formula similar to (27) for this local-moment counter-charge (LMCC) method. Its main content is to use periodic boundary conditions to solve the Kohn–Sham equations but not for the Poisson equation. One can then calculate the electrostatic energy of a single defect-containing supercell surrounded by cells with the perfect crystal charge density. In order to correctly align the arbitrarily referenced potentials, Schultz [87] has suggested a method where a common reference potential can be calculated for all types of defects and also for the valence-band edge of the perfect crystal. The LMCC method should, in principle, lead to a rigorous 1/L convergence of the supercell energy, with a prefactor proportional to (1 − ε−1 )q 2 . This method does not need a compensating background, and there are no interactions between the defect charge and its periodic images. It also provides a way to deﬁne a reference energy independent of the defect charge state for aligning the band edges. The implementation of the LMCC method would thus seem very much worth the eﬀort for calculations of charged defects.

15 Energy-Level References and Valence-Band Alignment As is obvious from (13), another important parameter for supercell-based total-energy calculations is the position of the valence-band maximum (VBM), Ev , which is usually taken as the reference energy for the electron chemical potential. The position of the VBM of the defect-containing supercell is diﬀerent from that of the defect-free supercell, and this diﬀerence depends, in general, on the charge state of the defect. Consequently, a valence-band alignment (VBA) correction is usually applied by matching the two values. The magnitude of this correction is eﬀ eﬀ − Vdefect , (29) ∆EVBA = Vbulk where V eﬀ is the eﬀective Kohn–Sham potential and the brackets denote averaging over the bulk and defect supercells, respectively. Other potential-energy references are naturally possible. One possibility is to align an electronic core or semicore level energy (in all-electron calculations), or deﬁne all energies with respect to the so-called crystal zero, the potential energy at the surface of a neutral Wigner–Seitz cell. This choice is particularly simple and useful when using the atomic-sphere approximation (ASA), for example in the context of the linear-muﬃn-tin-orbital (LMTO) method.

56

Risto M. Nieminen

16 Examples: The Monovacancy and Substitutional Copper in Silicon The literature on supercell calculations of defects in semiconductors is vast and not even a partial review is attempted here. Instead, we discuss in more detail a recent systematic case study, where the practical implementations of two popular approaches were critically examined. The study involves the prototypical (but far from trivial) point defects in Si, the monovacancy VSi and substitutional copper CuSi . The fundamental nature of VSi means that it is a much-studied defect. It has four unpaired electrons, and in a simple LCAO picture they occupy four orbitals in the atoms surrounding the vacancy in the diamond structure [66]. These induce electronic states in the gap, which are modiﬁed by symmetrylowering structural distortions driven by the Jahn–Teller eﬀect. A comprehensive study of the convergence of the formation energy of the neutral silicon vacancy as a function of the supercell size has been given by Puska et al. [18] (see also [88]). The result is shown in Fig. 5. It turns out that very large supercells are necessary for proper convergence of the vacancy formation energy, and that the relaxation pattern around the vacancy undergoes a qualitative change (from outward to inward relaxation) as the supercell size grows. This is also shown by calculations for large ﬁnite clusters [19]. The total-energy hypersurface is ﬂat, especially for negatively charged defects, which makes the unambiguous determination of the point symmetry diﬃcult. This is also reﬂected in the diﬃculty of determining the ionization levels accurately. This will now be discussed for both VSi and CuSi . CuSi has a similar structure to VSi : the vacancy is perturbed by the Cu 3d states that lie in the valence band. The Jahn–Teller theorem predicts that CuSi should undergo a symmetry-lowering distortion with magnitude constrained by the presence of the metal atom. Spin-orbit coupling eﬀects may also reduce the amount of distortion by lifting the orbital degeneracy. 16.1 Experiments The greater structural freedom of VSi introduces another possible (and often encountered) complication. The total energy gained by pairing electrons in dangling bonds, associated with a structural distortion, can outweigh their mutual Coulomb repulsion. This is the famous “negative” eﬀective-U phenomenon, which leads to unexpected ordering of the ionization levels in the bandgap. In the case of VSi the pairing for the neutral defect is much stronger than for the singly positive +1 state, which shifts the ionization (donor) level Ed (0/ + 1) below that for the second donor Ed (+1/ + 2). Thus the singly positive silicon vacancy is a metastable state, a fact conﬁrmed with DLTS and EPR measurements by Watkins and Troxell [89]. The energy position measured in these experiments gives for the double donor level + the value Ed (+1/ + 2) ≈ Ev + 0.13 eV, while EPR studies show that VSi

Supercell Methods for Defect Calculations

57

Fig. 5. Formation energy of the neutral vacancy in Si. The supercell size (number of atoms) is given on the top of each panel, and the k-point set used for Brillouin-zone sampling is indicated as 1 = Γ , 2 = 23 , 3 = 33 , 4 = (1/4, 1/4, 1/4) and 5 = Γ + L. From [18]

ionized by photoexcitation decays to the neutral state from a donor level at Ed (0/ + 1) ≈ Ev + 0.05 eV. EPR studies together with stress-alignment experiments also demonstrate that the Jahn–Teller eﬀect causes structural distortions in accord with a straightforward one-electron model. This model predicts that the neutral and positively charged defects have D2d symmetry, while the negative charge states have C2v symmetry. The energies of the acceptor levels Ed (−1/0) and Ed (−2/ − 1) are experimentally unknown. For CuSi , there are accurate experimental values [90, 91] for its ionization levels and thus it provides a good testing ground for theory and computation, even if experimental structural information is lacking. The defect has a single donor level at Ed (0/ + 1) ≈ Ev + 0.207 eV, an acceptor level Ed (−1/0) at ≈ Ev + 0.478 eV ≈ Ec − 0.69 eV, and a double acceptor at Ed (−2/ − 1) at Ec − 0.167 eV. The Jahn–Teller distortions for VSi and CuSi (and more generally substitutional transition-metal impurities in Si) possess two components. The main one is tetragonal in character and gives the defects D2d symmetry. The direction of this distortion may occur in two senses, and this determines the relative energetic ordering of the resulting electronic states. The two senses correspond to two diﬀerent shapes for the bounding box with {100} faces that contains the four atoms surrounding the center: one is short and broad

58

Risto M. Nieminen

while the other is long and thin. They correspond to diﬀerent relative lengths for the six Si–Si distances between these four atoms. For the D2d point group, four of the distances belong to one equivalent set and two belong to the second equivalent set. One type of distortion (type A) has the pair longer than the four, and for the other (type B) it is the other way round. Type A splits the t2 state into a singlet a1 state above the doublet e state, while type B does the opposite. Transition-metal impurities relax in the A pattern, and monovacancies in Si relax in the opposite sense, B. When the system contains suﬃcient electrons to occupy the e state, a weaker trigonal distortion is expected. It lowers the symmetry to C2v . The equivalent pair of Si–Si lengths in the D2d case become unequal. This splits the e state into orbitals of b1 and b2 character. Spin-orbit coupling may also aﬀect the splitting of these states for transition-metal impurities [92]. 16.2 Calculations In a recent study, Latham et al. [93] carried out a systematic quantitative study of the electrical levels and associated structural relaxations of VSi and CuSi . To conduct the study, two diﬀerent computer programs, AIMPRO [94] and VASP [95, 96] were used. The former uses localized Gaussian orbitals as the basis set for the Kohn–Sham wavefunctions, while the charge density is expanded in plane waves. VASP uses plane waves throughout. In AIMPRO, the core electrons of atoms are represented by pseudopotentials constructed according to the Hartwigsen–Goedecker–H¨ utter (HGH) normconserving scheme [45]. The VASP package includes pseudopotentials based on the Vanderbilt ultrasoft [46] construction or, alternatively, the projectedaugmented-wave (PAW) method [48]. The Cu 3d electrons are included explicitly in the HGH and PAW schemes, while they are not in the Vanderbilt pseudopotential. In both methods, the exchange-correlation energy is evaluated using the LSDA formula described by Perdew and Wang [97]. Unit cells of 216 atoms are used in all cases, and the supercell band structure is sampled by using the Monkhorst–Pack scheme with 23 k points, folded according to the symmetry of the system and shifted to avoid the Γ point. This enables the total energy convergence of better than 10−4 eV per supercell, with the plane-wave kinetic energy cutoﬀs chosen to meet this requirement (in AIMPRO the Coulomb energy is evaluated also using the plane-wave expansion). The actual value of the cutoﬀ depends on the atoms present and the chosen pseudopotential. For charged defects, a compensating background charge is introduced as discussed in Sect. 13, and a ﬁnite-size scaling is performed. For bulk Si, both methods reproduce the lattice parameter a and the bulk modulus B0 well (see Table 1). The calculation of the bandgap Eg is a deﬁciency of LSDA-DFT formalism, as discussed above. The two methods give similar values, Eg (AIMPRO) = 0.71 while Eg (VASP) = 0.60 eV. The

Supercell Methods for Defect Calculations

59

VASP results do not depend on whether the core electrons are treated by the ultrasoft pseudopotential or PAW. Table 1. Calculated and measured values for the lattice parameter a and the bulk modulus B0 of Si Method

a (˚ A) B0 (GPa)

AIMPRO+HGH VASP+VUS VASP+PAW Experiment

5.395 5.390 5.403 5.431

97.0 87.7 72.8 97.9

All the defect electron levels considered here are suﬃciently deep so that the energies of donors can be given with respect to Ec and acceptors with respect to Ev . As reference (marker) energies Latham et al. choose addition/removal energies of ideal Si supercells with the same size (216 atoms) as used for the defect calculations. This means that the energy levels are referenced to the nearest ideal-crystal band edge (i.e., the marker method with respect to the two band edges). None of the studied defects are so shallow that their energy would be between the theoretical and true bandgap. If this were the case, it would be necessary to use the opposite ideal-crystal band edge as the reference potential. A summary of the calculated electrical levels, compared with experimental data, is presented in Table 2. Table 2. Calculated and measured electrical levels [93] for VSi and CuSi Transition AIMPRO VASP state VUS VSi VSi VSi VSi VSi VSi CuSi CuSi CuSi

0/+2 +1/+2 0/+1 −1/0 −2/−1 −2/0 0/+1 −1/0 −2/−1

Ev + 0.0 Ev + 0.05 Ev − 0.04 Ec − 0.31 Ec − 0.43 Ec − 0.37 Ev + 0.17 Ec − 0.50 Ec − 0.24

VASP PAW

Ev + 0.06 Ev + 0.11 Ev + 0.02 Ec − 0.34 Ec − 0.23 Ec − 0.29 Ev + 0.07 Ev + 0.17 Ec − 0.45 Ec − 0.34 Ec − 0.18 Ec − 0.26

[15]

Expt. [66, 90, 91]

Ev + 0.15 Ev + 0.19 Ev + 0.11 Ec − 0.57 Ec − 0.40 Ec − 0.49

Ev + 0.09 Ev + 0.13 Ev + 0.05 exists exists Ev + 0.21 Ec − 0.69 Ec − 0.17

When both program packages are set to use similar thresholds in terms of energies and forces to decide structural optimization, the outcome shows some diﬀerences. The AIMPRO package ﬁnds that the direction of the main tetragonal distortion (D2d symmetry) is in the expected direction, type B

60

Risto M. Nieminen

for VSi and type A for CuSi . The VASP package also ﬁnds type B D2d for neutral VSi . VASP yields type A D2d distortion for CuSi when the Vanderbilt pseudopotential is used, but no signiﬁcant deviation from the perfect Td symmetry when PAW is used. Both methods give equal energies for the (0/ + 1) level of CuSi . Regardless of constraint choice, no clear evidence is seen for the expected trigonal component of the distortion of CuSi . The situation is more complex for VSi . While the optimized structure in positive and neutral charge states has D2d symmetry as expected, the unconstrained lowest-energy structure is a D3d symmetry “split-vacancy” conﬁguration. The split-vacancy conﬁguration is one where a Si atom is located between two unoccupied lattice sites, and is 0.04 eV lower in energy than the ideal Td monovacancy. This result for negatively charged vacancies was also found by Puska et al. [18]. According to Latham et al., the energy diﬀerences between the C2v and C3v conﬁgurations of VSi in the q = −1 and q = −2 charge states are 0.02 eV and 0.20 eV, respectively. This means that VSi in the C3v symmetry is calculated to have a negative-U behavior also for the acceptor levels. Little is presently known from experiment about the negative charge states other than that they apparently exist. The calculated energy for the (−1/0) acceptor level of CuSi near midgap is somewhat deeper than the measured value, while the second acceptor is shallower. The Jahn–Teller eﬀect moves these levels apart, moving each by 0.1 eV. Thus, the calculations seem to slightly underestimate the magnitude of the Jahn–Teller eﬀect. It is reasonable to suppose that a similar pattern will be found for the acceptor states of VSi if they can be measured, and the expected C2v model without a negative-U eﬀect would prevail.

17 Summary and Conclusions Calculations based on the density-functional theory and the supercell method enable quantitative estimates for the formation energies, diﬀusion barriers, structural parameters and electrical levels of defects in semiconductors. Moreover, vibrational entropies and free energies can be estimated from the calculated force ﬁelds, which also enable ﬁrst-principles molecular dynamics simulations. It is also possible to feed the ﬁrst-principles results for migration and reaction barriers into kinetic Monte Carlo simulations based on master equations. This opens up the possibility for multiscale simulations of annealing kinetics and related phenomena. Quantitatively accurate total-energy calculations open the way to ﬁrst-principles thermodynamics and kinetics. However, reaching the desired quantitative accuracy in the total-energy calculations is not always straightforward, and requires careful consideration of several possible sources of error. In particular, the positioning of defectrelated electronic levels in the fundamental semiconducting gap can be quite problematic. The sources of errors may be divided into three main categories.

Supercell Methods for Defect Calculations

61

One is the underlying theory, especially the treatment of electronic exchange and correlation. Local and semilocal approximations do not properly describe the discontinuity of the corresponding density functional, which contributes to the underestimation of the fundamental gap. The second source of error are the ﬁnite-size eﬀects inherent in the supercell method, which need proper scaling analysis as a function of the cell size. These errors include the spurious defect–defect interaction, dispersion of defect-related electronic states, incomplete sampling of the reciprocal cell, and the constrained relaxation of atoms around the defect. The third source of errors are the approximations required to construct a speciﬁc implementation, including the pseudopotential generation, basis-set construction, and numerical accuracy of the algorithms. The power of the density-functional methods is considerable in revealing and rationalizing the systematic trends in electronic and structural properties of defects in semiconductors. These include the nature (acceptor or donor) of the deep levels, their spin structure, point symmetry, and energetics. They can also predict the localized vibrational modes associated with defects, and provide the starting point (for example, the ground-state electron density) for quantitative calculations of many experimentally observed characterizing signals (such as positron-annihilation parameters). Total-energy calculations also reveal the details of the potential-energy hypersurfaces for defects moving in the lattice, which makes it possible to study the long-time kinetics by using Monte Carlo techniques. Quantitatively accurate supercell calculations for defects in semiconductors are notoriously diﬃcult and demand considerable computational resources. While many confusing and seemingly contradictory results have been published in the scientiﬁc literature, the available computational methods have steadily matured. With the increase of computer power available for such calculations, it is now possible to perform well-benchmarked calculations with considerable predictive power. Acknowledgements I have beneﬁted from several useful discussions with Chris Latham and Maria Ganchenkova. This work has been supported by the Academy of Finland through the Center of Excellence Grant (2000–2005).

References [1] J. Bourgoin, M. Lannoo: Point Defects in Semiconductors II. Experimental Aspects, vol. 35, Springer Series in Solid State Sciences (Springer, Berlin, Heidelberg 1983) 29 [2] R. M. Nieminen: J. Phys.: Condens. Matter 14, 2859 (2002) 30 [3] W. Kohn, L. J. Sham: Phys. Rev. 136, B864 (1964) 30 [4] R. Martin: Electronic Structure: Basic Theory and Practical Methods (Cambridge University Press, Cambridge 2004) 30

62

Risto M. Nieminen

[5] A. E. Mattsson, P. A. Schultz, M. P. Desjarlais, T. R. Mattsson, K. Leung: Modelling Simul. Mater. Sci. Eng. 13, R1 (2005) 32 [6] M. J. Puska, R. M. Nieminen: Rev. Mod. Phys. 66, 841 (1994) 32 [7] C. G. van de Walle, P. E. Bl¨ ochl: Phys. Rev. B 47, 4244 (1993) 32 [8] C. J. Pickard, F. Mauri: Phys. Rev. B 63, 245101 (2001) 32 [9] C. J. Pickard, F. Mauri: Phys. Rev. Lett. 88, 086403 (2002) 32 [10] R. P. Messmer, G. D. Watkins: Phys. Rev. Lett. 25, 656 (1970) 33 ¨ [11] S. Ogut, H. Kim, J. R. Chelikowsky: Phys. Rev. B 56, R11353 (1997) 33 [12] G. Baraﬀ, M. Schl¨ uter: Phys. Rev. B 19, 4965 (1979) 33 [13] O. Gunnarsson, O. Jepsen, O. K. Andersen: Phys. Rev. 27, 7144 (1983) 33 [14] M. J. Puska, O. Jepsen, O. Gunnarsson, R. M. Nieminen: Phys. Rev. B 34, 2695 (1986) 33 [15] S. K. Estreicher, D. S. Marinyck: Phys. Rev. Lett. 56, 1511 (1986) 33, 59 [16] S. B. Zhang, J. E. Northrup: Phys. Rev. Lett. 67, 2339 (1991) 34, 49 [17] H. Dreyss´e (Ed.): Electronic Structure and Physical Properties of Solids. The Uses of the LMTO Method, Lecture Notes in Physics (Springer, Berlin, Heidelberg 2000) 35 [18] M. J. Puska, S. P¨ oykk¨ o, M. Pesola, R. M. Nieminen: Phys. Rev. B 58, 1318 (1998) 35, 36, 56, 57, 60 ¨ [19] S. Ogut, J. R. Chelikowsky: Phys. Rev. B 64, 245206 (2001) 35, 56 [20] K. Laaksonen, H. P. Komsa, E. Arola, T. T. Rantala, R. M. Nieminen: Phys. Rev. B in press 37 [21] M. St¨ adele, J. A. Majewski, P. Vogl, A. G¨ orling: Phys. Rev. Lett. 79, 2089 (1997) 37 orling: Phys. Rev. B [22] M. St¨ adele, M. Moukara, J. A. Majewski, P. Vogl, A. G¨ 59, 10031 (1999) 37 [23] R. J. Magyar, A. Flezsar, E. K. U. Gross: Phys. Rev. B 69, 045111 (2004) 37 [24] D. Vogel, P. Kr¨ uger, J. Pollmann: Phys. Rev. B 54, 5495 (1996) 37 [25] S. Sharma, J. K. Dewhurst, C. Ambrosch-Draxl: Phys. Rev. Lett. 95, 136402 (2005) 37 [26] A. Seidl, A. G¨ orling, P. Vogl, J. A. Majewski, M. Levy: Phys. Rev. B 53, 3764 (1996) 38 [27] J. Lento, R. M. Nieminen: J. Phys.: Condens. Matter 15, 4387 (2003) 38 [28] M. S. Hybertsen, S. G. Louie: Phys. Rev. B 34, 5390 (1986) 38 [29] S. Ismail-Beigi, S. G. Louie: Phys. Rev. Lett. 95, 156401 (2005) 38 [30] J. Laegsgaard, K. Stokbro: Phys. Rev. Lett. 86, 2834 (2001) 38 [31] M. d’Aveszac, M. Calandra, F. Mauri: Phys. Rev. B 71, 205210 (2005) 39 [32] J. Perdew, A. Zunger: Phys. Rev. B 23, 5048 (1981) 39 [33] A. Svane, O. Gunnarsson: Phys. Rev. B 37, 9919 (1988) 39 [34] L. Hedin: Phys. Rev. 139, A796 (1965) 39 [35] G. Onida, L. Reining, A. Rubio: Rev. Mod. Phys. 74, 601 (2002) 39 [36] M. Rohlﬁng, S. G. Louie: Phys. Rev. B 62, 4927 (2000) 39 [37] A. Janotti, C. G. van de Walle: Appl. Phys. Lett. 87, 122102 (2005) 40 [38] S. Lang, A. Zunger: Phys. Rev. B 72, 035215 (2005) 40 [39] V. I. Anisimov, F. Aryasetiawan, A. I. Liechtenstein: J. Phys.: Condens. Matter 9, 767 (1997) 40 [40] W. K. Leung, R. J. Needs, G. Rajagopal, S. Itoh, S. Ihara: Phys. Rev. Lett. 83, 2351 (1999) 40

Supercell Methods for Defect Calculations

63

[41] R. Q. Hood, P. R. C. Kent, R. J. Needs, P. R. Briddon: Phys. Rev. Lett. 91, 076403 (2003) 40 [42] C. G. Van de Walle, J. Neugebauer: J. Appl. Phys. 95, 3851 (2004) 40 [43] D. R. Hamann: Phys. Rev. B 40, 2980 (1989) 41 [44] N. Troullier, J. L. Martins: Phys. Rev. B 43, 1993 (1991) 41 [45] C. Hartwigsen, S. Goedecker, J. H¨ utter: Phys. Rev. B 58, 3641 (1998) 41, 58 [46] D. Vanderbilt: Phys. Rev. B 41, 7892 (1990) 41, 58 [47] L. Kleinman, D. M. Bylander: Phys. Rev. Lett. 48, 1425 (1982) 41 [48] P. E. Bl¨ ochl: Phys. Rev. B 50, 17953 (1994) 41, 58 [49] G. Kresse, D. Joubert: Phys. Rev. B 59, 1758 (1999) 41 [50] S. G. Louie, S. Froyen, M. L. Cohen: Phys. Rev. B 26, 1738 (1982) 41 [51] D. Porezag, M. R. Pederson, A. V. Liu: Phys. Rev. B 60, 14132 (1999) 41 [52] D. Vogel, P. Kr¨ uger, J. Pollmann: Phys. Rev. B 55, 12836 (1997) 41 [53] M. Fuchs, M. Bockstedte, E. Pehlke, M. Scheﬄer: Phys. Rev. B 57, 2134 (1998) 42 [54] P. Ordejon, E. Artacho, J. M. Soler: Phys. Rev. B 53, R10441 (1995) 42 [55] J. M. Soler, E. Artacho, J. D. Gale, A. Garcia, J. Junquera, P. Ordej´ on, D. Sanchez-Portal: J. Phys.: Condens. Matter 14, 2745 (2002) 42 [56] O. Treutler, R. Ahlrichs: J. Chem. Phys. 102, 346 (1995) 42 [57] T. L. Beck: Rev. Mod. Phys. 72, 1041 (2000) 43 [58] M. Heiskanen, T. Torsti, M. J. Puska, R. M. Nieminen: Phys. Rev. B 63, 245106 (2001) 43 [59] S. Nos´e: J. Chem. Phys. 81, 511 (1984) 43 [60] G. H. Hoover: Phys. Rev. A 31, 1695 (1985) 43 [61] M. Parrinello, A. Rahman: J. Appl. Phys. 52, 7182 (1980) 44 [62] E. Runge, E. K. U. Gross: Phys. Rev. Lett. 52, 997 (1984) 44 [63] M. Petersilka, U. J. Gossmann, E. K. U. Gross: Phys. Rev. Lett. 76, 1212 (1996) 44 [64] G. Vignale, W. Kohn: Phys. Rev. Lett. 77, 2037 (1996) 44 [65] H. A. Jahn, E. Teller: Proc. Roy. Soc. A 161, 220 (1937) 45 [66] G. D. Watkins: The Lattice Vacancy in Silicon (Gordon and Breach, Yverdon 1992) 45, 56, 59 [67] G. Baraﬀ, E. O. Kane, M. Schl¨ uter: Phys. Rev. Lett. 43, 956 (1979) 46 [68] G. D. Watkins: Physica B 117–118, 9 (1983) 46 [69] L. Torpo, R. M. Nieminen, S. P¨ oykk¨ o, K. Laasonen: Appl. Phys. Lett. 74, 221 (1999) 46 [70] S. Baroni, S. de Gironcoli, A. Dal Corso: Rev. Mod. Phys. 73, 515 (2001) 47 [71] J. M. Pruneda, S. K. Estreicher, J. Junquera, J. Ferrer, P. Ordejon: Phys. Rev. B 65, 075210 (2002) 47 [72] J. Coutinho, V. J. B. Torres, R. Jones, P. R. Briddon: Phys. Rev. B 67, 035205 (2003) 50 [73] D. J. Chadi, M. L. Cohen: Phys. Rev. B 8, 5747 (1973) 52 [74] H. J. Monkhorst, J. D. Pack: Phys. Rev. B 13, 5188 (1976) 52 [75] G. Makov, R. Shah, M. C. Payne: Phys. Rev. B 53, 15513 (1996) 52 [76] J. Shim, E.-K. Lee, Y. J. Lee, R. M. Nieminen: Phys. Rev. B 71, 035206 (2005) 52 [77] S. W. de Leeuw, J. W. Perram, E. R. Smith: Proc. Roy. Soc. London, Ser. A 373, 27 (1980) 53 [78] M. Leslie, M. J. Gillan: J. Phys. C 18, 973 (1985) 53

64

Risto M. Nieminen

[79] G. Makov, M. C. Payne: Phys. Rev. B 51, 4014 (1995) 53 [80] M. R. Jarvis, I. D. White, R. W. Godby, M. C. Payne: Phys. Rev. B 56, 14972 (1997) 53 [81] L. N. Kantorovich: Phys. Rev. B 60, 15476 (1999) 53 [82] J. Lento, J.-L. Mozos, R. M. Nieminen: J. Phys.: Condens. Matter 14, 2637 (2002) 54 [83] D. Segev, S. H. Wei: Phys. Rev. Lett. 91, 126406 (2003) 54 [84] J. Shim, E.-K. Lee, Y. J. Lee, R. M. Nieminen: Phys. Rev. B 71, 245204 (2005) 54 [85] P. Bl¨ ochl: J. Chem. Phys. 103, 7482 (1995) 54 [86] P. A. Schultz: Phys. Rev. B 60, 1551 (1999) 54 [87] P. A. Schultz: Phys. Rev. Lett. 84, 1942 (2000) 55 [88] D. A. Drabold, J. D. Dow, P. A. Fedders, A. E. Carlsson, O. F. Sankey: Phys. Rev. B 42, 5345 (1990) 56 [89] G. D. Watkins, J. R. Troxell: Phys. Rev. Lett. 44, 593 (1980) 56 [90] S. Knack, J. Weber, H. Lemke: Physica B 273–274, 387 (1999) 57, 59 [91] S. Knack, J. Weber, H. Lemke, H. Riemann: Phys. Rev. B 65, 165203 (2002) 57, 59 [92] G. D. Watkins, P. M. Williams: Phys. Rev. B 52, 16575 (1995) 58 [93] C. D. Latham, M. Ganchenkova, R. M. Nieminen, S. Nicolaysen, M. Alatalo, ¨ S. Oberg, P. R. Briddon: Phys. Scr. T126, 61 (2006) 58, 59 ¨ [94] J. Coutinho, R. Jones, P. R. Briddon, S. Oberg: Phys. Rev. B 62, 10824 (2000) 58 [95] G. Kresse, J. Furthm¨ uller: Comp. Mater. Sci. 6, 15 (1996) 58 [96] G. Kresse, J. Furthm¨ uller: Phys. Rev. B 54, 11169 (1996) 58 [97] J. P. Perdew, Y. Wang: Phys. Rev. B 46, 12947 (1992) 58

Index Γ point, 34, 52, 58 absorption, 44, 49 acceptor, 34, 40, 57, 59–61 AIMPRO, 58, 59 algorithm, 43, 44, 61 alignment, 35, 49, 50, 55, 57 all-electron, 41, 55 amorphous, 43 anharmonic, 48 annealing, 60 atomic-sphere approximation, 35, 55 autocorrelation function, 48 background charge, 35, 53, 58 band edge, 30, 35, 40, 49, 50, 55, 59 band structure, 38, 41, 58 bandwidth, 34

basis set, 32, 34, 39, 42, 43, 47, 58, 61 Bethe–Salpeter, 39 Born–Oppenheimer, 42, 43 Brillouin zone, 34, 35, 38, 51, 52 bulk, 36, 41, 47, 49, 50, 52, 55, 58 canonical, 43 charge delocalization, 39 charge state, 30, 34, 38, 46–50, 52, 55, 57, 60 charged defect, 35, 53–58 chemical potential, 36, 49–51, 55 classical, 53, 54 cluster, 32, 33, 35, 36, 55, 56 concentration, 36, 48 conduction band, 35, 38, 40, 50, 51 conductivity, 30, 49 core, 35, 37, 41, 55, 58, 59

Supercell Methods for Defect Calculations core radius, 41 core-valence, 37, 41 correlation, 31, 32, 37–40, 61 Coulomb, 35, 39, 40, 46, 53, 55, 56, 58 coupling, 46, 48, 56, 58 covalent, 35 cutoﬀ, 36, 42, 58 dangling bond, 56 decay, 57 deep level, 34, 61 deep-level transient spectroscopy, 29 defect band, 34, 35 degeneracy, 30, 44–46, 56 delocalization, 39 delocalized, 39, 52, 54 density of states, 37, 48 density-functional theory, 30, 31, 44, 60 DFT, 30–33, 36–38, 40, 42, 45, 47, 50, 58 diamond, 40, 46, 52, 54, 56 diﬀusion, 29, 60 dipole, 53, 54 dislocation, 33 disorder, 43 dispersion, 35, 38, 47, 61 distortion, 30, 45, 46, 54, 56–60 DLTS, 30, 49, 56 donor, 34, 40, 56, 57, 59, 61 doping, 30 double-zeta, 43 dynamical matrix, 48 DZP, 43 eigenvalues, 36, 39, 50 electrical level, 58–60 electron, 30, 31, 33, 36, 40, 41, 45–47, 56, 58, 59 electron aﬃnity, 36 electron states, 32, 38 electron-nuclear double resonance, 30 electrostatic energy, 54, 55 embedding, 32, 33 emission, 49 ENDOR, 30, 38 energetics, 29, 30, 32, 34, 61 energy cutoﬀ, 42, 58 energy level, 30, 34, 49, 59 entropy, 48

65

EPR, 30, 56, 57 equilibrium, 30, 43, 47–49 ergodic, 44 exact exchange, 37, 38 exchange, 31, 32, 37–40, 49, 61 exchange-correlation, 31, 32, 36, 39, 42, 44, 58 excitation, 32, 38, 39, 44, 49, 57 excited state, 34, 38 exciton, 38 fast Fourier transform, 41 Fermi level, 30, 36, 37, 45, 49 Fermi–Dirac, 51 ﬁnite diﬀerence, 43, 48 ﬁnite element, 43 ﬁrst principles, 32, 42, 43, 60 ﬂoating orbitals, 43 force, 32–34, 36, 40, 42, 43, 48, 59, 60 formation energy, 32, 40, 48, 49, 56 Fourier, 34, 48 free energy, 44, 60 frozen phonon, 48 fundamental gap, 34, 36, 45, 61 gap, 30, 31, 35–38 gap levels, 30 gap states, 30, 35, 45, 46, 50 Gaussian, 42, 54, 58 general gradient approximation, 32, 37 GGA, 32, 37–39, 42 ghost, 41 Green’s function, 33, 34, 36 ground state, 30, 32, 34, 36, 47–49, 51, 61 GW, 38, 39 Hall conductivity, 30 Hamiltonian, 44 Hartree, 31 Hartree–Fock, 32, 37–39 Hedin, 39 Hellmann–Feynman, 32, 36, 48 Helmholtz, 44 hole, 39 hybrid, 32, 37, 38 hyperﬁne, 32–34, 39 impurity, 30, 36, 45, 46, 48, 49 interstitial, 52, 54

66

Risto M. Nieminen

Jahn–Teller, 44–46, 56, 57, 60 jellium, 53

potential, 32, 34–37, 41, 42, 44, 45, 49–51, 55, 59, 61 projected augmented wave, 41, 58 pseudopotential, 40–42, 58, 60, 61

Kohn–Sham, 31, 32, 34–39, 42, 44, 50–52, 55, 58

quantum Monte Carlo, 40 quasiparticle, 38

LCAO, 56 LDA, 37–40, 42 LDA+U , 40 liquid, 43 localization, 30 LSDA, 32, 37, 58

real space, 42, 43 reciprocal space, 32, 34, 42 recombination, 34 relativistic, 32 relaxation, 33, 35, 36, 45, 58 repulsive, 45 resonance, 29, 38, 45

ionization, 34–36, 38, 41, 49, 50, 56, 57

Madelung, 53, 54 Makov–Payne, 54 marker, 50, 51, 59 microcanonical, 43 midgap, 60 migration, 29, 34, 42, 60 minimal basis, 35 molecular dynamics, 42–44, 60 multipole, 53 multiscale, 60 negative-U , 60 Newton, 43 nonlocal, 32, 37, 38 normal mode, 48 optical, 30, 34, 39, 40, 49 oxygen, 39, 40 pairing, 46, 56 Pauli, 32, 40 Perdew–Wang, 58 periodic, 33–36, 52–55 periodic boundary conditions, 33, 34, 43, 44, 54, 55 periodicity, 34 perturbation, 44, 54 phonon, 47, 48 photoluminescence, 30 PL, 30 plane wave, 34, 39, 41–43, 58 point defect, 30, 33, 35, 56 Poisson, 54, 55 polarization, 43, 54 positron annihilation, 29, 32, 34, 61

Schr¨ odinger, 31, 44 scissor, 39 screened exchange, 32, 38 screening, 38, 54 self-interaction, 31, 37, 39, 41 self-interstitial, 40 self-trapped, 38 semicore, 42, 55 shallow, 49, 59, 60 Si, 38–40, 45, 46, 56–60 silicon, 35, 36, 46, 52, 56 Slater, 40 special point, 52 spin, 29, 30, 32, 37, 39, 41, 46, 61 spin-orbit, 46, 56, 58 split-vacancy, 60 statistical, 43 stoichiometry, 34, 49 Stokes, 49 strain, 35, 43 stress, 35, 42, 57 substitutional, 38, 45, 46, 56, 57 supercell, 31–36, 38–40, 43–56, 58–61 surface, 33, 36, 42, 43, 55, 61 symmetry, 30, 35, 38, 44–46, 56, 57, 59, 60 symmetry breaking, 30, 54 Taylor, 47 temperature, 30, 42, 43, 49 tetrahedral, 35, 38, 45 thermal equilibrium, 48 thermodynamic integration, 44

Supercell Methods for Defect Calculations

67

thermodynamic ionization, 49 thermostat, 43 Thomas–Fermi, 38 time-dependent density-functional theory (TDDFT), 39, 44 time-dependent Schr¨ odinger equation (TDSE), 44 total energy, 30–32, 34, 43, 45, 47–53, 56, 58 trajectory, 44 transferability, 41 transition, 49 transition level, 30, 49, 51 transition metal, 57, 58 trigonal, 46, 58, 60

vacancy, 35, 38, 40, 45, 46, 52, 54, 56, 60 valence band, 35, 38, 40, 49–51, 55, 56 variational, 31, 43 VASP, 58–60 velocity autocorrelation, 48 vibrational dynamics, 30 vibrational entropy, 48, 60 vibrational free energy, 60 vibrational modes, 29, 33, 34, 47, 48, 61 vibrational spectroscopy, 29

ultrasoft pseudopotential, 41, 58, 59

ZnO, 40

Watkins, 45, 46, 56 wavelength, 52 Wigner–Seitz, 35, 55

Marker-Method Calculations for Electrical Levels Using Gaussian-Orbital Basis Sets J.P. Goss, M.J. Shaw, and P.R. Briddon School of Natural Science, University of Newcastle, Newcastle upon Tyne, NE1 7RU {J.P.Goss,M.J.Shaw,Patrick.Briddon}@newcastle.ac.uk Abstract. The introduction of defect-related states in the bandgap of semiconductors can be both advantageous and deleterious to conduction, and it is therefore of great importance to have quantitative computational methods for determining the location of electrical levels. In particular, where the defect levels are deep in the bandgap, the states involved are typically highly localized and the application of real-space, localized basis sets have clear advantages. In this chapter the use of such basis sets both for cluster and supercell geometries is discussed. Agreement with experiment is often hampered by problems such as the underestimate of bandgaps when using density-functional theory. We show that these can be somewhat mitigated by the use of “markers”, either experimental or theoretical, to largely eliminate such systematic errors.

1 Introduction It is well known that the electrical and optical properties of a crystalline material are inﬂuenced by impurities and other defects. In particular, conductivity at a given temperature is related to the free-carrier concentration, that in turn depends on the depth of the donor or acceptor level of the dominant dopant. Therefore one requires dopants with the smallest ionization energy, a value that is limited to the eﬀective-mass level of the host material [1]. Conversely, electron and hole traps deep in the bandgap are detrimental to the conductivity because they reduce the free-carrier concentration and the resultant charged defects are scattering centers that reduce carrier mobility. Deep levels are also nonradiative recombination centers aﬀecting optical properties. The importance of the electrical characteristics of defects has driven a huge eﬀort to develop reliable computational methods that can both explain experimental observations and predict new dopants with the desired properties. Currently, most calculations in this ﬁeld are performed using densityfunctional theory (DFT) [2, 3], chieﬂy simulating crystalline materials using periodic boundary conditions (PBCs), and plane wave (PW) basis sets1 to represent the wavefunctions of the electrons. 1

Plane waves represent functions in a Fourier-transformed phase space and are of the form exp(ik.r), where k is the wavevector that is related to an energy by E = 2 k2 /2m.

D. A. Drabold, S. K. Estreicher (Eds.): Theory of Defects in Semiconductors, Topics Appl. Physics 104, 69–94 (2007) © Springer-Verlag Berlin Heidelberg 2007

70

J.P. Goss et al.

With PBCs, a section of host material containing the dopant or defect is constructed and this “supercell” is repeated periodically throughout space. Such a construction represents a crystal of defects, and thus the use of PWs is a natural choice. If the defect and its periodic images are suﬃciently spatially separated they do not interact signiﬁcantly and the calculated properties represent those of isolated defects. This means that in order to obtain reliable data for defects (especially shallow dopants with large wavefunction extents) large supercells must be used. However, the computational cost increases rapidly with system size and in practice most of today’s calculations contain up to a few hundred atoms. The DFT-PBC approach has at least two major problems when calculating electrical properties. The ﬁrst is that within most commonly used localdensity (LDA) or generalized-gradient (GGA) approximations, the bandgap is underestimated, sometimes catastrophically. For example, crystalline Ge, in reality a semiconductor with a bandgap 0.74 eV [4], is found to be a semimetal [5]! Secondly, in order to obtain information about the capacity for defects to adopt diﬀerent charge states one needs to know the properties of charged systems. Strictly this is not possible with PBCs, but charged systems can be approximated by the use of a uniform background charge that exactly cancels the charge on the defect. Even then, this represents a space-ﬁlling array of charges that have an associated electrostatic energy that does not correspond to the properties of isolated defects. These problems are both mitigated by the use of atomic clusters. Here, defects are imbedded into large sections of the host material, but instead of repeating it periodically, the surface of the material is passivated (usually by hydrogen) eﬀectively forming a large molecule. The cluster geometry imposes an artiﬁcial conﬁning potential increasing the bandgap and localizing electronic states. However, although this eﬀect counteracts the inherent underestimate of the bandgap, the surface–defect interactions are of a similar nature to the defect–defect interactions in supercells. Although there are several sources of error in the calculations, many of them are somewhat systematic in nature, and hence relative locations of electrical levels may be more reliable than absolute values. This has led to the use of so-called marker methods [6–8], where one references the system of interest to one that is well understood: for example, the donor level of P in diamond is known, whereas those of As and Sb are not. Theory shows that they are shallower than phosphorus [9] and may therefore represent an improvement in the production of n-type diamond. (Of course, such calculations do not reﬂect on the relative solubilities of these dopants.) Finally, let us introduce the role of the basis functions used to describe the electrons in our problem. The use of PWs does not represent a fundamental problem, but in order to treat many systems of interest where the wavefunctions and charge density vary rapidly in space, the use of PWs often necessitates additional eﬀort (such as high-energy cutoﬀs) or the use of so-called ultrasoft pseudopotentials where one systematically removes the as-

Electrical Levels with Gaussian Bases

71

pects of the electrons that are diﬃcult to represent eﬃciently with PWs due to their localized nature. It is true that PWs may be viewed as a near-ideal basis set for eﬀective-mass-like shallow levels, since such donor and acceptor states are built out of the band-edge Bloch states. However, for deep levels the wavefunctions are often highly localized and can be characterized rather more simply by the use of molecular orbitals. The DFT package AIMPRO (Ab-Initio Modeling PROgram) uses a realspace basis made up from Gaussian functions [10, 11]. The real-space basis also allows the same electronic-structure methods to be applied to atomic clusters and molecules. In this Chapter, we ﬁrst present a detailed description of the basis sets used in our calculations. In Sect. 3 we describe the computational methods for calculating electrical levels, and in particular the marker method and present a review a range examples of its use in diﬀerent group-IV materials in Sect. 4.

2 Computational Method Our intention is to detail the calculation of electrical levels and not review the entire formalism used in the calculations. However, brieﬂy, AIMPRO is an electronic-structure program using LDA- and GGA-DFT. Atoms are treated using pseudopotentials [12] to remove the core electrons, and the distribution of the electrons solved self-consistently for a given set of atoms. AIMPRO can be used with a range of pseudopotential types, including the seminonlocal forms [13–15], and the dual-space separable pseudopotentials [16]. In addition to the eﬃciencies oﬀered by their separability, the latter pseudopotentials oﬀer extended norm conservation, accounting for a large number of occupied and unoccupied atomic levels. Currently, by default, AIMPRO uses the Perdew– Wang functional [17] for PBC calculations and a Pad´e approximation to this functional [18] for cluster calculations, although a number of alternative functionals are available. Historically, cluster calculations used an extremely fast parameterized analytic form for the exchange-correlation functional as described in detail previously [11]. GGA calculations are performed using a White–Bird [19] implementation of the GGA functional [20]. AIMPRO can be used both in periodic and cluster modes and the atomic structures optimized either using static minimization methods or molecular dynamics. From these calculations a range of observables can be derived, such as the electrical levels introduced above, vibrational-mode frequencies and symmetries, electronic-structures, hyperﬁne and zero-ﬁeld splitting tensors, electron energy loss spectra, migration barriers, and so on. However, in contrast to the majority of PBC calculations, AIMPRO represents the wavefunctions using a range of real-space, Gaussian-orbital functions.

72

J.P. Goss et al.

2.1 Gaussian Basis Set In order to construct and solve the Hamiltonian for our systems we expand our wavefunctions in terms of a basis set. Many diﬀerent basis types are used for ﬁrst-principles calculations, and each has associated advantages and disadvantages. There is no ﬁrm consensus on the optimum basis set to use, and since the choice of basis set plays a signiﬁcant role in determining the structure and nature of the calculations, the particular bases used and issues concerning them are worthy of some comment here. In the discussion that follows we shall consider only the arguments surrounding the selection of basis sets for pseudopotential calculations: clearly all-electron calculations, which must describe the rapid ﬂuctuations of the wavefunctions in the ionic core region place additional demands on the basis set. As alluded to above, of the many basis sets that are routinely used, perhaps the most signiﬁcant distinction lies between the expansion in terms of PWs, and the use of basis functions that are localized functions in real space. AIMPRO uses the latter type, speciﬁcally a set of Cartesian Gaussian orbitals (CGOs) centered on atoms and possibly other positions. These basis functions are products of a simple Gaussian and a polynomial in the position vector relative to the center of the Gaussian: φi,n1 n2 n3 (r) = xn1 y n2 z n3 e−αi r , 2

(1)

where αi reﬂects the spatial extent of the function; larger (smaller) values correspond to more localized (diﬀuse). The term xn1 y n2 z n3 deﬁnes the angular dependence, and relates to the spherical-harmonic associated with the angular-momentum and magnetic quantum numbers, l and m. For example, a px -orbital has n1 = 1, n2 = n3 = 0. These polynomial combinations enable the basis to describe atomic-like states of arbitrary angular momentum. The basis-set is deﬁned by the combination of Gaussian exponents and angular-momentum to which the combinations of polynomial functions extend. The advantages and disadvantages of PW and these real-space basis sets are already documented in the literature [11], however, it is useful to consider some of the key diﬀerences between them. A key advantage of CGOs is that they can be nonuniformly distributed in space, lending a more ﬂexible basis to regions that require it (for example in the region of a defect in a crystal). Such an approach cannot be taken with PW bases: the region with greatest complexity deﬁnes the density of PWs everywhere. For systems containing a small region in which the wavefunctions vary rapidly a high-energy cutoﬀ might be required, and this dense PW basis set must exist throughout the whole crystal. This leads to a very large Hamiltonian and slow calculation. A particular example of this problem is where surfaces are treated using a PBC via the inclusion of regions of vacuum. An advantage of a PW representation is that the basis functions are necessarily orthogonal. Consequently, the number of PWs can be increased without

Electrical Levels with Gaussian Bases

73

limit while retaining the stability of the calculation. CGOs are not orthogonal and the use of too large a basis set can result in numerical instability developing. The stability of the basis becomes a signiﬁcant issue when one attempts to address the question of how one should choose the basis for a particular problem. For a PW calculation it is possible to ensure that one has arrived at a converged result by systematically increasing the PW cutoﬀ. For a CGO basis set it is not possible to perform a systematic test to ensure that a convergent basis has been arrived at. Indeed, the choice of exponents for the functions in the basis set is a nontrivial one. We shall discuss the details of the basis set optimization procedure in more detail below. We now consider the CGOs in more detail. The task is to obtain a set of exponents for which the pseudowavefunctions are accurately described without rendering the calculations unstable. In order to achieve this, the variational principle is employed: when one compares any two basis sets, that which allows the wavefunctions to describe the true wavefunction most accurately results in the lowest total energy. The minimization of the total energy with respect to the exponents of the CGOs therefore results in the optimum basis set for a given number of functions. This process may then be repeated for diﬀerent numbers of functions to assess whether the basis is large enough. Again, the number of CGOs included cannot be increased without limit as the calculations become unstable. However, it is typically possible to obtain a convergent set of exponents prior to the onset of instability. Of course, an increased number of exponents increases the size of the Hamiltonian, and in turn the computational cost. Typically, the optimum number of basis functions is obtained by balancing the absolute quality of the basis and the associated accuracy of the results against the computational load. In addition to the number and value of the exponents, αi , the polynomial functions included with a given Gaussian (s, p, d, f and so on) must also be chosen. In general, a basis set contains a range of values of angular momentum and each CGO is treated independently. The angular momentum has a dramatic impact upon the number of functions in the basis set: for example, angular momentum up to s, p and d results in 1, 4 and 10 functions per exponent, respectively2 . As an example, four exponents per atom each of which include s and p, gives rise to 16 functions per atom. Increasing the basis to include d-functions increases the basis size to 40, and since diagonalization of the Hamiltonian scales as the cube of the basis size, the time to obtain a total energy would increase by more than an order of magnitude. 2

It should be noted that the linear combinations of six functions with n1 + n2 + n3 = 2 in (1) produce the ﬁve d-type functions (xy, xz, yz, 2z 2 − x2 − y 2 and x2 −y 2 ), and an s-type function (x2 +y 2 +z 2 ). Our standard practice in using the uncontracted basis sets discussed here is to include this additional s-type function, and hence the n1 = n2 = n3 = 0, n1 + n2 + n3 = 1 and n1 + n2 + n3 = 2 terms yield ten rather than nine functions.

74

J.P. Goss et al.

It is therefore paramount that basis functions of higher angular momentum are used selectively where the physical demands of the system merit them. Indeed, using a small number of high angular momentum functions is common practice in Hartree–Fock calculations where the basis sets are relatively small due to the extreme computational cost of this method, and are built up using the angular momentum of the atomic species with the addition of a single, higher angular momentum orbital as a polarization function. For most calculations all of the CGOs are centered on atoms, and move with the atoms during structural optimization. It is also possible to center basis functions at sites where there are no atoms. For example, historically, centering basis functions at appropriate positions on the bonds between adjacent atoms in the crystal was used to improve the description of the angular variations due to the formation of bonding orbitals. Locating basis functions at bond centers allows for polarization to be incorporated without increasing the maximum angular momentum, reducing the computational cost, but introducing a poorly deﬁned set of sites: during relaxation, structural changes may change the atoms between which bonding is present. However, increases in the speed of computational resources, together with improved algorithms has meant that bond-centered orbitals have largely been superseded by the use of basis sets containing higher angular momentum. The higher angular momentum components provide the necessary angular ﬂuctuations without the need for the additional complexity of bond-centered basis functions. Another situation in which localized basis functions may be centered away from atoms is the use of “ghost” atoms when treating surfaces. In this case, basis functions are placed in the vacuum region as though atoms were there (although of course, no atomic potential is included). This approach can provide additional basis functions to help describe the evanescent wavefunction variations close to the surface. For the majority of calculations the basis functions are atom-centered CGOs. A set of basis functions is therefore associated with each atom. The size of the basis set, and the particular exponents in it, will be optimized for each species of atom. Additionally, it is sometimes appropriate to treat diﬀerent atoms of the same species with diﬀerent basis sets within the same calculation (for example, surface atoms may require a larger basis than bulk atoms in a surface calculation). In the basis sets speciﬁed so far, all of the CGOs are independent basis functions, with coeﬃcients free to change during the calculation, and each contributes to the overall dimension of the Hamiltonian. It is possible, however, to exploit the physical properties of the system to take linear combinations CGOs to form more complex basis functions that provide a comparable accuracy but with a reduced number of independent parameters. These are referred to as contracted basis sets and are developed in the following way.

Electrical Levels with Gaussian Bases

75

A small reduction in the basis sets involving d-type (and higher angular momentum) functions can be obtained by taking linear combinations of the functions in (1). Formally, cnlm,n1 n2 n3 φi,n1 n2 n3 . (2) ψi,nlm = In the case containing up to quadratic prefactors there are ten functions φ, from which we may choose to produce a set of nine functions, ψ, which transform with angular momentum l = 0, 1, 2. A more radical approach to reduce the size of a basis set uses combinations of these ψi,nlm : Ψnlm = Cinl ψi,nlm , (3) where the number of functions of the form of Ψ is dramatically less than the related set of ψ. Particular examples of these contracted bases appear below in Sect. 2.3. 2.2 Choice of Exponents As mentioned above, the values of αi may be chosen by consideration of the total energy. Typically, this optimization process is performed for a prototypical example of the system to be studied. For example, in the case of studies of defects in silicon, the basis associated with the Si atoms is chosen to best represent a bulk Si cell. A problem of optimizing the values of the exponents is a multidimensional minimization problem, and may be tackled by one of the many standard minimization procedures available. AIMPRO allows for the optimization of the exponents by a downhill simplex or a conjugate gradient minimization of the total energy. Given that a typical element will require of the order of four diﬀerent exponents in its basis set, the free optimization of the exponents is a fourdimensional minimization problem. Calculations have shown that the fourdimensional energy surface generally is very ﬂat and undulating, resulting in many local minima, and causing diﬃculties in producing a unique choice of exponent. This is mitigated by the use of “even-tempered” basis sets in which the n exponents are constrained to be in a geometric series, and although it is generally true that an unrestricted basis set will lower the total energy, it is found that this is often not a signiﬁcant eﬀect. For contracted basis sets, as with the full Gaussian basis sets, ﬁxed parameters (in this case both coeﬃcients and exponents) may be obtained with reference to an appropriate prototypical system. Each combined contracted basis function adds just one to the dimension of the Hamiltonian, and yet contains variations over a number of diﬀerent length scales that reﬂect the properties of the physical system used in the ﬁtting procedure. Once the contraction coeﬃcients have been optimized, which is typically performed

76

J.P. Goss et al.

Fig. 1. Total energy of Si bulk unit cell during basis-exponent optimization. The energy is shown as a function of the number of simplex iterations

using a simplex optimization within AIMPRO, they remain ﬁxed during the subsequent self-consistent ﬁeld calculations. The optimization of the exponents is an important step prior to commencing a real calculation. Clearly, a poorly chosen basis may impact on the accuracy of the ﬁnal calculation, by aﬀecting the accuracy of the wavefunction description. However, as we shall demonstrate in the example below, the physical properties of the material (for example lattice constant and bulk modulus) are not sensitive to the ﬁne tuning of the basis. Only when the basis set has been carelessly chosen is there a signiﬁcant impact upon the physical properties. 2.3 Case Study: Bulk Silicon Let us consider the case of a range of basis sets for bulk silicon. Here, we shall consider the optimization of exponents in a four-exponent basis set, with angular momenta up to d on the ﬁrst and second exponent, and up to p on the third and fourth exponent (where the ﬁrst α is smallest). We refer to this as a ddpp basis. As an initial guess for the exponents we shall use the values {0.1, 0.3, 1.5, 4.0}. The range of these values results from a simple consideration of the length scales of the CGOs, the lowest exponent (longest-ranging Gaussian) allowing our basis to represent functions extending into the space between adjacent atoms, the highest exponent (shortest-range Gaussian) allowing us to describe the short-ranged variations of the valence pseudowavefunctions. (Note: the basis sets are described here for pseudopotential calculations – if all-electron calculations are to be performed, very much larger bases would be required, the highest exponents of which would be far greater than those needed for pseudopotentials.)

Electrical Levels with Gaussian Bases

77

We show in Fig. 1 the total energy as a function of the number of steps in a simplex optimization of this basis. Note how the reduction in energy is relatively steep in the early stages followed by a long tail, reﬂecting how a modest attempt to obtain exponents that reﬂect the properties of the system is suﬃcient to obtain a reasonably well-converged total energy. Several of the partially optimized bases were used to compute the lattice constant and bulk modulus of the Si by ﬁtting to the Birch–Murnaghan equation of state. These data are presented in Table 1. Table 1. Total energies (Hartrees) at energy minimum, lattice constants (au ) and bulk moduli (GPa ) for Si basis sets at various stages of optimization. For comparison, the experimental lattice constant and bulk modulus of silicon are 10.263 au and 97.9 GPa, respectively [21, 22] Iterations

Total energy

Lattice constant

Bulk modulus

1 4 6 15 24 30 100

−7.9234 −7.9250 −7.9269 −7.9271 −7.9276 −7.9280 −7.9280

10.24 10.23 10.21 10.21 10.21 10.21 10.20

91 91 94 95 93 94 96

Since the LDA is generally expected to obtain lattice constants to around 1 % accuracy, and bulk moduli to around 5 % to 10 % it can be seen from Table 1 that the variation in the structural parameters with basis is relatively small. In particular, the initial, somewhat arbitrary parameters yield reasonable results, and after only around ten iterations do the changes in lattice constant and bulk modulus become minimal on this scale. Table 2. Total energies (Hartrees) at energy minimum, lattice constants (au ) and bulk moduli (GPa ) for diﬀerent optimized Si basis sets Basis

No. functions per atom

Total energy

Lattice constant

Bulk modulus

dddd ddpp pdpp pppp

40 28 22 12

−7.9335 −7.9280 −7.9268 −7.8974

10.17 10.20 10.21 10.35

95 96 95 85

We must also consider the role of the angular momentum in the CGOs. The size of basis set increases with higher angular momentum, slowing the calculation but providing a more ﬂexible and accurate basis set. There is a

78

J.P. Goss et al.

compromise to make between accuracy and computational cost. Typically, for materials like diamond and silicon pdpp or ddpp bases are found to be suﬃcient. However, in calculations of defects it is often the case that heavier bases are used for the atoms at the defect itself, such as dddd. This exploits the localized nature of the CGOs, improving the accuracy of the basis in a particular region with little eﬀect on the overall accuracy or computational cost of the calculation. Table 2 details the eﬀect on the structural properties of silicon for various basis sets. The additional cost of the extra functions in the dddd basis is unnecessary since the results are eﬀectively the same as the computationally cheaper pdpp basis. However, the pppp basis set is seen to be too small and the omission of any higher angular momentum functions prevents a suﬃciently accurate description of the directional bonds found in covalent semiconductors. As with the plain CGO basis, a number of diﬀerent contracted basis sets can be deﬁned according to the number of diﬀerent combinations of the functions, and the angular momentum to which they extend. To label these contracted basis sets we draw on the conventional nomenclature of quantum chemistry, and specify, for example, a 4G basis to be one in which four CGOs (the “G”) of diﬀerent exponents are combined into ﬁxed functions. Separate combinations are formed for n and l representing the occupied atomic valence states of the element in question. For example, for the s and p orbitals in silicon this results in a total of four independent functions, one s- and three p-polynomial combinations. The same contraction coeﬃcients are used for diﬀerent components of a given function (for example px , py and pz ), although they are of course included as independent basis functions. This level of contraction is known as a minimal basis set as they cannot change shape during the calculation. To improve the ﬂexibility of the basis set, a second set of contracted coefﬁcients may be deﬁned resulting in an additional set of four basis functions (a total of eight basis functions, two s-types and 6 p-type). In our nomenclature this would be referred3 to as 44G. Such basis sets are greatly restricted due to the fact that the highest angular momentum that can be represented is limited to the angular momentum of the occupied atomic states. Although these can describe the isolated atom well, higher angular momentum components are needed to describe directional bonds. To account for these we may introduce additional “polarization” functions of higher angular momentum CGOs (for example d functions in silicon) with a single free exponent. The inclusion of polarization functions in a basis set is indicated by a ∗ in the notation, for example 44G∗ . The addition of the polarization functions increases the basis 3

This is similar to the “31” part of the quantum chemists standard 6-31G basis set. The only diﬀerence is that in our two contractions are combinations of all four underlying Gaussians; the 6-31G basis has 3 functions contracted together and one function left uncontracted, a more restrictive prescription.

Electrical Levels with Gaussian Bases

79

from 8 to 13 functions per atom, which remains considerably smaller than the ddpp plain Gaussian basis. We have extensively studied the eﬀect of reducing the degrees of freedom in our basis sets by moving to increasingly small contracted sets. In Table 3, the minimum total energy, lattice parameter and bulk modulus are presented for contracted basis sets, and compared with the uncontracted ddpp basis. Table 3. Total energies (Hartrees) at energy minimum, lattice constants (au ) and bulk moduli (GPa ) for contracted basis sets 44G∗ , 4G∗ , and 4G, as deﬁned in the text Basis No. functions per atom Total energy Lattice constant Bulk modulus ddpp 44G∗ 4G∗ 4G

28 13 9 4

−7.9280 −7.9269 −7.9226 −7.8854

10.20 10.19 10.21 10.39

96 97 103 91

A 44G∗ basis for materials such as Si and diamond is found to be as effective as a 28-function ddpp basis. In other words, the 44G∗ basis provides a convergent description of our wavefunctions for our typical host elements, at a much reduced cost in terms of the Hamiltonian. These contracted basis sets are therefore used in many of our calculations, giving an optimum performance with regard to computational cost. Cheaper bases still, such as the 4G basis are found to result in wider variations of lattice constant and bulk modulus, as well as giving poor electronic band structures, particularly in the conduction band. Although the 4G bases are not suitable for routine calculations, there are a number of potential applications for these basis sets. One possibility is that these extremely cheap bases (just four functions per atom in Si) could be used for bulk regions in very large unit cell calculations. Fuller bases could be used to describe the essential regions of the material (for example the defect region and adjacent atoms) with the 4G bases ﬁlling the remainder of the bulk-like unit cell. For such schemes to work it is necessary to match the optimum lattice constant of the two bases to avoid unphysical internal strain at the boundary between the two diﬀerent bases. Although we have implemented this approach and tested the idea with encouraging results, it has yet to be used in a real application.

80

J.P. Goss et al.

2.4 Charge-Density Expansions In AIMPRO the charge density, n(r), is also ﬁtted to a set of basis functions. With the PBC n(r) is expanded in PWs, so that the approximate charge density n ˜ (r) = n(G)eiG · r , (4) G

where all PWs with G2 /2 < Ecut-oﬀ are included, with the energy cutoﬀ chosen according to the atomic species present. The number of PWs is suﬃcient to make n ˜ a very accurate representation of the charge density n(r) given by the underlying Gaussian basis set. This does not incur signiﬁcant penalties in either speed or memory as the expansion is performed only for one function, n(r), rather than each occupied band as is the case in conventional fully PW basis set calculations. As a consequence, the energy cutoﬀ can be very large: typical values are 300 Ry and 80 Ry for carbon and silicon, respectively. In a cluster calculation, the charge density is expanded in uncontracted Gaussians (1) typically up to d-type functions. More details regarding the charge-density basis functions in cluster calculations can be found elsewhere [11].

3 Electrical Levels We now turn our attention to the calculation of electrical levels. Since the marker method, which forms the main part of this section, can be understood in terms of the more commonly used formation-energy method, we brieﬂy describe this and its associated problems. Before we do so, however, it is important to deﬁne what is meant by an electrical level. The electrical levels of a dopant (or any active defect) correspond to a thermodynamic property of the system, and relate to the chemical potential, µe of the electrons (sometimes erroneously referred to as a Fermi level, which is strictly only a zero-temperature quantity). Where µe lies below, say, the donor level of an impurity, energy is released by moving an electron from the defect to the electron reservoir at µe , and so this transfer of charge proceeds. Conversely, if µe is higher in the bandgap than the donor level of the defect it would cost energy to move the electron from the donor to the electron reservoir, and therefore it does not happen. It should therefore be noted that these levels relate to a change of charge state and cannot be obtained from the electronic-structure of any one of the charge states involved alone.

Electrical Levels with Gaussian Bases

81

3.1 Formation Energy The charge-state- (q) dependent, zero-temperature formation energy of a system of atoms and electrons (X) is usually written [23]: µi + q {Ev (X, q) + µe } + ξ(X, q) , (5) E f (X, q) = E t (X, q) − atoms

where E t is the total energy calculated for the system such as that obtained using AIMPRO, µi and µe are the atomic and electron chemical potentials, Ev (X, q) is the energy of the valence-band top and ξ(X, q) is a term that takes into account artifacts introduced by the computational framework. For PBCs ξ(X, q) reﬂects defect–defect interactions, whereas for clusters it relates to defect–surface interactions including quantum conﬁnement. Usually, the relevant E t (X, q) is that of the lowest-energy conﬁguration of X in charge state q, but not always, as noted below. For PBCs ξ may take the form of a power series in moments of the electron distribution, which can be viewed as terms arising from an array of monopoles, dipoles, quadrupoles and so on. The magnitudes of each term may be taken from a simple model, such as that of Makov and Payne [24] where only the terms in a Madelung energy and a quadrupole term are typically retained. The material is taken into account simply using the static dielectric constant, ε. Note, the Madelung term scales as q 2 and hence grows rapidly with q so that, for example, for a cubic supercell of diamond of side length 2a0 , the Madelung correction for q = ±3e is already of the order of the bandgap! This simple approach has received considerable criticism over recent years, so other, often computationally demanding, approaches have been adopted [25–28]. Notwithstanding the details of ξ(X, q), one can use E f (X, q) to estimate the electrical levels of X. The approach is to determine the thermodynamically most stable charge state for all relevant values of µe , and the critical values at which charge states change are the electrical levels. For example, the acceptor level is given by the value of µe that satisﬁes E f (X, 0) = E f (X, −1): µe = E t (X, −1) − E t (X, 0) + [ξ(X, −1) − ξ(X, 0)] − Ev (X, −1) , (6) as illustrated in Fig. 2. The diagram also illustrates the diﬃculties in interpreting levels that lie in the energy range between the theoretical and experimental bandgaps. Note, usually the electrical levels represent the transition between the lowest-energy structural conﬁgurations of each charge state, but not always. For example, there may be a considerable energy barrier between conformations of a set of atoms, so that the electrical levels relate to the change of charge state of a speciﬁc arrangement of atoms. An example of this is that of boron-vacancy complexes in silicon, where the equilibrium number of host sites between the impurity and the lattice vacancy is charge state

82

J.P. Goss et al.

Fig. 2. Illustration of the use of the formation energy to obtain an acceptor level for the system X in silicon. Above the acceptor level X − is thermodynamically more stable that X 0 , whereas below the reverse is true. The shaded area indicates the region between the theoretical and experimental bandgaps. The inclusion of ξ in the charged formation energy pushes the acceptor level above the theoretical value for Ec , but it remains deep in the experimental bandgap

dependent [29]. Such metastability must be taken into account when trying to assign calculated electrical transitions to those measured experimentally. This approach has perhaps three chief problems, the ﬁrst of which is the poorly deﬁned correction term, ξ which we have already touched upon. The second is that µe is deﬁned relative to the valence-band top in the defective system, which may be diﬃcult to establish with any precision. If one does not wish simply to use the approximation Ev (X, −1) = Ev (bulk, 0) then one might use corrections obtained either by examination of the lowest occupied Kohn–Sham level [30], or of the electrostatic potentials in bulk and defective systems [31] (see Sect. 3.2). The third, and often most critical problem that may aﬀect the location of electrical levels is the underestimate of the bandgap. For instance, the bandgap of hexagonal ZnO is around 3.4 eV [4], but simple application of the LDA- or GGA-DFT leads to bandgaps around 1 eV. Recently, hydrogen has been shown to be a shallow donor in this material [32, 33], but chargedependent formation energies yield donor levels around Ev + 2 eV [34, 35]. However, as previously suggested, for a given material it is often found that many of the problems introduce systematic errors. Therefore, one chooses alternative reference states that mitigate the charged systems, bandgap error and other interactions introduced by the geometry: this is the marker method.

Electrical Levels with Gaussian Bases

83

3.2 Calculation of Electrical Levels Using the Marker Method We may avoid the problems highlighted above by referencing, say, the acceptor level of one system to that of another. Equation (6) for two diﬀerent systems, X and Y , where the acceptor level µe (Y ) is known combine to yield the expression: µe (X) = µe (Y ) + E t (X, −1) − E t (Y, −1) − E t (X, 0) − E t (Y, 0) − [Ev (X, −1) − Ev (Y, −1)] + [{ξ(X, −1) − ξ(Y, −1)} − {ξ(X, 0) − ξ(Y, 0)}] .

(7)

If terms in ξ cancel and Ev (X, −1) = Ev (Y, −1) this simply reduces to: µe (X) = µe (Y ) + E t (X, −1) − E t (Y, −1) − E t (X, 0) − E t (Y, 0) . (8) This deﬁnes an unknown acceptor level, µe (X), with respect to the known marker at µe (Y ) with reference only to total energies. Note, (7) and (8) explicitly show that the calculations involve diﬀerences of energies between systems with the same charge. However, we have made at least two rather bold assumptions, and it is necessary to explore where and why they are likely to be valid. We ﬁrst examine the notion that Ev (X, q) = Ev (Y, q). Since one can add a constant potential to any system (i.e., the zero of the potential energy scale is often poorly deﬁned in PBC calculations), the valence-band states may be rigidly oﬀset from those of a defect-free system, and one can estimate the potential diﬀerence between X and Y by ﬁnding the average electrostatic potential in bulk-like regions of these systems [31]. For example, for substitutional impurities in a diamond-structure material, one might characterize the diﬀerence in the background potentials by ﬁnding the diﬀerence in the total electrostatic potentials at the T-interstitial sites far from the impurities. Alternatively, the potential diﬀerence between two systems can be estimated by the diﬀerence in the energies of the lowest occupied levels in X and Y [30] under the assumption that these characterize the average potentials in these systems. In our experience, such corrections may be up to a few tenths of an eV, but are usually small [31]. We now turn to the assumption that the ξ terms cancel. The suggested corrections for PBCs of Makov and Payne [24] assume an array of point charges, but it is clear from several studies that this approach tends to give a rather poor estimate. However, it is instructive to consider ξ(X, q) as arising from a series of multipole interactions. For chemically similar systems, the larger terms in the series would naturally be close in magnitude. Therefore, the best accuracy using the marker method is expected when comparing structurally and chemically similar systems. This remains true even when considering transitions between highly charged states, which is important because of the q 2 dependence of the simple Makov–Payne type of correction. However, there are two important areas where the marker method may be diﬃcult to apply. The ﬁrst is where the available markers are far in energy and

84

J.P. Goss et al.

chemical nature from that of the system of interest, such as using a shallow donor as a reference for a very deep donor. Under these circumstances there is unlikely to be very complete cancellation in the ξ, and hence the error bars in the calculation become more signiﬁcant. Furthermore, problems associated with the underestimate of the bandgap will also become more important. The second is that in some materials there may be no experimental data. For example, to our knowledge there are no unambiguous observations of double donors or acceptors in diamond. Where there are no appropriate markers, one might use a bulk system as the reference, Y , in (7) and (8). Such an approach was detailed for boron in silicon [7] and defects in diamond [8]. Here, the ﬁrst donor and acceptor levels of a bulk system are, by deﬁnition, Ev and Ec , respectively. However, one should exercise some caution in using a bulk system as a marker; deep levels and band edges are typically very diﬀerent in character. Furthermore, the levels of shallow defects are referenced to markers at the other extreme of the bandgap, making the underestimate of the bandgap a signiﬁcant factor. Finally, in the preceding discussion we have largely emphasized the use of the marker method for PBCs, but the principles are the same for cluster calculations. Indeed, the use of clusters for narrow-gap materials has two important advantages over the supercell approach. The ﬁrst is that the lack of periodicity means that there is no dispersion in the electronic-structure. Secondly, the conﬁnement of an atomic cluster tends to oppose the typical underestimation of the bandgap. For materials such as germanium for which the underestimation is acute, this is a very signiﬁcant, qualitative eﬀect, as reﬂected in the results presented below. In the ﬁnal section we review a number of examples of the application of the marker method using AIMPRO in both supercell and cluster modes.

4 Application to Defects in Group-IV Materials 4.1 Chalcogen–Hydrogen Donors in Silicon AIMPRO was recently used to analyze the properties of a range of chalcogens and their complexes with hydrogen in silicon. In this study [31] many of the issues raised above were explicitly examined, including the role of supercell size, Brillouin-zone sampling, basis and the average electrostatic potentials. One signiﬁcant factor in using chalcogens and their complexes with hydrogen in this study is that they have been characterized extensively by experiment, with spin densities, vibrational modes and for the substitutional chalcogens, electrical levels being available. It was therefore possible to show that the calculations were able to reproduce important aspects of the defects of interest other than the electrical characteristics, thereby validating the conclusions drawn. In particular, Mulliken bond-population analysis indicated that the donor wavefunctions were being faithfully reproduced in

Electrical Levels with Gaussian Bases

85

Fig. 3. Schematics of the partially passivated chalcogen–H complex in silicon. White and black circles represent host and impurity atoms, respectively, H being represented by the smaller black circle. Dashed lines indicated the cubic axes

these calculations, and that the characteristics were similar for the diﬀerent chalcogen species, indicating that the marker method should be appropriate. Additionally, for the chalcogens the defect-level dispersions are very similar suggesting that this eﬀect also would cancel out using an empirical marker. The chalcogens S, Se, and Te lie onsite, each having two donor levels, as listed in Table 4. The calculated donor levels listed were obtained using the formation energies with a Madelung correction and the marker method using bulk silicon and S as references. Table 4. Electrical levels relative to Ec ( eV ) of chalcogen and chalcogen–hydrogen complexes in silicon (see [31]). Experimental data from [36]

Defect

Experiment (0/+) (+/2+)

Formation energy (0/+) (+/2+)

Bulk marker (0/+) (+/2+)

Sulfur marker (0/+) (+/2+)

S Se Te S–H Se–H Te–H

0.29 0.29 0.20 – – –

0.78 0.79 0.75 0.41 0.37 0.27

0.42 0.40 0.27 0.13 0.10 0.00

0.29 0.28 0.25 0.01 −0.02 −0.12

0.59 0.54 0.36 – – –

1.25 1.23 1.22 1.78 1.77 1.77

0.48 0.45 0.28 1.18 1.18 1.18

0.59 0.55 0.38 1.28 1.28 1.28

The shallow nature predicted for the X–H complexes, the structure of which is shown schematically in Fig. 3, was viewed to be consistent with the fact that they had not been detected using deep-level transient spectroscopy [37, 38], but had been detected via their vibrational modes [39]. Three important conclusions can be drawn from this study. The ﬁrst is that the formation-energy approach yields qualitatively erroneous results: S, Se, and Te have no double-donor level in the bandgap, and the single-

86

J.P. Goss et al.

Fig. 4. Schematics of the VO center in Si and Ge. White and black circles represent host and oxygen atoms, respectively. The dark bond in (a) indicates the reconstruction present in the neutral charge state. (b) shows the unreconstructed center characteristic of the negative charge state

donor levels are far too deep. This can be traced to the underestimate in the bandgap and the nature of the correction terms, ξ. The second is that, although the single-donor levels are reasonably reproduced using the bulkmarker method, the second donor level is very poor, due to an underestimate of the correlation energy. Finally, the positive result is that, at least for classes of similar defects, the empirical marker method yields very good agreement with experiment. 4.2 VO Centers in Silicon and Germanium The properties of oxygen in silicon and germanium have been studied extensively as a consequence of the incorporation of O during growth and the properties that it lends to the materials. Of all the various roles and structures in which oxygen is involved, one of the most primitive is oxygen substituting for a host atom. Oxygen is a relatively small atom so that this center is generally referred to as a complex of (interstitial) oxygen with a lattice vacancy (VO), the structure of which is shown schematically in Fig. 4. VO centers in the neutral charge state can be understood as follows. The removal of a host atom creates four “dangling bonds”. Divalent oxygen passivates two of these and the remaining two dangling-bonds then combine together in a reconstruction, resulting in a defect that is fully chemically coordinated. However, these centers can trap additional electrons by breaking the relatively weak reconstruction, and the resultant dangling bonds lead to states in the bandgap. Experimentally, the VO center in silicon has an acceptor level at Ev + 1 eV [40]. However, the DFT calculations using supercells and formation energies have resulted in a rather poor agreement, predicting an acceptor level at Ev + 0.4 eV [41]. However, recalling that in these calculations the bandgap of bulk silicon is underestimated by more than 50 % of the experimental value, this donor level is approximately the correct depth below

Electrical Levels with Gaussian Bases

87

the theoretical Ec , which might be viewed as agreeing with experiment, and it is not clear how to interpret this calculation. The marker method using atomic clusters [6] where the bandgap underestimate is mitigated and using the acceptor level of interstitial carbon (Ec − 0.10 eV [42]) as a marker yielded an acceptor level for VO in silicon at Ec − 0.13 eV, in close agreement with the experimental level. Indeed, the small error is a testament to how robust the method is since, although they are close by in energy, the character of the acceptor wavefunctions for the VO and carbon interstitials are not closely related. The importance of the bandgap error is even greater when considering Ge. Recent calculations have also adopted the cluster conﬁguration of AIMPRO to analyze a range of defects in this material [43]. In particular, VO experimentally has acceptor and double-acceptor levels at Ev + 0.27 eV and Ev + 0.49 eV, respectively [44]. Using AIMPRO and atomic clusters that have approximately the experimental bandgap of 0.7 eV the two acceptor levels of VO have been calculated relative to the acceptor and double-acceptor levels of substitutional Zn at Ev + 40 m eV and Ev + 100 m eV, respectively [4]. The calculated second acceptor level is in excellent agreement with the experimental result, lying at Ev + 0.47 eV. However, the ﬁrst acceptor level calculated at around Ev + 0.42 eV is in less good agreement, but still within 0.2 eV. The reason for the larger deviation in the single-acceptor level is unclear, but even such an error bar is useful in the context of the more traditional supercell approaches that suggest this material has no bandgap at all. 4.3 Shallow and Deep Levels in Diamond In contrast to Si and Ge, diamond, with an indirect bandgap of around 5.5 eV [4], is a good example of an insulator, not obviously to be associated with the semiconductor industry. However, p- and n-type diamond can be produced via doping with boron and phosphorus, respectively, with heavily boron-doped materials becoming metallic and opaque. However, although phosphorus acts as a donor, the activation energy is very high at around 0.6 eV, so the room-temperature ionization fraction, and hence the number of free electrons, is rather small. This has led to an eﬀort to deduce which, if any, other system may result in a shallow donor level. As well as the electrical properties of diamond, the optical transparency, especially in the infrared, of the pure material has led to applications in high-speciﬁcation optics. However, as-grown diamond may contain deep-level defects that absorb and luminesce, and an understanding of these centers is also obviously of relevance. Regrettably, the number of deﬁnitively characterized donor and acceptor levels in diamond is relative small, and it is unsurprising that computational methods have been used in an attempt to assess both shallow and deep centers. We ﬁrst address examples of potential shallow donors. Since P is the

88

J.P. Goss et al.

Fig. 5. Location of donor levels in the bandgap relative to Ev for pnictogen donors in diamond. (a) and (b) shows values calculated using phosphorus and the bulk supercell being used as a marker, respectively. Empty and ﬁlled circles show 64 and 216 atom cells, respectively. The dashed and dotted lines show the experimental donor levels for P and N, and the shaded area shows the experimental conduction band

best-established shallow donor in diamond, it seems a good idea to establish if, as in silicon, the other pnictogens may have useful donor properties. Figure 5 plots the calculated donor levels using AIMPRO as described in [9]. Figure 5a shows the use of the experimental donor level [45] for P at Ec − 0.6 eV as a marker for supercells containing 64 or 216 atoms (cubes of side length 2a0 and 3a0 , respectively). The trends are the same for both curves and both supercells reproduce the experimental donor level of nitrogen. Figure 5b shows the same data, but referenced to bulk diamond. Now, the marker is the valence-band top, so it is far (around 5 eV!) from the anticipated location of the pnictogen donor levels. This exempliﬁes the need for appropriate markers for the method to have a quantitative role. However, irrespective of the marker, the important result in this application is that shallower donors of a simple nature, i.e., As and Sb, are expected to lead to improved n-type diamond. Recently, we also used supercell calculations to compare the use of the more traditional formation energy approach with the marker method for a range of centers, and in particular for those for which electrical levels are known experimentally [8]. Table 5 lists some of these results. The overall agreement between the marker method and experiment is conspicuously better than using the formation-energy approach, indicating that the marker method may usefully be applied to wide-gap materials for both deep and shallow electrical levels. For the small set of data presented in Table 5 one could adopt any acceptor and donor as an empirical marker and get very similar accuracy.

Electrical Levels with Gaussian Bases

89

Table 5. Electrical levels ( eV ) for various centers in diamond from experiment, compared to those calculated using the formation-energy method and the marker method using a bulk cell as a marker. For the formation-energy method, we quote the levels above Ev and below the theoretical and experimental locations of Ec (Ecth = Ev + 4.2 eV and Ecexpt = Ev + 5.5 eV). Asterisks indicate the markermethod results where the bandgap energy of 5.5 eV has been used to reference to the opposite band edge. Subscript s indicate substitutional impurities and v represents a lattice vacancy

Defect

Experiment

Formation energy Ev Ecth Ecexpt

Bulk marker Ev Ec

Ev + 0.37 [46] Ec − 2.49 [47, 48] Ec − 2.583 [49]

0.2 3.3 1.8

4.0 0.9 2.4

5.3 2.2 3.7

0.5* 3.0* 2.2*

5.0 2.5 3.3

Ec − 1.7 [50] Ec − 0.6 [45] Ec − 3.8 [51]

3.0 4.2 0.8

1.2 0.0 3.6

2.5 1.3 4.7

4.0 5.2 1.8

1.5* 0.3* 3.7*

Acceptors Bs Nis V–Ns Donors Ns Ps Ns –Ns

5 Summary The characterization of the electrical properties of defects and dopants using standard methodologies such as LDA- and GGA-DFT is a demanding problem. The most common approach of calculating charge-dependent formation energies has well-publicized frailties associated with periodic boundary conditions for charged systems, but these may be somewhat reduced by employing schemes where the electrical levels of two or more systems are compared. Additionally, when comparing total energies for chemically and structurally similar systems in the PBC approach, the dispersion of the defect levels in the ﬁrst Brillouin-zone and multipole interaction, which are present even for neutral systems, are likely to be comparable and cancel to a large degree. In addition, for electrical levels in narrow-gap materials, such as germanium, the use of carefully constructed atomic clusters also signiﬁcantly reduces the underestimation of bandgaps in these methods, allowing a fully quantitative analysis of the levels in these materials. We have also shown that the marker method is eﬀective in wide-gap materials where excellent agreement may be obtained over the full range of the bandgap, provided that one has a suitable marker available. Since the marker method is applicable when looking at similar systems, it may be of particular use when studying dilute alloys such as SiGe. Here, a known marker in silicon (for a Si-rich alloy) could be used to determine the eﬀect of having a nearby Ge atom, such as that of VO centers in such alloys [52].

90

J.P. Goss et al.

The use of bulk materials as markers is a qualiﬁed success in the sense that single donor and acceptor levels are in many cases in good agreement with experiment. However, multiple charges introduce larger errors and, for example with the chalcogen species in silicon, the second donor levels are in much less good agreement. We conclude that where experimental data allow, the most accurate quantitative method for predicting electrical levels in crystalline semiconductors and insulators is by comparison of a chemically and structurally similar defect for which the electrical levels are known. Other marker species, including the bulk supercells, are likely to introduce larger errors, but in our experience even then the results are rather favorable. Acknowledgements The authors would like to thank J. Coutinho, R. Jones and colleagues for useful discussions and access to data presented in this Chapter.

References [1] G. Burns: Solid State Physics, International ed. (Academic, Orlando, Florida 1985) 69 [2] P. Hohenberg, W. Kohn: Phys. Rev. 136, 864 (1964) 69 [3] W. Kohn, L. J. Sham: Phys. Rev. 140, A1133 (1965) 69 [4] S. M. Sze: Physics of Semiconductor Devices, 2nd ed. (Wiley-Interscience, New York 1981) 70, 82, 87 [5] G. E. Engel, W. E. Pickett: Phys. Rev. B 54, 8420 (1996) 70 ¨ [6] A. Resende, R. Jones, S. Oberg, P. R. Briddon: Phys. Rev. Lett. 82, 2111 (1999) 70, 87 [7] J.-W. Jeong, A. Oshiyama: Phys. Rev. B 64, 235204 (2001) 70, 84 [8] J. P. Goss, P. R. Briddon, S. J. Sque, R. Jones: Diamond Relat. Mater. 13, 684 (2004) 70, 84, 88 [9] S. J. Sque, R. Jones, J. P. Goss, P. R. Briddon: Phys. Rev. Lett. 92, 017402 (2004) 70, 88 [10] R. Jones, P. R. Briddon: Identiﬁcation of defects in semiconductors, in M. Stavola (Ed.): Semicond. Semimet., vol. 51A (Academic, Boston 1998) Chap. 6, p. 287 71 [11] P. R. Briddon, R. Jones: Phys. Stat. Sol. B 217, 131 (2000) 71, 72, 80 [12] W. E. Pickett: Comput. Phys. Rep. 9, 115 (1989) 71 [13] D. R. Hamann, M. Schl¨ uter, C. Chiang: Phys. Rev. Lett. 43, 1494 (1979) 71 [14] G. B. Bachelet, D. R. Hamann, M. Schl¨ uter: Phys. Rev. B 26, 4199 (1982) 71 [15] N. Troullier, J. L. Martins: Phys. Rev. B 43, 1993 (1991) 71 [16] C. Hartwigsen, S. Goedecker, J. Hutter: Phys. Rev. B 58, 3641 (1998) 71 [17] J. P. Perdew, Y. Wang: Phys. Rev. B 45, 13244 (1992) 71 [18] S. Goedecker, M. Teter, J. Hutter: Phys. Rev. B 54, 1703 (1996) 71 [19] J. A. White, D. M. Bird: Phys. Rev. B 50, R4954 (1994) 71 [20] J. P. Perdew, K. Burke, M. Ernzerhof: Phys. Rev. Lett. 77, 3865 (1996) 71

Electrical Levels with Gaussian Bases [21] [22] [23] [24] [25] [26] [27] [28] [29] [30] [31] [32]

[33]

[34] [35] [36] [37] [38] [39] [40] [41] [42] [43] [44] [45] [46] [47] [48] [49] [50]

91

E. R. Cohen, B. N. Taylor: J. Res. Nat. Bur. Standards 92, 85 (1987) 77 H. J. McSkimin, P. Andreatch, Jr.: J. Appl. Phys. 35, 2161 (1964) 77 S. B. Zhang, J. E. Northrup: Phys. Rev. Lett. 67, 2339 (1991) 81 G. Makov, M. C. Payne: Phys. Rev. B 51, 4014 (1995) 81, 83 H. Nozaki, S. Itoh: Phys. Rev. E 62, 1390 (2000) 81 U. Gerstmann, P. De´ ak, R. Rurali, B. Aradi, T. Frauenheim, H. Overhof: Physica B 340–342, 190 (2003) 81 C. W. M. Castleton, S. Mirbt: Phys. Rev. B 70, 195202 (2004) 81 J. Shim, E.-K. Lee, Y. J. Lee, R. M. Nieminen: Phys. Rev. B 71, 035206 (2005) 81 ¨ J. Adey, R. Jones, D. W. Palmer, P. R. Briddon, S. Oberg: Phys. Rev. B 71, 165211 (2005) 82 P. De´ ak, B. Aradi, A. Gali, U. Gerstmann: Phys. Stat. Sol. B 325, 139 (2003) 82, 83 J. Coutinho, V. J. B. Torres, R. Jones, P. R. Briddon: Phys. Rev. B 67, 035205 (2003) 82, 83, 84, 85 S. F. J. Cox, E. A. Davis, S. P. Cottrell, P. J. C. King, J. S. Lord, J. M. Gil, H. V. Alberto, R. C. Vil˜ ao, J. Piroto Duarte, N. Ayres de Campos, A. Weidinger, R. L. Lichti, S. J. C. Irvine: Phys. Rev. Lett. 86, 2601 (2001) 82 D. M. Hofmann, A. Hofstaetter, F. Leiter, H. Zhou, F. Henecker, B. K. Meyer, S. B. Orlinskii, J. Schmidt, P. G. Baranov: Phys. Rev. Lett. 88, 45504 (2002) 82 C. G. Van de Walle: Phys. Rev. Lett. 85, 1012 (2000) 82 M. G. Wardle, J. P. Goss, P. R. Briddon: Phys. Rev. B 71, 155205 (2005) 82 H. G. Grimmeiss, E. Janz´em: in S. T. Pantelides (Ed.): Deep Centers in Semiconductors, 2nd ed. (Gordon and Breach, Switzerland 1996) p. 97 85 G. Pensl, G. Roos, C. Holm, E. Sirtl, N. M. Johnson: Appl. Phys. Lett. 51, 451 (1987) 85 G. Roos, G. Pensl, N. M. Johnson, C. Holm: J. Appl. Phys. 67, 1897 (1990) 85 R. E. Peale, K. Muro, A. J. Sievers: Mater. Sci. Forum 65–66, 151 (1990) 85 G. D. Watkins, J. W. Corbett: Phys. Rev. 121, 1001 (1961) 86 M. Pesola, J. von Boehm, T. Mattila, R. M. Nieminen: Phys. Rev. B 60, 11449 (1999) 86 L. W. Song, G. D. Watkins: Phys. Rev. B 42, 5759 (1990) 87 ¨ R. Jones, A. Carvalho, J. Coutinho, V. J. B. Torres, S. Oberg, P. R. Briddon: Sol. St. Phenom. 108–109, 697 (2005) 87 V. P. Markevich, I. D. Hawkins, A. R. Peaker, V. V. Litvinov, L. I. Murin, L. Dobaczewski, J. L. Lindstr¨ om: Appl. Phys. Lett. 81, 1821 (2002) 87 E. Gheeraert, S. Koizumi, T. Teraji, H. Kanada, M. Nesl´ adek: Phys. Stat. Sol. A 174, 39 (1999) 88, 89 P. A. Crowther, P. J. Dean, W. F. Sherman: Phys. Rev. 154, 772 (1967) 89 D. M. Hofmann, M. Ludwig, P. Christmann, D. Volm, B. K. Meyer, L. Pereira, L. Santos, E. Pereira: Phys. Rev. B 50, 17618 (1994) 89 R. N. Pereira, W. Gehlhoﬀ, N. A. Sobolev, A. J. Neves, D. Bimberg: J. Phys. Condens. Matter 13, 8957 (2001) 89 J. W. Steeds, S. J. Charles, J. Davies, I. Griﬃn: Diamond Relat. Mater. 9, 397 (2000) 89 R. Farrer: Solid State Commun. 7, 685 (1969) 89

92

J.P. Goss et al.

[51] G. Davies: J. Phys. C 9, L537 (1976) 89 ¨ [52] V. P. Markevich, A. R. Peaker, J. Coutinho, R. Jones, V. J. B. Torres, S. Oberg, P. R. Briddon, L. I. Murin, L. Dobaczewski, N. V. Abrosimov: Phys. Rev. B 69, 125218 (2004) 89

Index acceptor, 69, 71, 81, 83, 84, 86–88, 90 AIMPRO, 71, 72, 75, 76, 80, 81, 84, 87, 88 algorithm, 74 all-electron, 72, 76 background charge, 70 band edge, 84 band structure, 79 basis set, 69, 71–80 Bloch, 71 bond-centered, 74 boron, 81, 84, 87 Brillouin zone, 84, 89 bulk, 74, 76, 79, 84, 86, 90 bulk modulus, 76, 77, 79 carbon, 80, 87 chalcogen, 84, 85, 90 charge state, 70, 80, 81, 86 chemical potential, 80 cluster, 70, 71, 80, 81, 84, 87, 89 complex, 81, 84–86 concentration, 69 conduction band, 79 conductivity, 69 conformation, 81 conjugate gradient, 75 core, 71, 72 correlation, 86 covalent, 78 deep level, 69, 71, 84, 87 density-functional theory, 69 DFT, 69–71, 82, 86, 89 diamond, 70, 78, 79, 81, 83, 84, 87, 88 dipole, 81 dispersion, 84, 85, 89 DLTS, 85 donor, 69–71, 80, 82, 84–88, 90

dopant, 69, 70, 80, 89 doping, 87 electrical level, 71, 80, 81, 88–90 electron, 69–71, 80, 81, 86, 87 electrostatic energy, 70 empirical, 85, 86, 88 energy barrier, 81 equilibrium, 81 exchange-correlation, 71 ﬁrst principles, 72 ﬂuctuation, 72, 74 formation energy, 80, 81, 88 Fourier, 69 gap, 81, 82, 89 Gaussian, 71–73, 75, 76, 79, 80 Ge, 70, 87, 89 general gradient approximation, 70 germanium, 84, 86, 89 GGA, 70, 71, 82, 89 ghost, 74 Hamiltonian, 72–75, 79 Hartree–Fock, 74 hole, 69 hydrogen, 70, 82, 84 hyperﬁne, 71 impurity, 80 interstitial, 87 ionization, 69, 87 Kohn–Sham, 82 LDA, 71, 77, 82, 89 Madelung, 81, 85 magnetic, 72 Makov–Payne, 83

Electrical Levels with Gaussian Bases marker, 71, 80, 82–90 metastablity, 82 migration, 71 mobility, 69 molecular dynamics, 71 Mulliken, 84 multipole, 83, 89 narrow-gap, 84, 89 optical, 69, 87 oxygen, 86 Perdew–Wang, 71 periodic, 70, 71 periodic boundary conditions, 69, 89 periodicity, 84 phosphorus, 70, 87 plane wave, 69–73, 80 pnictogen, 88 polarization, 74, 78 population, 84 potential, 70, 74, 79–84, 87 pseudopotential, 71, 72, 76

real space, 71, 72 recombination, 69 scattering, 69 shallow, 70, 71, 82, 84, 85, 87, 88 Si, 75, 77, 79, 87 SiGe, 89 silicon, 75, 76, 78, 80, 81, 84–90 spherical harmonics, 72 spin, 84 strain, 79 substitutional, 83, 84, 87 supercell, 70, 81, 84, 86–88, 90 surface, 70, 72, 74, 75, 81 temperature, 69, 80, 81, 87 total energy, 73, 75, 79 transition, 81–83 ultrasoft pseudopotential, 70

quadrupole, 81

vacancy, 81, 86 valence band, 81–83, 88 variational, 73 vibrational modes, 71, 84, 85

radiative, 69

ZnO, 82

93

Dynamical Matrices and Free Energies Stefan K. Estreicher and Mahdi Sanati Physics Department, Texas Tech University, Lubbock, TX 79409-1051 [email protected]

Abstract. The calculation of the entire dynamical matrix of a periodic supercell (containing a defect or not) provides several most useful pieces of information. At ﬁrst, the eigenvalues of this matrix are all the normal mode frequencies of the cell, including the local, pseudolocal, and resonant modes associated with the defect under study. The eigenvalues can also be used to construct phonon densities of state which in turn allow the calculation of (Helmholtz) free energies, vibrational entropies, and speciﬁc heats. The eigenvectors of the dynamical matrix can be used to prepare a system in thermal equilibriumat a desired temperature. This allows constant-temperature MD simulations to be peformed without thermalization or thermostat. Applications to the calculation of vibrational lifetimes and decay channels are discussed. Finally, the vibrational, rotational, and charge-carrier contributions to the free energy are described. Conﬁgurational entropies are calculated in realistic systems.

1 Introduction Vibrational spectroscopy provides essential experimental data about defects in semiconductors, not only because of the microscopic nature of the information it provides but also because many of the quantities measured can be calculated from ﬁrst principles. Fourier transform infrared absorption (FTIR) and Raman spectroscopies often produce sharp lines associated with local vibrational modes (LVMs) of impurities lighter than the hosts atoms. These lines are often above the highest normal mode of the crystal, the Γ phonon but, when the phonon density of states has a gap (as in the case of GaN [1]), they can be between the acoustic and optic modes as well. Isotope substitutions provide element identiﬁcation as well as information about how many atoms of a given species are part of the defect. Uniaxial stress experiments give the symmetry of the defect through the splitting of the IR or Raman lines. Annealing studies provide various activation energies. Examples of such studies and a discussion of the techniques are found in [2]. By themselves, the measured LVMs, isotope shifts, symmetry, and activation energies are often insuﬃcient to identify a unique structure for the defect. However, they are precious to theorists who use ﬁrst-principles techniques to calculate the structures (symmetry), LVMs and their isotope shifts, binding, migration and/or reorientation energies, and thus prove or disprove D. A. Drabold, S. K. Estreicher (Eds.): Theory of Defects in Semiconductors, Topics Appl. Physics 104, 95–114 (2007) © Springer-Verlag Berlin Heidelberg 2007

96

Stefan K. Estreicher and Mahdi Sanati

the assignment of an IR or Raman spectrum to a speciﬁc defect. The interplay between vibrational spectroscopy and ﬁrst-principles theory has led to the unambiguous identiﬁcation of many defects and has provided realistic tests of the accuracy of theory. For many years, the calculation of defect-related vibrational modes has been limited to those LVMs that are IR or Raman active. The stretch mode of a Si–H bond, in a Si vacancy for example, can be predicted quite accurately by calculating the total energy of a supercell containing this defect in its equilibrium conﬁguration as well as for several (at least 2) positions of H along the Si–H bond. The 1-dimensional potential along this axis is ﬁtted to a polynomial and the frequency and zero-point energy of this mode are calculated. The same can also be done for wag modes. There are many examples of such calculations [3–5]. This method works well, but a lot of additional and very useful information can be obtained when the entire dynamical matrix of the supercell is calculated. For a system of N atoms and therefore 3N normal modes, the dimension of this matrix is 3N × 3N and its calculation is computationally expensive. The eigenvalues of the dynamical matrix are all the normal mode frequencies of the supercell: acoustic and optic phonons as well as defectrelated modes. These can be LVMs, located above the Γ phonon, resonant and/or pseudolocal vibrational modes (pLVMs). Resonant modes occur when the strain (associated with a defect) stretches or compresses host–atom bonds, resulting in new vibrational frequencies near the Γ phonon. pLVMs are localized impurity-related modes buried in the phonon continuum. Such modes are sometimes visible experimentally as phonon sidebands in photoluminescence (PL) spectra [6, 7]. Two copper-related centers in Si have recently been theoretically identiﬁed [8,9] thanks to such pLVMs. Further, the knowledge of all the normal mode frequencies allows the construction of phonon densities of state, which are needed to calculate (Helmholtz) free energies. The eigenvectors of the dynamical matrix make it possible to ﬁnd (and identify the symmetry of) all the localized modes associated with any atom or group of atoms in the supercell. The eigenvectors can also be used to prepare the supercell in thermal equilibrium and any temperature, thus allowing constant-temperature molecular dynamics (MD) simulations to be performed without the need for thermalization or even a thermostat. This in turn makes it possible to calculate vibrational lifetimes and decay channels of speciﬁc modes as a function of temperature. For all these reasons, the calculation of dynamical matrices is well worth its cost. Our results are obtained from self-consistent, ﬁrst-principles theory based on local density-functional theory in 64-host-atom periodic supercells. The calculations are performed with the SIESTA code [10, 11]. The exchangecorrelation potential is that of Ceperley–Alder [12] as parameterized by Perdew and Zunger [13]. Norm-conserving pseudopotentials in the Kleinman– Bylander form [14] are used to remove the core regions from the calculations. The basis sets for the valence states are linear combinations of numerical

Dynamical Matrices and Free Energies

97

atomic orbitals of the Sankey type [15–17], generalized to be arbitrarily complete with the inclusion of multiple-zeta orbitals and polarization states [10]. We use double-zeta (two sets of s and p orbitals) for ﬁrst- and second-row atoms (H through Ne) and add a set of polarization functions (e.g., one set of d orbitals) for third-row atoms and below. The charge density is projected on a real-space grid with an equivalent cutoﬀ of 150 Ry to calculate the exchange-correlation and Hartree potentials. A 2 × 2 × 2 Monkhorst–Pack k-point sampling [18] is used to optimize the structures. An overview of dynamical matrices is given in Sect. 2. Examples of LVMs and pLVMs are given in Sect. 3. The calculation of vibrational lifetimes is given in Sect. 4. Vibrational free energies and speciﬁc heats are discussed in Sect. 5, and the properties of defects at ﬁnite temperatures in Sect. 6.

2 Dynamical Matrices The calculation of dynamical matrices is a well-known topic discussed in many textbooks, such as [19]. Further, the calculation of the force-constant matrix F is implemented in many (if not all) software packages that have MD capabilities. The brief summary below is therefore only necessary in order to deﬁne the notation to be used in this Chapter and make a few comments. We consider a solid represented by periodic supercells of N atoms of mass mα (with α = 1, 2, . . . , N ). The nuclei oscillate around their equilibrium positions. The dynamical matrix is related to the force-constant matrix by Fαβ,ij Dαβ,ij = √ , mα mβ

(1)

where i, j = x, y, z are Cartesian indices. The calculation of Fαβ,ij is computationally intensive for the type of systems required in the study of defects in semiconductors. Today’s typical supercells contain of the order of 100 atoms, and there is little doubt that several hundred (or even thousand) atoms will become the norm in the near future. Once F is known, changing the masses of selected atoms (that is, playing with isotopes) is trivial. Techniques to calculate F are well known, ranging from the direct “frozen phonon” approach implemented in many MD software packages to MD-based methods based on correlation functions [20, 21], or linear-response theory [22–25]. Note that dynamical matrices can also be computed using order-N methods [26]. The eigenvalues of the dynamical matrix are the normal mode frequencies of the system ωs , and the corresponding eigenvectors esα,i are orthonormal: α,i

esα,i esα,i = δss

and

s

esα,i esβj = δαβ δij .

(2)

98

Stefan K. Estreicher and Mahdi Sanati

In the harmonic approximation, the normal-mode coordinates qs are √ qs (t) = As cos(ωs t + ϕs ) = mα uα,i esα,i ,

(3)

α,i

where the amplitudes As are temperature dependent and the uα,i are Cartesian displacements of the nucleus α away from equilibrium. This relationship can be used to prepare a system in equilibrium at a temperature T , then perform MD runs at constant temperature without the need for thermalization or even a thermostat [27]. Indeed, the unknown amplitudes of the normal modes can be obtained by requiring that the kinetic energy of each mode is, on the average, kB T /2, that is 1 ∂q 2 s

2

∂t

=

1 2 2 2 ωs As

sin2 (ωs t + ϕs ) = 14 ωs2 A2s = 12 kB T .

(4)

√ Thus, the average amplitude of the normal mode s is As = 2kB T /ωs . Note that assigning the amplitudes As = As to each mode s implies that the total energy of each mode is exactly kB T . It is better to pick a random distribution Es 1 −E/kB T e dE (5) ζs = k BT 0 with 0 < ζs < 1. This leads to As = −2kB T ln(1 − ζs )/ωs . Thus, in the harmonic approximation, the Cartesian coordinates and corresponding velocities needed to prepare the system in equilibrium at the temperature T are 2kB T 1 uαi = − ln(1 − ζs ) cos(ωs t + ϕs )esαi , (6) mα s ω s and ∂uαi =− ∂t

2kB T − ln(1 − ζs ) sin(ωs t + ϕs )esαi . mα s

(7)

The initial phases 0 ≤ ϕs < 2π are random, as each mode has a random amount of kinetic and potential energy at the time t = 0. A similar transformation has been used by Gavartin and Stoneham [28] to calculate the energy dissipation in quantum dots. However, we discuss it here in the context of establishing initial conditions with the appropriate random distribution of energies and phases. This is used in Sect. 4 to calculate vibrational lifetimes and decay channels from ﬁrst principles.

Dynamical Matrices and Free Energies

99

Fig. 1. LVMs pLVMs associated with H+ bc in the Si64 supercell. The plots and 2 s 2 |e | , where α is H (left), or its two Si nearest neighbors (right) of d (α) = α,i i show the vibrational modes localized on the impurity and its two Si neighbors. The vertical dashed lines show the calculated Γ phonon

3 Local and Pseudolocal Modes The simplest and most immediate consequence of the knowledge of the dynamical matrix is the identiﬁcation of all the localized modes of a defect, and their symmetry. Indeed, a plot of i |esα,i |2 vs. s (that is, vs. the normal mode frequencies ω) for a speciﬁc atom α (or set of atoms) provides quantitative information about the localization of the modes associated with the given atom(s). For example, Fig. 1 shows the localized modes associated with bond-centered (bc) hydrogen in crystalline Si (H+ bc ): the asymmetric stretch (IR active) of H is a LVM at 2004 cm−1 (observed [29] at 1998 cm−1), the two degenerate wag modes (not observed) are pLVMs, far below the Γ phonon, at 264 cm−1 , and the symmetric stretch is a pLVM at 452 cm−1 (also not observed). The latter does not involve any H motion at all, but shows up when i |esα,i |2 includes the two Si nearest neighbors to H. Figure 2 shows the eigenvectors of the dynamical matrix in one of the two degenerate wag modes at 264 cm−1 . The H displacement in this mode accounts for about 70 % the displacements of all the atoms in the cell. Note that the eigenvectors only give the relative amplitudes of the atomic displacements. Their absolute values depend on the temperature, and are exaggerated in the ﬁgure. Thus, plotting i |esα,i |2 quantiﬁes the localization of all the local modes associated with an atom or group of atoms. The corresponding eigenvectors allow the identiﬁcation of the symmetry of the mode, which is needed to establish whether a mode is IR active or not, and whether it can produce phonon sidebands in PL spectra or not [6]. This is precisely how two lowfrequency copper-related defects have recently been identiﬁed [8, 9]. A very

100

Stefan K. Estreicher and Mahdi Sanati

Fig. 2. Eigenvectors of the dynamical matrix in one of the 264 cm−1 wag modes of H+ bc . The H atom is the small black ball, the gray balls are all Si. The size of the arrows is exaggerated to make the smaller oscillation amplitude more visible. The arrows only show the relative amplitudes of the motion of the atoms in this mode

useful software package1 readily reads dynamical matrices and graphically displays the eigenvectors for any chosen normal mode.

4 Vibrational Lifetimes and Decay Channels The vibrational lifetimes of the LVMs of light impurities in Si have recently been measured by transient bleaching spectroscopy [30, 31]. Surprisingly, the lifetimes of nearly identical H-related LVMs diﬀer by some two orders of magnitude. For example, at low temperatures, the measured lifetimes of the 2072 cm−1 mode of the divacancy–dihydrogen complex (VH · HV), the −1 1998 cm−1 mode of H+ mode of the H∗2 pair [31] are bc [30], and the 2062 cm 295 ps, 8 ps, and 4 ps, respectively. Since the decay of all these modes must involve at least four phonons (six phonon processes are proposed [29, 31]), it is not clear why the lifetimes of LVMs with almost identical frequencies vary by two orders of magnitude or why any of them would be short-lived at all. 1

For information about the Molekel visualization package, see www.cscs.ch/ molekel/.

Dynamical Matrices and Free Energies

101

The calculations of vibrational lifetimes begin with the dynamical matrices of the supercells containing the defects. The eigenvectors of this matrix determine the equilibrium background temperature of the cell at the time t = 0, as discussed in Sect. 2. This is used to prepare the cell in equilibrium at the same sample temperatures as in the experimental work. The initial excitation of the LVM of interest is assigned to be its zero-point energy plus one phonon, that is 3ω/2 (kinetic energy at t = 0). This mimics the laser excitation of the speciﬁc LVM. Then, constant-temperature (classical) MD simulations are performed, with a time step of 0.3 fs in the case of H. Since ab initio MD simulations are limited to real times of a few times 10 ps, it is critical to be able to begin the MD runs at a relatively elevated background temperature, because the measured lifetimes are much shorter at higher temperatures. The calculations are then repeated at lower temperatures to monitor the increase in the lifetime until such low temperatures that the calculations become computationally prohibitive. Note that at very low temperatures, all the normal modes of the system have amplitudes consistent with their zero-point energy. In classical MD simulations, these amplitudes go to zero, the modes become harmonic and the lifetimes very long [27]. At every time step, the 3N Cartesian coordinates of the atoms are written as linear combinations of the 3N normal modes of the supercell. Thus, the energies of all the modes can be plotted as a function of time. This approach allows not only the decay of the LVM of interest to be calculated, but also the identiﬁcation of the receiving modes, all of it as a function of time for various background temperatures of the cell. The pLVMs of the defect play a critical role in the decay process. We illustrate this approach with the case of the asymmetric stretch of H+ bc [30]. The result of the run performed at a background temperature of 75 K is shown in Fig. 3. The calculated decay of the LVM produces a good exponential ﬁt leading to a calculated lifetime of 7.8 ps at 75 K, a value that agrees very well with experiment [30]. An analysis of the time dependence of the energies of the normal modes of the cell shows that both wag modes and the symmetric stretch of the defect (at 262 cm−1 and 452 cm−1 , respectively) play important roles in the decay.

5 Vibrational Free Energies and Speciﬁc Heats Although the calculation of potential-energy surfaces is playing a most useful role in our understanding of the behavior of defects in semiconductors, the real-world involves nonzero temperatures. Samples undergo various thermal anneals, they are implanted and exposed to light, and most devices function at or above room temperature. The physics and chemistry of defects is obviously temperature dependent, as one observes processes such as diﬀusion and association or dissociation at various temperatures.

102

Stefan K. Estreicher and Mahdi Sanati

−1 Fig. 3. Plot of the energy (eV) of the asymmetric stretch mode of H+ bc at 2004 cm in the Si64 supercell, at the background temperature of 75 K vs. time (ps). The energies of 194 other modes of the cell are plotted as well. The ﬁrst step of the decay involves the pLVMs of the defect, which themselves have very short lifetimes

In all these processes, the Gibbs free energy is the most relevant quantity since virtually all experiments are done at constant pressure. However, we focus here on the Helmholtz free energy. Working at constant volume rather than constant pressure is appropriate up to several hundred degrees Celsius in most semiconductors because their thermal expansion coeﬃcient is very small. In Si for example, this coeﬃcient is 4.68 ×10−6 K−1 at room temperature and the phonon frequencies shift slowly with T . Indeed, the diﬀerence between the constant-pressure and constant-volume speciﬁc heats [32]2 CP − CV is 0.0165 J/mol · K at room temperature, a correction of only 0.08 % to CP = 20 J/mol · K. Thus, in the case of semiconductors such as Si and in the temperature range where the use of harmonic dynamical matrices is justiﬁed, calculating the phonon density of states g(ω) at T = 0 K and ignoring the temperature dependence of the lattice constant are reasonable approximations. Note that this ignores the frequency shifs associated with the anharmonicity. This greatly simpliﬁes the calculations. In fact, it renders them possible since calculating temperature-dependent phonon densities of state is a formidable task. 2

In this paper, “cal/g atom” should read “cal/mol” (or the numbers be divided by the atomic mass of Si).

Dynamical Matrices and Free Energies

103

Fig. 4. Phonon densities of state g(ω) calculated from harmonic dynamical matrices of the Si64 supercell evaluated at 90 q points in the BZ of the cell. The dashed line (ﬁrst peak at low frequency) was obtained with a double-zeta basis set and a 1×1×1 Monkhorst–Pack k-point sampling, the solid line (second peak) with a double-zeta polarized basis set and a 2 × 2 × 2 k-point sampling, and the long-dash line with a double-zeta polarized basis set and a 1 × 1 × 1 k-point sampling. As expected, the solid line best matches the experimental data [33]

The phonon densities of states of perfect (defect-free) crystals are normally calculated from the dynamical matrix of the primitive unit cell evaluated at thousands of q points in the Brillouin zone (BZ) of the crystal. When studying defects, large periodic supercells must be used, and the BZ of the supercell is distinct from that of the perfect solid. The eigenvalues of the dynamical matrix only provide a small number of normal mode frequencies, and the phonon density of states extrapolated from those few hundred frequencies lead to rather poor g(ω)s. However, evaluating the dynamical matrix at many q points in the BZ of the supercell works very well. Figure 4 shows three phonon densities of state obtained from harmonic dynamical matrices extrapolated at about 90 q points in the BZ of the supercell. The dynamical matrices were calculated with diﬀerent basis sets and Monkhorst–Pack k-point sampling in the Si64 supercell. The best ﬁt to the measured data [33] is obtained with the largest basis set (double-zeta polarized) and k-point sampling (2 × 2 × 2). In the harmonic approximation, the Helmholtz free energy is given by ∞ ln{sinh(ω/2kB T )}g(ω) dω , (8) Fvib (T ) = kB T 0

104

Stefan K. Estreicher and Mahdi Sanati

Fig. 5. Calculated and measured peak in the speciﬁc heat over T 3 for various isotopically pure samples of Ge. The dashed line (expt: crosses) is for 73 Ge, the solid line (expt: circles) is for the natural isotopic abundance, and the dotted line (expt: squares) is for 70 Ge

where kB is the Boltzmann constant. In the perfect cell, the integration is carried out up to the Γ phonon. With a defect in the supercell, the integral extends up to the highest normal mode of the cell (perturbed Γ phonon) and becomes a simple sum for the higher LVMs. Note that Fvib (T = 0) gives the total zero-point energy. Once Fvib is calculated, the vibrational entropy and speciﬁc heat at constant volume are given by 2 ∂Fvib ∂ Fvib CV = −T . (9) Svib = − ∂T ∂T 2 V V The latter can be compared to the measured Cp in order to determine up to what temperature the constant-volume and harmonic approximations are appropriate. We have demonstrated that the approximations work quite well up to some 700 K in the case of c-C, Si, Ge, and GaN (see [1, 34, 35]), and that the agreement with even ﬁne features is very good at low temperature. Figure 5 shows the calculated isotope-dependent peak in C/T 3 in Ge. The temperature at which it is predicted to occur and the splitting associated with various isotopes quantitatively reproduce the experimental data [36]. These tests give us conﬁdence that the phonon densities of states calculated in the manner described above are also accurate when defects are present in the same supercell, and therefore that the calculated Helmholtz vibrational free energies are accurate up to several hundred degrees Celsius. Of course, the Fvib obtained for a defect in a 64-host-atom cell correspond to a defect concentration of about 1.5 atomic per cent, which is very high. However, the few calculations we have performed with 128- and 216-atom cells

Dynamical Matrices and Free Energies

105

show that cell-size eﬀects are not very signiﬁcant, probably because g(ω) is only the weight function used in the integration, and small changes in this function have a minor impact on the result.

6 Theory of Defects at Finite Temperatures We are always interested in energy diﬀerences. This could be the energy diﬀerence between two conﬁgurations of the same defect, the energy diﬀerence between a bound complex and its dissociation products (binding energy), etc. At ﬁnite temperatures, such a total free-energy diﬀerence may contain several contributions: ∆F = ∆U + ∆Fvib + ∆Fe/h + ∆Frot + · · · − T ∆Sconﬁg .

(10)

∆U is the potential-energy diﬀerence obtained (in this Chapter) from ﬁrstprinciples density-functional theory. The vibrational free energy ∆Fvib has been discussed above. Depending on the defect under study, there may be diﬀerent concentrations of electrons (in the conduction band) or holes (in the valence band) because diﬀerent conﬁgurations of a given defect have diﬀerent electrical activities. This has nothing to do with the electrons or holes provided by the background dopants, which can be numerous. Instead, ∆Fe/h refers only to the change in the number of free carriers associated with the two conﬁgurations of the defect under study and the contributions of the background (dopant-associated) charge carriers cancel out. Unless one is dealing with unusually high changes in carrier concentrations, this term is very small and can be neglected [37]. Additional contributions to the free energy are associated with energy levels arising from rotational, magnetic, spin or other degrees of freedom speciﬁc to a particular defect. These terms can often be calculated directly from the appropriate partition functions [37]. One example is provided by the rotational free energies of interstitial H2 , HD, and D2 molecules (for a review of interstitial hydrogen molecules in semiconductors, see [38]) in Si. The rotational energies are Ej = j(j + 1)2 /M R2 , where M is the nuclear mass and R the internuclear separation. Since H2 consists of two protons (fermions), there are three ortho states (even combinations of spin: ↑↑, ↓↓, and ↑↓ + ↓↑) for which only odd values of j are allowed, and one para state (odd combination of spin: ↑↓ − ↓↑) for which only even values of j are allowed. This leads to the familiar set of two Raman lines with 3 : 1 intensity ratio. Since D2 consists of two bosons, the total wavefunction must be symmetric, and a similar argument leads to two Raman lines with 1 : 2 intensity ratios. Thus, the rotational free energy per molecule is given by Frot (T ) = −go kB T ln Zo − gp kB T ln Zp ,

(11)

106

Stefan K. Estreicher and Mahdi Sanati

where the partition functions are Zo = Σj=1,3,5,... (2j + 1)e−j(j+1)θ/T Zp = Σj=0,2,4,... (2j + 1)e

−j(j+1)θ/T

(12) ,

(13)

and {go , gp } = {3/4, 1/4} for H2 and {1/3, 2/3} for D2 . Since HD has no symmetry restrictions, all the values of j are allowed (single Raman line) and Frot (T ) = −kB T ln Z with Z = Σj (2j + 1)e−j(j+1)θ/T . The eﬀective temperature θ = 2 /2IkB contains the (classical) moment of inertia I of the molecule, which depends on the host. For free H2 , θ = 85.4 K. In Si, the molecule has a longer bond length than in free space [39] and θ = 73.0 K, 48.7 K and 36.5 K for H2 , HD and D2 , respectively. The values of the rotational free energies at 77 K, 300 K, and 800 K for interstitial H2 , HD, and D2 in Si are in Table 1. The largest rotational free energy per molecule occurs in the case of HD. When comparing the free energies of the interstitial H2 molecule with the interstitial H∗2 complex (which consists of a Si–Si replaced by two Si–H bonds: Si–Hbc · · · Si–Hab along a trigonal axis) which has no rotational degrees of freedom, the sum ∆Fvib + ∆Frot clearly favors H2 at higher temperatures [37]. This prediction is consistent with the fact that samples hydrogenated at high temperatures then rapidly quenched [40] show the presence of only H2 molecules. Table 1. Rotational free energy Frot (eV) for interstitial H2 , HD, and D2 in Si T (K)

77

300

800

H2 HD D2

−0.005 −0.004 −0.004

−0.030 −0.048 −0.040

−0.129 −0.194 −0.168

The importance of the conﬁgurational entropy term depends on the situation. When comparing the two metastable conﬁgurations of the CH∗2 complex [37], ∆Sconﬁg is exactly zero. When comparing interstitial H2 and H∗2 , the conﬁgurational entropy contribution is not zero but very small. Indeed, interstitial H2 occupies tetrahedral interstitial (t) sites, while H∗2 is at a bc site. Since there are twice as many bc as t sites, a (very) small ∆Sconﬁg results. The situation is very diﬀerent when calculating binding free energies. Indeed, for a complex {A, B} with dissociation products A and B, there are often vastly diﬀerent numbers of conﬁgurations for the dissociated species than for the complexes, sometimes leading to large values for ∆Sconﬁg . The calculation must be done using realistic concentrations of the species involved, and its details depend on the speciﬁc situation. The diﬀerence in conﬁgurational entropy per complex is ∆Sconﬁg = (kB /[{A, B}]) ln(Ωpair /Ωnopair ), where [{A, B}] is the number of complexes,

Dynamical Matrices and Free Energies

107

and Ωpair and Ωnopair are the number of conﬁgurations with all possible complexes forming and with all complexes dissociated, respectively. We set {A, B} to be “dissociated” when no B species is within a sphere of radius rc (eﬀective capture radius) of any A. The results are not very sensitive to the actual value of rc . The sites of A, B, and {A, B} are known and the concentrations [A] and [B] are estimated from experiment. If [A] is larger than [B], the maximum number of complexes is [{A, B}] = [B]. Although a real sample has traps for the dissociation products A and/or B that are distinct from isolated A and/or B in a perfect crystal, we ignore this additional complication. We consider here two boron–oxygen complexes in Si. Both of them contain an interstitial oxygen dimer ({Oi }2 ) trapped at either substitutional (Bs ) or interstitial (Bi ) boron. Thus, we consider the binding free energies of the {Bs , Oi , Oi } and {Bi , Oi , Oi } complexes (both in the +1 charge state). We do not discuss here the reasons why these complexes are important, how they form, and the consequences of complex formation for the sample at hand. These issues are discussed elsewhere [41, 42]. The conﬁgurations of the complexes and their dissociation products have been obtained from conjugate gradient geometry optimizations in the appropriate charge states. The binding energies at T = 0 K are ∆U = 0.54 eV and 0.61 eV for {Bs , Oi , Oi } and {Bi , Oi , Oi }, respectively. All the vibrational free energies have been calculated. We are faced now with the calculation of ∆Sconﬁg . Since we know the equilibrium sites of all the species involved, we know the number of equivalent orientations. However, we need to assume the concentrations of the various species in order to calculate the total number of conﬁgurations. We assume a sample with N = 5 × 1022 substitutional sites, [{Oi }2 ] = 1014 oxygen dimers, [Bs ] = 1019 substitutional and [Bi ] = 1014 interstitial boron impurities. The numbers depend on the sample, but these are realistic values that could correspond to an actual experimental situation. In a 1 cm3 sample, the number of sites for Bs , split-interstitial sites for Bi and staggered or square conﬁgurations [42] for {Oi }2 is 5 × 1022 . At low temperatures, all the Bs s trap one {Oi }2 . The number of ways one can arrange [{Oi }2 ] dimers among N sites is N !/[{Oi }2 ]!(N − [{Oi }2 ])!. Each {Oi }2 traps at one Bs and each {Bs , Oi , Oi } has 12 equivalent orientations. leading to 12[{Oi }2 ] possibilities. The remaining [Bs ] − [{Oi }2 ] borons are distributed among the remaining N − 12[{Oi }2 ] sites. Thus, the number of conﬁgurations for {Bs , Oi , Oi } complexes is Ωpairs =

12[{Oi }2 ] N !(N − 12[{Oi }2 ])! . [{Oi }2 ]!(N − [{Oi }2 ])!([Bs ] − [{Oi }2 ])!(N − [Bi ] − 11[{Oi }2 ])! (14)

At high temperatures, all the {Bs , Oi , Oi } complexes are dissociated. We can arrange [Bs ] borons among N substitutional sites in N !/[Bs ]!(N − [Bs ])! ways. If rc = 10 ˚ A, no oxygen dimer is within a sphere of radius 10 ˚ A of any boron, implying that about 150 substitutional sites around each Bs are

108

Stefan K. Estreicher and Mahdi Sanati

not allowed, which means that the number of sites available for the [{Oi }2 ] oxygen dimers is N − 150[Bs ]. The number of conﬁgurations for the {Oi }2 ’s is therefore (N − 150[Bs ])!/[{Oi }2 ]!(N − 150[Bs ] − [{Oi }2 ])!. Thus, the number of conﬁgurations for the dissociated complexes is Ωnopairs =

N !(N − 150[Bs ])! . [Bs ]!(N − [Bs ])![{Oi }2 ]!(N − 150[Bs ] − [{Oi }2 ])!

(15)

Using Sterling’s formula and an expansion for ln(1 + ε) with ε 1, we get 12[Bs ] 278[Bs ] [{Oi }2 ] ∆Sconﬁg = kB ln + − . (16) N N [Bs ] Similar calculations for {Bi , Oi , Oi } lead to [Bi ] [{Oi }2 ] 24[{Oi }2 ] − 1 + 32 + ∆Sconﬁg = kB ln . N N N

(17)

With the concentrations assumed, this gives ∆Sconﬁg = −0.515 meV/K and −1.538 meV/K for {Bs , Oi , Oi } and {Bi , Oi , Oi }, respectively. The diﬀerence between these situations is huge, and the reason for it is quite obvious. Consider an {A, B} complex that dissociates into A and B. If A and/or B are abundant (as is the case for Bs ), there are many conﬁgurations resulting in pairs and relatively few conﬁgurations with A away from B. On the other hand, when both A and B are scarce (as is the case for Bi and {Oi }2 ), there are far fewer ways to make pairs and a great number of dissociated conﬁgurations. The binding free energies of the {Bs , Oi , Oi } and {Bi , Oi , Oi } complexes are plotted as a function of temperature in Fig. 6. As shown in [41], the contribution of ∆Fvib is very small and the slope is almost entirely determined by the diﬀerence in conﬁgurational entropy. Thus, for a given {A, B} complex, the smaller the concentration of A or B, the larger the conﬁgurational entropy associated with the dissociated species and the smaller the entropy associated with complex formation. Then, the slope of the binding free energy Eb (T ) is much steeper. The opposite holds if A and/or B exist in high concentrations. In the example discussed in this Chapter, changing one component of the complex from Bs to Bi changes the relevant concentration from 1019 to 1014 , and this change of ﬁve orders of magnitudes roughly triples ∆Sconﬁg . Note that above the temperature T0 where Eb (T0 ) = 0, the interactions become repulsive. The value of T0 depends on Eb (0) and on the slope, that is on ∆Sconﬁg , which in turn depends on the concentrations of the dissociation products in the sample.

7 Discussion First-principles calculations of the properties of defects in periodic supercells have become quantitative in many respects. The conﬁgurations, energetics,

Dynamical Matrices and Free Energies

109

Fig. 6. Binding free energies of the {Bs , Oi , Oi } and {Bi , Oi , Oi } complexes in Si. The latter complex will not form above room temperature, where the interactions between Bs and {Oi }2 are repulsive because of conﬁgurational entropy

selected LVMs, spin densities and, to a lesser extent, electrical activities of localized defects can be predicted with very good accuracy. However, the knowledge of the entire dynamical matrix of the system provides much more information. The eigenvalues of this matrix give all the local, pseudolocal, and resonant defect-related modes, as well as the crystal phonon frequencies. They can be used to obtained high-quality phonon densities of states that in turn allow the calculation of vibrational free energies. Although the latter are limited to the constant-volume (and, in our case, harmonic) approximation, the calculated speciﬁc heats show that the results are reliable up to several hundred degrees Celsius. The eigenvectors of the dynamical matrix allow the localization of local modes to be quantiﬁed and their symmetry predicted. The eigenvectors can also be used to prepare a system in thermal equilibrium at any temperature without the need for lengthy thermalizations or even a thermostat. This feature is needed to calculate vibrational lifetimes as a function of temperature. The calculation of defect energetics at ﬁnite temperatures is relatively straightforward once the vibrational free energy is known. Indeed, rotational and other contributions can be obtained (or approximated) analytically. The most tricky, and sometimes most critical, part is the contribution of the conﬁgurational entropy. One example has been discussed here in detail. The result depends on the concentrations of the species involved, that is, on the sample. The binding free energy of an {A, B} complex in a crystal varies linearly with temperature, with a slope largely dominated by the diﬀerence in

110

Stefan K. Estreicher and Mahdi Sanati

conﬁgurational entropy between {A, B} and A away from B. If R is a dissociation rate, R exp{−Eb /kB T } = R exp{∆Sconﬁg /kB } exp{−Eb (0)/kB T }, and an Arrhenius plot yields a straight line with slope −Eb (0)/kB and intercept (ln R + ∆Sconﬁg /kB ). Thus, Arrhenius plots of the dissociation of an {A, B} complex in samples containing diﬀerent concentrations of A and/or B should produce parallel lines since the slopes are the same but the intercepts diﬀer. This suggests a way to measure conﬁgurational entropies. If we take R = 1011 and ∆Sconﬁg = −0.5 meV/K or −1.0 meV/K, the intercepts will be at 25.3 − 5.8 = 19.5 or 25.3 − 11.6 = 13.7, a measurable change. Even though the potential energy surface describing the interactions between A and B has a pronounced minimum when the {A, B} complex forms, these interactions become repulsive at temperatures T > T0 , where the critical temperature T0 is deﬁned from Eb (T0 ) = 0. If complex formation begins at a temperature near (but below) T0 , the variations of the slope of Eb (T ) with time (that is: as complex formation takes place and the concentrations of the various species change) will cause the interactions to shift from attractive to repulsive, probably resulting in a maximum precipitate size. Finally, since the diﬀerence in conﬁgurational entropy depends on the concentrations [A] and [B] in the sample, the binding free energy of a speciﬁc complex {A, B} at a speciﬁc temperature will be diﬀerent in samples containing diﬀerent concentrations of A or B. Many of these consequences of the temperature dependence of binding free energies are unexpected, not to say counterintuitive, because many of us are used to thinking in terms of potential energy alone. Yet, regardless of the value of the conﬁgurational entropy or the way it is calculated, the consequences are inescapable. Acknowledgements This work is supported in part by the R. A. Welch Foundation and the National Renewable Energy Laboratory.

References [1] R. K. Kremer, M. Cardona, E. Schmitt, J. Blumm, S. K. Estreicher, M. Sanati, M. Bockowski, I. Grzegory, T. Suski, A. Jezowski: Phys. Rev. B 72, 075209 (2005) 95, 104 [2] S. J. Pearton, J. W. Corbett, M. Stavola: Hydrogen in Crystalline Semiconductors (Springer, Berlin, Heidelberg 1991) 95 [3] S. Limpijumnong, C. G. Van de Walle: Phys. Rev. B 68, 235203 (2003) 96 [4] A. F. Wright, C. H. Seager, S. M. Myers, D. D. Koleske, A. A. Allerman: J. Appl. Phys. 94, 2311 (2003) 96 [5] A. Carvalho, R. Jones, J. Coutinho, P. R. Briddon: J. Phys.: Condens. Matter 17, L155 (2005) 96

Dynamical Matrices and Free Energies

111

[6] G. Davies: Phys. Rep. 176, 83 (1989) 96, 99 [7] S. Knack: Mater. Sci. Semic. Proc. 7, 125 (2005) 96 [8] S. K. Estreicher, D. West, J. Goss, S. Knack, J. Weber: Phys. Rev. Lett. 90, 035504 (2003) 96, 99 [9] S. K. Estreicher, D. West, M. Sanati: Phys. Rev. B 72, R13532 (2005) 96, 99 [10] D. S´ anchez-Portal, P. Ordej´ on, E. Artacho, J. M. Soler: Int. J. Quant. Chem. 65, 453 (1997) 96, 97 [11] E. Artacho, D. S´ anchez-Portal, P. Ordej´ on, A. Garc´ıa, J. M. Soler: phys. stat. sol. (b) 215, 809 (1999) 96 [12] D. M. Ceperley, B. J. Adler: Phys. Rev. Lett. 45, 566 (1980) 96 [13] S. Perdew, A. Zunger: Phys. Rev. B 32, 5048 (1981) 96 [14] L. Kleiman, D. M. Bylander: Phys. Rev. Lett. 48, 1425 (1982) 96 [15] O. F. Sankey, D. J. Niklevski: Phys. Rev. B 40, 3979 (1989) 97 [16] O. F. Sankey, D. J. Niklevski, D. A. Drabold, J. D. Dow: Phys. Rev. B 41, 12750 (1990) 97 [17] A. A. Demkov, J. Ortega, O. F. Sankey, M. P. Grumbach: Phys. Rev. B 52, 1618 (1995) 97 [18] H. J. Monkhorst, J. D. Pack: Phys. Rev. B 13, 5188 (1976) 97 [19] T. Inui, Y. Tanabe, Y. Onodera: Group Theory and Its Applications in Physics (Springer, Berlin, Heidelberg 1990) 97 [20] M. P. Allen, D. J. Tildesley: Computer Simulations of Liquids (Clarendon, Oxford 1987) 97 [21] J. L. Gavartin, D. J. Bacon: Comp. Mater. Sci. 10, 75 (1998) 97 [22] S. Baroni, P. Gioannozzi, A. Testa: Phys. Rev. Lett. 58, 1861 (1987) 97 [23] A. Fleszar, X. Gonze: Phys. Rev. Lett. 64, 2961 (1990) 97 [24] X. Gonze, C. Lee: Phys. Rev. B 55, 10355 (1997) 97 [25] J. M. Pruneda, S. K. Estreicher, J. Junquera, J. Ferrer, P. Ordej´ on: Phys. Rev. B 65, 075210 (2002) 97 [26] P. Ordej´ on, D. A. Drabold, R. M. Martin, S. Itoh: Phys. Rev. Lett. 75, 1324 (1995) 97 [27] D. West, S. K. Estreicher: Phys. Rev. Lett. 96, 115504 (2006) 98, 101 [28] J. L. Gavartin, A. M. Stoneham: Phil. Trans. Roy. Soc. Lond. A 361, 275 (2003) 98 [29] M. Budde, G. Luepke, C. Parks Cheney, N. H. Tolk, L. Feldman: Phys. Rev. Lett. 85, 1452 (2000) 99, 100 [30] M. Budde, G. Luepke, C. Parks Cheney, N. H. Tolk, L. C. Feldman: Phys. Rev. Lett. 85, 1452 (2000) 100, 101 [31] G. Lupke, X. Zhang, B. Sun, A. Fraser, N. H. Tolk, L. C. Feldman: Phys. Rev. Lett. 88, 135501 (2002) 100 [32] P. Flubacher, A. J. Leadbetter, J. A. Morrison: Philos. Mag. 4, 273 (1959) 102 [33] F. Widulle, T. Ruf, M. Konuma, I. Silier, M. Cardona, W. Kriegseis, V. I. Ozhogin: Solid State Commun. 118, 1 (2002) 103 [34] M. Cardona, R. K. Kremer, M. Sanati, S. K. Estreicher, T. R. Anthony: Solid State Commun. 133, 465 (2005) 104 [35] M. Sanati, S. K. Estreicher, M. Cardona: Solid State Commun. 131, 229 (2004) 104 [36] W. Schnelle, E. Gmelin: J. Phys.: Condens. Matter 13, 6087 (2001) 104

112

Stefan K. Estreicher and Mahdi Sanati

[37] S. K. Estreicher, M. Sanati, D. West, F. Ruymgaart: Phys. Rev. B 70, 125209 (2004) 105, 106 [38] S. K. Estreicher: Acta Phys. Polon. A 102, 403 (2002) 105 [39] S. K. Estreicher, K. Wells, P. A. Fedders, P. Ordej´ on: J. Phys.: Condens. Matter 13, 62 (2001) 106 [40] E. E. Chen, M. Stavola, W. B. Fowler: Phys. Rev. B 65, 245208 (2002) 106 [41] M. Sanati, S. K. Estreicher: Phys. Rev. B 72, 165206 (2005) 107, 108 ¨ [42] J. Adey, R. Jones, D. W. Palmer, P. R. Briddon, S. Oberg: Phys. Rev. Lett. 93, 055504 (2004) 107

Index ab initio, 101 absorption, 95 anharmonic, 102 annealing, 95 asymmetric, 99, 101 basis set, 96, 103 Boltzmann, 104 bond-centered, 99–101, 106 boron, 107, 108 Brillouin zone, 103 charge state, 107 classical, 101, 106 complex, 100, 105–110 concentration, 104–110 conduction band, 105 conﬁgurational entropy, 106, 108–110 conjugate gradient, 107 core, 96 correlation, 97 cutoﬀ, 97 decay, 96, 98, 100, 101 density of states, 95, 102, 103 density-functional theory, 96, 105 diﬀusion, 101 divacancy, 100 dopant, 105 double-zeta, 97, 103 dynamical matrix, 96, 97, 99, 103, 109 eigenvalues, 96, 97, 103, 109 eigenvectors, 96, 97, 99–101, 109 electron, 105

energetics, 108, 109 energy level, 105 entropy, 104, 106, 108–110 equilibrium, 96–98, 101, 107, 109 exchange-correlation, 96, 97 excitation, 101 fermion, 105 ﬁrst principles, 95, 96, 98, 105, 108 force, 97 force-constant matrix, 97 Fourier, 95 free carrier, 105 free energy, 96, 97, 102–110 frozen phonon, 97 FTIR, 95 GaN, 95, 104 Ge, 104 Gibbs, 102 Hartree, 97 Helmholtz, 96, 102–104 hole, 105 hydrogen, 96, 99, 100 impurity, 96, 99 interstitial, 105–107 isotope, 95, 104 linear response, 97 localization, 99, 109 magnetic, 105 migration, 95 molecular dynamics, 96

Dynamical Matrices and Free Energies Monkhorst–Pack, 97, 103 normal mode, 95–101, 103, 104 order-N , 97 oxygen, 107, 108 partition function, 105, 106 periodic, 96, 97, 103, 108 phonon, 95–97, 99–104, 109 photoluminescence, 96, 99 PL, 96, 99 polarization, 97 potential, 96–98, 101, 105, 110 proton, 105 pseudopotential, 96 quantum dot, 98 Raman, 95, 96, 105, 106 real space, 97 repulsive, 108, 110 resonant, 96, 109 rotational, 105, 106, 109 Sankey, 97 Si, 96, 99, 100, 102, 104–107 SIESTA, 96 speciﬁc heat, 97, 102, 104, 109

113

spin, 105, 109 strain, 96 stress, 95 substitutional, 107 supercell, 96, 97, 101, 103, 104, 108 surface, 101, 110 symmetric, 99, 101, 105 symmetry, 95, 96, 99, 106, 109 temperature, 96–102, 104, 106–110 tetrahedral, 106 thermal equilibrium, 96, 109 thermostat, 96, 98, 109 total energy, 96, 98 uniaxial stress, 95 vacancy, 96 valence band, 105 vibrational entropy, 104 vibrational free energy, 97, 104, 105, 107, 109 vibrational lifetime, 96–98, 100, 101, 109 vibrational modes, 95, 96, 99 vibrational spectroscopy, 95, 96 wag, 96, 99, 101

The Calculation of Free-Energies in Semiconductors: Defects, Transitions and Phase Diagrams E. R. Hern´ andez1 , A. Antonelli2 , L. Colombo3 , and P. Ordej´ on1 1

2

3

Institut de Ci`encia de Materials de Barcelona (ICMAB–CSIC), Campus de Bellaterra, 08193 Barcelona, Spain [email protected] Instituto de F´ısica Gleb Wataghin, Universidade Estadual de Campinas, Unicamp, 13083-970, Campinas, S˜ ao Paulo, Brazil SLACS (INFM-CNR) and Department of Physics, University of Cagliari, Cittadella Universitaria, I-09042 Monserrato (Ca), Italy

Abstract. In this chapter we review a series of novel techniques that make possible the eﬃcient calculation of free energies in condensed-matter systems, without resorting to the quasiharmonic approximation. Employing these techniques, it is possible to obtain the free energy of a given system not just at a predeﬁned temperature, but in a whole range of temperatures, from a single simulation. This makes possible the study of phase transitions, as well as the determination of equilibrium concentrations of defects as a function of temperature, as will be illustrated by examples of speciﬁc applications. The same techniques, coupled with a scheme to integrate the Clausius–Clapeyron equation, can lead to the eﬃcient determination of phase diagrams, a capability that will be illustrated with the calculation of the phase diagram of silicon.

1 Introduction The free-energy plays a central role in understanding the thermal properties of materials. From it, other properties of a material may be derived, such as the internal energy, the volume, entropy, etc. The phase behavior of a material is controlled by the values of the free-energy of its diﬀerent phases, and the concentrations of defects or impurities, as well as their partition among coexisting phases, are deﬁned by their chemical potentials, which are themselves obtained from the free-energy. It is clear, therefore, that it is highly desirable to have eﬃcient computational tools that can evaluate the free-energy of modeled materials in diﬀerent conditions of temperature and pressure (or volume). These methods should be accurate, and ideally it should be possible to combine them with ﬁrst-principles electronic structure methods, which provide an accurate picture of the structure, bonding and energetics of materials. In this Chapter we provide a self-contained description of recent theoretical developments that have contributed to making free-energy calculations D. A. Drabold, S. K. Estreicher (Eds.): Theory of Defects in Semiconductors, Topics Appl. Physics 104, 115–140 (2007) © Springer-Verlag Berlin Heidelberg 2007

116

E. R. Hern´ andez et al.

more accessible and eﬃcient, and we illustrate their capabilities with a series of applications, mostly in the ﬁeld of semiconductors, the topic of this book. Our intention in writing this Chapter has been to illustrate the potential of these techniques, some of which are still relatively little known. On the other hand, we have not intended to provide an exhaustive review of free-energy techniques, nor to dwell overmuch on the technical details of implementation. Both topics are covered at length in the excellent book by Frenkel and Smit [1], and also to some extent in the earlier book by Allen and Tildesley [2]. Nor has it been our intention to list the many examples of applications of free-energy techniques to problems in materials science, chemical physics, geology or biomolecular systems. Applications in some of these ﬁelds are reviewed to some extent in the articles by Rickman and LeSar [3] and by Ackland [4]. A very recent review of some of the techniques that will be discussed here, in particular the reversible scaling technique, is that of de Koning and Reinhardt [5].

2 The Calculation of Free-Energies Unlike the total internal energy, which depends only on the positions and velocities of the system at a single point in phase-space, the free-energy depends on all conﬁgurations (all state points) in the phase-space volume accessible to the system of interest in its given conditions of temperature and volume (or pressure). This is, in essence, why it is more arduous to calculate the free-energy in atomistic simulations of condensed-matter systems. From statistical mechanics we have that the free-energy at temperature T has the form F = −kB T ln Z ,

(1)

where kB is Boltzmann’s constant and Z is the partition function. In canonical ensemble conditions, i.e., constant number of particles N , constant volume V and constant temperature T , the partition function has the following expression: 1 ZN V T = dΓ e−βH(Γ ) , (2) N ! h3N V where Γ represents a point in phase-space, i.e., the 6N -dimensional space formed by the 3N momenta and 3N coordinates of the system, dΓ is the corresponding volume element, h is Planck’s constant, H is the Hamiltonian of the system, β = (kB T )−1 , and only conﬁgurations of volume V contribute to the integral. By writing an integral we are implicitly assuming that the system under consideration is being described by classical mechanics. In the quantum case the integral would be replaced by a discrete sum over quantum states.

Free-Energies in Semiconductors

117

Frequently it is desirable to consider the system under conditions of constant temperature and constant pressure (instead of constant volume), conditions that correspond to the so-called isothermal-isobaric or N P T ensemble. In this case, the partition function Z is generalized to ∞ 1 −βP V −βH(Γ ) dV e dΓ e ZNPT = . (3) N ! h3N 0 V In this case the free-energy is called the Gibbs free-energy (and we will label it G), to distinguish it from the canonical free energy (also called the Helmholtz free energy). The partition function plays the role of a normalization factor in thermodynamical averages. Consider, for example, some property A, which depends on the positions, and/or velocities of the particles in the system. Then, the canonical thermal average of A would be given by dΓ A(Γ ) e−βH(Γ ) , (4) AN V T = V −βH(Γ ) V dΓ e where the denominator can be recognized as the canonical partition function of (2) save for some factors that are canceled when taking the quotient of integrals. Such thermal averages are readily estimated by the standard simulation techniques of (canonical) molecular dynamics (MD) or Monte Carlo (MC), but it is important to note that these techniques directly estimate the quotient of integrals appearing in (4), and they cannot evaluate each of the integrals separately. Also, note that the free-energy is not itself a thermal average [it does not have the form of (4)], and therefore it cannot be obtained by direct MD or MC simulation. 2.1 Thermodynamic Integration and Adiabatic Switching Equations (2) and (3) clearly illustrate the diﬃculty of evaluating the freeenergy. These integrals are multidimensional, with as many dimensions as degrees of freedom in the system, and except for very simple models such as the ideal gas or the harmonic solid, they cannot be evaluated analytically. Furthermore, their high dimensionality precludes any attempt of evaluation by numerical quadrature methods. Thus it would seem that we are faced with an unsurmountable diﬃculty, though fortunately this is not the case. A way out of the problem is given by considering the dependence of the Hamiltonian H on some parameter λ, and asking ourselves how does the free-energy change with λ. It is immediately apparent that −βH(Γ ) dΓ ∂H ∂H ∂F ∂λ e V = = . (5) −βH(Γ ) ∂λ ∂λ V dΓ e Equation (5) shows that, while the free energy itself is not a thermal average, its derivative with respect to any parameter λ is a thermal average,

118

E. R. Hern´ andez et al.

and therefore it can be evaluated by employing conventional simulation techniques. This observation forms the basis of the technique known as the thermodynamic integration or coupling parameter [6, 7] method for evaluating free-energies, or rather free-energy diﬀerences. Consider a system, for example a solid, described by some potential U (r ), where r stands for the set of (generalized) coordinates specifying the positions of all degrees of freedom, for which we wish to evaluate the free-energy at some given temperature and volume. Now imagine that there is another system, similar in some sense to the system of interest, for which the free-energy is known at the temperature and volume at which we wish to know it for the system of interest. We noted earlier that one of the systems for which the canonical partition function can be evaluated analytically is the harmonic solid in which each atom is tied to its equilibrium lattice site by means of a harmonic spring. We will refer to the system for which the free-energy is known as the reference system, and will assume it is described by a potential Uref (r ). Let us now deﬁne the λ-dependent Hamiltonian Hλ =

1 p 2i + λU (r ) + (1 − λ)Uref (r ) . 2 i mi

(6)

Notice that when λ = 0 the Hamiltonian corresponds to that of the reference system (in our example the Einstein solid), while when λ = 1 it is that of the system of interest. A direct application of (5) tells us that the derivative of the free-energy Fλ associated with Hλ at λ ∈ [0, 1] is ∂Fλ = U (r ) − Uref (r )λ . ∂λ

(7)

Thus, to obtain the free-energy diﬀerence between the system of interest and the reference all we need to do is to integrate over λ, 1 dλ U (r ) − Uref (r )λ . (8) ∆F = F − Fref = 0

Since Fref is known, the sought F follows immediately. As stated above, the λ-dependent thermal averages U (r)−Uref (r )λ are readily obtained from standard simulation techniques. In practice, a discrete set of λ values in the interval [0, 1] is chosen (usually of the order of 5 to 10), and at each one of them an equilibrium simulation is carried out with Hamiltonian Hλ , from which the average U (r ) − Uref (r )λ is obtained. Then the integral in (8) is evaluated numerically. Note that because one samples directly the potential U (r ) − Uref(r ) using either MD or MC simulation techniques, no harmonic approximation is involved here, and thus anharmonic eﬀects are automatically taken into account. For this procedure to work, the chosen reference system must be in some sense similar to the target system. By this we mean that as λ is changed,

Free-Energies in Semiconductors

119

the system described by Hamiltonian Hλ (6) should not undergo any phase transitions. If that were to occur, some of the work spent in transforming the reference system into the system of interest (or vice versa) would actually be spent in the latent heat of the phase transition, and the resulting free-energy estimate would be inaccurate. Also, with a view to making the numerical integration of (8) accurate, it is desirable that the quantity U (r ) − Uref (r ) is subject to ﬂuctuations as small as possible, and this is another criterion of similarity between target and reference systems. We have already mentioned that a useful reference for free-energy calculations of solids is the Einstein crystal, but this would not be a good reference for a liquid. Fortunately, there are a number of simple model liquids, such as the Lennard–Jones ﬂuid [8] or the inverse-power ﬂuid [9], which have been extensively studied, and for which the free-energy has been tabulated over a wide range of temperature and pressure (density) conditions, and therefore these models serve the purpose of reference systems for liquids. Of course, for systems in the gas phase the ideal gas is an adequate reference. Equation (8) reminds us again of the fact that it is harder to obtain free-energies than it is to calculate thermal averages. A thermal average is typically obtained from a single equilibrium (MD or MC) simulation, while to evaluate the free-energy of the same system one needs several simulations. The eﬀort is increased further if the free-energy must be evaluated at other temperatures or volumes (pressures). It can easily be seen that the amount of work necessary to ﬁnd a coexistence point, let alone map out a phase boundary (where two coexisting phases have the same free-energy), soon becomes a daunting task, if one must resort to the schemes described thus far. Fortunately, starting in the early 1990s, a number of alternative techniques of increased eﬃciency have been developed, which considerably ameliorate this situation, and thanks to them the task of calculating phase boundaries, and even entire phase diagrams is nowadays more accessible. The ﬁrst such development was proposed by Watanabe and Reinhardt [10], who showed that accurate estimations of ∆F could be obtained from a single simulation with Hamiltonian Hλ (6), during which the parameter λ is slowly (i.e., quasiadiabatically) switched from 0 to 1 (or vice versa). Thus, the task of performing several equilibrium simulations at diﬀerent values of λ to obtain ∆F is reduced to that of performing a single nonequilibrium simulation on a system that quasiadiabatically transmutes from the reference system to the system of interest (or the reverse). During this nonequilibrium simulation one computes the irreversible work (reversible in the adiabatic limit) Wirr (t, λ = 0 → 1), given by Wirr (t, λ = 0 → 1) =

t

dt λ˙ {U [r (t )] − Uref [r (t )]} ,

(9)

0

where λ˙ = dλ/ dt is the rate of change of λ, and the time variable corresponds to either real time in an MD simulation, or to simulation time in

120

E. R. Hern´ andez et al.

an MC simulation (each MC sweep corresponding to a unit of simulation time). In the adiabatic limit, Wirr (t = ∞, λ = 0 → 1) would be equal to the free-energy diﬀerence ∆F , but since in practice strict adiabaticity cannot be attained, Wirr (t, λ = 0 → 1) is only an approximation to ∆F , due to entropic dissipation eﬀects (see below). Nevertheless, experience shows that (9) provides satisfactorily accurate results with modest computational eﬀorts, indeed more modest than those required in a full thermodynamic integration calculation. We will refer to the method of Watanabe and Reinhardt as the adiabatic switching method. The adiabatic switching method is based on two key observations. The ﬁrst one is that, by virtue of Liouville’s theorem, any classical trajectory, even one generated by a time-dependent Hamiltonian, preserves the phasespace volume. In other words, the trajectory generated by a time-dependent classical Hamiltonian will evolve on a phase-space hypersurface that, though itself changing shape with time, encloses a ﬁxed amount of phase-space volume. The second observation, due to Hertz [10], applies when the evolution of the Hamiltonian is slow, or adiabatic. Under these conditions, the evolving hypersurface of phase-space on which the trajectory moves corresponds, at each instant t, to a constant energy shell of energy H(t). Therefore, a trajectory generated by an adiabatically evolving Hamiltonian preserves the entropy, deﬁned as S = kB ln Ω, where Ω is the (invariant) phase-space volume enclosed by the adiabatically evolving phase-space hypersurface. This is the mechanical analog of the observation in thermodynamics that an adiabatic process (i.e., one that proceeds along a succession of equilibrium states) exerted on a system preserves its entropy. The consequence of this is that, since ∆S = 0 when λ in (6) is adiabatically switched along the trajectory generated by Hλ in canonical ensemble conditions, the free-energy change involved in this switching process can be measured by the internal energy change alone. As pointed out above, in the limit of strict adiabaticity, we would have that ∆F = Wirr (t = ∞, λ = 0 → 1), but since the switching process cannot be truly adiabatic there will be some entropic dissipative effects, which will cause Wirr (t, λ = 0 → 1) to be an upper bound of ∆F . In fact, one can also run the switching simulation in reverse, i.e., switching λ from 1 to 0, and the resulting irreversible work, −Wirr (t, λ = 1 → 0) then provides a lower bound to ∆F . This proves to be a convenient way of determining error bars for the estimated free-energy [5]. 2.2 Reversible Scaling Another important development allows one to obtain the free energy in a quasicontinuous range of temperatures, starting from a reference temperature at which the free-energy is known, from either a previous adiabatic switching or thermodynamic integration calculation. This method, known as reversible scaling, was introduced by de Koning et al. [11], and is based on the

Free-Energies in Semiconductors

121

formal equivalence that exists, from a statistical-mechanics perspective, between scaling the temperature and scaling the potential. Indeed, the canonical partition function of a system described by potential U (r ) at temperature T is U (r ) 1 −k T B , dr e (10) ZN V T = N ! Λ3N (T ) V where the factor Λ(T ) = (h2 /2πmkB T )1/2 results from integrating out the momenta, and we have assumed that all particles are identical. Now, consider a system described by a scaled potential, λU (r ), at a diﬀerent temperature T0 . For this system, the partition function would be λU (r ) 1 − ZN V T0 (λ) = dr e kB T0 3N N ! Λ (T0 ) V λ3N/2 − k UT(r )/λ B 0 = dr e . (11) N ! Λ3N (T0 /λ) V Now, it is easy to see that, except for a factor of λ3N/2 , the partition function of the scaled system at temperature T0 /λ and that of the unscaled system at temperature T are identical, if we impose that T0 = λT . From this it is easy to derive the following relation between the free-energies of the scaled and unscaled systems: F (T ) Fs (T0 , λ) 3 = + N kB ln λ . T T0 2

(12)

In words, we have related the free-energy of a system at temperature T to that of an appropriately scaled system at temperature T0 such that T0 = λT . From a formal point of view not much has been done. However, using the technique of adiabatic switching described in Sect. 2.1 it is very simple to calculate Fs (T0 , λ), at ﬁxed temperature T0 but in a quasicontinuous range of λ values in some interval λ ∈ [λmin , λmax ], and by virtue of (12), each of these Fs (T0 , λ) values corresponds to the free-energy of the unscaled system in a quasicontinuous range of temperatures T ∈ [T0 /λmax , T0 /λmin ]. Fs (T0 , λ) is obtained as NV T Fs (T0 , λ) = Fs (T0 , λ0 ) + Wirr (λ0 → λ),

(13)

where Fs (T0 , λ0 ) is the free-energy of the scaled system at the initial value of NV T (λ0 → λ) is the scaling parameter λ0 (usually either λmin or λmax ) and Wirr the work done by switching the scaling parameter from λ0 to λ, which, using the adiabatic switching technique is estimated as t NV T (λ0 → λ) = dt λ˙ U [r (t )] . (14) Wirr 0

122

E. R. Hern´ andez et al.

Thus, instead of having to run a separate adiabatic switching or thermodynamic integration calculation to obtain the free-energy of the system of interest for each temperature in a discrete set spanning the desired range of temperatures, one can perform a single adiabatic switching calculation of the scaled system at some appropriately chosen temperature T0 , and simply quasicontinuously vary the scaling parameter λ from λmin to λmax (or vice versa). Note that in (14) each time step leads to a new value of λ and a correNV T (λ0 → λ), which, through (12), leads to an estimate sponding value of Wirr of F (T ) at temperature T = T0 /λ. For the sake of simplicity, we have presented the method in the context of the canonical ensemble, but the same ideas can be applied in the isothermalisobaric case [12], which is of more interest when it comes to studying phase transitions. In this case one ﬁnds that it is necessary not only to scale the potential energy but the pressure as well, so that the scaled system pressure is Ps (λ) = λP , P being the pressure of the unscaled system. Then (12) transforms into Gs [T0 , Ps (λ)] 3 G(T, P ) = + N kB ln λ , T T0 2

(15)

relating the Gibbs free-energies of the scaled and unscaled systems, and NPT Gs (T0 , Ps , λ) = Gs [T0 , Ps (λ0 ), λ0 ] + Wirr (λ0 → λ), with

t dPs (λ) NPT ˙ V (t ) , dt λ U [r (t )] + (16) Wirr (λ0 → λ) = dλ 0 which is obtained from an adiabatic switching calculation carried out under isobaric-isothermal conditions. The reversible scaling technique discussed above provides an eﬃcient procedure for calculating coexistence points between diﬀerent phases of a given material or substance. Using reversible scaling in the isothermal-isobaric ensemble one can easily obtain the Gibbs free energy of the two diﬀerent phases, at constant pressure P , in a range of temperatures bounding the values where the coexistence point is expected to be located. The temperature at which the two free energies match is by deﬁnition the coexistence temperature of the two phases at pressure P . This strategy is illustrated for the particular case of the melting point of Si in the diamond phase at 0 pressure in Fig. 1. Si was simulated with the semiempirical tight-binding (TB) [13] Hamiltonian due to Lenosky and coworkers [14], which describes very well the structural and thermal properties of Si in several of its phases [15]. 2.3 Phase Boundaries and Phase Diagrams If one wishes to map out an entire phase boundary, rather than just a single coexistence point between two phases in equilibrium, one option would be to iterate the procedure illustrated in Fig. 1 to obtain new coexistence temperatures at diﬀerent pressures. However, an alternative method exists

Free-Energies in Semiconductors

123

Fig. 1. Gibbs free-energy of the diamond and liquid phases of Si in the neighborhood of the zero-pressure melting point, as obtained from reversible scaling simulations with the Lenosky et al. [14] model. The simulations contain 128 atoms in each phase, and four k-points were used to sample the Brillouin zone. It can be seen that the two free-energies become equal at approximately 1551 K, and above this temperature the liquid becomes thermodynamically more stable. More details of these calculations can be found in [15, 16]

that is often more eﬃcient and practical, since it does not require any further calculation of free-energies along the phase boundary. This technique was pioneered by Kofke [17, 18], and is known as Gibbs–Duhem or Clausius– Clapeyron integration. In this method, starting from some previously determined coexistence point along the desired phase boundary, one numerically solves the Clausius–Clapeyron equation: ∆V dT =T . dP ∆H

(17)

This equation relates the slope of the phase boundary, dT / dP , at the current coexistence point, given by temperature T and pressure P , with the diﬀerences of molar volumes ∆V and molar enthalpies ∆H of the coexisting phases. Thus, if ∆V and ∆H are known at the current coexistence point, one can estimate how the equilibrium temperature will change if the pressure changes by some small amount. ∆V and ∆H can be obtained from standard equilibrium simulations using MD or MC. Note that the interface between the coexisting phases need not be taken into account: each phase is independently simulated in a separate simulation box, at identical conditions of temperature and pressure. Once the average volume and enthalpy of each phase is known with suﬃcient accuracy, new coexistence conditions are derived from (17),

124

E. R. Hern´ andez et al.

and the process is iterated until the phase boundary has been mapped out. The stability and accuracy of the method have been analyzed in detail by Kofke [18]. This method has been extensively employed, and some particular examples of its use will be illustrated in the next section. A parallelism can be established between Kofke’s Clausius–Clapeyron integration method and thermodynamic integration. In the latter, one performs a series of equilibrium simulations at diﬀerent λ values in the range [0, 1] with the aim of obtaining the free-energy of the system. In Clausius–Clapeyron integration, one performs a series of equilibrium simulations at diﬀerent values of the independent variable (T or P ), and uses (17) to ﬁnd how the dependent variable (P or T ) adapts to the change in the independent variable such that the two phases remain in equilibrium. However, as we saw in Sect. 2.1, the calculation of the free energy can be made more eﬃciently using adiabatic switching, where instead of several (ca. 5–10) equilibrium simulations, a single nonequilibrium quasiadiabatic simulation is employed. It is therefore natural to ask if a similar gain in eﬃciency is possible in Clausius–Clapeyron integration, and the answer is aﬃrmative, as de Koning et al. [12] have shown. The Clausius–Clapeyron equation (17) is arrived at by demanding that the change in free-energy due to a small change in the independent variable be the same in both phases. For illustrative purposes, let us consider the case in which the temperature T plays the role of independent variable, while the pressure P is the dependent one. As in the reversible scaling method, let us now consider scaled versions of the two phases at constant temperature T0 and pressure Ps . When λ = 1 these correspond to some initial coexistence point. The free-energies of the scaled phases will be GS,a and GS,b , respectively. In the scaled case, now the temperature is ﬁxed, and the role of the independent variable is played by λ. Therefore, as λ is changed, the scaled phases will depart from equilibrium, unless the scaled pressure Ps (λ) evolves in such a way as to make the change in GS,a equal to that in GS,b . By requiring that this be the case, one arrives at a Clausius–Clapeyron equation for Ps (λ), which reads dPs (λ) ∆U =− , dλ ∆V

(18)

where ∆U is the diﬀerence of internal energies between the two phases. If λ is stationary, the values of ∆U and ∆V would be obtained from standard equilibrium simulations, and everything would be exactly as in the case of the Clausius–Clapeyron integration of Kofke, but working with the scaled phases. However, (18) suggests that, as in the reversible scaling method, λ can be varied quasicontinuously (i.e., quasiadiabatically). In these conditions, ∆U and ∆V will adapt to the changing value of λ, and Ps (λ) will evolve according to (18) such that the scaled phases remain in equilibrium. Through the scaling relations T = T0 /λ, P = λPs (λ), the equilibrium pressure P (T ) at temperature T will be obtained for the unscaled phases. De Koning et al. demonstrated the usefulness of the method by calculating the melting curve

Free-Energies in Semiconductors

125

of the Lennard–Jones model for pressures between 0 up to 160 reduced units, obtaining results matching those obtained previously by Agrawal and Kofke [19] employing the standard (equilibrium) Clausius–Clapeyron integration method. In the next section we will see another application, in which this dynamic Clausius–Clapeyron integration method has been recently used to obtain the phase diagram of Si as predicted by a semiempirical TB model.

3 Applications Let us now discuss some examples of applications of the techniques described in Sect. 2 to the study of thermal properties of defects, phase transitions and phase diagrams. Our focus, given the theme of this book, will be mostly on semiconductors, though occasionally we will mention examples of applications to other types of materials, due to their importance or to their illustrative value. Let us remark that we do not intend to provide an exhaustive review of the literature concerned with thermal properties of semiconducting materials, as this would be beyond the scope of this Chapter. Our aim is rather to illustrate the capabilities of the novel techniques discussed above. 3.1 Thermal Properties of Defects Most calculations of the free-energy and other thermal properties of defects in semiconductors to be found in the literature rely on the use of the quasiharmonic approximation, and since this topic is going to be covered at length in Chap. 8, we will not dwell much on it here. However, we must mention two studies that employed techniques described in Sect. 2, and that therefore go beyond the quasiharmonic approximation. Both studies illustrate nicely the potential of the techniques discussed in this Chapter, and make evident the need for incorporating the eﬀects of anharmonicity at suﬃciently high temperatures. The ﬁrst example is the study of J¨ a¨ askel¨ ainen et al. [20], who computed the free-energy of formation of the vacancy and self-interstitial in Si as a function of temperature. A thorough study of self-diﬀusion requires accurate free-energy calculations (aimed at predicting temperature-dependent equilibrium concentrations) and extensive diﬀusivity simulations (aimed at computing migration energies and diﬀusivity prefactors) for all relevant kinds of native defects. In their study, J¨ a¨ askel¨ainen and coworkers considered only self-interstitial (I) and vacancy (V) defects.

126

E. R. Hern´ andez et al.

f f f Once the formation free-energies FI,V = EI,V + T SI,V , as well as migram 0 tion energies EI,V and diﬀusivity prefactors dI,V are known, the self-diﬀusion coeﬃcient DSD (T ) can be cast in the form

EIf − T SIf 0 DSD (T ) = dI exp − exp (−EIm /kB T ) kB T

f E f − T SV m /kB T ) , (19) + d0V exp − V exp (−EV kB T

so that a direct theory vs. experiment comparison is possible. The thermodynamic integration (TI) method [1] was adopted by J¨ a¨ askef in c-Si by means of the tight-binding (TB) l¨ ainen et al. [20] to evaluate FI,V model provided by Kwon et al. [21]. The ensemble average appearing in (8) was performed during constant-volume, constant-temperature molecular dynamics (TBMD) simulations in a 64±1 atom periodically repeated cell. The thermodynamical integration was performed over 16 λ points, while freeenergy calculations were performed at four diﬀerent temperatures, namely 300 K, 500 K, 1000 K and 1400 K. The formation entropy SIf for the selfinterstitial defect was found to be almost constant with temperature, the average value being SIf = 11.2kB . First-principles calculations [22] predict a value of SIf ∼ 10kB when including anharmonic terms through TI calculations as well. The case of a vacancy is more complicated due to its high mobility [23], which eﬀectively adds a sizeable contribution of migration entropy in the TI free-energy calculations. This is conﬁrmed by the fact that f varied in the range 10.2kB to 11.7kB in the sethe computed value of SV f lected temperature interval, with an average value of SV ∼ 10.8kB . In the case of the vacancy, in order to prevent the double counting of the migration entropy, which is already taken into account by the TBMD simulations aimed at measuring d0V , short observation runs were performed, taking care to select only those simulations where V diﬀusion actually did not take place. The resulting average formation (i.e., conﬁgurational + vibrational) entropy f ∼ 8.8kB . was SV f are in good qualitative agreement with These TBMD results for SIf and SV ﬁrst-principles calculations by Bl¨ ochl and coworkers [22] in the sense that the diﬀerence in the entropies of formation for interstitials and vacancies is of the order of 1kB to 2kB in both studies, with a larger formation entropy for the interstitial. Diﬀusivity constants were ﬁnally obtained by using the migration prefactors and energies computed by means of the same TBMD functional, following Tang et al. [23]. The overall reliability of this TI-TBMD approach is summarized in Fig. 2, where the silicon TBMD total self-diﬀusion coeﬃcient DSD = DI + DV is compared with state-of-the-art experimental data [24, 25]. As can be seen, there is extremely good agreement between the diﬀerent sets of experimental data and the theoretical results. These temper-

Free-Energies in Semiconductors

127

-10 Expt. Expt. Theo.

2

Log10 DSD(cm s)

-12

-14

-16

-18

-20 0.55

0.65

0.75

0.85

0.95

-1

1000/T (K )

Fig. 2. Temperature dependence of the total self-diﬀusion coeﬃcient in silicon. The continuous line is the experimental results of [24], the dotted line is the experimental measurements of [25], and the dot-dash line is the theoretical results of [20]. Reprinted with permission from J¨ aa ¨skel¨ ainen et al. [20], Copyright (2001) by the American Physical Society

ature-dependent self-diﬀusion values should be therefore useful in modeling Si bulk processing. As noted above, J¨aa¨skel¨ainen et al. implicitly assumed that the main contributors to self-diﬀusion in Si are the vacancy and interstitial defects, thus neglecting the possible contribution of other kinds of defects, such as clusters of interstitials or vacancies. Indeed, both ﬁrst-principles simulations [26] and tight-binding temperature-accelerated MD simulations have revealed that small clusters of defects can also make substantial contributions to the mobility. In particular, the study of Cogoni et al. [27] shows quite conclusively that in all ranges of temperatures the mobility of the interstitial dimer is comparable to that of the single interstitial. At suﬃciently high temperatures (above 1400 K) even the trimer diﬀuses fairly rapidly. However, it should be noted that to better estimate the signiﬁcance of these clusters of interstitials to self-diﬀusion in Si, their concentrations, as well as their mobilities have to be taken into account. Since their formation energies are larger than that of the single interstitial, it is likely that in equilibrium conditions their net contribution to self-diﬀusion will be rather small. On the other hand, the processing of Si samples may incur nonequilibrium defect populations, and under these conditions the contribution of clusters of interstitials to self-diﬀusion could be important. Let us now focus on another aspect of the thermal properties of Si. At room temperature, Si is a brittle material, but as the temperature is raised, a dramatic change in its mechanical properties takes place in a very narrow

128

E. R. Hern´ andez et al.

range of temperatures around 873 K, and Si becomes a ductile material [28]. It is accepted that this change is due to the fact that at this temperature dislocations can be more easily nucleated and emitted at the tip of cracks, blunting the crack tip and making its propagation through the material more diﬃcult. In Si there are two sets of closely packed {111} slip planes, called shuﬄe and glide. While dislocations nucleated at the shuﬄe set have high Peierls stress and low mobility, the dislocations on the glide set can split into partials, having a smaller Peierls stress and higher mobility. It is believed that the brittle–ductile transition in silicon can be related to the change in dominance of one set over the other. Over 10 years ago, Rice and collaborators [29–31] proposed a model in which the resistance to nucleation of dislocations at the crack tip can be measured by the so-called unstable stacking energy, which is the lowest energy barrier that needs to be crossed when one half of a crystal slips relative to the other half. Through a combination of density-functional theory calculation with Vineyard’s transition state theory, Kaxiras and Duesbery [32] have shown that an abrupt transition from shuﬄe to glide dominance happens with temperature. In this approach, the temperature eﬀects were considered without taking into account the real dynamics of the atoms on either side of the slip plane. The calculations by de Koning et al. [33] using the adibatic switching method within MD simulations fully included such temperature eﬀects. Figure 3 shows the phase diagram for preferable nucleation of dislocations on shuﬄe plane versus glide set. One can see from the ﬁgure that the inclusion of all anharmonic eﬀects in the calculations by de Koning et al. did not change substantially the diagram previously obtained by Kaxiras and Duesbery. 3.2 Melting of Silicon Probably the ﬁrst calculation of the melting point of crystalline Si from simulation was carried out by Broughton and Li [34], employing the well-known Stillinger–Weber [35] potential. Broughton and Li calculated the zero-pressure melting point by obtaining the free-energy of the crystal and liquid phases at diﬀerent temperatures. The free-energy of the crystal was calculated by thermodynamic integration at diﬀerent temperatures, taking as a reference system the harmonic solid. For the liquid phase, the free-energy was obtained by ﬁrst switching oﬀ the attractive two-body part of the potential to avoid the occurrence of a possible ﬁrst-order liquid–vapour transition, and then expanding the system to zero density. They obtained a melting temperature of 1691 K, with an estimated error of ±20 K. This value is in very good agreement with the currently accepted experimental value of 1687 K [36], an agreement that is perhaps not so surprising, as the Stillinger–Weber potential was parametrized on the basis of data from both the crystal and liquid phases. The careful free-energy tabulation of the Stillinger–Weber potential for the crystal and liquid phases of Si achieved by Broughton and Li has al-

Free-Energies in Semiconductors

129

Fig. 3. Coexistence curves separating the preferable nucleation of dislocations on shuﬄe planes versus glide set. The full line is the results obtained from the EDIP potential after applying a correction for the overestimation of γus , the unstable stacking energy, by this potential. The dotted line shows the results obtained with DFT LDA calculations, and the dashed horizontal line gives the value of the experimental brittle fracture stress. Figure reprinted with permission from de Koning et al. [33]. Copyright (1998) by the American Physical Society

lowed subsequent studies (see below) to use this model as a reference system for free-energy calculations of Si employing higher levels of theory. In a subsequent study, Clancy and Cook [37] compared several empirical potential models in their ability to describe the thermal behavior of Si and Ge; in particular they considered the well-known Tersoﬀ potential [38–40], and a form of the embedded atom potential modiﬁed to describe covalent bonding (modiﬁed embedded atom method, MEAM) [41]. In this work the melting point for each model was determined by employing the two-phase coexistence method, i.e., by simulating the solid and liquid in a large cell in direct coexistence. It was found that the Tersoﬀ model for Si led to a melting temperature of 2547 K, well above the experimental value of 1687 K, while the MEAM showed the opposite behavior, underestimating the melting temperature at 1475 K. Both models correctly predict, as does the Stillinger– Weber potential, a slight increase of the density upon melting, though all models underestimate somewhat the crystal and liquid densities. A similar study, comparing several tight-binding models in their ability to reproduce

130

E. R. Hern´ andez et al.

the liquid structure, and the melting temperature of Si has been recently carried out by Kaczmarski et al. [15]. Very soon after the proposal of the adiabatic switching technique by Watanabe and Reinhardt [10], Sugino and Car [42] employed this technique, combined with ﬁrst-principles Car–Parrinello dynamics [43], to study the melting of Si. These authors employed as a reference system the Stillinger– Weber potential for both the crystal and liquid phases, for which the free energy had been previously determined by Broughton and Li [34] as a function of temperature, as discussed above. Sugino and Car thus calculated the free-energy diﬀerence between the reference model and a ﬁrst-principles description of Si employing density-functional theory (DFT) with the local-density approximation (LDA) for the exchange and correlation energy, combined with the pseudopotential approximation. They predicted a melting temperature of 1350 ± 100 K, some 300 K below the experimental value. This error was attributed to the relative destabilization of the solid phase with respect to the liquid in the LDA, which would result in a reduction of the melting point. Any small error in the diﬀerence of free energies translates into a rather large error in the melting temperature, and hence these kind of calculations require very stringent accuracy constraints. More recently, Alf`e and Gillan [44] have revisited the theme of the melting of Si from ﬁrst-principles simulations. These authors, employing the LDA approximation obtained a melting temperature of 1300 ± 50 K, in good agreement with the value reported earlier by Sugino and Car. They also performed calculations employing a generalized gradient approximation (GGA) to the exchange and correlation energy, obtaining in this case a somewhat improved value of the melting temperature of 1492 ± 50 K, which, although still below the experimental value by nearly 200 K, clearly improves upon the LDA result. This observation conﬁrms the suggestion made by Sugino and Car that the underestimation of the melting point was most likely attributable to errors in the exchange and correlation functional, and not in any other of the approximations involved in the simulations (pseudopotential, basis set, etc.). It is worth noting that Si is a troublesome case, as the melting point separates two phases of diﬀerent electronic character: while the crystal is semiconducting, the liquid is metallic. Errors due to the approximate nature of the functionals may, in general, be of diﬀerent size in insulators and metals. Indeed, when systems in which the electronic character of the material does not change upon melting have been studied, DFT methods can predict melting temperatures within a few tens of K of the experimental result. This is the case for Al, which has been studied by de Wijs et al. [45], who reported a value of Tm = 890 ± 20 K, compared to an experimental value of 933.47 K. Both liquid silicon (l-Si) and water present an anomalous behavior of the density and speciﬁc heat with temperature. Also, like water, l-Si is a very poor glass former, in the sense that it is extremely diﬃcult to experimentally obtain the amorphous phase by quenching from the melt. In the case of silicon, as a matter of fact, this has never been achieved. Due to these similarities, it has

Free-Energies in Semiconductors

131

Fig. 4. Kauzmann plot for the environment-dependent interatomic potential (EDIP)-Si. Normalized entropy diﬀerence between the disordered and crystalline phases according to the EDIP model as a function of normalized temperature. Reprinted with permission from [46]. Copyright (2004), American Institute of Physics

been proposed that, as in water, supercooled l-Si could present polymorphism, as well as polyamorphism. Experiments have suggested the existence of a ﬁrst-order-like liquid–liquid (l–l) transition in supercooled l-Si [47, 48]. Also, it has been considered, based on experimental results, that the transition from amorphous silicon (a-Si) to l-Si (l–a transition) would also be a discontinuous transition [47]. From the computational point of view, MD simulations using the Stillinger–Weber potential [49] have determined a l–l transition at about 1060 K, but have not found evidence of a l–a transition. Other computational results, using the EDIP [50] model for silicon, found a ﬁrst-order-like l–a transition at 1170 K and no evidence of a l–l transition [51]. In a recent study using the reversible scaling method within MC simulations and also using the EDIP model, Miranda and Antonelli [46] have shown that a l–l transition occurs at 1135 K and a l–a transition takes place at 843 K. Figure 4 shows the normalized excess entropy of the liquid phase with respect to the crystalline phase as a function of the normalized temperature. From the ﬁgure one can see that as the temperature is lowered, ﬁrst a discontinuous transition takes place, and as the temperature is lowered further, a glass-like transition occurs, beyond which the excess entropy becomes constant. This would be in agreement with recent experiments [52] that have indicated that a glasslike transition takes place at about 1000 K. Also, the conﬁgurational entropy obtained by Miranda and Antonelli for the amorphous phase is in agreement with that obtained by Vink and Barkema [53] using a methodology based on graph and information theories.

132

E. R. Hern´ andez et al.

Fig. 5. Phase diagram of water. The left panel shows the phase diagram predicted by the TIP4P potential; the left panel that obtained from the SPC/E model, and the central panel displays the experimental phase diagram. The SPC/E phase diagram has been shifted by 0.1 GPa in order to make phase I visible, as this phase appears at small negative pressures, according to this model. Figure reprinted with permission from Sanz et al. [54]. Copyright (2004) by the American Physical Society

3.3 Phase Diagrams As discussed above, the eﬃcient free-energy techniques exposed in Sect. 2, combined with Kofke’s Clausius–Clapeyron integration method, can be employed to calculate phase diagrams of materials entirely from simulation. Two particularly interesting examples of applications of these techniques are the determination of the phase diagram of water by Sanz et al. [54], and the phase diagram of carbon by Ghiringhelli et al. [55]. The phase diagram of water is very rich, with at least nine stable ice phases documented. Many diﬀerent empirical potentials aiming at describing this complicated system have been proposed in the literature, and Sanz and coworkers [54] have compared two of them, namely the so-called TIP4P model of Jorgensen et al. [56], and the SPC/E model of Berendsen et al. [57], in their ability to reproduce the experimental phase diagram of water. Sanz et al. used standard thermodynamic integration to locate coexistence points between the diﬀerent phases, and then obtained the corresponding coexistence lines by using Clausius–Clapeyron integration as proposed by Kofke [17, 18]. The theoretical phase diagrams derived from TIP4P and SPC/E models are compared with the experimental water phase diagram in Fig. 5. As can be seen in Fig. 5, the phase diagram predicted by the TIP4P model agrees fairly well with the experimental one, while that resulting from the SPC/E model deviates noticeably. The TIP4P model correctly predicts ice phases I, II, III, V, VI, VII and VIII to be stable, as indeed they are found to be in real water, while the SPC/E model, on the other hand, predicts wrongly that phases III and V are metastable (i.e., there is no temperature– pressure domain in which these phases are found to have the lowest Gibbs free-energy). A second example, more within the theme of this book, is provided by the phase diagram of carbon obtained by Ghiringhelli et al. [55]. If mod-

Free-Energies in Semiconductors

133

Fig. 6. Phase diagram of carbon as obtained by Ghiringhelli and coworkers [55]. This ﬁgure shows the phase diagram only up to pressures of 60 GPa, but the diamond melting line was followed up to pressures of 400 GPa. The solid black triangle, blue diamond and red square are the three coexistence points from which later the phase boundaries were obtained by Clausius–Clapeyron integration. The pink solid circle is an experimental estimate of the liquid–graphite–diamond triple point. Figure reprinted with kind perission from Ghiringhelli et al. [55]. Copyright (2005) by the American Physical Society

eling water accurately is a signiﬁcant challenge for empirical potentials, as the work of Sanz et al. [54] so nicely illustrates, the situation with carbon is by no means easier. The three phases considered in the study of Ghiringhelli and coworkers, namely graphite, diamond and the liquid phase, have markedly diﬀerent structures and types of bonding, and devising an empirical potential that is capable of reproducing not only these structural and bonding diﬀerences, but also the thermodynamic behavior of each phase, is a signiﬁcant achievement. In this study, the recently developed model of Los and Fasolino [58] was used. Ghiringhelli et al. proceeded, as in the previously discussed example of water, by ﬁrst locating coexistence points between the diﬀerent phases (graphite–diamond, graphite–liquid, and diamond–liquid), and then using Clausius–Clapeyron integration to determine the corresponding phase diagram. A portion of the phase diagram they obtained is shown in Fig. 6, where also some experimentally measured coexistence points are shown for comparison.1 The phase diagram of carbon is a challenge not only for simulation, but even more so for experiments. Indeed the melting temperature of graphite 1

Shortly after this Chapter was sent to the printer, ﬁrst principles calculations of the phase diagram of carbon were published by Wang, Scandolo and Car, [59].

134

E. R. Hern´ andez et al.

occurs well above 4000 K. The melting line of diamond has not to date been experimentally characterized. The situation is a little better for the graphite– diamond coexistence line, for which some measurements exist. As can be seen from Fig. 6, the carbon model of Los and Fasolino [58] predicts a phase diagram that agrees well with the available experimental data. In particular, the slope of the graphite–diamond coexistence curve seems to be well reproduced, although the model predicts this transition to occur at slightly higher pressures than observed experimentally. The graphite melting line occurs at somewhat lower temperatures (ca. 4000 K) than the experimental values, and is predicted to be monotonic with a slight positive pressure derivative, while it appears that the experimental curves show a maximum at around 6 GPa. It should be noticed, however, that the experimental values do not correspond to real measurements, and are in fact indirect estimations based on the ambient-pressure value [55]. A ﬁnal example that we wish to discuss is that of the phase diagram of Si obtained recently by Kaczkarski and coworkers [16]. These authors employed the tight-binding model of Lenosky et al. [14], as it is known that no empirical potential currently available predicts correctly the structure of the liquid phase in this system. The range of temperatures and pressures considered by Kaczmarski et al. encompassed four phases, namely the diamond phase, which is the stable one at ambient conditions, the liquid phase, the β-Sn structure, into which the diamond phase transforms when subject to a sufﬁcient amount of compressive pressure, and the Si36 clathrate phase, which becomes stable at negative (expansive) pressures. As in the case of C, not much experimental data exists concerning the equilibrium conditions of these phases of Si. It is known, however, that the zero-pressure melting point of the diamond phase occurs at 1687 K, and that its melting line has a negative slope, which results from the fact that the liquid phase is denser than the solid, while having a higher enthalpy. In fact, some potential models and even some tight-binding ones, fail to reproduce this behavior correctly, and would consequently produce a qualitatively wrong melting behavior, even if some of them predict the zero-pressure melting point rather accurately. In a previous study, Kaczmarski et al. [15] compared diﬀerent tight-binding models in their ability not only to accurately reproduce the melting temperature of the Si diamond phase, but also the structural properties of the liquid. The choice of the model due to Lenosky et al. for the study of the phase diagram was based on the results of that comparison. One diﬀerence between the previous examples of water and C and the work of Kaczmarski et al. [16] is that in the latter the dynamical version of the Clausius–Clapeyron integration method due to de Koning et al. was used. Also, coexistence points were located from free-energies obtained from the reversible scaling and adiabatic switching techniques. The combined use of these techniques considerably reduced the computational costs compared to what would have been required if standard thermodynamic and Clausius– Clapeyron integration had been used instead.

Free-Energies in Semiconductors

135

Fig. 7. Silicon phase diagram as predicted by the Lenosky model. The continuous and dashed black curves are calculated coexistence lines. Dashed curves indicate phase boundaries in regions where the separated phases are metastable, while continuous black curves separate thermodynamically stable phases; uncertainty bounds estimated at speciﬁc points of the phase diagram (marked by ﬁlled circles) are provided by the error bars. For comparison purposes, a schematic phase diagram summarizing the experimental data is shown with red dotted lines, and experimental data at speciﬁc temperatures and pressures is shown in the form of colored symbols. The asterisk corresponds to the zero-pressure melting point of phase I (diamond ), 1687 K [36]; the brown circle is the zero-pressure melting point of the (metastable) clathrate phase (C), at 1473 K [60]; the blue diamond is the diamond–liquid–β-Sn triple point, with estimated coordinates of 1003 ± 20 K and 10.5 ± 0.2 GPa [61]; red squares and triangles indicate the pressures at which the β-Sn phase (II) was ﬁrst observed and where the diamond phase ceased to be detected, respectively, in the experiments of Voronin et al. [61]; left and right pointing orange triangles give the same information as obtained by Hu et al. [62]; ﬁnally, the downward-pointing green triangle is the estimated diamond–clathrate–liquid triple point, at 1710 K and −2.5 GPa [60]. Figure reprinted from [16]. Copyright (2005) by the American Physical Society

Figure 7 shows the computed phase diagram for Si, compared with available experimental data. It is seen that the overall features of the phase diagram are qualitatively well reproduced by the model. In particular, the negative slope of the melting line of the diamond phase is correct, even if the actual absolute slope value is probably underestimated. The diamond–β-Sn coexistence line is also predicted to have a negative slope, though again the value seems to be smaller than the experimental one. The coexistence line between the diamond and clathrate phases is in good agreement with the only available experimental data on this transition [60].

136

E. R. Hern´ andez et al.

4 Conclusions and Outlook In this Chapter we have given an overview of recent theoretical developments in the methodology of free-energy calculations, and we have also provided a selection of applications, most of them in the ﬁeld of semiconductors, which illustrate current capabilities and provide a glimpse of what the future may bring in this topic. Many outstanding problems still remain, however, and applications in ﬁelds such as metallurgy and mineral science, particularly when variable chemical composition is involved, are still extremely challenging. We feel sure, nevertheless, that future theoretical and methodological developments will render such problems more accessible than they are at present. Acknowledgements E.R.H. and P.O. thank the Spanish Ministry of Education and Science (MEC) for funding their work through project BFM2003-03372-C03 and the bilateral Italian–Spanish collaborative action HI2003-0337; A. A. acknowledges the support from the Brazilian funding agencies FAPESP, CNPq and FAEP-UNICAMP; L. C. acknowledges ﬁnancial support under project MIUR-FIRB2001 (contract RBAU01LLX2).

References [1] D. Frenkel, B. Smit: Understanding Computer Simulation (Academic, New York 1996) 116, 126 [2] M. P. Allen, D. J. Tildesley: (Clarendon, Oxford 1987) 116 [3] J. M. Rickman, R. LeSar: Annu. Rev. Mater. Res. 32, 195 (2002) 116 [4] G. J. Ackland: J. Phys.: Condens. Matter 14, 2975 (2002) 116 [5] M. de Koning, W. P. Reinhardt: in S. Yip (Ed.): Handbook of Materials Modeling (Springer, Berlin, Heidelberg 2005) 116, 120 [6] J. G. Kirkwood: J. Chem. Phys. 3, 300 (1935) 118 [7] D. Frenkel, A. J. C. Ladd: J. Chem. Phys. 81, 3188 (1984) 118 [8] J. K. Johnson, J. A. Zollweg, K. E. Gubbins: Mol. Phys. 78, 591 (1993) 119 [9] D. A. Young, F. J. Rogers: J. Chem. Phys. 81, 2789 (1984) 119 [10] M. Watanabe, W. P. Reinhardt: Phys. Rev. Lett. 65, 3301 (1990) 119, 120, 130 [11] M. de Koning, A. Antonelli, S. Yip: Phys. Rev. Lett. 83, 3973 (1999) 120 [12] M. de Koning, A. Antonelli, S. Yip: J. Chem. Phys. 115, 11025 (2001) 122, 124 [13] C. M. Goringe, D. R. Bowler, E. R. Hern´ andez: Rep. Prog. Phys. 60, 1447 (1997) 122 [14] T. J. Lenosky, J. D. Kress, I. Kwon, A. F. Voter, B. Edwards, D. F. Richards, S. Yang, J. B. Adams: Phys. Rev. B 55, 1528 (1997) 122, 123, 134 [15] M. Kaczmarski, R. Rurali, E. R. Hern´ andez: Phys. Rev. B 69, 214105 (2004) 122, 123, 130, 134

Free-Energies in Semiconductors

137

[16] M. Kaczmarski, O. N. Bedoya-Mart´ınez, E. R. Hern´ andez: Phys. Rev. Lett. 94, 095701 (2005) 123, 134, 135 [17] D. A. Kofke: Mol. Phys. 78, 1331 (1993) 123, 132 [18] D. A. Kofke: J. Chem. Phys. 98, 4149 (1993) 123, 124, 132 [19] R. Agrawal, D. A. Kofke: Mol. Phys. 85, 43 (1995) 125 [20] A. J¨ aa ¨skel¨ ainen, L. Colombo, R. Nieminen: Phys. Rev. B 64, 233203 (2001) 125, 126, 127 [21] I. Kwon, R. Biswas, C. Z. Wang, K. M. Ho, C. M. Soukoulis: Phys. Rev. B 49, 7242 (1994) 126 [22] R. Car, P. Blochl, E. Smargiassi: Mater. Sci. Forum 83–87, 433 (1992) 126 [23] M. Tang, L. Colombo, J. Zhu, T. Diaz de la Rubia: Phys. Rev. B 55, 14279 (1997) 126 [24] H. Bracht, E. E. Haller, R. Clark-Phelps: Phys. Rev. Lett. 81, 393 (1998) 126, 127 [25] T. Y. Tan, U. G¨ osele: Appl. Phys. A: Solids Surf. 37, 1 (1985) 126, 127 [26] S. K. Estreicher, M. Garaibeh, P. A. Fedders, P. Ordej´ on: Phys. Rev. Lett. 86, 1247 (2001) 127 [27] M. Cogoni, B. P. Uberuaga, A. F. Voter, L. Colombo: Phys. Rev. B 71, 121203 (2005) 127 [28] J. Samuels, S. G. Roberts: Proc. Roy. Soc. London, Ser. A 421, 1 (1989) 128 [29] J. R. Rice: J. Mech. Phys. Solids 40, 239 (1992) 128 [30] J. R. Rice, G. E. Beltz: J. Mech. Phys. Solids 42, 333 (1994) 128 [31] Y. Sun, G. E. Beltz: Mater. Sci. Eng. A 170, 67 (1993) 128 [32] E. Kaxiras, M. S. Duesbery: Phys. Rev. Lett. 70, 3752 (1993) 128 [33] M. de Koning, A. Antonelli, M. Z. Bazant, E. Kaxiras, J. F. Justo: Phys. Rev. B 58, 12555 (1998) 128, 129 [34] J. Q. Broughton, X. P. Li: Phys. Rev. B 35, 9120 (1987) 128, 130 [35] F. H. Stillinger, T. A. Weber: Phys. Rev. B 31, 5262 (1985) 128 [36] R. Hull (Ed.): Properties of Crystalline Silicon (Inspec, London 1999) 128, 135 [37] S. J. Cook, P. Clancy: Phys. Rev. B 47, 7686 (1993) 129 [38] J. Tersoﬀ: Phys. Rev. Lett. 56, 632 (1986) 129 [39] J. Tersoﬀ: Phys. Rev. B 37, 6991 (1988) 129 [40] J. Tersoﬀ: Phys. Rev. B 38, 9902 (1988) 129 [41] M. I. Baskes, J. S. Nelson, A. F. Wright: Phys. Rev. B 40, 6085 (1989) 129 [42] O. Sugino, R. Car: Phys. Rev. Lett. 74, 1823 (1995) 130 [43] R. Car, M. Parrinello: Phys. Rev. Lett. 55, 2471 (1985) 130 [44] D. Alf`e, M. J. Gillan: Phys. Rev. B 68, 205212 (2003) 130 [45] G. A. de Wijs, G. Kresse, M. J. Gillan: Phys. Rev. B 57, 8223 (1998) 130 [46] C. R. Miranda, A. Antonelli: J. Chem. Phys. 120, 11672 (2004) 131 [47] E. P. Donovan, F. Spaepen, D. Turnbull, J. M. Poate, D. C. Jacobson: J. Appl. Phys. 57, 1795 (1985) 131 [48] S. K. Deb, M. Wilding, M. Somayazulu, P. F. McMillan: Nature 414, 528 (2001) 131 [49] S. Sastry, C. A. Angell: Nature Mater. 2, 739 (2003) 131 [50] J. F. Justo, M. Z. Bazant, E. Kaxiras, V. V. Bulatov, S. Yip: Phys. Rev. B 58, 2539 (1998) 131 [51] P. Keblinski, M. Z. Bazant, R. K. Dash, M. M. Treacy: Phys. Rev. B 66, 064104 (2002) 131

138

E. R. Hern´ andez et al.

[52] A. Hedler, S. L. Klaumunze, W. Wesch: Nature Mater. 3, 804 (2004) 131 [53] R. L. C. Vink, G. T. Barkema: Phys. Rev. Lett. 89, 076405 (2002) 131 [54] E. Sanz, C. Vega, J. L. F. Abascal, L. G. MacDowell: Phys. Rev. Lett. 92, 255701 (2004) 132, 133 [55] L. M. Ghiringhelli, J. H. Los, E. J. Meijer, A. Fasolino, D. Frenkel: Phys. Rev. Lett. 94, 145701 (2004) 132, 133, 134 [56] W. L. Jorgensen, J. Chandrasekhar, J. D. Madura, R. W. Impey, M. L. Klein: J. Chem. Phys. 79, 926 (1983) 132 [57] H. J. C. Berendsen, J. R. Grigera, T. P. Straatma: J. Phys. Chem. 91, 6269 (1987) 132 [58] J. H. Los, A. Fasolino: Phys. Rev. B 68, 024107 (2003) 133, 134 [59] X. Wang, S. Scandolo, R. Car: Phys. Rev. Lett. 95, 185701 (2005) 133 [60] P. F. McMillan: Nature Mater. 1, 19 (2002) 135 [61] G. A. Voronin, C. Pantea, T. W. Zerda, L. Wang, Y. Zhao: Phys. Rev. B 68, 020102 (2003) 135 [62] J. Z. Hu, L. D. Merkle, C. S. Menoni, I. L. Spain: Phys. Rev. B 34, 4679 (1986) 135

Index a-Si, 131 adiabatic, 119–122, 124, 130, 134 amorphous, 130, 131 anharmonic, 118, 125, 126, 128 basis set, 130 Berendsen, 132 Boltzmann, 116 bulk, 127 canonical, 116–118, 120–122 Car, 130 carbon, 132–134 classical, 116, 120 Clausius–Clapeyron, 123–125, 132–134 cluster, 127 concentration, 115, 125, 127 conﬁgurational entropy, 131 correlation, 130 coupling, 118 covalent, 129 crack, 128 density-functional theory, 128, 130 DFT, 130 diamond, 122, 133–135 diﬀusion, 126

dislocation, 128 EDIP, 131 embedded, 129 empirical, 132–134 energetics, 115 energy barrier, 128 entropy, 115, 120, 126, 131 equilibrium, 118–120, 122–125, 127, 134 exchange, 130 ﬁrst-principles, 115, 126, 127, 130 ﬂuctuation, 119 free-energy, 115–126, 128–130, 132, 134, 136 Ge, 129 general gradient approximation, 130 GGA, 130 Gibbs, 117, 122, 123, 132 glass, 130, 131 Hamiltonian, 116–120, 122 Helmholtz, 117 interface, 123 internal energy, 115, 116, 120 interstitial, 126, 127

Free-Energies in Semiconductors irreversible, 119 isothermal, 117 LDA, 130 Lennard–Jones, 119, 125 Liouville, 120 liquid, 119, 128–130, 133, 134 melting, 122, 124, 128–130, 133–135 migration, 125, 126 mobility, 126–128 molecular dynamics, 126 Parrinello, 130 partition function, 116–118, 121 periodic, 126 phase boundary, 119, 122–124 phase diagram, 119, 125, 128, 132–135 phase-space, 116, 120 population, 127 potential, 115, 116, 118, 121, 122, 125, 128–134 reversible, 116, 119, 120, 122, 124, 131, 134

139

self-diﬀusion, 125–127 self-interstitial, 125, 126 semiempirical, 122 Si, 122, 125–131, 134, 135 silicon, 126, 128, 130, 131 speciﬁc heat, 130 statistical, 116, 121 Stillinger–Weber, 128–131 stress, 128 surface, 120 temperature, 115–134 Tersoﬀ, 129 thermodynamic integration, 118, 120, 122, 124, 126, 128, 132 tight-binding, 122, 126, 127, 129, 134 trajectory, 120 transition, 119, 122, 125, 128, 131, 134, 135 vacancy, 125–127 vibrational entropy, 126 water, 130–134

Quantum Monte Carlo Techniques and Defects in Semiconductors R. J. Needs Theory of Condensed Matter Group, Cavendish Laboratory, University of Cambridge, J. J. Thomson Avenue, Cambridge, CB3 0HE, United Kingdom [email protected] Abstract. The continuum variational and diﬀusion quantum Monte Carlo (VMC and DMC) techniques are stochastic methods for obtaining expectation values of many-body wavefunctions. These methods are capable of achieving very high accuracy, yet the scaling with system size is suﬃciently favorable to allow applications to condensed-matter systems. Defects in semiconductors pose a variety of challenges to computational electronic-structure methods. As well as the large system sizes required, one is faced with calculating energy diﬀerences between rather disparate interatomic bonding conﬁgurations, and calculating excited state energies, sometimes including the energies of multiplets. Applications of VMC and DMC to defects in semiconductors are still in their infancy but, as I will describe, these methods possess features that make them well suited for addressing some important issues in the ﬁeld. In this chapter I ﬁrst discuss why we expect VMC and DMC calculations to be valuable in studying defects in semiconductors. I then review the techniques themselves, concentrating on the issues most pertinent to calculations for defects in solids. I describe recent applications to self-interstitial defects in crystalline silicon, the low-energy electronic states of the neutral vacancy in diamond, and the Schottky defect energy in magnesium oxide. The chapter ends with a perspective on the future of such studies.

1 Introduction Quantum Monte Carlo (QMC) methods in the variational (VMC) and diﬀusion (DMC) forms are stochastic methods for evaluating expectation values of many-body wavefunctions. (For a review of the VMC and DMC methods and applications to solids, see [1].) One of the main attractions of these methods is that the computational cost scales roughly as the square or cube of the number of particles, which is very favorable compared with quantumchemical many-body techniques, allowing applications to condensed-matter. Applications of QMC to defects in semiconductors are still in their infancy but, as I will describe, these methods possess features that make them well suited for addressing important issues in the ﬁeld. In this Chapter I ﬁrst discuss why we expect VMC and DMC calculations to be valuable in studying defects in semiconductors. I then review the techniques themselves, concentrating on the issues most pertinent to defects in solids. Finally, I describe recent applications to point defects in crystalline silicon, diamond and magnesium oxide, ending with a perspective on the future of such studies. D. A. Drabold, S. K. Estreicher (Eds.): Theory of Defects in Semiconductors, Topics Appl. Physics 104, 141–164 (2007) © Springer-Verlag Berlin Heidelberg 2007

142

R. J. Needs

It is important to treat electron-correlation eﬀects accurately when describing the energetics of condensed-matter systems. Defects in semiconductors are not special in this regard, but they exemplify almost all the diﬃculties that may be encountered. For example, we would like to calculate the formation and migration energies of defects. These quantities are related to the energy diﬀerences between structures, which may involve atoms with diﬀerent coordination numbers and bond lengths. We might also be interested, for example, in the properties of a 3d transition metal impurity in a semiconductor, whose electronic properties are diﬃcult to describe accurately. We may also be interested in the excited electronic states of defects, which may involve calculating the energies of multiplets. These are severe tests of electronicstructure methods, which can only be met by techniques that incorporate a sophisticated description of electronic correlation. QMC methods have the potential to provide very accurate energies and, in principle, there are no restrictions on the types of electronic state that can be treated. The N 2 − N 3 scaling of the computational cost with the number of electrons N allows applications to quite large systems, which are certainly suﬃcient for studies of defects in semiconductors. However, the prefactor is large, and a QMC calculation is generally much more expensive than the corresponding density-functional theory (DFT) one. The DMC calculations of Ceperley and Alder [2] provided accurate energies for the homogeneous electron gas, which have been used in constructing parameterized density functionals. Since then, the DMC method has been used in studies of the electrons in molecules, clusters and solids. The power of the DMC method for describing electronic correlation in large systems has been amply demonstrated by recent applications, including studies of point defects in semiconductors [3, 4], the reconstruction of the silicon (001) surface [5] and its interaction with H2 [6], and the calculation of optical excitation energies [7, 8]. The methodology of QMC calculations is being improved rapidly that, together with advances in computing technologies, will allow them to be applied to more complicated systems. I believe that QMC will play an important role in the future of electronic-structure computations. They will not replace DFT studies, but rather complement them by providing higher accuracy, albeit at considerably higher cost.

2 Quantum Monte Carlo Methods The VMC method is conceptually very simple, the energy being calculated as the expectation value of the Hamiltonian with an approximate manybody trial wavefunction. In the more sophisticated DMC method the estimate of the ground-state energy is improved by performing an evolution of the wavefunction in imaginary-time.

Quantum Monte Carlo Techniques and Defects in Semiconductors

143

2.1 The VMC Method The variational theorem of quantum mechanics states that, for a proper trial wavefunction ΨT , the variational energy, ∗ ˆ T (R) dR Ψ (R)HΨ EV = T∗ , (1) ΨT (R)ΨT (R) dR is an upper bound on the exact ground-state energy E0 , i.e., EV ≥ E0 . In (1), ΨT is the many-body wavefunction, the symbol R denotes the 3N ˆ is the many-body dimensional vector of the electron coordinates, and H Hamiltonian. The VMC method was ﬁrst used by McMillan in a study of liquid 4 He [9]. To facilitate the stochastic evaluation, EV is written as (2) EV = p(R)EL (R) dR , where the probability distribution p is p(R) =

|ΨT (R)|2 , |ΨT (R)|2 dR

(3)

and the local energy, EL , is ˆ T. EL (R) = ΨT−1 HΨ

(4)

In VMC one uses a Metropolis algorithm [10] to sample the distribution p, generating M conﬁgurations, Ri , drawn from p. The variational energy is then estimated as EV

M 1 EL (Ri ) . M i=1

(5)

Equation (2) is an importance sampling transformation of (1). Equation (2) exhibits the zero-variance property; as the trial wavefunction approaches an exact eigenfunction (ΨT → φi ), the local energy approaches the corresponding eigenenergy, Ei , everywhere in conﬁguration space. As ΨT is improved, EL becomes a smoother function of R and the number of sampling points, M , required to achieve an accurate estimate of EV is reduced. VMC is a simple and elegant method. There are no restrictions on the form of trial wavefunction that can be used and it does not suﬀer from a fermion sign problem. The main problem is, essentially, that you get out what you put in. Even if the underlying physics is well understood it is very diﬃcult to prepare trial wavefunctions of equivalent accuracy for diﬀerent systems, and therefore the energy diﬀerences between them will be biased. We use the VMC method mainly to optimize parameters in trial wavefunctions, see Sect. 2.4, and our main calculations are performed with the more sophisticated DMC method, which is described in the next section.

144

R. J. Needs

2.2 The DMC Method The DMC procedure largely overcomes the problem of bias inherent in VMC. ˆ is used to project out the ground-state In DMC the operator exp(−tH) from the initial state. This can be viewed as solving the imaginary-time Schr¨ odinger equation, ∂ ˆ − ET Φ(R, t) , (6) − Φ(R, t) = H ∂t where t is a real variable measuring the progress in imaginary-time and ET is an energy oﬀset. The solution of (6) can be obtained by expanding Φ(R, t) in the eigenstates of the Hamiltonian, ci (t)φi (R) , (7) Φ(R, t) = i

which leads to Φ(R, t) = exp[−(Ei − ET )t]ci (0)φi (R) .

(8)

i

For long times one ﬁnds Φ(R, t → ∞) exp[−(E0 − ET )t] c0 (0)φ0 (R) ,

(9)

which is proportional to the ground-state wavefunction, φ0 . If we interpret the initial state, i ci (0)φi , as a probability distribution, then the time-evolution process can be thought of as taking a set of points in conﬁguration space distributed according to the initial state and subjecting them to diﬀusion and branching (branching is also referred to as “birth” and “death” of conﬁgurations). The diﬀusion process arises from the kinetic energy operator and the branching from the potential energy. So far we have assumed that the wavefunction can be interpreted as a probability distribution, but a wavefunction for more than two identical fermions must have positive and negative regions. One can construct algorithms that use two distributions of conﬁgurations, one for positive regions and one for negative, but such algorithms suﬀer from a fermion sign problem that manifests itself by the signal-to-noise ratio decaying exponentially with imaginary-time. The ﬁxed-node approximation [11, 12] allows us to avoid these problems. This method is equivalent to placing inﬁnite potential barriers everywhere on the nodal surface of a trial wavefunction ΨT . (The nodal surface is the 3N − 1 dimensional surface in conﬁguration space on which the wavefunction is zero and across which it changes sign.) The inﬁnite potential barriers have no eﬀect if the trial nodal surface is correct, but if it is incorrect the energy is always raised. The DMC projection can then be done separately in each nodal pocket, which gives the lowest-energy solution in each pocket. It therefore follows that the DMC energy is always less than or equal to the VMC energy

Quantum Monte Carlo Techniques and Defects in Semiconductors

145

with the same trial wavefunction, and always greater than or equal to the exact ground-state energy, i.e., EV ≥ ED ≥ E0 . In addition, it turns out that all the nodal pockets of the exact fermion ground-state are equivalent [13] and, if ΨT has this tiling property, we do not need to sample all of the pockets. Such a ﬁxed-node DMC algorithm is extremely ineﬃcient and a vastly superior algorithm can be obtained by introducing an importance sampling transformation [14, 15]. Consider the mixed distribution, f (R, t) = ΨT (R)Φ(R, t) ,

(10)

which has the same sign everywhere if the nodal surface of Φ(R, t) is constrained to be the same as that of ΨT (R). Substituting in (6) for Φ we obtain 1 ∂f = − ∇2 f + ∇ · [vf ] + [EL − ET ]f , ∂t 2 where the 3N -dimensional drift velocity is deﬁned as −

(11)

v(R) = ΨT−1 (R)∇ΨT (R) .

(12)

The three terms on the right-hand side of (11) correspond to diﬀusion, drift, and branching processes, respectively. The importance sampling transformation has several consequences. First, the density of conﬁgurations is increased where ΨT is large. Second, the rate of branching is now controlled by the local energy that is generally a much smoother function than the potential energy. Finally, the importance sampling actually enforces the ﬁxed-node constraint in (11). In practice one has to use a short-time approximation (for a review of the VMC and DMC methods and applications to solids see [1]) for the Green’s function diﬀusion equation that means that occasionally conﬁgurations attempt to cross the nodal surface, but such moves are simply rejected. This algorithm generates the distribution f , but fortunately we can calculate the corresponding DMC energy using the formula f EL dR (13) ED = f dR M 1 EL (Ri ) . M i=1

(14)

The importance-sampled ﬁxed-node fermion DMC algorithm was ﬁrst used by Ceperley and Alder [2]. It is not possible to obtain directly from f the proper expectation values of operators that do not commute with the Hamiltonian, such as the chargedensity or pair-correlation functions. There are, however, three methods by which such expectation values can be obtained: the approximate (but often very accurate) extrapolation technique [16], the forward-walking technique (explained in Hammond et al. [17]) that is formally exact but statistically poorly behaved, and the reptation QMC technique of Baroni and Moroni [18], which is formally exact and well behaved, but quite expensive.

146

R. J. Needs

2.3 Trial Wavefunctions It should be clear that the trial wavefunction is of central importance in VMC and DMC calculations. The trial wavefunction introduces importance sampling and controls both the statistical eﬃciency and the accuracy obtained. In DMC the accuracy depends only on the nodal surface of the trial wavefunction via the ﬁxed-node approximation, while in VMC it depends on the entire trial wavefunction, so that VMC energies are more sensitive to the quality of the approximate wavefunction than DMC energies. QMC calculations require a compact trial wavefunction, and most studies of electronic systems have used the Slater–Jastrow form, in which a pair of up- and down-spin determinants is multiplied by a Jastrow correlation factor, ΨT = eJ(R) D↑ (R↑ )D↓ (R↓ ) ,

(15)

where eJ is the Jastrow factor and the D are determinants of single-particle orbitals. The quality of the single-particle orbitals is very important, and they are often obtained from DFT or Hartree–Fock (HF) calculations. The Jastrow factor is a positive, symmetric, function of the electron coordinates, which is chosen to be small when electrons are close to one another, thereby introducing electron-correlation into the wavefunction. The Jastrow factor is also used to enforce the electron–electron Kato cusp conditions [19]. The idea is that when two electrons are coincident the contribution to the local energy from the Coulomb interaction diverges, and therefore the exact wavefunction must have a cusp at this point so that the kinetic energy operator supplies an equal and opposite divergence. It seems very reasonable to enforce these conditions on a trial wavefunction as they are obeyed by the exact wavefunction, and in VMC, and more particularly DMC, calculations they are very important because divergences in the local energy can lead to poor statistical behavior. Many excellent QMC results have been obtained using Slater–Jastrow wavefunctions, but it may be proﬁtable to consider other forms. One variant is to use more than one pair of determinants, αi Di,↑ (R↑ )Di,↓ (R↓ ) , (16) ΨT = eJ(R) i

where the αi are coeﬃcients. This approach is not suitable for improving the energy per atom of a solid because the number of determinants required would have to increase exponentially with system size. It is, however, useful when considering a point defect with an open-shell electronic conﬁguration in a solid, in which case the electronic states of the multiplet may be described by a small number of determinants. An example of this is described in Sect. 6.3. Another possibility is to include backﬂow correlations, which may be derived by demanding that the wavefunction conserves the local current [20]. This approach has been used successfully in QMC studies of the

Quantum Monte Carlo Techniques and Defects in Semiconductors

147

electron gas [21], but it has not been explored much for electrons in real atomic systems [22]. Including backﬂow correlations improves the nodal surface of a wavefunction and leads to a compact form that is suitable for use in QMC calculations, although it is more complicated than the Slater–Jastrow form and the computational cost is increased. 2.4 Optimization of Trial Wavefunctions Optimizing trial wavefunctions is perhaps the most important technical issue in QMC calculations, and it consumes large amounts of human and computing resources. It is standard to include a number of variable parameters in the Jastrow factor whose values are determined by a stochastic optimization procedure. The determinant coeﬃcients, αi , in (16) may also be optimized, and in some calculations the orbitals themselves have been optimized. Developing better wavefunction-optimization techniques is currently a very active ﬁeld, with many new approaches being tested. Rather than delving into the technical details of this enterprise, I will mention some of the key issues. Ideally the wavefunction should be optimized within DMC, but this is generally much too costly and so optimizations are performed at the VMC level. Two measures of wavefunction quality have generally been considered. The most obvious idea is to minimize the expectation value of the VMC energy, although more commonly the variance of the VMC energy has been minimized. There are good reasons to suppose that better DMC results would be obtained by using energy-minimized trial wavefunctions, rather than variance-minimized ones. First, it seems likely that a better nodal surface would be obtained by minimizing the energy rather than the variance. Second, it turns out that the variance of the DMC energy is approximately proportional to the diﬀerence between the VMC and DMC energies, rather than the variance of the VMC energy [23]. Why then has it been more common to minimize the variance of the VMC energy? The answer is simply that it has proved easier to devise algorithms for minimizing the variance that are stable and eﬃcient in the presence of statistical noise [24–26]. Most of the current eﬀort is being devoted to developing energy-minimization schemes, although the applications to defects in semiconductors described in this Chapter were performed using variance minimization. 2.5 QMC Calculations within Periodic Boundary Conditions QMC calculations for defects in solids may be performed using cluster models or periodic boundary conditions, just as in other techniques. Periodic boundary conditions are preferred because they give smaller ﬁnite-size eﬀects. In the standard supercell approach a point defect in an otherwise perfect crystal is modeled by taking a large cell containing a single defect and repeating it throughout space. Just as in other techniques, one must ensure that the

148

R. J. Needs

supercell is large enough for the interactions between defects in diﬀerent supercells to be small. In techniques involving many-electron wavefunctions such as QMC it is not possible to reduce the problem to solving within a primitive unit cell (when a defect is present the primitive unit cell is the supercell). Such a reduction is allowed in single-particle methods because the Hamiltonian is invariant under the translation of a single electronic coordinate by a translation vector of the primitive lattice, but this is not a symmetry of the manybody Hamiltonian. Consequently QMC calculations may be performed only at a single k-point. It is possible to perform QMC calculations at diﬀerent k-points [27, 28] and average the results [29], but this is not exactly equivalent to a Brillouin-zone integration within single-particle theories. In the applications described in this Chapter a single k-point was used. Many-body techniques such as QMC also suﬀer from another source of ﬁnite-size eﬀects – the interaction of the electrons with their periodic images. Such an eﬀect is absent in local DFT calculations because the interaction energy is written in terms of the electronic charge density, but the eﬀect is present in HF calculations. These “Coulomb ﬁnite-size eﬀects” are often corrected for using extrapolation techniques (see [1] and references therein), and they may also be reduced using the so-called model periodic Coulomb (MPC) interaction [30]. 2.6 Using Pseudopotentials in QMC Calculations The cost of a DMC calculation increases rapidly with the atomic number, Z, as roughly Z 5.5 [23, 31]. This eﬀectively rules out applications to atoms with Z greater than about 10, and consequently pseudopotentials are commonly used in DMC calculations. The use of nonlocal pseudopotentials within VMC is quite straightforward, but DMC poses an additional problem, because the matrix element of the imaginary-time propagator is not necessarily positive, which leads to a sign problem analogous to the fermion sign problem. To circumvent this diﬃculty an additional approximation known as the pseudopotential localization approximation has been used [32]. If the trial wavefunction is accurate the error introduced by the localization approximation is small and is proportional to (ΨT − φ0 )2 [33], although the error term can be of either sign. Recently, Casula et al. [34] have introduced a fully variational technique for dealing with nonlocal pseudopotentials within DMC. Currently it is not possible to generate pseudopotentials entirely within a QMC framework, and therefore they are obtained from other sources. There is evidence that indicates that HF theory provides better pseudopotentials than DFT for use within QMC calculations [35], and recently we have developed smooth relativistic HF pseudopotentials for H to Ba and Lu to Hg that are suitable for use in QMC calculations [36, 37].

Quantum Monte Carlo Techniques and Defects in Semiconductors

149

3 DMC Calculations for Excited States It might appear that the DMC method cannot be applied to excited states because the imaginary-time propagation would evolve it towards the groundstate. However, the ﬁxed-node constraint ensures convergence to the lowestenergy state compatible with the nodal surface of the trial wavefunction. If the nodal surface is exactly that of an eigenstate then DMC gives the exact energy of that state. If the nodal surface is approximately that of an excitedstate then the DMC energy gives an approximation to the energy of that excited state. There is, however, an important diﬀerence from the groundstate case, in that the existence of a variational principle for the energy of an excited-state depends on the symmetry of the trial wavefunction [38]. In practice, DMC works quite well for excited-states [39, 40].

4 Sources of Error in DMC Calculations Here we summarize the potential sources of errors in DMC calculations. – Statistical error. The standard error in the mean is proportional to √ 1/ M , where M is the number of moves. It therefore costs a factor of 100 in computer time to reduce the error bars by a factor of 10. On the other hand, a random error is much better than a systematic one. – The ﬁxed-node error. This is the central approximation of the DMC technique, and is often the limiting factor in the accuracy of the results. – Timestep bias. The short-time approximation leads to a bias in the f distribution and hence in expectation values. This bias can be serious and is often corrected for by using several diﬀerent timesteps and extrapolating to zero timestep. – Population control bias. In DMC the f distribution is represented by a ﬁnite population of conﬁgurations that ﬂuctuates due to the branching procedure. The population is usually controlled by occasionally changing the trial energy, ET , in (11) so that the population returns towards a target size. This procedure results in a population-control bias. In practice, the population control bias is normally extremely small, in fact so small that it is diﬃcult to detect. – Pseudopotential errors including the localization error. Pseudopotentials inevitably introduce errors that can be signiﬁcant in some cases. The localization error also appears to be quite small, although this has not been tested in many cases. – Finite-size errors within periodic boundary conditions. It is important to study the ﬁnite-size eﬀects carefully, and to correct for them. A number of correction procedures have been devised, mainly involving extrapolation to the thermodynamic limit.

150

R. J. Needs

In electronic-structure theory one is almost always interested in the diﬀerence in energy between two similar systems. All electronic-structure methods for complex systems rely on large cancelations of the errors in the energy differences between systems. In DMC this helps with all the above sources of error except the statistical errors. Fixed-node errors tend to cancel because the DMC energy is an upper bound, but even though DMC often retrieves 95 % or more of the correlation energy, noncancelation of nodal errors is a severe problem for DMC calculations. As mentioned before, the most straightforward way forward is simply to improve the quality of the trial wavefunctions, but perhaps it might also be possible to balance the errors in diﬀerent systems more successfully than is currently possible.

5 Applications of QMC to the Cohesive Energies of Solids A number of VMC and DMC studies have been performed of the cohesive energies of solids. The cohesive energy is calculated as the energy diﬀerence between the isolated atom and an atom in the solid. This is a severe test of QMC methods because the trial wavefunctions used for the atom and solid must be closely matched in quality. Data for Si [30], Ge [28], C [4], Na [41] and NiO [42] have been collected in Table 1. The local spin density approximation (LSDA) data shows the standard overestimation of the cohesive energy, while the QMC data is in good agreement with experiment. These studies have been important in establishing DMC as an accurate method for calculating the energies of solids. Table 1. LSDA, VMC and DMC cohesive energies of solids in eV per atom (eV per 2 atoms for NiO), compared with the experimental values. The numbers in brackets indicate standard errors in the last signiﬁcant ﬁgure. All calculated values contain a correction for the zero-point energy of the solid Method

Si

Ge

C

Na

NiO

LSDA VMC DMC Exp.

5.28 4.48(1) 4.63(2) 4.62

4.59 3.80(2) 3.85(2) 3.85

8.61 7.36(1) 7.346(6) 7.37

1.20 0.9694(8) 1.0221(3) 1.13

10.96 8.57(1) 9.442(2) 9.45

Quantum Monte Carlo Techniques and Defects in Semiconductors

151

6 Applications of QMC to Defects in Semiconductors 6.1 Using Structures from Simpler Methods In the applications of QMC to defects in semiconductors reported to date, the structures were obtained from DFT calculations and the energies recalculated within QMC. Surely this leads to a bias in the energy diﬀerences that might be considerable? The answer must certainly be yes, it does lead to a bias, but here I argue that it may often be quite small. We can pose the question more clearly as “is it sensible to calculate structures using a simple method of limited accuracy and then recalculate the energy diﬀerence between the structures with a sophisticated method of much higher accuracy?”. Consider a system with a single structural coordinate Q, and suppose there are two structures of interest, denoted by 1 and 2, corresponding to local minima in the energy at coordinates Q1 and Q2 , with energies E1 and E2 . Around the two energy minima the energy can be expanded as Around Q1

E(Q) = E1 + α1 (Q − Q1 )2

(17)

Around Q2

E(Q) = E2 + α2 (Q − Q2 ) .

(18)

2

Suppose further that we have a simple method for calculating the energy E(Q) that gives a smoothly varying error of the form ∆E(Q) = βQ ,

(19)

where β is a constant. Within the simple method the errors in the coordinates of the equilibrium structures are obtained by minimizing E + ∆E, which gives ∆Q1 = −

β , 2α1

∆Q2 = −

β , 2α2

and the error in the energy diﬀerence between these structures is β2 1 1 ∆(E1 − E2 ) = β(Q1 − Q2 ) − − . 4 α1 α2

(20)

(21)

Now suppose that we use the structures from the simple method, but recalculate the energies within a sophisticated method that gives a negligible error in the energy. The error in the energy diﬀerence between the structures is then β2 1 1 . (22) − ∆(E1 − E2 ) = 2 α1 α2 Within the simple method the error in the energy diﬀerence is ﬁrst order in β, while for the sophisticated method it is second order. The error in

152

R. J. Needs

Fig. 1. The energy E versus a structural coordinate Q showing two minima for a model system. Solid line: exact energy, dashed line: approximate energy from a simple theory that has an error of 0.1Q. The error in the energy diﬀerence between the two minima obtained from the simple theory is 0.186, while the error in the energy diﬀerence calculated using the accurate energy curve, but evaluated at the minima obtained from the simple theory, is 0.000 45

the energy diﬀerence within the simple method is proportional to Q1 − Q2 , so that the error is large if the structures are very diﬀerent, while in the sophisticated method the error is independent of Q1 − Q2 . This behavior is illustrated in Fig. 1. We therefore conclude that using the sophisticated method to calculate the energy diﬀerence between structures obtained from the simple method leads to only quite small errors. Note also that within this model the quadratic coeﬃcients in the energy, α1 and α2 , are unaltered by the linear error term, so that the simple method gives accurate values for the vibrational frequencies. The model is, of course, highly simpliﬁed, but it illustrates my contention that it is reasonable to take structures from DFT calculations and recalculate the energy diﬀerences between them within QMC. 6.2 Silicon Self-Interstitial Defects The diﬀusion of dopant impurity atoms during thermal processing limits how small silicon devices can be made, and understanding this eﬀect requires a knowledge of diﬀusion on the microscopic scale in situations far from equilibrium. Dopant diﬀusion is mainly controlled by the presence of intrinsic defects such as self-interstitials and vacancies, and therefore it is important to improve our understanding of these defects. Both experimental and theoretical techniques have been brought to bear on these defects but, unfortunately, it has not been possible to detect silicon self-interstitials directly and we must rely on theoretical studies to elucidate

Quantum Monte Carlo Techniques and Defects in Semiconductors

153

their microscopic properties. Electron paramagnetic resonance studies [43] have determined unambiguously that the symmetry of neutral vacancies in silicon is D2d , which is consistent with a Jahn–Teller distortion. Positronlifetime experiments have given a value for the enthalpy of formation of a neutral vacancy in silicon of 3.6 ± 0.2 eV [44]. The self-diﬀusivity of silicon at high temperatures follows an Arrhenius behavior with an activation energy in the range 4.1 eV to 5.1 eV [45]. Signiﬁcant diﬃculties arise with the interpretation of experimental data when the contributions to the self-diﬀusivity from diﬀerent mechanisms are considered. The self-diﬀusivity is usually written as the sum of contributions from independent diﬀusive mechanisms. The contribution of a particular microscopic mechanism can be written as the product of the diﬀusivity, Di , and the concentration, Ci , of the relevant defect, i.e., Di Ci . (23) DSD = i

G¨ osele et al. [46] give estimates of the contributions to the self-diﬀusivity as DI CI = 914 exp(−4.84/kB T ) cm2 · s−1 ,

(24)

from self-interstitials and DV CV = 0.6 exp(−4.03/kBT ) cm2 · s−1 ,

(25)

from vacancies, where kB T is in units of eV. It is believed that self-diﬀusivity in silicon is dominated by vacancies at low temperatures and self-interstitials above 1300 K. The experimental situation regarding the individual values of Di and Ci is, however, controversial. Indeed, experimental data has been used to support values of the diﬀusivity of the silicon self-interstitial, DI , which diﬀer by ten orders of magnitude at the temperatures of around 1100 K at which silicon is processed [47]. The main challenge to theory is to identify the important defects and to predict their properties, comparing with experimental data where available. This includes identifying the diﬀusive mechanisms of the defects, providing accurate values for the Di and the equilibrium values of Ci , and reproducing the experimental data for the self-diﬀusivity. This programme represents an enormous challenge, and although many theoretical studies of point defects in silicon have been performed, the goal is still far away. A number of diﬀerent structures for silicon self-interstitials have been postulated, including the split-110, hexagonal and tetrahedral defects, see Fig. 2. The consensus view from modern DFT calculations is that the split110 and hexagonal structures are the lowest-energy self-interstitials in silicon [48–50], and that the tetrahedral interstitial is unstable. However, even here there has been a surprise. Recent DFT calculations have shown that the hexagonal interstitial is unstable to a distortion out of the hexagonal ring by

154

R. J. Needs

0.48 ˚ A, which lowers the formation energy by 0.03 eV [50]. Another surprise has been that, within DFT, it turns out that the lowest-energy point defect in silicon is neither an interstitial nor the vacancy! Goedecker et al. [49] found that a fourfold coordinated defect (FFCD) had a formation energy at least 0.5 eV lower than the interstitials and vacancy. It is not clear whether this defect could play a role in self-diﬀusion, as its possible diﬀusive mechanisms have not yet been studied. There are some discrepancies between DFT values reported for the formation energies of the split-110 and hexagonal self-interstitials and for the associated migration energies. However, modern calculations [48–50] indicate that the sum of the DFT formation and migration energies is signiﬁcantly smaller than the exponent of 4.84 eV deduced from experimental studies, see (24). An interesting suggestion by Pandey and coworkers [51, 52], based on the results of DFT calculations, was that an exchange of neighboring atoms in the perfect lattice atoms would contribute to self-diﬀusion in silicon. In Pandey’s concerted exchange mechanism two nearest-neighbor atoms interchange via a complicated 3-dimensional path that allows the atoms to avoid large energy barriers [51, 52]. One of the main planks of Pandey’s argument was that the calculated value for the activation energy for this concerted exchange was within the experimental range for self-diﬀusion of 4.1 eV to 5.1 eV [45]. However, as we have already noted, DFT gives even lower energies for interstitials and vacancies, and therefore Pandey’s argument is unsatisfactory. All of the calculations mentioned so far assumed no thermal motion at all, but it is also important, of course, to study ﬁnite-temperature eﬀects. Two DFT molecular dynamics studies have been reported [53, 54], but the energy barriers to interstitial self-diﬀusion are very small (at least within DFT) and highly accurate calculations are required to obtain reliable results. It is rather easier to calculate the equilibrium concentration of defects including the effects of thermal vibrations, and a recent study [50] using DFT perturbation theory gave results that are broadly in agreement with the rather scattered experimental data. Given this background, what role can QMC calculations play in unravelling this complicated problem? In the medium term its role must be to give accurate values for the energies of various defect structures. Given that the LSDA and generalized gradient approximation (GGA) self-interstitial defectformation energies can diﬀer by 0.5 eV it is valuable to quantify the errors in DFT calculations of the defect formation energies. As argued in Sect. 6.1, it should be suﬃcient to use defect structures obtained from DFT calculations for this purpose. 6.2.1 DFT Calculations on Silicon Self-Interstitials Leung et al. [3] and Needs [48] reported LSDA and PW91-GGA results for various interstitial defect formation energies and the saddle point of Pandey’s

Quantum Monte Carlo Techniques and Defects in Semiconductors

155

Fig. 2. The structures of the split-110, hexagonal, and tetrahedral interstitial defects, the saddle point of the concerted-exchange mechanism, and the perfect silicon crystal. After Needs [48]

concerted-exchange mechanism, see Table 2. This work also indicated that the LSDA and PW91-GGA equilibrium defect structures are very similar. One of the features of the various defect structures is the wide range of interatomic bonding they exhibit. In the split-110 structure the two atoms forming the defect are fourfold coordinated, but two of the surrounding atoms are ﬁvefold coordinated. The hexagonal interstitial is sixfold coordinated and its six neighbors are ﬁvefold coordinated. The tetrahedral interstitial is fourfold coordinated and has four neighbors, which are therefore ﬁvefold coordinated. At the saddle point of Pandey’s concerted exchange two bonds are broken so that the exchanging atoms and two other atoms are ﬁvefold coordinated. The DFT energy barriers to diﬀusive jumps between the low-energy structures were calculated, which gave a path for split-110-hexagonal diﬀusion with a barrier of 0.15 eV (LDA) and 0.20 eV (PW91-GGA), and a barrier for hexagonal–hexagonal diﬀusive jumps of 0.03 eV (LDA) and 0.18 eV (PW91GGA).

156

R. J. Needs

Table 2. LDA, PW91-GGA, and DMC formation energies in eV of the selfinterstitial defects and the saddle point of the concerted-exchange mechanism. a 16atom supercell, b 54-atom supercell Defect

LDA

GGA

DMCa

DMCb

Split-110 Hexagonal Tetrahedral Concerted exchange

3.31 3.31 3.43 4.45

3.84 3.80 4.07 4.80

4.96(24) 4.70(24) 5.50(24) 5.85(23)

4.96(28) 4.82(28) 5.40(28) 5.78(27)

6.2.2 QMC Calculations on Silicon Self-Interstitials The DMC calculations were performed for 16- and 54-atom fcc structures obtained from LDA calculations. The Slater–Jastrow trial wavefunctions were formed from determinants of LDA orbitals and Jastrow factors containing up to 64 parameters, whose optimal values were obtained by minimizing the variance of the energy. The DMC defect-formation energies are shown in Table 2. Note that the DMC results for the 16- and 54-atom simulation cells are consistent, indicating that the residual ﬁnite-size eﬀects are small. The clearest conclusion is that the DMC formation energies are roughly 1 eV larger than the PW91GGA values and 1.5 eV larger than the LDA values. The hexagonal interstitial has the lowest formation energy within DMC, while the split-110 interstitial is slightly higher in energy, and the tetrahedral interstitial has a considerably higher energy. The saddle point of the concerted exchange has an energy that is too high to explain self-diﬀusion in silicon. Calculating the energy barriers to diﬀusion within DMC is currently prohibitively expensive, but they can be roughly estimated as follows. The tetrahedral interstitial is a saddle point of a possible diﬀusion path between neighboring hexagonal sites. The DMC formation energy of 5.4 eV for the tetrahedral interstitial is therefore an upper bound to the formation plus migration energy of the hexagonal interstitial. The true formation plus migration energy is expected to be less than this. Within the LDA there is a diﬀusion path for the hexagonal interstitial with a barrier of only 25 % of the tetrahedralhexagonal energy diﬀerence. Applying the same percentage reduction to the DMC barrier then gives an estimate of the formation plus migration energy of the hexagonal interstitial of 5 eV. This estimate is in good agreement with the experimental activation energy for self-interstitial diﬀusion of 4.84 eV [46]. This study demonstrated the importance of a proper treatment of electron correlation when calculating defect-formation energies in silicon. DFT predicts formation plus migration energies that are smaller than those deduced from experiment. The larger defect-formation energies found in the DMC calculations indicate a possible resolution of this problem, which might be an important step in improving our understanding of self-diﬀusion in silicon.

Quantum Monte Carlo Techniques and Defects in Semiconductors

157

6.3 Neutral Vacancy in Diamond The vacancy in diamond is a dominant defect associated with radiation damage, and it exhibits a wider variety of physical phenomena than its counterpart in silicon. Self-diﬀusion in diamond is relevant to growing single-crystal diamond thin ﬁlms on nondiamond substrates. DFT studies have suggested that self-diﬀusion in diamond is dominated by vacancies [55] and that interstitials do not play a signiﬁcant role. A vacancy may be formed by removing an atom, leaving four danglingbonds. The simplest model of the electronic structure of a vacancy is a oneelectron molecular defect picture in which symmetry-adapted combinations of the four dangling-bond states have a1 and t2 symmetry. These levels are, respectively, singly and triply degenerate. In the neutral defect four electrons are placed in the dangling-bond states, giving a a21 t22 conﬁguration. This system is unstable to Jahn–Teller distortion and a spontaneous reduction in symmetry occurs in which the t2 states split into a doubly occupied a1 and empty e state, and a structure with D2d symmetry results. This model is appropriate for the vacancy in silicon but, because of the large electron–electron interaction eﬀects, not for diamond. The prominent GR1 optical transition at 1.673 eV [56] is associated with the neutral vacancy. Uniaxial stress perturbations show that the GR1 transition is between a ground state that is orbitally doubly degenerate with symmetry E and an orbitally triply degenerate excited-state of T symmetry [57]. Both the ground and excited-states undergo Jahn–Teller relaxations, but the eﬀects are dynamic during absorption and the vacancy therefore appears to maintain the Td point group of an atomic site in diamond [58]. Correlation eﬀects among the electrons in the dangling-bonds are very important, but the strong coupling to the solid-state environment must also be included. The electronic states of the defect form a multiplet requiring a multideterminant description [59, 60]. The GR1 optical transition cannot be expressed as a transition between one-electron states, which makes a ﬁrst-principles approach very diﬃcult. For example, approaches based on one-electron states, such as Kohn–Sham DFT or the GW self-energy approach [61, 62], cannot give a full description of the multiplet structure. Von Barth has suggested an approximate scheme for obtaining multiplet energies from DFT calculations [63], but unfortunately this scheme does not permit the calculation of the energy of what is believed to be the excited-state of the GR1 band [64, 65]. QMC appears to be an ideal method for this problem, as one can use a multideterminant description of the defect states while maintaining the favorable scaling with system size. 6.3.1 VMC and DMC Calculations on the Neutral Vacancy in Diamond Hood et al. [4] performed VMC and DMC calculations of the neutral vacancy in diamond using periodic boundary conditions and a simulation cell

158

R. J. Needs

containing 53 atoms. The relaxed ionic positions were obtained from an LSDA calculation in which each of the t2 states was fractionally occupied. The nearest-neighbor atoms of the vacancy were found to relax outwards by 0.1 ˚ A, while the relaxation of the next nearest neighbors was negligible. The trial wavefunctions were of the Slater–Jastrow type with the singleparticle orbitals obtained from an LSDA calculation using a Gaussian basis set. To calculate the multiplet structure of the electronic states of the vacancy, symmetrized multideterminants were used with the conﬁguration in which the a1 states were fully occupied and the t2 states were doubly occupied. This gives rise to 1 A1 , 1 E, 1 T2 , and 3 T1 states, with orbital degeneracies of 1, 2, 3, 3, respectively. The corresponding trial wavefunctions took the form, Ψ1 A1 = eJ(R) D↑x D↓x + D↑y D↓y + D↑z D↓z (26) Ψ1 E = eJ(R) 2D↑x D↓x − D↑y D↓y − D↑z D↓z (27) (28) Ψ1 T2 = eJ(R) D↑y D↓z − D↑z D↓y Ψ3 T1 = eJ(R) D↑yz D↓ .

(29)

In this notation, the superscripts x, y, z label which of the t2 orbitals are included in the determinant, in addition to the a1 and lower-energy orbitals. The values of the parameters in the Jastrow factors were optimized by minimizing the variance of the local energy [24, 25]. Figure 3 shows the DMC energies of the states obtained by Hood et al. [4]. The 1 E state was found to be the ground-state, in agreement with experiment. The state with the lowest-energy electronic excitation from the groundstate that is spin and orbitally dipole allowed was the 1 T2 state, and these states are identiﬁed as giving rise to the GR1 line. The associated DMC transition energy was calculated to be 1.51(34) eV, which lie within the statistical error bars of the experimental value of 1.673 eV. The vacancy-formation energy was calculated to be 6.98 eV within the LSDA, and 5.96(34) eV within DMC. Both of these values include a correction for the Jahn–Teller relaxation energy of the vacancy, which is estimated to be 0.36 eV [64]. The DMC formation energy indicates that it is approximately one eV more favorable to form a neutral vacancy in diamond than predicted by the LSDA. The vacancy-formation energy in diamond has yet to be measured. 6.4 Schottky Defects in Magnesium Oxide Alf`e and Gillan [66] recently used DMC to study the Schottky defect formation energy in MgO. Although MgO is classiﬁed as an insulator rather than a semiconductor, these calculations illustrate very nicely the methodology that can be used to calculate the energetics of charged defects within QMC.

Quantum Monte Carlo Techniques and Defects in Semiconductors

159

Fig. 3. DMC energy diﬀerences from the ground-state in eV with statistical errors for the lowest-symmetry states of the neutral vacancy in diamond. The dotted arrow indicates the lowest spin and orbitally dipole allowed transition. After Hood et al. [4]

Oxide materials are, of course, of great importance as insulating layers in semiconductor devices. The Schottky defect energy of MgO is deﬁned to be the energy change when a Mg2+ and an O2− ion are removed from a perfect MgO crystal, the ions being replaced to form an additional unit cell of perfect crystal. The Schottky defect energy, ES , governs the concentration of vacancies present in thermal equilibrium. The methodology used for calculating ES follows that used in DFT calculations. One way to model the Schottky defect would be to remove an Mg atom and an O atom from a large supercell, but in electronic-structure calculations it is normally preferable to study supercells containing only a single defect, because otherwise the interactions between the defects would be large. Consider a crystal containing N cation and N anion sites. Let EN (ν + , ν − ) denoted the total energy of a crystal containing ν + cation vacancies and ν − anion vacancies. The Schottky defect energy is then ES = EN (1, 0) + EN (0, 1) −

2(N − 1) EN (0, 0) . N

(30)

The systems with a single Mg2+ vacancy and a single O2− vacancy were modeled by supercells subject to periodic boundary conditions. These supercells would each carry a net charge, in which case the electrostatic energy of the system cannot be deﬁned, and therefore an appropriate uniform background charge was added to each supercell to make them charge neutral. In the limit of large N the presence of the uniform background charges makes no diﬀerence to ES . In reality, a ﬁnite value of N must be used, which introduces ﬁnite-size errors. The ﬁnite-size error due to the interaction between the periodic images of the defects was corrected for by a standard method [67]. The DMC calculations used N = 27, i.e., 53 atoms for the defective crystals and 54 for the perfect crystals, and the relaxed atomic positions were

160

R. J. Needs

obtained from LSDA calculations. Slater–Jastrow wavefunctions were used, with orbitals obtained from plane-wave LSDA calculations, and optimized Jastrow factors. For eﬃcient evaluation within the QMC calculations the orbitals were re-expanded in a basis of B-splines or “blips”, which are functions that are strongly localized in real space [68]. The DMC calculations gave ES = 7.5 ± 0.53 eV, while equivalent LSDA calculations using the same pseudopotentialand cell size gave ES = 6.99 eV, and a highly converged LSDA calculation gave ES = 6.76 eV. It is very diﬃcult to measure the Schottky defect energy, but it is estimated to lie within the range 4 eV to 7 eV.

7 Conclusions QMC techniques provide a uniﬁed treatment of both the ground- and excited-state energies of correlated electron systems. They are therefore widely applicable and hold great promise as a computational method to enhance our understanding of defects in solids. Considering that QMC is very costly, there seems little point in using it unless the results are reliably more accurate than those obtained from less costly methods such as DFT. The pursuit of higher accuracy in QMC calculations is, in my opinion, the most important practical issue facing today’s practitioners. Very high accuracy has already been demonstrated for small systems, but the situation for larger systems is less clear. I believe that many careful studies are required before we can conﬁdently assert that QMC techniques reliably achieve highly accurate results for complicated systems such as defects in semiconductors. QMC techniques are currently in a phase of rapid development. The most challenging problem in fermion QMC is the infamous fermion sign problem. Solving the sign problem is certainly extremely diﬃcult and perhaps impossible [69]. It is thought that exact fermion methods that avoid the sign problem will be exponentially slow on a classical computer. However, it is clear that QMC methods can deliver highly accurate results provided the trial wavefunctions are accurate enough. It is important to appreciate that trial wavefunctions can be improved using optimization techniques, whereas improving DFT results requires the development of better density functionals, which seems likely to be a much harder problem. Another important issue is that currently it is not possible to calculate accurate atomic forces within QMC for large systems, and therefore it is not possible to relax defect structures. So far this problem has been avoided by using relaxed structures obtained from DFT calculations. The problem of calculating accurate forces within QMC for large systems is unlikely to be insurmountable, and I believe that a satisfactory solution will be developed in due course. Although QMC methods have a long way to go before they are routinely applied to defects

Quantum Monte Carlo Techniques and Defects in Semiconductors

161

in semiconductors I hope that I have persuaded the reader that such a goal is both desirable and possible. I have discussed applications of the DMC method to self-interstitials in silicon, the neutral vacancy in diamond and Schottky defects in magnesium oxide. These studies have demonstrated the feasibility of DMC studies of defects in semiconductors, and have already produced interesting results that challenge those from other methods. Acknowledgements I would like to thank all of my collaborators who have contributed so much to our QMC project. Much of this work has been supported by the Engineering and Physical Sciences Research Council (EPSRC), UK.

References [1] W. M. C. Foulkes, L. Mitas, R. J. Needs, G. Rajagopal: Rev. Mod. Phys. 73, 33 (2001) 141, 145, 148 [2] D. M. Ceperley, B. J. Alder: Phys. Rev. Lett. 45, 566 (1980) 142, 145 [3] W.-K. Leung, R. J. Needs, G. Rajagopal, S. Itoh, S. Ihara: Phys. Rev. Lett. 83, 2351 (1999) 142, 154 [4] R. Q. Hood, P. R. C. Kent, R. J. Needs, P. R. Briddon: Phys. Rev. Lett. 91, 076403 (2003) 142, 150, 157, 158, 159 [5] S. B. Healy, C. Filippi, P. Kratzer, E. Penev, M. Scheﬄer: Phys. Rev. Lett. 87, 016105 (2001) 142 [6] C. Filippi, S. B. Healy, P. Kratzer, E. Pehlke, M. Scheﬄer: Phys. Rev. Lett. 89, 166102 (2002) 142 [7] A. J. Williamson, J. C. Grossman, R. Q. Hood, A. Puzder, G. Galli: Phys. Rev. Lett. 89, 196803 (2002) 142 [8] N. D. Drummond, A. J. Williamson, R. J. Needs, G. Galli: Phys. Rev. Lett. 95, 096801 (2005) 142 [9] W. L. McMillan: Phys. Rev. A 138, 442 (1965) 143 [10] N. Metropolis, A. W. Rosenbluth, M. N. Rosenbluth, A. H. Teller, E. Teller: J. Chem. Phys. 21, 1087 (1953) 143 [11] J. B. Anderson: J. Chem. Phys. 63, 1499 (1975) 144 [12] J. B. Anderson: J. Chem. Phys. 65, 4121 (1976) 144 [13] D. M. Ceperley: J. Stat. Phys. 63, 1237 (1991) 145 [14] R. C. Grimm, R. G. Storer: J. Comput. Phys. 7, 134 (1971) 145 [15] M. H. Kalos, D. Levesque, L. Verlet: Phys. Rev. A 9, 257 (1974) 145 [16] D. M. Ceperley, M. H. Kalos: Monte Carlo Methods in Statistical Physics (Springer, Berlin, Heidelberg 1979) pp. 145–194 145 [17] B. L. Hammond, W. A. Lester, Jr., P. J. Reynolds: Monte Carlo Methods in ab initio Quantum Chemistry (World Scientiﬁc, Singapore 1994) 145 [18] S. Baroni, S. Moroni: Phys. Rev. Lett. 82, 4745 (1999) 145 [19] T. Kato: Comm. Pure Appl. Math. 10, 151 (1957) 146 [20] R. P. Feynman, M. Cohen: Phys. Rev. 102, 1189 (1956) 146

162

R. J. Needs

[21] Y. Kwon, D. M. Ceperley, R. M. Martin: Phys. Rev. B 58, 6800 (1998) 147 [22] M. Holzmann, D. M. Ceperley, C. Pierleoni, K. Esler: Phys. Rev. E 68, 046707 (2003) 147 [23] D. M. Ceperley: J. Stat. Phys. 43, 815 (1986) 147, 148 [24] C. J. Umrigar, K. G. Wilson, J. W. Wilkins: Phys. Rev. Lett. 60, 1719 (1988) 147, 158 [25] P. R. C. Kent, R. J. Needs, G. Rajagopal: Phys. Rev. B 59, 12344 (1999) 147, 158 [26] N. D. Drummond, R. J. Needs: Phys. Rev. B 72, 085124 (2005) 147 [27] G. Rajagopal, R. J. Needs, S. Kenny, W. M. C. Foulkes, A. James: Phys. Rev. Lett. 73, 1959 (1994) 148 [28] G. Rajagopal, R. J. Needs, A. James, S. Kenny, W. M. C. Foulkes: Phys. Rev. B 51, 10591 (1995) 148, 150 [29] C. Lin, F. H. Zong, D. M. Ceperley: Phys. Rev. E 64, 016702 (2001) 148 [30] P. R. C. Kent, R. Q. Hood, A. J. Williamson, R. J. Needs, W. M. C. Foulkes, G. Rajagopal: Phys. Rev. B 59, 1917 (1999) 148, 150 [31] A. Ma, N. D. Drummond, M. D. Towler, R. J. Needs: Phys. Rev. E 71, 066704 (2005) 148 [32] M. M. Hurley, P. A. Christiansen: J. Chem. Phys. 86, 1069 (1987) 148 [33] L. Mitas, E. L. Shirley, D. M. Ceperley: J. Chem. Phys. 95, 3467 (1991) 148 [34] M. Casula, C. Filippi, S. Sorella: unpublished 148 [35] C. W. Greeﬀ, W. A. Lester, Jr.: J. Chem. Phys. 109, 1607 (1998) 148 [36] J. R. Trail, R. J. Needs: J. Chem. Phys. 122, 014112 (2005) 148 [37] J. R. Trail, R. J. Needs: J. Chem. Phys. 122, 224322 (2005) 148 [38] W. M. C. Foulkes, R. Q. Hood, R. J. Needs: Phys. Rev. B 60, 4558 (1999) 149 [39] A. J. Williamson, R. Q. Hood, R. J. Needs, G. Rajagopal: Phys. Rev. B 57, 12140 (1998) 149 [40] M. D. Towler, R. Q. Hood, R. J. Needs: Phys. Rev. B 62, 2330 (2000) 149 [41] R. Maezono, M. D. Towler, Y. Lee, R. J. Needs: Phys. Rev. B 68, 165103 (2003) 150 [42] R. J. Needs, M. D. Towler: Int. J. Mod. Phys. B 17, 5425 (2003) 150 [43] G. D. Watkins: Defects and Their Structure in Non-Metallic Solids (Plenum, New York 1976) p. 2003 153 [44] S. Dannefaer, P. Mascher, D. Kerr: Phys. Rev. Lett. 56, 2195 (1986) 153 [45] W. Frank, U. G¨ osele, H. Mehrer, A. Seeger: Diﬀusion in Crystalline Solids (Academic, Orlando 1985) p. 64 153, 154 [46] U. G¨ osele, A. Pl¨ ossl, T. Y. Tan: Process Physics and Modeling in Semiconductor Technology (Electrochemical Society, Pennington 1996) p. 309 153, 156 [47] D. Eaglesham: Phys. World 8, 41 (1995) 153 [48] R. J. Needs: J. Phys.: Condens. Matter 11, 10437 (1999) 153, 154, 155 [49] S. Goedecker, T. Deutsch, L. Billard: Phys. Rev. Lett. 88, 235501 (2002) 153, 154 [50] O. Al-Mushadani, R. J. Needs: Phys. Rev. B 68, 235205 (2003) 153, 154 [51] K. C. Pandey: Phys. Rev. Lett. 57, 2287 (1986) 154 [52] E. Kaxiras, K. C. Pandey: Phys. Rev. B 47, 1659 (1993) 154 [53] P. E. Bl¨ ochl, E. Smargiassi, R. Car, D. B. Laks, W. Andreoni, S. T. Pantelides: Phys. Rev. Lett. 70, 2435 (1993) 154

Quantum Monte Carlo Techniques and Defects in Semiconductors

163

[54] S. J. Clark, G. J. Ackland: Phys. Rev. B 56, 47 (1997) 154 [55] J. Bernholc, A. Antonelli, T. M. Del Sole, Y. Bar-Yam, S. T. Pantelides: Phys. Rev. Lett. 61, 2689 (1988) 157 [56] G. Davies, C. P. Foy: J. Phys. C 13, 4127 (1980) 157 [57] C. D. Clark, J. Walker: Proc. Roy. Soc. London Ser. A 234, 241 (1973) 157 [58] G. Davies: Rep. Prog. Phys. 44, 787 (1981) 157 [59] C. A. Coulson, M. J. Kearsley: Proc. Roy. Soc. London Ser. A 241, 433 (1957) 157 [60] M. Lannoo, J. Bourgoin: Point Defects in Semiconductors I: Theoretical Aspects (Springer, Berlin, Heidelberg 1981) pp. 141–145 157 [61] L. Hedin: Phys. Rev. 139, A796 (1965) 157 [62] G. Onida, L. Reining, A. Rubio: Rev. Mod. Phys. 74, 601 (2002) 157 [63] U. von Barth: Phys. Rev. A 20, 1693 (1979) 157 [64] S. J. Breuer, P. R. Briddon: Phys. Rev. B 51, 6984 (1995) 157, 158 [65] A. Zywietz, J. Furthm¨ uller, F. Bechstedt: Phys. Rev. B 62, 6854 (2000) 157 [66] D. Alf`e, M. J. Gillan: Phys. Rev. B 71, 220101 (2005) 158 [67] M. Leslie, M. J. Gillan: J. Phys. C 18, 973 (1985) 159 [68] D. Alf`e, M. J. Gillan: Phys. Rev. B 70, 161101 (2004) 160 [69] M. Troyer, U.-J. Wiese: Phys. Rev. Lett. 94, 170201 (2005) 160

Index absorption, 157 algorithm, 143–145, 147 backﬂow, 146, 147 background charge, 159 basis set, 158 Brillouin-zone, 148 charged defect, 158 classical, 160 cluster, 142, 147 cohesive energy, 150 concentration, 153, 154, 159 concerted exchange, 154–156 coordination, 142 correlation, 142, 145–147, 150, 156, 157 Coulomb, 146, 148 coupling, 157 cusp, 146 dangling-bond, 157 decay, 144 density-functional theory, 142 DFT, 142, 146, 148, 151–157, 159, 160 diamond, 141, 146, 157, 158, 161

diﬀusion, 141, 144, 145, 152, 155, 156 dipole, 158 distortion, 153, 157 dopant, 152 eigenstates, 144 electron, 142, 146–148, 157 electron paramagnetic resonance, 153 electron states, 157 electrostatic energy, 159 energetics, 142, 158 energy barrier, 154–156 equilibrium, 151–155, 159 exchange, 154 excitation, 142, 158 excited-state, 149, 157, 160 fermion, 143–145, 148, 160 ﬁrst principles, 157 force, 160 formation energy, 154, 156, 158 fourfold, 154, 155 Gaussian, 158 Ge, 150

164

R. J. Needs

general gradient approximation, 154 GGA, 154, 155 Green’s function, 145 ground-state, 142–145, 149, 157, 158, 160 GW, 157 Hamiltonian, 142–145, 148 Hartree–Fock, 146, 148 hydrogen, 148 imaginary, 142, 144, 148, 149 impurity, 142, 152 interstitial, 153–157 Jahn–Teller, 153, 157, 158 Kohn–Sham, 157 LDA, 156 liquid, 143 localization, 148, 149 LSDA, 150, 154, 155, 158, 160 Metropolis, 143 migration, 142, 154 molecular dynamics, 154 nonlocal, 148 optical, 157 periodic, 148, 159 periodic boundary conditions, 147, 149 perturbation, 154, 157 plane wave, 160 point defect, 146, 147, 153, 154 population, 149 potential, 142, 144, 145, 149

pseudopotential, 148, 149, 160 quantum Monte Carlo, 141, 142, 145–148, 150–152, 154, 157, 158, 160, 161 real space, 160 relaxation, 158 resonance, 153 Schottky, 158–161 Schr¨ odinger, 144 self-diﬀusion, 154, 156, 157 self-energy, 157 self-interstitial, 152–154, 156, 161 Si, 150 silicon, 141, 142, 152–154, 156, 157, 161 Slater, 146, 147, 156, 158, 160 spin, 146, 150, 158 statistical, 145–147, 149, 150, 158 stress, 157 supercell, 148, 159 surface, 142, 144–147, 149 symmetric, 146 symmetry, 148, 149, 153, 157 temperature, 153, 154 tetrahedral, 153, 155, 156 thermal equilibrium, 159 tiling, 145 total energy, 159 transition, 157, 158 transition metal, 142 uniaxial stress, 157 vacancy, 153, 154, 157–159, 161 variational, 141, 143, 148, 149

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces Arno Schindlmayr1,2 and Matthias Scheﬄer2 1

2

Institut f¨ ur Festk¨ orperforschung, Forschungszentrum J¨ ulich, 52425 J¨ ulich, Germany [email protected] Fritz-Haber-Institut der Max-Planck-Gesellschaft, Faradayweg 4–6, 14195 Berlin-Dahlem, Germany [email protected]

Abstract. We present a quantitative parameter-free method for calculating defect states and charge-transition levels of point defects in semiconductors. It combines the strength of density-functional theory for ground-state total energies with quasiparticle corrections to the excitation spectrum obtained from many-body perturbation theory. The latter is implemented within the G0 W0 approximation, in which the electronic self-energy is constructed non-self-consistently from the Green’s function of the underlying Kohn–Sham system. The method is general and applicable to arbitrary bulk or surface defects. As an example we consider anion vacancies at the (110) surfaces of III–V semiconductors. Relative to the Kohn–Sham eigenvalues in the local-density approximation, the quasiparticle corrections open the fundamental band gap and raise the position of defect states inside the gap. As a consequence, the charge-transition levels are also pushed to higher energies, leading to close agreement with the available experimental data.

1 Introduction The electric properties of semiconductors, and hence their applicability in electronic devices, are to a large degree governed by defects that are either intrinsic or incidentally or intentionally introduced impurities. Considerable eﬀorts, therefore, focus on determining the factors that lead to the formation of point defects and their inﬂuence on a material’s electric properties. The progress in the understanding of the atomic structure of point defects at cleaved III–V semiconductor surfaces, which serve as an illustration in this work, was recently reviewed by Ebert [1]. The possibility to image individual defects using scanning tunneling microscopy (STM) with atomic resolution, in particular, has yielded a wealth of data, but as STM provides a somewhat distorted picture of the electronic states close to the Fermi energy, these results cannot (and should not) be identiﬁed directly with the atomic geometry. Electronic-structure calculations have hence turned out to be an indispensable tool for the interpretation of the experimental ﬁndings. A deeper discussion of this point together with an example for the practical structure determination of a semiconductor surface is given in [2]. For point D. A. Drabold, S. K. Estreicher (Eds.): Theory of Defects in Semiconductors, Topics Appl. Physics 104, 165–192 (2007) © Springer-Verlag Berlin Heidelberg 2007

166

Arno Schindlmayr and Matthias Scheﬄer

defects at the (110) surfaces of III–V semiconductors several calculations were reported [3–8]. They are based on density-functional theory [9], where the exchange-correlation energy is typically treated in the local-density approximation (LDA) [10] or generalized gradient approximations (GGA) [11]. The agreement with experimental STM data appears to be very good. For example, the enhanced contrast of the empty pz orbitals of the two Ga atoms nearest to an anion vacancy in p-type GaAs(110) observed under positive bias and initially interpreted as an outward relaxation [12] could thus be understood to result, instead, from a downward local band bending accompanied by an inward relaxation [3]. The band bending itself is caused by the positive charge of the defect. Another controversy centers on the lateral relaxation of the positively charged anion vacancy. While STM images show a density of states preserving the mirror symmetry of the surface at the defect site [12], early theoretical studies of the lattice geometry based on total-energy minimization produced conﬂicting evidence for [3] and against [4, 5] a possible breaking of the mirror symmetry. Well-converged electronic-structure calculations later conﬁrmed that the distortion is indeed asymmetric [6–8] and that the apparently symmetric STM image results from the thermally activated ﬂip motion between two degenerate asymmetric conﬁgurations. In contrast, theoretical predictions of the electronic properties of point defects have been less successful and still show signiﬁcant quantitative deviations from experimental results. The principal quantities of interest are the location of defect states in the fundamental band gap as well as the charge-transition levels. We will carefully distinguish in this chapter between these two quantities: “defect states” or “defect levels” on the one hand and “charge-transition levels” on the other. The former are part of the electronic structure and can, in principle, be probed by photoemission spectroscopy, although standard spectroscopic techniques are often not applicable due to the low density of the surface defects. The Franck–Condon principle is typically well justiﬁed, because the rearrangement of the atoms happens on a much slower timescale than the photoemission process. Nevertheless, the coupling of the electrons to the lattice may be visible in the linewidths and lineshapes. The defect levels thus contain the full electronic relaxation in response to the created hole in direct photoemission or the injected extra electron in inverse photoemission, but no atomic relaxation. Although investigations of electronic properties frequently rely on the Kohn–Sham eigenvalues from density-functional theory, these only provide a ﬁrst approximation to the true band structure, and quantitative deviations from experimental results must be expected. In particular, for many materials the eigenvalue gap both in the LDA and the GGA underestimates the fundamental band gap signiﬁcantly. Likewise, the position of defect states in the gap cannot be determined without systematic errors. With these words of warning we note, however, that the Kohn–Sham eigenvalues constitute a good and well-justiﬁed starting point for calculating band structures and defect states [13]. Therefore, a

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces

167

perturbative approach starting from the Kohn–Sham eigenvalue spectrum is indeed appropriate. While the measurement of the defect levels (see the discussion on the page previous of this Chapter) probes the geometry before the electron is added or removed, the charge-transition levels are thermodynamic quantities and specify the values of the Fermi energy where the stable charge state of the defect changes. Therefore, the charge-transition levels are aﬀected noticeably by the atomic relaxation taking place upon the addition or removal of an electron. A quantitative analysis must hence be able to accurately compare the formation energies of competing conﬁgurations with diﬀerent numbers of electrons. Density-functional theory at the level of the LDA or GGA is capable of giving a good account of the atomic geometries for many materials. A critical feature is the nonlinearity of the exchange-correlation functional. The pseudopotential approximation, which eﬀectively removes the inner shells from the calculation by modeling their interaction with the valence electrons in terms of a modiﬁed potential, linearizes the core–valence interaction and thus does not treat this contribution correctly. In particular, freezing the d electrons in the core of a pseudopotential leads to poor lattice constants and a distorted electronic structure for some III–V semiconductors, such as GaN, where the Ga 3d states resonate strongly with the N 2s states [14]. For GaAs and InP this is a lesser problem, because the cation d states are energetically well below the anion 2s states and thus are relatively inert. As a result, the LDA and the GGA yield only small deviations from the experimental lattice constants and provide a good starting point for quasiparticle band-structure calculations. However, when competing conﬁgurations with a diﬀerent number of electrons are compared, the relevant energy diﬀerences lack the required quantitative accuracy. As we will show in more detail below, the reason is that these jellium-based approximations of the exchange-correlation energy ignore important features of the exact functional, such as the discontinuity of the exchange-correlation potential with respect to a change in the particle number. As a consequence, previous calculations of charge-transition levels based on the LDA exhibit systematic errors, for example for anion vacancies at InP(110) [6]. As an alternative approach to the electronic structure of point defects, we employ techniques adapted from many-body perturbation theory that we have found to be very fruitful in the past [15]. Exchange and correlation eﬀects are here described by a nonlocal and frequency-dependent self-energy operator. The solutions of the ensuing nonlinear eigenvalue equations have a rigorous interpretation as excitation energies and can be identiﬁed with the electronic band structure. We discuss the calculation of defect states as well as charge-transition levels within this framework and show that the results improve signiﬁcantly upon earlier values obtained from the Kohn– Sham scheme in the LDA. As an example we consider anion vacancies at GaAs(110) and InP(110), but the method is general and can also be applied to other defects at surfaces as well as in the bulk. The (110) surfaces are not only

168

Arno Schindlmayr and Matthias Scheﬄer

the natural cleavage planes of III–V semiconductors, but they have several characteristics that make them particularly interesting for defect studies. As no surface states exist inside the fundamental band gap [16, 17], the Fermi energy of a system that is clean and free from intrinsic defects is not pinned but controlled by the doping of the crystal. Only imperfections, such as anion vacancies or antisite defects, can introduce gap states and pin the Fermi energy at the surface. STM can probe ﬁlled and empty surface states by reversing the bias voltage [12], and both the GaAs(110) and the InP(110) surface are well characterized experimentally. This Chapter is organized as follows. We start in Sect. 2 by reviewing the computational methods. In Sect. 3 we then explain the physics of the defect-free GaAs(110) and InP(110) surfaces. The calculation of defect levels is discussed in Sect. 4 and that of charge-transition levels in Sect. 5, together with a comparison with the available theoretical and experimental data. Finally, Sect. 6 summarizes our conclusions. Unless explicitly indicated otherwise, we use Hartree atomic units.

2 Computational Methods A quantitative analysis of the electronic properties of point defects requires computational schemes that describe not only the ground state but also the excitation spectrum. While density-functional theory with state-of-theart exchange-correlation functionals can be used to determine ground-state atomic geometries, many-body perturbation theory is the method of choice for excited states. In this work we take the Kohn–Sham eigenvalues in the LDA as a ﬁrst estimate and then apply the G0 W0 approximation for the electronic self-energy as a perturbative correction. The latter provides a good account of the discontinuity as well as other shortcomings of the LDA. For this reason we ﬁrst review both schemes, emphasizing their strengths as well as limitations. 2.1 Density-Functional Theory Density-functional theory is based on the Hohenberg–Kohn theorem [9], which observes that the total energy EN,0 of a system of N interacting electrons in an external potential Vext (r) is uniquely determined by the ground-state electron density nN (r). While the Hohenberg–Kohn theorem itself makes no statement about the mathematical form of this functional, it has inspired algorithms that exploit the reduced number of degrees of freedom compared to a treatment based on many-particle wavefunctions. In the Kohn–Sham scheme [10], which underlies all practical implementations, the

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces

169

density is constructed from the orbitals of an auxiliary noninteracting system according to nN (r) = 2

∞

2

fN,j |ϕN,j (r)| .

(1)

j=1

The occupation numbers fN,j are given by the Fermi distribution; at zero temperature they equal one for states below the Fermi energy and zero for states above. The factor 2 stems from the spin summation. Here we only consider nonmagnetic systems and thus assume two degenerate spin channels throughout, although the formalism can easily be generalized if necessary. The energy functional is decomposed as 3 EN,0 ≡ E[nN ] = Ts [nN ] + Vext (r)nN (r) d r + EH [nN ] + Exc [nN ] , (2) where Ts [nN ] is the kinetic energy of the auxiliary noninteracting system and EH [nN ] the Hartree energy. The last term incorporates all remaining exchange and correlation contributions and is not known exactly. In practical implementations it must be approximated, for example by the LDA, which replaces the exchange-correlation energy Exc [nN ] by that of a homogeneous electron gas with the same local density [10]. A variational analysis ﬁnally shows that the total energy is minimized if the single-particle orbitals satisfy 1 2 − 2 ∇ + Vext (r) + VH ([nN ]; r) + Vxc ([nN ]; r) ϕN,j (r) = εKS N,j ϕN,j (r) . (3) The Hartree potential VH ([nN ]; r) and the exchange-correlation potential Vxc ([nN ]; r) are deﬁned as functional derivatives of the corresponding energy terms with respect to the density. The eigenvalues εKS N,j are Lagrange parameters that enforce the normalization of the orbitals. We use the Kohn–Sham scheme to determine the equilibrium geometry of clean surfaces and surface defects by relaxing the atomic coordinates and allowing the system to explore its energetically most favorable conﬁguration. Although the Kohn–Sham eigenvalues diﬀer from the true excitation energies and constitute only an approximation to the quasiparticle band structure, they are often numerically close in practice. This follows from the transitionstate theorem of Slater [18] and Janak [19] and allows a correction within perturbation theory. Here, we are interested in the position of the defect state, which may be occupied or unoccupied, relative to the surface valence-band maximum. As the defect state is separated from the valence-band maximum by a ﬁnite energy diﬀerence, the location obtained from the Kohn–Sham eigenvalue spectrum contains two sources of errors: In addition to the chosen approximation for the exchange-correlation functional, there is another systematic error that is due to fundamental limitations of the Kohn–Sham scheme and would also be present if the exact functional was employed. In order to understand the latter, we now brieﬂy sketch its origin.

170

Arno Schindlmayr and Matthias Scheﬄer

One rigorous result is that the eigenvalue of the highest occupied Kohn– Sham state matches the corresponding quasiparticle energy [20], which is in turn equal to the ionization potential that marks the threshold for photoemission, i.e., εKS N,N = EN,0 −EN −1,0 . If the highest occupied state corresponds to the valence-band maximum, then the unoccupied defect state equals the electron aﬃnity εKS N +1,N +1 = EN +1,0 −EN,0 , because it is the next to be populated by one extra electron added to the system. Unfortunately, this is not the same as the eigenvalue εKS N,N +1 of the ﬁrst unoccupied state obtained from (3). The diﬀerence is due to the fact that the exchange-correlation potential of an insulator Vxc ([nN +1 ]; r) = Vxc ([nN ]; r) + ∆xc + O(1/N ) with ∆xc > 0 changes discontinuously upon addition of an extra electron [21, 22]. A similar argument can be made if the defect state is occupied. As a consequence, the Kohn–Sham eigenvalue gaps diﬀer systematically from the gaps in the true quasiparticle band structure. The magnitude of the discontinuity is still a matter of controversy but is believed to be signiﬁcant. For pure sp-bonded semiconductors like GaAs the LDA underestimates the experimental band gap by about 50 %. The GGA, designed only to improve the total energy, yields a very similar eigenvalue spectrum as the LDA when applied to the same atomic geometry. An entirely diﬀerent construction that permits a more systematic treatment of exchange and correlation is the optimized eﬀective potential method [23]. When evaluated to ﬁrst order in the coupling constant, this approach yields the exact exchange potential, which can be used in band-structure calculations [24]. Remarkably, for many semiconductors the resulting Kohn–Sham eigenvalue gaps are very close to the true quasiparticle band gaps [25]. The signiﬁcance of this observation is under debate, however, because there are indications that it may not uphold if correlation is treated on the same footing. Preliminary results suggest that the eigenvalue gaps are again close to the LDA values if correlation is included within the random-phase approximation [26, 27], but there is currently too little data to make a deﬁnite statement, and all existing calculations at this level also contain additional simpliﬁcations, for example a shape approximation for the potential in the linearized muﬃn-tin orbital method in [27]. The reasoning above suggests that density-functional theory is still, in principle, applicable for calculating the diﬀerence in total energy between ground-state conﬁgurations with diﬀerent electron numbers, which is needed to determine the energetically most favorable charge state of a point defect. However, all jellium-based functionals lack the derivative discontinuity ∆xc of the exact exchange-correlation potential. This neglect reduces the electron aﬃnity EN +1,0 −EN,0 both in the LDA and the GGA if the additional electron occupies a state separated from the valence-band maximum by a ﬁnite energy diﬀerence. For systems in contact with an electron reservoir, such as defects in solids, it hence lowers the threshold for an increase of the electron population. This is consistent with the observation that the calculated charge-transition levels for materials like InP are signiﬁcantly smaller than the available values deduced from experimental measurements [6]. The exact exchange potential,

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces

171

an implicit functional of the density deﬁned in terms of the Kohn–Sham orbitals, includes a derivative discontinuity [13], but the latter exceeds the experimental band gap signiﬁcantly and must hence be partially canceled by a correlation contribution with similar magnitude and opposite sign [25]. As the total energies are by construction close to the corresponding Hartree– Fock values, the electron aﬃnities EN +1,0 − EN,0 are grossly overestimated, and no reliable charge-transition levels can be obtained in this way. Our implementation of density-functional theory employs the plane-wave pseudopotential method in combination with the LDA. We use the parametrization by Perdew and Zunger [28], which is in turn based on the quantum Monte-Carlo data of Ceperley and Alder for the homogeneous electron gas [29]. The norm-conserving pseudopotentials are of the fully separable Kleinman–Bylander form [30]. We choose d as the local component for all pseudopotentials except for In, where p is used instead. The Kohn–Sham wavefunctions are expanded in plane waves with a cutoﬀ energy of 15 Ry. Our calculations are performed with the FHImd code [31, 32]. The bulk lattice constants obtained in this way, 5.55 ˚ A for GaAs and 5.81 ˚ A for InP in the absence of zero-point vibrations, are in good agreement with previously published data [33] and slightly smaller than the experimental values at room temperature by 1.8 % and 1.1 %, respectively [34]. We use the theoretical lattice constants in order to prevent errors resulting from a nonequilibrium unit-cell volume during the relaxation of the surface geometries. 2.2 Many-Body Perturbation Theory Many-body perturbation theory [35] provides powerful techniques to analyze the electronic structure in the gap region, because the framework is designed speciﬁcally to give access to excited states. Quasiparticle excitations created by the addition or removal of one electron are obtained from the one-particle Green’s function ˆ t)ψˆ† (r , t )}|ΨN,0 , G(r, r ; t − t ) = −iΨN,0 |T {ψ(r,

(4)

where |ΨN,0 denotes the ground-state wavefunction of the interacting elecˆ )ψˆ† (r ) exp(−iHt ˆ ) tron system in second quantization, ψˆ† (r , t ) = exp(iHt ˆ t) = exp(iHt) ˆ exp(−iHt) ˆ ψ(r) ˆ are the electron creation and annihiand ψ(r, lation operators in the Heisenberg picture, respectively, and the symbol T sorts the subsequent list of operators according to ascending time arguments from right to left with a change of sign for every pair permutation. The Green’s function can be interpreted as a propagator: For t > t it describes a process in which an extra electron is added to the system at time t . The ˆ but resulting wavefunction is, in general, no eigenstate of the Hamiltonian H a linear combination of many eigenstates |ΨN +1,j . Between the times t and t each projection evolves with its own characteristic phase, and a Fourier analysis of this oscillatory behavior immediately yields the energy spectrum

172

Arno Schindlmayr and Matthias Scheﬄer

εN,j = EN +1,j − EN,0 of the accessible excited states. Likewise, for t > t the Green’s function describes the propagation of an extra hole between t and t , yielding the energies εN,j = EN,0 − EN −1,j . In mathematical terms, we insert a complete set of eigenstates between the ﬁeld operators in (4) and Fourier transform to the frequency axis. The resulting expression G(r, r ; ω) = lim

η→+0

∞

fN,j

j=1 ∞

(1 − fN,j )

+ lim

η→+0

∗ ψN,j (r)ψN,j (r ) ω − εN,j − iη

j=1

∗ ψN,j (r)ψN,j (r ) ω − εN,j + iη

(5)

shows that the poles of the Green’s function correspond directly to the quasiparticle energies εN,j . Signiﬁcantly, these not only yield the true band structure, but the highest occupied state also equals the exact ionization potential EN,0 − EN −1,0 and the lowest unoccupied state the exact electron aﬃnity EN +1,0 − EN,0 . Therefore, many-body perturbation theory provides a convenient way to analyze both defect states and the energetics of charge tranˆ sitions. The wavefunctions ψN,j (r) = ΨN −1,j |ψ(r)|Ψ N,0 for occupied and ˆ ψN,j (r) = ΨN,0 |ψ(r)|Ψ for unoccupied states are obtained from the N +1,j quasiparticle equations 1 2 − 2 ∇ + Vext (r) + VH (r) ψN,j (r) 3 + Σxc (r, r , εN,j )ψN,j (r ) d r = εN,j ψN,j (r) . (6) The self-energy Σxc (r, r , ε) incorporates all contributions from exchange and correlation processes. In contrast to the exchange-correlation potential of density-functional theory, it is nonlocal, energy dependent and has a ﬁnite imaginary part, which is proportional to the damping rate resulting from electron–electron scattering. Together with other relevant decay channels, such as scattering from phonons or impurities, this mechanism is responsible for a ﬁnite lifetime of the excitations. For real materials the self-energy can only be treated approximately. Like the majority of practical applications, we use the G0 W0 approximation [36] Σxc (r, r ; t − t ) = lim iG0 (r, r ; t − t )W0 (r, r ; t − t + η) . η→+0

(7)

The Fourier transform of G0 (r, r ; t − t ) on the frequency axis is constructed in analogy to (5) from the eigenstates of an appropriate mean-ﬁeld system, in our case from the Kohn–Sham orbitals ϕN,j (r) and eigenvalues εKS N,j . The dynamically screened Coulomb interaction W0 (r, r ; t − t ) can be modeled in diﬀerent ways. Many implementations use plasmon-pole models, in which the frequency dependence is described by an analytic function whose parameters are determined by a combination of known sum rules and asymptotic limits [37,38]. This simpliﬁcation has the advantage that it facilitates an analytic

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces

173

treatment, but it ignores details of the dynamic screening processes in a material and thus constitutes a potential source of errors. Here we take the full frequency dependence of the dielectric function into account by employing the random-phase approximation W0 (k, ω) = v(k) + v(k)P0 (k, ω)W0 (k, ω)

(8)

with the bare Coulomb potential v(k) = 4π/|k|2 and the polarizability P0 (r, r ; t − t ) = −2iG0 (r, r ; t − t )G0 (r , r; t − t) .

(9)

The inclusion of dynamic screening derives from the concept of quasiparticles, which comprise an electron or hole together with its surrounding polarization cloud. The composite is called a quasiparticle because it behaves in many ways like a single entity. The polarization cloud is created by the repulsive Coulomb potential and reduces the eﬀective charge of the quasiparticle compared to that of the bare particle at its center. The G0 W0 expression (7) constitutes the leading term in the expansion of the self-energy and is of ﬁrst order in the dynamically screened interaction. Finally, we exploit the formal similarity between (6) and the Kohn–Sham equations (3) by evaluating the quasiparticle energies within ﬁrst-order perturbation theory as εN,j = εKS N,j + ϕN,j |Σxc (εN,j ) − Vxc [nN ]|ϕN,j .

(10)

The treatment within ﬁrst-order perturbation theory is justiﬁed if the eigenvalues of the underlying Kohn–Sham system are already suﬃciently close to the expected quasiparticle band structure. This is guaranteed by the transition-state theorem [18, 19]. Besides, the orbitals ϕN,j (r) are usually a good approximation to the true quasiparticle wavefunctions. For the homogeneous electron gas both are plane waves and thus coincide exactly. Numerical calculations for bulk semiconductors indicate an overlap close to unity between the Kohn–Sham orbitals in the LDA and the quasiparticle wavefunctions obtained from (6) with the G0 W0 approximation for states near the band edges [39]. Larger eﬀects have been observed for surfaces, especially for image states, because the latter are located outside the surface in a region where the LDA potential is qualitatively wrong [40, 41]. Changes in the wavefunctions of other surface states can also be identiﬁed but have only a minor inﬂuence on the quasiparticle energies in the gap region. For GaAs(110) this has been conﬁrmed explicitly [42]. In principle, the equations (4) to (9) could be solved self-consistently by successively updating the self-energy with the quasiparticle orbitals derived from it. This approach is appealing on formal grounds because it makes the results independent of the original mean-ﬁeld approximation. In addition, the self-consistent Green’s function satisﬁes certain sum rules, including particlenumber conservation [43]. In practice, however, this procedure produces a poor excitation spectrum. The reason lies in the mathematical structure of

174

Arno Schindlmayr and Matthias Scheﬄer

Hedin’s equations, which describe the recipe for constructing the self-energy from the Green’s function by means of functional-derivative techniques [36]. The G0 W0 approximation is the result of a single iteration. Further iterations would not only ensure self-consistency in the Green’s function but would also introduce higher-order self-energy terms, so-called vertex corrections. If the latter are neglected, then the spectral features deteriorate, as was ﬁrst demonstrated for the homogeneous electron gas [44]. For bulk semiconductors self-consistency appears to lead to a gross overestimation of the fundamental band gap [45] in combination with poor spectral weights and linewidths. We hence follow the established procedure for practical applications and terminate the cycle at the G0 W0 approximation. Of course, the ﬁnal results depend on the input Green’s function in this case. Another point that has been raised in the same context concerns possible errors resulting from the pseudopotential approach, which has traditionally dominated applications of the G0 W0 approximation. Numerical deviations must be expected because the matrix elements of the self-energy in (10) are inﬂuenced by the pseudoization of the wavefunctions – that is the neglect of core states plus appropriate smoothening of the valence states in the core region – and the treatment of the core–valence interaction in pseudopotential calculations. Indeed, a number of early all-electron implementations of the G0 W0 approximation, based on the linearized augmented plane-wave or the linearized muﬃn-tin orbital method, found quasiparticle band gaps for prototype semiconductors that were signiﬁcantly smaller than previously reported values and blamed the discrepancy on the pseudopotential approximation [46, 47]. However, this claim was later refuted by all-electron calculations using plane waves [48, 49]. The issue is currently still under debate, but there is mounting evidence that a large part of the observed discrepancy is due to insuﬃcient convergence of the early calculations in combination with deﬁciencies of the linearized basis sets for the description of high-lying unoccupied states [48, 50]. If these factors are properly accounted for, then the deviation is signiﬁcantly reduced, and the all-electron results are again in good agreement with experimental measurements. A certain discrepancy with respect to pseudopotential calculations still remains, although the diﬀerence is small compared to that from the Kohn–Sham eigenvalues. While some errors of the pseudopotential approach can be partially suppressed, for example through a better description of the core–valence interaction [51], many others are inherent. In particular, the pseudopotential construction also entails an incorrect description of high-lying states. A careful analysis of the quantitative implications of the pseudopotential approximation is the subject of active research. The good quantitative agreement between the G0 W0 approximation and experimental band structures has been demonstrated for a wide range of bulk materials, including III–V semiconductors [52–54]. Due to the high computational cost in present implementations, which stems from the evaluation of the nonlocality of the propagators, their frequency dependence, and the

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces

175

Fig. 1. Bulk band structure of GaAs. The G0 W0 approximation (straight lines) opens the too small Kohn–Sham eigenvalue gap in the LDA (dashed lines) and is in very good agreement with the experimental band gap. The calculation is carried out at the theoretical lattice constant 5.55 ˚ A, and the valence-band maximum is set to zero in both schemes

need to include a large number of unoccupied states, there have been relatively few applications to more complex systems so far, however. Furthermore, these often contain additional simpliﬁcations: the two available studies of the quasiparticle band structure of GaAs(110) both employed plasmon-pole models instead of the more accurate random-phase approximation [55, 56], and the only published results for InP(110) were obtained within an even more restrictive tight-binding formalism [57]. For a quasiparticle band-structure calculation the matrix elements of the self-energy in (6) must be evaluated in the frequency domain for states with a given wavevector k. Therefore, most practical implementations of the G0 W0 approximation choose a reciprocal-space representation for all propagators. The cell-periodic part of the wavefunctions is often expanded in plane waves [52, 55], although localized basis sets like Gaussian orbitals have also been used [54]. The disadvantage of the representation in reciprocal space is that the products (7) and (9) turn into numerically expensive multidimensional convolutions. Therefore, we employ a representation in real space and imaginary time [58, 59], in which the self-energy and the polarizability can be calculated by simple multiplications. The projection on wavevectors and imaginary frequencies used to solve the Dyson-type equation (8) can be done eﬃciently by exploiting fast Fourier transforms. The imaginary time and frequency arguments are chosen because the functions are smoother on these axes and can be sampled with fewer grid points, although they contain

176

Arno Schindlmayr and Matthias Scheﬄer

exactly the same information. The physical self-energy on the real frequency axis is eventually recovered by an analytic continuation. As an illustration of the G0 W0 approximation we show the calculated bulk band structure of GaAs in Fig. 1. The band gap is direct and located at Γ in the center of the Brillouin zone. While the LDA underestimates the fundamental band gap and yields a Kohn–Sham eigenvalue gap of only 0.78 eV at a lattice constant of 5.55 ˚ A, the subsequent addition of the self-energy correction opens the band gap to 1.55 eV, which is in very good agreement with the experimental value of 1.52 eV [34]. As we measure all energies relative to the valence-band maximum, we set the latter to zero and align the two sets of curves at this point. The principal eﬀect of the G0 W0 approximation is a rigid upward shift of the conduction bands, although the dispersion is also slightly modiﬁed, as can be seen by the reduced bandwidth at the bottom of the valence band. The band structure of InP looks very similar. In this case we obtain a Kohn–Sham eigenvalue gap of 0.76 eV at the theoretical lattice constant 5.81 ˚ A and a quasiparticle band gap of 1.52 eV that is again close to the experimental value 1.42 eV [34]. Incidentally, the band gap depends sensitively on the lattice constant. For GaAs it decreases at a rate of −4.07 eV/˚ A in the LDA and −4.59 eV/˚ A in the G0 W0 approximation when the lattice constant increases. For InP the values are −3.13 eV/˚ A and −3.68 eV/˚ A.

3 Electronic Structure of Defect-Free Surfaces Before focusing on defect states we ﬁrst brieﬂy discuss the electronic structure of the defect-free GaAs(110) and InP(110) surfaces. The nonpolar (110) surface, illustrated in Fig. 2, is the natural cleavage plane of the zincblende lattice, because it cuts the smallest number of bonds per unit area. Both the cations and anions in the terminating layer are threefold coordinated, and each possess one dangling bond extending into the vacuum. Due to the diﬀerent electron aﬃnities of the two species, charge is transfered from the dangling bonds of the cations to those of the anions. This charge transfer is the driving force for a structural relaxation, which consists of an outward movement of the anion atoms and a corresponding inward movement of the cation atoms [33]. As a result, the orbitals of the latter rehybridize from an sp3 towards an energetically more favorable sp2 bonding situation in a nearly planar environment; the empty pz -like orbitals perpendicular to this plane are pushed to higher energies and form an unoccupied surface band. At the same time, the three bonds between the anions and their neighboring group-III atoms are rearranged at almost right angles and become more p-like in character; the nonbonding electron pairs in the fourth orbital pointing away from the surface are in turn lowered in energy and give rise to an occupied surface band. The relaxation preserves the C1h point-group symmetry with a single mirror plane perpendicular to the [¯ 110] direction.

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces

177

Fig. 2. Geometry of the anion vacancy at the GaAs(110) surface. The As atoms are shown in light and the Ga atoms in dark gray. The three Ga atoms nearest to the vacancy are indicated by arrows

In Fig. 3 we show the calculated band structure of the clean and defectfree GaAs(110) surface at the theoretical lattice constant 5.55 ˚ A, modeled as a slab element placed in a supercell with periodic boundary conditions in all directions. The slab consists of six atomic layers, of which the top three layers are allowed to relax, while the three base layers are kept ﬁxed at their ideal bulk positions. The dangling bonds at the bottom of the slab are passivated by pseudoatoms with noninteger nuclear charges of 0.75 and 1.25 for anion and cation termination, respectively. The slabs are separated by a vacuum region equivalent to four atomic layers. The gray-shaded regions in the ﬁgure mark the projection of the G0 W0 bulk bands onto the two-dimensional surface Brillouin zone, shown in the inset. The dashed lines indicate the occupied and unoccupied surface bands obtained from the LDA, the straight lines are the corresponding G0 W0 results. For the calculation of the groundstate density and the Kohn–Sham eigenvalues we used four Monkhorst–Pack k-points [60] in the irreducible part of the Brillouin zone, while the self energy was evaluated at the four high-symmetry points Γ, X , M, and X. In our implementation the k-point set enters merely as the reciprocal grid of the real-space mesh used to describe the nonlocality of G0 (r, r ; t − t ) and Σxc (r, r ; t − t ) [58]; the four selected k-points correspond to a real-space mesh that extends over four surface unit cells. This is suﬃcient, because the correlation length is of the order of the interatomic distance [61]. The position of the Kohn–Sham surface bands relative to the corresponding bulk bands was determined by aligning the electrostatic potential in the central part of the slab with that of the bulk. We then applied the self-energy correction independently to surface and bulk bands and again chose the valence-band maximum as the energy zero. From the ﬁgure it is evident that the G0 W0 approximation has only a small eﬀect on the dispersion of the surface bands.

178

Arno Schindlmayr and Matthias Scheﬄer

Fig. 3. Surface band structure of GaAs(110) in the LDA (dashed lines) and the A. The G0 W0 approximation (straight lines) at the theoretical lattice constant 5.55 ˚ gray-shaded regions mark the projected G0 W0 bulk bands. The inset indicates the two-dimensional surface Brillouin zone

While the position of the occupied surface band relative to the valence-band edge at Γ remains almost unchanged, the upward shift of the unoccupied surface band (0.86 eV) slightly exceeds that of the bulk conduction bands (0.77 eV). The larger impact of the self-energy correction on the surface gap was noticed before [55, 56]; our result for the gap correction lies between the two previously published values. Small deviations of about 0.1 eV are due to diﬀerences in the implementations, for example the reliance on plasmon-pole models in [55, 56] compared to the random-phase approximation for the dynamically screened Coulomb interaction in this work. Both the occupied and the unoccupied surface bands are in close proximity to the projected bulk bands and, in fact, overlap with them in large parts of the Brillouin zone. As neither extends into the fundamental gap between the bulk valence and conduction band edges at Γ, they do not pin the surface Fermi level. Although prevalent in electronic-structure calculations for surfaces, the supercell approach is a drastic alteration of the system’s geometry whose inﬂuence must be carefully monitored, because the occurrence of electric multipole moments may lead to artiﬁcial long-range interactions between the periodic slabs. Static dipoles, if present, can be eliminated in density-functional theory [62]. With this correction the limit of isolated slabs is quickly reached. Dynamic dipoles are always created in dielectric media, however, and contribute to the polarizability in the G0 W0 approximation. Actually, there are two contributions that must be distinguished. The ﬁrst is the dynamic polarization between the slabs, which gives rise to an additional slowly varying potential that reduces the band gap. This eﬀect can be understood and even

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces

179

quantitatively modeled in terms of classical image charges [63]; for the geometry used in this work it amounts to about 0.1 eV. The model thus allows an a-posteriori extrapolation to the limit of an isolated slab. The second contribution is the ﬁnite width of the slab, which increases the gap due to quantization eﬀects. At present there is no obvious cure for this problem within the G0 W0 approximation, and as the two eﬀects counteract each other, we have not applied any partial correction to eliminate the dynamic polarization between the slabs either. In principle, both problems could be avoided by studying systems comprised of semi-inﬁnite matter and vacuum regions. Within density-functional theory several methods have indeed been proposed for this purpose [64–67]. Their eﬃciency relies on the fact that a perturbation breaking the translational symmetry, such as a surface or defect, modiﬁes the eﬀective potential only in its immediate vicinity. In the G0 W0 formalism this cannot be exploited to the same degree, because all propagators are explicitly nonlocal, and a much larger simulation cell must hence be taken into account. So far, only one G0 W0 calculation for an eﬀectively one-dimensional system, a semi-inﬁnite jellium surface, has been reported [68]. In preparation for later applications to larger supercells, we repeated the G0 W0 calculation with lower cutoﬀ energies and found that the self-energy correction to the surface gap remained stable up to 10 Ry. The reason for the rapid convergence, which is well known and can be exploited to reduce the computational expense considerably, is that the kinetic energy and the electrostatic Hartree potential, the two largest contributions to the quasiparticle energies, are already included in the Kohn–Sham eigenvalues in (10); the matrix elements of the self-energy are less sensitive to the number of plane waves. Besides, we obtained essentially the same surface gap when reducing the width of the slab to four layers. For this geometry and a cutoﬀ energy of 10 Ry, we performed test calculations in which we included up to 1049 unoccupied bands in the Green’s function. With 379 bands the results are already converged within 0.02 eV, suﬃcient for our purpose.

4 Defect States The geometry of the anion vacancy is illustrated in Fig. 2 for the GaAs(110) surface. The removal of the As atom leaves each of the three Ga atoms surrounding the vacancy with a dangling bond. As a consequence, the two GaI atoms in the ﬁrst layer move downwards while the GaII atom in the second layer moves upwards and forms two new bonds with the GaI atoms across the void. Its coordination number thus increases from four to ﬁve, while the threefold coordination of the GaI atoms remains unchanged. The relaxation preserves the C1h point-group symmetry, except in the positive charge state where an asymmetric distortion that pushes the unoccupied defect level in the band gap to higher energies is more favorable [6, 8]. We ﬁnd that the distortion lowers the total energy by 0.17 eV for GaAs and 0.11 eV for InP.

180

Arno Schindlmayr and Matthias Scheﬄer

The anion vacancy gives rise to three electronic states, all localized at the GaI –GaII bond pair. They are labeled as 1a , 1a and 2a , where a denotes states that are even with respect to the mirror plane and a denotes states that are odd. Although the asymmetric relaxation in the positive charge state destroys this symmetry and deforms the orbitals slightly, it leaves the order of the states intact, and we continue to use the same notation for simplicity. The 1a state is located several eV below the valence-band maximum and thus always ﬁlled with two electrons, while the 2a state is too high in energy to become populated. Only the 1a state falls inside the fundamental band gap. Depending on the doping, it can be occupied either by zero, one or two electrons, which corresponds to the positive, neutral or negative charge state, respectively. It is important to note that the charge state inﬂuences the defect geometry, as the GaI –GaII bonds contract with increasing electron occupancy, reﬂecting the bonding character of the 1a state. In the following we examine the position of this defect level for a given charge state; the question of which charge state is preferred under speciﬁc conditions, such as doping, is answered in the next section. For the density-functional calculations we choose a supercell consisting of 2 × 4 surface unit cells and six atomic layers. For charged systems we include a uniform charge density with opposite sign in order to compensate the extra electron or hole and restore overall neutrality in the supercell. Instead of a well-deﬁned defect state, the supercell periodicity gives rise to an artiﬁcial dispersion as illustrated in Fig. 4. At the surface of each slab the defects form a rectangular grid whose lattice parameters ax and ay equal the dimensions of the supercell. Since the 1a state is odd with respect to the mirror plane, one can regard it as a p orbital that exhibits π-type bonding along the [001] and σ-type bonding along the [¯ 110] direction. We hence consider a tight-binding model KS KS KS εKS k = ε1a + 2V1π cos(kx ax ) + 2V1σ cos(ky ay ) KS KS cos(2kx ax ) + 2V3σ cos(2ky ay ) + V2KS cos(kx ax ) cos(kx ax ) + 2V3π (11)

with parameters ﬁtted to the calculated Kohn–Sham band, where εKS 1a equals the eigenvalue of a single defect and the other parameters have the meaning of hopping integrals. The above expression includes interactions up to thirdnearest neighbors and reproduces the dispersion with a correlation coeﬃcient close to 0.999 9 for all systems under consideration. As the G0 W0 formalism involves nonlocal propagators, the amount of data that must be processed grows rapidly with the system size. In order to limit the computational expense we use a smaller (2 × 2) supercell and four atomic layers instead of the (2 × 4) cell to determine the self-energy correction of the 1a state. The stronger defect–defect interaction along the [¯110] direction increases the dispersion but does not change it qualitatively. As the presence of the defect does not modify the range of the nonlocal propagators appre-

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces

181

Fig. 4. Calculated 1a defect level of the As vacancy at GaAs(110) in the (a) positive and (b) negative charge state (dashed line: LDA; solid line: G0 W0 ). The artiﬁcial dispersion in the LDA is due to the supercell periodicity; the horizontal lines mark the actual defect level εKS 1a and the corresponding G0 W0 result. As the calculations in (a) refer to the constrained symmetric relaxation, the additional shift due to the asymmetric distortion is shown separately. The inset in (b) indicates the downfolded Brillouin zone for the (2 × 4) supercell

ciably, we use one k-point and 1500 unoccupied bands for the construction of the Green’s function G0 , which corresponds to the same Brillouin-zone sampling as the four k-points and 379 bands that we found satisfactory for the (1 × 1) unit cell of the defect-free surface. For the positively charged As vacancy at GaAs(110) we evaluated the self-energy correction in the entire Brillouin zone [15]. By relating the calculated quasiparticle dispersion to a tight-binding model equivalent to (11), we found very similar values for the parameters V3π and V3σ as in the LDA, which implies that the inﬂuence of the third-nearest neighbors on the self-energy correction is negligible. This observation can be exploited as follows. At k = (2π/4)(1/ax , 1/ay , 0) the contributions from the ﬁrst- and second-nearest neighbors vanish, so that the Kohn–Sham eigenvalue is given by KS KS KS εKS k = ε1a − 2V3π − 2V3σ ,

(12)

and the corresponding quasiparticle energy by εk = ε1a − 2V3π − 2V3σ .

(13)

182

Arno Schindlmayr and Matthias Scheﬄer

If the surviving hopping integrals on the right-hand sides coincide, then KS the identity ε1a − εKS 1a = εk − εk holds. On the other hand, the self-energy correction is deﬁned through the relation KS KS KS εk − εKS k = ϕk |Σ(εk ) − Vxc |ϕk .

(14)

Instead of a scan over the whole Brillouin zone, we can hence determine the self-energy correction for an isolated defect from a single calculation at k . The quasiparticle results are obtained by adding this correction to the Kohn– Sham value εKS 1a of the larger (2×4) supercell, where the position of the latter relative to the valence-band maximum can be established more accurately. We estimate that the uncertainty of the ﬁnal quasiparticle energies, which results from the discrete k-point sampling, the approximate treatment of the core–valence interaction in the pseudopotential approach, the ﬁnite size of the supercell, and other convergence factors amounts to 0.1 eV to 0.2 eV. We performed explicit G0 W0 calculations for the positive and negative charge states, in the ﬁrst case using a constrained symmetric relaxation. The results for GaAs(110) are displayed in Fig. 4. For the neutral anion vacancy the supercell contains an odd number of electrons; in combination with the requirement of spin degeneracy this leads to fractional occupation numbers in each spin channel. At present we cannot treat such systems. For the positive charge state with the proper asymmetric distortion the defect level in the G0 W0 approximation is not calculated directly but deduced as follows. As the lowest unoccupied state, the 1a defect level equals the electron aﬃnity, i.e., ε1a = E vac (0, Qasym ) − E vac (+, Qasym ), where E vac (q, Q) denotes the + + total energy of a surface featuring an anion vacancy with the actual electron population q ∈ {+, 0, −} and a geometric structure optimized for the charge , Qsym state Q ∈ {Qasym + + , Q0 , Q− }. This expression can be rewritten as ε1a = E vac (0, Qasym ) − E vac (0, Qsym + + ) vac + E vac (0, Qsym (+, Qsym + )−E + ) vac + E vac (+, Qsym (+, Qasym ) (15) + )−E + by adding and subtracting intermediate conﬁgurations. The term in the second line on the right-hand side equals the quasiparticle energy for the corresponding symmetric relaxation, which can be calculated with less computational cost by exploiting the C1h point-group symmetry. The other two terms are simple total-energy diﬀerences between the symmetric and the asymmetric geometry for a constant number of electrons; both are positive and can be obtained from density-functional theory. The calculated defect levels are summarized in Table 1 for GaAs(110) and Table 2 for InP(110). Our LDA results are consistent with most of the previously published calculations [3, 5, 7]. A notable exception are the values by Zhang and Zunger [3] for the negative charge state of the As vacancy at GaAs(110) and for the constrained symmetric geometry of the positive charge

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces

183

Table 1. Calculated defect levels for the As vacancy at GaAs(110) in eV relative to the valence-band maximum. For the positive charge state the ﬁrst column refers to the asymmetric and the second to the constrained symmetric relaxation. The quasiparticle band gap of 1.55 eV in this work, calculated at the theoretical lattice constant 5.55 ˚ A, is close to the experimental value of 1.52 eV Charge state LDA (this work) LDA [3] LDA [5] G0 W0 (this work)

(+1) 0.70 0.73 1.08

(0.06) (0.41) (0.06) (0.59)

(0)

(−1)

0.13

0.24 0.5 0.24 0.48

0.23

Table 2. Calculated defect levels for the P vacancy at InP(110) in eV relative to the valence-band maximum. For the positive charge state the ﬁrst column refers to the asymmetric and the second to the constrained symmetric relaxation. The quasiparticle band gap of 1.52 eV in this work, calculated at the theoretical lattice constant 5.81 ˚ A, slightly exceeds the experimental value of 1.42 eV Charge state LDA (this work) LDA [7] G0 W0 (this work)

(+1) 0.89 1.36

(0.39) (0.326) (0.91)

(0)

(−1)

0.49 0.479

0.60 0.580 1.01

state in Table 1. After a full relaxation of the asymmetric distortion in the latter case, the discrepancy vanishes, however. The agreement with the results of Kim and Chelikowsky [5] for the same system is very good, except for a diﬀerence of 0.1 eV for the neutral charge state. The origin of these deviations cannot be traced, because both groups of authors give very little information about their computational details, and the size of the corresponding Kohn– Sham eigenvalue gap is not stated. For all conﬁgurations with symmetric geometries the defect level moves steadily upwards with increasing electron population. The asymmetric distortion has a large eﬀect on the unoccupied defect level and pushes it to signiﬁcantly higher energies. Concomitant with the opening of the fundamental band gap, the G0 W0 approximation adds a positive quasiparticle correction to all defect levels and predicts larger values than the LDA for all charge states. The size of the self-energy shift depends both on the charge state and the geometry, although the diﬀerences are of the same order as the error bar of the calculation. We note that our numerical values diﬀer slightly from those reported earlier in [15]. The discrepancy is due to an improved description of the anisotropic screening in the slab geometry in this work but lies within the estimated overall error bar of the calculation.

184

Arno Schindlmayr and Matthias Scheﬄer

For the P vacancy at InP(110) we obtain a similar picture, although the defect levels are at higher energies both in the LDA and the G0 W0 approximation. Unfortunately, due to experimental diﬃculties, no direct measurements of the defect states by photoemission are available. In this situation one can only try to extract values from indirect methods like surface photovoltage imaging with STM. One study using this technique claimed a value of 0.62 ± 0.04 eV for the As vacancy in the positive charge state, based on the known position of the sample’s Fermi energy 0.09 eV above the valence-band maximum and a local band bending of 0.53 eV [69]. An STM measurement on a diﬀerent sample found a band bending of only 0.1 eV, however [12]. The origin of this discrepancy is unclear but points to a strong inﬂuence of experimental conditions and/or sample quality. Because of this uncertainty, no experimental values are included in the tables.

5 Charge-Transition Levels The occurrence of diﬀerent charge states is a direct consequence of the position of the defect level inside the fundamental band gap: in p-doped materials the defect state lies above the Fermi energy and is hence depopulated, whereas it is fully occupied in n-doped materials with a higher Fermi energy close to the conduction-band edge. Indeed, a charge state of (+1) has been conﬁrmed experimentally for anion vacancies at p-GaAs(110) [70] and p-InP(110) [71] and a charge state of (−1) at n-GaAs(110) [72] and n-InP(110) [73]. In a theoretical treatment the stable charge state can be identiﬁed by comparing the diﬀerent formation energies E form (q, µA , εF ) = E vac (q, Qq ) + µA + qεF − E surf ,

(16)

where we use the same notation for the total energy of the vacancy as in the previous section. The chemical potential µA of the anion atoms is controlled by the partial pressure and temperature, εF denotes the Fermi level and E surf is the total energy of the defect-free surface. The qualitative behavior of the formation energies is illustrated in Fig. 5: due to their diﬀerent slopes the stable charge state with the lowest formation energy changes from positive to negative as the Fermi energy varies between the valence-band maximum and the conduction-band minimum. In between there may be a region where the neutral vacancy is stable. The charge-transition levels are deﬁned as the values of the Fermi energy where the curves intersect and the stable charge state changes. They are given explicitly by ε+/0 = E vac (0, Q0 ) − E vac (+, Q+ ) for the transition from q = +1 to q = 0 and ε0/− = E vac (−, Q− )−E vac (0, Q0 ) for the transition from q = 0 to q = −1. All quantities in (16) are ground-state energies and can, in principle, be calculated within density-functional theory. As explained above, however, the parametrizations most commonly used in practical implementations lack

formation energy

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces

0

VA +

VA

εVBM

0

185

−

VA

ε +/0 ε 0/− Fermi energy

εCBM0

Fig. 5. Qualitative behavior of the formation energies for anion vacancies in the − 0 positive (V+ A ), neutral (VA ), and negative (VA ) charge state. The Fermi energy is limited by the valence-band maximum and the conduction-band minimum. The charge-transition levels ε+/0 and ε0/− mark the values of the Fermi energy where the stable charge state with the lowest formation energy changes

essential properties of the exact exchange-correlation functional, so that the charge-transition levels obtained in this way suﬀer from systematic errors. For a more accurate quantitative description we use the same trick as in (15) and rewrite ε+/0 as ε+/0 = [E vac (0, Q0 ) − E vac (0, Q+ )] + [E vac (0, Q+ ) − E vac (+, Q+ )]

(17)

by adding and subtracting the total energy E vac (0, Q+ ) of a conﬁguration with the atomic geometry of the positively charged vacancy but with one extra electron. In this way the charge-transition level is naturally decomposed into two distinct contributions. The ﬁrst term on the right-hand side is purely structural and describes the relaxation energy of the neutral system from the atomic structure optimized for the positive charge state to its own equilibrium geometry. It is always negative and can be calculated within density-functional theory. We obtain −0.59 eV for GaAs(110) and −0.54 eV for InP(110) when taking the asymmetric distortion into account. The second term on the right-hand side is purely electronic and equals the electron aﬃnity of the positively charged vacancy, which in a many-body framework corresponds to the lowest unoccupied state, i.e., the empty 1a defect level in the band gap. This was already calculated within the G0 W0 approximation in the preceding section and can be taken from Tables 1 and 2. In the same spirit we rewrite ε0/− as ε0/− = [E vac (−, Q− ) − E vac (0, Q− )] + [E vac (0, Q− ) − E vac (0, Q0 )] . (18) The ﬁrst term now equals the ionization potential of the negatively charged vacancy, corresponding to the highest occupied quasiparticle state. Again this is the 1a defect level, which in this case is ﬁlled with two electrons, and the G0 W0 results can be taken from the tables in the previous section.

186

Arno Schindlmayr and Matthias Scheﬄer

The second term is the energy diﬀerence between the electrically neutral system in the atomic structure optimized for the positive charge state and its own relaxed geometry. This contribution is always positive and can be obtained from density-functional theory. We obtain 0.12 eV for GaAs(110) and 0.08 eV for InP(110). The structural component is much smaller than for ε+/0 because there is no symmetry-breaking distortion in this case, only a minor reduction of the Ga–Ga bond length across the vacancy. Incidentally, the charge-transition levels within the LDA, which are usually obtained according to the deﬁnitions ε+/0 = E vac (0, Q0 ) − E vac (+, Q+ ) and ε0/− = E vac (−, Q− ) − E vac (0, Q0 ) by evaluating the total-energy diﬀerences directly, can also be decomposed into structural and electronic energy contributions. The latter are not given by the Kohn–Sham eigenvalues in Tables 1 and 2, however. Instead, they must be calculated with the help of the transition-state theorem [18] from intermediate conﬁgurations with halfinteger occupation numbers of 1/2 and 3/2 electrons, respectively. Table 3. Calculated charge-transition levels for the As vacancy at GaAs(110) in eV relative to the valence-band maximum. For ε+/0 the ﬁrst column refers to the asymmetric and the second to the constrained symmetric relaxation ε+/0

Transition level LDA (this work) LDA [3] LDA [5] G0 W0 (this work)

0.24 0.32 0.49

(0.07) (0.10) (0.32)

ε0/− 0.15 0.4 0.24 0.60

In Table 3 we summarize the results for the As vacancy at GaAs(110). In contrast to earlier studies [3, 5] that found a small energy window in which the neutral charge state is stable, our own calculation at the level of the LDA predicts ε+/0 > ε0/− if the correct asymmetric distortion is taken into account and hence a direct transition from the positive to the negative charge state, but the small energy diﬀerence is within the uncertainty of the calculation. The G0 W0 approximation, on the other hand, reverses this ordering and simultaneously moves all charge-transition levels to higher energies. The values for the constrained symmetric relaxation are merely shown for the purpose of comparison with earlier work. The deviations from earlier LDA studies, especially by Zhang and Zunger [3], are related to diﬀerences of similar magnitude in the defect states, which were already mentioned above. The results for the P vacancy at InP(110) are given in Table 4. For this material an indirect experimental measurement of ε+/0 , obtained with a combination of scanning tunneling microscopy and photoelectron spectroscopy, is available [6]. Consistent with previous studies [6, 7], we ﬁnd that the LDA signiﬁcantly underestimates the experimentally deduced value. The larger

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces

187

Table 4. Calculated charge-transition levels for the P vacancy at InP(110) Transition level LDA (this work) LDA [6] LDA [7] G0 W0 (this work) Expt. [6]

ε+/0

ε0/−

0.47 (0.39) 0.52 (0.45) 0.388 0.82 (0.79) 0.75 ± 0.1

0.54 0.576 1.09

G0 W0 result, however, lies within the error bar of the experimental measurement. We take this as a conﬁrmation of our approach and an indicator that the other defect states and charge-transition levels calculated within the same framework are also meaningful. Nevertheless, further calculations for diﬀerent systems are necessary to establish the general validity of this scheme.

6 Summary We have presented a parameter-free method for calculating defect states and charge-transition levels of point defects in semiconductors. Compared to previous studies that extracted these quantities directly from the self-consistent iteration of the Kohn–Sham equations, it apparently corrects important errors that are inherent in all jellium-based exchange-correlation functionals and employs a separation of structural and electronic energy contributions. While the former are accurately obtainable in density-functional theory, we use many-body perturbation theory and the G0 W0 approximation for the self-energy to calculate the latter with proper quasiparticle corrections. The scheme is general and can be applied to arbitrary bulk or surface defects. As an example we examined the electronic structure of anion vacancies at the (110) surfaces of III–V semiconductors. For the As vacancy at GaAs(110) our calculation indicates that all three charge states including the neutral conﬁguration are stable, in contrast to the LDA that predicts a direct transition from the positive to the negative charge state. Due to a general lack of experimental data, a direct comparison between theoretical and experimental values is only possible for the charge-transition level ε+/0 of the P vacancy at InP(110). In this case our calculation is in good agreement with the experimentally deduced result and constitutes a clear improvement over previous LDA treatments. Nevertheless, besides an improvement of experimental techniques, further developments in theoretical and computational procedures are highly desirable. Our method only opens the door to novel approaches; with present implementations the results are derived at a cost that may be infeasible for more complex systems, and the numerical uncertainty of 0.1 eV to 0.2 eV is often of the same order as the relevant energy diﬀerences. The

188

Arno Schindlmayr and Matthias Scheﬄer

study of excitons, which, e.g., play an important role at GaAs(110) [74], further requires an extension of the mathematical framework beyond single quasiparticles. Acknowledgements We thank Magnus Hedstr¨ om, G¨ unther Schwarz, and J¨ org Neugebauer for fruitful collaborations in the course of this work and Philipp Ebert for useful discussions. This work was funded in part by the EU through the Nanophase Research Training Network (Contract No. HPRN-CT-2000-00167) and the Nanoquanta Network of Excellence (Contract No. NMP-4-CT-2004-500198).

References [1] P. Ebert: Curr. Opin. Solid State Mater. Sci. 5, 211 (2001) 165 [2] V. P. LaBella, H. Yang, D. W. Bullock, P. M. Thibado, P. Kratzer, M. Scheﬄer: Phys. Rev. Lett. 83, 2989 (1999) 165 [3] S. B. Zhang, A. Zunger: Phys. Rev. Lett. 77, 119 (1996) 166, 182, 183, 186 [4] H. Kim, J. R. Chelikowsky: Phys. Rev. Lett. 77, 1063 (1996) 166 [5] H. Kim, J. R. Chelikowsky: Surf. Sci. 409, 435 (1998) 166, 182, 183, 186 [6] P. Ebert, K. Urban, L. Aballe, C. H. Chen, K. Horn, G. Schwarz, J. Neugebauer, M. Scheﬄer: Phys. Rev. Lett. 84, 5816 (2000) 166, 167, 170, 179, 186, 187 [7] M. C. Qian, M. G¨ othelid, B. Johansson, S. Mirbt: Phys. Rev. B 66, 155326 (2002) 166, 182, 183, 186, 187 [8] M. C. Qian, M. G¨ othelid, B. Johansson, S. Mirbt: Phys. Rev. B 67, 035308 (2003) 166, 179 [9] P. Hohenberg, W. Kohn: Phys. Rev. 136, B864 (1964) 166, 168 [10] W. Kohn, L. J. Sham: Phys. Rev. 140, A1133 (1965) 166, 168, 169 [11] J. P. Perdew, K. Burke, M. Ernzerhof: Phys. Rev. Lett. 77, 3865 (1996) 166 [12] G. Lengel, R. Wilkins, G. Brown, M. Weimer: Phys. Rev. Lett. 72, 836 (1994) 166, 168, 184 [13] A. G¨ orling: Phys. Rev. A 54, 3912 (1996) 166, 171 [14] V. Fiorentini, M. Methfessel, M. Scheﬄer: Phys. Rev. B 47, 13353 (1993) 167 [15] M. Hedstr¨ om, A. Schindlmayr, M. Scheﬄer: phys. stat. sol. (b) 234, 346 (2002) 167, 181, 183 [16] L. Sorba, V. Hinkel, H. U. Middelmann, K. Horn: Phys. Rev. B 36, 8075 (1987) 168 [17] B. Reihl, T. Riesterer, M. Tschudy, P. Perfetti: Phys. Rev. B 38, 13456 (1988) 168 [18] J. C. Slater: Adv. Quant. Chem. 6, 1 (1972) 169, 173, 186 [19] J. F. Janak: Phys. Rev. B 18, 7165 (1978) 169, 173 [20] C.-O. Almbladh, U. von Barth: Phys. Rev. B 31, 3231 (1985) 170 [21] J. P. Perdew, M. Levy: Phys. Rev. Lett. 51, 1884 (1983) 170 [22] L. J. Sham, M. Schl¨ uter: Phys. Rev. Lett. 51, 1888 (1983) 170 [23] A. G¨ orling, M. Levy: Phys. Rev. A 50, 196 (1994) 170

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces

189

[24] A. G¨ orling: Phys. Rev. B 53, 7024 (1996) 170 [25] M. St¨ adele, J. A. Majewski, P. Vogl, A. G¨ orling: Phys. Rev. Lett. 79, 2089 (1997) 170, 171 [26] R. W. Godby, M. Schl¨ uter, L. J. Sham: Phys. Rev. B 37, 10159 (1988) 170 [27] T. Kotani: J. Phys.: Condens. Matter 10, 9241 (1998) 170 [28] J. P. Perdew, A. Zunger: Phys. Rev. B 23, 5048 (1981) 171 [29] D. M. Ceperley, B. J. Alder: Phys. Rev. Lett. 45, 566 (1980) 171 [30] L. Kleinman, D. M. Bylander: Phys. Rev. Lett. 48, 1425 (1982) 171 [31] M. Bockstedte, A. Kley, J. Neugebauer, M. Scheﬄer: Comput. Phys. Commun. 107, 187 (1997) 171 [32] M. Fuchs, M. Scheﬄer: Comput. Phys. Commun. 119, 67 (1999) 171 [33] J. L. A. Alves, J. Hebenstreit, M. Scheﬄer: Phys. Rev. B 44, 6188 (1991) 171, 176 [34] O. Madelung, U. R¨ ossler, M. Schulz (Eds.): Landolt-B¨ ornstein: Numerical Data and Functional Relationships in Science and Technology – New Series, vol. III/41A (Springer, Berlin, Heidelberg 2001) 171, 176 [35] G. D. Mahan: Many-Particle Physics, 3rd ed. (Springer, Berlin, Heidelberg 2000) 171 [36] L. Hedin: Phys. Rev. A 139, 796 (1965) 172, 174 [37] W. von der Linden, P. Horsch: Phys. Rev. B 37, 8351 (1988) 172 [38] G. E. Engel, B. Farid: Phys. Rev. B 47, 15931 (1993) 172 [39] M. S. Hybertsen, S. G. Louie: Phys. Rev. B 34, 5390 (1986) 173 [40] I. D. White, R. W. Godby, M. M. Rieger, R. J. Needs: Phys. Rev. Lett. 80, 4265 (1998) 173 [41] M. Rohlﬁng, N.-P. Wang, P. Kr¨ uger, J. Pollmann: Phys. Rev. Lett. 91, 256802 (2003) 173 [42] O. Pulci, F. Bechstedt, G. Onida, R. Del Sole, L. Reining: Phys. Rev. B 60, 16758 (1999) 173 alez, R. W. Godby: Phys. Rev. B 64, 235106 [43] A. Schindlmayr, P. Garc´ıa-Gonz´ (2001) 173 [44] B. Holm, U. von Barth: Phys. Rev. B 57, 2108 (1998) 174 [45] W.-D. Sch¨ one, A. G. Eguiluz: Phys. Rev. Lett. 81, 1662 (1998) 174 [46] W. Ku, A. G. Eguiluz: Phys. Rev. Lett. 89, 126401 (2002) 174 [47] T. Kotani, M. van Schilfgaarde: Solid State Commun. 121, 461 (2002) 174 [48] M. L. Tiago, S. Ismail-Beigi, S. G. Louie: Phys. Rev. B 69, 125212 (2004) 174 [49] K. Delaney, P. Garc´ıa-Gonz´ alez, A. Rubio, P. Rinke, R. W. Godby: Phys. Rev. Lett. 93, 249701 (2004) 174 [50] C. Friedrich, A. Schindlmayr, S. Bl¨ ugel, T. Kotani: Phys. Rev. B 74, 045104 (2006) 174 [51] E. L. Shirley, X. Zhu, S. G. Louie: Phys. Rev. B 56, 6648 (1997) 174 [52] R. W. Godby, M. Schl¨ uter, L. J. Sham: Phys. Rev. B 35, 4170 (1987) 174, 175 [53] X. Zhu, S. G. Louie: Phys. Rev. B 43, 14142 (1991) 174 [54] M. Rohlﬁng, P. Kr¨ uger, J. Pollmann: Phys. Rev. B 48, 17791 (1993) 174, 175 [55] X. Zhu, S. B. Zhang, S. G. Louie, M. L. Cohen: Phys. Rev. Lett. 63, 2112 (1989) 175, 178 [56] O. Pulci, G. Onida, R. Del Sole, L. Reining: Phys. Rev. Lett. 81, 5374 (1998) 175, 178 [57] S. J. Jenkins, G. P. Srivastava, J. C. Inkson: Surf. Sci. 254, 776 (1996) 175

190

Arno Schindlmayr and Matthias Scheﬄer

[58] M. M. Rieger, L. Steinbeck, I. D. White, H. N. Rojas, R. W. Godby: Comput. Phys. Commun. 117, 211 (1999) 175, 177 [59] L. Steinbeck, A. Rubio, L. Reining, M. Torrent, I. D. White, R. W. Godby: Comput. Phys. Commun. 125, 105 (2000) 175 [60] H. J. Monkhorst, J. D. Pack: Phys. Rev. B 13, 5188 (1976) 177 [61] A. Schindlmayr: Phys. Rev. B 62, 12573 (2000) 177 [62] J. Neugebauer, M. Scheﬄer: Phys. Rev. B 46, 16067 (1992) 178 [63] P. Eggert, C. Freysoldt, P. Rinke, A. Schindlmayr, M. Scheﬄer: Verhandl. DPG (VI) 40, 2/491 (2005) 179 [64] N. D. Lang, A. R. Williams: Phys. Rev. B 18, 616 (1978) 179 [65] P. J. Braspenning, R. Zeller, A. Lodder, P. H. Dederichs: Phys. Rev. B 29, 703 (1984) 179 [66] M. Scheﬄer, C. Droste, A. Fleszar, F. M´ aca, G. Wachutka, G. Barzel: Physica B 172, 143 (1991) 179 [67] J. Bormet, J. Neugebauer, M. Scheﬄer: Phys. Rev. B 49, 17242 (1994) 179 [68] G. Fratesi, G. P. Brivio, L. G. Molinari: Phys. Rev. B 69, 245113 (2004) 179 [69] S. Aloni, I. Nevo, G. Haase: Phys. Rev. B 60, R2165 (1999) 184 [70] K. J. Chao, A. R. Smith, C. K. Shih: Phys. Rev. B 53, 6935 (1996) 184 [71] P. Ebert, X. Chen, M. Heinrich, M. Simon, K. Urban, M. G. Lagally: Phys. Rev. Lett. 76, 2089 (1996) 184 [72] C. Domke, P. Ebert, K. Urban: Phys. Rev. B 57, 4482 (1998) 184 [73] P. Ebert, K. Urban, M. G. Lagally: Phys. Rev. Lett. 72, 840 (1994) 184 [74] O. Pankratov, M. Scheﬄer: Phys. Rev. Lett. 75, 701 (1995) 188

Index alignment, 176, 177 anion vacancy, 166, 179–182, 184–187 antisite, 168 asymmetric, 166, 179, 180, 182, 183, 185, 186 band bending, 166 band edge, 173, 178, 184 band structure, 166, 167, 169, 170, 172–177 Brillouin zone, 176–178, 181, 182 bulk, 165, 171, 173, 174, 176–178, 187 charge state, 167, 170, 179, 180, 182–187 charge-transition level, 165–167, 170, 171, 184–187 charge-transition state, 169, 172, 173, 184, 186, 187 chemical potential, 184 cleavage, 168, 176

conduction band, 176, 178, 184 coordination, 179 core-valence interaction, 167, 174, 182 correlation, 167, 169–172, 177, 180 dangling bond, 176, 177, 179 decay, 172 defect state, 180 density of states, 166 density-functional theory, 165–168, 170–172, 178, 179, 182, 184–187 dielectric function, 173 dipole, 178 dispersion, 176, 177, 180, 181 distortion, 166, 179, 182, 183, 185, 186 doping, 168, 180 eigenstates, 171, 172 eigenvalues, 165, 166, 168, 169, 172–174, 177, 179, 186 electron aﬃnity, 170, 172, 182, 185

Quasiparticle Calculations for Point Defects at Semiconductor Surfaces exact exchange, 185 exchange-correlation, 166–170, 172, 185, 187 excitation, 165, 167–169, 171–173 exciton, 188 Fermi level, 165, 167–169, 178, 184 formation energy, 184 functional derivative, 169, 174 fundamental gap, 170, 174, 178 G0 W0 approximation, 165, 168, 172–180, 182–187 GaAs(110) surface, 176 GaN, 167 gap states, 168 general gradient approximation (GGA), 166, 167, 170 Green’s function, 165, 171–174, 179, 181 ground state, 165, 168, 170, 171, 177, 184 Hamiltonian, 171 Hartree, 168, 169, 179 Hedin, 174 Heisenberg picture, 171 hole, 166, 172, 173, 180 hopping integral, 180, 182 InP(110) surface, 176 ionization potential, 170, 172, 185 Lagrange parameter, 169 LDA, 166–171, 173, 176, 177, 181–184, 186, 187 many-body perturbation theory, 171 multipole, 178

191

phonon, 172 photoemission, 166, 170, 184 plane wave, 171, 173–175, 179 plasmon, 172, 175, 178 point defect, 165–168, 170 polarizability, 173, 175, 178 polarization, 173, 178, 179 pseudopotential, 167, 171, 174, 182 quasiparticle, 165, 167, 169–176, 179, 181–183, 185, 187, 188 quasiparticle equation, 172 random-phase approximation, 170, 173, 175, 178 real space, 175, 177 reciprocal space, 175 relaxation, 166, 167, 171, 176, 179, 180, 182, 183, 185, 186 scanning tunneling microscopy (STM), 165, 166, 168, 184, 186 scattering, 172 screening, 173, 183 self-energy, 165, 167, 168, 172–183, 187 Slater transition state, 169 spin, 169, 182 supercell, 177–180, 182 surface, 165–169, 171, 173, 176–182, 184, 187 surface band, 176 symmetry, 166, 176, 179, 180, 182, 183, 186 termination, 177 tight binding, 175, 180, 181 total energy, 168–170, 179, 182, 184, 185

nonlocal, 167, 172, 174, 179, 180 periodic, 175, 177, 178, 180 perturbation, 165, 167–169, 171–173, 179, 187

valence band, 169, 170, 176–178, 180, 182, 184 zincblende lattice, 176

Multiscale Modeling of Defects in Semiconductors: A Novel Molecular-Dynamics Scheme G´ abor Cs´anyi1 , Gianpietro Moras2, James R. Kermode1 , Michael C. Payne1, Alison Mainwood2 , and Alessandro De Vita2,3 1

2

3

Cavendish Laboratory, University of Cambridge, Madingley Road, CB3 0HE, United Kingdom {gc121,jrk33,mcp1}@cam.ac.uk Department of Physics, King’s College London, Strand, London, United Kingdom {gianpietro.moras,alison.mainwood,alessandro.de vita}@kcl.ac.uk DEMOCRITOS National Simulation Center and CENMAT-UTS, Trieste, Italy

Abstract. Now that the modeling of simple semiconductor systems has become reliable, accurate and routine, attention is focusing on larger scale, more complex simulations. Many of these necessarily involve multiscale aspects and can only be tackled by addressing the diﬀerent length scales simultaneously. We discuss some of the types of problems that require multiscale approaches. Finally we describe the LOTF (learn-on-the-ﬂy) hybrid scheme with a series of examples to show its versatility and power.

1 Introduction Over the last twenty years, the improvement in computational modeling of materials problems has been remarkable. This is due to the signiﬁcant increase in the capacity and speed of computers matched (and arguably surpassed) by the ingenuity of those who write the computational codes. It would be invidious to do other than refer the reader to other Chapters in this volume to support these assertions. However, these advances are also challenged by the complexities of systems that need to be modeled. There has been a great deal written about diﬀerent scales of modeling, usually where the results of calculations on one scale are used to determine the parameters that are used to model the material at a larger scale. Many of the embedding approaches are designed in this way. Additionally, where dynamic processes are being modeled, it may be useful to treat diﬀerent timescales by diﬀerent means. A combination of molecular-dynamics and quantum-mechanical modeling using a ﬁrst-principles technique for example, can model only a few hundred atoms for a period of a few picoseconds. Using more approximate methods, one may be able to extend the number of atoms to hundreds or thousands, or the time period by a few orders of magnitude. In order to extend the time period to the several seconds for some biological processes, D. A. Drabold, S. K. Estreicher (Eds.): Theory of Defects in Semiconductors, Topics Appl. Physics 104, 193–212 (2007) © Springer-Verlag Berlin Heidelberg 2007

194

G´ abor Cs´ anyi et al.

or years or aeons for geological ones, the activation energies and reaction pathways from the static or picosecond MD calculations have to be inserted into Monte Carlo models or analytical rate equations and their variants. In this Chapter, we suggest a selection of problems where the complexity of such an approach makes it diﬃcult or impossible to treat every length scale with a separate calculation, largely because the physical processes on the various length scales are strongly coupled to each other. We then go on to describe a method that allows some of these complex problems to be tackled.

2 A Hybrid View Radiation or Implantation Damage An important technique for doping semiconductors is to implant the dopant with an energy (or range of energies) that determines the location of the doped area or layer. However, in this process damage in the form of vacancies and interstitials and their complexes are formed, some of which can be electrically active. Annealing may heal most of the damage (e.g., [1]), but invariably some defects remain and can be detected by photoluminescence and positron-annihilation spectroscopy [2]. Intrinsic defects have very low activation energies for diﬀusion, so they may migrate long distances before they are trapped by dopants, or other radiation-induced defects. The same problems arise when the radiation damage of silicon particle detectors is modeled. A very comprehensive empirical analysis of the processes involved in the annealing of damage was undertaken by Huhtinen [3], but he did not attempt to understand the microscopic processes. However, his analysis showed that some long-range migration of radiation damage products and displaced impurities was occurring. It is well within the current state-of-the-art to model the dynamics of the initial impact of a particle or ion with a silicon atom in a small ﬁnite cluster (or periodic supercell), and the subsequent displacement of that atom. If the damage trail formed by the particle, the knock-on atom and any further damage products can all be contained in the ﬁnite cluster or supercell, then a reasonable model of the full process can be built up. More commonly, though, one or more of the damage products may exit the cluster in a direction not easily predicted from the initial conditions, or the intrinsic defects may migrate longer distances than the dimensions of the largest clusters. The problem is then to construct a method to follow the important species such that their interactions are treated with the required level of accuracy, while keeping the whole problem to within acceptable computational limits. Point-Defect Diﬀusion A very similar problem is the annealing of point defects in semiconductors, where an additional complication is the chemical interaction between the im-

Multiscale Modeling of Defects in Semiconductors

195

purity and the defects in the host lattice. As an example, atomic hydrogen in silicon has a stable site in a bond-centered position, which is only stable when the bond is greatly elongated – a self-trapped site [4]. It also has a metastable site at the tetrahedral site, where the migration barrier is very low. To model the migration, a full molecular-dynamics model must be used, but it must also be capable of following the long-range migration of the hydrogen through the tetrahedral-site routes. For hydrogen, a proper model using quantum mechanics for the proton as well as for the electrons is necessary, and has been developed in a limited way [5], but the principles illustrated by this example apply to the diﬀusion of many other impurities and defects. Classical interatomic potentials are available for some of the simpler chemical systems, but they tend to be constructed for bonding situations that are close to equilibrium, and have rather more questionable validity where the local environment of the host–defect complex is greatly distorted. Both the relative stability and the rate of migration of point defects can be altered by the presence of strain ﬁelds and strain gradients that are ubiquitous in semiconductor systems. While the point defects typically alter the local atomic structure only on a scale of a nanometer, the strain ﬁelds of epitaxial layers extend much further due to lattice mismatch. Dislocations also give rise to a slow-decaying strain ﬁeld. This means that while the quantum-mechanical treatment of new bonding arrangements near each individual defect can be accomplished using a few hundred atoms, the environment in which the diﬀusion and possible interaction of the defects takes place needs to be represented by tens of thousands of atoms or more. Dislocation Motion The strength of real materials is dominated by the behavior of its dislocations. Around the core of a dislocation, there is a 1-D region in which the bonding of the host is distorted. Once there is a kink in the dislocation, by which means it moves, the distortions become much more pronounced, and this part of the crystal must be modeled by particularly accurate techniques, see Fig. 1 for a schematic view. Moreover, the movement of the kink means that this highly distorted region also moves, which typically involves bond breaking and forming. More complexity arises when dislocations interact with each other or with grain boundaries, and they may also be sources (or sinks) for point defects. Grain Boundaries Nanocrystalline silicon and other semiconductors are becoming more and more technologically important. Similarly, the crystal quality of many of the newer wide-bandgap semiconductors used in electronics (the nitrides, silicon carbide, diamond) is not nearly as perfect as silicon – it is no longer acceptable to ignore dislocations and grain boundaries when trying to understand the

196

G´ abor Cs´ anyi et al.

Fig. 1. Schematic view of a screw dislocation with a double kink. In covalent materials, dislocations move by the formation of double kinks. Gray circles approximately indicate the region in which active rebonding takes place

degradation or limitations of their electronic properties. The exact role that grain boundaries play in plasticity is far from being completely understood. In particular, the grain boundaries need to be investigated as sources and sinks for dislocations. Signiﬁcant departure from the equilibrium crystalline structure is present. This takes the form of a mixture of locally disordered bonding and longer-range elastic distortion – a situation that needs a multiscale description. Furthermore, the grain boundaries can act as traps for dopants, electrons and holes, adding to the local chemical complexity. Once again, although the longer-range interactions are well described by empirical potentials, the description of the local chemistry requires quantum-mechanical accuracy. Fracture Fracture is perhaps the textbook example of a multiscale problem. The importance of understanding both the catastrophic failure of brittle materials and the conditions under which normally ductile materials become brittle cannot be overemphasized. Classical continuum models of the stress ﬁeld do an excellent job in predicting the enhancement of stress near the crack tip. However, the divergence of components of the stress tensor at the tip imply that elasticity theory must break down in this region since it is not applicable when distortions go beyond the harmonic range. Indeed, during failure the interatomic bonds are stretched well into the anharmonic region and ultimately are broken. In covalent systems this leaves dangling bonds, whose energetics can only be described by a fully quantum-mechanical treatment. Moreover,

Multiscale Modeling of Defects in Semiconductors

197

Fig. 2. Displacement ﬁeld of a propagating crack under uniaxial tension in the opening mode (analytical continuum solution)

the inﬂuence of impurities and corrosive agents on failure processes has never been explored theoretically at this level of detail, yet there is evidence for the critical role they play, e.g., in fracture of silicon notches in a wet environment [6, 7] and in the controlled fabrication of thin Si ﬁlms by hydrogen implantation [8–10]. The key aspect of brittle fracture that makes it amenable to hybrid modeling is that the propagating crack is atomically sharp [11]. Thus, although the crack surface that is opening up is two-dimensional, the active region, where bonds are being broken, is a one-dimensional line, perpendicular to the direction of propagation. The strongly coupled multiscale aspect of crack propagation comes about because the opening crack gives rise to a stress ﬁeld √ that has a singularity (in the continuum approximation), diverging as 1/ r where r is the distance ahead of the crack tip, and in turn, it is this large stress that breaks the bonds and thus advances the crack forward. The extension of the stress ﬁeld is nevertheless very large. If we wish to represent all the atoms that contribute signiﬁcantly to elastic relaxation as the stress ﬁeld advances, we need to include several tens of thousands of atoms. Only then can we hope to be able to quantitatively predict critical loading levels.

3 Hybrid Simulation The general pretext in a hybrid simulation is that we are going to use two diﬀerent physical models to describe the system. It is understood that one of these is accurate enough to describe the physics of the activated regions properly, which, in practice, means we will use some sort of quantum-mechanical

198

G´ abor Cs´ anyi et al.

description, e.g., a tight-binding (TB) formalism, or indeed density-functional theory (DFT); henceforth this ﬁrst model will be referred to as the QM model. Using such sophisticated modeling comes at a price, in the very real terms of computing costs. With the currently available hardware, it is typically possible to simulate thousands of atoms using TB, and hundreds of atoms using DFT for tens of picoseconds. These are evidently modest capabilities if we are faced with any of the above problems, and hence we need to employ a second model, to be used in parts of the system that are not activated at a given instant in time. This second model should capture correctly the basic topology of bonding and the response to small deformations, while at the same time be relatively inexpensive to compute. Empirical atomistic models ﬁt the bill perfectly. It should be noted that the recent progress in the ﬁeld of empirical “ball and spring”-type modeling has been in the direction of reﬁning the analytical forms in an attempt to extend their range of applicability [12–15]. However, once we have decided to employ a hybrid technology there is little beneﬁt in complicating this second, classical model . It is more important that it is as robust as possible and uses only a small number of free parameters since in any particular situation where the classical model would fail we will use the QM model. In theory, one could consider not just two models, but a whole hierarchy of ever more coarse-grained descriptions of physical systems. The next one up from classical atomistic models would be a continuum ﬁnite element model. In our experience, the cost ratio between the QM and the classical models is so extreme, that for all intents and purposes the classical atoms can be regarded as “free” in most applications. If we are at liberty to consider millions of classical atoms, the necessity of a continuum description is less pressing. The standard technical tools of classical molecular-dynamics can thus be used on this large, atomistically modeled region to impose the correct elastic or thermal boundary conditions of the problem under study. The boundary regions between the QM and classical zones need, on the contrary, a special treatment and a separate discussion. Boundary Problems It is not hard to recognize that the biggest challenge in designing a hybrid simulation scheme is to overcome the problems associated with the artiﬁcial boundary that separates regions of the system that are described by the two diﬀerent models. In fact there are two distinct issues that have to be addressed. The ﬁrst one generally goes under the name of termination, and it concerns the accurate computation of forces on atoms near the boundary. If we attempt the most naive partitioning and simply omit the classical atoms from the quantum-mechanical calculation and vice versa, the atoms close to the boundary will behave like those near an open surface. This is clearly wrong. To get accurate forces on these atoms, we should “trick” the system into believing that these surface atoms are really bulk atoms, while avoiding

Multiscale Modeling of Defects in Semiconductors

199

implicit inclusion of all the atoms from the other region (which is the point of the hybrid simulation in the ﬁrst place). The next simplest solution is to use so-called “termination atoms”, which is standard practice in the hybrid simulation schemes of biological systems (called “QM/MM” models [16]). Here, atoms from the region we are presently not considering are also taken away, but wherever covalent bonds are broken by this removal, a monovalent atom (typically a hydrogen) is placed to saturate the dangling bond. For the classical model, this procedure can be seen to be suﬃcient. The classical description of covalent bonding is very near-sighted, i.e., the energy of the “last” classical atom can be essentially perfectly recovered using the terminator-atom technique. Moreover, since the classical total energy is usually expressed as a simple sum of atomic energies, the terminator atom can simply be excluded from this sum. It has to be noted that if we are dealing with a strongly ionic material, even our classical model will not be so near-sighted, and the problems that are usually associated with the termination of the quantum region in standard QM/MM treatments apply to the classical part as well. Terminating the quantum-mechanical subsystem is more tricky. Quantum mechanics is not a nearest-neighbor model, so even if our free surface is terminated by monovalent terminator atoms, the atoms close to the boundary will feel an artiﬁcial environment. Secondly, it is more or less impossible in any QM scheme to exclude the terminator atoms from the total energy in a consistent fashion, so we have just traded artiﬁcial surface atoms for artiﬁcial terminator atoms – not an altogether satisfactory situation. These two problems are solved by the same trick: we stop worrying about the total energy and concentrate on obtaining accurate forces on the atoms in the QM region, which is achieved by allowing a thicker termination region, rather than just terminator atoms. In other words, we include a shell of nominally classical atoms (a thickness of about a nanometer is suﬃcient in silicon) in the QM calculation, which ensures that the forces that we compute for the QM atoms are accurate. Now in contrast to the total energy, the forces are local quantities, so it is trivial to exclude the forces on atoms in the “contaminated” termination region from the subsequent calculations: from the QM calculation, we only keep the forces on atoms in the original QM region, not the termination region. Mechanical Matching And thus we squarely arrive at the second major issue associated with the boundary. Suppose we have computed forces with the desired method in each region, we now have to propagate the system forward in time along its trajectory. On the two sides of the boundary, we originally resolved to compute with diﬀerent models, but these yield diﬀerent, and incompatible trajectories for the atoms on the two sides. The set of forces we just computed (from two diﬀerent models) are not the derivatives of some total energy and do

200

G´ abor Cs´ anyi et al.

not necessarily add up to zero for an isolated system. If we simply plugged them into an integrator formula (e.g., velocity, Verlet [17]), the trajectory may be unstable. The solution to this problem forms the basis of our recently developed method [18–20] called “learn on the ﬂy” (LOTF): instead of using the set of forces directly, we consider a simplistic universal “ball and spring” model, but allow every spring to be diﬀerent, and also to change with time. At every time step, the set of forces we computed using the classical and quantum models are used as targets in an optimization of the spring constants, which are tuned until the forces derived from the universal model match their targets. The trajectory integrator is then used on the universal model, whose forces are now consistent across the whole system. The universal model in eﬀect “interpolates” across the boundary, closely matching the target on both sides, while maintaining global consistency. In practice, a number of simpliﬁcations immediately arise. The target forces do not have to be computed at every time step, as the universal model can be considered an instantaneous interpolator not just in space, but also in time and so it can be used with unchanged spring constants for a few time steps without incurring a signiﬁcant deviation from the true hybrid trajectory. More importantly however, the scheme is greatly simpliﬁed if the universal model is chosen to be the classical model itself! Thus an alternative and complementary point of view is that we take the classical model and remove the constraints from its parameters, allowing them to be diﬀerent for each atom. We then tune them in the QM region to incorporate the quantum-mechanically accurate force information. Another important consequence of this scheme is that we are at liberty to move the QM region in space without upsetting the stability of the simulation. The universal model will adapt to the target forces at each optimization, regardless of where and how we obtained the set of target forces. The use of a thick transition region to pad the quantum-mechanical calculation means that as we shift the quantum region in space together with its padding the Hamiltonian in the nominal quantum region changes smoothly.

4 The LOTF Scheme The Universal Potential We now describe in detail the LOTF scheme that is based on the above ideas. The choice of the universal force model that we will use to interpolate the quantum and classical models is crucial. There are two obvious choices. One, already alluded to above, is to use the classical model itself. This means that there would only be two force models in our scheme, a classical model with variable parameters and a quantum model. Most of the applications in the following sections have been carried out using this approach. An alternative and more ﬂexible choice is to pick a universal force model that oﬀers a good

Multiscale Modeling of Defects in Semiconductors

201

Fig. 3. Examples of cubic spline potentials for the two-body (top) and three-body terms (bottom). The large dots represent spline knots, the red dotted lines are the corresponding functions of the Stillinger–Weber potential [22]

compromise between expressive power and robustness. In particular, we will be changing the model parameters on the ﬂy, so we would like the potential form to change smoothly as we change these parameters. In our search for the parameter set optimized at any given point in the simulation, we will make use of gradient search techniques, so the derivative of the potential with respect to its parameters should be straightforward and easy to evaluate. Keeping the bond lengths and bond angles as fundamental coordinates, a cubic spline functional form ﬁts the above criteria [21]. For the two-body term, we can take a spline with four knots (e.g., at r = {1.5, 2.0, 2.5, 3.5} ˚ A for Si, for other elements scaled appropriately by the atomic radius). The spline function is completely determined by its values at the knot points and its derivatives at the two endpoints. We ﬁx both the value and the derivative at the outer endpoint to be zero, and at the inner endpoint to match the corresponding values of the quantum model for a dimer. This leaves two free parameters, the value of the spline at the two inner knots. Keeping these two values negative guarantees the existence of a single minimum in the spline function between the endpoints. For the three-body term, we could keep the traditional quadratic form in the cosine of the bond angle θ, but with a variable curvature and position of the minimum. To allow more ﬂexibility, and in particular, an asymmetric angular dependence, we can again take a cubic spline of cos θ, with two knots at −1 and 1, the free parameters are then the values and derivatives at the endpoints. As long as we restrict the derivatives to have the appropriate sign,

202

G´ abor Cs´ anyi et al.

we can guarantee that the spline will have a single minimum in (−1, 1) for any set of values of the parameters. Figure 3 shows a pictorial illustration of the splines. Since the spline functions are linear functions of the values at the knot points, our free parameters, evaluating the splines and their derivatives at ﬁxed atomic positions for different parameter values is trivial and fast. Parameters Since we want to optimize potential parameters associated with atoms close to the quantum region, the choice of initial values is important. Unless the elastic constants of our classical and quantum models match closely, acoustic waves will partially reﬂect from the artiﬁcial quantum/classical boundary. Therefore, the starting values of classical parameters have to be set to match the elastic constants of our quantum model. During the dynamics, as the quantum region moves, we have two choices for atoms that are no longer in the quantum region: either we reset the classical parameters to their initial values, or we leave them with the last-ﬁtted parameters. Which is best depends on the application. In the case of defect diﬀusion, once the defect leaves a particular area, it makes sense to reset the parameters. In other cases, if the physical eﬀects in the quantum region have resulted in some permanent topological change, e.g., the opening of a new surface, possibly followed by surface reconstruction, we might want to keep the last-ﬁtted parameters, as they could give a better description of the new topology than the original parameters. It seems diﬃcult to formulate an optimal strategy for the general case. Algorithm The following sequence of steps constitutes the hybrid scheme, a graphical illustration is shown in Fig. 4. 1. Initialize universal force-model parameters. 2. Extrapolate the atomic trajectory for n steps using ﬁxed model parameters. 3. Identify atoms that need quantum treatment. This is done using geometric and topological criteria, e.g., atoms are selected if they are under- or overcoordinated. For each new application, a suitable selection criterion has to be designed that captures the relevant processes. The user-deﬁned goal of the calculation may determine the exact recipe used here. Indeed in calculations involving surface-chemical reactions in a slab geometry, we may choose to treat quantum-mechanically only one surface of the slab, thus eﬀectively halving the accurately rendered area but doubling the simulation time for a given computer budget.

Multiscale Modeling of Defects in Semiconductors

203

Fig. 4. Predictor–corrector-style parameter ﬁtting. The black and red lines represent the predictor and corrector part of the trajectory, respectively. The gray circles denote the assumed domain of validity of the newly ﬁtted parameters at each ﬁt point (black dots)

4. Quantum-mechanical calculations are carried out to obtain accurate forces on the selected quantum atoms. 5. Optimize the force-model parameters to match the target forces both in the quantum and classical regions. 6. Interpolate the trajectory over the previous n steps between the old and new parameters. This achieves a smooth evolution of parameters in time. 7. Back to 2.

5 Applications Point Defects We now present a series of applications of the LOTF scheme in silicon. In all cases, the classical model is that of Stillinger–Weber [22] and, unless stated otherwise, the quantum model is empirical tight-binding with various parametrizations [23,24]. The ﬁrst application is more of a quantitative test of the algorithm, rather than a real application that necessitates a hybrid methodology. We consider the diﬀusion of point defects in crystalline Si, and show that the LOTF scheme, using a spherical QM region around the moving defect, recovers the same diﬀusion coeﬃcient as that calculated from a fully quantum-mechanical trajectory, while both are signiﬁcantly diﬀerent from the case of a purely classical trajectory. Figure 5 shows the diﬀusivity as a function of temperature for a vacancy in silicon calculated in three diﬀerent ways. The LOTF simulations have been performed with two diﬀerent QM

204

G´ abor Cs´ anyi et al.

Fig. 5. Vacancy diﬀusion rate in Si as a function of inverse temperature, as computed using fully quantum (black ), classical (blue) and hybrid (red ) models. The unit cell had 63 atoms

packages (diﬀerent orthogonal tight-binding parametrizations), which – not surprisingly – give diﬀerent values. Critically however, the LOTF simulation reproduces the correct curve, corresponding to whichever QM package was used to get the target forces. Further details can be found in [19] and [20]. Figure 6 shows the mean square displacement of a hydrogen atom, diﬀusing in crystalline silicon at 1000 K. This test shows up an interesting aspect of the LOTF simulation. Because the algorithm retunes the classical model continuously, it eﬀectively uses a time-dependent Hamiltonian, and thus we can no longer deﬁne a total energy that is a constant of motion. A slow (local) heating or cooling of the systems may occur during microcanonic simulations, or in constant-temperature simulations using an inappropriately tuned thermostat, in spite of the forces being all the time accurate within a few per cent. The problem is, however, lifted in the canonic ensemble if a suitable thermostat is used to stabilize the dynamics. In the present case, with two diﬀerent atomic species and a large mass ratio (∼ 28), a simple velocityrescaling thermostat is unable to maintain the correct kinetic temperature for both the hydrogen and the silicon atoms. This problem can be corrected with the use of a more sophisticated thermostat. Figure 7 shows the temperature evolution of the same system, where instead of a real QM engine, LOTF was used to track the classical forces, but the force on the H atoms was scaled by 0.9. The same behavior is observed as shown in Fig. 6: without a thermostat, the system is unstable. With a simple velocity-rescaling thermostat, the kinetic temperature of the hydrogen is diﬀerent from the system (in this case, much larger), while using a Langevin thermostat [25] eliminates this discrepancy. The Langevin thermostat adds a dissipative and a ﬂuctuat-

Multiscale Modeling of Defects in Semiconductors

205

Fig. 6. Mean square displacement of a H atom diﬀusing in Si. Quantum and classical runs are represented by black, blue lines, respectively. The green curve corresponds to the hybrid simulation with a Nos´e–Hoover thermostat, which is unable to maintain, by itself, the correct kinetic temperature of the H atom. Once this is corrected for results match the diﬀusion rate of the fully quantum-mechanical simulation (red line)

ing term to the forces and these are precisely balanced to achieve the desired temperature. In contrast to other schemes, the Langevin thermostat does not rely on eﬃcient coupling of phonons of the hydrogen and the bulk, but couples to each particle directly and separately. Dislocation Glide To demonstrate a simple application of the hybrid scheme in a system that deﬁnitely needs quantum-mechanical accuracy yet is already too large for an ordinary simulation, we consider the glide of partial dislocations. Silicon partial dislocations move by forming kinks that zip along the dislocation line. The most prevalent partial dislocation in silicon is the 30◦ partial, and the kink that most easily forms and migrates on it is the left kink [26]. Figure 8 shows a pair of such partials, oppositely directed, so that the whole unit cell is periodic, and the partials enclose a stacking fault. The unit cell is also skewed slightly, thus forcing the existence of a left kink on each partial. In a molecular-dynamics simulation at high temperature (900 K to 1100 K), the partials move toward each other, and eventually annihilate, leaving behind a number of scattered point defects (mostly fourfold-coordinated

206

G´ abor Cs´ anyi et al.

Fig. 7. Temperature evolution of a hydrogen atom in a 64-atom silicon cell using diﬀerent thermostats with the hybrid scheme. The top panel shows that in such a small system, there is a signiﬁcant energy drift due to the time-dependent Hamiltonian. The middle panel shows that a simple velocity-rescaling thermostat that, like the Nos´e–Hoover, couples to the entire system via one extra degree of freedom to the entire system, is unable to maintain the correct kinetic temperature for the light H atom. The bottom panel shows that a more sophisticated Langevin thermostat, which couples to each atom individually, maintains the correct temperature for all species of atoms

defects [27]). There are a number of salient features of the LOTF simulation that are worth pointing out and that are not observed in a purely classical simulation. First, the glide is an order of magnitude faster in the hybrid simulation. This does not just indicate a lower energy barrier for kink migration, but the conﬁgurations that are most prevalent in the hybrid simulation are very diﬀerent from those in the classical case. The most striking example is the equilibrium state of the left kink itself, shown in Fig. 9. Although the equilibrium conﬁgurations in the quantum and classical models agree at zero temperature, at high temperature, the quantum-mechanical free-energy minimum corresponds to a kink conﬁguration with a square and an ejected antiphase defect. During the classical simulation, the kink spent a large proportion of the time trapped in a metastable state that had the eﬀect of pinning the partial. A unique advantage of a modular hybrid scheme with a black-box quantum engine is that it is easy to investigate the eﬀect of chemical defects. Swapping the empirical tight-binding quantum engine for density-functional tight-binding (DFTB)[28] enables us to simulate the interaction of the partial with dopants without having to worry about constructing a classical model for a new type of atom. If we start the simulation after placing a boron atom

Multiscale Modeling of Defects in Semiconductors

207

Fig. 8. A pair of oppositely directed 30◦ partial dislocations enclosing a stacking fault. The complete unit cell consists of 4536 atoms, but only the (111) plane containing the stacking fault is shown. The red (Si) and green (B impurity) atoms are undercoordinated, so they and the surrounding blue (Si) atoms are treated quantum-mechanically

Fig. 9. Detail of the dislocation kink, showing the conﬁguration that corresponds to equilibrium at zero temperature (dotted lines), and to what is prevalent at 900 K in the hybrid simulation

at the position shown in green in Fig. 8, the right-hand partial is pinned and remains completely stationary, while the left-hand partial advances as before.

208

G´ abor Cs´ anyi et al.

Fig. 10. Von-Mises strain ﬁeld around a stationary crack tip in the opening mode in silicon

Brittle Fracture In recent years, the problem of brittle fracture of covalent materials has been a prototypical problem addressed using hybrid methodology [29–31]. Figure 10 depicts the von-Mises strain around a stationary crack tip, as calculated using the Stillinger–Weber potential by optimizing the positions of the interior atoms, while holding the top and bottom rows of atoms ﬁxed, corresponding to a given load in the opening mode. The stress concentrates near the tip and when the load reaches a critical level, the most strained bond gives way and the crack propagates forward. While analytical values for the required loading for crack propagation are easy to compute in the continuum approximation, it is well known that the discreteness of the atomic lattice gives rise to a barrier to this process, called lattice trapping [32–34]. The height of this barrier depends sensitively on the atomistic model employed and classical models typically overestimate this barrier, resulting in a much higher critical loading. The barrier associated with the Stillinger–Weber potential in particular is so high that, when the crack ﬁnally does propagate, so much elastic energy is released that the opening surfaces roughen, the crack tip blunts, emits dislocations, resulting in a reduction of the local stress ﬁeld and an arrest to crack propagation: in other words, the ductile behavior is incorrectly predicted. An example of such “ductile” crack propagation is shown in Fig. 11. In contrast, real cracks in silicon at low temperature are atomically ﬂat and propagate continuously above the critical load. This is reproduced by the hybrid simulation, a snapshot of which is shown in Fig. 12. This simulation at 300 K shows the 5–7–5 Pandey reconstruction of the opening (111) surfaces. The motion of the crack tip is tracked with the quantum region by noting which atoms have changed their number of nearest neighbors since the start of the simulation, and treating all atoms quantum-mechanically within 5˚ A of these.

Multiscale Modeling of Defects in Semiconductors

209

Fig. 11. Snapshot of “ductile” crack propagation using the Stillinger–Weber model. Defects are produced in the crack-opening region and dissipate energy; the onset of cracking is not sharp

Fig. 12. Snapshot from brittle crack propagation, using the hybrid method at 300 K. Red atoms have been ﬂagged as “active” because they have changed their neighbor count since the start of the simulation, and together with the blue atoms, are treated quantum-mechanically. In contrast to the ductile case, the crack propagates continuously above critical loading

210

G´ abor Cs´ anyi et al.

6 Summary To conclude this overview, we reiterate that a large class of problems in the area of semiconductor mechanical properties are inherently multiscale, and that signiﬁcant advances in computer simulation will only be made by addressing the diﬀerent length scales directly and simultaneously. We have introduced a promising new scheme that scales well to large system sizes and that deals with the intricacies of a hybrid simulation with fully controllable approximations. The scheme is very general, and can be extended to deal with arbitrary classical force-ﬁeld potentials, one foreseen extension being, in particular, in the direction of modeling long-range (classical electrostatic) interactions.

References [1] [2] [3] [4] [5] [6] [7] [8] [9] [10] [11] [12] [13] [14] [15] [16]

[17] [18] [19]

L. Pelaz, L. A. Marques, J. Barbolla: J. Appl. Phys. 96, 5947 (2004) 194 M. Bruzzi, et al.: Nucl. Instr. Meth. A 514, 189 (2005) 194 M. Huhtinen: Nucl. Instr. Meth. A 491, 194 (2002) 194 S. K. Estreicher: Mater. Sci. Eng. Rep. 14, 319 (1995) 195 A. Kerridge, A. H. Harker, A. M. Stoneham: J. Phys. Condens. Matter 16, 8743 (2004) 195 C. L. Muhlstein, E. A. Stach, R. O. Ritchie: Acta Mater. 50, 3579 (2002) 197 H. Kahn, R. Ballarini, J. J. Bellante, A. H. Heuer: Science 298, 1215 (2002) 197 J. Du, W. H. Ko, D. J. Young: Sens. Actuators A 112, 116 (2004) 197 P. Nguyen, I. Cayrefourcq, K. K. Bourdelle, A. Bougassol, E. Guiot, N. B. Mohamed, N. Sousbie, T. Akatsu: J. Appl. Phys. 97, 083527 (2005) 197 J. Weber, T. Fischer, E. Hieckmann, M. Hiller, E. V. Lavrov: J. Phys.: Condens. Matter 17, S2303 (2005) 197 B. Lawn: Fracture of Brittle Solids (Cambridge University Press, Cambridge 1993) 197 A. C. T. van Duin, S. Dasgupta, F. Lorant, W. A. Goddard: J. Phys. Chem. A 105, 9396 (2001) 198 S. J. Stuart, A. B. Tutein, J. A. Harrison: J. Chem. Phys. 112, 6472 (2000) 198 D. G. Pettifor, I. I. Oleinik, D. Nguyen-Manh, V. Vitek: Comp. Mater. Sci. 23, 33 (2002) 198 D. W. Brenner: phys. stat. sol. B 217, 23 (2000) 198 J. Molecular Structure – Theochem, Special Issue, vol. 632 (Elsevier Science BV 2003) Combined QM/MM Calculations in Chemistry and Biochemistry 199 W. C. Swope, H. C. Andersen, P. H. Berens, K. R. Wilson: J. Chem. Phys. 76, 637 (1982) 200 A. De Vita, R. Car: MRS Proc. 491, 473 (1998) 200 G. Cs´ anyi, T. Albaret, M. C. Payne, A. De Vita: Phys. Rev. Lett. 93, 175503 (2004) 200, 204

Multiscale Modeling of Defects in Semiconductors

211

[20] G. Cs´ anyi, T. Albaret, G. Moras, M. C. Payne, A. De Vita: J. Phys. Condens. Matter 17, R691 (2005) 200, 204 [21] W. H. Press, S. A. Teukolsky, W. T. Vetterling, B. P. Flannery: Numerical Recipes in C, 2nd ed. (Cambridge University Press, Cambridge 1992) 201 [22] F. Stillinger, T. Weber: Phys. Rev. B 31, 5262 (1985) 201, 203 [23] I. Kwon, R. Biswas, C. Z. Wang, K. M. Ho, C. M. Soukoulis: Phys. Rev. B 49, 7242 (1994) 203 [24] T. J. Lenosky, J. D. Kress, L. A. Collins, I. Kwon: Phys. Rev. B 55, 1528 (1997) 203 [25] D. Quigley, M. I. J. Probert: J. Chem. Phys. 120, 11432 (2004) 204 [26] V. V. Bulatov, J. F. Justo, W. Cai, S. Yip, A. S. Argon, T. Lenosky, M. de Koning, T. D. de la Rubia: Philos. Mag. A 81, 1257 (2001) 205 [27] S. Goedecker, T. Deutsch, L. Billard: Phys. Rev. Lett. 88, 235501 (2002) 206 [28] T. Frauenheim, G. Seifert, M. Elstner, Z. Hajnal, G. Jungnickel, D. Porezag, S. Suhai, R. Scholz: phys. stat. sol. B 217, 41 (2000) 206 [29] N. Bernstein: Europhys. Lett. 55, 52 (2001) 208 [30] F. F. Abraham, J. Q. Broughton, N. Bernstein, E. Kaxiras: Comp. Phys. 12, 538 (1998) 208 [31] S. Ogata, E. Lidorikis, F. Shimojo, A. Nakano, P. Vashishta, R. K. Kalia: Comp. Phys. Comm. 138, 143 (2001) 208 [32] R. P´erez, P. Gumbsch: Phys. Rev. Lett. 84, 5347 (2000) 208 [33] P. Gumbsch: Brittle fracture and the breaking of atomic bonds, in Materials Science for the 21st Century, vol. A (The Society of Materials Science, JSMS, Japan) pp. 50–58 208 [34] N. Bernstein, D. W. Hess: Phys. Rev. Lett. 91, 025501 (2003) 208

Index algorithm, 203, 204 anharmonic, 196 annealing, 194 asymmetric, 201 bond-centered, 195 boron, 206 bulk, 198 carbide, 195 classical, 195, 196, 198–200, 202–204, 206, 208, 210 cluster, 194 complex, 194, 195 core, 195 coupling, 205 covalent, 196, 199, 208 crack, 196, 197, 208

dangling bond, 196, 199 decay, 195 density-functional theory, 198 DFT, 198 DFTB, 206 diamond, 195 diﬀusion, 194, 195, 202, 203 dislocation, 195, 196, 205, 208 disorder, 196 distortion, 195, 196 dopant, 194, 196, 206 doping, 194 electron, 195, 196 embedding, 193 empirical, 194, 196, 198, 206 energetics, 196 equilibrium, 195, 196, 206

212

G´ abor Cs´ anyi et al.

ﬁnite element, 198 ﬁrst-principles, 193 force, 198–200, 202–205, 210 free-energy, 206 grain, 195, 196 grain boundary, 195, 196 Hamiltonian, 200, 204 hole, 196 hybrid, 197–200, 202, 203, 205, 206, 208, 210 hydrogen, 195, 197, 199, 204, 205 impurity, 195 interstitial, 194

phonon, 205 photoluminescence, 194 point defect, 194, 195, 203 positron annihilation, 194 potential, 195, 196, 201, 202, 208, 210 proton, 195 radiation damage, 194 relaxation, 197 Si, 197, 201, 203, 205 silicon, 194, 195, 197, 199, 203–205, 208 Stillinger–Weber, 203, 208 strain, 195, 208 stress, 196, 197, 208 supercell, 194 surface, 197–199, 202, 208

kink, 195, 205, 206

nanometer, 195

temperature, 203–206, 208 termination, 198, 199 tetrahedral, 195 thermostat, 204, 205 tight-binding, 198, 203, 204, 206 total energy, 199, 204 trajectory, 199, 200, 203 transition, 200

periodic, 194, 205

vacancy, 203

LOTF, 200, 203, 204, 206 migration, 194, 195, 206 molecular-dynamics, 193, 195, 198, 205 multiscale, 196, 197, 210

Empirical Molecular Dynamics: Possibilities, Requirements, and Limitations Kurt Scheerschmidt Max Planck Institute of Microstructure Physics, Weinberg 2, D-06120 Halle, Germany [email protected] Abstract. Classical molecular dynamics enables atomistic structure simulations of nanoscopic systems to be made. The method is extremely powerful in solving the Newtonian equations of motion to predict static and dynamic properties of extended particle systems. However, to yield macroscopically relevant and predictive results, suitable interatomic potentials are necessary, developed on ab-initio-based approximations. The fundamental requirements for performing classical molecular dynamics are presented as well as the relation to statistical methods and particle mechanics, suitable integration and embedding techniques, and the analysis of the trajectories. The applicability of the technique is demonstrated by calculating quantum-dot relaxations and interaction processes at wafer-bonded interfaces.

1 Introduction: Why Empirical Molecular Dynamics? Classical molecular dynamics (MD) enable atomistic structure simulations of nanoscopic systems and are, in principle, a simple tool to approach the manyparticle problem. For given interatomic or intermolecular forces one has to integrate the Newtonian equations of motion assuming suitable boundary conditions for the box containing the model structure. There are at least two advantages of this technique. The molecular dynamics is deterministic and provides the complete microscopic trajectories, i.e., the full static and dynamic information of all particles is available, from which a large number of thermodynamic and mechanically relevant properties of the models can be calculated. Further, one can perform simulations that are macroscopically relevant with the present computational power of even desktop computers. With reasonable computational eﬀort models of nanoscale dimension can be treated for several million particles and up to microseconds of real time. Thus, empirical MD has two main ﬁelds of application: The search for the global energetic minima by relaxing nanoscopic structures and the calculation of dynamical parameters by analyzing the lattice dynamics. Computer simulations are performed on models simulating the reality by using approximations, reduction, localization, linearization, etc., the validity of which has to be critically evaluated for each problem considered. As sketched in Fig. 1, increasing the time and length scales of the models (which is necessary to increase the macroscopic validity and robustness of the calculations) requires an increasing number of approximations and thus leads D. A. Drabold, S. K. Estreicher (Eds.): Theory of Defects in Semiconductors, Topics Appl. Physics 104, 213–244 (2007) © Springer-Verlag Berlin Heidelberg 2007

214

Kurt Scheerschmidt

Fig. 1. Length and timescales in various modeling methods: DFT = densityfunctional theory, TB = tight-binding approximations, BOP = bond-order potentials, MD = empirical molecular dynamics, MC, CGM = Monte-Carlo/conjugategradient techniques, FEM = ﬁnite element methods, CM = continuum mechanics

to a reduction in the ability to predict some physical properties. Densityfunctional theory (DFT) and its approximations (e.g., local-density LDA, generalized gradient GGA), and the diﬀerent kinds of tight-binding treatments (TB) up to the bond-order potential (BOP) approximations start with the Born–Oppenheimer (BO) approximation, thus decoupling the ionic and electronic degrees of freedom. Additional approximations such as pseudopotentials, gradient corrections to the exchange-correlation potential, and incomplete basis sets for the single-particle states are required for DFT calculations. The speciﬁcs of the various methods are discussed in various Chapters in the present book and in a number of review articles on DFT, TB, linear scaling techniques and programs such as SIESTA and CASTEP [1–9]. In ﬁrst-principle MD [10], e.g., using DFT or DFT-TB, the electronic system is treated as parameter free and the resulting Hellmann–Feynman forces are the glue of the ionic interactions. Such simulations are computationally too expensive for large systems. Figure 1 shows that the empirical MD closes the gap between ﬁrst-principles, macroscopic, and continuum techniques (FEM = ﬁnite element methods, CM = continuum mechanics). The latter neglect the underlying interatomic interactions but allow the description of defects, defect interactions, diﬀusion, growth processes, etc. Stochastic Monte Carlo techniques (MC) enable the further increase of the timescales, also at the ﬁrst-principles level, but without access to the dynamics. On the other hand, static energy minimization (e.g., conjugate gradient methods, CGM) enable a drastic increase in the model size. However, this does not necessarily provide the global mini-

Empirical Molecular Dynamics

215

Fig. 2. Interface structures at 90◦ twist boundaries ((a): P mm(m)-layer, (b): 42m-dreidl, cf. text in Sect. 4.2), predicted by empirical MD and revealed by abnitio DFT simulations yielding semimetallic/isolating behavior as a function of the interface bonding state as demonstrated by the corresponding DFT band structures (c) and (d), respectively

mum of the potential energy surface. The largest model dimensions (number of atoms) accessible to empirical MD (or MC, CGM) has approximately the same extension as the smallest devices in microelectronics and micromechanics. Thus, today’s atomistic modeling approaches the size of actual nanoscale systems. The assumption of the existence, validity, and accuracy of known empirical interatomic potentials or force ﬁelds in analytic form always ignores the underlying electronic origin of the forces, i.e., the quantum structure of the interactions (cf. Sect. 2.4). Therefore, it is important to have better approximations, such as the bond-order potential (BOP), which is developed from tight-binding approximations and discussed brieﬂy in Sect. 3.2. Other possibilities to include electronic properties of the interaction consist in continuously reﬁtting an empirical potential during the calculation, called learning on the ﬂy (see Chap. 9 and [11]). Separated subsystems can be treated at an ab-initio level. Suitable handshaking methods can be designed to bridge the embedded subsystem with its surrounding, which is treated semiclassically (cf. [12–15]). However, well-constructed potentials describing suﬃciently accurate physical properties also give physical insights and enable a thorough understanding of the underlying processes [2]. Figure 2 shows a simple example demonstrating the diﬀerence in the approximation levels. Using empirical MD the correct structural relaxation of special interfaces created by wafer bonding can be treated, as described later

216

Kurt Scheerschmidt

in Sect. 4.2. Two conﬁgurations exist, a metastable one (Fig. 2a) and the global minimum structure shown in Fig. 2b, called dreidl [16]. The electronic properties demand ab-initio level simulations, done here using a smaller periodic subunit of the interface and applying DFT techniques. It is shown that the higher-level approximation reproduces the structure predicted by the semiempirical techniques, whereas the correct energies and electronic properties (the band structure and the semimetallic or isolating behavior of the interfaces as shown in Figs. 2c,d) can only be described using the DFT formalism. A second kind of embedding problem occurs because even millions of particles only describe a small part of reality that, even for smaller pieces of matter, is characterized by Avogadro’s number (6 × 1023 mol−1 ). Since isolated systems introduce strong surface eﬀects, each model has to be embedded in suitable surroundings. For a discussion of various types of boundary conditions, see Sect. 3.1, Chap. 9 and [13–15]. The fundamental requirements of classical MD simulations, the relation to statistical methods and particle mechanics, suitable integration and embedding techniques and the analysis of the trajectories are presented in Sect. 2. The enhancements of potentials (bond-order potentials) and boundary conditions (elastic embedding) are discussed in Sect. 3. Selected application of semiempirical MD (relaxation of quantum dots and wafer-bonded interfaces) are given in Sect. 4 together with some examples from the literature. They strongly depend on the approximations assumed in the simulations.

2 Empirical Molecular Dynamics: Basic Concepts The main steps for applying empirical molecular dynamics consist of the integration of the basic equations (cf. Sect. 2.1) using a suitable interaction potential and embedding the model in a suitable surrounding (cf. Sect. 2.4 and Sect. 2.3, respectively). Textbooks of classical molecular dynamics, e.g., [17– 23], describe the technical and numerical details, and provide a good insight into possible applications and the physical properties, which may be predictable. Here, only the main ideas of empirical MD simulations, viz. the basic equations, methods of numerical treatment and the analysis of the trajectories are discussed. 2.1 Newtonian Equations and Numerical Integration The basic equations of motion solved in empirical MD are the Newtonian equations for N particles (i = 1, . . . , N ) characterized by their masses mi , f i . These may their coordinates ri , and the forces acting on each particle include external forces F i and interatomic interactions f i = j=i f ij : ¨i = f i = − mi r

∂V(r1 , r 2 , . . . , r N ) . ∂ri

(1)

Empirical Molecular Dynamics

217

The assumption that a potential V exists presupposes conservative (nondissipative) interactions and needs some more general considerations, cf. 2.2. Sect. V(r If one assumes pairwise central potentials, V(r1 , r 2 , ..., r N ) = ij ) i,j with rij = |r j − r i | (the dash means that the sum is restrictedto i < j), it follows that the virial of the external and internal forces is M = i,j rij f ij = the conservation i r i F i . If the system is isolated (microcanonical ensemble), of total energy E = K + V (with kinetic energy K = i mi r˙i 2 ) is guaranteed: r˙ i f i = 0 . E˙ = K˙ + V˙ = mi r˙i · r¨i − (2) i

i

Given an initial conﬁguration of particles and suitable boundary conditions (cf. Sect. 2.3), the diﬀerential equations can be integrated using one of the standard methods, e.g., Runge–Kutta techniques, predictor–corrector methods, Verlet or Gear algorithm. The numerical integration is equivalent to a Taylor expansion of the particle positions ri (t + δt) at a later time in terms of atomic positions ri and velocities v i . The forces f i are the time derivatives of r i with an increasing order at previous time steps: ri (t + δt) = ri (t) + a1 δtv i (t) + a2 (δt)2 f i (t) + . . . + O(δtn ) .

(3)

In addition to good potentials and system restrictions (cf. Sect. 2.3 and Sect. 2.4, respectively) an eﬃcient and stable integration procedure is required to accurately propagate the system. The conservation of energy during the simulation is an important criterion. An increase in order allows larger time increments δt to be used, if the evaluation of the higher derivatives is not too time consuming, which happens with more accurate potentials, like the BOP (Sect. 3.2). The eﬃciency and the accuracy of the integration can be controlled by choosing suitable series-expansion coeﬃcients aj , j = 1, 2, ..., n − 1 and the order n of the method or by mixing the derivatives of r i at diﬀerent times in (3) to enhance the procedure. However, the increment δt, of the order of fs, must be at least so small that the fastest particle oscillations are suﬃciently sampled. Better or faster MD calculations may be performed using special acceleration techniques, the three most important methods being: 1) Localization: By using the linked-cell algorithm and/or neighbor lists, it is assumed that for suﬃciently rapidly decaying potentials (faster than Coulomb 1/r for r → ∞) only a small number of particles have a direct and signiﬁcant interaction. A cutoﬀ rc is deﬁned and the interaction potential is assumed to be zero for r > rc . A transition region is ﬁtted using splines or other suitable functions. Then the system is divided into cells. Their minimum dimension is given by 2rc to avoid self-interaction of the particles (minimum image convention). Only the interactions of the atoms within a cell and its 26 neighboring cells are considered, which reduces the simulation time drastically from the ∝ N 2 behavior for all particle interactions to linear behavior ∝ 729cN N , where cN is the average number of particles per cell.

218

Kurt Scheerschmidt

The problem is to ﬁnd a suitable rc for a smooth transition and screening behavior that includes a suﬃcient number of next-neighbor atoms and cells. One also needs a suitable criterion to update the neighbor lists and reorder the cells whenever particles leave a cell during the propagation of the system. The Coulomb potential may also be screened. However, summations over the long-range 1/r potential, representing inﬁnite point-charge distributions, are only conditionally convergent. Thus, it is better to apply the Ewald method (originally developed to calculate cohesive energies and Madelung constants [24]) and its extensions [25, 26] based on successive charge neutralization by including next-neighbor shells around the origin. 2) Parallelization: Using replicas, or dividing the structure into several parts, which are then distributed to diﬀerent processors, thus allowing parallelization [27, 28]. The replica technique needs suitable criteria for dividing the system into small parts with minimum interaction. More importantly, one must bear in mind that the replicas are not independent over long times. A careful control of the time interval after which the communication between the diﬀerent parts is required in order to achieve the same results as nonparallelized simulations. This issue is the bottleneck of the technique. 3) Time stretching: Such techniques as hyperdynamics, temperature acceleration, basin-constrained dynamics, on-the-ﬂy Monte-Carlo, and others are subsumed brieﬂy here, because their common idea consists in replacing the true time evolution by a shorter one increasing the potential minima, transition frequencies, system temperature, etc. (see [28]). 2.2 Particle Mechanics and Nonequilibrium Systems In classical mechanics a system is characterized either by its Lagrangian L(q, q) ˙ = K(q, q) ˙ − V(q) or its Hamiltonian related to the Lagrangian by q˙i pi − L = K + V(q), where q i , pi are a Legendre transform H(q, p) = generalized coordinates and momenta (conjugate coordinates), respectively, which have to be independent or unrestricted. One derives the generalized momenta from the derivatives of the Lagrangian pi = ∂∂L q˙ i , whereas the derivatives of the Hamiltonian q˙i =

∂H , ∂pi

p˙i = −

∂H ∂qi

(4)

reproduce Newton’s law of motion (1). Hamilton’s principle of least action enables a simple generalization of the mechanics of many-particle systems. The integral over the Lagrangian function has to be an extremum. Variational methods yields, applying the extremal principle: ∂L d ∂L − = 0. dt ∂ q˙ i ∂q i

(5)

Empirical Molecular Dynamics

219

The advantage of the general formulation (5) is that it allows a simple extension to nonconservative systems by including an explicit time dependence or to systems with constraints, such as ﬁxed bond lengths in subsystems, friction of particles, outer forces, etc. If there are holonomic constraints describing relations between the coordinates fl (q k ) = 0, one gets the generalized additional coordinates alk = ∂fl /∂qk and al = ∂f l /∂t creating an additional term on the right-hand side of (5) in the form l λl alk with the set of Lagrange multipliers λl . This formalism is the basis for the enhancement of the boundary conditions in Sect. 3.1 and the handshaking methods mentioned above. In addition, the Lagrangian and Hamiltonian formalisms correlate classical dynamics to statistical thermodynamics and to quantum theory, and allow the evaluation of properties from the trajectories (cf. Sect. 2.5). The set of time-dependent coordinates q (the conﬁguration space) and timedependent momenta p (momentum space) together is called the phase space Γ = (q, p) = (q 1 , q 2 , ..., q n , p1 , p2 , ..., pn ). Presenting Γ in a 6-dimensional hyperspace yields N trajectories, one for each molecule, and allows the study of the behavior of the system using statistical methods. It is called the µ-space (following Ehrenfest) or the Boltzmann molecule phase space. The whole Γ set as one trajectory in a 6N -dimensional hyperspace presents the Gibbs phase space, with the advantage to include better interactions and restrictions. However, the system must now be described as a virtual assembly for statistical relations. The phase space Γ contains the complete information on the microscopic state of the many-particle system. Several basic quantities ˙ p). ˙ may be derived such as the phase-space ﬂow or the “velocity ﬁeld” Γ˙ = (q, Applying the relations (4) yields the Liouville equation ∂ q˙i ∂ p˙i + = 0, (6) ∇Γ Γ = ∂q i ∂pi showing that the ﬂow Γ˙ behaves like an incompressible liquid, i.e., although the µ-trajectories are independent, their related phase-space volume is constant. An equivalent formulation of the Liouville statement (6) is the equation of continuity for Γ˙ , ρ, ˙ and the local change of the density ρ(q, p, t), similar to the Heisenberg equation for observables in quantum theory. The density ρ(q, p, t) describes the probability of ﬁnding the system within the region p, q and p + dp, q + dq of the phase-space volume dpdq. Because the systems must be somewhere in the phase space, the density can be normalized in the entire phase space. The integral over the whole phase space of the non-normalized density yields the partition function. Integration over (N − k) particles yields the k-particle phase-space density ρ(k) (q, p, t) = ρ(N ) (q, p, t)dp(N −k) dq (N −k) , and the integration over the whole momentum space the corresponding k-particle distribution function n(k) (q) = ρ(N ) (q, p, t)dq (N −k) dp. Very important for the trajectory analy-

220

Kurt Scheerschmidt

sis (Sect. 2.5) are the cases k = 1, 2 deﬁning the (radial) pair-distribution functions g(q i , q j ): n(1) (q i )n(1) (q j )g(q i , q j ) = n(2) (q i , q j ).

(7)

The phase-space trajectories allow the classiﬁcation of the dynamics of many-particle systems. They may be Poincare-recurrent (the same phasespace conﬁguration occurs repeatedly), Hamiltonian (nondissipative), conservative (no explicit time dependence for the Hamiltonian), or integrable (number of constants of motion equals the number of degrees of freedom, resulting in stable periodic or quasiperiodic systems). Nonintegrable systems may be ergodic or mixing, etc., i.e., the trajectory densely covers diﬀerent hypersurfaces in the phase space, and allow the characterization of diﬀerent kinds of instabilities of the system. 2.3 Boundary Conditions and System Control As mentioned above, even for systems considered large in MD simulations, the number of atoms is small compared to real systems and therefore dominated by surface eﬀects. They are caused by interactions at free surfaces or with the box boundaries. In order to reduce nonrealistic surface eﬀects, periodic boundary conditions are applied, or the box containing the model (supercell) has to be enlarged so that the inﬂuence of the boundaries may be neglected. For further discussion and enhancements including elastic embedding, see Sect. 3.1. Periodic boundary conditions means that the supercell is repeated periodically in all space directions with identical image frames or mirror cells. In contrast to the case of ﬁxed boundaries, under periodic boundary conditions the particles can move across the boundaries. If this happens, the positions r have to be replaced by r −α where α is a translation vector to the image frame to which the particle is moved. Particle number, total mass, total energy, and momenta are conserved in periodic boundary conditions, but the angular momenta are changed and only an average of them is conserved. It should be mentioned here that periodic boundary conditions repeat defects, which in small supercells create high defect concentrations. Antiperiodic and other special boundary conditions may be chosen, where additional shifts of the positions and momenta along the box borders allow correction of a disturbed periodic continuation and a description of reﬂective walls at free surfaces to be obtained. According to the boundary conditions and system restrictions, the virtual Gibbs entities are either isolated microcanonical ensembles with constant volume, total energy, and particle numbers (N V E ensembles) or systems that exchange and interact with the environment. Closed ensembles (e.g., canonical N V T or isothermic-isobar N P T systems) have only an energy exchange with a thermostat, whereas open systems have in addition particle exchange with the environment (e.g., grand-canonical T µV , where µ is the chemical potential).

Empirical Molecular Dynamics

221

Simple tools exist to equilibrate systems at a well-deﬁned temperature. For example, velocity rescaling is numerically equivalent to a simple extension of the original microcanonical system with nonholonomic constraints in the Lagrangian formalism and is called the Berendsen thermostat. A similar simple extension may be used for pressure rescaling. It is called the Berendsen barostat [29]. The simple velocity rescaling works by conserving the Maxwell distribution and yielding maximum entropy. However, such nonisolated ensembles are better described using constraints in the Lagrangian similar to those discussed in Sect. 2.2. The extension of L in (5) by adding terms Lconstr introduces additional generalized variables having extra equations of motion and also additional force terms in the Newtonian equations (1). Some of the most important methods for Lconstr are given below without further comments: – Nos´e–bath and generalized Nos´e–Hoover thermostat [30–32]: Lconstr = mi , the M s˙ 2 /2 − nf T ln(s) with the ﬁctive or the whole mass M = degrees of freedom nf = 3N + 1, and the new generalized variable s playing the role of an entropy. – Andersen isothermic-isobaric system control (NPH ensemble) Lconstr = V˙ 2 /2 + P V introduces volume and pressure as generalized variables [33]. – Generalized stresses according to Parrinello and Rahman [34] N T Lσensembles: the Lagrangian is extended by Lconstr = −1/2T rΣG with a generalized symmetric tensor Σ and the metric tensor G of the crystal structure. A further specialization, e.g., for constant strain rates N T Lxσyy σzz -ensemble [35], is in principle a mixture of the isothermicisobaric system with the generalized stress constraint. – Brownian ﬂuctuations, transport and ﬂow processes, density and other gradients, Langevin damping ∝ v(t), etc. demand nonequilibrium MD [36, 37], which is mostly done by including the perturbation as a suitable virtual ﬁeld F (p, q, t) into the equations of motion via the Lagrange formalism. 2.4 Many-Body Empirical Potentials and Force Fields Empirical potentials and force ﬁelds exist with a wide variety of forms, and also diﬀerent classiﬁcation schemes are used according to their structure, applicability, or physical meaning. It makes no sense to describe a large number of potentials or many details in the present review, therefore only some of the existing and most used potentials are brieﬂy listed below (a good overview can be found in [38–48]. A classiﬁcation by Finnis [2] (and many references therein) describes recent developments and discusses in an excellent way the justiﬁcation of the potentials by ﬁrst-principle approximations, which is important for the physical reliability and the insight into the electronic structure of potentials. Interatomic forces are accurate only if the inﬂuence of the local environment according to the electronic structure is included. The most

222

Kurt Scheerschmidt

important property of a potential is transferability, that is the applicability of the potential to varied bonding environments. An important additional criterion is its ability to predict a wide range of properties without reﬁtting the parameters. The number of ﬁt parameters decreases as the sophistication of the force ﬁelds increases. According to [2] one has: Pair potentials – Valid for s-p bonded metals and mostly approximated by a sum of pairwise potentials. They may be derived as the response to a perturbation in jellium, which can be visualized in the pseudoatom picture as an ionic core and a screening cloud of electrons. Ionic potentials – To use Coulomb interactions directly for ionic structures, the problem of screening (Ewald summation, Madelung constant) has to be considered as mentioned above. The interactions were originally described by Born and others as the rigid-ion approximation. Starting from the Hohenberg–Kohn–Sham formulation of the DFT-LDA, shell or deformable ion models may be developed beyond the rigid-ion approximation, where the additional shell terms [49] look like electron-density diﬀerences in noble gases. Tight-binding models – Diﬀerent derivations and approximations for TBrelated potentials exist and are nowadays applicable to semiconductors, transition metals, alloys and ionic systems. The analytic bond-order potential is such an approximation and will be discussed in more detail in Sect. 3.2. Hybrid schemes – Combinations of pair potentials with TB approximations are known as generalized pseudopotentials, eﬀective media theories (EMT [50]), environmental-dependent ionic potentials (EDIP [51]), or embedded atom models (EAM [52]); for details see [2]. From the empirical point of view the simplest form of potentials may be considered to be a Taylor-series expansion of the potential energy with respect to 2-, 3-,. . ., n-body atomic interactions. Pair potentials have a shortrange repulsive part, and a long-range attractive part, e.g., of the Morse or Lennard–Jones (LJ) type, mostly “12–6”, i.e., ar−12 − br−6 . LJ potentials are successfully applied to noble gases, biological calculations, or to model long-range van der Waals interactions (e.g. [53]). For quasicrystals [54] an LJ potential was constructed with two minima in a golden number distance relation. However, simple pair potentials are restricted in their validity to very simple structures or to small deviations from the equilibrium. Therefore many-body interactions are added and ﬁtted for special purposes, e.g., the MD of molecules and molecule interactions [55,56]. Separable 3-body interactions are widely used: Stillinger–Weber [57] (SW), Biswas–Hamann [58], and Takai–Halicioglu–Tiller [59] potentials. The SW is perhaps the best-known 3-body-type potential. It includes anharmonic eﬀects necessary to reproduce the thermal lattice expansion of Si and Ge [60]. Hybrid force ﬁelds are sometimes used to include the interaction of diﬀerent types of atoms, such as Born–

Empirical Molecular Dynamics

223

Mayer–Huggins, Rahmann–Stillinger–Lemberg terms and others applicable to silicate glasses and interdiﬀusing metal ions or water molecules [61–65]. As mentioned above, other force ﬁelds are developed from ﬁrst-principle approximations that combine suﬃcient simplicity with high rigor. They are not based upon an expansion involving N -body interactions (cluster potentials). The more or less empirical forms of TB potentials and eﬀective medium force ﬁelds are the modiﬁed embedded atom model (MEAM, [66] for cubic structures and references therein for other structures), the Finnis–Sinclair (FS) [67] and the Tersoﬀ-type (TS) potentials [68–70]. The TS potential is an empirical bond-order potential with the functional form: V (rij ) = ae−λrij − bij e−µrij .

(8)

The bonds are weighted by the bond order bij = F (r ik , r jk , γijk ) including all next neighbors k = i, j, which gives the attractive interaction the form of an embedded many-body term. The diﬀerent parameterizations (TI, TII, TIII) of the Tersoﬀ potential have been intensively tested. Other parameterizations exist [71]. They involve other environmental functions and ﬁrst-principle derivations [72, 73], as well as extensions to include further interactions, H in Si [74], C, Ge [75], C–Si–H [76, 77], AlAs, GaAs, InAs, etc. [78]. Finally, a reﬁtted MEAM potential with SW terms is available for Si [79]. Multipole expansions replaced by spherical harmonics [80] are an alternative to TS potentials. A comparative study of empirical potentials shows advantages and disadvantages in the range of validity, physical transparency, ﬁtting and accuracy as well as applicability [81]. Restrictions exist for all empirical potential types, even if special environmental dependencies are constructed to enhance the elastic properties near defects. In addition, not all potentials are applicable to long-range interactions, and the electronic structure and the nature of the covalent bonds can only be described indirectly. Thus, it is of importance to ﬁnd physically motivated semiempirical potentials, as mentioned above and discussed in Sect. 3.2 for TB-based analytic BOPs. The parameters of the empirical force ﬁeld have to be ﬁtted to experimental data or ﬁrst-principle calculations. First, the cohesive energy, lattice parameter and stability of the crystal structures have to be tested or ﬁtted. The bulk modulus, elastic constants, and phonon spectra are very important properties for the ﬁt. The following section describes some of the quantities that may be used for the ﬁt or to be evaluated from the MD simulations if not ﬁtted. Very important details concerning point defects and defect clusters – necessary to get the higher-order interaction terms – are given by the energy and structure of such defects. The data may be given by DFT or TB dynamics or geometry optimizations, as, e.g., [82–85].

224

Kurt Scheerschmidt

2.5 Determination of Properties Static properties of systems simulated by empirical MD can be directly calculated from the radial- or pair-distribution function (7). Dynamic properties follow from the trajectories using averages or correlations: t 1 dtA[r(t)], C(t) = A(τ )B(t + τ )τ , (9) At = lim t→∞ t − t0 t 0 which in principle correspond to time averages. However, they are sampled at discrete points, so that it is necessary to choose suitable sampling procedures to reduce the eﬀects of the ﬁnite size of the system, stochastic deviations, and large MD runs. Two basic relations are central for the analysis of the properties. The ergodic hypothesis states that the ensemble average Ae is equal to the time average At , which relates the averages to the measurement of a sin2 0 )] t gle equilibrium system. The Green–Kubo formula limt→∞ [A(t)−A(t = t−t 0 ∞ ˙ ˙ with time correlations. t0 dτ (A(τ )A(t0 )e ) relates mean square deviations 1 2 The diﬀusion coeﬃcient D = limt→∞ 6N [r (t) − r j j (0)] (Einstein relat tion) is equivalent to the velocity autocorrelation function, which is a special ∞ 1 v (t) · v (0). Similarly, one form of the Green–Kubo formula D = 3N j j 0 uses the crosscorrelation of diﬀerent stress components to obtain shear viscosities. Other transport coeﬃcients may be derived analogously. In thermodynamic equilibrium the kinetic energyK per degree of freedom is determined by the equipartition theorem K = i mi v˙ i2 /2 = 3N kB T /2 (kB = Boltzmann constant) which yields a measure of the system temperature T . The strain tensor σ and the pressure P are obtained from the generalized virial theorem σkl = 1/V [ j v jk · v jl + ij r ijk · f ijl ]. Thus, the pressure is the canonical expectation value P = 1/3V [2K − M] of the total virial M. Alternatively, one can use the pair distribution in the ∞ 3 4πr dr, which may be useful for correcting form P = ρkB T − ρ2 0 g(r) ∂U ∂r sampling errors. Using the densities ρ(r, p) as deﬁned above and Z = ρ(r, p)dr as normalization, statistical mechanics deals with ensemble averages, which in general are written as (10) Qe = 1/Z Q(r, p)ρ(r, p)dr . All thermodynamic functions may be derived from the partition function Z, for example the free energy F (T, V, N ) = −kB T ln[Q(T, V, N )]. In addition, one can obtain all the thermodynamic response coeﬃcients. With the internal energy U , one computes the isochoric heat capacity CV = (∂U/∂T )N,V and thus a measure for the quality of the temperature equilibration (T 2 − T 2 )/T 2 = 3/2N (1 − 3kN )/2cV . From the volume V follows the isothermal compression χT = −1/V (∂V /∂P )N,T , etc. One has to choose according to the diﬀerent ensembles:

Empirical Molecular Dynamics

225

– Microcanonical: ρN V E = δ[H(r, p) − E] conserving entropy S(E, N, V ). – Canonical: ρN V T = e(H/kB T ) ∝ eV (r)/kB T conserving free energy F (T, V, N ) – Isothermic-isobaric: ρN P T = e(H−T S)/kB T conserving Gibbs free energy G(T, P, N ) – Grand canonical: ρT µV = e(H−µN )/kB T conserving Massieu function J(T, µ, V ) (Legendre transformation in entropy representation). Finally, it should be mentioned that the Fourier transform of pair distributions is connected to the scattering functions in X-ray, neutron and electron diﬀraction. MD-relaxed structure models allow the simulation of the transmission electron microscope (TEM) or high-resolution electron microscope (HREM) image contrast and therefore make the contrast analysis more quantitative. For this purpose, snapshots of the atomic conﬁgurations are cut into thin slices, which are folded with atomic scattering amplitudes and each other to describe the electron scattering (multislice formulation of the dynamical scattering theory), cf. the applications in Sect. 4 using this technique to interpret HREM investigations of quantum dots and bonded interfaces.

3 Extensions of the Empirical Molecular Dynamics Coupling of length and timescales in empirical MD means bridging the ﬁrstprinciples particle interactions and the box environment (1). It can be done either using embedding and handshaking or by a separate treatment and a transfer parameter between the subsystems. MD simulations of the crack propagation [86] and the analysis of submicrometer MEMS [87] are successfully applications of the FEM coupling between MD and an environmental continuum. In Sect. 3.1 enhanced boundary conditions for MD are discussed: where the coupling between MD and an elastic continuum is a handshaking method based on an extended Lagrangian [88, 89]. The main steps in the development of an analytic TB-based BOP [90] are sketched in Sect. 3.2 as an example of using enhanced potentials. 3.1 Modiﬁed Boundary Conditions: Elastic Embedding Elastic continua may be coupled to MD when the potential energy of an inﬁnite crystal with a defect as shown in Fig. 3a is approximated in the outer region II by generalized coordinates ak [89]: E({ri }, {rj }) = E({ri }, {ak }) .

(11)

In the defect region I, characterized by large strains, the positions of atoms r i (i = 1, . . . , N ) are treated by empirical MD. The atomic positions rj (j > N ) in the outer regions II and III result from the linear theory of elasticity rj = Rj + u(0) (Rj ) + u(Rj , {ak }) ,

(12)

226

Kurt Scheerschmidt

Fig. 3. Dislocation geometry ((a), I = MD region, II = elastic, III = overlap, cf. text) to apply elastic boundary conditions for a dipole of 60◦ dislocations, and snapshots during MD annealing: 500 K (b), 600 K (c), 0 K (d)

where the ﬁelds u0 (R) and u(R) describe the displacements of atoms from their positions Rj in the perfect crystal, and satisfy the equilibrium equations of a continuous elastic medium with defects; u0 (R) is the static displacement ﬁeld of the defect and independent of the atomic behavior in I; u(R) is related to the atomic shifts in region I and can be represented as a multipole expansion: u(R, {ak }) =

∞

ak U (k) (R)

(13)

k=1

over homogeneous eigensolutions U (k) (R) [88]. The U (k) are rapidly decreasing with R, thus the sum in (13) is truncated to a ﬁnite number K of terms. The equilibrium positions of atoms in the entire crystal are obtained from the minimization of the potential energy given in (11) with respect to r i and ak . This is equivalent to a dynamic formulation based on the extended Lagrangian as discussed above (Sect. 2.2 and Sect. 2.3) with the extension (11): L=

N mi r˙ 2 i

i=1

2

+

K µa˙k 2 k=1

2

− E({r i }, {ak }) .

(14)

Here, mi are the atomic masses and µ is a parameter playing the role of mass for the generalized coordinates ak . If µ is properly chosen, the phonons are smooth from I to II and the outer regions oscillate slower than the MD subsystem as demonstrated in the snapshots Figs. 3b–d. The corresponding system deﬁning the forces reads Fi = −

∂E({ri }, {ak }) , ∂r i

Fk = −

∂E({ri }, {rj }) ∂rj ∂E({ri }, {ak }) =− = F j U (k) (Rj ) . ∂ak ∂rj ∂ak

(15)

j>N

j∈II

(16)

Empirical Molecular Dynamics

227

These must vanish in the equilibrium F i = Fk = 0. The sum in (16) expands only over the atoms in region II surrounding region I, since in region III the linear elasticity alone is suﬃcient and the forces on these atoms are nearly vanishing. However, region II must be completely embedded in region III. The forces on atoms in region II must be derived from the interatomic potential, therefore the size of region II must be extended beyond the potential cutoﬀ rc . The Lagrangian (14) results in the equations of motion m¨ ri = F i ,

(i = 1, . . . , N ) ,

µ¨ ak = Fk ,

(k = 1, . . . , K) ,

(17)

thus extending Newton’s equations by equivalent ones for the generalized coordinates. 3.2 Tight-Binding-Based Analytic Bond-Order Potentials As discussed before, the use of TB methods allows much larger models than accessible to DFT. TB formulations exist in many forms (e.g., [2, 6–8, 91– 93]). The application of an analytical BOP, developed mainly by Pettifor and coworkers [90, 94–98], may further enhance empirical MD by providing better justiﬁed force ﬁelds while allowing faster simulations than numerical TB-MD. The approximations to develop analytic TB potentials from DFT may be summarized by the following steps (cf. also [2, 99]): 1. Construct the TB matrix elements by Slater–Koster two-center integrals including s- and p-orbitals, 2. transform the matrix to the bond representation, 3. replace the diagonalization by Lanczos recursion, 4. get the momenta of the density of states from the continued fraction representation of the Green’s function up to order n for an analytic BOP-n potential. The basic ideas sketched with a few more details are as follows. The cohesive energy of a solid in the TB formulation can be written in terms of the pairwise repulsion Urep of the atomic cores and the energy due to the formation of electronic bonds Ucoh = Urep + Uband − Uatoms 1 atom = φ(rij ) + 2 (n) − Niα εiα , 2 i,j iα

(18)

n(occ)

where the electronic energy ε of the free atoms has to be subtracted from the energy of the electrons on the molecular orbitals . Replacing (n) with the eigenstates of the TB-Hamiltonian for orbital α at atom i, (n) (n) (n) = (n) n|n = n| (n) |n = n|H|n = Ciα Hiα,jβ Cjβ , (19) iα,jβ

the electronic contributions to the cohesive energy Uband − Uatom = Ubond + Uprom can be rearranged and separated in the diagonal and oﬀdiagonal parts: atom 2ρiα,iα − Niα εiα . Ubond = 2 ρjβ,iα Hiα,jβ , Uprom = (20) iα,jβ

iα

228

Kurt Scheerschmidt

The third contribution, the promotion energy Uprom compares the occupancy of the atomic orbitals of the free atoms with the occupation of the corresponding molecular orbitals [100]. The bond energy Ubond describes the energy connected with the exchange or hopping of electrons between arbitrary pairs of atomic neighbors {i(j), j(i)}, the factor 2 is due to the spin degeneracy. The transition matrix elements of the Hamiltonian are hopping energies, and their transition probability is given by the corresponding element of the density matrix. The contribution for one bond between the atoms i and j is thus characterized by the part of the density called the bond order Θjβ,iα that may be expressed as a trace: i,j Ubond = Hiα,jβ Θjβ,iα = T r(HΘ) . (21) α,β

Besides the bond energy, the force exerted on any atom i must be given analytically and therefore one needs the gradient of the potential energy in (18) at the position of the atom i: ∂Ucoh ∂Ubond 1 ∂φ(rij ) = + . −F i = ∂ri ∂r i 2 j ∂r i j=i

(22)

This expression includes electronic bonds and ionic pairwise repulsions from all atoms of the system. The general form is still expensive to cope with for the simulation of mesoscopic systems. O(N ) scaling behavior is provided if the cohesive energy of the system is approximated by the Tersoﬀ potential i,j and a suitable cutoﬀ with resulting in (8), where bij e−µrij is replaced by Ubond balanced interatomic forces is added. To ﬁnd an eﬃcient way to obtain the bond energy in a manner that scales bond of the bond energy linearly with the system size, too, the derivative ∂U∂r i in (22) is replaced assuming a stationary electron density ρ in the electronic ground state and applying the Hellmann–Feynman theorem. The forces can now be obtained without calculating the derivatives of the electronic states and leads to the Hellmann–Feynman force [101, 102]: ∂Hiα,jβ −F HF = Θjβ,iα . (23) i ∂r i iα,jβ

Both the elements of the density matrix and the hopping elements of the Hamiltonian are functions of the relative orientation and separation of the bonding orbitals and have been calculated by Slater and Koster [103] assuming a linear combination of atomic orbitals (LCAO). To introduce the Slater–Koster matrix elements, usually denoted by ssσ, spσ, ppπ, etc., corresponding to the contributing orbitals and its interaction type, the TB Hamiltonian operator is transformed to a tridiagonal form. This can be done using the Lanzcos transformation [104]: Um HUn = an δm,n + bn δm,n−1 + bn+1 δm,n+1 ,

(24)

H|Un = an |Un + bn |Un−1 + bn+1 |Un+1 ,

(25)

Empirical Molecular Dynamics

229

where the orthonormal basis at the higher level n is recursively developed from |U0 . The coeﬃcients an , bn are the elements of the continuous fraction of the Green’s function below. The oﬀdiagonal elements of the density matrix are related to the Green’s function [105], ρiα,jβ

1 = − lim π η→0

Ef

dE Giα,jβ (Z) ,

(26)

where the complex variable Z = E + iη is the real energy E with a positive, imaginary inﬁnitesimal to perform the integration (theorem of residues). This intersite Green’s function can be connected to the site-diagonal Green’s function [105] via Giα,jβ (Z) =

∂GΛ 00 (Z) + GΛ 00 (Z)δi,j δα,β , ∂Λiα,jβ

(27)

and the latter can be evaluated recursively [106] using the coeﬃcients of the Lanczos recursion algorithm as mentioned above: GΛ 00 (Z) =

1 Z − aΛ 0 −

(bΛ1 )2 (bΛ2 )2 Z−aΛ − 1

.

(28)

Z−aΛ −... 2

The bond order can now be expressed in terms of the derivatives of the Λ recursion coeﬃcients aΛ n and bn , ∞

∞ ∂aΛ ∂bΛ n n Λ Λ χ0n,n0 +2 χ0(n−1),n0 , (29) Θiα,jβ = −2 ∂Λiα,jβ ∂Λiα,jβ n=0 n=1 E Λ with the response function χ0m,n0 (Ef ) = π1 limη→0 f dEGΛ 0m (Z)Gn0 (Z) and the elements G0n = Gn0 following from the system of equations (Z − an )Gnm (Z) − bn Gn−1,m (Z) − bn+1 Gn+1,m (Z) = δn,m . The more recursion coeﬃcients included in (29), the more accurately the bond order will be approximated. The recursion coeﬃcients are related to the moments of the local density of states (LDOS) [105] and the site-diagonal Green’s function of (26) and (27) relates to the LDOS itself. Therefore, the recursive solution of (28) gives an approximation to LDOS in terms of its moments [107] (n) Hiα,j1 β1 Hj1 β1 ,j2 β2 . . . Hjn−1 βn−1 ,iα (30) µiα = E n niα (E)dE = alljk βk

and may be interpreted as self-returning (closed) loops of hops of length n for electrons over neighboring atoms. The local atomic environment deﬁnes the LDOS via the moments (30), which in turn is used to calculate the bond

230

Kurt Scheerschmidt

order in (21) and the (local) atomic force (23). The remaining free paramei,j instead of bij may be ﬁtted in the ters in the analytic form (8) with Ubond usual way. This is still a hard task, because the bond and the promotion energy involve diﬀerent parameters as the repulsive part and cutoﬀ parameters and screening functions for all terms have to be included. Besides an accurate ﬁt, the BOP requires well-parameterized TB matrix elements or parameter optimizing, and the problem of transferability [99, 108–110] has to be considered separately. For BOP of order n = 2 the bond-order term in the TS-representation reads bij = (−ssσij + ppσij )Θiσ,jσ − 2ppπij Θiπ,jπ and the numerical behavior of BOP2 and TS are approximately equivalent. The details for higher-order BOP are given in the papers of Pettifor’s group [2, 99]. The bij terms of the analytic BOP4 involve complex angular dependencies, partially beyond those neglected in Pettifor’s formalism. For structures with defects as well as the wafer bonding of diamond surfaces where π-bonds cannot be neglected, BOP can be found in [111–114] and will soon be published elsewhere with detailed derivations.

4 Applications It is impossible to review the rapidly growing number of successful applications of empirical MD in materials research. A few representative examples may give an impression of the wide range of problems considered. Isolated point defects are mainly simulated to check the quality of the ﬁt of the potential parameters. Surface reconstructions, adatom and absorption phenomena, growth processes, and especially extended defect structures and interactions can be investigated in detail. The analysis of dislocation core-structures [115], the use of core-structure data for studying dislocation kink motion [116] or the dislocation motion during nanoindentation [117] are examples. Interface investigations have a long tradition, as illustrated in the standard book for grain-boundary structure [118] and growth [119]. Heterophase interfaces, e.g., using a Khor–de-Sama potential for Al and TS for SiC [120] to simulate Al/SiC interfaces, demand special attention to the correct description of the misﬁt [121] to get good interface energies. Simulations with the Tersoﬀ potential and its modiﬁcations yield the correct diameter of the critical nuclei for the growth of Ge nanocrystals in an amorphous matrix [122], allow the study of growth, strains, and stability of Si- and C-nanotubes [123, 124], and SiC surface reconstructions to propose SiC/Si interface structures [125]. A review of atomistic simulations of diﬀusion and growth on and in semiconductors [126] demonstrates the applicability of SW and TS potentials in comparison with data from TB and DFT calculations. In the following, two examples of our work are discussed. Empirical MD simulations of ﬁrst, high-resolution electron microscopy (HREM) image contrasts in quantum dots (Sect. 4.1) and second, the physical processes at interfaces during wafer bonding (Sect. 4.2).

Empirical Molecular Dynamics

231

4.1 Quantum Dots: Relaxation, Reordering, and Stability A quantum dot (QD) is a nanometer-scaled island or region of suitable material free-standing on or embedded in semiconductor or other matrices. The possibility to arrange QDs into complex arrays implies many opportunities for scientiﬁc investigations and technological applications. However, depending on the growth techniques applied (mainly MBE and MOCVD), the islands diﬀer in size, shape, chemical composition and lattice strain, which strongly inﬂuences the conﬁnement of electrons in nanometer-scaled QDs. The shape, size and strain ﬁeld of single QDs, as well as quality, density, and homogeneity of equisized and equishaped dot arrangements determine the optical properties, the emission and absorption of light, the lasing eﬃciency, and other optoelectronic device properties [127, 128]. A critical minimum QD size is required to conﬁne at least one electron/exciton in the dot. A critical maximum QD size is related to the separation of the energy levels for thermally induced decoupling. Uniformity of the QD size is necessary to ensure coupling of states between QDs. The localization of states and their stability depend further on composition and strain of the QDs. The strain relaxation at facet edges and between the islands is the driving force behind self-organization and lateral arrangement, vertical stacking on top or between buried dots, or preordering by surface structuring. In addition, an extension of the emission range towards longer wavelengths needs a better understanding and handling of the controlled growth via lattice mismatched heterostructures or self-assembling phenomena (see, e.g., [129]). A wide variety of imaging methods are used to investigate growth, selfassembly, and physical properties of quantum dots. Among these the crosssectional HREM and the plan-view TEM imaging techniques are suitable methods to characterize directly shape, size, and strain ﬁeld [130]. But the HREM and TEM techniques images are diﬃcult to interpret phenomenologically, especially when separating shape and strain eﬀects. Modeling is essential to uniquely determine the features and provide contrast rules. In Fig. 4, the atomic structure of an InGaAs-QD in a GaAs matrix (for other systems cf. [130, 131]) is prescribed by geometric models and relaxed by MD simulations. Very diﬀerent dot shapes have been proposed and theoretically investigated: lens-shaped dots, conical islands, volcano-type QDs, and pyramids with diﬀerent side facets of type {011}, {111}, {112}, {113}, {136}, and both {011} + {111} mixed, etc. Some of these and a spherical cap are schematically presented in Fig. 4a; in simulations one or two monolayers (ML) thick wetting layers are included, too. The most important diﬀerence between the various structures is the varying step structure of the facets due to their diﬀerent inclination. There are at least two reasons to investigate these conﬁgurations [130]. First, small embedded precipitates always have facets; a transition between dome-like structure and pyramids due to changes in spacer distance, change the number and arrangement of the facets, and thus strain and electronic properties. Second, for highly faceted struc-

232

Kurt Scheerschmidt

Fig. 4. Structure modeling and image simulation of diﬀerent pyramidal-shaped quantum-dot conﬁgurations: (a) diﬀerent faceting, truncation, and wetting of pyramidal start models (matrix removed, models related to (001)-base planes), (b) relaxed complete model of a {011} pyramid (base length about 6 nm, 10 × 10 × 10supercell length 10 nm), (c) energy relaxation of a {011} quantum dot (potential Epot and total Etot energy versus time steps), (d) cross-sectional HREM and bright-ﬁeld diﬀraction contrast simulated for model (b) before and after relaxation assuming a standard 400 kV microscope at the Scherzer focus (i.e., ∆ = −40 nm, Cs = 1 mm, α = 1.2 nm−1 , t = 9 nm, δ = 8 nm−1 , cf. [130])

Empirical Molecular Dynamics

233

tures the continuum elasticity is practically inapplicable and ﬁnite element calculations must be done in 3-D instead of 2-D. However, the technique of ab-initio MC provides a more accurate prediction of the QD shapes than empirical MD [132]. The embedding of one perfect {011} pyramid in a matrix is demonstrated in Fig. 4b after prerelaxation. Figure 4c shows typical annealing behavior during empirical MD calculation, characterized by the potential Epot and the total energy Etot per atom. The energy diﬀerence Etot − Epot is equal to the mean kinetic energy and is thus directly related to the temperature of the system. After the prerelaxation of 5 ps at 0 K, an annealing cycle follows, 60 ps stepwise heat up to 600 K and cool down to 0 K, equilibrating the system at each heating step. The example here demonstrates a short cycle; most of the embedded QDs are relaxed at each T -step for at least 10 000 timesteps of 0.25 fs, followed by annealing up to about 900 K (the temperature is not well deﬁned with empirical potentials but is below the melting temperature). Whereas the structure in Fig. 4b is less strained, highly strained conﬁgurations occur due to the self-interaction of the QD in small supercells that correspond to a stacked sequence with very small dot distances. The extension of the supercell chosen in the simulations depends on the extension of the QD to be investigated, as well as on the overlap of the strain ﬁelds at the borders, to avoid self-interactions. Whereas Fig. 4b shows a relatively small supercell, investigations are made for supercells of up to 89 × 89 × 89 unit cells with a base length of the QD of 9 nm containing several million atoms. For the image simulations, subregions of the supercells are used, sliced into one atomic layer and applying the multislice image simulation technique. By comparing imaging for structures before and after relaxation, Fig. 4d demonstrates the enormous inﬂuence of the relaxations on the image contrast in cross-sectional HREM and TEM [130, 131]. In summarizing some of the results one can state that MD calculations with SW (CdZnSe) and TII (InGaAs, Ge) allow us to obtain well-relaxed structures, in contrast to the static relaxations performed with the Keating potential [133, 134]. With this insight into the atomic processes of rearranging and straining QDs at an atomic level the growth conditions for quantum dots may be enhanced as a ﬁrst step to tailoring their properties. 4.2 Bonded Interfaces: Tailoring Electronic or Mechanical Properties? Wafer bonding, i.e., the creation of interfaces by joining two wafer surfaces, has become an attractive method for many practical applications in microelectronics, micromechanics or optoelectronics [135]. The macroscopic properties of bonded materials are mainly determined by the atomic processes at the interfaces (clean and polished hydrophobic or hydrophilic surfaces, as schematically shown in Fig. 5) during the transition from adhesion to chemical bonding. For this, elevated temperatures or external forces are required, as could be revealed by MD simulations of hydrogen-passivated interfaces [136]

234

Kurt Scheerschmidt

Fig. 5. Wafer bonding at Si[100] surfaces: simulations of surface rearrangement for perfect alignment and slow heating. The ﬁgure describes the evolution of the atomic relaxation leading to bonded wafers

or of silica bonding [65]. Thus, describing atomic processes is of increasing interest to support experimental investigations or to predict bonding behavior. Already, slightly rescaled SW potentials predict the bond behavior via bond breaking and dimer reconﬁguration as shown in the snapshots explaining the possibility of covalent bonding at room temperature for very clean hydrophobic surfaces under UHV conditions [137]. Whereas the bonding of two perfectly aligned, identical wafers gives a single, perfectly bonded wafer without defects, miscut of the wafer results in steps on the wafer surfaces and edge dislocations at the bonded interfaces are created. In Fig. 6 the red color describes the potential energy above the ground state during wafer bonding over two-atomic steps. The upper terraces behave like perfect surfaces and the dimerized starting conﬁguration of Fig. 6a is rearranged and new bonds are created. The energy gained is dissipated and for slow heat transfer the avalanche eﬀect leads to bonding of the lower terraces, too. Two 60◦ dislocations remain and, depending on the rigid shift of the start conﬁguration, an additional row of vacancies [137]. The dislocations may split as simulated and observed in experiments [138].

Empirical Molecular Dynamics

235

Fig. 6. MD simulation of wafer bonding over surface steps. Note the dislocation relaxation for the initial conﬁguration (left), a snapshot during annealing up to 900 K, after 12.5 ps (middle) and the ﬁnal relaxed state (right)

Bonding wafers with rotational twist leads to a network of screw dislocations at the interface. A special situation is the 90◦ twist, which always occurs between monoatomic steps. A Stillinger–Weber potential applied to a 90◦ twist bonded wafer pair [16] yields a metastable ﬁvefold-coordinated interface with a mirror symmetry normal to the interface characterized by a P mm(m)layer group (cf. Fig. 2a). Using the Tersoﬀ or BOP-like potentials [113] and metastable or well-prepared starting conﬁgurations allows further structure relaxation and energy minimization. Figure 2b shows this relaxed conﬁguration, which is (2 × 2) reconstructed and consists of structural units with a 42m-(D2d) point group symmetry, called the 42m-dreidl. It should be emphasized that the dreidl structure is found to be the minimum energy conﬁguration also in DFT-LDA simulations [16]. However, the energies diﬀer from those given in [139, 140]. Much more important is the modiﬁcation of the band structure due to the diﬀerent interface relaxation that may enable engineering of the electronic properties: whereas the metastable conﬁguration (cf. Fig. 2c) yields semimetallic behavior, the dreidl structure (cf. Fig. 2d) yields a larger bandgap than in perfect lattices. The dreidl interface structure and its band-structure modiﬁcation is very similar to the essential building blocks proposed by Chadi [141] for group-IV materials. They describe geometry and properties of the transformation of Si and Ge under pressure and the special allo-phases as a new class of crystalline structures. A small misalignment of the wafers during wafer bonding yields bonded interfaces with twist rotation resulting in a checkerboard-like interface structure [142, 143]. Figure 7 shows some of the resulting minimum structures gained for higher annealing temperatures and diﬀerent twist rotation angles. Before the bonding process takes place, the superposition of the two wafers looks like a Moir´e pattern in the projection normal to the interface. After bonding and suﬃcient relaxation under slow heat-transfer conditions, almost all atoms have a bulk-like environment separated by misﬁt screw dislocations, which may have many kinks. The screw dislocation-network of the bonded wafer has a period half that of the Moir´e pattern. One ﬁnds more imperfectly bonded regions around the screw dislocations for smaller twist

236

Kurt Scheerschmidt

Fig. 7. MD relaxations of bonding rotationally twisted wafers ([001] and [110] views) with diﬀerent angles: (a) 2.8◦ , 22 nm box, orthogonal dimers, [001] view; (b) 6.7◦ , 9.2 nm box, orthogonal dimers, [001] and [110] views; (c) as (a) and (d) as (b) with parallel dimers

angles, whereas bonding at higher angles results in more or less widely spread strained interface regions. In Fig. 7 bonding with orthogonal start conﬁgurations (a,b) is compared to those with parallel dimer start conﬁgurations (c,d). Thus the bonding of Figs. 7a and b may be considered as bonding with an additional 90◦ twist rotation. Clearly the periodicity of the defect region is twice those of Figs. 7b and c smoothing out the interface, but creating additional shear strains. Irrespective of the chosen twist angles and box dimensions all ﬁnal structures yield bond energies of approximately 4.5 eV/atom at 0 K, however, varying slightly with the twist angle. A maximum occurs between 4◦ and 6◦ twist related to a change of the bonding behavior itself. The higher the annealing temperature the better the screw formation. In conclusion, simulation of the atomic processes at wafer-bonded interfaces oﬀers not only the tailoring of electronic properties, it is also an important step in understanding how to control the creation of special interface structures for strain accommodation or prepatterned templates (compliant substrates) [135] by rotational alignment.

5 Conclusions and Outlook Molecular dynamics simulations based on empirical potentials provide a suitable tool to study atomic processes that inﬂuence macroscopic materials properties. The applicability of the technique is demonstrated by calculating quantum-dot relaxations and interaction processes with defect creation at wafer-bonded interfaces. A brief overview describes the method itself and its advantages and limitations, i.e., the macroscopic relevance of the simulations versus the limited transferability of the potentials. The quality of the simulations and the reliability of the results depend on the coupling of the

Empirical Molecular Dynamics

237

atomistic simulations across length and timescales. Whereas the Lagrange formalism is well established for the embedding into suitable environments at the continuum level, the approximations of ﬁrst-principles-based potentials need continuous future work.

References [1] W. Kohn: Rev. Mod. Phys. 71, 1253 (1999) 214 [2] M. W. Finnis: Interatomic forces in condensed matter, in Oxford Series on Materials Modelling (Oxford University Press, Oxford 2003) 214, 215, 221, 222, 227, 230 [3] K. Ohno, K. Esforjani, Y. Kawazoe: Computational Materials Science: From ab initio to Monte Carlo Methods (Springer, Berlin, Heidelberg 1999) 214 [4] M. C. Payne, M. P. Teter, D. C. Allen, et al: Rev. Mod. Phys. 64, 1045 (1992) 214 [5] G. Galli, A. Pasquarello: First-principles molecular dynamics, in M. P. Allen, D. J. Tildesley (Eds.): Computer Simulation in Chemical Physics (Academic Publisher, Dordrecht, Netherlands 1993) pp. 261–313 214 [6] T. Frauenheim, G. Seifert, M. Elstner, et al: phys. stat. sol. B 217, 41 (2000) 214, 227 [7] D. R. Bowler, T. Miyazaki, M. J. Gillan: J. Phys.: Condens. Matter 14, 2781 (2002) 214, 227 [8] J. M. Soler, E. Artacho, J. D. Gale, et al: J. Phys.: Condens. Matter 14, 2745 (2002) 214, 227 [9] M. D. Segall, P. J. D. Lindan, M. J. Probert, et al: J. Phys.: Condens. Matter 14, 2717 (2002) 214 [10] R. Car, M. Parinello: Phys. Rev. Lett. 55, 2471 (1985) 214 [11] G. C. Csany, T. Albaret, M. C. Payne, A. DeVita: Phys. Rev. Lett. 93, 175503 (2004) 215 [12] P. Ruggerone, A. Kley, M. Scheﬄer: Bridging the length and time scales: from ab initio electronic structure calculations to macroscopic proportions, Comm. Condens. Matter Phys. 18, 261 (1998) 215 [13] R. M. Nieminen: J. Phys.: Condens. Matter 14, 2859 (2002) 215, 216 [14] R. E. Rudd, J. Q. Broughton: phys. stat. sol. B 217, 251 (2000) 215, 216 [15] B. I. Lundquist, A. Bogicevic, S. Dudy, et al: Comput. Mater. Sci. 24, 1 (2002) 215, 216 [16] K. Scheerschmidt, D. Conrad, A. Belov: Comput. Mater. Sci. 24, 33 (2002) 216, 235 [17] J. M. Haile: Molecular Dynamics Simulation: Elementary Methods (Wiley, New York 1992) 216 [18] D. C. Rapaport: The Art of Molecular Dynamics Simulation (Cambridge Univ. Press, Cambridge 1998) 216 [19] R. Haberlandt: Molekulardynamik: Grundlagen und Anwendungen (Vieweg, Braunschweig, Wiesbaden 1995) 216 [20] W. G. Hoover: Molecular dynamics, in Lecture Notes in Physics, vol. 258 (Springer, Berlin, Heidelberg 1986) 216

238

Kurt Scheerschmidt

[21] I. G. Kaplan: Theory of molecular interactions, in Studies in Physical and Theoretical Chemistry, vol. 42 (Elsevier Science Ltd., Amsterdam 1986) 216 [22] M. Sprik: Introduction to molecular dynamics methods, in K. Binder, G. Cicotti (Eds.): Monte Carlo and Molecular Dynamics of Condensed Matter Systems, vol. 49, Conf. Proc. Vol. (SIF, Bologna 1996) Chap. 2, pp. 47–87 216 [23] D. W. Heermann: Computer Simulation Methods in Theoretical Physics (Springer, Berlin, Heidelberg 1990) 216 [24] J. M. Ziman: Principles of the Theory of Solids (Cambridge Univ. Press, Cambridge 1972) 218 [25] S. W. deLeeuw, J. W. Perram, E. R. Smith: Proc. Roy. Soc. London A 373, 27 (1980) 218 [26] D. Wolf, P. Keblinski, S. R. Phillpot, J. Eggebrecht: J. Chem. Phys. 110, 8254 (1999) 218 [27] A. F. Voter: Phys. Rev. B 57, 13985 (1998) 218 [28] A. F. Voter, F. Montalenti, T. C. Germann: Ann. Rev. Mater. Res. 32, 321 (2002) 218 [29] W. Rullmann, H. Gunsteren, H. Berendsen: Mol. Phys. 44, 69 (1981) 221 [30] S. Nos´e: Mol. Phys. 52, 255 (1984) 221 [31] S. Nos´e: J. Chem. Phys. 81, 511 (1984) 221 [32] W. G. Hoover: Phys. Rev. A 31, 695 (1985) 221 [33] H. C. Andersen: J. Chem. Phys. 72, 2384 (1980) 221 [34] M. Parinello, A. Rahman: J. Appl. Phys. 52, 7182 (1981) 221 [35] L. Yang, D. J. Srolowitz, A. F. Yee: J. Chem. Phys. 107, 4396 (1997) 221 [36] G. P. Morriss, D. J. Evans: Phys. Rev. A 35, 792 (1987) 221 [37] D. J. Evans, G. P. Morriss: Statistical Mechanics of Nonequilibrium Liquids (Academic, London, New York 1990) 221 [38] J. D. Gale: Special Issue: Interatomic Potentials, Philos. Mag. B 73, 3 (1996) 221 [39] A. Horsﬁeld: Special Issue: Interatomic Potentials, Philos. Mag. B 73, 85 (1996) 221 [40] S. C. Price: Special Issue: Interatomic Potentials, Philos. Mag. B 73, 95 (1996) 221 [41] J. N. Murrell: Special Issue: Interatomic Potentials, Philos. Mag. B 73, 163 (1996) 221 [42] D. L. Cooper, T. Thorsteinsson: Special Issue: Interatomic Potentials, Philos. Mag. B 73, 175 (1996) 221 [43] M. C. Payne, I. J. Robertson, D. Thomssen, V. Heine: Special Issue: Interatomic Potentials, Philos. Mag. B 73, 191 (1996) 221 [44] Guest Editor A. F. Voter, V. Vitek: MRS-Bull. 21, 20 (1992) 221 [45] S. M. Foiles: MRS-Bull. 21, 24 (1992) 221 [46] M. Stoneham, J. Hardy, T. Harker: MRS-Bull. 21, 29 (1992) 221 [47] D. W. Brenner: MRS-Bull. 21, 36 (1992) 221 [48] A. P. Sutton, P. D. Goodwin, A. P. Horseﬁeld: MRS-Bull. 21, 42 (1992) 221 [49] N. A. Marks, M. W. Finnis, J. H. Harding, N. C. Pyper: J. Chem. Phys. 114, 4406 (2001) 222 [50] K. W. Jacobsen, J. K. Norskov, M. J. Puskas: Phys. Rev. B 35, 7423 (1987) 222 [51] N. A. Marks: J. Phys. Condens. Matter 14, 2901 (2002) 222 [52] M. S. Daw: Phys. Rev. B 39, 7441 (1989) 222

Empirical Molecular Dynamics

239

[53] Y. C. Wang, K. Scheerschmidt, U. G¨ osele: Phys. Rev. B 61, 12864 (2000) 222 [54] H. R. Trebin: Comp. Phys. Commun. 121–122, 536 (1999) 222 [55] A. K. Rappe, C. J. Casewit, K. S. Colwell, et al: J. Am. Chem. Soc. 114, 10024 (1992) 222 [56] W. F. van Gunsteren, H. J. C. Berendsen: Angew. Chem., Int. Ed. Engl. 29, 992 (1990) 222 [57] F. H. Stillinger, T. A. Weber: Phys. Rev. B 31, 5262 (1985) 222 [58] R. Biswas, D. R. Hamann: Phys. Rev. B 36, 6434 (1987) 222 [59] T. Takai, T. Halicioglu, W. A. Tiller: Scr. Metal. 19, 709 (1985) 222 [60] C. P. Herrero: J. Mater. Res. 16, 2505 (2001) 222 [61] A. K. Nakano, B. J. Berne, P. Vashista, R. K. Kalia: Phys. Rev. B 39, 12520 (1989) 223 [62] S. H. Garofalini: J. Non-Cryst. Solids 120, 1 (1990) 223 [63] D. Timpel, K. Scheerschmidt, S. H. Garofalini: J. Non-Cryst. Solids 221, 187 (1997) 223 [64] D. Timpel, K. Scheerschmidt: J. Non-Cryst. Solids 232–234, 245 (1998) 223 [65] D. Timpel, M. Schaible, K. Scheerschmidt: J. Appl. Phys. 85, 2627 (1999) 223, 234 [66] M. I. Baskes: Phys. Rev. B 46, 2727 (1992) 223 [67] M. W. Finnis, J. E. Sinclair: Philos. Mag. A 50, 45 (1984) 223 [68] J. Tersoﬀ: Phys. Rev. Lett. 56, 632 (1986) 223 [69] J. Tersoﬀ: Phys. Rev. B 38, 9902 (1989) 223 [70] J. Tersoﬀ: Phys. Rev. B 39, 5566 (1989) 223 [71] W. Dodson: Phys. Rev. B 35, 2795 (1987) 223 [72] G. C. Abell: Phys. Rev. B 31, 6184 (1985) 223 [73] D. W. Brenner: phys. stat. sol. B 217, 23 (2000) 223 [74] M. V. R. Murty, H. A. Atwater: Phys. Rev. B 51, 4889 (1995) 223 [75] D. W. Brenner: Phys. Rev. B 42, 9458 (1990) 223 [76] A. J. Dyson, P. V. Smith: Surf. Sci. 355, 140 (1996) 223 [77] K. Beardmore, R. Smith: Philos. Mag. A 74, 1439 (1996) 223 [78] K. Nordlund, J. Nord, J. Frantz, J. Keinonen: Comput. Mater. Sci. 18, 504 (2000) 223 [79] T. J. Lenosky, B. Sadigh, E. Alonso, et al: Model. Simul. Mater. Sci. Eng. 8, 825 (2000) 223 [80] S. D. Chao, J. D. Kress, A. Redondo: J. Chem. Phys. 120, 5558 (2004) 223 [81] H. Balamane, T. Halicioglu, W. A. Tiller: Phys. Rev. B 46, 2250 (1992) 223 [82] M. Kohyama, S. Takeda: Phys. Rev. B. 60, 8075 (1999) 223 [83] M. Gharaibeh, S. K. Estreicher, P. A. Fedders: Physica B 273–274, 532 (1999) 223 [84] S. K. Estreicher: phys. stat. sol. B 217, 513 (2000) 223 [85] W. Windl: phys. stat. sol. B 226, 37 (2001) 223 [86] S. Kohlhoﬀ, P. Gumbsch, H. F. Fischmeister: Philos. Mag. A 64, 851 (1991) 225 [87] R. E. Rudd, J. Q. Broughton: Phys. Rev. B 58, R5893 (1998) 225 [88] A. Y. Belov: Dislocations emerging at planar interfaces, in V. L. Indenbom, J. Lothe (Eds.): Elastic Strain Fields and Dislocation Mobility (Elsevier, Amsterdam 1992) pp. 391–446 225, 226 [89] J. E. Sinclair: J. Appl. Phys. 42, 5321 (1971) 225

240

Kurt Scheerschmidt

[90] D. G. Pettifor: Phys. Rev. Lett. 63, 2480 (1989) 225, 227 [91] C. M. Goringe, D. R. Bowler, E. Hernandez: Rep. Prog. Phys. 60, 1447 (1997) 227 [92] A. P. Horsﬁeld, A. M. Bratkovsky: J. Phys. Condens. Matter 12, R1 (2000) 227 [93] D. A. Papaconstantopoulos, M. J. Mehl: J. Phys. Condens. Matter 15, R413 (2003) 227 [94] D. G. Pettifor, I. I. Oleinik, D. Nguyen-Manh, V. Vitek: Comput. Mater. Sci. 23, 33 (2002) 227 [95] D. Pettifor: From Exact to Approximate Theory: The Tight Binding Bond Model and Many-Body Potentials., vol. 48, Springer Series (Springer, Berlin, Heidelberg 1990) 227 [96] D. G. Pettifor, I. I. Oleinik: Phys. Rev. B 59, 8487 (1999) 227 [97] D. G. Pettifor, I. I. Oleinik: Phys. Rev. Lett. 18, 4124 (2000) 227 [98] D. G. Pettifor, M. W. Finnis, D. Nguyen-Manh, et al: Mater. Sci. Eng. A 365, 2 (2004) 227 [99] A. P. Sutton: Electronic Structure of Materials (Clarendon Press, Oxford 1994) 227, 230 [100] A. P. Sutton, M. W. Finnis, D. G. Pettifor, Y. Ohta: J. Phys. C 35, 35 (1988) 228 [101] H. Hellmann: Einf¨ uhrung in die Quantenchemie (Deuticke, Leipzig 1937) 228 [102] R. P. Feynman: Phys. Rev. 56, 340 (1939) 228 [103] J. C. Slater, G. F. Koster: Phys. Rev. 94, 1498 (1954) 228 [104] C. Lanczos: J. Res. Natl. Bur. Stand. 45, 225 (1950) 228 [105] A. P. Horsﬁeld, A. M. Bratovsky, M. Fear, et al: Phys. Rev. B 53, 12694 (1996) 229 [106] R. Haydock: Recursive Solution of the Schr¨ odinger Equation, vol. 35, Solid State Physics (Academic, London, New York 1980) 229 [107] F. Ducastelle: J. Phys. 31, 1055 (1970) 229 [108] O. F. Sankey, D. J. Niklewski: Phys. Rev. B 40, 3979 (1989) 230 [109] I. Kwon, R. Biswas, C. Z. Wang, et al: Phys. Rev. B 49, 7242 (1994) 230 [110] T. J. Lenosky, J. D. Kress, I. Kwon, et al: Phys. Rev. B 55, 1528 (1997) 230 [111] D. Conrad: Molekulardynamische Untersuchungen f¨ ur Oberﬂ¨ achen und Grenzﬂ¨ achen von Halbleitern, Thesis, Martin-Luther-Universit¨ at, Halle (1996) 230 [112] V. Kuhlmann: Entwicklung analytischer bond-order Potentiale f¨ ur die empirische Molekulardynamik, Thesis, Martin-Luther-Universit¨ at, Halle (2006) 230 [113] D. Conrad, K. Scheerschmidt: Phys. Rev. B 58, 4538 (1998) 230, 235 [114] D. Conrad, K. Scheerschmidt, U. G¨ osele: Appl. Phys. Lett. 77, 49 (2000) 230 [115] T. Harry, D. Bacon: Acta Mater. 50, 195 (2002) 230 [116] V. V. Bulatov, J. F. Justo, W. Cai, et al: Philos. Mag. A 81, 1257 (2001) 230 [117] E. T. Lilleodden, J. A. Zimmermann, S. M. Foiles, W. D. Nix: J. Mech. Phys. Solids 51, 901 (2003) 230 [118] D. Wolf, S. Yip (Eds.): Materials Interfaces: Atomic-Level Structure and Properties (Chapman & Hall, London 1992) 230 [119] A. J. Haslam, D. Moldovan, S. R. Phillpot, et al: Comput. Mater. Sci. 23, 15 (2002) 230 [120] X. Luo, G. Qian, E. G. Wang, C. Chen: Phys. Rev. B 59, 10125 (1999) 230

Empirical Molecular Dynamics

241

[121] R. Benedek, D. N. Seidman, C. Woodward: J. Phys. Condens. Matter 14, 2877 (2002) 230 [122] K. J. Bording, J. Tafto: Phys. Rev. B 62, 8098 (2000) 230 [123] J. W. Kang, J. J. Seo, H. J. Hwang: J. Nanosci. Nanotechnol. 2, 687 (2002) 230 [124] D. Srivasta, D. W. Brenner, J. D. Schall, et al: J. Phys. Chem. B 103, 4330 (1999) 230 [125] C. Koitzsch, D. Conrad, K. Scheerschmidt, U. G¨ osele: J. Appl. Phys. 88, 7104 (2000) 230 [126] E. Kaxiras: Comput. Mater. Sci. 6, 158 (1996) 230 [127] D. Bimberg, M. Grundmann, N. N. Ledentsov: Quantum Dot Heterostructures (John Wiley & Sons., Chicester 1999) 231 [128] L. W. Wang, A. Zunger: Pseudopotential theory of nanometer silicon quantum dots, in P. V. Kamat, D. Meisel (Eds.): Semiconductor Nanoclusters – Physical, Chemical, and Catalytic Aspects (Elsevier, Amsterdam, New York 1997) 231 [129] H. Lee, J. A. Johnson, M. Y. He, et al: Appl. Phys. Lett. 78, 105 (2001) 231 [130] K. Scheerschmidt, P. Werner: Characterization of structure and composition of quantum dots by transmission electron microscopy., in M. Grundmann (Ed.): Nano-Optoelectronics: Concepts, Physics and Devices (Springer, Berlin, Heidelberg, New York, Tokyo 2002) Chap. 3, pp. 67–98 231, 232, 233 [131] K. Scheerschmidt, D. Conrad, H. Kirmse, R. Schneider, W. Neumann: Ultramicroscopy 81, 289 (2000) 231, 233 [132] E. Pehlke, N. Moll, A. Kley, M. Scheﬄer: Appl. Phys. A 65, 525 (1997) 233 [133] P. N. Keating: Phys. Rev. 145, 637 (1966) 233 [134] Y. Kikuchi, H. Sugii, K. Shintani: J. Appl. Phys. 89, 1191 (2001) 233 [135] Q. Y. Tong, U. G¨ osele: Semiconductor Wafer Bonding: Science and Technology (Wiley, New York 1998) 233, 236 [136] D. Conrad, K. Scheerschmidt, U. G¨ osele: Appl. Phys. Lett. 71, 2307 (1997) 233 [137] D. Conrad, K. Scheerschmidt, U. G¨ osele: Appl. Phys. A 62, 7 (1996) 234 [138] A. Y. Belov, R. Scholz, K. Scheerschmidt: Philos. Mag. Lett. 79, 531 (1999) 234 [139] A. Y. Belov, D. Conrad, K. Scheerschmidt, U. G¨ osele: Philos. Mag. 77, 55 (1998) 235 [140] A. Y. Belov, K. Scheerschmidt, U. G¨ osele: Phys. Status Solidi A 159, 171 (1999) 235 [141] D. J. Chadi: Phys. Rev. B 32, 6485 (1985) 235 [142] K. Scheerschmidt: MRS Proc. 681E, I2.3 (2004) 235 [143] K. Scheerschmidt, V. Kuhlmann: Interf. Sci. 12, 157 (2004) 235

Index ab-initio, 215, 216, 233

algorithm, 217, 229

absorption, 230, 231

alignment, 234–236

adatom, 230

amorphous, 230

242

Kurt Scheerschmidt

anharmonic, 222 annealing, 233, 235, 236 autocorrelation function, 224 band structure, 216, 235 basis set, 214 Berendsen, 221 Boltzmann, 219, 224 bond order, 216, 222, 223, 228–230 bond-order potential, 214, 215, 217, 223, 227, 230, 235 Born–Oppenheimer, 214 bulk modulus, 223 canonical, 220, 224, 225 chemical potential, 220 classical, 213, 216, 218, 219 cluster, 223 cohesive energy, 218, 223, 227, 228 concentration, 220 conjugate gradient, 214, 215 conservative, 217, 220 correlation, 224 Coulomb, 217, 218, 222 coupling, 225, 231, 236 covalent, 223, 234 crack, 225 cutoﬀ, 217, 228 decay, 217 degeneracy, 228 density matrix, 228, 229 density of states, 227, 229 density-functional theory, 214 DFT, 214, 216, 222, 223, 227, 230, 235 diamond, 230 diﬀusion, 214, 224, 230 dislocation, 230, 234, 235 distribution function, 219 EDIP, 222 eigenstates, 227 elastic embedding, 216, 220 electron, 222, 227–229, 231 embed, 216, 220, 225, 231, 233, 237 embedded, 215, 216, 222, 223, 227, 231, 233 empirical, 213–216, 222–225, 230, 233, 236

EMT, 222 energy level, 231 entropy, 221, 225 equilibrium, 222, 224, 226, 227 ergodic, 220, 224 Ewald, 218, 222 exchange, 220, 228 exchange-correlation, 214 exciton, 231 ﬁnite element, 214 ﬁrst principles, 214, 225, 237 ﬂuctuation, 221 force, 213–217, 219, 221–223, 226–228, 230, 231, 233 Fourier, 225 free energy, 224, 225 Ge, 223, 230, 233, 235 general gradient approximation, 214 GGA, 214 Gibbs, 219, 220, 225 glass, 223 grain boundary, 230 grand-canonical, 220, 225 Green’s function, 227, 229 Green–Kubo, 224 ground state, 228, 234 Hamiltonian, 218–220, 227, 228 handshaking, 215, 219, 225 Heisenberg, 219 Hellmann–Feynman, 214, 228 heterostructure, 231 hopping, 228 hybrid, 222 hydrogen, 233 imaginary, 229 interface, 215, 216, 225, 230, 233–236 internal energy, 224 isothermal, 224 jellium, 222 kink, 230 Lagrange, 219, 221, 237 Lagrangian, 218, 219, 221, 225–227 LDA, 214

Empirical Molecular Dynamics Lennard–Jones, 222 Liouville, 219 liquid, 219 localization, 213, 217, 231 Madelung, 218, 222 Maxwell, 221 melting, 233 microcanonical, 217, 220, 221, 225 misﬁt, 230, 235 molecular dynamics, 213, 216 Morse, 222 multipole, 223, 226 nanometer, 231 Newton, 227 Nos´e, 221 optical, 231 optoelectronic, 231 pair-distribution function, 220, 224 Parrinello, 221 partition function, 219, 224 periodic boundary conditions, 220 periodicity, 236 perturbation, 221, 222 phase space, 219, 220 phonon, 223, 226 point defect, 223, 230 potential, 214–218, 220–223, 225–228, 230, 233–235 precipitates, 231 pseudoatom, 222 pseudopotential, 214, 222 quantum dot, 225, 230, 231, 233, 236 radial-distribution function, 224 recursion, 227, 229 relaxation, 215, 216, 231, 233, 235, 236 repulsive, 222, 230 rotational, 235, 236

243

scattering, 225 screening, 218, 222, 230 self-interaction, 217, 233 self-organization, 231 semiempirical, 216, 223 shear, 224, 236 Si, 222, 223, 230, 235 SIESTA, 214 Slater, 227, 228 spherical harmonic, 223 spin degeneracy, 228 statistical, 216, 219, 224 Stillinger–Weber, 222, 235 strain, 221, 224, 225, 230, 231, 233, 236 stress, 221, 224 supercell, 220, 233 surface, 215, 216, 220, 230, 231, 233, 234 symmetric, 221 symmetry, 235 Taylor, 217, 222 temperature, 218, 221, 224, 233–236 Tersoﬀ, 223, 228, 230, 235 thermostat, 220, 221 tight binding, 214, 215, 222 total energy, 217, 220, 233 trajectory, 219, 220 transferability, 222, 230, 236 transition, 217, 218, 222, 228, 231, 233 transport, 221, 224 Van der Waals, 222 variational, 218 velocity autocorrelation, 224 Verlet, 217 wafer bonding, 215, 230, 233–235 water, 223 wavelength, 231 X-ray, 225

Defects in Amorphous Semiconductors: Amorphous Silicon D.A. Drabold and T.A. Abtew Department of Physics and Astronomy, Ohio University, Athens, Ohio [email protected]

Abstract. Defects in disordered (amorphous) semiconductors are discussed, with an emphasis on hydrogenated amorphous silicon. The general diﬀerences between defect phenomena in crystalline and amorphous hosts are described, and the special importance of the electron–phonon coupling is stressed. Detailed calculations for amorphous Si are presented using accurate ﬁrst principles (density-functional) techniques. The various approximations of ab-initio simulation aﬀect aspects of the network structure and dynamics, and suitably accurate approximations are suggested. Defect dynamics and the motion of hydrogen in the network are reported.

1 Introduction This book is primarily concerned with defects in crystalline materials. In this Chapter, we depart from this and discuss defects in amorphous materials. In the Chapter of Simdayankin and Elliott, a most interesting feature of amorphous materials, photoresponse, is discussed in detail. As in the case of crystals, defects determine key features of the electronic, vibrational and transport properties of amorphous materials [1–3]. These are often precisely the properties that are relevant to applications. In this Chapter we strongly emphasize amorphous silicon (a-Si), while not focusing on it exclusively. This is signiﬁcantly due to the background of the authors and constraints on the length of the Chapter, but it is also true that a-Si oﬀers at least a somewhat generic theoretical laboratory for the study of disorder, defects, and other aspects of amorphous materials in general. The outline of this Chapter is as follows: First, we brieﬂy survey amorphous semiconductors. Next, we deﬁne the notion of a defect, already a somewhat subtle question in an environment that is intrinsically variable in structure. In the fourth section, we discuss the generic electronic and vibrational attributes of defects in amorphous solids, and brieﬂy comment on the current methods for studying these systems. In Sect. 5, we discuss calculations of the dynamics of defects in the a-Si:H network, of critical importance to the stability and practical application of the material.

D. A. Drabold, S. K. Estreicher (Eds.): Theory of Defects in Semiconductors, Topics Appl. Physics 104, 245–268 (2007) © Springer-Verlag Berlin Heidelberg 2007

246

D.A. Drabold and T.A. Abtew

2 Amorphous Semiconductors Amorphous materials and glasses are among the most important to human experience with applications ranging from primitive obsidian weapons to optoelectronics. Today, every oﬃce in the world contains storage media for computers (for example DVD-RW compact disks) that exploit the special reversible laser-driven amorphization/crystallization transition properties of a particular GeSbTe glass. The same computer uses crystalline Si chips that depend critically upon the dielectric properties of a-SiO2 . With increasing pressure on global energy markets, it is notable that some of the most promising photovoltaic devices are based upon amorphous materials such as a-Si:H because of the low cost of the material (compared to crystalline devices) and the ability to grow thin ﬁlms of device-quality material over wide areas. The internet depends upon ﬁber-optic glass light pipes that enable transmission of information with bandwidth vastly exceeding that possible with wires. This list is the proverbial tip of the iceberg. Experimental measurements for structure determination, such as X-ray or neutron diﬀraction, lead easily to a precise determination of the structure of crystals. Nowadays, protein structures with thousands of atoms per unit cell are readily solved. The reason for this impressive success is that the diﬀraction data (structure factor) consists of a palisade of sharply deﬁned spikes (the Bragg peaks), arising from reﬂection from crystal planes. For amorphous materials, the same experiments are rather disappointing; smooth broad curves replace the Bragg peaks. The wavelength-dependent structure factor may be interpreted in real space through the radial distribution function (RDF), which is easily obtained with a Fourier transform of the structure factor. In crystals, the RDF consists again of spikes, and the radii at which the spikes occur are the neighbor distances. In the amorphous case, the RDF is smooth, and normally has broadened peaks near the locations of the ﬁrst few peaks of the crystal. This similarity in the small-r peak positions reﬂects a tendency of amorphous materials to attempt to mimic the local order of the crystalline phase in the amorphous network, but usually with modest bond-length and bond-angle distortions. At distances beyond several nearest-neighbor spacings, similarities between crystalline and amorphous pair correlations wane, and the pair correlations decay to zero after tens of ˚ Angstroms in the amorphous material (this number is system dependent). From an information theoretic point of view (for example, consideration of the Shannon–Jaynes information entropy [4]), it is clear that there is less information inherent in the (smooth) data for the amorphous case relative to the crystal. So, while it is possible to invert the diﬀraction data from crystals to obtain structure determination (with some assumptions to ﬁx the phase problem), such a process fails for the amorphous case and many studies have emphasized the multiplicity of distinct structures possible that can reproduce measured diﬀraction data. In this sense we are in a situation rather like highenergy or nuclear physics where there are sum rules that must be obeyed,

Defects in Amorphous Semiconductors: Amorphous Silicon

247

but the sum rules by themselves oﬀer an extremely incomplete description of the physical processes. The ﬁrst goal of theoretical work in amorphous materials is to obtain an experimentally realistic model consistent with all trusted experiments and also accurate total energy and force calculations. Early models of amorphous materials were made by hand, but this approach was soon supplanted by simulations with the advent of digital computers. A variety of modeling schemes based upon simulated atomic dynamics (so-called molecular-dynamics), Monte Carlo methods, methods based upon attempts to obtain the structure from the diﬀraction measurements (most sensibly done with constraints to enforce rules on bonding) and even hybrids between the last two are in current use [5–8]. Impressive progress has been made in the last 25 years of modeling, and highly satisfactory models now exist for many amorphous materials, among these: Si, Si:H, Ge, C, silica, elemental and binary chalcogenides [9–12]. Empirically, systems with lower mean coordination (ﬂoppier in the language of Thorpe [13]) are easier to model than higher-coordination systems. Multinary materials tend to be more challenging than elemental systems as the issue of chemical ordering becomes important and also these systems are harder to model accurately with conventional methods. Empirical potentials, tight-binding schemes and ab-initio methods are used for modeling the interatomic interactions [5, 14– 16]. In the area of defects in amorphous semiconductors, it is usually the case that ﬁrst-principles interactions are required. Where electronic properties of amorphous semiconductors are concerned, k-space methods are not useful as the crystal momentum is not a good quantum number (the translation operator does not commute with the Hamiltonian). Rather, one focuses on the density of electron states, and on individual eigenvectors of the Hamiltonian, especially those near the Fermi level. The electronic density of states is usually qualitatively like that of a structurally related crystal, but broadened by disorder. In Fig. 1, we illustrate these features with a “real” calculation on a 10 000-atom model of a-Si [11, 17]. The sharp band edges expected in crystals are broadened into smooth “bandtails”. The tails are created by structural disorder; early Bethe lattice calculations demonstrated that strained bond angles lead to states pushed out of the band (into the forbidden optical gap), and loosely, the more severe the defect, the further into the gap. It is known from optical studies of amorphous semiconductors that all such systems have band-tails decaying exponentially into the gap. While the optical spectrum is a convolution involving both tails, photoemission studies have separately probed the valence tail and conduction tails particularly in a-Si:H [18], and found that both decay exponentially, albeit with diﬀerent rates and a temperature dependence (quite diﬀerent for the two tails) that suggests the importance of thermal disorder beside the structural order we have stressed so far [19]. The ﬁeld of amorphous semiconductors is a vast area in which many books and thousands of papers have been written, and it is impossible to do justice even to the specialized topic of defects. For this reason, we emphasize a few

248

D.A. Drabold and T.A. Abtew

Fig. 1. Electronic density of states near a band edge in a 10 000-atom model of amorphous Si. Insets show |ψ|2 , indicating parts of the cell in which the defect wavefunctions are localized. The mobility edge separating localized and extended states is indicated. The “band-tail” extends from about −15.5 eV to the mobility edge [17]

questions of particular current interest, and recommend the comprehensive treatments of Elliott and Zallen [20, 21] for general discussion of amorphous materials including defects.

3 Defects in Amorphous Semiconductors 3.1 Deﬁnition of Defect Static Network A complete discussion of defects in amorphous materials may be found in Chap. 6 of the book by Elliott [20]. Evidently, the term defect implies a departure from the typical disorder of an amorphous network. Perhaps it is not surprising that it is not possible to produce a deﬁnition of defect without some arbitrary character. Thus, in deﬁning a coordination defect, one introduces a distance that deﬁnes whether a pair of atoms is bonded or not. So long as the model structure contains no bonds very close to the critical length, the deﬁnition is unambiguous. In amorphous materials there is usually

Defects in Amorphous Semiconductors: Amorphous Silicon

249

a well-deﬁned (deep) minimum in the pair-correlation function between the ﬁrst- and second-neighbor peaks, which gives a reasonable justiﬁcation for selecting the distance at which the minimum occurs as a cutoﬀ length for deﬁnition of coordination. When one accounts for thermal motion of the atoms, the situation is murkier, as we describe below. If the primary interest is electronic properties of the amorphous semiconductor, one can introduce an electronic criterion to identify defects. As for the geometrical criterion, such a deﬁnition is necessarily formulated as a suﬃcient departure from the mean. An electronic defect may be deﬁned as a structural irregularity that produces a suﬃciently localized electronic eigenstate. The ambiguous point here is the modiﬁer “suﬃciently”: isolated states in the middle of the gap (such as a threefold “dangling-bond” state in a-Si) are easily recognized as defects with a spatially conﬁned wavefunction. Other less-localized states stemming from other network defects may be better characterized as part of the band-tailing. In the same spirit, the chemical bond order (essentially oﬀdiagonal elements of the single-particle density matrix) may be used to identify defects, but a cutoﬀ will be required as always to deﬁne the line between bonded and not! A simple quantitative measure of localization is given below. To contrast the geometrical and electronic deﬁnitions of defects, welllocalized electronic eigenstates do correspond to network irregularities (either structural, chemical or both) and suﬃciently large geometrical irregularities manifest themselves as localized states in a spectral gap in the electronic spectrum (note that this does not necessarily have to be the optical gap (the gap that contains the Fermi level) – other spectral gaps or even the extremal band edges can exhibit these states). Dynamic Network The schemes to deine defects outlined above are consistent for suﬃcient departure from the mean structure. To a surprising degree, however, room-temperature thermal disorder implies the existence of thermally induced geometrical defect ﬂuctuations. Thus, in an ab-initio simulation of a-Si, the number of ﬁvefold “ﬂoating” bonds varied between 0 and 10 in a 2 ps roomtemperature run for a 216-atom unit cell with coordination deﬁned by a 2.74 ˚ A bond distance [19]. At face value this is astonishing, suggesting that 5 % of the atoms change their coordination in thermal equilibrium at room temperature! If the electronic and geometrical deﬁnitions were identical, it would imply that states should be jumping wildly into and out of the gap. Of course this is not the case, though it is true that instantaneous Kohn–Sham energy eigenvalues in the gap do thermally ﬂuctuate [19]. This example illustrates that geometrical defects are not necessarily electronic defects. One can also easily see that electronic defects are not necessarily coordination defects: while an atom may nominally possess ideal (8-N rule) coordination,

250

D.A. Drabold and T.A. Abtew

substantial bond-angle distortions can also induce localized electronic states. We present new simulations of defect dynamics in Sect. 5. 3.2 Long-Time Dynamics and Defect Equilibria It is apparent from a variety of experiments in a-Si:H that there are reversible, temperature-dependent changes that occur in defect type and concentration. At its simplest, the idea is that particular defects have a characteristic energy in an amorphous material. It may be that these energies are not substantially removed from the typical conformations of the host. Because the amorphous network does not possess long-range order, it is possible for a small number of atoms to move to convert one kind of defect into another, without a huge cost in energy. These ideas can predict the temperature dependence of some electronic properties, for example quantities like the density and character of band-tail states [22–25]. By analyzing a variety of experiments, Street and coworkers [26] have demonstrated that the idea of defect equilibrium is essential. At present the approach is phenomenological to the extent that the microscopic details of the defects involved are not certainly known or even needed, but in principle these ideas could be merged with formation energies and other information from ab-initio simulations to make a ﬁrst-principles theory of defect equilibria. The potential union between the phenomenological modeling and simulation is also potentially a good example of “bridging timescales” though there is much work still required on the simulation side to realize this goal. 3.3 Electronic Aspects of Amorphous Semiconductors Localization A remarkable feature of electron states in crystals is that the wavefunctions have support (are nonzero) throughout the crystal, apart from surface effects. Such states are called extended. The utility of Bloch’s theorem is that it reduces the formulation of the electronic structure problem for the inﬁnite periodic system to a simpler form: calculation within a single unit cell on a grid of k crystal momentum points. Thus, for crystals, information about the electronic structure is provided by band-structure diagrams. Such diagrams are not useful in amorphous systems, and furthermore, in amorphous materials, some states may not be extended. To model the electronic consequences of disorder, it is usual to adopt a tight-binding (either empirical or ab initio) description of the electron states, and a Hamiltonian schematically of the form: εi |ii| + Jij |ij| . (1) H= i

ij,i=j

Defects in Amorphous Semiconductors: Amorphous Silicon

251

To keep the number of indexes to a minimum, we suppose that there is one orbital per site (indexed by i). In this equation, the εi specify the atomic energy at each site (in an elemental system, this would be constant for all sites) and Jij is a hopping integral that depends on the coordinates of the atoms located at sites i and j. The topological disorder of a particular realization of an amorphous network (e.g., a structural model) is manifested through the oﬀdiagonal or hopping terms Jij . An enormous eﬀort has been devoted to studying the properties of the eigenvectors of H, and also the critical properties (e.g., of quantum phase transitions [17]). In realistic studies of the electronic localized–delocalized transition [17] (here “realistic” means large-scale electronic structure calculations in which the disorder in the Hamiltonian matrix is obtained from experimentally plausible structural models, rather than by appealing to a random number generator), it is found that the eigenstates near midgap are spatially compact (localized) and for energies varied from midgap into either the valence or conduction-bands, the states take “island” form: a single eigenstate may consist of localized islands of charge separated by volumes of low charge density. The islands themselves exhibit exponential decay, and the decay lengths for the islands increase modestly from near midgap to the mobility edge. The states become extended with approach to the mobility edge by proliferation (increasing number) of the islands [17, 22]. The qualitative nature of this localized to extended transition is similar for electronic and vibrational disorder of diverse kinds and also conventional Anderson models. Thus, in important ways the localized to extended transition is universal [17]. Characterizing Localized States As we have discussed, the concept of localized states is a central one for amorphous materials and indeed defective systems in general. The question immediately arises: given an electronic eigenvector expressed in some representation, how can we quantify the degree of localization? The most widely adopted gauge of localization is the so-called “inverse participation ratio” (IPR), which is deﬁned as: I(E) =

N

q(n, E)2 ,

(2)

n=1

where N is the number of atoms and q(n, E) is a Mulliken (or other) charge on atom n, and the analysis is undertaken for a particular energy eigenstate with energy E. This measure ranges from N −1 (N number of sites) for an ideally extended state to 1 for a state perfectly localized to one site. One can use other measures, such as the information entropy, but at a practical level, we have found that the IPR and information entropy produce qualitatively (not quantitatively) similar results for the localization. IPR is a simple tool for categorizing the zoo of extended, localized and partly localized states of

252

D.A. Drabold and T.A. Abtew

amorphous semiconductors with defects [27]. As quantum chemists know, all such deﬁnitions are basis dependent, and thus care is needed in the interpretation of local charges, IPR and related quantities [28]. Locality of Interatomic Interactions For atomistic simulation of any materials, a fundamental measure of the spatial nonlocality of interatomic interactions is the decay of the single-particle density matrix, or equivalently, the decay characteristics of the best localized Wannier functions that may be constructed in the material. The density matrix is deﬁned as: ψi∗ (r )ψi (r) , (3) ρ(r, r ) = ioccupied

where ψi are eigenfunctions of the Hamiltonian in position representation. In a typical condensed-matter system, the ψi are oscillating functions, almost all of which will be delocalized through space. Consequently, one can expect “destructive interference” eﬀects as in other wave phenomena when many wiggling functions are superposed as in (3), which can make ρ(r, r ) decay ˆ is the Hamiltonian, then the electronic conrapidly for large |r − r |. If H ˆ If the trace is carried out in tribution to the total energy is E = T r(ˆ ρH). the position representation, one can then see that the decay of the density matrix provides information about the locality of the interatomic potential. The details of the chemistry and structure of the material determine this decay length, and the full results even for the asymptotic decay in a greatly simpliﬁed two-band model are too complicated to reproduce here [29]. For a material with a ﬁnite optical gap as we assume in this Chapter, the decay is ultimately exponential and the decay is faster for larger optical gaps. Recently, the density matrix has been explicitly computed for a structurally realistic 4096-atom model [10] of a-Si that was fourfold coordinated, but with some large bond-angle distortions. There are two key conclusions from this work: 1. the spatial nonlocality of interatomic interactions is very similar in a-Si and c-Si (because the density matrix decays in a similar fashion for both) and 2. defect centers in a-Si (in this model associated with bondangle distortions) have Wannier functions with asymptotic decay similar to ordinary (tetrahedral) sites (of course the short-range behavior involving the ﬁrst few neighbors may be quite diﬀerent) [22]. 3.4 Electron Correlation Energy: Electron–Electron Eﬀects For a localized single-particle defect state, one must consider the possibility of the state being occupied by zero, one or two (opposite spin) electrons. Consideration of the energetics of these various occupations led in the 1970s and 1980s to insights into the nature of defects, particularly in chalcogenide materials. Typically the electron–electron Coulomb repulsion costs a net energy

Defects in Amorphous Semiconductors: Amorphous Silicon

253

(usually labeled “U ”) to enable two electrons to occupy the same localized spatial state. This is called a “positive U ” defect center (the name comes from the symbol used in a Hubbard Hamiltonian to model the electron–electron interaction). In a-Si:H, U > 0 for the dangling-bond. It is worth mentioning that the accurate calculation of U is a challenging task for the conventional density-functional methods, as these are essentially mean-ﬁeld methods and appear to consistently overestimate the delocalization of defect states. When the possibility of structural relaxation is considered as the second opposite-spin electron is added to the localized state, a negative eﬀective U , implying a net energy lowering for double occupation, can emerge. This is observed in chalcogens, and as pointed out by early workers, explains the pinned Fermi level and the diamagnetism of the materials (that is, lack of unpaired spins and so the absence of an ESR signal). It follows that double occupancy implies that defects are charged, and the chemistry (p bonding) of the chalcogens like S or Se leads to the occurrence of “valence alternation pair” defects. Thus, careful simulations reveal that isolated dangling-bonds in a-Se are unstable, and are likely to convert instead into VAPs [30]. Elliott discusses these points thoroughly [20].

4 Modeling Amorphous Semiconductors 4.1 Forming Structural Models For amorphous materials we immediately face a challenging problem: What is the atomistic structure of the network? Usually there is a strong tendency for particular local structure (chemical identity of neighbors, and geometrical bonding characteristics), but this preference is only approximately enforced: there is a characteristic distribution of bond lengths and bond angles that is dependent upon both the material and its preparation. Thus, in “better-quality” a-Si samples, almost all of the atoms are four-coordinated, and the bond angle between a reference Si atom and two neighbors is within about 10 degrees of the tetrahedral angle: a strong echo of the chemistry and structure of diamond. In binary glasses (for example GeSe2 ), Ge is essentially always fourfold coordinated, and Ge only rarely bonds to Ge. Also, as one would expect from crystalline phases of GeSe2 or simple considerations of chemical bonding, the glass is made up predominantly of GeSe4 tetrahedral, again with Se–Ge–Se bond angles close to the tetrahedral angle [31–37]. As reviewed by Thorpe [38], the ﬁrst attempt to understand glasses was based upon the idea that amorphous materials were microcrystalline with a very ﬁne grain size. Eventually, it became clear that this model could not explain the structural experiments that were available. The idea that was ultimately accepted was advanced in 1932 by Zachariasen [39] for amorphous SiO2 , the “continuous random network” (CRN) model. Here, the local chemical requirements (four-coordinated Si bonded only to two-coordinated O, and

254

D.A. Drabold and T.A. Abtew

no homopolar bonds) were enforced, but there was local disorder in bond angles and to a smaller degree, bond lengths. Such networks do not possess long-range structural order. Zachariesen’s ideas were taken seriously much later starting in the 1960s, when comparisons to experiment showed that the idea had real promise. The next step was to use computers to help in making the models. An early computation was performed using a Monte Carlo approach. The idea was to put atoms inside a simulated box and move the atoms at random [40]. At each step the radial distribution function was computed and if a random move pushed the model closer to the experimental data, the move was kept, otherwise moves were retained with Metropolis probability. This is very similar in spirit to a current method, the so-called reverse Monte Carlo (RMC) method [8]. These approaches are information theoretic in spirit: use the available information to produce the model. While this is an eminently reasonable idea, the problem is that merely forcing agreement with diﬀraction data (pair correlations) grossly underconstrains the model: there are many conﬁgurations that agree beautifully with diﬀraction data but make no sense chemically or otherwise. In the 1980s, Wooten, Weaire and Winer (WWW) [9], introduced a Monte Carlo scheme for tetrahedral amorphous materials with special bondswitching moves, and energetics described by Keating springs and by requiring the network to be fourfold coordinated. They applied their method to a-Si and a-Ge with remarkable success. Here, the disorder of the real material was somehow captured by what appeared then to be a completely ad-hoc procedure. This method and improved versions of it are still the “gold standard” for creating models of amorphous Si. Years later, Barkema and Mousseau [11] showed that the likely reason for the success of the WWW scheme is that on long time-scales, the WWW moves occur quite naturally! Nowadays, the great majority of computer simulations are done using the molecular-dynamics method. The idea is to mimic the actual process of glass formation. To start with, one needs an interatomic potential that describes the interactions in the material. Typically, a well-equilibrated liquid is formed not far above the melting point, then the kinetic energy of the system is gradually reduced (by using some form of dissipative dynamics, such as velocity rescaling at each time step). Eventually there is structural arrest (the computer version of the glass transition), and a structural model results that may be useful for further study. Such calculations are often useful, but it needs to be clearly understood that there is little real similarity to the actual quenching process for glasses, which proceeds far more slowly in nature. As a ﬁnal oddity, the “melt-quench” approach is often used even for materials that do not form glasses (for example, a-Si). Results are especially poor for this case.

Defects in Amorphous Semiconductors: Amorphous Silicon

255

4.2 Interatomic Potentials To perform a molecular-dynamics simulation, or even a simulation of a mere relaxation of a network near a defect, it is necessary to compute the forces on the atoms in the material. This is never easy, and oﬀers a particular challenge in amorphous materials, as there are usually a variety of bonding environments in the network, and empirical potentials tend to be most accurate/reliable near conformations that were used in a ﬁtting process used to obtain them. The presence of defects exacerbates this further, as coordination or chemical order may be radically diﬀerent for the defect relative to the rest of the material (and thus harder to describe with a simple interatomic interaction). Also, the complexity of interatomic potentials grows rapidly with the number of distinct atomic species, so that even for binary systems, there are very few reliable empirical potentials available. The reason why it is diﬃcult to compute accurate interatomic potentials is that the interatomic forces are obtained from the electronic structure of the material. Thus, the details of bonding, electron hybridization, all depend in minute detail upon the local environment (coordination, bond lengths, bond angles, on the environment of the neighboring atoms and so on). The way out is to adopt an approach in which the electronic structure is directly computed in some approximate form. This has been done with some success using empirical tight-binding Hamiltonians [41, 42]. A tremendous advance for defects in semiconductors, but a particular beneﬁt for study of amorphous materials was the advent of practical densityfunctional codes. The union of density-functional methods and molecular-dynamics is now mature, and one can obtain excellent canned codes that can be used to undertake simulations of complex systems. Of course there is important background knowledge (of amorphous materials, electronic structure and simulation) needed. 4.3 Lore of Approximations in Density-Functional Calculations Defect calculations typically must be carried out using robust approximations for the Kohn–Sham states. The density-functional basis set upon which the Kohn–Sham orbitals are represented, and spin polarization are the main quantities that need to be considered. Where the basis set is concerned, the prime issue is completeness: the adequacy of the basis functions to approximate the “true” (complete basis limit) Kohn–Sham orbitals. Spin polarization is of particular importance in simulations if there are unpaired spins in the model (as for example a singly occupied dangling-bond state at the Fermi level). The choice of density-functionals is most important for an accurate estimate of energetics: the use of gradient approximations tends to ameliorate the tendency of LDA to overbind. One of the most important quantities for calculations involving defects is the positioning of defect energy levels, and also accurate estimates of the defect wavefunctions. DFT is in principle the wrong choice for either of these,

256

D.A. Drabold and T.A. Abtew

Fig. 2. GeSe2 density of electron states: comparison of experiment and theory (Gaussian-broadened Kohn–Sham eigenvalues) [43]. The Fermi-level is at zero for both curves

since it is formally only a ground-state theory, and also because only the charge density (that is, sum of the squares of the occupied Kohn–Sham orbitals) is formally meaningful within the derivation of the Kohn–Sham equations. However, it is clear that this viewpoint is unduly restrictive, and the density of Kohn–Sham eigenvalues is useful for comparing to the single-particle density of states as measured for example in photoemission (see Fig. 2 taken from [43]). The Kohn–Sham DOS systematically underestimates the optical gap (often by a factor of 2). Curiously, local basis function calculations with a limited (single-zeta) basis tend to give approximately the correct gap as the incompleteness of the basis tends to exaggerate the gap thus partly (and fortuitously) ﬁxing the underestimate intrinsic to the Kohn–Sham calculation. A proper job of describing these states requires methods beyond DFT. In this book, there are two relevant Chapters, that of Scheﬄer on the so-called “GW” methods (these provide self-energy corrections to DFT) and also the Chapter of Needs on quantum Monte Carlo. GW calculations of Blase and coworkers have shown that the Kohn–Sham orbitals tend to exaggerate the extent of localized states in crystalline systems; one should expect a similar eﬀect for amorphous systems. Unfortunately, the understanding of these points is only empirical at present.

Defects in Amorphous Semiconductors: Amorphous Silicon

257

4.4 The Electron–Lattice Interaction We have recently shown in some generality that localized electron states associated with defects exhibit a large coupling to the lattice [27]. Thus, for localized electronic eigenstates, deformations of the lattice in the vicinity of the localized state lead to signiﬁcant changes in the associated electronic eigenvalue. This eﬀect is easily tracked with ﬁrst-principles MD (in such an approach, Kohn–Sham eigenvectors are computed for each instantaneous ionic conﬁguration). Beside this empirical observation, it is possible to do a simple analysis of the vibration-induced changes in electron energies using the Hellmann–Feynman theorem [44] and exploiting the locality of the states to show that the electron–lattice coupling is roughly proportional to the localization (as gauged by the inverse participation ratio). Previous thermal simulations with Bohn–Oppenheimer dynamics have indicated that there exists a large electron–phonon coupling for the localized states in the band-tails and in the optical gap [45]. Earlier works on chalcogenide glasses by Cobb and Drabold [46] have emphasized a strong correlation between the thermal ﬂuctuations as gauged by root mean square (RMS) variation in the LDA eigenvalues and wavefunction localization of a gap or tail state (measured by the inverse participation ratio (2). Drabold and Fedders [24] have shown that localized eigenvectors may ﬂuctuate dramatically even at room temperature. Recently, Li and Drabold relaxed the adiabatic (Born–Oppenheimer) approximation to track the time development of electron packets scattered by lattice vibrations [45]. We have recently shown for localized electron states, that the electron–phonon coupling Ξn (ω) (coupling electron n and phonon ω) approximately satisﬁes: Ξn2 (ω) ∼ In × f (ω) ,

(4)

where f (ω) does not depend upon n, In is the IPR of electron state n. It is also the case that the thermally induced variance of electronic eigenvalue n, δλ2n ∝ In . It is remarkable that a simple correlation exists between a static property of the network (the IPR) and a dynamical feature of the system, the thermally induced ﬂuctuation in the Kohn–Sham energy eigenvalues. These predictions are easily veriﬁed from thermal simulation as reported elsewhere. The main assumption in obtaining this connection is that the electron states under study are localized. Beside the thermally induced changes in electronic energies, there are also signiﬁcant variations in the structure of the Kohn– Sham eigenstates, another consequence of the large electron–phonon coupling for localized states.

258

D.A. Drabold and T.A. Abtew

5 Defects in Amorphous Silicon Geometry/Topology Probably the most heavily studied amorphous semiconductor is Si. In its unhydrogenated form, the material is not electronically useful, as there are too many defect states in the optical gap. On the other hand, hydrogenated a-Si (a-Si:H) can be grown in a variety of ways, and can be prepared with defect concentrations of order 10−16 , which is small enough to enable many electronic applications [47]. Of critical importance for these applications, it is possible to dope a-Si:H n(p) type with P(B) donors (acceptors). The doping eﬃciency of the material is very low (meaning that large amounts – of order 1 % impurity is needed to move the Fermi level signiﬁcantly). In a-Si, diﬀraction measurements show that these materials are very tetrahedral (typically more than 99.9 % of atoms are four-coordinated) and have bond angles distributed around the tetrahedral angle (typically with a FWHM of order 10 degrees). The key defect is the threefold-coordinated Si atom, the sp3 dangling-bond, which is known on the basis of experiment and simulation to produce a midgap state. Such states are directly observable in electron spin resonance (ESR) measurements [48, 49]. Several papers have speculated on the importance of ﬁvefold ﬂoating bonds [50], but their signiﬁcance is still uncertain, and it appears that such defects would not produce midgap states, but rather states near the conduction-band edge. Depending upon the details of the local bonding environment, the levels associated with these states could move slightly from their ideal locations. Such conﬁgurations are popular in MD simulations of a-Si (quenches from the liquid). It is unclear, however, whether this implies the existence of ﬂoating bonds in a-Si:H or if there is an overemphasis on higher-coordinated sites because the liquid is roughly 6-fold coordinated. Defects play many roles in a-Si:H, and one of the most interesting defect-dependent properties is associated with light-induced metastability, the “Staebler–Wronski” eﬀect [51], which is usually interpreted as lightinduced creation of defect centers (probably dangling-bonds). A remarkable collection of experiments and models have been undertaken to understand this eﬀect that is obviously important for photovoltaic applications, but for thin-ﬁlm device applications (like thin-ﬁlm transistors) as well [52–65]. This eﬀect is addressed in the Chapter of Simdayankin and Elliott. Level of Approximations: A Cautionary Tale We have undertaken a systematic study of the level of calculation needed to faithfully represent the electron states, total energies and forces in a-Si within the density-functional LDA approximations. This work was performed with the powerful local basis code SIESTA [66]. This calculation was carried out for a-Si:H, but we expect that many of the conclusions should at least be

Defects in Amorphous Semiconductors: Amorphous Silicon

259

considered when applying density-functional techniques to other amorphous or glassy materials. In fact studies analogous to ours for silicon should be implemented for more complex amorphous materials. For a unique “one-stop reference” to methodological issues for density-functional methods, see the book of Martin [67]. In a nutshell, a proper calculation of defect states and geometry, especially in amorphous materials, is diﬃcult. Every approximation needs to be checked and optimized. Depending upon the type of question being asked more or less sophisticated approximations may be required. We divide the discussion into several categories: (1) Pseudopotentials: One of the most important and fortunately reliable approximations used in electronic-structure calculations is the pseudopotential. This is a means to separate the atomic core and valence regions, and enables the use of only valence electrons in the calculation of the Kohn–Sham orbitals. Even for a relatively light atom like Si, this allows a calculation involving 4 electrons per atom rather than 14. When one reﬂects that mere diagonalization of the Hamiltonian scales as the cube of the number of electrons, the payoﬀ is clear. After many years of work, the lore of pseudopotentials is fairly mature, though one must test a new potential carefully before using it widely. (2) Basis Set: The most obvious approximation in any large-scale DF calculation is the use of a ﬁnite basis set to represent a set of continuous functions (the Kohn–Sham orbitals and the charge density). In a planewave calculation, it is easy to check for completeness, as the only “knob” is the plane-wave cutoﬀ (or number of reciprocal lattice vectors). Care is needed with plane-wave calculations as defect states can be quite spatially compact and therefore diﬃcult to approximate without a large collection of reciprocal lattice vectors. For local basis codes, ab initio or empirical, completeness is a delicate question. Most current codes use basis orbitals much in the spirit of the linear combination of atomic orbitals (LCAO) method of chemistry, with s, p, d, f states. The minimal basis is deﬁned to be a set of atom-centered functions that is just adequate to represent the occupied atomic orbitals on that atom. The minimal basis has very limited variational freedom. The ﬁrst improvement on the minimal basis is introducing two functions with the symmetry of the original single-zeta (SZ) functions. Quantum chemists call this a “double-zeta” (DZ) basis. A suitably selected doublezeta basis can reproduce expansion and contraction in local bonding. The zeta proliferation can continue, though it is uncommon to proceed beyond triple-zeta in practical calculations. After adequately ﬁlling out the basis orbitals with the symmetries of the states for the ground-state atom, one proceeds to the next shell of states that are unoccupied in the atomic ground-state. These are called polarization functions (so named because the loss of symmetry caused by application of a (polarizing)

260

D.A. Drabold and T.A. Abtew

electric ﬁeld distorts the ground-state functions into the next angular momentum shell). In a-Si:H we ﬁnd that the choice of basis aﬀects virtually everything. The localization of the Kohn–Sham states depends dramatically on the basis. As one might guess, the less complete basis sets tend to overestimate the localization of the Kohn–Sham eigenvectors (as there are fewer channels for these states to admix into). What was surprising is that the degree of localization, measured by IPR for a well-isolated dangling-bond defect, varies by a factor of two between a single-zeta (four orbitals per site) and a double-zeta polarized (DZP) (thirteen orbitals per site) basis. Similar eﬀects are seen for defects in crystals. Since the single-particle density matrix, the total energy and interatomic forces depend upon the Kohn– Sham eigenvectors, it is to be expected that defect geometry, vibrational frequencies and dynamical properties are all inﬂuenced by the choice of basis. (3) Spin Polarization: Fedders and coworkers [68] have shown that, in order to correlate the degree of localization from dangling-bond states with ESR experiments, it is not enough to look at the wavefunctions, but to the net spin polarization near the danglin-bond. The reason is that the spin density includes contributions from electronic states other than the localized defect wavefunction, which contribute to make the spin polarization more localized than the speciﬁc localized state wavefunction. In order to conﬁrm this result (obtained by Fedders et al. on cells of aSi:H) in our structural models, we performed calculations allowing for spin polarization in our frozen lattice models, using the DZP basis set. We were not able to ﬁnd a spin-polarized solution for any of the amorphous cells. The reason is the existence of two interacting dangling-bonds, which favors the formation of a spin singlet with two electrons paired. In order to force the appearance of a spin moment in our models, we introduce an unpaired spin by removing a single electron from the system. We ﬁnd a contribution of almost 50 % to net spin by the central dangling-bond and its neighbors (the central atom alone contributing 38 %). However, the Mulliken charge contribution to the wavefunction of the corresponding localized state from the defect site is only 0.29e. The hydrogen-terminated dangling-bond sites also contribute about 10 % of the net spin. The remainder is somewhat distributed uniformly at the other sites. For well-isolated dangling-bonds in a-Si, about 54 % of the net spin-localization sits on the dangling-bond and its nearest neighbors, in reasonable agreement with the experiment [49, 69]. The conclusion is that, for a dangling-bond defect state, there is a large diﬀerence between spin localization and wavefunction localization. The degree of spin localization is greater than that of the wavefunction localization at the dangling-bond site. To our knowledge, no experimental methods exist for measuring the extent of wavefunction localization on the dangling-bond orbital as opposed to spin.

Defects in Amorphous Semiconductors: Amorphous Silicon

261

(4) Gradient-Corrected Density-Functional: This has been inadequately studied, although there is no reason to expect large changes in structure with the use of gradient corrections. Typically, bond lengths may change modestly and cohesive energies improve when compared to experiment. Generally one expects gradient corrections to at least partly repair the tendency of LDA to overbind. (5) Brillouin-Zone Sampling: Many current calculations of defects are carried out with a cell that is then periodically repeated to eliminate surface eﬀects. In particular, this construction clearly yields a crystal with a unit cell with typically several hundred or more atoms (such a number is necessary to meaningfully sample the disorder characteristic of the material). Thus, the use of periodic (Born–Von-Karman) boundary conditions really amounts to consideration of a crystal with a large unit cell. Thus, there is a new (and completely artiﬁcial) band-structure (k dispersion) associated with the construction, a Brillouin-zone, etc. It is of course true that as the cell gets larger, the bands become ﬂatter, thus reducing the signiﬁcance of the periodicity. For computational convenience, total energies and forces are inevitably computed at the center (k = 0) of the Brillouin-zone, though in principle these quantities involve quadrature over the ﬁrst Brillouin-zone. However, if results for total energies and especially forces depend upon k in any signiﬁcant way, then it is doubtful that the cell was selected to be large enough in the ﬁrst place. For delicate energetics (an all too familiar state of aﬀairs for defects), it is particularly important to test that the cell is big enough. In our experience a few hundred atoms in a cubic cell is adequate. Defect Identiﬁcation From simulation studies, one ﬁnds the expected point defects of coordination type (threefold dangling-bonds and ﬁvefold atoms ﬂoating bonds), and also strain defects (nominally four-coordinated structures with large deviations in the bond angles). The dangling-bond defect produces electronic states near the middle of the gap, and ﬂoating bonds near the conduction edge. Strain defects are associated with the valence- and conduction-band tails. Defect Dynamics and Diﬀusion An important, but underappreciated aspect of defects in amorphous semiconductors, is their dynamics. In hydrogenated amorphous silicon, the motion of defects and the motion of hydrogen (which are evidently related) are correlated with some of the most important physical properties of the amorphous matrix, such as the light-induced degradation of the material (Staebler–Wronski eﬀect) [51, 70]. The expectation is that H motion consists of small oscillations in a particular potential well associated with a given local environment with rare escape events until the diﬀusing particle falls into

262

D.A. Drabold and T.A. Abtew

Fig. 3. Trajectory for two diﬀerent hydrogen atoms, showing diﬀusion and trapping between silicon bond centers in a 223 atom model of hydrogenated amorphous silicon. The simulation time is 10.0 ps and the temperature is 300 K. ‘Light-oﬀ’ implies that the dynamics are in the electronic ground state

another trap. The time between such rare events depends upon the height of the barrier separating the two metastable conﬁgurations. Sophisticated methods exist for determining diﬀusion pathways and events, particularly the activation-relaxation technique (ART) of Barkema and Mousseau [71]. In a remarkable paper, these authors applied ART with a simple potential to directly compute the atomic “moves” in a model of a-Si. For large barriers and very rare events, there is no substitute for a study of “ART” type. For smaller barriers, we have seen that it is possible to extract interesting short-time diﬀusive dynamics directly from MD simulation. In simulations of Ag dynamics in chalcogenide glass hosts, we found that it was not diﬃcult to track the motion of the Ag atoms from simulations of order 50 ps. The existence of trapping centers, and even some information about trap geometry, and temperature-dependent residence times was obtained [72]. In a-Si:H, we have found that an analogous computation produces new insight into the motion of both Si and H atoms. Using a small cell (61 Si and 10 H atoms) with two dangling-bonds and no other defects, we employed SIESTA with high-level approximations (a double-zeta polarized basis) to monitor atomic motion. On the time-scale of 1 ps we have shown the trajectory of one of the H atoms in Fig. 3 [73]. Representative of the majority of H atoms in the cell, this particular trajectory shows the diﬀusion of the hydrogen atom, including trapping. While the H atoms are diﬀusing in the cell it is followed by breaking old bonds and forming new bonds. We have plotted the time evolution of undercoordinated and ﬂoating bonds formed as a consequence of hydrogen diﬀusion in Fig. 4 [73].

Defects in Amorphous Semiconductors: Amorphous Silicon

263

Fig. 4. (a) Total number of undercoordinated atoms and (b) Total number of overcoordinated atoms in our simulation at T = 300 K. The total time for the graph is 1.0 ps

Fig. 5. Time evolution of coordination for a few selected atoms (H-69, H-65, Si-24, and Si-51) at room temperature T = 300 K. (a) time evolution of atoms, Si-24 which is far from the diﬀusing H with coordination 4 and H-69. (b) time evolution of selected atoms: Si-51, which is close to the diﬀusing H, and H-65

In our simulation we have observed rearrangements of the atoms while the hydrogen atoms are diﬀusing in the cell. The diﬀusion of H causes formation and breaking of bonds. We have also observed the formation of metastable states that trap the mobile hydrogen atoms. The mechanisms for the formation of these structures follow breaking of H atoms from the Si–H bonds and followed by diﬀusion in the cell. These mobile H atoms then collide with another Si+DB structure and form a bond. These processes continue until two hydrogens form a bond to a single Si atom or to two nearby Si atoms to form a metastable conformation. In Fig. 5, [73] we have shown the time evolution of the coordination for selected atoms. Figure 5a shows the stable coordination of a Si atom (Si-24) that is fully coordinated since there is no

264

D.A. Drabold and T.A. Abtew

diﬀusing atom in its vicinity and of H-69 that has an average coordination of 1. However, the Si atom (Si-51) and H-65, which are shown in Fig. 5b, shows change in the coordination as a function of time. This change in the coordination becomes more stable (1 for H and 4 for Si) after the formation of a metastable conﬁguration. Our results suggest that atoms that are reasonably far from the diﬀusing hydrogen have an average coordination of 4 for Si and 1 for H. However, the coordination of the atoms, for instance Si-51, in the direction of the diﬀusing H atoms changes with time. This suggests that while the H atoms are diﬀusing in the cell there is breaking and formation of bonds. Other researchers have emphasized the signiﬁcance of defect and H motion. In particular, Street [74] has pioneered a phenomenological approach to the long-time dynamics with the defect-pool model. Our work on extremely short timescales should ultimately be smoothly connected to the inferred long-time defect dynamics from the defect-equilibria models. While we are very far from this goal at present, it is possible to imagine impacts of both approaches on each other within a few years. Ideally, the short-time simulations could provide ab-initio input into the energetics of the dynamics, and even information about residence times for various defects. Acknowledgements It is a pleasure to thank a number of collaborators for their contributions to the work reported here: R. Atta-Fynn, P. Biswas, J. Dong, S. R. Elliott, P. A. Fedders, H. Jain, J. Li, J. Ludlam, N. Mousseau, P. Ordej´ on, S. N. Taraskin and X. Zhang. We acknowledge the support of the National Science Foundation under NSF-DMR 0600073, 0605890 and the Army Research Oﬃce under MURI W911NF-06-2-0026.

References [1] C. R. A. Catlow (Ed.): Defects and Disorder in Crystalline and Amorphous Solids, vol. 418 (Kluwer, Netherlands 1994) 245 [2] J. D. Joannopoulos, G. Lucovsky (Eds.): The Physics of Hydrogenated Amorphous Silicon II, vol. 56 (Springer, Berlin, Heidelberg 1984) 245 [3] M. Stutzmann, D. K. Biegelsen, R. A. Street: Phy. Rev. B 35, 5666 (1987) 245 [4] E. T. Jaynes: Probability Theory: The Logic of Science (Cambridge University Press, Cambridge 2003) 246 [5] R. Car, M. Parrinello: Phy. Rev. Lett. 60, 204 (1988) 247 [6] O. Gereben, L. Pusztai: Phys. Rev. B 50, 14136 (1994) 247 [7] J. K. Walters, R. J. Newport: Phys. Rev. B 53, 2405 (1996) 247 [8] R. L. McGreevy: J. Phys.: Condens. Matter 13, R877 (2001) 247, 254 [9] F. Wooten, K. Winer, D. Weaire: Phy. Rev. Lett. 54, 1392 (1985) 247, 254

Defects in Amorphous Semiconductors: Amorphous Silicon

265

[10] B. R. Djordjevic, M. F. Thorpe, F. Wooten: Phys. Rev. B 52, 5685 (1995) 247, 252 [11] G. T. Barkema, N. Mousseau: Phy. Rev. B 62, 4985 (2000) 247, 254 [12] R. L. C. Vink, G. T. Barkema: Phys. Rev. B 67, 245201 (2003) 247 [13] M. F. Thorpe: J. Non-Cryst. Solids 57, 355 (1983) 247 [14] A. E. Carlsson: Solid State Physics, Advances in Research and Applications, vol. 43 (Academic, New York 1990) p. 1 247 [15] F. Ercolessi, J. B. Adams: Europhys. Lett. 26, 583 (1994) 247 [16] A. Nakano, L. Bi, R. K. Kalia, P. Vashishta: Phys. Rev. B 49, 9441 (1994) 247 [17] J. J. Ludlam, S. N. Taraskin, S. R. Elliott, D. A. Drabold: J. Phys.: Condens. Matter 17, L321 (2005) 247, 248, 251 [18] S. Aljishi, L. Ley, J. D. Cohen: Phys. Rev. Lett. 64, 2811 (1990) 247 [19] D. A. Drabold, P. A. Fedders, S. Klemm, O. F. Sankey: Phys. Rev. Lett. 67, 2179 (1991) 247, 249 [20] S. R. Elliott: Physics of Amorphous Materials, 2nd ed. (Longman Scientiﬁc, London; New York 1990) 248, 253 [21] R. Zallen: The Physics of Amorphous Solids (Wiley-Interscience, New York 1998) 248 [22] J. Dong, D. A. Drabold: Phys. Rev. Lett. 80, 1928 (1998) 250, 251, 252 [23] P. A. Fedders, D. A. Drabold, S. Nakhmanson: Phys. Rev. B 58, 15624 (1998) 250 [24] D. A. Drabold, P. A. Fedders: Phys. Rev. B 60, R721 (1999) 250, 257 [25] D. A. Drabold: J. Non-Cryst. Solids 269, 211 (2000) 250 [26] R. A. Street, J. Kakalios, T. M. Hayes: Phys. Rev. B 34, 3030 (1986) 250 [27] R. Atta-Fynn, P. Biswas, P. Ordej´ on, D. A. Drabold: Phys. Rev. B 69, 085207 (2004) 252, 257 [28] N. Szabo, N. S. Ostlund: Modern Quantum Chemistry (Dover, New York 1996) 252 [29] S. N. Taraskin, D. A. Drabold, S. R. Elliott: Phys. Rev. Lett. 88, 196405 (2002) 252 [30] X. Zhang, D. A. Drabold: Phys. Rev. Lett. 83, 5042 (1999) 253 [31] M. Cobb, D. A. Drabold, R. L. Cappelletti: Phys. Rev. B 54, 12162 (1996) 253 [32] C. Massobrio, A. Pasquarello, R. Car: Phys. Rev. Lett. 80, 2342 (1998) 253 [33] I. Petri, P. S. Salmon, H. E. Fischer: Phys. Rev. Lett. 84, 2413 (2000) 253 [34] X. Zhang, D. A. Drabold: Phys. Rev. B 62, 15 695 (2000) 253 [35] P. S. Salmon, I. Petri, J. Phys.: Condens. Matter 15, S1509 (2003) 253 [36] D. A. Drabold, J. Li, D. Tafen: J. Phys.: Condens. Matter 15, S1529 (2003) 253 [37] D. N. Tafen, D. A. Drabold: Phys. Rev. B 68, 165208 (2003) 253 [38] M. F. Thorpe, D. J. Jacobs, B. R. Djordjevic: The structure and rigidity of network glasses, in P. Boolchand (Ed.): Insulating and Semiconducting Glasses (World Scientiﬁc, Singapore 2000) p. 95 253 [39] W. H. Zachariasen: J. Am. Chem. Soc. 54, 3841 (1932) 253 [40] R. Kaplow, T. A. Rowe, B. L. Averbach: Phys. Rev. 168, 1068 (1968) 254 [41] A. P. Sutton, M. W. Finnis, D. G. Pettifor, Y. Ohta: J. Phys. C: Solid State Phys. 21, 35 (1988) 255 [42] N. Bernstein, E. Kaxiras: Phys. Rev. B 56, 10488 (1997) 255

266 [43] [44] [45] [46] [47] [48] [49] [50] [51] [52] [53] [54] [55] [56] [57] [58] [59] [60] [61] [62] [63] [64] [65] [66] [67] [68] [69] [70] [71] [72] [73] [74]

D.A. Drabold and T.A. Abtew P. Biswas, D. N. Tafen, D. A. Drabold: Phys. Rev. B 71, 054204 (2005) 256 R. P. Feynman: Phys. Rev. 56, 340 (1939) 257 J. Li, D. A. Drabold: Phys. Rev. B 68, 033103 (2003) 257 M. Cobb, D. A. Drabold: Phys. Rev. B 56, 3054 (1997) 257 J. D. Joannopoulos, G. Lucovsky (Eds.): The Physics of Hydrogenated Amorphous Silicon I, vol. 55 (Springer, Berlin, Heidelberg 1984) 258 R. A. Street, D. K. Biegelsen, J. C. Knights: Phys. Rev. B 24, 969 (1981) 258 D. K. Biegelsen, M. Stutzmann: Phys. Rev. B 33, 3006 (1986) 258, 260 S. T. Pantelides: Phys. Rev. Lett. 57, 2979 (1986) 258 D. L. Staebler, C. R. Wronski: Appl. Phys. Lett. 31, 292 (1977) 258, 261 H. Fritzsche: Annu. Rev. Mater. Res. 31, 47 (2001) 258 T. Su, P. C. Taylor, G. Ganguly, D. E. Carlson: Phys. Rev. Lett. 89, 015502 (2002) 258 S. B. Zhang, W. B. Jackson, D. J. Chadi: Phys. Rev. Lett. 65, 2575 (1990) 258 D. J. Chadi: Appl. Phys. Lett. 83, 3710 (2003) 258 M. Stutzmann, W. B. Jackson, C. C. Tsai: Phys. Rev. B 32, 23 (1985) 258 R. Biswas, I. Kwon, C. M. Soukoulis: Phys. Rev. B 44, 3403 (1991) 258 S. Zafar, E. A. Schiﬀ: Phys. Rev. B 40, 5235 (1989) 258 S. Zafar, E. A. Schiﬀ: Phys. Rev. Lett. 66, 1493 (1991) 258 S. Zafar, E. A. Schiﬀ: J. Non-Cryst. Solids 138, 323 (1991) 258 H. M. Branz: Phys. Rev. B 59, 5498 (1999) 258 R. Biswas, Y.-P. Li: Phys. Rev. Lett. 82, 2512 (1999) 258 N. Kopidakis, E. A. Schiﬀ: J. Non-Cryst. Solids 269, 415 (2000) 258 S. B. Zhang, H. M. Branz: Phys. Rev. Lett. 87, 105503 (2001) 258 T. A. Abtew, D. A. Drabold, P. C. Taylor: Appl. Phys. Lett. 86, 241916 (2005) 258 J. M. Soler, E. Artacho, J. D. Gale, A. Garcia, J. Junquera, P. Ordej´ on, D. Sanch´ez-Portal: J. Phys.: Condens. Matter 14, 2745 (2002) 258 R. M. Martin: Electronic Structure: Basic Theory and Practical Methods (Cambridge University Press, Cambridge 2004) 259 P. A. Fedders, D. A. Drabold, P. Ordej´ on, G. Fabricius, E. Artacho, D. Sanchez-Portal, J. Soler: Phys. Rev. B 60, 10594 (1999) 260 T. Umeda, S. Yamasaki, J. Isoya, et al.: Phys. Rev. B 59, 4849 (1999) 260 T. A. Abtew, D. A. Drabold: J. Phys.: Condens. Matter 18, L1 (2006) 261 N. Mousseau, G. T. Barkema: Phys. Rev. E 57, 2419 (1998) 262 D. N. Tafen, D. A. Drabold, M. Mitkova: phys. stat. sol. (b) 242, R55 (2005) 262 T. A. Abtew, D. A. Drabold: Phys. Rev. B 74, 085201 (2006) 262, 263 R. A. Street: Hydrogenated Amorphous Silicon (Cambridge University Press, Cambridge 1991) 264

Index a-Si, 245–247, 249, 250, 252–254, 258, 260, 262

ab-initio, 247, 249, 250, 259, 264 acceptor, 258

Defects in Amorphous Semiconductors: Amorphous Silicon adiabatic, 257 amorphous, 245–256, 258–261 Anderson, 251 band edge, 247, 249, 258 band-structure, 250, 261 band-tail, 247, 249, 250, 257, 261 bandwidth, 246 basis set, 255, 259, 260 Bloch, 250 bond order, 249 Born–Oppenheimer, 257 Born–von-Karman, 261 Bragg, 246 Brillouin-zone, 261 chalcogen, 253 chalcogenide, 247, 252, 257, 262 cohesive energy, 261 concentration, 250, 258 conduction, 247, 261 conduction-band, 251, 258, 261 conformation, 250, 255, 263 coordination, 247–249, 255, 261, 263, 264 core, 259 Coulomb, 252 coupling, 257 crystal momentum, 247, 250 cutoﬀ, 249, 259 dangling-bond, 249, 253, 255, 258, 260–262 decay, 246, 247, 251, 252 delocalized, 251, 252 density matrix, 249, 252, 260 density of states, 247, 256 DFT, 255, 256 diamond, 253 diﬀusion, 262, 263 disorder, 245, 247–251, 254, 261 dispersion, 261 distortion, 246, 250, 252 donor, 258 doping, 258 double-zeta, 259, 260, 262 DZ, 259 DZP, 260 eigenstates, 249, 251, 257

267

eigenvalues, 249, 256, 257 eigenvectors, 247, 251, 257, 260 electron, 252, 253, 259, 260 electron spin resonance, 258 electron states, 247, 250, 257, 258 electron–phonon, 257 empirical, 247, 250, 255–257, 259 energetics, 252, 254, 255, 261, 264 energy level, 255 entropy, 246, 251 equilibrium, 249, 250 ESR, 253, 258, 260 Fermi level, 247, 249, 253, 255, 258 ﬁrst-principles, 247, 250, 257 ﬂoating bond, 258, 261, 262 ﬂuctuation, 249, 257 force, 247, 255, 258, 260, 261 fourfold, 252–254 Fourier, 246 gap, 249, 252 Ge, 247, 253, 254 general gradient approximation, 255 glass, 246, 253, 254, 257, 262 grain, 253 ground-state, 256, 259, 260 GW, 256 Hamiltonian, 247, 250–253, 255, 259 Hellmann–Feynman, 257 hopping, 251 Hubbard, 253 hybrid, 247, 255 hydrogen, 260–264 impurity, 258 IPR, 251, 252, 257, 260 Kohn–Sham, 249, 255–257, 259, 260 LDA, 255, 257, 258, 261 liquid, 254, 258 localization, 249, 251, 257, 260 melting, 254 metastablity, 258 Metropolis, 254 midgap, 251, 258

268

D.A. Drabold and T.A. Abtew

minimal basis, 259 mobility, 251 molecular-dynamics, 247, 254, 255 Mulliken, 251, 260 neutron diﬀraction, 246 optical, 247, 249, 252, 256–258 pair-correlation function, 246, 249, 254 periodic, 250, 261 periodic boundary conditions, 261 periodicity, 261 phonon, 257 photoemission, 247, 256 photovoltaic, 246, 258 plane-wave, 259 point defect, 261 polarization, 255, 259, 260 potential, 247, 250, 252, 254, 255, 259, 261, 262 pseudopotential, 259

self-energy, 256 Si, 245–247, 249, 250, 252–254, 258–260, 262–264 SIESTA, 258, 262 silicon, 245, 259, 261 spin, 252, 253, 255, 258, 260 Staebler–Wronski, 258, 261 strain, 247, 261 stress, 247 structure factor, 246 surface, 250, 261 symmetry, 259 temperature, 247, 249, 250, 257, 262 tetrahedral, 252–254, 258 thermal disorder, 247, 249 thermal equilibrium, 249 tight-binding, 247, 250, 255 total energy, 247, 252, 260 trajectory, 262 transition, 246, 251, 254 transport, 245

quantum Monte Carlo, 256 variational, 259 radial-distribution function, 246, 254 real space, 246 relaxation, 253, 255, 262 resonance, 258 reversible, 246, 250

Wannier, 252 wavelength, 246 X-ray, 246

Light Induced Eﬀects in Amorphous and Glassy Solids S. I. Simdyankin and S. R. Elliott Department of Chemistry, University of Cambridge, Lensﬁeld Road, Cambridge CB2 1EW, United Kingdom {sis24,sre1}@cam.ac.uk Abstract. In this Chapter, we discuss how exposure to light can aﬀect the properties of disordered materials and review our recent computational studies of these phenomena. Familiarity with the preceding contribution by Drabold and Abtew is beneﬁcial for understanding this Chapter.

1 Photoinduced Metastability in Amorphous Solids: An Experimental Survey 1.1 Introduction Electromagnetic (EM) radiation can interact with amorphous solids in a number of ways, depending on the wavelength of the radiation. EM radiation can be either absorbed or scattered by a solid. In the resonant process of absorption, the photon energy must match a transition energy between two quantum states in the material, e.g., for atomic vibrations corresponding to infrared (IR) wavelengths, or electronic transitions from valence to conduction band across a bandgap in a semiconductor, corresponding to visible/near ultraviolet (UV) wavelengths (depending on the magnitude of the bandgap energy, Eg ). Scattering of EM radiation may be elastic, or inelastic when energy is exchanged between a photon and quantum states of a solid. Examples include X-ray scattering (diﬀraction) from the electrons in atoms, Raman (inelastic light) scattering from atomic vibrations (e.g. molecular-like modes) and Brillouin (inelastic light) scattering from acoustic phonon-like vibrational excitations. The photon–solid interaction can be interrogated in terms of either the ultimate state of the photon (as in the above examples), or in terms of changes in the internal state of the solid. In the latter case, it is often changes in the electronic degrees of freedom that are probed: for the case of most amorphous semiconductors with bandgaps in the range 1 eV < Eg < 3 eV, this involves near-IR or visible-light excitation (although for more ionic oxides, e.g., vitreous (v-)SiO2 with Eg ≈ 10 eV, UV-light excitation is required). Electrons optically excited into the conduction band (CB), or holes excited into the valence band (VB), can be probed, for example, by their enhanced electrical transport (photoconductivity) or by their radiative recombination D. A. Drabold, S. K. Estreicher (Eds.): Theory of Defects in Semiconductors, Topics Appl. Physics 104, 269–286 (2007) © Springer-Verlag Berlin Heidelberg 2007

270

S. I. Simdyankin and S. R. Elliott

(photoluminescence or ﬂuorescence). At suﬃciently high light intensities, the light–solid interaction can become nonlinear, this optical nonlinearity permitting many new phenomena, such as second-harmonic generation, three- and four-wave mixing, to occur. Electronic excitation of structural coordination defects, e.g., dangling bonds, can be probed by electron spin (paramagnetic) resonance (ES(P)R). The optically induced phenomena outlined above can be exhibited by all kinds of semiconducting/insulating solid, whether crystalline or amorphous. However, certain features unique to the amorphous state in general, and to certain types of amorphous materials in particular, mean that some photoinduced phenomena are special to amorphous semiconducting materials, particularly those that are metastable, i.e., which remain after cessation of irradiation. One general characteristic of amorphous semiconductors of relevance in this connection is the occurrence of disorder-induced spatial localization of electronic states in the band-tail states extending into the gap between the VB and CB [1]. The presence of continuous bands of localized states in these tail states, in the energy interval between the “mobility” edges in the VB and CB, marking the transition point between localized and delocalized (extended) electron states [2], as well as localized states deep in the bandgap arising from coordination defects [1], can have a profound inﬂuence on the nature of the photon–solid interaction. These localized states have an enhanced electron–lattice interaction (see the preceding Chapter by Drabold and Abtew ), meaning that optical excitation of such electronic states can have a disproportionate eﬀect on the surrounding atomic structure. Secondly, the radiative-recombination lifetime for an optically created electron–hole pair trapped in localized tail states can be very considerably longer than when the photoexcited carriers are in extended states (as is always the case for crystals), thereby allowing possible nonradiative channels to become signiﬁcant (e.g., involving atomic-structural reconﬁguration). Other relevant aspects are more materials speciﬁc. Optically induced metastability associated with structural reorganization is likely to be more prevalent in those materials in which (some) atoms have a low degree of nearest-neighbor connectivity (e.g., being twofold coordinated, rather than fourfold coordinated), thereby imparting a considerable degree of local structural ﬂexibility. In addition, structural reorganization following optically induced electronic excitation is more probable if the (VB) electronic states involved correspond to easily broken weak bonds. One class of materials satisfying the above constraints consists of chalcogenide glasses, namely alloys of the Gp-VI chalcogen elements (S, Se, Te) with other (metalloid) elements, e.g., B, Ga, P, As, Sb, Si, Ge, etc. These materials are “lone-pair” semiconductors in which (if the chalcogen content is suﬃciently high) the top of the VB comprises chalcogen p-π lone-pair (LP) states [3]. Interatomic, “nonbonding” (Van der Waals-like) interactions involving such LP states are appreciably weaker than for normal covalent

Light Induced Eﬀects in Amorphous and Glassy Solids

271

bonds (those states lying deeper in the VB). Since the ground-state electronic conﬁguration of chalcogen atoms is s2 p4 , the occurrence of nonbonding LP electron states means that each chalcogen atom is ideally twofold coordinated by covalent bonds to its nearest neighbors. Thus, chalcogenide glasses, having a combination of localized electronic tail states, low atomic coordination and weak bonds associated with optically accessible states at the top of the VB, are ideal candidates for exhibiting photoinduced eﬀects. 1.2 Photoinduced Eﬀects in Chalcogenide Glasses Amorphous chalcogenide materials exhibit a plethora of photoinduced phenomena. Such changes can be variously dynamic (i.e., present only whilst a material is illuminated) or metastable (i.e., the eﬀects remain after cessation of illumination). Furthermore, the changes may be either scalar or vectoral in nature (respectively, independent or dependent on either the polarization state, or the propagation direction, of the inducing light). Finally, metastable changes may be irreversible, or reversible with respect to thermal or optical annealing. Examples of dynamic eﬀects are the afore-mentioned phenomena of photoluminescence and photoconductivity [1] and optical nonlinearity [4], which are common to all materials. (Chalcogenide glasses generally exhibit extremely large optical nonlinearities because of the highly electronically polarizable nature of chalcogen atoms present [4].) However, a (scalar) dynamic eﬀect, which is characteristic of chalcogenide glasses, is photoinduced ﬂuidity, wherein the viscosity of a glass (e.g. As2 S3 ) decreases on illumination with subbandgap light or, in other words, light can cause viscous relaxation in a stressed glass [5, 6]. An example of a vectoral dynamic photoeﬀect in chalcogenide glasses is the optomechanical eﬀect [7, 8], wherein linearly polarized light incident on a chalcogenide-coated clamped microcantilever causes it to displace upwards or downwards, depending on whether the polarization axis is, respectively, parallel or perpendicular to the cantilever axis, as a result of anisotropic photoinduced strains introduced into the chalcogenide–cantilever bimorph. Metastable photoinduced changes are perhaps the most interesting (and applicable) of the eﬀects observed in chalcogenide glasses. One such is photodarkening (or bleaching), wherein the optical absorption edge of the material shifts to lower energies (hence the material gets darker at a given wavelength), or to higher energies (bleaching), on illumination with (sub-) bandgap light. For reviews, see [9, 10]. Arsenic-based materials with higher sulfur contents and germanium sulﬁde materials seem to favor photobleaching, for reasons that are not clear at present. Irreversible shifts of the optical absorption edge occur in virgin (as-evaporated) thin ﬁlms of amorphous chalcogenides containing structurally unstable molecular fragments from the vapor phase [11] that are particularly vulnerable to photoinduced (or thermal) change. Reversible photodarkening is observed in bulk glasses and well-annealed thin

272

S. I. Simdyankin and S. R. Elliott

ﬁlms: optical illumination causes a redshift of the absorption edge, whilst subsequent thermal annealing to the glass-transition temperature, Tg , erases the eﬀect [9, 10]. Photodarkening (bleaching) appears to be associated with photoinduced structural changes, such microscopic changes being manifested as macroscopic volume changes. Photocontraction is particularly prevalent in virgin obliquely deposited thin ﬁlms of amorphous chalcogenides having a columnarlike microstructure [12], but photoexpansion is commonly associated with photodarkening in chalcogenide bulk glasses or thin ﬁlms [9, 10]. Giant photoexpansion (up to 5 % expansion) occurs for subbandgap illumination [13]. Another metastable photoinduced structural change exhibited by chalcogenide materials is photoinduced crystallization and amorphization, as used in rewriteable “phase-change” CDs and DVDs [14, 15]. The amorphization process there is believed to result from a photoinduced melting and subsequent very rapid quenching of the material to the glassy state. However, illumination of certain crystalline chalcogenide materials (e.g., As50 Se50 ) can also cause athermal photoamorphization [16]. Light can also cause “chemical” changes in chalcogenide glasses. For example, overlayers of certain metals (notably silver) diﬀuse into the undoped bulk glass on illumination [17, 18]. On the other hand, Ag-containing chalcogenide glasses, rich in Ag, exhibit the opposite eﬀect, namely photoinduced surface deposition, wherein the metal exsolves from the glassy matrix on illumination [19, 20]. A particularly interesting metastable vectoral photoinduced eﬀect exhibited by chalcogenide glasses is photoinduced optical anisotropy (POA), ﬁrst observed in [21], and manifested in absorption, reﬂection (i.e., refractive index) and scattering (for a review, see [10, 22]). Illumination of an initially optically isotropic glass by linearly polarized light causes the material to become dichroic and birefringent. In the case of well-annealed thin ﬁlms and bulk glasses, the eﬀect is completely reversible optically (i.e., the induced optical axis is fully rotated when the light-polarization vector is rotated), and the POA can be annealed out thermally (but at a lower temperature than is the case for scalar photodarkening) or optically (using unpolarized or circularly polarized light).

2 Theoretical Studies of Photoinduced Excitations in Amorphous Materials From the above very brief review, it is apparent that amorphous chalcogenide materials exhibit a wide range of interesting photoinduced phenomena. Although the experimental phenomenology is, for the most part, well developed, a proper theoretical understanding is still lacking. Until very recently, theoretical models have been conﬁned to “hand-waving” models [9,10], involving simple notions of chemical bonding and the eﬀects of light (e.g., bond breaking and defect formation). However, the predictive, and even descriptive, power

Light Induced Eﬀects in Amorphous and Glassy Solids

273

of such approaches is very limited, and for a microscopic (atomic-level) understanding of photoinduced phenomena in amorphous chalcogenides, proper quantum-mechanical calculations need to be performed. Obviously, this is an extremely challenging task, and two essentially opposing methods for making progress in this regard, using diﬀerent approximations, can be employed. The ﬁrst employs all-electron quantum-chemical calculations on small clusters (a few tens) of atoms, in which the optimized electronic and atomic conﬁgurations and energies are found for the ground and electronically excited states (see, e.g. [23–26]). This favors accuracy over dynamics. The other method, (discussed in the Chapter by Drabold and Abtew ), namely ab-initio molecular-dynamics (MD) simulations, takes a converse approach: atomic dynamics are followed at the expense of accuracy. More detail will be given in the following, but the advantages and disadvantages of these two approaches can be summarized as follows. Quantum-chemical methods can only deal with very small clusters (particularly for excited-state calculations) and only initial (ground-state) and ﬁnal (excited-state) conﬁgurations can be studied, not the intermediate dynamics, but the energetics are the most accurate. Ab-initio MD, on the other hand, provides full information about atomic dynamics, but only over very short timescales (typically a few picoseconds) and for relatively few atoms (typically less than a hundred). In order to make the calculations involved tractable, numerous more-or-less severe approximations need to be invoked (e.g., the local-density approximation (LDA) in density-functional theory (DFT)), which make certain results imprecise (e.g., underestimation of the bandgap). Moreover, the Kohn–Sham (KS) orbitals resulting from DFT are ground-state quantities and hence formally inadmissible for a consideration of excited-state behavior. Nevertheless, use of these theoretical methods has provided very useful atomistic information of help in understanding photoinduced phenomena in chalcogenide glasses. Some justiﬁcation for using both occupied and virtual KS orbitals for qualitative, and sometimes partially quantitative, analysis of electronic structure is provided by comparing the shape and symmetry properties, as well as the energy order, of these orbitals with those obtained by wavefunction-based (e.g., at the Hartree–Fock level of theory [27]) and GW [28] calculations. There is a very strong similarity between GW and LDA states, and often identical DFT and GW quasiparticle wavefunctions are assumed in practical calculations [29]. 2.1 Application of the Density-Functional-Based Tight-Binding Method to the Case of Amorphous As2 S3 One approximate ab-initio-based MD scheme that has proved very useful in understanding the electronic behavior of chalcogenide glasses is the densityfunctional-based tight-binding (DFTB) method developed by Frauenheim and coworkers. Although this is reported in [30–32], since this approach is not described elsewhere in this book, we give here a brief description of this

274

S. I. Simdyankin and S. R. Elliott

method and review our recent results on the canonical chalcogenide glass a-As2 S3 obtained by using the DFTB method [33–35]. Although the DFTB method is semiempirical, it allows one to improve upon the standard tight-binding description of interatomic interactions by including a DFT-based self-consistent second order in charge ﬂuctuation (SCC) correction to the total energy [31]. The ﬂexibility in choosing the desired accuracy while computing the interatomic forces brings about the possibility to perform much faster calculations when high precision is not required, and reﬁne the result if needed. As described in [36], the SCC-DFTB model is derived from densityfunctional theory (DFT) by a second-order expansion of the DFT total energy functional with respect to the charge-density ﬂuctuations δn = δn(r ) around a given reference density n0 = n0 (r ): E=

occ i

ˆ 0 |ψi ψi |H

δ 2 Exc 1 + (1) δn δn |r − r | δn δn n0 n0 n0 1 + E − [n ] − Vxc [n0 ]n0 + Eii , xc 0 2 |r − r | ˆ0 = where dr and dr are expressed by and , respectively. Here, H ˆ 0 ] is the eﬀective Kohn–Sham Hamiltonian evaluated at the reference H[n density and the ψi are Kohn–Sham orbitals. Exc and Vxc are the exchangecorrelation energy and potential, respectively, and Eii is the core–core repulsion energy. To derive the total energy of the SCC-DFTB method, the energy contributions in (1) are further subjected to the following approximations: 1. The ˆ 0 |ψi are represented in a basis of conHamiltonian matrix elements ψi |H ﬁned, pseudoatomic orbitals φµ , ψi = ciµ φµ . (2) 1 + 2

µ

To determine the basis functions φµ , the atomic DFT problem is solved by adding an additional harmonic potential ( rr0 )2 to conﬁne the basis func0 , are tions [30]. The Hamiltonian matrix elements in this LCAO basis, Hµν 0 then calculated as follows. The diagonal elements Hµµ are taken to be the 0 are calculated in a atomic eigenvalues and the nondiagonal elements Hµν two-center approximation: 0 Hµν = φµ |Tˆ + veﬀ [n0α + n0β ]|φν µα, νβ,

(3)

which are tabulated, together with the overlap matrix elements Sµν with respect to the interatomic distance Rαβ . veﬀ is the eﬀective Kohn–Sham potential and n0α are the densities of the neutral atoms α.

Light Induced Eﬀects in Amorphous and Glassy Solids

275

2. The charge-density ﬂuctuations δn are written as a superposition of atomic contributions δnα , δn = δnα , (4) α

which are approximated by the charge ﬂuctuations at the atoms α, ∆qα = qα − qα0 . qα0 is the number of electrons of the neutral atom α and the qα are determined from a Mulliken-charge analysis. The second derivative of the total energy in (1) is approximated by a function γαβ , whose functional form for α = β is determined analytically from the Coulomb interaction of two spherical charge distributions, located at Rα and Rβ . For α = β, it represents the electron–electron self-interaction on atom α. 3. The remaining terms in (1), Eii and the energy contributions, which depend on n0 only, are collected in a single energy contribution Erep . Erep is then approximated as a sum of short-range repulsive potentials, U [Rαβ ], (5) Erep = α=β

which depend on the interatomic distances Rαβ . With these deﬁnitions and approximations, the SCC-DFTB total energy ﬁnally reads: Etot =

iµν

0 ciµ ciν Hµν +

1 γαβ ∆qα ∆qβ + Erep . 2

(6)

αβ

Applying the variational principle to the energy functional (6), one obtains the corresponding Kohn–Sham equations: cνi (Hµν − i Sµν ) = 0, ∀ µ, i (7) ν

1 Hµν = φµ |H0 |φν + Sµν (γαζ + γβζ )∆qζ , 2

(8)

ζ

which have to be solved iteratively for the wavefunction expansion coeﬃcients ciµ , since the Hamiltonian matrix elements depend on the ciµ due to the Mulliken charges. Analytic ﬁrst derivatives for the calculation of interatomic forces are readily obtained, and second derivatives of the energy with respect to atomic positions are calculated numerically. The repulsive pair potentials U [Rαβ ] are constructed by subtracting the DFT total energy from the SCC-DFTB electronic energy (ﬁrst two terms on the right-hand side of (6)) with respect to the bond distance Rαβ for a small set of suitable reference systems. To summarize, in order to determine the appropriate parameters for a new element, the following steps have to be taken. First, DFT calculations have to be performed for the neutral atom to determine the LCAO basis functions φµ

276

S. I. Simdyankin and S. R. Elliott

and the reference densities n0α . Here the conﬁnement radius can, in principle, be chosen to be diﬀerent for the density (r0n ) and each type of atomic orbital (r0s,p,d ). The value of r0 is usually taken to be the same for s- and p-functions. In a minimal basis, this yields a total number of two adjustable parameters for elements in the ﬁrst and second rows, while there are three if d-functions are included. After this, the diﬀerent matrix elements can be calculated and the pair potentials U [Rαβ ] are obtained as stated above for every combination of the new element with the ones already parameterized. The single-particle KS occupied, ψi , and unoccupied, ψj , orbitals and the corresponding KS excitation energies ωij = j − i are sometimes used for qualitative analysis of electronic excitations. Although the KS excitation energies can be considered as an approximation to true excitation energies ωI [37] (see also end of the introduction to Sect. 2), the correction terms to this approximation can be very signiﬁcant in many cases. Modeling electronic excitations by varying the occupation of the KS orbitals results in mixed quantum states with undeﬁned contributions from singlet and triplet states. We have performed modeling of electronic excitations at the level of KS orbitals and energies and have attempted to validate the results by using more exact methods. One such method is based on time-dependent densityfunctional response theory (TD-DFRT) [38, 39], where the true excitation energies are found by solving the following eigenvalue problem: √ √ 2 I I [ωij δik δjl δστ + 2 ωij Kijσ,klτ ωkl ]Fijσ = ωI2 Fklτ . (9) ijσ

Here σ and τ are spin indices. The indices i, k correspond to occupied, and j, l to unoccupied, KS orbitals, respectively. The coupling matrix K is deﬁned as (see [40] for a more detailed description of the method): 1 δ 2 Exc + Kijσ,klτ = ψi (r)ψj (r) (10) ψk (r )ψl (r ), |r − r | δnσ δnτ where we use a notation consistent with that in (2). Our structural models of a-As2 S3 were obtained by a “melt-and-quench” procedure [35] similar to the one described in the preceding Chapter by Drabold and Abtew. The structural quality of models can be assessed by examining the radial-distribution function (RDF) and the structure factor (see Fig. 1). Apart from general good agreement with experimental data, an interesting feature revealed by Fig. 1a is the shape of the ﬁrst peak of the RDF. The shoulders on both sides of this peak indicate the presence of homopolar (As–As or S–S) bonds in the material. Such bonds (chemical defects), as well as coordination (or topological) defects, are easily detectable in computer models. An example of a conﬁguration featuring an As–As bond is shown in Fig. 2. Special signiﬁcance can be attributed to the presence of ﬁve-membered rings in models with an appreciable concentration of homopolar bonds (models with all-heteropolar bonds contain only an even number of

Light Induced Eﬀects in Amorphous and Glassy Solids

277

Fig. 1. (a) Pair-correlation functions for a 200-atom model of a-As2 S3 and the neutron-diﬀraction experiment [41]. (b) Reduced structure factors (interference functions) for the same model and experiment

atoms in all rings). When such rings share some of the bonds, the resulting local structure is close to that of cage-like molecules (e.g., As4 S4 ), as found in the vapor phase and in some chalcogenide molecular crystals. Figure 2a shows two such bond-sharing rings. Upon breaking the two bonds connecting the rings to the rest of the network, the distance between the two freed arsenic atoms (connected by a dashed line in Fig. 2a) could be reduced, thus producing another As–As homopolar bond and this group of atoms would then form an As4 S4 molecule (shown in Fig. 2b). Evidence of the presence of such molecules in bulk Asx S1−x glasses from Raman-scattering experiments

278

S. I. Simdyankin and S. R. Elliott

Fig. 2. (a) Fragment of a 200-atom model of a-As2 S3 : two bond-sharing ﬁvemembered rings and the two AsS3 groups connected to this structure. The dangling bonds show where the displayed conﬁguration connects to the rest of the amorphous network. The dashed line connects two As atoms, which, if brought nearer together, would close up to form an As4 S4 molecule shown in panel (b). The shading of the As atoms (all with three neighbors) is darker than that of the S atoms (all with two neighbors)

has recently been reported in [42]. Our result shows that the As4 S4 fragments may not only form discrete cage-like molecules but also may be embedded into the amorphous network. We veriﬁed that the vibrational signatures of the As4 S4 fragment from models 1 and 2 are similar to those from an isolated As4 S4 molecule, apart from a few very symmetric modes of the latter. The observed tendency for formation of quasimolecular structural groups suggests that amorphous chalcogenides can be viewed as nanostructured materials. Localization of the electronic states near the optical bandgap edges is of great interest for studies of photoinduced phenomena. The inverse participation ratios (IPR, deﬁned in the Chapter by Drabold and Abtew ) for a model of a-As2 S3 are shown in Fig. 3. The general picture is that, at the top of the valence band, the eigenstates are predominantly localized at what can be called sulfur-rich regions, where several sulfur atoms are closer than about 3.45 ˚ A, i.e., their interatomic distances are on the low-r side of the second peak in g(r) shown in Fig. 1a or some of these atoms form homopolar S–S bonds. For instance, most of the HOMO (highest occupied molecular orbital) level in this model is localized at two sulfur atoms separated by 3.42 ˚ A and which are part of the molecule-like fragment depicted in Fig. 2a. By inspecting the projected (local) IPRs in Fig. 3b at the optical gap edges, it is seen that the IPRs are greatest for the S atoms. It appears that the localization at the top of the valence band is facilitated by the proximity of the lone-pair p orbitals in the sulfur-rich regions. This observation is consistent with a result for a-GeS2 [44].

Light Induced Eﬀects in Amorphous and Glassy Solids

279

Fig. 3. Local and total electronic density of states (a) and inverse participation ratios (b) for a 200-atom model of a-As2 S3 . The Fermi energy is at the energy origin. The experimental data in (a) are obtained from [43]

At the bottom of the conduction band, the states tend to localize at various anomalous local conﬁgurations, such as four-membered rings, S–S homopolar bonds (some of these bonds are in ﬁve-membered rings) and valencealternation pairs (coordination defects). For example, the LUMO (lowest unoccupied molecular orbital) state for the structure depicted in Figs. 5a,b is localized on an overcoordinated S atom (with three bonded neighbors). We found that a basis set of s, p and d Slater-type orbitals for all atoms is an essential prerequisite for the observation of overcoordinated defects [36,45].

280

S. I. Simdyankin and S. R. Elliott

(a)

(b)

(c)

Fig. 4. Planar trigonal, [S3 ]+ (marked by the letter “A”), and “seesaw”, [As4 ]− (marked by letter “E”), conﬁgurations in (a) a fragment of a 60-atom model of a-As2 S3 (the dangling bonds show where the displayed conﬁguration connects to the rest (not shown) of the network) and, (b) and (c), charged isolated clusters (the dangling bonds are terminated with hydrogen atoms). The shading of the atoms is the same as in Fig. 2

It is possible to analyze individual contributions of orbitals of each type to the total EDOS and IPR, and these contributions are shown in Fig. 3. As mentioned above, in the context of photoinduced metastability, a great deal of signiﬁcance is attributed to the presence of topological and/or chemical defects [9]. It is therefore imperative to create models both with and without such defects in a theoretical investigation that attempts to be conclusive. Defect-free models can be produced by “surgical” manipulations. For example, atoms with undesired coordination can be removed from the model, and, in order to eliminate chemical defects, one can iteratively apply the following algorithm. First, a sulfur atom is inserted in the middle of each As–As homopolar bond. Second, each S–S bond is replaced by a single sulfur atom located at its midpoint so that each local As–S–S–As conﬁguration is turned into As–S–As. Third, the distance between each newly introduced S atom and its two nearest arsenic atoms in the newly created As–S–As units is reduced in order to increase the bonding character of the As–S bonds stretched by the above manipulation. Fourth, the modiﬁed conﬁguration is relaxed in an MD run. We have found that only a few iterations can be suﬃcient in order to obtain models with all-heteropolar (As–S) bonds.

Light Induced Eﬀects in Amorphous and Glassy Solids

(a)

(c)

(b)

(d)

281

Fig. 5. An As4 S10 H8 cluster containing both defect centers [As4 ]− (marked by letter “A”) and [S3 ]+ (“B”). The shading of the atoms is the same as in Fig. 2. The black solid lines signify elongated bonds. (a) Optimized ground-state geometry. Bond lengths are (˚ A): AC = 3.00, AD = 2.32, and BE = 2.4. (b) Isosurfaces corresponding to the value of 0.025 of electron density in the HOMO (darker red surface) and LUMO (lighter cyan surface) states for the structure shown in (a). (c) Optimized geometry in the ﬁrst singlet excited state. Bond lengths are (˚ A): AC = 2.43, AD = 2.44, and BE = 2.82. (d) Same as (b), but for the structure shown in (c)

Elimination of the defects in our models removes some electronic states in the optical bandgap. As a result, the bandgap broadens, which can be viewed as an artiﬁcial bleaching of the material. The states at the band edges, however, are still localized due to disorder. It is possible that exposure to light may lead to bond breaking and defect creation even in such “all-heteropolar” models. Indeed, As–S bond elongation/breaking has been observed in allheteropolar clusters [23,24] and cage-like molecules (unpublished). Such bond breaking under irradiation can lead to the creation of self-trapped excitons (STEs), i.e., oppositely charged defect pairs, as shown in [29] for silicon dioxide where, following Si–O bond breaking, the hole is localized at the oxygen defect center and the electron at the silicon defect center. In analogy with the case of SiO2 , it is possible that positively charged chalcogen defects and negatively charged nonchalcogen defects are introduced in amorphous chalcogenides by a similar mechanism. In the As–S system, such STEs can possibly lead to creation of the [As4 ]− –[S3 ]+ defect pairs described below.

282

S. I. Simdyankin and S. R. Elliott

These defects, as well as those that are always present in real materials and “as-prepared” models, may mediate local structural rearrangements upon photon absorption. Creation of additional states at optical bandgap edges (photodarkening) of a-As2 S3 exposed to light has long been attributed to the generation by illumination of defects in excess of the thermal equilibrium concentration [9], but the exact mechanism of defect creation and the nature of the defects are still enigmatic. Possible candidate defect types, notably valence-alternation pairs, have been proposed over the years [9]. Normally, such defect pairs contain singly coordinated chalcogen atoms having distinct spectroscopic signatures [46]. Experimentally, the concentration of these defects is estimated to be rather small [47], i.e., 1017 cm−3 , compared with the atomic density of about 2 × 1025 cm−3 , in order quantitatively to account for the observed magnitude of the photoinduced eﬀects. In our simulations, in addition to the charged coordination defects previously proposed to exist in chalcogenide glasses, a novel defect pair, [As4 ]− – [S3 ]+ (see Fig. 4), consisting of a fourfold coordinated arsenic site in a “seesaw” conﬁguration and a threefold coordinated sulfur site in a near-planar trigonal conﬁguration, was found in several models [33]. Such defect pairs are unusual in two ways. First, there is an excess of negative charge in the vicinity of the normally electropositive pnictogen (As) atoms and, second, there are no undercoordinated atoms with dangling bonds in these local conﬁgurations. The latter peculiarity may be why such defect pairs have not yet been identiﬁed experimentally. These defect pairs, however, are consistent with the STEs described above. Although electronic excitations, where one electron is promoted from HOMO to LUMO Kohn–Sham states [48], are not especially realistic, we simulate such excitations in order qualitatively to assess defect stability with respect to (optically induced) electronic excitations. In some models, [S3 ]+ – − + S− 1 defect pairs are converted into [As4 ] –[S3 ] pairs as a result of the electronic excitation. The presence of these defect pairs introduces additional localized states at the optical bandgap edges with energies quantitatively consistent with the phenomenon of photodarkening [34]. − A possible mechanism of conversion of [S3 ]+ –S− 1 defect pairs into [As4 ] – + [S3 ] pairs is illustrated in Fig. 5, which shows an As4 S10 H8 cluster containing an [S3 ]+ –S− 1 pair in the ground state. Geometry optimization in the ﬁrst singlet excited state within the linear-response approximation to time-dependent (TD) density-functional theory (which gives a much better description of excited states compared with HOMO-to-LUMO electron excitations [40]) leads to a redistribution of electron density, so that the singly coordinated S atoms become attached to a normally coordinated As atom, thus forming an [As4 ]− defect. At the same time, the [S3 ]+ defect breaks up (we observed that bond breaking/elongation in all our models generally occurs at the groups of atoms where the LUMO is localized, indicating the expected antibonding character of LUMO states.). Perhaps in bulk materials similar rearangements can lead to the creation of an [S3 ]+ center at a diﬀer-

Light Induced Eﬀects in Amorphous and Glassy Solids

283

ent location, which is suggested by the observation that, in our simulations of photoexcitations in supercell models, the [S3 ]+ centers after excitation are not necessarily located at the same S atom as before the excitation.

References [1] S. R. Elliott: Physics of Amorphous Materials, 2nd ed. (Longman Scientiﬁc and Technical, London 1990) 270, 271 [2] J. J. Ludlam, S. N. Taraskin, S. R. Elliott: J. Phys. Condens. Matter 17, L321 (2005) 270 [3] S. R. Elliott: Chalcogenide glasses, in J. Zarzycki (Ed.): Materials Science and Technology, vol. 9 (VCH, Weinheim 1991) p. 375 270 [4] A. Zakery, S. R. Elliott: J. Non-Cryst. Solids 330, 1 (2003) 271 [5] H. Hisakuni, K. Tanaka: Science 270, 974 (1995) 271 [6] S. N. Yannopoulos: Photo-plastic eﬀects in chalcogenide glasses: Raman scattering studies., in A. V. Kolobov (Ed.): Photo-Induced Metastability in Amorphous Semiconductors (Wiley-VCH, Weinheim 2003) p. 119 271 [7] P. Krecmer, A. M. Moulin, T. Rayment, R. J. Stephenson, T. Rayment, M. E. Welland, S. R. Elliott: Science 277, 1799 (1997) 271 [8] M. Stuchlik, S. R. Elliott: Proc. IEE A: Science, Measurement and Technology 151, 131 (2004) 271 [9] A. V. Kolobov (Ed.): Photo-Induced Metastability in Amorphous Semiconductors (Wiley-VCH, Weinheim 2003) 271, 272, 280, 282 [10] K. Shimakawa, A. Kolobov, S. R. Elliott: Adv. Phys. 44, 475 (1995) 271, 272 [11] S. A. Solin, G. V. Papatheodorou: Phys. Rev. B 15, 2084 (1977) 271 [12] S. Rajagopalan, K. S. Harshavardhan, L. K. Malhotra, K. L. Chopra: J. NonCryst. Solids 50, 29 (1982) 272 [13] H. Hisakuni, K. Tanaka: Appl. Phys. Lett. 65, 2925 (1994) 272 [14] S. R. Ovshinsky: Phys. Rev. Lett. 21, 1450 (1968) 272 [15] T. Ohta, S. R. Ovshinsky: Phase-change optical storage media., in A. V. Kolobov (Ed.): Photo-Induced Metastability in Amorphous Semiconductors (Wiley-VCH, Weinheim 2003) p. 310 272 [16] S. R. Elliott, A. V. Kolobov: J. Non-Cryst. Solids 128, 216 (1991) 272 [17] A. Kolobov, S. R. Elliott: Adv. Phys. 40, 625 (1991) 272 [18] T. Wagner, M. Frumar: Optically-induced diﬀusion and dissolution in metals in amorphous chalcogenides., in A. V. Kolobov (Ed.): Photo-Induced Metastability in Amorphous Semiconductors (Wiley-VCH, Weinheim 2003) p. 160 272 [19] S. Maruno, T. Kawaguchi: J. Appl. Phys. 46, 5312 (1975) 272 [20] T. Kawaguchi: Photo-induced deposition of silver particles on amorphous semiconductors., in A. V. Kolobov (Ed.): Photo-Induced Metastability in Amorphous Semiconductors (Wiley-VCH, Weinheim 2003) p. 182 272 [21] V. G. Zhdanov, V. K. Malinovskii: Sov. Tech. Phys. Lett. 3, 943 (1977) 272 [22] V. M. Lyubin, M. L. Klebanov: Photo-induced anisotropy in chalcogenide glassy semiconductors., in A. V. Kolobov (Ed.): Photo-Induced Metastability in Amorphous Semiconductors (Wiley-VCH, Weinheim 2003) p. 91 272 [23] T. Uchino, D. C. Clary, S. R. Elliott: Phys. Rev. Lett. 85, 3305 (2000) 273, 281

284

S. I. Simdyankin and S. R. Elliott

[24] T. Uchino, D. C. Clary, S. R. Elliott: Phys. Rev. B 65, 174204 (2002) 273, 281 [25] T. Uchino, S. R. Elliott: Phys. Rev. B 67, 174201 (2003) 273 [26] T. Mowrer, G. Lucovsky, L. S. Sremaniak, J. L. Whitten: J. Non-Cryst. Solids 338, 543 (2004) 273 [27] R. Stowasser, R. Hoﬀman: J. Am. Chem. Soc. 121, 3414 (1999) 273 [28] M. S. Hybertsen, S. G. Louie: Phys. Rev. B 34, 5390 (1986) 273 [29] S. Ismail-Beigi, S. G. Louie: Phys. Rev. Lett. 95, 156401 (2005) 273, 281 [30] D. Porezag, T. Frauenheim, T. K¨ ohler, G. Seifert, R. Kaschner: Phys. Rev. B 51, 12947 (1995) 273, 274 [31] M. Elstner, D. Porezag, G. Jungnickel, J. Elstner, M. Haugk, T. Frauenheim, S. Suhai, G. Seifert: Phys. Rev. B 58, 7260 (1998) 273, 274 [32] T. Frauenheim, G. Seifert, M. Elstner, T. Niehaus, C. K¨ ohler, M. Amkreutz, M. Sternberg, Z. Hajnal, A. Di Carlo, S. Suhai: J. Phys. Condens. Matter 14, 3015 (2002) 273 [33] S. I. Simdyankin, T. A. Niehaus, G. Natarajan, T. Frauenheim, S. R. Elliott: Phys. Rev. Lett. 94, 086401 (2005) 274, 282 [34] S. I. Simdyankin, M. Elstner, T. A. Niehaus, T. Frauenheim, S. R. Elliott: Phys. Rev. B 72, 020202 (2005) 274, 282 [35] S. I. Simdyankin, S. R. Elliott, Z. Hajnal, T. A. Niehaus, T. Frauenheim: Phys. Rev. B 69, 144202 (2004) 274, 276 [36] T. A. Niehaus, M. Elstner, T. Frauenheim, S. Suhai: J. Mol. Struct. THEOCHEM 541, 185 (2001) 274, 279 [37] A. G¨ orling: Phys. Rev. A 54, 3912 (1996) 276 [38] M. E. Casida: Recent Advances in Density Functional Methods, Part I (World Scientiﬁc, Singapore 1995) p. 155 276 [39] M. E. Casida: Developments and applications of modern density functional theory, in J. M. Seminario (Ed.): Theoretical and Computational Chemistry, vol. 4 (Elsevier Science, Amsterdam 1996) p. 391 276 [40] T. A. Niehaus, S. Suhai, F. Della Sala, P. Lugli, M. Elstner, G. Seifert, T. Frauenheim: Phys. Rev. B 63, 085108 (2001) 276, 282 [41] J. H. Lee, A. C. Hannon, S. R. Elliott: eprint: cond-mat/0402587 277 [42] D. G. Georgiev, P. Boolchand, K. A. Jackson: Philos. Mag. 83, 2941 (2003) 278 [43] S. G. Bishop, N. J. Shevchik: Phys. Rev. B 12, 1567 (1975) 279 [44] S. Blaineau, P. Jund: Phys. Rev. B 70, 184210 (2004) 278 [45] S. I. Simdyankin, S. R. Elliott, T. A. Niehaus, T. Frauenheim: Eﬀect of defects in amorphous chalcogenides on the atomic structure and localisation of electronic eigenstates, in P. Vincenzini, A. Lami, F. Zerbetto (Eds.): Computational Modeling and Simulation of Materials III, vol. A (Techna Group s.r.l., Faenza 2004) p. 149 279 [46] M. Kastner, D. Adler, H. Fritzsche: Phys. Rev. Lett. 37, 1504 (1976) 282 [47] A. Feltz: Amorphous Inorganic Materials and Glasses (VCH, Weinheim 1993) p. 203 282 [48] X. Zhang, D. A. Drabold: Phys. Rev. Lett. 83, 5042 (1999) 282

Light Induced Eﬀects in Amorphous and Glassy Solids

Index a-As2 S3 , 274, 276, 278, 282 ab-initio, 273 absorption, 269, 271, 272, 282 algorithm, 280 all-electron, 273 amorphous, 269–273, 278, 281 anisotropy, 271, 272 annealing, 271, 272 As4 S4 , 277, 278 band edge, 281 basis set, 279 Brillouin scattering, 269 bulk, 271, 272, 277, 282 canonical, 274 chalcogen, 270, 271, 281, 282 chalcogenide, 270–274, 277, 278, 281, 282 cluster, 273, 279, 281, 282 concentration, 276, 282 conduction band, 269, 270, 279 coordination, 270, 271, 276, 279, 280, 282 core, 274 Coulomb, 275 coupling, 276 covalent, 270, 271

excitation, 269, 270, 276, 282, 283 excited state, 273, 282 exciton, 281 ﬂuctuation, 274, 275 force, 274, 275 fourfold, 270, 282 gap, 269 Ge, 270 germanium, 271 glass, 270–274, 277, 282 ground state, 271, 273, 282 GW, 273 Hamiltonian, 274, 275 Hartree–Fock, 273 hole, 269, 270, 281 HOMO, 278, 282 IPR, 280 irreversible, 271 Kohn–Sham, 273–275, 282 LCAO, 275 LDA, 273 localization, 270, 278 LUMO, 279, 282

dangling bond, 270, 282 delocalized, 270 density-functional theory, 273, 274, 276 DFT, 273–275 DFTB, 273–275 disorder, 269, 270, 281

metastability, 280 minimal basis, 276 molecular-dynamics, 273 Mulliken, 275

eigenstates, 278, 284 eigenvalues, 274 electromagnetic radiation, 269 electron, 269, 275 electron spin resonance, 270 electron states, 270 embedded, 278 energetics, 273 equilibrium, 282 exchange, 269 exchange-correlation, 274

phonon, 269 photoconductivity, 269, 271 photodarkening, 271, 272, 282 photoexpansion, 272 photoluminescence, 270, 271 pnictogen, 282 polarization, 271, 272 potential, 274–276 pseudoatom, 274

optical, 270–272, 278, 282 oxygen, 281

quasiparticle, 273

285

286

S. I. Simdyankin and S. R. Elliott

radial-distribution function, 276 radiative, 269, 270 Raman, 269, 277 recombination, 269, 270 relaxation, 271 repulsive, 275 resonance, 270 resonant, 269 reversible, 271, 272 scalar, 271, 272 scattering, 269, 272, 277 self-interaction, 275 self-trapped, 281 semiempirical, 274 Si, 269, 270, 281 silicon, 281 Slater, 279 spin, 270, 276 strain, 271 stress, 271 supercell, 283

surface, 272 symmetric, 278 symmetry, 273 temperature, 272 thermal equilibrium, 282 tight binding, 273, 274 time-dependent density-functional theory (TDDFT), 282 total energy, 274, 275 transition, 269, 270, 272 transport, 269 trigonal, 282 valence band, 269–271, 278 Van der Waals, 270 variational, 275 vectoral, 271, 272 wavelength, 269, 271 X-ray, 269

Index

Γ point, 34, 52, 58 a-As2 S3 , 274, 276, 278, 282 a-Si, 131, 245–247, 249, 250, 252–254, 258, 260, 262 ab initio, 16, 21, 101 ab-initio, 215, 216, 233, 247, 249, 250, 259, 264, 273 absorption, 13, 44, 49, 95, 157, 230, 231, 269, 271, 272, 282 acceptor, 34, 40, 57, 59–61, 69, 71, 81, 83, 84, 86–88, 90, 258 adatom, 230 adiabatic, 119–122, 124, 130, 134, 257 AIMPRO, 16, 58, 59, 71, 72, 75, 76, 80, 81, 84, 87, 88 algorithm, 43, 44, 61, 74, 143–145, 147, 203, 204, 217, 229, 280 alignment, 35, 49, 50, 55, 57, 176, 177, 234–236 all-electron, 41, 55, 72, 76, 273 amorphous, 1, 2, 6, 9, 22, 23, 43, 130, 131, 230, 245–256, 258–261, 269–273, 278, 281 Anderson, 251 anharmonic, 48, 102, 118, 125, 126, 128, 196, 222 anion vacancy, 166, 179–182, 184–187 anisotropy, 271, 272 annealing, 12, 13, 60, 95, 194, 233, 235, 236, 271, 272 antisite, 12, 168 As4 S4 , 277, 278 asymmetric, 99, 101, 166, 179, 180, 182, 183, 185, 186, 201 atomic-sphere approximation, 35, 55 autocorrelation function, 48, 224 backﬂow, 146, 147

background charge, 35, 53, 58, 70, 159 band bending, 166 band edge, 12, 13, 30, 35, 40, 49, 50, 55, 59, 84, 173, 178, 184, 247, 249, 258, 281 band structure, 14, 15, 38, 41, 58, 79, 166, 167, 169, 170, 172–177, 216, 235 band-structure, 250, 261 band-tail, 247, 249, 250, 257, 261 bandwidth, 34, 246 basis set, 14–16, 21, 22, 32, 34, 39, 42, 43, 47, 58, 61, 69, 71–80, 96, 103, 130, 158, 214, 255, 259, 260, 279 Berendsen, 132, 221 Bethe–Salpeter, 39 Bloch, 14, 71, 250 Bohr, 13 Boltzmann, 104, 116, 219, 224 bond order, 216, 222, 223, 228–230, 249 bond-centered, 14, 16, 21, 74, 99–101, 106, 195 bond-order potential, 214, 215, 217, 223, 227, 230, 235 Born–Oppenheimer, 17, 42, 43, 214, 257 Born–von-Karman, 15, 261 boron, 81, 84, 87, 107, 108, 206 Bragg, 246 Brillouin scattering, 269 Brillouin zone, 2, 34, 35, 38, 51, 52, 84, 89, 103, 176–178, 181, 182 Brillouin-zone, 148, 261 bulk, 36, 41, 47, 49, 50, 52, 55, 58, 74, 76, 79, 84, 86, 90, 127, 165, 171, 173, 174, 176–178, 187, 198, 271, 272, 277, 282 bulk modulus, 76, 77, 79, 223

288

Index

canonical, 43, 116–118, 120–122, 220, 224, 225, 274 Car, 21, 130 carbide, 195 carbon, 80, 87, 132–134 chalcogen, 84, 85, 90, 253, 270, 271, 281, 282 chalcogenide, 247, 252, 257, 262, 270–274, 277, 278, 281, 282 charge delocalization, 39 charge state, 14, 30, 34, 38, 46–50, 52, 55, 57, 60, 70, 80, 81, 86, 107, 167, 170, 179, 180, 182–187 charge-transition level, 165–167, 170, 171, 184–187 charge-transition state, 169, 172, 173, 184, 186, 187 charged defect, 15, 35, 53–58, 158 chemical potential, 36, 49–51, 55, 80, 184, 220 classical, 19, 20, 53, 54, 101, 106, 116, 120, 160, 195, 196, 198–200, 202–204, 206, 208, 210, 213, 216, 218, 219 Clausius–Clapeyron, 123–125, 132–134 cleavage, 168, 176 cluster, 2, 12, 15, 16, 32, 33, 35, 36, 55, 56, 70, 71, 80, 81, 84, 87, 89, 127, 142, 147, 194, 223, 273, 279, 281, 282 cohesive energy, 150, 218, 223, 227, 228, 261 complex, 12, 15, 81, 84–86, 100, 105–110, 194, 195 concentration, 11, 13, 36, 48, 69, 104–110, 115, 125, 127, 153, 154, 159, 220, 250, 258, 276, 282 concerted exchange, 154–156 conduction, 247, 261 conduction band, 12, 35, 38, 40, 50, 51, 79, 105, 176, 178, 184, 269, 270, 279 conduction-band, 251, 258, 261 conductivity, 11, 30, 49, 69 conﬁgurational entropy, 106, 108–110, 131 conformation, 81, 250, 255, 263 conjugate gradient, 75, 107, 214, 215 conservative, 217, 220

coordination, 142, 179, 247–249, 255, 261, 263, 264, 270, 271, 276, 279, 280, 282 core, 16, 35, 37, 41, 55, 58, 59, 71, 72, 96, 195, 259, 274 core radius, 41 core-valence, 37, 41 core-valence interaction, 167, 174, 182 correlation, 15, 16, 19, 31, 32, 37–40, 61, 86, 97, 130, 142, 145–147, 150, 156, 157, 167, 169–172, 177, 180, 224 Coulomb, 18, 35, 39, 40, 46, 53, 55, 56, 58, 146, 148, 217, 218, 222, 252, 275 coupling, 46, 48, 56, 58, 118, 157, 205, 225, 231, 236, 257, 276 covalent, 15, 35, 78, 129, 196, 199, 208, 223, 234, 270, 271 crack, 128, 196, 197, 208, 225 crystal momentum, 247, 250 cusp, 146 cutoﬀ, 36, 42, 58, 97, 217, 228, 249, 259 cyclic cluster, 15 Czochralski, 14 dangling bond, 15, 56, 176, 177, 179, 196, 199, 270, 282 dangling-bond, 157, 249, 253, 255, 258, 260–262 decay, 18, 57, 96, 98, 100, 101, 144, 172, 195, 217, 246, 247, 251, 252 deep level, 12, 13, 34, 61, 69, 71, 84, 87 deep-level transient spectroscopy, 13, 29 defect band, 34, 35 defect engineering, 11 defect state, 180 degeneracy, 30, 44–46, 56, 228 delocalization, 39 delocalized, 13, 39, 52, 54, 251, 252, 270 density matrix, 228, 229, 249, 252, 260 density of states, 17, 18, 37, 48, 95, 102, 103, 166, 227, 229, 247, 256 density-functional theory, 16, 19–22, 30, 31, 44, 60, 69, 96, 105, 128, 130, 142, 165–168, 170–172, 178, 179, 182, 184–187, 198, 214, 273, 274, 276

Index DFT, 22, 30–33, 36–38, 40, 42, 45, 47, 50, 58, 69–71, 82, 86, 89, 130, 142, 146, 148, 151–157, 159, 160, 198, 214, 216, 222, 223, 227, 230, 235, 255, 256, 273–275 DFTB, 206, 273–275 diamond, 16, 40, 46, 52, 54, 56, 70, 78, 79, 81, 83, 84, 87, 88, 122, 133–135, 141, 146, 157, 158, 161, 195, 230, 253 dielectric function, 173 diﬀusion, 12, 14, 21, 29, 60, 101, 126, 141, 144, 145, 152, 155, 156, 194, 195, 202, 203, 214, 224, 230, 262, 263 dipole, 53, 54, 81, 158, 178 Dirac, 17 dislocation, 12, 33, 128, 195, 196, 205, 208, 230, 234, 235 disorder, 22, 43, 196, 245, 247–251, 254, 261, 269, 270, 281 dispersion, 35, 38, 47, 61, 84, 85, 89, 176, 177, 180, 181, 261 distortion, 14–16, 30, 45, 46, 54, 56–60, 153, 157, 166, 179, 182, 183, 185, 186, 195, 196, 246, 250, 252 distribution function, 219 divacancy, 14, 16, 100 DLTS, 13, 30, 49, 56, 85 donor, 12, 34, 40, 56, 57, 59, 61, 69–71, 80, 82, 84–88, 90, 258 dopant, 3, 4, 12, 13, 69, 70, 80, 89, 105, 152, 194, 196, 206 doping, 12, 13, 30, 87, 168, 180, 194, 258 double-zeta, 43, 97, 103, 259, 260, 262 DX, 5 dynamical matrix, 48, 96, 97, 99, 103, 109 DZ, 259 DZP, 43, 260 EDIP, 131, 222 eﬀective mass, 3–5, 13 eigenstates, 21, 144, 171, 172, 227, 249, 251, 257, 278, 284 eigenvalues, 12–15, 36, 39, 50, 96, 97, 103, 109, 165, 166, 168, 169,

289

172–174, 177, 179, 186, 249, 256, 257, 274 eigenvectors, 96, 97, 99–101, 109, 247, 251, 257, 260 EL2, 5 elastic embedding, 216, 220 electrical level, 58–60, 71, 80, 81, 88–90 electromagnetic radiation, 269 electron, 12, 13, 17–20, 30, 31, 33, 36, 40, 41, 45–47, 56, 58, 59, 69–71, 80, 81, 86, 87, 105, 142, 146–148, 157, 195, 196, 222, 227–229, 231, 252, 253, 259, 260, 269, 275 electron aﬃnity, 36, 170, 172, 182, 185 electron paramagnetic resonance, 12, 153 electron spin resonance, 258, 270 electron states, 32, 38, 157, 247, 250, 257, 258, 270 electron–phonon, 6, 7, 257 electron-nuclear double resonance, 30 electrostatic energy, 54, 55, 70, 159 embed, 216, 220, 225, 231, 233, 237 embedded, 129, 215, 216, 222, 223, 227, 231, 233, 278 embedding, 32, 33, 193 emission, 49 empirical, 15, 22, 85, 86, 88, 132–134, 194, 196, 198, 206, 213–216, 222–225, 230, 233, 236, 247, 250, 255–257, 259 EMT, 13, 222 ENDOR, 30, 38 energetics, 29, 30, 32, 34, 61, 108, 109, 115, 142, 158, 196, 252, 254, 255, 261, 264, 273 energy barrier, 81, 128, 154–156 energy cutoﬀ, 42, 58 energy level, 22, 30, 34, 49, 59, 105, 231, 255 entropy, 48, 104, 106, 108–110, 115, 120, 126, 131, 221, 225, 246, 251 EPR, 4, 12–15, 30, 56, 57 equilibrium, 30, 43, 47–49, 81, 96–98, 101, 107, 109, 118–120, 122–125, 127, 134, 151–155, 159, 195, 196, 206, 222, 224, 226, 227, 249, 250, 282 ergodic, 44, 220, 224

290

Index

ESR, 253, 258, 260 Ewald, 218, 222 exact exchange, 37, 38, 185 exchange, 19, 31, 32, 37–40, 49, 61, 130, 154, 220, 228, 269 exchange-correlation, 20, 21, 31, 32, 36, 39, 42, 44, 58, 71, 96, 97, 166–170, 172, 185, 187, 214, 274 excitation, 32, 38, 39, 44, 49, 57, 101, 142, 158, 165, 167–169, 171–173, 269, 270, 276, 282, 283 excited state, 34, 38, 273, 282 excited-state, 149, 157, 160 exciton, 38, 188, 231, 281 exclusion principle, 19 fast Fourier transform, 41 Fermi level, 30, 36, 37, 45, 49, 165, 167–169, 178, 184, 247, 249, 253, 255, 258 Fermi–Dirac, 51 fermion, 18, 105, 143–145, 148, 160 ﬁnite diﬀerence, 43, 48 ﬁnite element, 43, 198, 214 ﬁrst principles, 16, 21, 22, 32, 42, 43, 60, 72, 95, 96, 98, 105, 108, 157, 214, 225, 237 ﬁrst-principles, 115, 126, 127, 130, 193, 247, 250, 257 ﬂoating bond, 258, 261, 262 ﬂoating orbitals, 43 ﬂuctuation, 19, 72, 74, 119, 221, 249, 257, 274, 275 force, 14, 18, 20, 21, 32–34, 36, 40, 42, 43, 48, 59, 60, 97, 160, 198–200, 202–205, 210, 213–217, 219, 221–223, 226–228, 230, 231, 233, 247, 255, 258, 260, 261, 274, 275 force-constant matrix, 97 formation energy, 32, 40, 48, 49, 56, 80, 81, 88, 154, 156, 158, 184 fourfold, 154, 155, 252–254, 270, 282 Fourier, 13, 34, 48, 69, 95, 225, 246 free carrier, 105 free energy, 22, 44, 60, 96, 97, 102–110, 224, 225 free-energy, 115–126, 128–130, 132, 134, 136, 206 frozen phonon, 48, 97

FTIR, 13, 95 functional derivative, 169, 174 fundamental gap, 34, 36, 45, 61, 170, 174, 178 G0 W0 approximation, 165, 168, 172–180, 182–187 GaAs, 3–5 GaAs(110) surface, 176 GaN, 12, 95, 104, 167 gap, 12–16, 18, 30, 31, 35–38, 81, 82, 89, 249, 252, 269 gap levels, 13, 14, 30 gap states, 30, 35, 45, 46, 50, 168 Gaussian, 16, 42, 54, 58, 71–73, 75, 76, 79, 80, 158 Ge, 5–7, 11, 70, 87, 89, 104, 129, 150, 223, 230, 233, 235, 247, 253, 254, 270 general gradient approximation, 32, 37, 70, 130, 154, 214, 255 general gradient approximation (GGA), 166, 167, 170 germanium, 84, 86, 89, 271 gettering, 12 GGA, 32, 37–39, 42, 70, 71, 82, 89, 130, 154, 155, 214 ghost, 41, 74 Gibbs, 102, 117, 122, 123, 132, 219, 220, 225 glass, 11, 130, 131, 223, 246, 253, 254, 257, 262, 270–274, 277, 282 grain, 195, 196, 253 grain boundary, 12, 195, 196, 230 grand-canonical, 220, 225 Green’s function, 5, 6, 14, 15, 33, 34, 36, 145, 165, 171–174, 179, 181, 227, 229 Green–Kubo, 224 ground state, 30, 32, 34, 36, 47–49, 51, 61, 165, 168, 170, 171, 177, 184, 228, 234, 271, 273, 282 ground-state, 18, 20–22 ground-state, 142–145, 149, 157, 158, 160, 256, 259, 260 GW, 4, 7, 15, 22, 38, 39, 157, 256, 273 H¨ uckel, 15 Hall conductivity, 30

Index Hamiltonian, 4, 5, 14, 44, 72–75, 79, 116–120, 122, 142–145, 148, 171, 200, 204, 218–220, 227, 228, 247, 250–253, 255, 259, 274, 275 handshaking, 215, 219, 225 Hartree, 18, 20, 31, 97, 168, 169, 179 Hartree–Fock, 15, 16, 18, 19, 32, 37–39, 74, 146, 148, 273 Hedin, 39, 174 Heisenberg, 219 Heisenberg picture, 171 Hellmann–Feynman, 32, 36, 48, 214, 228, 257 Helmholtz, 44, 96, 102–104, 117 heterostructure, 231 hole, 12, 13, 39, 69, 105, 166, 172, 173, 180, 196, 269, 270, 281 HOMO, 278, 282 hopping, 228, 251 hopping integral, 180, 182 Hubbard, 253 hybrid, 32, 37, 38, 197–200, 202, 203, 205, 206, 208, 210, 222, 247, 255 hydrogen, 12, 13, 15, 16, 21, 70, 82, 84, 96, 99, 100, 148, 195, 197, 199, 204, 205, 233, 260–264 hyperﬁne, 32–34, 39, 71 imaginary, 142, 144, 148, 149, 229 impurity, 12, 14, 16, 30, 36, 45, 46, 48, 49, 80, 96, 99, 142, 152, 195, 258 InP(110) surface, 176 interface, 12, 123, 215, 216, 225, 230, 233–236 internal energy, 115, 116, 120, 224 interstitial, 14, 15, 52, 54, 87, 105–107, 126, 127, 153–157, 194 ionization, 34–36, 38, 41, 49, 50, 56, 57, 69, 87 ionization potential, 170, 172, 185 IPR, 251, 252, 257, 260, 280 irreversible, 119, 271 isothermal, 117, 224 isotope, 4, 6, 13, 95, 104 Jahn–Teller, 14, 44–46, 56, 57, 60, 153, 157, 158 jellium, 53, 222 kink, 195, 205, 206, 230

291

Kohn–Sham, 31, 32, 34–39, 42, 44, 50–52, 55, 58, 82, 157, 249, 255–257, 259, 260, 273–275, 282 Lagrange, 219, 221, 237 Lagrange parameter, 169 Lagrangian, 218, 219, 221, 225–227 LCAO, 15, 22, 56, 275 LDA, 5, 37–40, 42, 71, 77, 82, 89, 130, 156, 166–171, 173, 176, 177, 181–184, 186, 187, 214, 255, 257, 258, 261, 273 LDA+U , 40 Lennard–Jones, 119, 125, 222 linear response, 97 Liouville, 120, 219 liquid, 43, 119, 128–130, 133, 134, 143, 219, 254, 258 localization, 22, 30, 99, 109, 148, 149, 213, 217, 231, 249, 251, 257, 260, 270, 278 LOTF, 200, 203–205 LSDA, 32, 37, 58, 150, 154, 155, 158, 160 LUMO, 279, 282 Madelung, 53, 54, 81, 85, 218, 222 magnetic, 11–13, 72, 105 Makov–Payne, 54, 83 many-body perturbation theory, 171 marker, 22, 50, 51, 59, 71, 80, 82–90 Maxwell, 221 melting, 11, 122, 124, 128–130, 133–135, 233, 254 metastability, 280 metastablity, 82, 258 Metropolis, 143, 254 microcanonical, 43, 217, 220, 221, 225 midgap, 60, 251, 258 migration, 29, 34, 42, 60, 71, 95, 125, 126, 142, 154, 194, 195, 206 minimal basis, 16, 35, 259, 276 misﬁt, 230, 235 mobility, 69, 126–128, 251 molecular dynamics, 16, 22, 42–44, 60, 71, 96, 126, 154, 213, 216 molecular-dynamics, 273 molecular-dynamics, 193, 195, 198, 205, 247, 254, 255

292

Index

Monkhorst–Pack, 97, 103 Morse, 222 muﬃn-tin, 15 Mulliken, 84, 251, 260, 275 multipole, 53, 83, 89, 178, 223, 226 multiscale, 22, 60, 196, 197, 210 nanometer, 12, 195, 231 nanoscience, 12 narrow-gap, 84, 89 negative-U , 60 neutron diﬀraction, 246 Newton, 43, 227 nonlocal, 17, 32, 37, 38, 148, 167, 172, 174, 179, 180 normal mode, 48, 95–101, 103, 104 Nos´e, 221 optical, 11, 12, 30, 34, 39, 40, 49, 69, 87, 157, 231, 247, 249, 252, 256–258, 270–272, 278, 282 optoelectronic, 231 order-N , 18, 97 oxygen, 12, 14, 39, 40, 86, 107, 108, 281 pair-distribution function, 220, 224 pair-correlation function, 246, 249, 254 pairing, 46, 56 Parrinello, 21, 130, 221 partition function, 105, 106, 116–118, 121, 219, 224 Pauli, 32, 40 Perdew–Wang, 58, 71 periodic, 12, 16, 33–36, 52–55, 70, 71, 96, 97, 103, 108, 126, 148, 159, 175, 177, 178, 180, 194, 205, 250, 261 periodic boundary conditions, 15, 22, 33, 34, 43, 44, 54, 55, 69, 89, 147, 149, 220, 261 periodicity, 12, 15, 16, 34, 84, 236, 261 perturbation, 12–14, 19, 44, 54, 154, 157, 165, 167–169, 171–173, 179, 187, 221, 222 phase boundary, 119, 122–124 phase diagram, 22, 119, 125, 128, 132–135 phase space, 219, 220 phase-space, 116, 120

phonon, 6, 47, 48, 95–97, 99–104, 109, 172, 205, 223, 226, 257, 269 phosphorus, 70, 87 photoconductivity, 269, 271 photodarkening, 271, 272, 282 photoemission, 166, 170, 184, 247, 256 photoexpansion, 272 photoluminescence, 12, 13, 30, 96, 99, 194, 270, 271 photovoltaic, 246, 258 PL, 12, 30, 96, 99 plane wave, 34, 39, 41–43, 58, 69–73, 80, 160, 171, 173–175, 179 plane-wave, 21, 22 plane-wave, 259 plasmon, 172, 175, 178 platelet, 12 pnictogen, 88, 282 point defect, 30, 33, 35, 56, 146, 147, 153, 154, 165–168, 170, 194, 195, 203, 223, 230, 261 Poisson, 54, 55 polarizability, 173, 175, 178 polarization, 43, 54, 74, 78, 97, 173, 178, 179, 255, 259, 260, 271, 272 population, 22, 84, 127, 149 positron annihilation, 29, 32, 34, 61, 194 potential, 14, 18–21, 32, 34–37, 41, 42, 44, 45, 49–51, 55, 59, 61, 70, 74, 79–84, 87, 96–98, 101, 105, 110, 115, 116, 118, 121, 122, 125, 128–134, 142, 144, 145, 149, 195, 196, 201, 202, 208, 210, 214–218, 220–223, 225–228, 230, 233–235, 247, 250, 252, 254, 255, 259, 261, 262, 274–276 PRDDO, 16 precipitates, 12, 231 projected augmented wave, 41, 58 proton, 105, 195 pseudoatom, 222, 274 pseudopotential, 16, 40–42, 58, 60, 61, 71, 72, 76, 96, 148, 149, 160, 167, 171, 174, 182, 214, 222, 259 quadrupole, 81 quantum dot, 98, 225, 230, 231, 233, 236

Index quantum Monte Carlo, 18, 22, 40, 141, 142, 145–148, 150–152, 154, 157, 158, 160, 161, 256 quasiparticle, 38, 165, 167, 169–176, 179, 181–183, 185, 187, 188, 273 quasiparticle equation, 172 radial-distribution function, 224, 246, 254, 276 radiation damage, 14, 194 radiative, 69, 269, 270 Raman, 13, 95, 96, 105, 106, 269, 277 random-phase approximation, 170, 173, 175, 178 real space, 15, 42, 43, 71, 72, 97, 160, 175, 177, 246 reciprocal space, 32, 34, 42, 175 recombination, 12, 14, 34, 69, 269, 270 recursion, 227, 229 relativistic, 32 relaxation, 14, 33, 35, 36, 45, 58, 158, 166, 167, 171, 176, 179, 180, 182, 183, 185, 186, 197, 215, 216, 231, 233, 235, 236, 253, 255, 262, 271 repulsive, 45, 108, 110, 222, 230, 275 resonance, 29, 38, 45, 153, 258, 270 resonant, 96, 109, 269 reversible, 116, 119, 120, 122, 124, 131, 134, 246, 250, 271, 272 rotational, 105, 106, 109, 235, 236 Sankey, 21, 97 scalar, 271, 272 scanning tunneling microscopy (STM), 165, 166, 168, 184, 186 scattering, 15, 69, 172, 225, 269, 272, 277 scattering-Xα, 15 Schottky, 158–161 Schr¨ odinger, 13, 15, 18, 31, 44, 144 scissor, 39 screened exchange, 32, 38 screening, 38, 54, 173, 183, 218, 222, 230 self-diﬀusion, 125–127, 154, 156, 157 self-energy, 22, 157, 165, 167, 168, 172–183, 187, 256 self-interaction, 31, 37, 39, 41, 217, 233, 275

293

self-interstitial, 12, 14, 40, 125, 126, 152–154, 156, 161 self-organization, 231 self-trapped, 38, 281 semicore, 42, 55 semiempirical, 15, 16, 122, 216, 223, 274 shallow, 12, 49, 59, 60, 70, 71, 82, 84, 85, 87, 88 shear, 224, 236 Si, 6, 7, 11, 12, 14, 16, 22, 38–40, 45, 46, 56–60, 75, 77, 79, 87, 96, 99, 100, 102, 104–107, 122, 125–131, 134, 135, 150, 197, 201, 203, 205, 222, 223, 230, 235, 245–247, 249, 250, 252–254, 258–260, 262–264, 269, 270, 281 SIESTA, 21, 96, 214, 258, 262 SiGe, 89 silicon, 14, 16, 21, 22, 35, 36, 46, 52, 56, 75, 76, 78, 80, 81, 84–90, 126, 128, 130, 131, 141, 142, 152–154, 156, 157, 161, 194, 195, 197, 199, 203–205, 208, 245, 259, 261, 281 Slater, 6, 18, 40, 146, 147, 156, 158, 160, 227, 228, 279 Slater transition state, 169 special point, 52 speciﬁc heat, 97, 102, 104, 109, 130 spherical harmonic, 223 spherical harmonics, 72 spin, 12–14, 29, 30, 32, 37, 39, 41, 46, 61, 84, 105, 109, 146, 150, 158, 169, 182, 252, 253, 255, 258, 260, 270, 276 spin degeneracy, 228 spin-orbit, 3, 5, 46, 56, 58 split-vacancy, 60 Staebler–Wronski, 258, 261 statistical, 43, 116, 121, 145–147, 149, 150, 158, 216, 219, 224 Stillinger–Weber, 128–131, 203, 208, 222, 235 stoichiometry, 34, 49 Stokes, 49 strain, 35, 43, 79, 96, 195, 208, 221, 224, 225, 230, 231, 233, 236, 247, 261, 271

294

Index

stress, 13, 35, 42, 57, 95, 128, 157, 196, 197, 208, 221, 224, 247, 271 structure factor, 246 substitutional, 13, 38, 45, 46, 56, 57, 83, 84, 87, 107 supercell, 15, 16, 22, 31–36, 38–40, 43–56, 58–61, 70, 81, 84, 86–88, 90, 96, 97, 101, 103, 104, 108, 148, 159, 177–180, 182, 194, 220, 233, 283 surface, 12, 13, 15, 16, 19, 33, 36, 42, 43, 55, 61, 70, 72, 74, 75, 81, 101, 110, 120, 142, 144–147, 149, 165–169, 171, 173, 176–182, 184, 187, 197–199, 202, 208, 215, 216, 220, 230, 231, 233, 234, 250, 261, 272 surface band, 176 symmetric, 99, 101, 105, 146, 221, 278 symmetry, 13–16, 21, 30, 35, 38, 44–46, 56, 57, 59, 60, 95, 96, 99, 106, 109, 148, 149, 153, 157, 166, 176, 179, 180, 182, 183, 186, 235, 259, 273 symmetry breaking, 30, 54 Taylor, 47, 217, 222 temperature, 11, 12, 20, 22, 30, 42, 43, 49, 69, 80, 81, 87, 96–102, 104, 106–110, 115–134, 153, 154, 203–206, 208, 218, 221, 224, 233–236, 247, 249, 250, 257, 262, 272 termination, 177, 198, 199 Tersoﬀ, 129, 223, 228, 230, 235 tetrahedral, 35, 38, 45, 106, 153, 155, 156, 195, 252–254, 258 thermal disorder, 247, 249 thermal equilibrium, 48, 96, 109, 159, 249, 282 thermodynamic integration, 44, 118, 120, 122, 124, 126, 128, 132 thermodynamic ionization, 49 thermostat, 43, 96, 98, 109, 204, 205, 220, 221 Thomas–Fermi, 19, 21, 38 tight binding, 21, 175, 180, 181, 214, 215, 222, 273, 274 tight-binding, 122, 126, 127, 129, 134, 198, 203, 204, 206, 247, 250, 255

tiling, 145 time-dependent density-functional theory (TDDFT), 39, 44, 282 time-dependent Schr¨ odinger equation (TDSE), 44 total energy, 19, 21, 30–32, 34, 43, 45, 47–53, 56, 58, 73, 75, 79, 96, 98, 159, 168–170, 179, 182, 184, 185, 199, 204, 217, 220, 233, 247, 252, 260, 274, 275 trajectory, 44, 120, 199, 200, 203, 219, 220, 262 transferability, 15, 41, 222, 230, 236 transient-enhanced diﬀusion, 12 transition, 49, 81–83, 119, 122, 125, 128, 131, 134, 135, 157, 158, 200, 217, 218, 222, 228, 231, 233, 246, 251, 254, 269, 270, 272 transition level, 30, 49, 51 transition metal, 11, 12, 14, 57, 58, 142 transport, 221, 224, 245, 269 trigonal, 46, 58, 60, 282 ultrasoft pseudopotential, 41, 58, 59, 70 uniaxial stress, 13, 95, 157 vacancy, 12, 14–16, 35, 38, 40, 45, 46, 52, 54, 56, 60, 81, 86, 96, 125–127, 153, 154, 157–159, 161, 203 valence band, 12, 35, 38, 40, 49–51, 55, 56, 81–83, 88, 105, 169, 170, 176–178, 180, 182, 184, 269–271, 278 Van der Waals, 222, 270 variational, 18, 20, 31, 43, 73, 141, 143, 148, 149, 218, 259, 275 VASP, 58–60 vectoral, 271, 272 velocity autocorrelation, 48, 224 Verlet, 217 vibrational dynamics, 30 vibrational entropy, 48, 60, 104, 126 vibrational free energy, 60, 97, 104, 105, 107, 109 vibrational lifetime, 96–98, 100, 101, 109 vibrational modes, 22, 29, 33, 34, 47, 48, 61, 71, 84, 85, 95, 96, 99

Index vibrational spectroscopy, 12, 13, 29, 95, 96 wafer bonding, 215, 230, 233–235 wag, 96, 99, 101 Wannier, 14, 252 water, 130–134, 223 Watkins, 15, 45, 46, 56

wavelength, 52, 231, 246, 269, 271 Wigner–Seitz, 35, 55 X-ray, 225, 246, 269 zincblende lattice, 176 ZnO, 40, 82

295

Our partners will collect data and use cookies for ad personalization and measurement. Learn how we and our ad partner Google, collect and use data. Agree & close